Nonlinear Mechanics of Crystals
SOLID MECHANICS AND ITS APPLICATIONS Volume 177
Series Editor:
G.M.L. GLADWELL Department of Civil Engineering University of Waterloo Waterloo, Ontario, Canada N2L 3GI
Aims and Scope of the Series The fundamental questions arising in mechanics are: Why?, How?, and How much? The aim of this series is to provide lucid accounts written by authoritative researchers giving vision and insight in answering these questions on the subject of mechanics as it relates to solids. The scope of the series covers the entire spectrum of solid mechanics. Thus it includes the foundation of mechanics; variational formulations; computational mechanics; statics, kinematics and dynamics of rigid and elastic bodies: vibrations of solids and structures; dynamical systems and chaos; the theories of elasticity, plasticity and viscoelasticity; composite materials; rods, beams, shells and membranes; structural control and stability; soils, rocks and geomechanics; fracture; tribology; experimental mechanics; biomechanics and machine design. The median level of presentation is the first year graduate student. Some texts are monographs defining the current state of the field; others are accessible to final year undergraduates; but essentially the emphasis is on readability and clarity.
For other titles published in this series, go to www.springer.com/series/6557
John D. Clayton
Nonlinear Mechanics of Crystals
John D. Clayton US Army Research Laboratory RDRLWMPB Bldg 390, Room 212 Aberdeen Proving Ground Maryland 210055066 USA
[email protected] ISSN 09250042 eISBN 9789400703506 ISBN 9789400703490 DOI 10.1007/9789400703506 Springer Dordrecht Heidelberg London New York © Springer Science+Business Media B.V. 2011 No part of this work may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, microfilming, recording or otherwise, without written permission from the Publisher, with the exception of any material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work. Cover design: SPI Publisher Services Printed on acidfree paper
Springer is part of Springer Science+Business Media (www.springer.com)
Preface
This book presents mathematical descriptions of behavior of crystalline solids following theoretical methods of modern continuum mechanics. Emphasis is placed on geometrically nonlinear descriptions, i.e., finite or large deformations. Topics include elasticity, plasticity, and ways of representing effects of distributions of defects or flaws in the solid on the material’s thermomechanical response. Defects may include crystal dislocations, point defects such as vacancies or interstitial atoms, rotational defects, deformation twins, voids or pores, and microcracks. Representative substances towards which modeling techniques forwarded here may be applied are single crystalline and polycrystalline metals and alloys, ceramics, minerals, and other geologic materials and their constituents. An early and substantial part of the text is devoted to kinematics of finite deformations, multiplicative inelasticity, and representations of lattice defects in a differentialgeometric setting. An accurate depiction of kinematics is deemed necessary in order to accompany rigorous models of thermodynamics and kinetics of material behavior, since kinematic assumptions tend to enter, implicitly or explicitly, subsequent thermodynamic and kinetic relations. Descriptions and derivations of fundamental mechanical and thermodynamic balance laws and inequalities are then given. Constitutive frameworks are provided for representing thermomechanical behaviors of various classes of crystalline materials: elastic solids, elasticplastic solids, generalized inelastic solids with lattice defects, and dielectric solids. In each case, material responses corresponding to large deformations are emphasized, though complementary geometrically linear theories are included in some cases for completeness and for comparison with their nonlinear counterparts. General kinetic concepts are described, but relatively less attention is directed towards development of specific kinetic relations, since these tend to be more strongly dependent upon microstructures of particular materials (e.g., crystal structure or chemical composition) within each general class of materials considered. Appendices provide supporting discussion on crystal symmetry and material coefficients, atomistic methods (i.e., lattice statics and origins of stress and elastic coefficients), and elastic models of discrete line and point defects in crystals. The content of this book consists of a combination of the author’s
vi
Preface
interpretation and consolidation of existing science from historic and more recent literature, as well as a number of novel—and sometimes less conventional—theoretical modeling concepts, the latter often presented, developed, or refined by the author (and collaborators in many cases) in a number of archival publications over the past ten years. With a few exceptions, the text is written in the context of generalized (e.g., curvilinear) coordinates, a rarity among other recent texts and monographs dealing with similar subject matter. This book is intended for use by scientists and engineers involved in advanced constitutive modeling of nonlinear mechanical behavior of crystalline materials. Knowledge of fundamentals of continuum mechanics and tensor calculus is a prerequisite for accessing much of the material in the text. The book could conceivably be used as supplemental material in graduatelevel courses in continuum mechanics, elasticity, plasticity, micromechanics, or dislocation mechanics, for students in various disciplines of engineering, materials science, applied mathematics, or condensed matter physics. A number of individuals have contributed, directly or indirectly, to the content or production of this work; a number have suggested specific changes to early drafts resulting in significant overall improvement to the final manuscript. Technical discussions, interactions, and/or close collaborations with the following individuals over the past decade are gratefully acknowledged (in alphabetical order): Doug Bammann, Peter Chung, Datta Dandekar, Misha Grinfeld, Jarek Knap, Dave McDowell, Rich Regueiro, Mike Scheidler, and Tim Wright. However, any technical inconsistencies, unjust omissions, or errors that may remain are entirely my own. I also appreciate support and resources of the U.S. Army Research Laboratory (formerly known as U.S. Army Ballistics Research Laboratories), including a diligent library staff that was able to efficiently provide or obtain a number of historical works referenced in this text. Finally, I am most appreciative of my wife and daughter, who have remained supportive and patient during the many hours I have spent working on this book over the past 3½ years.
John D. Clayton Aberdeen, Maryland, USA 2010
Contents
1 Introduction............................................................................................. 1 1.1 Objectives and Scope........................................................................ 1 1.2 Background....................................................................................... 6 1.3 Notation ............................................................................................ 7 2 Mathematical Foundations .................................................................. 11 2.1 Geometric Description of a Deformable Body ............................... 12 2.1.1 Terminology ............................................................................ 12 2.1.2 Manifolds, Coordinates, and Metrics....................................... 15 2.2 Linear Connections......................................................................... 22 2.2.1 The Covariant Derivative and Connection Coefficients.......... 22 2.2.2 Torsion and Curvature ............................................................. 25 2.2.3 Identities for the Connection Coefficients and Curvature ....... 26 2.2.4 The LeviCivita Connection .................................................... 28 2.3 Notation, Differential Operators, and Other Identities ................... 31 2.4 Physical Components ..................................................................... 35 2.4.1 General Orthogonal Coordinates ............................................. 35 2.4.2 Cylindrical Coordinates........................................................... 36 2.4.3 Spherical Coordinates.............................................................. 37 2.5 The Deformation Gradient.............................................................. 38 2.5.1 Fundamentals........................................................................... 38 2.5.2 Derived Kinematic Quantities and Identities........................... 43 2.5.3 Linearization............................................................................ 47 2.6 Velocities and Time Differentiation ............................................... 48 2.6.1 The Material Time Derivative ................................................. 48 2.6.2 The Lie Derivative................................................................... 51 2.6.3 Rate Kinematics....................................................................... 52 2.7 Theorems of Gauss and Stokes....................................................... 53 2.7.1 Gauss’s Theorem ..................................................................... 53 2.7.2 Stokes’s Theorem .................................................................... 55 2.8 Anholonomic Spaces and Compatibility ........................................ 57 2.8.1 Anholonomicity ....................................................................... 57 2.8.2 Strain Compatibility ................................................................ 59
viii
Contents
2.8.3 Connection Compatibility........................................................ 61 2.8.4 The Jacobian Determinant for Anholonomic Mappings ......... 62 3 Kinematics of Crystalline Solids.......................................................... 65 3.1 Crystals and Lattice Deformation................................................... 67 3.1.1 Crystal Structures .................................................................... 67 3.1.2 The CauchyBorn Hypothesis ................................................. 75 3.1.3 Elastic Deformation and Thermal Deformation ...................... 78 3.2 Multiplicative Inelasticity............................................................... 80 3.2.1 Background.............................................................................. 80 3.2.2 The Multiplicative Decomposition .......................................... 81 3.2.3 The Metric Tensor in the Intermediate Configuration............. 87 3.2.4 Kinematics, Rates, and Kinematic Approximations................ 92 3.2.5 Dislocation Plasticity............................................................... 95 3.2.6 Crystal Plasticity.................................................................... 108 3.2.7 Macroscopic Plasticity........................................................... 111 3.2.8 Inelastic Volumetric Deformation ......................................... 112 3.2.9 Residual Deformation and a Multiscale Description............. 116 3.2.10 Multiplicative Atomistic Plasticity ...................................... 125 3.3 A Linear Connection for Lattice Defects...................................... 127 3.3.1 General Form and Properties of the Connection ................... 129 3.3.2 Dislocations and the Crystal Connection............................... 136 3.3.3 Disclinations .......................................................................... 146 3.3.4 Point Defects ......................................................................... 160 3.3.5 Summary................................................................................ 164 4 Thermomechanics of Crystalline Solids ........................................... 167 4.1 Classical Balance Laws and Definitions....................................... 169 4.1.1 Definitions ............................................................................. 169 4.1.2 Mass Conservation ................................................................ 173 4.1.3 Momentum Conservation ...................................................... 174 4.1.4 Energy Conservation ............................................................. 178 4.2 Internal State Variables and the Dissipation Inequality................ 181 4.2.1 Constitutive and Internal Variables for Crystalline Solids .... 183 4.2.2 The ClausiusDuhem Inequality ............................................ 188 4.3 Kinetics and Inelastic Rates.......................................................... 191 5 Thermoelasticity ................................................................................. 197 5.1 Nonlinear Elasticity and Thermoelasticity ................................... 199 5.1.1 Constitutive Assumptions...................................................... 199 5.1.2 Thermodynamics ................................................................... 203 5.1.3 Materially Nonlinear Hyperelasticity .................................... 207
Contents
ix
5.1.4 Materially Linear Hyperelasticity.......................................... 213 5.1.5 Symmetry .............................................................................. 214 5.2 Thermostatic Relationships .......................................................... 221 5.2.1 Threedimensional Stress States ............................................ 221 5.2.2 Hydrostatic Stress States ....................................................... 226 5.3 Finite Elastic Volume Changes .................................................... 235 5.4 Geometrically Linear Elasticity .................................................... 238 5.4.1 Constitutive Assumptions...................................................... 238 5.4.2 Thermodynamics ................................................................... 240 5.4.3 Materially Nonlinear Hyperelasticity .................................... 241 5.4.4 Materially Linear Hyperelasticity.......................................... 245 5.4.5 Symmetry .............................................................................. 246 5.5 Explicitly Resolved Thermal Deformation................................... 248 5.5.1 Constitutive Assumptions...................................................... 249 5.5.2 Thermodynamics ................................................................... 250 5.5.3 Representative Free Energy................................................... 252 5.6 Lagrangian Field Theory of Elasticity .......................................... 255 5.6.1 The Variational Derivative .................................................... 256 5.6.2 Hamilton’s Principle in Nonlinear Elasticity......................... 257 5.7 Elasticity of Grade Two................................................................ 262 6 Elastoplasticity .................................................................................... 273 6.1 Twoterm Multiplicative Elastoplasticity ..................................... 275 6.1.1 Constitutive Assumptions...................................................... 277 6.1.2 Thermodynamics ................................................................... 280 6.1.3 Representative Free Energy................................................... 288 6.2 Dislocation Plasticity .................................................................... 292 6.3 Crystal Plasticity........................................................................... 297 6.4 Macroscopic Plasticity.................................................................. 305 6.5 Geometrically Linear Elastoplasticity .......................................... 311 6.5.1 Constitutive Assumptions...................................................... 311 6.5.2 Thermodynamics ................................................................... 312 6.5.3 Representative Free Energy................................................... 313 6.5.4 Linearized Dislocation Plasticity........................................... 314 6.5.5 Linearized Crystal Plasticity.................................................. 315 6.5.6 Linearized Macroscopic Plasticity......................................... 316 6.6 The Eshelby Stress........................................................................ 317 6.7 Elastoplasticity of Grade Two ...................................................... 323 6.7.1 Covariant and Variational Derivatives .................................. 324 6.7.2 Constitutive Assumptions and Governing Equations ............ 326 6.7.3 Relationship to Dislocation Theory ....................................... 333
x
Contents
7 Residual Deformation from Lattice Defects ..................................... 337 7.1 Multiplicative Kinematics ............................................................ 339 7.1.1 Plastic Deformation ............................................................... 340 7.1.2 Lattice Deformation............................................................... 342 7.1.3 Multiplicative Decomposition of Total Deformation ............ 343 7.2 Nonlinear Elastic Interpretation of Residual Elasticity ................ 344 7.2.1 Selfequilibrium Conditions .................................................. 345 7.2.2 Hyperelasticity....................................................................... 346 7.2.3 Average Residual Elastic Strain ............................................ 347 7.2.4 Residual Elastic Volume Changes......................................... 351 7.2.5 Straight Edge and Screw Dislocations................................... 357 7.2.6 Approximate Volume Changes ............................................. 360 7.2.7 Examples: Dislocations and Disclinations in Copper............ 361 7.3 Atomistic Interpretation of Residual Elasticity ............................ 365 7.3.1 Atomic Stress Measures ........................................................ 366 7.3.2 Harmonic and Anharmonic Interactions................................ 367 7.3.3 Residual Deformation in a Selfequilibrated Lattice ............. 369 7.4 Point Defects and Residual Elasticity........................................... 373 7.4.1 Spherical Deformation from a Point Defect .......................... 373 7.4.2 Example: Vacancies in Copper.............................................. 376 8 Mechanical Twinning in Crystal Plasticity ...................................... 379 8.1 Mechanisms: Elasticity, Slip, and Twinning ................................ 382 8.1.1 Elasticity ................................................................................ 382 8.1.2 Plastic Slip ............................................................................. 384 8.1.3 Deformation Twinning .......................................................... 385 8.2 Crystal Plasticity with Twins and Inelastic Volume Changes ...... 394 8.2.1 Kinematics............................................................................. 394 8.2.2 Constitutive Assumptions...................................................... 401 8.2.3 Thermodynamics ................................................................... 403 8.2.4 Representative Free Energy................................................... 406 8.2.5 Kinetics.................................................................................. 416 9 Generalized Inelasticity...................................................................... 423 9.1 Threeterm Elastoplasticity: General Principles ........................... 425 9.1.1 Kinematics and Summary of Physical Mechanisms.............. 425 9.1.2 Constitutive Assumptions...................................................... 427 9.1.3 Thermodynamics ................................................................... 430 9.2 Porous Elastoplasticity ................................................................. 435 9.2.1 Void Nucleation and Growth................................................. 436 9.2.2 Continuum Damage Mechanics............................................. 443 9.2.3 Volumetric Compaction and Pore Collapse .......................... 446
Contents
xi
9.3 Multiscale Description of Residual Elasticity .............................. 449 9.4 Inelasticity with Dislocations and Disclinations........................... 451 9.4.1 Background............................................................................ 452 9.4.2 Kinematics............................................................................. 455 9.4.3 Constitutive Assumptions...................................................... 457 9.4.4 Thermodynamics ................................................................... 460 9.4.5 Macroscopic and Microscopic Momentum Balances............ 461 9.4.6 Representative Free Energy................................................... 465 9.4.7 Kinetics and Evolution Equations ......................................... 472 9.4.8 Dislocation Theory ................................................................ 477 10 Dielectrics and Piezoelectricity ........................................................ 481 10.1 Maxwell’s Equations .................................................................. 483 10.1.1 Classical Electrodynamics ................................................... 484 10.1.2 Lorentz and Galilean Invariance.......................................... 487 10.2 Electrostatics of Dielectric Media .............................................. 490 10.2.1 Maxwell’s Equations of Electrostatics ................................ 490 10.2.2 Material Forms of Maxwell’s Equations ............................. 495 10.2.3 Momentum Conservation .................................................... 496 10.2.4 Energy Conservation ........................................................... 500 10.2.5 Entropy Production.............................................................. 503 10.3 Elastic Dielectric Solids.............................................................. 504 10.3.1 Constitutive Assumptions.................................................... 504 10.3.2 Thermodynamics ................................................................. 508 10.3.3 Material Coefficients ........................................................... 511 10.3.4 Representative Free Energy................................................. 519 10.3.5 Materially Linear Electroelasticity ...................................... 523 10.3.6 Symmetry ............................................................................ 525 10.3.7 Comparison with Other Theories......................................... 529 10.4 Linear Elastic Dielectric Solids .................................................. 534 10.4.1 Governing Equations ........................................................... 535 10.4.2 Constitutive Assumptions.................................................... 535 10.4.3 Thermodynamics ................................................................. 536 10.4.4 Representative Free Energy................................................. 537 10.4.5 Constitutive Equations of Linear Piezoelectricity ............... 541 Appendix A: Crystal Symmetries and Elastic Constants................... 543 A.1 Crystal Classes, Point Groups, and Laue Groups ........................ 543 A.2 Generic Material Coefficients...................................................... 547 A.3 Elastic Constants.......................................................................... 553 A.3.1 Cubic Symmetry ................................................................... 558 A.3.2 Transverse Isotropy .............................................................. 559
xii
Contents
A.3.3 Isotropy................................................................................. 560 Appendix B: Lattice Statics and Dynamics ......................................... 567 B.1 Dynamics ..................................................................................... 567 B.1.1 Newton’s Equations .............................................................. 567 B.1.2 Lagrange’s Equations............................................................ 568 B.1.3 Hamilton’s Equations............................................................ 569 B.2 Statics........................................................................................... 571 B.2.1 Governing Equations ............................................................ 571 B.2.2 Interatomic Potentials and Forces ......................................... 572 B.2.3 Kinematics of Homogeneous Deformation........................... 576 B.2.4 Stresses and Moduli for Homogeneous Deformations ......... 578 B.2.5 Harmonic and Anharmonic Interactions ............................... 583 B.2.6 Examples: Pair Potential and Embedded Atom Method....... 587 Appendix C: Discrete Defects in Linear Elasticity ............................. 593 C.1 Volterra Defects ........................................................................... 594 C.1.1 Edge Dislocation................................................................... 598 C.1.2 Screw Dislocation ................................................................. 602 C.1.3 Twist Disclination................................................................. 604 C.1.4 Wedge Disclination............................................................... 609 C.1.5 Mixed Line Defects .............................................................. 612 C.1.6 Dislocation Energies in Anisotropic Crystals ....................... 613 C.2 Defect Loops................................................................................ 616 C.3 Point Defects................................................................................ 619 C.3.1 Rigid Defect in Infinite Body ............................................... 621 C.3.2 Rigid Defect in Finite Body.................................................. 623 C.3.3 Deformable Defect in Finite Body........................................ 625 C.4 Dislocation Nucleation and Motion ............................................. 627 C.4.1 Frenkel Model....................................................................... 627 C.4.2 Loop Nucleation in a Perfect Crystal.................................... 628 C.4.3 Peierls Model ........................................................................ 630 Appendix D: Kinematic Derivations .................................................... 641 D.1 Total Covariant Derivative of Deformation Gradient.................. 641 D.2 Piola’s Identity for the Jacobian Determinant ............................. 642 D.3 Compatibility Conditions via Convected Coordinates ................ 646 D.4 Anholonomic Connection Coefficients ....................................... 648 Appendix E: SI Units and Fundamental Constants............................ 653 E.1 Units ............................................................................................. 653 E.2 Fundamental Constants ................................................................ 654
Contents
xiii
References............................................................................................... 657 Index........................................................................................................ 691
1 Introduction
1.1 Objectives and Scope This book presents modeling techniques, primarily from the standpoint of modern continuum mechanics, for describing the nonlinear response of crystalline solids subjected to mechanical loading or deformation. This response may be deformation induced by applied loading, or the forces required to induce such deformation. Nonlinearity may emerge in the geometric sense, pertaining to finite deformations, and/or in the material sense, pertaining to nonlinear relationships among independent and dependent state variables, for example relationships between strain and stress. Though mechanical behavior is of primary interest in this book, thermodynamic principles are exercised for developing descriptions of material behavior also dependent on temperature and internal state variables and consistent with known balance laws or inequalities such as conservation of energy and production of entropy. Though some physical and mathematical principles applicable towards descriptions of all kinds of materials are supplied in early Chapters, the content of this book is primarily focused on crystalline solids. A crystal refers to a body whose atoms occupy an ordered, repeating structure called a lattice. Defects in the crystal may disrupt the regularity of the lattice, and certain types of point, line, and surface defects are addressed explicitly in this book. A body with defects is still considered here to be crystalline so long as a large percentage of its atoms maintain a repeating, ordered structure. In various instances throughout the text, single or polycrystalline materials are considered, as are homogeneous and heterogeneous solids. In a single crystal, the lattice is for the most part aligned in a uniform orientation, whereas a polycrystal consists of multiple single crystals or grains aligned in potentially different directions, with constituent crystals separated by grain boundaries. Heterogeneous materials exhibit spatial variations in material properties, for example composites consisting of different phases with different chemical compositions or different crystal
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_1, © Springer Science+Business Media B.V. 2011
1
2
1 Introduction
structures. Specific examples of heterogeneous solids include metalmatrix composites and geologic and cementious materials with several crystalline constituents, e.g., minerals of various crystal structures. In contrast, single crystals are conventionally idealized as homogeneous, at least when their defect content is low. During the course of deformation or a change in environment, initially homogeneous single crystals can become heterogeneous. For example, misoriented subgranular regions can emerge within metallic crystals deformed plastically to large strains. Detailed consideration of material nonlinearity requires a description of microstructure and defects in the solid, including effects of such defects on kinematics of deformation and on the thermodynamic state of the material. Furthermore, kinetic relations are often required to dictate the temporal evolution of defect distributions and to account for their motions and dissipated energy during timedependent problems. Defects considered explicitly in this text include distributions of dislocations, rotational line defects, deformation twins, vacancies, and voids. Chapter 2 provides mathematical background used subsequently throughout the text. Chapter 2 begins with a description of general curvilinear coordinates and related definitions from differential geometry and tensor algebra on manifolds. Such definitions emerge frequently later in presentations of theories of continuously distributed lattice defects. A thorough treatment of the deformation gradient, a fundamental kinematic variable used in continuum mechanical descriptions of constitutive behavior, is provided. This treatment includes discussion of pushforward and pullback operations, useful identities associated with the deformation gradient, and deformation measures derived from it. Chapter 2 also presents two identities from tensor calculus used often later in the text: Gauss’s theorem—a particular version of which is often called the divergence theorem—and Stokes’s theorem. Compatibility conditions for finite deformation are discussed, and anholonomic spaces are introduced. Chapter 3 focuses on descriptions of deformation kinematics of crystalline bodies. This Chapter begins with the fundamental hypothesis of Cauchy and Born describing homogeneous deformations of Bravais lattice vectors and basis vectors comprising the structure of a perfect crystal. Kinematics of multiplicative inelasticity is then considered. The intermediate configuration that emerges under the assumption of multiplicative deformation gradient kinematics is addressed from a general geometric point of view, regardless of the physical origin of inelastic response. Then particular physical sources of nonrecoverable deformation are treated in various kinematic descriptions. These include dislocationbased large deformation plasticity of single and polycrystalline materials, generation and motion of point defects, porosity evolution, and sources of residual elastic
1.1 Objectives and Scope
3
deformation of the lattice emerging from multiscale considerations. Chapter 3 then addresses generalized continua embedded with additional kinematic degrees of freedom that describe spatial gradients of deformation of lattice director vectors, whereby locally inhomogeneous deformations can often be associated with the presence of lattice defects. These additional degrees of freedom are introduced in the differentialgeometric context of a linear connection on a spatial manifold whose tangent bundle is spanned by a field of deformed director vectors. Geometric properties of the connection enable physical characterization of deformation incompatibilities resulting from continuous distributions of line and point defects. Chapter 4 features general, traditional thermodynamic relationships and balance laws governing nonlinear behaviors of continuous bodies. The discussion begins with presentation of traditional mass, momentum, and energy balances. Mappings of balance equations among configurations or deformation states are given. Thermodynamic potentials are defined. The internal state variable concept is introduced, enabling representation of effects of defects or evolving microstructure in the description of the thermodynamic state of the material. The dissipation inequality is presented, followed by a brief introduction to kinetic relations and dissipation potentials. Governing equations for generalized continua supporting higherorder stresses (e.g., couple stresses) and those incorporating electromechanical effects are addressed on a casebycase basis in later Chapters. Chapter 5 considers elastically deforming solids, a description most applicable to defectfree crystals or to those wherein any effects of defects are not considered explicitly. Constitutive functions and thermodynamic relationships are presented for crystals displaying a hyperelastic response with temperature changes. Thermoelastic material coefficients pertinent to arbitrary threedimensional stress states, and then those specifically applicable to (but not always limited to) spherical stress states, are defined or derived. Reductions of the general theory of nonlinear anisotropic thermoelasticity under conditions of material linearity, geometric linearity, and isotropic symmetry are described. A thorough presentation of symmetry operations, anisotropy, and material coefficients for all thirtytwo crystal classes is provided as supplementary supporting material in Appendix A. An alternative version of finite elasticity with explicitly delineated mechanical and thermal deformations is then developed. Next, Lagrangian field theory of elasticity is presented, wherein governing equations are deduced from Hamilton’s principle. Chapter 5 concludes with a discussion of secondgrade hyperelasticity, a kind of generalized continuum theory. Chapter 6 deals with elastoplastic materials. The kinematic description consists of a multiplicative decomposition of the deformation gradient into two terms: the latticealtering thermoelastic deformation associated with
4
1 Introduction
mechanical stresses and temperature changes, and the latticepreserving plastic deformation resulting from glide of dislocations. Thermodynamic relationships are derived via consideration of thermodynamic potentials on a perunitvolume basis in the thermoelastically unloaded intermediate configuration. A variant of the socalled Eshelby stress emerges as a work conjugate stress measure to the plastic velocity gradient. This stress measure is examined in some detail in a later Section of Chapter 6. The stored energy of cold working—reflected via internal state variables related to defects and microstructural features—is considered. Specific applications of the general finite deformation theory towards describing plasticity resulting from distributed line defects (i.e., dislocation dynamics) and crystallographic slip on discrete glide systems (i.e., crystal plasticity) are discussed in turn. Kinetic equations for plastic flow and time rates of internal variables are considered briefly in each case. Reduction of the finite deformation theory to geometrically linear elastoplasticity is presented for completeness. Chapter 6 concludes with description of a generalized continuum theory incorporating secondgrade elasticity with multiplicative elasticplastic kinematics. Chapter 7 addresses large deformation kinematics and internal forces arising from defects in crystalline solids by combining a nonlinear kinematic description with multiscale averaging concepts. An element of material containing defects such as dislocation lines and loops is considered. The average deformation gradient for this element is decomposed multiplicatively into terms accounting for effects of dislocation flux, recoverable elastic stretch and rotation, and residual elastic deformation associated with selfequilibrating internal forces induced by defects. Two methods are considered for quantifying the average residual elastic deformation gradient: continuum nonlinear elasticity and discrete lattice statics. Volume changes resulting from point defects such as vacancies are discussed in the final Section of Chapter 7. Supporting background information on lattice statics pertinent to the content of Chapter 7, including atomic origins of elasticity coefficients, is provided in Appendix B. Pertinent supporting information on residual elastic stress fields and strain energies induced by line and point defects is provided in Appendix C. Chapter 8 extends the introductory treatment of crystal plasticity developed in Chapter 6 to encompass thermoelasticity, residual elastic volume changes, plastic slip, and mechanical twinning in anisotropic single crystals subjected to arbitrarily large deformations. Dislocation glide and deformation twinning are treated as dissipative mechanisms, while energy storage mechanisms associated with dislocation lines and twin boundaries are described via internal state variables. Shear strain rates for discrete glide and twinning systems are modeled explicitly. Residual elastic vol
1.1 Objectives and Scope
5
ume changes, predicted from nonlinear elasticity using theoretical methods developed in Chapter 7, are proportional to dislocation line length per unit volume and twin boundary area per unit volume. Chapter 9 broadens the constitutive description of elastoplastic materials to encompass a number of more general modes of inelastic deformation. The kinematic description forwarded in Chapter 9 features a threeterm decomposition of the deformation gradient into recoverable elastic deformation, latticepreserving plastic deformation, and an intermediate term associated with irreversible lattice rearrangements. A general thermodynamic analysis proceeds with the intermediate term of the deformation gradient entering the thermodynamic potentials as a generic independent state variable, leading to general constitutive relationships and a reduced dissipation inequality. Particular versions of this generic framework for inelasticity are then developed to address physics of isotropic void growth, pore compaction, and residual lattice deformation from defects. The last Section of Chapter 9 describes a secondgrade theory of elastoplasticity accounting for geometrically necessary dislocations and disclinations. Micropolar kinematics and microscopic balance laws featuring higherorder stresses enter the description. This nonlocal theory is intended to represent the constitutive response of ductile crystals exhibiting drastic microstructural changes such as grain refinement occurring during severe plastic deformation processes. Chapter 10 depicts the geometrically nonlinear response of dielectric crystalline solids. A dielectric crystal is defined as an insulator (i.e., a nonconductor of electricity) that may exhibit electric polarization. Maxwell’s complete set of electrodynamic equations are presented; however, electrodynamics and magnetization are not formally addressed in the constitutive theory developed later in Chapter 10. Rather, mechanical, thermal, and quasielectrostatic behaviors, and their couplings, are considered simultaneously. Forces of electromechanical origin contribute to balance laws of momentum and energy and the dissipation inequality, resulting in discrepancies from the traditional continuum mechanical description of Chapter 4. In particular, the presence of Maxwell’s stress associated with nonlinear electromechanics can render the Cauchy stress, as defined in the present context, nonsymmetric. A thermodynamic treatment is developed that addresses dielectric, piezoelectric, pyroelectric, and electrostrictive phenomena. Material coefficients of various orders, and relationships among these coefficients, are defined or derived. Reduction of the nonlinear theory to the traditional geometrically and materially linear theory of piezoelectric materials is presented for completeness. The following topics are not addressed extensively in this book: viscoelastic behavior, lattice vibrations, acoustic wave propagation, electrody
6
1 Introduction
namics (including optics), electrical conduction, magnetism, phase transformations, mass transport, liquid crystals, or fracture mechanics of discrete cracks. Brief coverage of atomic lattice statics and dynamics is given in Appendix B; this Appendix does not, however, contain a complete description of classical particle mechanics, nor does it include discussion of electronic structure or fundamental topics in quantum mechanics. Because of the inherent nonlinearity of many of the models presented, numerical methods become necessary for obtaining solutions of the governing equations of mechanics when used in conjunction with many constitutive relationships discussed in this book. Methods for numerically approximating solutions of governing equations (with requisite boundary and initial conditions) of thermomechanical problems involving nonlinear constitutive models are beyond the scope of this book. Discussions of solutions of specific boundary value problems are primarily limited, in this book, to those considered in the context of discrete, elastic defect models of Appendix C.
1.2 Background An attempt to provide adequate historical perspective for the content of this book would require an entire volume in itself. Instead, a brief collection of books and review articles is suggested below, and presumably adequate historical context can be found, collectively, in these references. The list is limited to books and review articles published in the 20th century or later, and is divided into relevant categories. Some of the listed references clearly could belong to multiple categories. Omission of other relevant references is certain but is not intentional; those references listed below have been particularly useful during preparation of this book. • • • •
Mathematics and geometry: Eisenhart (1926), Schouten (1954), Brillouin (1964), Marsden and Hughes (1983), Epstein and Elzanowski (2007) Continuum mechanics: Eringen (1962), Sedov (1966), Malvern (1969), Gurtin (1981) Elasticity: Love (1927), Landau and Lifshitz (1959), Wang and Truesdell (1973), Thurston (1974) Plasticity: Hill (1950), Schmid and Boas (1950), Kocks et al. (1975), Lubliner (1990), Havner (1992), Khan and Huang (1995), NematNasser (2004)
1.3 Notation
• •
7
Defect mechanics and micromechanics: Eshelby (1956), Nabarro (1967), Hirth and Lothe (1982), Mura (1982), Teodosiu (1982), NematNasser and Hori (1999), Phillips (2001), Buryachenko (2007) Electromechanics: Stratton (1941), Landau and Lifshitz (1960), Maugin (1988), Jackson (1999)
Also notable are books of Born and Huang (1954), Maradudin et al. (1971), and Wallace (1972) that consider atomic, and in some instances quantum mechanical, origins of thermoelastic and/or electromechanical behavior in crystals. Finally, works by Truesdell and Toupin (1960) and Truesdell and Noll (1965), the former with an Appendix by Ericksen (1960), address many relevant topics in mechanics and provide an extensive bibliography of historical contributions to the field.
1.3 Notation Throughout the text, boldface type is generally used to denote vectors and tensors of higher order, while italic type is usually used for scalars and individual components of vectors and tensors. Notable exceptions are the zero vector and null tensor, both of which are simply written in Roman font (i.e., not boldface). The index notation is used frequently for describing vector and tensor variables. The index notation complements the direct or boldface notation, often providing increased clarification. Another advantage of the index notation is that it is straightforwardly converted to computer programming languages enabling matrix operations (e.g., addition and multiplication) often involved in numerical solutions of boundary value problems. The Einstein summation convention is followed unless noted otherwise, with summation implied over repeated contravariant (superscript) and covariant (subscript) pairs. For example, a scalar or dot product is computed as V aWa = V 1W1 + V 2W2 + V 3W3 for components of contravariant vector V and covariant vector W in threedimensional vector space. In the index notation, fonts used for indices of vectors and higherorder tensors also follow a certain convention. Specifically, indices associated with the spatial (i.e., deformed or current) configuration are usually written in lower case Roman font, e.g., V a . Indices associated with the reference (i.e., undeformed or initial) configuration are usually written in upper case Roman font, e.g., V A . Indices associated with other configurations (for example, one or more intermediate configuration(s) of multiplicative inelasticity) are usually written in Greek font, e.g., V α .
8
1 Introduction
Regarding higherorder tensors, indices in parentheses are symmetric, and indices in braces are antisymmetric (i.e., skew). For example, let Aab be covariant components of an arbitrary secondorder tensor A. Then A( ab ) = (1/ 2)( Aab + Aba ) , A[ab] = (1/ 2)( Aab − Aba ) , and A( ab ) + A[ab] = Aab . Following the usual notation scheme of continuum mechanics, labels “order” and “rank” are used interchangeably throughout the text to denote the total number of associated indices (both contravariant and covariant) of tensors, matrices, and more general mathematical objects. For example, a tensor A with contravariant components Aab is said to be of second order, or rank two. A vector can be interpreted as a tensor of rank one, and a scalar can be considered a tensor of rank zero. The term “rank” as used here differs from formal definitions often encountered in linear algebra, wherein the rank of a matrix can depend on the number of linearly independent rows or columns in that matrix. Another notational scheme concerns the differentiability of mathematical functions. Terms “sufficiently differentiable” and “sufficiently smooth” are used interchangeably throughout the text to specify that derivatives of adequate order exist, enabling validity of mathematical formulae or definitions in a given context. Formally, the term “smooth” usually refers to a function of class C ∞ , while “sufficiently smooth” as used herein can be a weaker, i.e., less stringent, requirement. An additional point of clarification involves notation for the square root operation. Let x denote a scalar. Then the square root and its reciprocal are written in this book as x = x1/ 2 and −1 x = 1/ x = x −1/ 2 , respectively. Hence,
−1
x ≠ x −1 for any x. To avoid confusion, roots other than the sec
ond are written as exponents, i.e., as x1/ n ( n ≠ ±2 ) rather than as n x . In many cases, derivations of equations and relationships are written out in full, including algebraic and indicial manipulations that experienced readers may find routine. While such a presentation results in some rather lengthy equations, it is hoped that the derivations will provide insight, for the novice, into the final expressions so obtained and enable the reader to easily verify correctness of the results. An attempt is made to minimize use of the same symbol to represent quantities with different meanings; when such duplication is unavoidable, the meaning of a given symbol is clarified either explicitly or implicitly from the context in which it is used. Certain literary conventions are used throughout the text, and some of these should be clear to the reader already. References are labeled in (author year) format and are compiled alphabetically at the end of the book, rather than in footnotes or on a chapterbychapter basis. References to historical works published prior to year 1900 are omitted. Author’s names
1.3 Notation
9
of nonAnglican origin are written in standard English language, with special characters replaced in some cases by letters most similar in appearance. A subject index is provided at the end of the book, following the list of references.
2 Mathematical Foundations
Chapter 2 includes notation, definitions, and a number of identities that are applied subsequently in later Chapters of the text. Emphasized are differentialgeometric aspects of kinematics of finite deformations, linear connections and covariant differentiation, the deformation gradient of continuum mechanics, time derivatives and rate kinematics, theorems of Gauss and Stokes, and compatibility conditions. As will be clear in later Chapters, from the standpoint of crystals with defects, a geometric approach is advantageous for dealing with incompatible material configurations not globally homeomorphic to, i.e., configurations topologically inequivalent to, threedimensional Euclidean space (Eckart 1948; Kondo 1949, 1964; Bilby et al. 1955; Truesdell and Noll 1965; Noll 1967; Teodosiu 1967a, b). Detailed descriptions invoking formalisms of tensor algebra and tensor calculus on differential manifolds have been devoted elsewhere to elasticity theory (Marsden and Hughes 1983; Yavari et al. 2006) and general nonlinear continuum mechanics (Van der Giessen and Kollmann 1996; Stumpf and Hoppe 1997; Clayton et al. 2005; Epstein and Elzanowski 2007). In many instances, the differentialgeometric approach is favored over conventional Cartesian formulations for the former’s generality in terms of available choices of coordinates (e.g., curvilinear coordinates in the former versus rectangular coordinates in the latter) and representation of spaces with nonvanishing curvature (e.g., curved surfaces such as shells). Compact, coordinatefree (i.e., componentfree) representations are possible for many mathematical expressions and identities, and have become popular among many authors in recent literature. However, coordinatebased representations are frequently exercised in this text for clarity of presentation and for drawing comparisons with other treatments from historic and more recent literature. Hence, the index notation is used often in Chapter 2, especially in the context of geometric objects such as connections, torsion, curvature, and important properties and mathematical identities for these objects. Included in Chapter 2 is only that content deemed relevant and necessary for development of theories of material behavior in later Chapters. Comprehensive supplementary treatment of topics in differential geometry can be found in historical texts of Eisenhart (1926) and Schouten (1954),
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_2, © Springer Science+Business Media B.V. 2011
11
12
2 Mathematical Foundations
while more modern presentations can be found in monographs of Boothby (1975) and Kosinski (1993). Indepth descriptions of continuum mechanics in the setting of general curvilinear coordinates and finite deformations can be found in a number of texts, including those of Truesdell and Toupin (1960), Eringen (1962), Sedov (1966), Malvern (1969), Wang and Truesdell (1973), and Marsden and Hughes (1983).
2.1 Geometric Description of a Deformable Body Section 2.1 addresses the following topics: terminology of geometric spaces in the context of continuum mechanics; configurations of a body subjected to large deformations; manifolds and associated tangent and cotangent spaces; coordinate systems; basis vectors and their reciprocal vectors; and metric tensors. 2.1.1 Terminology The definitions given immediately below are free of notation and hence are somewhat qualitative. More precise mathematical formulae and supplementary figures follow in Section 2.1.2 and later in Section 2.2. A configuration denotes a timedependent realization of a body. A body is said to consist of a number of material particles, each encompassing a representative set of atoms or molecules pertinent to the scale of resolution afforded by the continuum description. A configuration may be actual or virtual (i.e., real or fictitious). In finite deformation continuum mechanics, the terms reference, initial, undeformed, or Lagrangian configuration most often refer to a description of the body at zero time, though broader definitions enabling multiple and evolving reference configurations are possible. Similarly, the current, spatial, deformed, or Eulerian configuration usually corresponds to the current instant of time. In the absence of discontinuities, reference and current configurations are holonomic to one another, implying that current coordinates of a material particle can be written as singlevalued functions of reference coordinates of that particle, and viceversa. In contrast, as will be demonstrated in Chapter 3, a virtual intermediate, relaxed, or unloaded configuration is often introduced, for example to describe crystals with distributions of defects or those undergoing large inelastic deformations. Such an intermediate configuration is anholonomic when its “coordinates” cannot be prescribed as singlevalued functions of reference or current coordinates of material particles. The term placement
2.1 Geometric Description of a Deformable Body
13
(Noll 1967; Maugin 1993) has also been used to refer to a configuration of a deformable body. A connection is a rank three construct that enables evaluation of the covariant derivative of vectors and tensors of higher rank. The covariant derivative operation defines the connection coefficients, also called Christoffel symbols of the connection in the context of Riemannian geometry. The content of this book only deals with linear connections, also called affine connections. Nonlinear connections can arise in more generalized spaces such as Finsler spaces (Rund 1959; Bejancu 1990) and are not addressed in this text. A metric tensor, or simply a metric, is a rank two covariant tensor that defines the scalar product of contravariant vectors, and consequently, the squared length of a vector. A metric tensor that is both symmetric and positive definite is called a Riemannian metric tensor1; nonRiemannian metrics are not considered explicitly in this text. Metric tensors perform other consequential functions, such as raising and lowering of vector and tensor indices and defining scalar products of higherorder tensors. A particular configuration can be assigned more than one connection, just as it can be assigned more than one metric tensor. The pair of {configuration, connection} or triplet of {configuration, connection, metric tensor} can often be classified as one or more of the following five types of geometric spaces: Euclidean, anholonomic, nonmetric, Cartan, and/or Riemannian. For a space to be classified as Euclidean or nonEuclidean, it must include a configuration, a metric tensor, and a connection. A Euclidean space satisfies three requirements: (i) the torsion tensor of the connection vanishes, (ii) the covariant derivative of the metric tensor vanishes, and (iii) the RiemannChristoffel curvature tensor constructed from the connection coefficients vanishes. A Euclidean nspace permits at each location a transformation from local, possibly curvilinear ndimensional coordinates to a global ndimensional Cartesian coordinate system. In continuum mechanics, both the reference and current configurations are typically viewed as threedimensional Euclidean spaces, with the motion acting as a diffeomorphism, i.e., a differentiable homeomorphism, or a differentiable onetoone, invertible mapping, between these two configurations (Stumpf and Hoppe 1997). Notice the distinction between Euclidean 1 A nonRiemannian metric tensor need not be positive definite. Such metrics can arise in more general geometric settings such as Finsler spaces, or for example Minkowski’s spacetime (Rund 1959; Synge 1960) wherein the determinant of the metric in 4space can be negative in sign. A nonsymmetric fundamental tensor was suggested in Einstein’s unified field theory (Einstein 1945; Schouten 1954).
14
2 Mathematical Foundations
and Cartesian: a general coordinate system in the former, for example spherical coordinates in three dimensions, admits a global transformation to a more specific kind of coordinate system in the latter, i.e., coordinate axes consisting of three constant orthonormal basis vectors. An anholonomic space is a configuration associated with a nonintegrable, twopoint deformation map. For example, in multiplicative elastoplasticity theory, since elastic and plastic deformation maps (i.e., tangent maps) taken individually are generally nonintegrable or anholonomic functions of current and reference coordinates, respectively, the corresponding intermediate configuration is generally anholonomic. Continuous coordinates on such an anholonomic space do not exist; rather, anholonomic coordinates can be regarded as discontinuous, multivalued functions of holonomic coordinates of the current or reference configuration. Anholonomicity is related to Cartan’s torsion tensor of a special connection constructed from the nonintegrable, twopoint deformation map. Anholonomic coordinates are analyzed at length by Schouten (1954), and to a lesser extent, by Ericksen (1960). Designation of a general space as metric or nonmetric requires that the configuration be assigned both a linear connection and a metric tensor; i.e., one must examine the triad of {configuration, connection, metric tensor}. In a nonmetric space, the covariant derivative of the metric tensor taken with respect to the connection is nonzero. On the other hand, in a metric space the covariant derivative of the metric tensor vanishes identically. A configuration with a connection admitting a nonvanishing torsion tensor is labeled a Cartan space, sometimes called a nonsymmetric space. Only the pair {configuration, connection} need be considered to enable labeling a space as Cartan or nonCartan. A space with vanishing torsion is called a symmetric space. For a space to be labeled as Riemannian or nonRiemannian, it must include the pair {configuration, connection}—a metric is not needed for such a designation as defined herein. A Riemannian space is defined here as a configuration with connection coefficients whose components yield a nonzero RiemannChristoffel curvature tensor2. A space with nonvanishing curvature is necessarily nonEuclidean. For example, a global twodimensional Cartesian coordinate system cannot be used to parameterize a shell unless the shell is flat. Conversely, a space with vanishing curvature is nonRiemannian and is said to be flat, and the connection in a nonRiemannian space is said to be integrable. 2 The mathematical field of study traditionally referred to as Riemannian geometry considers metric spaces with vanishing torsion, but in general nonvanishing curvature (Eisenhart 1926; Schouten 1954).
2.1 Geometric Description of a Deformable Body
15
Euclidean spaces by definition exclude the other four types of (nonEuclidean) spaces: anholonomic, nonmetric, Cartan, and Riemannian spaces. On the other hand, the four types of nonEuclidean spaces are not mutually exclusive. The above terminology is not always consistent in the literature (Schouten 1954; Bilby et al. 1955; Kondo 1964; Noll 1967; Marsden and Hughes 1983; Steinmann 1996; Clayton et al. 2005). However, definitions given here are deemed as those used either most frequently or most logically for describing kinematics of deformable crystalline solids, as will become clear later in Chapter 3. 2.1.2 Manifolds, Coordinates, and Metrics Denoted by χt (B ):B → Ε3 is a smooth, invertible, timedependent embedding of a material body B into threedimensional Euclidean space Ε3 . The configuration of body B at time t is denoted by Bt = χt (B ) , henceforth written simply as B for t > 0 . Initially, i.e., at t = 0 , material particles X ∈ B are said to occupy reference configuration B0 = χ 0 (B ) and are
assigned reference coordinates X A = χ 0A (X ) . Particles of material mapped to current configuration B are assigned spatial coordinates x a = χta (X ) . A description of the motion of all material particles is furnished by the continuous, invertible mapping ϕ = χt χ 0 −1: B0 → B . The operator denotes the composition, such that for two functions f and g, (f g )(X ) = f (g (X )) . The inverse obeys f f −1 = i , with i the identity operator. The local motion for a material particle identified by particular reference coordinates X A = χ 0Α (X ) is written ϕ X . Restricting the motion so that no two material particles occupy the same spatial location may limit the domain of ϕ ( X , t ) to open regions of the body, e.g., when two points at different referential locations of the boundary of a body may come into contact as a result of deformation. Mappings χ 0 , χt , and ϕ can be applied pointwise or globally and are not vector fields. For this reason, and since these mappings may operate without explicit introduction of coordinate basis vectors, boldface notation is not used to symbolically represent these functions. As indicated implicitly already and as will be made clear later, contravariant indices (i.e., indices in the upper position) are appended to such mappings as needed when coordinate systems are involved. A point in space occupied by the body in the reference configuration is denoted by X ∈ B0 , while a point in space occupied by the body in the
16
2 Mathematical Foundations
current configuration is denoted by x ∈ B . Functions depending on position in the reference configuration are denoted by f ( X ) , while functions depending on position in the current configuration are written f ( x) . No distinction is made here between functions depending on material particle, e.g., a material description f ( X ) (Malvern 1969), and those depending on the reference coordinates X A of that particle, e.g., a Lagrangian description f ( X) . Because the reference configuration is embedded in Euclidean space, a unique vector of coordinates X can always be assigned to each material particle at X. Similar arguments hold for the spatial description, since at any given time t, each location x can be assigned a unique vector of coordinates x. Thus the notation for a function of spatial position, f ( x) , is hereafter used interchangeably with f (x) . In indicial notation, timedependent components of the motion and its inverse, respectively, are expressed in functional form as (2.1) x a = x a ( X , t ) , X A = X A ( x, t ) . The first of (2.1) implies that spatial coordinates x a of each material particle depend upon the choice of point X, or equivalently the material particle located at that point in the reference configuration, and time t. The second of (2.1) assigns a set of reference coordinates X A to a material particle that occupies spatial location x at time t. Spatial coordinates x a of a material particle corresponding to location X will generally change with time as a result of motion, and spatial locations x occupied by the body at one instance of time may not coincide with those occupied at a different instance. The manifold concept, in the context of differential geometry, is now formally introduced (Boothby 1975). An nmanifold is a set M such that for each point P ∈ M there is a subset U of M containing P, and a onetoone mapping called a chart or coordinate system from U onto an open set in the ndimensional space of real numbers n . Multiple charts or coordinate systems may be introduced on (regions of) a given manifold. Transformations between different coordinate systems over (regions of) the manifold are assumed to be infinitely differentiable if the manifold is smooth; i.e., such changes in coordinates are of continuity class C ∞ for smooth manifolds. A collection of charts covering M is called an atlas. As will be discussed in Section 2.2.4, the chart of a smooth nmanifold can be embedded in ndimensional Euclidean space Ε n if and only if the curvature tensor of its corresponding LeviCivita connection vanishes.
2.1 Geometric Description of a Deformable Body
17
Fig. 2.1 Twodimensional manifold embedded in 3D Euclidean space
The tangent space of M at P is the ndimensional space of contravariant vectors emanating from P, written as TP M . The collection of base points P and tangent vectors at all P comprises the tangent bundle T M (i.e., the tangent bundle is the union of tangent spaces over all points P on M ), and the map π M from a tangent vector to its base point is called that vector’s projection. Inverse mappings π M−1 comprise sections of the tangent bundle. Similarly, the cotangent space of M at P, written as TP* M , is the ndimensional space of covariant vectors—also called covectors, oneforms, reciprocal vectors, or dual vectors—emanating from P. The cotangent bundle, denoted by T * M , is defined analogously to the tangent bundle, i.e., the cotangent bundle is the union of cotangent spaces over manifold M . Shown in Fig. 2.1 is a twodimensional manifold M with nonvanishing curvature embedded in Ε3 , with a point X described by a pair of coordinates X = ( X 1 , X 2 ) . Tangent space TX M is also shown. Each timedependent configuration of a deformable body can be regarded as a manifold, with locations of particles of material in that configuration identified in a onetoone manner with points X of B ; the latter itself can also be viewed as a manifold since charts of smooth coordinates (e.g., Xa) can, in principle, be introduced to cover B . Referential locations X and spatial locations x can be associated with base points on corresponding manifolds B0 and B, respectively. Tangent spaces to reference and current manifolds at points X and x are written TX B0 and Tx B , respectively. Body B , configurations B0 and B, and tangent spaces TX B0 and Tx B are illustrated in Fig. 2.2. Reference and current tangent bundles are
18
2 Mathematical Foundations
TB0 = ∪ X ∈B0 TX B0 and TB = ∪ x∈B Tx B , respectively. Analogously, cotangent spaces are written as TX* B0 and Tx* B , with T * B0 = ∪ X ∈B0 TX* B0 and
T * B = ∪ x∈B Tx* B the corresponding cotangent bundles in reference and current configurations, respectively.
Fig. 2.2 Configurations, mappings, and tangent spaces
Natural or holonomic basis vectors in reference and current configurations are defined, respectively, by ∂ ∂ GA = ∈ TX B0 , g a = a ∈ Tx B , (2.2) A ∂X ∂x and are tangent to local coordinate curves at X or x; for example, see Fig. 2.1 in which M can represent the reference configuration B0 . Sometimes the basis vectors in (2.2) are called covariant basis vectors because their indices occupy lower positions, though this can cause confusion because these vectors act as the basis for general contravariant vectors. Basis vectors in (2.2) are sometimes written as G A = ∂ A X = X, A and g a = ∂ a x = x,a . Dual or reciprocal bases to (2.2) are written as G A = dX A ∈ TX* B0 , g a = dx a ∈ Tx* B . (2.3) Basis vectors (2.2) and their duals (2.3) satisfy the orthonormality relations (2.4) G A ,G B = δ .BA , g a ,g b = δ .ba . B0
B
In (2.4), dual pairings (i.e., scalar product of vector and covector) in reference and spatial configurations correspond to the respective operations . , . B :TX* B0 × TX B0 → and . , . B :Tx* B × Tx B → . The dual basis 0
vectors are sometimes called contravariant basis vectors because their indices occupy upper positions. Also introduced in (2.4), Kronecker delta symbols satisfy
2.1 Geometric Description of a Deformable Body
19
⎧1 ∀ A = B, a ⎧1 ∀ a = b, (2.5) δ .b = ⎨ ⎩0 ∀ A ≠ B , ⎩0 ∀ a ≠ b. Location of the placeholder (index) denoted by the period is arbitrary in the special symbols defined in (2.5), but such placeholders are not always arbitrary for general tensorvalued quantities defined later in this book. Henceforward, subscripts on scalar product operations as in (2.4) denoting configuration(s) of arguments in angled brackets are omitted since the appropriate configuration(s) can always be inferred from the arguments. Summation over repeated indices produces δ . AA = δ .aa = δ .11 + δ .22 + δ .33 = 3 . From (2.2)(2.4), TX B0 is the linear vector space of all contravariant
δ .BA = ⎨
vectors V = V AG A emanating from point X ∈ B0 . Cotangent space TX* B0 is the linear vector space of all oneforms α = α AG A emanating from point X ∈ B0 . In the context of dual products, vectors and oneforms are linear functions, V: TX* B0 →
and α : TX B0 →
, and correspondingly
α, V = α ( V ) = α AV = V α A = V ( α ) = V , α , (2.6) invoking the symmetry property of the scalar product operation. Similar arguments hold for vectors and oneforms on respective tangent and cotangent spaces referred to current configuration B. Contravariant component V A of vector V can be obtained via the scalar product operation as V , G A = V B G B , G A = V Bδ .BA = V A , where (2.4) has been used. A
A
be a symmetric, positive definite biLet G:(V ∈ TX B0 , W ∈ TX B0 ) → linear form assigning a real number to any two vectors V and W in TX B0 . Object G is called a metric tensor, or simply a metric. Since G is symmetric, its components obey GAB = G( AB ) , where indices in parentheses are symmetric: 2 A( AB ) = AAB + ABA for arbitrary secondorder tensor A. Metric G maps a contravariant vector V into its associated covariant vector V# :
V# = GV = ( GAB G A ⊗ G B )(V B G B ) = VAG A , VA = GABV B .
(2.7)
The outer product (also called tensor product) of vectors and/or covectors, corresponding to a juxtaposition of indices, is denoted by ⊗ and satisfies the identity (G A ⊗ G B )G C = G A G B , G C . The inverse of the metric tensor G −1 , or simply the inverse metric, maps covectors α into associated vectors α # : α# = G −1α = ( G AB G A ⊗ G B )(α B G B ) = α AG A , α A = G ABα B . (2.8)
20
2 Mathematical Foundations
The standard notational convention of denoting components of G −1 with G AB (i.e., (G −1 ) AB = G AB ) is followed henceforth. On vector space TX B0 , metric tensor G enables evaluation of the inner product or dot product of vectors: V i W = V ,GW = V AGABW B . (2.9) Covariant component VA of vector V can be obtained via use of the dot product operation as follows: V iG A = V B G B iG A = V B GBA = VA . Similarly to (2.9), the inverse of the metric tensor, i.e., its contravariant form, enables evaluation of the inner product or dot product of covectors: α iβ = α ,G −1β = α AG AB β B . (2.10) In the current configuration B, the metric tensor associated with spatial coordinates x is denoted by g : ( v ∈ Tx B, w ∈ Tx B) → , with inverse g −1 . Equations analogous to (2.7)(2.10) apply for spatial metric g and its inverse in the current configuration. From (2.4), (2.9), and (2.10), it is implied that matrix components of metric tensors and their inverses in reference and current configurations are given, respectively, by G AB = G A iG B , G AB = G A iG B ; (2.11)
g ab = g a ig b , g ab = g a ig b . (2.12) Metrics and their inverses are related, by definition, as follows: (2.13) G AB GBC = δ .CA , g ab gbc = δ .ac . Relationships between basis vectors and their reciprocal vectors are G A = G AB G B , G A = GAB G B , g a = g ab g b , g a = g ab g b . (2.14) In addition to their role in scalar product operations, metric tensors (or their inverses) may be used to lower (or raise) indices of tensors of arbitrarily higher order. For example, let A = A AB G A ⊗ G B be a generic contravariant tensor of order two. The fully covariant representation of A is A # = GAC GBD ACD G A ⊗ G B = AAB G A ⊗ G B . (2.15) When considering multiple configurations, it often becomes necessary to express components of vectors or tensors introduced in one configuration, with one set of coordinates, with respect to bases in another configuration with a different set of coordinates. For example, a vector V defined in a parallel manner on TX B0 and Tx B is written (Eringen 1962) V = V AG A ( X ) = V a g a ( x) . (2.16) Taking the inner product with dual basis vectors in each configuration, it follows that
2.1 Geometric Description of a Deformable Body
21
V B = V A G A , G B = V a g a , G B = V a g.Ba , g a = g a. AG A ;
(2.17)
V b = V a g a , g b = V A G A , gb = V A g.bA , G A = g .Aa g a ;
(2.18)
where mixedvariant components of shifters, examples of twopoint tensors, are defined as g.Aa ( x, X ) = G A , g a = g a. A , g.aA ( x, X ) = g a , G A = g .Aa . (2.19) Similarly, fully covariant and fully contravariant components of shifter tensors are, respectively, g Aa ( x, X ) = G A ig a = g aA , g Aa ( x, X ) = G A ig a = g aA . (2.20) From (2.14), it follows that components of the shifters are raised and lowered by components of metric tensors of the corresponding configuration: g Aa = g ab g.bA = GAB g.Ba = g ab GAB g Bb . (2.21) Moreover, summation over one set of indices leads to the identities g.Ab g.aA = δ .ba , g.Aa g.aB = δ . BA . (2.22) It follows that det( g.Aa ) = 1/ det( g.aA ) = det( g ab ) / det(GAB ) , where det is the usual determinant of a secondorder tensor. Shifters can also be used to express components of vectors and tensors introduced in one frame of coordinates with respect to a different coordinate frame in the same configuration via parallel transport (Toupin 1956; Ericksen 1960). Differentiation indices cannot usually be shifted; e.g., generally ∂ a ≠ g.Aa ∂ A . Components of metric tensors on Euclidean spaces can be defined equivalently in terms of transformations to Cartesian coordinates and the dot product of vectors. For example, let X A denote general curvilinear coordinates on B0 , and let Z A = Z A (X ) denote Cartesian coordinates on B0 . Since tangent vectors to Z A are orthonormal by definition, ∂ ∂ ∂Z C ∂Z D ⎛ ∂ ∂ ⎞ ∂Z C ∂Z D i i δ CD , (2.23) = ⎜ ⎟= ∂X A ∂X B ∂X A ∂X B ⎝ ∂Z C ∂Z D ⎠ ∂X A ∂X B with δ CD covariant Kronecker delta symbols. From (2.23), the determinant of the matrix of metric tensor components is always nonnegative: det(GAB ) = [det(∂Z A / ∂X B )]2 ≥ 0 . Similarly for the inverse metric tensor, GAB =
det(G AB ) = 1/ det(GAB ) = [det(∂X A / ∂Z B )]2 ≥ 0 . The metric tensor (or its inverse) may have zero determinant along certain singular points or curves (e.g., at R = 0 in cylindrical or spherical coordinates) but is nonsingular over any volume (Malvern 1969). In Cartesian space, the metric is simply GAB = δ AB , and distinction between covariant and contravariant indices is not necessary. Analogously for a shifter, components can be computed via
22
2 Mathematical Foundations
∂ ∂ ∂Z B ∂z b ⎛ ∂ ∂ ⎞ ∂Z B ∂z b (2.24) i i δ Bb , = ⎜ ⎟= ∂X A ∂x a ∂X A ∂x a ⎝ ∂Ζ B ∂z b ⎠ ∂X A ∂x a where x a and z a = z a (x ) denote curvilinear and Cartesian coordinates, respectively, in spatial configuration B , and δ Bb reduces to Kronecker’s g Aa =
delta when coincident Cartesian coordinate frames for Z A and z a are prescribed, respectively, in reference and current configurations. Generally nonvanishing components of metric tensors for several common threedimensional coordinate systems are listed in Table 2.1. Metric tensor components listed in Table 2.1 can be applied towards representations in either of the reference or current configurations. Table 2.1 Metric tensors for common threedimensional coordinate systems Coordinate system
Nonvanishing components of G AB
Cartesian: ( X 1 , X 2 , X 3 ) → ( X , Y , Z )
GXX = GYY = GZZ = 1
Cylindrical: ( X , X , X ) → ( R,θ , Z ) X = R cosθ , Y = R sin θ , Z = Z R ≥ 0, θ ∈ (−π , π ]
GRR = GZZ = 1 , Gθθ = R 2
Spherical: ( X 1 , X 2 , X 3 ) → ( R,θ ,ϕ ) X = R sin θ cos ϕ , Y = R sinθ sin ϕ , Z = R cosθ R ≥ 0, θ ∈ [0, π ], ϕ ∈ (−π , π ]
GRR = 1 , Gθθ = R 2 , Gϕϕ = R 2 sin 2 θ
1
2
3
2.2 Linear Connections The following topics are addressed in Section 2.2: the definition of a generic linear connection, its covariant derivative, and connection coefficients; torsion and curvature of a connection; identities from differential geometry describing properties of the connection and its torsion and curvature; and a special kind of connection called the LeviCivita connection. 2.2.1 The Covariant Derivative and Connection Coefficients
A linear connection, also often called an affine connection, on a manifold B0 induces an operation ∇ that assigns to two vector fields V , W ∈ TB0 a third vector field ∇ V W ∈ TB0 , called the covariant derivative of W along V, such that
2.2 Linear Connections
23
(i) ∇ V W is linear in both V and W; (ii) ∇ fV W = f ∇ V W for scalar function f ;
(2.25)
(iii) ∇ V ( f W ) = f ∇ V W + V , Df W.
The derivative of f is Df, and in coordinates the derivative of f in the direction of V is V , Df = V A f , A = V A ∂ A f = V A∂f / ∂X A . The covariant derivative of W along V is written in indicial notation as .. A B .. A B ∇ V W = (V B ∂ BW A + Γ BC V W C )G A = (V BW.,AB + Γ BC V W C )G A , (2.26) where the notation ( . ) , B = ∂ B ( . ) = ∂( . ) / ∂X B is used interchangeably throughout this text for partial coordinate differentiation. The n3 coeffi.. A . Conneccients of the connection in ndimensional space are written Γ BC tion coefficients do not follow conventional coordinate transformation laws for thirdorder tensors. Consider a coordinate transformation X A → X A . Since vector field ∇ V W of (2.26) transforms conventionally under a change of basis as (Schouten 1954) ∂W A A .. A B V WC ( ∇V W ) = V B B + Γ BC ∂X B C ∂ X B ∂ ⎛ C ∂X A ⎞ .. A B ∂X C ∂X =V B + W V W Γ ⎟ BC B ⎜ ∂X B ∂X ⎝ ∂X B ∂X C ⎠ ∂X C B ⎛ C ∂X A ⎞ ∂X C B C .. A ∂X + Γ BC V W ⎜W B C ⎟ ∂X ∂X C ∂X ⎠ ⎝
=V B
∂ ∂X B
=V B
∂W C ∂X A ⎛ .. A ∂X B ∂X C ∂ ∂X A ⎞ B C Γ + + ⎜ ⎟V W BC ∂X B ∂X C ⎝ ∂X B ∂X C ∂X B ∂X C ⎠
=
(2.27)
∂X A B ∂W A ∂X A ⎛ .. D ∂X A ∂X B ∂X C + V ⎜ Γ BC ∂X D ∂X B ∂X C ∂X B ∂X A ⎜⎝ ∂X A +
∂X A ∂ ∂X C ∂X C ∂X B ∂X C
⎞ B C ⎟⎟V W ⎠
⎞ ∂X A ∂X A ⎛ B ∂W A C .. A B + Γ (∇V W ) A , V V W ⎜ ⎟⎟ = BC A ∂X B ∂X A ⎜⎝ ∂ X ⎠ transformation formulae for the connection coefficients are deduced as =
24
2 Mathematical Foundations
∂X B ∂X C ∂X A ..A ∂X A ∂ ∂X C Γ BC + C A ∂X ∂X B ∂X C ∂X B ∂X C ∂X (2.28) ∂X B ∂X C ⎛ ∂X A ..A ∂ ∂X A ⎞ = Γ BC − B ⎜ ⎟, A ∂X ∂X C ⎟⎠ ∂X B ∂X C ⎜⎝ ∂X with the second equality in (2.28) following readily from the identity (∂ C X A ∂ C X C ),B = (δ .CA ) ,B = 0 . Furthermore, the covariant derivative of a A = Γ BC
vector field, ∇W ( X ) , is a
{ } tensor field, expressed in components as 1 1
.. A ∇W ( X ) = (∂ BW A + Γ BC W C )G A ⊗ G B
(2.29)
.. A = (W.,AB + Γ BC W C )G A ⊗ G B .
An affine connection on tangent bundle TB0 enables parallel transport of vectors across different tangent spaces in TB0 . A vector is said to undergo parallel transport with respect to a connection with covariant derivative ∇ along paths for which its covariant derivative vanishes. For example, a vector W is considered to be parallel along a curve λ (t ) if ∇ V W = 0 , where V = ∂λ / ∂t is tangent to the curve parameterized by t. A vector W is then parallel transported along λ if it is extended to a parallel vector field W (t ) for all values of t. The covariant derivative is applied to covector fields and to tensor fields of higher order as follows (Schouten 1954): ∇ N A A... F G... M = A A... F G... M , N .. A RB... F .. F A... ER + Γ NR A G ... M + ... + Γ NR A G ... M
(2.30)
− Γ A RH ...M − ... − Γ A G... LR , where the index of covariant differentiation is a subscript immediately following the ∇ operator. Notice that the first covariant index of the connection coefficients corresponds to that of the differentiation. The covariant derivative of an absolute or true scalar function is defined in the same way as its ordinary partial derivative: ∇ N A = ∂ N A = A, N . Hence the covariant derivative of a constant scalar vanishes identically. Another useful .. A C ..C A .. A .. A identity is ∇ N δ .BA = δ .BA, N + Γ NC δ . B − Γ NB δ .C = δ . BA, N + Γ NB − Γ NB = δ . BA, N = 0 . From the linearity property of the connection, the covariant derivative of a sum of objects is equal to the sum of the covariant derivatives of these objects. Covariant differentiation obeys the product rule of Leibniz; e.g., ∇C (V AW B ) = V A∇CW B + W B ∇ CV A . Analogous to terminology for parallel .. R NG
A... F
.. R NM
A... F
2.2 Linear Connections
25
transport of vectors, a tensor is said to be parallel transported along a curve if its covariant derivative vanishes as the tensor is dragged along the curve. 2.2.2 Torsion and Curvature
The torsion tensor T of a connection is defined by the operation 2T ( V , W ) = ∇ V W − ∇ W V − [ V , W ] ,
(2.31)
where the Lie bracket of vector fields V and W on TB0 is
[ V, W ] = (V BW.,AB − W BV.,AB ) G A .
From (2.26), (2.31), and (2.32), the torsion tensor is A B C T = Γ [..BC ]G ⊗ G ⊗ G A ,
(2.32) (2.33)
where pairs of indices in square brackets are antisymmetric, e.g., for a secondrank tensor 2 Α[ AB] = AAB − ABA . A connection is torsionfree when its torsion tensor vanishes, or equivalently, when its connection coefficients are symmetric in covariant indices. The torsion tensor of a linear connection on a manifold is often called Cartan’s torsion, by association with geometer E. Cartan (Cartan 1922). A connection with vanishing torsion is said to be symmetric. Sometimes twice the quantity in (2.31) and (2.33) is used as the definition of the torsion (Marsden and Hughes 1983; Clayton et al. 2004a, b, 2005, 2006, 2008). One may verify that the torsion transforms like a true tensor of order { 12 } under a change of holonomic coordinate basis, by direct substitution of (2.33) into (2.28). The RiemannChristoffel curvature tensor associated with a linear connection with covariant derivative ∇ , R: TX* B0 × TX B0 × TX B0 × TX B0 → , is a
{ } tensor with component representation 1 3
... A .. A .. A .. A .. E .. A .. E RBCD = Γ CD , B − Γ BD ,C + Γ BE Γ CD − Γ CE Γ BD
= 2∂ [ B Γ C.. A]D + 2Γ [..BAE Γ C.. E] D ,
(2.34)
where indices in vertical bars are excluded from the antisymmetry operation. Order and placement of indices used in the definition of R vary among authors (Schouten 1954; Fosdick 1966; Marsden and Hughes 1983; Clayton et al. 2005); conventions adopted in this book for the RiemannChristoffel curvature tensor and quantities derived from it follow those of Schouten (1954) and Minagawa (1979). The RiemannChristoffel curvature tensor transforms like a true tensor of order {13 } under a change of holonomic coordinates (Schouten 1954). From definition (2.34), R is al
26
2 Mathematical Foundations
ways antisymmetric in the first two covariant indices. Definitions, in indicial components, of several quantities constructed from the RiemannChristoffel curvature tensor include its fully covariant version ... E RBCDA = RBCD GEA , (2.35) called simply the curvature tensor by Eringen (1962) and the Riemann tensor by Fosdick (1966), though again the placement of indices varies among authors. Components of the Ricci curvature are ... A . (2.36) RCD = RACD Recalling that n is the dimensionality of the space, scalar curvature κ is defined as 1 1 κ= RAB G AB = R, (2.37) n(n − 1) n(n − 1) with R the trace of the Ricci curvature. For n = 2 , R of (2.37) is equivalent to the Gaussian curvature. Finally, Einstein’s tensor θ has components (2.38) 4θ AB = ε ACDε BEF RCDEF , where components of the permutation tensor ε ACD are introduced formally later in (2.64). The skew second covariant derivatives of a contravariant vector V and covariant vector α can be expressed as (Schouten 1954) 1 ... A D .. D ∇[ B ∇ C ]V A = RBCD V − TBC ∇ DV A , (2.39) 2 1 ... A .. A ∇[ B ∇C ]α D = − RBCD α A − TBC ∇ Aα D . (2.40) 2 Skew differential operator ∇[ B ∇ C ] obeys the product rule of Leibniz, e.g.,
∇[ B ∇ C ] (V Aα D ) = α D ∇[ B ∇ C ]V A + V A∇[ B ∇ C ]α D .
(2.41)
2.2.3 Identities for the Connection Coefficients and Curvature
Coefficients of an arbitrary linear connection can be written in the form (Schouten 1954) 1 .. A .. A A.. .. A Γ BC = { ..BCA } + TBC − TC. A. B. + T. BC + ( M BC + M C. A. B. − M .ABC.. ) , (2.42) 2 where for a symmetric, three times differentiable, and invertible but otherwise arbitrary secondrank tensor with components GAB and inverse components G AB , the quantities
2.2 Linear Connections
{ } = 12 G .. A BC
AD
(GCD , B + GBD ,C − GBC , D )
27
(2.43)
are called Christoffel symbols3 of the tensor GAB . Christoffel symbols in (2.43) are symmetric in covariant indices. Also in (2.42), the thirdorder object .. A M BC = G AD M BCD = −G AD ∇ B GCD = GCD ∇ B G AD , (2.44) with the final equality following from identity ∇ B (GCD G AD ) = ∇ Bδ .CA = 0 . The covariant derivative of GAB is, from (2.30) and coefficients in (2.42), .. D .. D ∇ AGBC = GBC , A − Γ AB GDC − Γ AC GBD = − M ABC .
(2.45)
Symmetry conditions M ABC = M A( BC ) follow immediately from conditions
GAB = GBA . When ∇ AGBC = 0 , or equivalently when M ABC = 0 , the connection is said to be metric with respect to GAB . In that case, covariant differentiation via ∇ and raising (or lowering) of indices via G AB (or GAB ) or commute. In general, GAB of (2.43)(2.45) need not be the metric tensor used to define scalar products of vectors. However, when the connection of (2.42) is metric, and when GAB is in fact the metric tensor of the space with connection (2.42), then GAB is called the fundamental tensor of the space (Schouten 1954). In the particular case of Riemannian geometry, .. A = 0 ) and by definition the connection is simultaneously symmetric ( ΤBC .. A metric ( M BC = 0 ), leading to
.. A Γ BC = { ..BCA } (Riemannian geometry).
(2.46)
Returning now to the general case in (2.42) with possibly nonvanishing torsion and nonmetric connection, the RiemannChristoffel curvature tensor of (2.34) exhibits the following properties (Schouten 1954): R(...BCA ) D = 0 , (2.47) A .. A .. E .. A R[...BCD ] = 2∇[ BTCD ] − 4T[ BC TD ] E ,
(2.48)
..E RAB ( CD ) = ∇[ A M B ]CD + TAB M ECD ,
(2.49)
∇[ E R
... A BC ] D
= 2T R .. F [ EB
... A C ] FD
,
where antisymmetry over three indices is expressed as 6 A[ ABC ] = AABC + ABCA + ACAB − ABAC − ACBA − AACB . 3
⎣⎡ BC ,A⎦⎤
= GAD
(2.51)
{ } are often labeled Christoffel symbols of the second { } are often labeled Christoffel symbols of the first kind. ..A BC
In tensor analysis,
kind, and
(2.50)
..D BC
28
2 Mathematical Foundations
Relation (2.50) is often called Bianchi’s identity. For a symmetric connection the right sides of (2.48) and (2.50) vanish, and for a metric connection the right side of (2.49) vanishes. For a Riemannian connection of the type (2.46) that is both symmetric and metric, R( BC ) DA = 0 , R[ BCD ] A = 0 , RBC ( DA) = 0 , RBCDA = RDABC , (2.52) and the number of independent components of R is n 2 (n 2 − 1) /12 , for example one independent component for a twodimensional space and six independent components for a threedimensional space. In Riemannian geometry, the Ricci tensor of (2.36) and Einstein’s tensor of (2.38) are both symmetric and satisfy 1 1 ⎛ ⎞ θ AB = RAB − RGAB , ∇ Aθ.BA = ∇ A ⎜ RCB G AC − Rδ. BA ⎟ = 0 . (2.53) 2 2 ⎝ ⎠ A space with connection for which the covariant derivative of the Ricci tensor of (2.36) vanishes, i.e., for which ∇ A RCD = 0 , is called a Ricci space. A space in Riemannian geometry—that is a symmetric space with connection and metric in which (2.46) applies—in which the Ricci curvature and metric differ only by a scalar factor as 1 RCD = RGCD = (n − 1)κ GCD (2.54) n is called an Einstein space. From vanishing of the right side of Bianchi’s identity (2.50) for a symmetric space, it follows that the scalar curvature of an Einstein space is constant, i.e., ∇ Aκ = 0 (Schouten 1954). 2.2.4 The LeviCivita Connection
For a smooth manifold B0 with metric tensor G = (G A iG B )G A ⊗ G B , there is a unique affine connection with the covariant derivative operator G
G
G
∇ on B0 that is torsionfree ( T = 0 ) and metric ( ∇ G = 0 ), i.e., for which parallel transport preserves the dot products of vectors. It is called the LeviCivita connection (Marsden and Hughes 1983). The LeviCivita connection is a particular example of (2.46) and hence is often called the Riemannian connection (Hou and Hou 1997). In this book the term LeviCivita connection is reserved for the particular Riemannian connection G
whose curvature tensor vanishes as discussed below. Coefficients of ∇ are defined as G G 1 Γ ..BCA = G AD (GBD ,C + GCD , B − GBC , D ) = Γ ..CBA . (2.55) 2
2.2 Linear Connections
29
Superscript G (or G) of the LeviCivita connection and its corresponding covariant derivative or gradient operator is not subject to the summation convention. The RiemannChristoffel curvature tensor formed by inserting Christoffel symbols of LeviCivita connection (2.55) into definition (2.34) G
is denoted by R . This curvature tensor can be expressed completely in terms of metric G and its first and second partial derivatives with respect G
to coordinates X A . A space B0 with metric G and having R = 0 is called G
flat. One may show (Schouten 1954) that R = 0 if and only if one may assign parallel orthonormal coordinate basis vectors at each point X ∈ B0 such that GAB → δ AB . Thus, the curvature tensor vanishes identically and G
the space is flat when B0 is Euclidean. In fact, R = 0 are compatibility G
conditions for the existence of connection coefficients Γ ..BCA derived from a Euclidean metric tensor G via (2.55) (Schouten 1954; Ciarlet 1998). Henceforward in this book, space B0 with metric G and associated conG
nection (2.55) is always assumed Euclidean, meaning that R = 0 by definiG
tion. Thus, the notation Γ
.. A BC
is used to denote components of
{ } ..A BC
of
(2.46) when GAB = G A iG B and when the Riemann Christoffel curvature tensor formed from
{ } ..A BC
vanishes. On the other hand, on a curved sur
face—for example a twodimensional shell parameterized by a pair of coordinates X A : M → 2 embedded in Ε3 such as shown in Fig. 2.1—the single independent component of the curvature from { ..A BC } does not vanish. In terms of LeviCivita connection (2.55), partial coordinate derivatives of natural basis vectors and dual basis vectors are G
G A, B = − Γ
.. A BC
G
G C , G A, B = Γ
..C BA
GC = G B, A ,
(2.56)
and partial derivatives of components of the metric tensor are G
G
GAB ,C = (G A iG B ),C = Γ ..CBD GAD + Γ ..CAD GBD . (2.57) Viewed another way, (2.56) and (2.57) imply that the basis vectors, dual basis vectors, and metric tensor are all parallel (i.e., have vanishing covariant derivatives) with respect to the LeviCivita connection. Since the curvature and torsion of the connection (2.55) vanish by definition, (2.39) imG
G
plies that skew second covariant derivatives vanish, i.e., ∇[ B ∇ C ] V A = 0
30
2 Mathematical Foundations
for a vector field with components V A ( X ) . From the second of (2.56), G
G [ A, B] = 0 . However, in general ∂[ B ∇ C ]V A ≠ 0 , meaning that partial and covariant differentiation do not always commute. From the first of (2.4) and the second of (2.56), referential Christoffel symbols of (2.55) can also G
be computed as Γ
..C BA
G
=Γ
G
δ =Γ
.. D C BA . D
.. D BA
G D , G C = G A, B , G C .
In the context of geometrically nonlinear continuum mechanics, (2.55)(2.57) may be formulated in spatial configuration B by replacing reference coordinates X A with current coordinates x a , replacing reference metric G with spatial metric g, and replacing reference configuration basis (co)vectors with current configuration basis (co)vectors. Christoffel symg
bols of the second kind for covariant derivative operator ∇ on B are g g 1 Γ ..bca = g ad ( g bd ,c + g cd ,b − g bc ,d ) = Γ ..bca , (2.58) 2 g
g
..a and the curvature tensor derived from Γ bc using (2.34) is denoted by R . Configuration B with connection (2.58) and metric g is always assumed a g
..a , g ab } constitutes a Euclidean Euclidean space. Since the set { B , Γ bc space, torsion and curvature tensors formed from (2.58) vanish identically. Analogs of (2.56) and (2.57) in the current configuration are g
g a,b = − Γ
..a bc
g
g c , g a ,b = Γ g
g ab ,c = (g a ig b ),c = Γ g
.. d cb
..c ba
g c = g b,a ; g
g ad + Γ
..d ca
gbd ;
(2.59)
(2.60)
g
and ∇[b ∇c ] V a = 0 for a spatial vector field with components V a ( x) . From the symmetry properties evident in (2.58), g[ a ,b] = 0 . From the second of (2.4) and the second of (2.59), spatial Christoffel symbols of (2.58) g
can also be computed as Γ
..c ba
g
=Γ
..d ba
g
δ .cd = Γ
..d ba
g d , g c = g a ,b , g c .
In terms of transformation formulae to Cartesian coordinates introduced in (2.23) and (2.24), coefficients in (2.55) and (2.58) satisfy G ∂ 2 Z D ∂X A g ..a ∂ 2 z d ∂x a Γ ..BCA = , Γ bc = b c d . (2.61) ∂X B ∂X C ∂Z D ∂x ∂x ∂z LeviCivita connection coefficients for cylindrical and spherical coordinate systems are listed in Table 2.2, where the superscript G has been dropped for brevity.
2.3 Notation, Differential Operators, and Other Identities
31
Since metric tensor components GAB = δ AB = constant in Cartesian coordinates, Christoffel symbols obtained from G AB all vanish by (2.55) in Cartesian coordinates. So long as basis vectors G A are spatially constant (but not necessarily orthogonal), Christoffel symbols formed from G
GAB = G A iG B vanish identically, and covariant differentiation via ∇ A and partial differentiation via ∂ A = ∂ / ∂X A are equivalent operations. Table 2.2 Connection coefficients for common coordinate systems Coordinate system
.. A Nonzero components of Γ BC
Cartesian: ( X , X , X ) → ( X , Y , Z )
None
Cylindrical: ( X , X , X ) → ( R,θ , Z ) X = R cosθ , Y = R sin θ , Z = Z
Γ R..θθ = Γ θ..θR = 1/ R , Γ θθ.. R = − R
Spherical: ( X 1 , X 2 , X 3 ) → ( R,θ ,ϕ ) X = R sin θ cos ϕ , Y = R sin θ sin ϕ , Z = R cosθ
Γ R..θθ = Γ θ..θR = Γ R..ϕϕ = Γ ϕ..ϕR = 1/ R ,
1
2
1
3
2
3
.. R Γ θθ.. R = − R , Γ ϕϕ = − R sin 2 θ ,
..θ Γ ϕϕ = − sin θ cosθ ,
Γ θϕ..ϕ = Γ ϕθ..ϕ = cot θ
2.3 Notation, Differential Operators, and Other Identities To avoid frequent writing of the gradient operator for covariant derivatives, the following compact notation is used henceforward for covariant differentiation with respect to associated LeviCivita connections with coefficients in (2.55) and (2.58): G
∇ N A( X ) A...H I ...M = A A...H I ...M ; N ,
(2.62)
g
∇ n B ( x) a...h i...m = B a...h i...m; n , (2.63) where A( X ) and B( x) are tensors of arbitrary order referred to reference and current coordinate systems, respectively. From (2.55)(2.60), it follows that G ;AB = 0 , G A; B = 0 , GAB ;C = 0 , g ;ab = 0 , g a ;b = 0 , and g ab;c = 0 . Contravariant and covariant components of third rank permutation tensors on configurations B0 and B , respectively, are defined by
ε ABC =
ε
abc
−1
Ge ABC , ε ABC = GeABC ;
= −1 ge
abc
, ε abc = geabc ;
(2.64) (2.65)
32
2 Mathematical Foundations
where henceforth the standard abbreviated notation G = det G = det(GAB ) and g = det g = det( g ab ) is used for determinants of metric tensors. Recall also the compact notation used in this text for reciprocals of square roots: −1 G = 1 / G and −1 g = 1 / g . Permutation symbols, also often called LeviCivita symbols, satisfy e
ABC
e
abc
= eABC
= eabc
⎧ 0 when any two indices are equal ⎪ = ⎨ +1 for ABC = 123, 231, 312 ⎪ − 1 for ABC = 132, 213, 321; ⎩ ⎧ 0 when any two indices are equal ⎪ =⎨ +1 for abc = 123, 231, 312 ⎪ − 1 for abc = 132, 213, 321. ⎩
(2.66)
(2.67)
Permutation tensors and symbols in (2.64)(2.67) are antisymmetric in all AB C A BC ABC ABC pairs and triplets of indices, e.g., ε ABC = ε [ ] = ε [ ] = ε [ ] = ε [ ] (refer to (2.51)). Covariant derivatives of permutation tensors in (2.64) and (2.65) with respect to LeviCivita connections vanish since G; A = 0 and g;a = 0 (Malvern 1969). However, in general, G, A ≠ 0 and g ,a ≠ 0 since G ( X ) and g ( x) are not invariant under general changes of coordinates and hence are not absolute scalars. Identities for symbols of (2.66) are tabulated in Table 2.3. Analogous identities apply for spatial symbols eabc and eabc of (2.67) and for the permutation tensors of (2.64) and (2.65). Table 2.3 Identities for permutation symbols Identity
e ABC eDEF
e ABC eABE
Identity
⎡δ .DA ⎢ = det ⎢δ .BD ⎢δ .CD ⎣ = 2δ .CE
δ .EA δ .FA ⎤ ⎥ δ .BE δ .BF ⎥ δ .CE δ .CF ⎥⎦
e ABC eADE = δ .BDδ .CE − δ .BE δ .CD e ABC eABC = 2δ. AA = 6
Several mathematical operations are now introduced in reference coordinates. Analogous definitions apply for spatial coordinates. The trace of a secondorder tensor A is defined as summation over its mixedvariant indices: trA = A.AA = A AB GAB = AAB G AB . (2.68) The transpose is identified as a horizontal switch of indices:
2.3 Notation, Differential Operators, and Other Identities
33
T AAB = ABA , ( AT ) AB = ABA . (2.69) The gradient of a scalar function f is equivalent to its partial or covariant derivative:
G
(2.70) ∇ f = f ; A G A = f , AG A . From (2.56) and (2.62), the gradient of a contravariant vector field V is G
∇ V = V, B ⊗ G B = (V AG A ), B ⊗ G B = (V.,AB G A + V AG A, B ) ⊗ G B G
= V.,AB G A ⊗ G B + V A Γ
..C BA
(2.71)
GC ⊗ G B
G
= (V.,AB + V C Γ ..BCA )G A ⊗ G B = V; BAG A ⊗ G B . The divergence of a contravariant vector field V satisfies G
G
∇, V = tr ∇ V = V, A , G A = (V G B ), A , G B
=V = G
A
−1
A ;A
(
GV
A
)
(2.72) .
,A
The final equality in (2.72) follows from the identity (Eringen 1962)
( ln G )
G
,A
=Γ
.. B AB
G
=Γ
.. B BA
.
(2.73)
The curl of a covariant vector field α satisfies G
∇× α = G A × (α B G B ), A = G A × G Bα B ; A = ε ABCα C ; B G A , (2.74) where the vector cross product of two contravariant or covariant vectors, respectively, is V × W = ε ABCV BW C G A , α × β = ε ABCα B βC G A . (2.75) Since the LeviCivita connection is symmetric, the covariant derivative in (2.74) can be replaced with a partial derivative: G
ε ABCα C ; B = ε ABCα C , B − ε ABC Γ
α A = ε ABCα C , B = ε ABC ∂ Bα C .
.. A [ BC ]
(2.76)
The Laplacian of a scalar function f is computed in general curvilinear coordinates as ∇ 2 f = ( G AB f , A ) ; B = G AB ( f, A ) ; B = −1 G G
(
GG AB f , A
)
,B
.
(2.77)
A number of other identities can be derived immediately from definitions in (2.68)(2.77). For example, G
G
∇, ∇× α = ε ABCα C ; BA = ε ABCα C ;( BA) = 0 ,
(2.78)
34
2 Mathematical Foundations G
G
∇× ∇ f = ε ABC f;CB G A = ε ABC f;( CB )G A = 0 .
(2.79)
Many others can be found in books on vector calculus, electromagnetism (Stratton 1941; Jackson 1999), or continuum mechanics (Malvern 1969). Two mathematical operations for second and higherorder tensors are defined next: the generalized dual product and the doubledot product. These operations will become particularly useful in Chapter 4 (and in subsequent Chapters) for defining energetic quantities in the context of the continuum thermodynamics of deformable bodies. The generalized dual product written for rank two tensors extends (2.4) to secondorder tensors, providing a scalar product of two such quantities. For example, A, B = A AB BBA {∀A ∈ TX B0 × TX B0 , B ∈ TX* B0 × TX* B0 } , (2.80) a, b = a ab bba C, D = C.aA D.aA
{∀a ∈ T B × T B, b ∈ T B × T B} , {∀C ∈ T B × T B , D ∈ T B × T B} . x
x
x
* X
* x
0
* x
X
* x
0
(2.81) (2.82)
In (2.82), C and D are examples of twopoint tensors. The doubledot product, denoted by boldface colon : , implies summation over two sets of adjacent indices of second and higherorder tensors. As with the generalized dual product, the doubledot product may be applied to quantities defined on the tangent and/or cotangent spaces of one or more configurations, i.e., twopoint tensors. For example, A : B = A AB BAB {∀A ∈ TX B0 × TX B0 , B ∈ TX* B0 × TX* B0 } , (2.83) a : b = a ab bab C : D = C aA DaA
{∀a ∈ T B × T B, b ∈ T B × T B} , {∀C ∈ T B × T B , D ∈ T B × T B } , x
x
x
X
* x
0
* x
* x
* x
0
(2.84) (2.85)
E : F = E abcd Fcd g a ⊗ g b {∀E ∈ Tx B × Tx B × Tx B × Tx B, F ∈ Tx* B × Tx* B} . (2.86) Notice from (2.86) that when tensors of rank greater than two are involved, the doubledot product operation does not yield a scalar as the result. In situations where there is no chance for confusion, e.g., scalar products of mixed contravariantcovariant pairs along the lines of (2.82), the dual product and doubledot product notations may be used interchangeably. In terms of the trace operation of (2.68), A, B = tr ( AB ) = tr ( AT BT ) , A : B = tr ( ABT ) = tr ( AT B ) . (2.87)
2.4 Physical Components
35
2.4 Physical Components Components of vectors and tensors expressed in general curvilinear coordinates generally do not all exhibit the same dimensional units. In general curvilinear systems, basis vectors need not be dimensionless. Physical components of these objects can be introduced so that all components exhibit the same dimensions, and so that all basis vectors are dimensionless and of unit length. Developments that follow in Section 2.4 are expressed with respect to the reference configuration; analogous expressions apply for spatial coordinates. Physical components are referred to dimensionless basis vectors E A obtained by normalizing basis vectors of a general curvilinear coordinate system by their lengths: GA EA = = G A −1 GAA , (2.88) (G A iG A )1/ 2 where underlined indices are not subject to the summation convention. An arbitrary vector V ∈ TX B0 can be written as V = V AG A = V A GAA E A = V
A
EA ,
where contravariant physical components of V are A V = V A GAA . Covariant components satisfy VA = G ABV B = G AB −1 GBB V
B
(2.89) (2.90)
.
(2.91)
Physical components of a tensor of higher order can be defined by considering the way the tensor represents phenomena in physics; however, transformation formulae for higherorder tensors from general curvilinear components to physical components often involve lengthy manipulations (Malvern 1969). Listed next are useful expressions for general orthogonal curvilinear coordinates, cylindrical coordinates, and spherical coordinates. Other kinds of curvilinear coordinate systems—elliptic, parabolic, bipolar, spheroidal, paraboloidal, and ellipsoidal—are addressed by Stratton (1941).
2.4.1 General Orthogonal Coordinates General orthogonal coordinates are defined by the requirement that at each point X, the coordinate curves X A passing through X are mutually orthogonal. This requirement results in a diagonal metric tensor
36
2 Mathematical Foundations
⎧ G ∀A = B, GAB = G A iG B = ⎨ AA ∀A ≠ B. ⎩0
(2.92)
Thus dXidX = dX AGAB dX B = G11 (dX 1 ) 2 + G22 ( dX 2 ) 2 + G33 ( dX 3 ) 2 , GAA = 1/ G
AA
,
−1
(2.93) (2.94)
(2.95) G = G11G22G33 , G = G G G . Nonvanishing Christoffel symbols are G G G G 1 Γ ..AAB = − GAA, B , Γ ..BAB = Γ ..ABB = (ln GBB ), A , Γ ..AAA = (ln G AA ), A , (2.96) 2GBB 11
22
33
and otherwise G
Γ
= 0 (A ≠ B ≠ C ) . (2.97) In contravariant physical components of orthogonal coordinates, the gradient and Laplacian of a scalar function f ( X ) and the divergence and curl of a vector field V ( X ) are, respectively (Eringen 1962) .. A BC
G
∇ f = −1 G11 f,1E1 + −1 G22 f,2 E2 + −1 G33 f,3E3 ,
(2.98)
G
∇ 2 f = −1 G ⎡⎣ (−1 G11 G22 G33 f,1 ),1 + ( G22 G33G11 f,2 ),2 + ( G33 −1
−1
G
∇, V = −1 G ⎡⎣( G22 G33V 1 ),1 + ( G33G11V G
2
G11G22 f,3 ),3 ⎤⎦ ,
),2 + ( G11G22 V 3 ),3 ⎤⎦ , (2.100)
3 ∇× V = −1 G22G33 ⎣⎡( G33V ),2 − ( G22 V
2
),3 ⎦⎤ E1
1 3 + −1 G33G11 ⎡⎣( G11V ),3 − ( G33V ),1 ⎤⎦ E 2
+ −1 G11G22 ⎡⎣( G22 V
2
(2.99)
(2.101)
1 ),1 − ( G11V ),2 ⎤⎦ E3 .
2.4.2 Cylindrical Coordinates
Cylindrical coordinates ( X 1 , X 2 , X 3 ) → ( R,θ , Z ) are a particular kind of orthogonal curvilinear coordinates. Transformation formulae to Cartesian coordinates and metric tensor components are listed in Table 2.1, and Christoffel symbols are listed in Table 2.2. In particular, a squared increment of distance is
2.4 Physical Components
37
dXi dX = dX AG AB dX B = GRR ( dR ) 2 + Gθθ (dθ ) 2 + GZZ (dZ ) 2
(2.102) = (dR ) 2 + R 2 (dθ ) 2 + (dZ ) 2 . In physical components of cylindrical coordinates, the gradient and Laplacian of a scalar f ( X ) and the divergence and curl of a vector field V ( X ) are, respectively, G
∇ f = f , R E R + R −1 f ,θ Eθ + f , Z E Z ,
(2.103)
∇ 2 f = f , RR + R −1 f, R + R −2 f,θθ + f , ZZ ,
(2.104)
G
G
∇, V = R −1 ( RVR ), R + R −1Vθ ,θ + VZ , Z ,
(2.105)
G
∇× V = ⎡⎣ R −1VZ ,θ − Vθ , Z ⎤⎦ E R + ⎡⎣VR , Z − VZ , R ⎤⎦ Eθ + R −1 ⎡⎣( RVθ ), R − VR ,θ ⎤⎦ E Z .
(2.106)
By convention, indices of physical components of a vector in cylindrical coordinates are written in the subscript position, with angled brackets on indices omitted: V 1 = V R = VR , V 2 = V θ = Vθ , and V 3 = V Z = VZ . 2.4.3 Spherical Coordinates
Spherical coordinates ( X 1 , X 2 , X 3 ) → ( R,θ ,ϕ ) are a second particular kind of orthogonal curvilinear coordinates. Transformation formulae to Cartesian coordinates and metric tensor components are listed in Table 2.1; Christoffel symbols are listed in Tables 2.2. In particular, a squared increment of distance is dXidX = dX AGAB dX B = GRR (dR ) 2 + Gθθ (dθ ) 2 + Gϕϕ (d ϕ ) 2 (2.107) = (dR )2 + R 2 (dθ ) 2 + R 2 sin 2θ (dϕ ) 2 . In physical components of spherical coordinates, the gradient and Laplacian of a scalar f ( X ) and the divergence and curl of a vector field V ( X ) are computed, respectively, as follows: G
∇ f = f , R E R + R −1 f,θ Eθ + ( R sin ϕ ) −1 f ,ϕ Eϕ ,
(2.108)
∇ 2 f = R −2 ( R 2 f , R ), R + ( R 2 sin θ ) −1 ( f ,θ sin θ ) ,θ + ( R sin θ ) −2 f ,ϕϕ ,
(2.109)
G
G
∇, V = R −2 ( R 2VR ), R + ( R sin θ ) −1 ⎡⎣(Vθ sin θ ),θ + Vϕ ,ϕ ⎤⎦ ,
(2.110)
38
2 Mathematical Foundations G
∇× V = ( R sin θ ) −1 ⎡⎣ (Vϕ sin θ ),θ − Vθ ,ϑ ⎤⎦ E R + R −1 ⎡⎣(sin θ ) −1VR ,ϕ − ( RVϕ ), R ⎤⎦ Eθ
(2.111)
+ R −1 ⎡⎣ ( RVθ ), R − VR ,θ ⎤⎦ Eϕ . By convention, indices of physical components of a vector in spherical coordinates are written in the subscript position, with angled brackets on indices omitted: V 1 = V R = VR , V 2 = V θ = Vθ , and V 3 = V ϕ = Vϕ .
2.5 The Deformation Gradient The deformation gradient is a fundamental descriptor of kinematics of deformable bodies, and is of particular importance in the context of nonlinear solid mechanics. In Section 2.5, the definition and interpretation of the deformation gradient are provided, followed by definitions and identities for key quantities derived from the deformation gradient. 2.5.1 Fundamentals
Recall from Section 2.1.2 that motion from the reference configuration to the current configuration of a deformable body is denoted by continuous, invertible, onetoone function ϕ = χt χ0 −1: B0 → B . The deformation gradient field is defined as the tangent of ϕ , mapping vectors in TB0 to vectors in TB , or locally at material point X, F( X ) = T ϕ X : TX B0 → Tx B . A visual interpretation is provided in Fig. 2.2. When coordinate systems x a and X a are introduced on B0 and B , respectively, such that x a = ϕ a ( X A , t ) , then deformation gradient F can be written as ∂ϕ a g a ⊗ G A ∈ Tx B × TX* B0 . (2.112) ∂X A In components, the deformation gradient is often written4 F. Aa ( X , t ) = x.,aA . F = F. Aa g a ⊗ G A =
At any particular time t, spatial coordinates x a occupied by the body are assumed onetoone functions of X A and (usually) differential of class C r ( r ≥ 1 ) with respect to X A . Also at any time t, reference locations occupied by the body with coordinates X A are assumed onetoone and of 4
Partial differentiation proceeds as ∂ A (⋅) = (⋅), A = (⋅), a ∂ A x a = (⋅), a x.,aA = ∂ a (⋅) F. Aa .
2.5 The Deformation Gradient
39
class C r with respect to spatial coordinates x a . Thus det( x.,aA ) ≠ 0 . If r = 0 across certain singular surfaces within an otherwise “smooth” body, then F may be discontinuous across such surfaces. Because it is referred to (possibly) distinct coordinate systems in different configurations, F is said to be a twopoint tensor or double tensor (Ericksen 1960) whose components each transform like those of a vector (upper index) or covector (lower index) under transformations of only one set of coordinates. The deformation gradient operates on an arbitrary vector V = V B G B ∈ TX B0 as FV = F. Aa g a ⊗ G A (V B G B )
= F. AaV B g a G A , G B = F. AaV A g a ∈ Tx B,
(2.113)
where the first of (2.4) has been used. From (2.113) it is clear why the deformation gradient is called a tangent map: F maps a reference vector V that is a linear combination of tangent basis vectors at a point X on the reference configuration to a spatial vector FV that is a linear combination of tangent basis vectors at a point x on the current configuration. The deformation gradient provides the firstorder approximation of the length and direction of a differential line element dx ∈ Tx B mapped to the current configuration from its referential representation dX ∈ TX B0 . For example, a Taylorlike series expansion can be written (Toupin 1964) dx a = x a ( X ′) − x a ( X ) 1 1 = x.,aA dX A + x:aAB dX A dX B + x:aABC dX A dX B dX C + ... , (2.114) X X X 2! 3! F. aA
F. aA:B
F. aA:BC
with dX = X ′ − X an infinitesimal vector between reference points X and X ′ . Section D.1 of Appendix D contains a complete tensor derivation of (2.114), to second order in dX. To first order in dX, dx = FdX , dx a = F. Aa dX A = x.,aA dX A . (2.115) In (2.114), the total covariant derivative of the deformation gradient, i.e., the secondorder position gradient, obeys (Eringen 1962; Toupin 1964) A
A
A
G
x:aAB = F. Aa:B = F. Aa , B − Γ =x
a ., AB
G
−Γ
g
F +Γ
a ..C BA .C
g
x +Γ
..C a BA .,C
..a bc
F. Ac F. Bb
(2.116)
b ..a c bc ., A ., B
x x .
The total covariant derivative of a generic twopoint or double tensor of arbitrary order, A( X , x) , is defined as (Ericksen 1960; Eringen 1962) ( ADA......CF
) = ( ADA......CF
a ...c d ... f :K
= ( ADA......CF
) + ( ADA......CF
a ...c d ... f ; K
a ...c d ... f ;k
) F.Kk = ( ADA......CF
a ...c d ... f :k
) F.Kk a ...c d ... f :k
) x.,kK .
(2.117)
40
2 Mathematical Foundations
Partial covariant derivatives of A are found by applying the usual rules of covariant differentiation in (2.30) to only one index. For example, G
A.aA; B = A.aA, B − Γ
..C BA
g
A.aC , A.aA;b = A.aA,b + Γ
..a bc
A.cA .
(2.118)
In (2.116), regarding x = x ( X ) leads to inclusion of only one secondorder partial derivative in the total covariant derivative of F (Eringen 1962; Toupin 1964), though in general F. Aa ,b = F. Aa , B F −1.Bb ≠ 0 . From the chain a ., A
a ., A
rule, F. Aa:B = F. Aa:b F.Bb and F. Aa:b = F. Aa:B F −1.Bb (Ericksen 1960). Thirdorder position gradient x:aABC can be computed by taking the total covariant derivative of F. Aa:B via another iteration of (2.117). Partial covariant derivatives of twopoint shifter tensors vanish: g.Aa;b = 0 , g.aA; B = 0 , g.aA;b = 0 , and g.Aa; B = 0 (Toupin 1956; Ericksen 1960). For example, g.Aa ;b = G A ig a ;b = 0 . Then from (2.117), total covariant derivatives of shifters must vanish: g.Aa:b = 0 , g.aA:B = 0 , g.aA:b = 0 , and g.Aa:B = 0 . Thus it follows that partial covariant differentiation and total covariant differentiation both commute with shifting, raising, and lowering of indices. The dual map F* of the twopoint tensor F is defined by F*α, V = α,FV ∀ α ∈ Tx* B,V ∈ TX B0 . (2.119) From the properties of the mapping ϕ , deformation gradient tensor F is nonsingular, and its inverse satisfies F −1F = 10 , X .,Aa x.,aB = δ .BA ; FF −1 = 1 , x.,aA X .,Ab = δ .ba ; (2.120) where 10 = δ .BA G A ⊗ G B and 1 = δ .ba g a ⊗ g b are identity tensors on B0 and
B . In components, the inverse F −1.Aa ( x, t ) = X .,Aa , and partial differentiation ∂ a (.) = ∂ A (.) F −1.Aa . The dual and inverse commute: F* −1 = F −1* = F −* . In components, the dual, inverse, and dualinverse of F are, respectively, F* = FA*.a G A ⊗ g a ∈ TX* B0 × Tx B , (2.121) F −1 = F −1 A.a G A ⊗ g a ∈ TX B0 × Tx* B ,
F
−*
=F
−* .A a
*
g ⊗ G A ∈ Tx B × TX B0 . a
(2.122) (2.123)
T
The transpose map F between metric vector spaces (TX B0 ,G ) and (Tx B,g) is defined by the operation (FT w )iV = w i(FV ) ∀ w ∈ Tx B,V ∈ TX B0 . (2.124) Upon inspection of (2.119) and (2.124), the relationship between the transpose and dual maps is apparent:
2.5 The Deformation Gradient
41
FT = G −1F* g . (2.125) Notice that the transpose map depends on the metric tensors of each configuration, while the dual map is defined independently of the metric in either configuration. In index notation, the dual map corresponds to a horizontal switch of indices, while the transpose corresponds to a diagonal switch. In coordinates, transpose and inversetranspose maps are written FT = G AB FB*.b gba G A ⊗ g a ∈ TX B0 × Tx* B , (2.126) F −T = g ab F −* b.B GBA g a ⊗ G A ∈ Tx B × TX* B0 . (2.127) Two specific kinds of coordinate representation of the motion (and hence the deformation gradient) are common: convected coordinate representations and Cartesian coordinate representations. For one kind of representation in convected coordinates, basis vectors of the spatial frame are updated with the motion in such a way that numerical values of the coordinates of a material particle in reference and spatial descriptions always coincide: x a ( X , t ) = δ .aA X A , F. Aa = δ .aA , F = g a (x,t ) ⊗ G A (X ) . (2.128) Alternatively, convected coordinates can be expressed in terms of spatial basis vectors fixed in time and updated reference basis vectors, again resulting in coincident numerical values of coordinates of a material particle: x a ( X , t ) = δ .aA X A , F. Aa = δ .aA , F = g a (x) ⊗ G A (X ,t ) . (2.129) Because basis vectors for spatial and reference coordinates, respectively, in (2.128) and (2.129) evolve with time, associated metric tensors will also change with time as the body deforms. Convected coordinates of types (2.128) and (2.129) will not be used henceforward in this book for describing the relationship between reference and spatial coordinates of a material particle. Definition (2.112)—which is applicable in general curvilinear coordinates—is used this book, but it is henceforth restricted to nondeforming, inertial coordinate systems on B0 and B , thus ruling out use of convected coordinates. Accordingly, natural basis vectors and metric tensors do not depend explicitly on time: in the reference configuration G A = G A (X ) , G A = G A (X ) , and hence GAB = GAB (X ) . Likewise in the
current configuration, g a = g a (x) , g a = g a (x) , and g ab = g ab (x) . Thus in the remainder of this book, holonomic basis vectors can change with position (X or x) as is the case for curvilinear coordinates, but the origin of each coordinate system for X A and x a remains fixed in both time and space. The presentation of kinematics of deformable bodies simplifies considerably in Cartesian coordinates, also often called rectangular coordinates, rectilinear coordinates, or flat coordinates. If coincident Cartesian coordi
42
2 Mathematical Foundations
nate axes5 are specified with e A = G A = δ .aA g a , e A = G A = δ .aAg a , GAB = δ AB ,
g ab = δ ab , g .Aa = δ .Aa , and g.aA = δ .aA , then (2.112) becomes, quite simply, F = F.BA e A ⊗ e B . (2.130) Occasionally Cartesian representation (2.130) is used in this book, again assuming that the orientation of each basis vector remains fixed in time. Restriction of validity of a corresponding expression to Cartesian coordinates will be stated explicitly. In (2.130), notice F.BA = δ .aA x.,aB ≠ X .,AB = δ .BA . Pushforward and pullback operations are now defined. The push forward of a scalar f : B0 → is defined by ϕ* f = f ϕ −1 . The pullback of
a scalar h : B →
is defined by ϕ * h = h ϕ . The pushforward ϕ* V of a
vector V ∈ TX B0 , the pullback ϕ* w of a vector w ∈ Tx B , the pushforward ϕ* α of a covector α ∈ TX* B0 , and the pullback ϕ* β of a covector β ∈ Tx* B are defined by
ϕ* V = Tϕ X ( V ) ϕ −1 = FV ϕ −1 ∈ Tx B ,
ϕ * w = (T ϕ X )
( w ) ϕ = F −1w ϕ ∈ TX B0 , −* ϕ* α = (T ϕ X ) ( α ) ϕ −1 = F −* α ϕ −1 ∈ Tx* B , * ϕ* β = (T ϕ X ) ( β ) ϕ = F* β ϕ ∈ TX* B0 . −1
(2.131) (2.132) (2.133)
(2.134) By extension, the pushforward to the current configuration of arbitrary tensor A of rank { MN } referred to the reference configuration is defined as
ϕ* A ( w1 ,...w M ,β1 ,...β N ) = A ( F −1w1 ,...F −1w M ,F* β1 ,...F* β N )
(2.135) ∀ w i ∈ Tx B, β i ∈ Tx* B. Similarly, the pullback from the spatial configuration of arbitrary tensor b of order { MN } to the reference configuration is defined as
ϕ* b ( V1 ,...VM ,α1 ,...α N ) = b ( FV1 ,...FVM ,F −* α1 ,...F −* α N ) ∀ Vi ∈ TX B0 , α i ∈ TX* B0 .
(2.136)
Composition with ϕ −1 and ϕ for respective pushforward and pullback operations in (2.131)(2.134) is often implied rather than written explicitly and is omitted henceforth when there is no chance of confusion. 5 This is a stricter requirement than noncoincident Cartesian coordinates, wherein the metric tensors reduce to Kronecker delta symbols, but the shifters represent rigid rotations independent of location.
2.5 The Deformation Gradient
43
Since reference and current configurations are embedded in Euclidean space, it is possible to introduce, for each material particle, a displacement function u with spatial components (Eringen 1962) u a = xa − X a + ξ a , (2.137) where x a are spatial components of the vector from the origin of a fixed Cartesian coordinate frame to the particle in the deformed body, X a = g.aA X A are spatial components of the vector from the origin of a different fixed Cartesian coordinate frame to the same particle in the undeformed body, and ξ a are spatial components of the vector extending from the origin of the Cartesian frame in the reference configuration to the origin of the Cartesian frame in the current configuration. Using shifters and metric tensors of Section 2.1.2, u A = g.Aa u a = g Aa ua = G AB uB . (2.138) Since ξ a are components of a constant vector, deformation gradient components F. Aa ( X , t ) can be represented as (Toupin 1956; Suhubi and Eringen 1964) F. Aa = x.,aA = (u a + X a − ξ a ), A = (u B g.aB ), A + ( X B g.aB ), A − (ξ B g.aB ), A = (u.,BA + X .,BA − ξ.,BA ) g.aB + ( X B + u B − ξ B )(g a iG B , A )
(2.139)
= (u + δ ) g . B ;A
B .A
a .B
Similarly, components of the inverse deformation gradient, F −1.Aa ( x, t ) , can be expressed as F −1.Aa = X .,Aa = (δ .ba − u;ba ) g.Ab . (2.140) It is emphasized that the deformation gradient and its inverse cannot be represented by (2.139) and (2.140) when reference and current configurations are nonEuclidean spaces, in which case (2.137) does not apply. 2.5.2 Derived Kinematic Quantities and Identities
The Jacobian determinant of F provides the relationship between a differential reference volume element dV = GdX 1dX 2 dX 3 ⊂ B0 and its deformed counterpart in the current configuration dv = gdx1dx 2 dx3 ⊂ B : JdV = dv . (2.141) In coordinates (Truesdell and Toupin 1960; Eringen 1962; Marsden and Hughes 1983; Dluzewski 1996), the Jacobian determinate is computed as follows:
44
2 Mathematical Foundations
1 1 J = ε abcε ABC F.aA F.bB F.cC = g / Geabc e ABC F.aA F.bB F.cC 6 6 (2.142) 1 1 a = detF g / G = det( x., A ) det( g ab ) / det(GAB ), 6 6 where (2.64) and (2.65) have been used. For the inverse deformation6, 6 J −1 = ε abcε ABC F −1.Aa F −1B.b F −1C.c = G / g det F −1 . From (2.64)(2.67) and Table 2.3, it follows that permutation tensors map between configurations via ε abc = J −1ε ABC F. Aa F.bB F.Cc and ε abc = J ε ABC F −1.Aa F −1B.b F −1C.c . Jacobian J ( X , t ) , unlike detF , is an absolute scalar, invariant under coordinate transformations (Marsden and Hughes 1983). Since volume v remains positive and bounded, 0 < J < ∞ . When there is no deformation, e.g., when a body undergoes only rigid translation, then F = 1 = g.aA g a ⊗ G A , and in that case J = g / G det( g.aA ) = 1 follows from (2.142). The following identity applies for the derivative of the determinant of a nonsingular, secondorder matrix A (Ericksen 1960; Thurston 1974): ∂(det A) = A−1.BA det A . (2.143) ∂A.AB Applying (2.143) to J and J −1 produces the following identities: ∂J ∂J −1 −1 A JF = , = J −1 F. Aa , (2.144) .a ∂F. Aa ∂F −1.Aa as can be verified directly via inspection of (2.142). The total covariant derivative of the second of (2.144), using (2.73) and the chain rule (see the full derivation in Section D.2 of Appendix D), is G
(∂J −1 / ∂F −1.Aa ):a = ( J −1 F. Aa ):a = −1 g ( g J −1 F. Aa ),a − J −1 F.Ca Γ = J −1 F −1.Ba ⎡⎣ x.,aAB − x.,aBA ⎤⎦ = 0.
..C BA
F −1.Ba
(2.145)
Analogously, the divergence of the first of (2.144) produces the identity g
(∂J / ∂F. Aa ):A = ( JF −1.Aa ):A = −1 G ( G JF −1.Aa ), A − J Γ ..bab = 0 . (2.146) Relations (2.145) and (2.146) are often called Piola identities. Using the definition of the determinant and (2.139), the Jacobian satisfies J = g / G det( g.aA ) det ⎡⎣u;AB + δ .BA ⎤⎦ = det ⎡⎣u;AB + δ .BA ⎤⎦ (2.147) ≈ 1 + u;AA + (1/ 2) ⎡⎣(u;AA ) 2 − u;AB u;BA ⎤⎦ . Recall that for two generic, nonsingular square matrices A and B the following identities apply: det( AB) = (det A)(det B) and det( A −1 ) = (det A ) −1 . 6
2.5 The Deformation Gradient
45
Terms of order three in referential displacement gradients are omitted in the final approximation in (2.147). Let oriented differential area elements referred to configurations B0 and B be labeled NdS and nds , respectively, where unit normal covariant vectors N ∈ TX* B0 and n ∈ Tx* B . These area elements are related by the transformation formula nds = J ϕ* NdS , na ds = JF −*.aA N A dS = JF −1.Aa N A dS . (2.148) Relation (2.148) is called Nanson’s formula (Malvern 1969) and represents the Piola transformation between differential forms NdS and nds (Marsb c den and Hughes 1983). Let na ds = ε abc dx[ dx ] = ε abc dx b ∧ dx c / 2 and N A dS = ε ABC dX [ dX B
C]
= ε ABC dX B ∧ dX C / 2 , where for two rankone ob
jects, the wedge product satisfies (α ∧ β ) AB = α A ∧ β B = α A β B − α B β A . Schouten (1954) calls dx a ∧ dxb an infinitesimal bivector. From the above definitions of oriented differential area elements and the properties of the permutation tensor in Table 2.3, it follows that dx a ∧ dx b = ε abc nc ds and dX A ∧ dX B = ε ABC N C dS . Notice that dx a and dx b are treated as components of distinct vectors in the definition of the area element; otherwise the dyad dx a dx b would be symmetric. Notice also that the oriented area eleb c ment na ds = ε abc dx[ dx ] = ε abc dxb dx c . Decomposition of the deformation gradient into the product of two tensors—a rotation and a symmetric positive definite tensor called a stretch tensor—is always possible since F is nonsingular. This separation into stretch and rotation is called the polar decomposition and is written as F = RU = VR , (2.149) where rotation R : TX B0 → Tx B is a proper orthogonal twopoint tensor,
i.e., R −1 = R T and R has positive Jacobian determinant of unit magnitude: RT R = 10 , RRT = 1 , ε abc ε ABC R .aA R .bB R .cC = 6 . (2.150) Right stretch tensor U : TX B0 → TX B0 and left stretch tensor V : Tx B → Tx B satisfy the following symmetry conditions: GABU .BC = GCBU .BA , g abV.cb = g cbV.ab . (2.151) The stretch tensors in (2.151) are determined uniquely by the polar decomposition of F, and are related to the right and left CauchyGreen deformation tensors, C and B respectively, as C = FT F = U 2 , B = FFT = V 2 . (2.152) Since det R = G / g > 0 by convention (2.150), J = det U = det V > 0 .
46
2 Mathematical Foundations
The covariant version of C is the pullback of spatial metric g, and the contravariant version of B is the pushforward of reference metric G −1 : C = ϕ * (g ) , C AB = F. Aa g ab F.Bb = C( AB ) ; (2.153) B = ϕ* (G −1 ) , B ab = F. Aa G AB F. Bb = B ( ab ) . (2.154) The tensors defined in (2.153) and (2.154) are clearly symmetric. From (2.115) and (2.153), C assigns, to first order, the length of an infinitesimal line element after deformation:
dx = FdX =
dX ,CdX .
(2.155)
Furthermore, the right CauchyGreen strain tensor 1 1 E = (C − G ) , E AB = (C AB − GAB ) = E( AB ) , (2.156) 2 2 provides a relationship for the difference in squared lengths of deformed and undeformed line elements as dxidx − dXidX = 2 dX, EdX . (2.157) A number of other finite strain measures not described here may be constructed from F or its inverse (Malvern 1969; Marsden and Hughes 1983). Notice that it is customary to represent the rotation R of (2.149) and (2.150) as a twopoint tensor. If instead R is referred exclusively to reference coordinates, for example, then a shifter must be introduced into the deformation gradient, e.g., F. Aa = R.aCU .CA = g.aB R.BCU .CA = g.aB R.BC (C 1/ 2 ).CA . More kinematic identities emerge from straightforward differentiation7: ∂C AB ∂C AB ∂E AB 1 (C D ) = F. Aa F.Bb , = 2 g abδ .(CA F. Bb ) , = δ .( Aδ . B ) . (2.158) a ∂g ab ∂F.C ∂CCD 2 The following identity is derived from (2.143) and the symmetry of C: ∂ (det C) = C −1BA det C = C −1 AB det C . (2.159) ∂C AB Then because det C = det(C.AB ) = det(G AC F.Cc g cb F.Bb ) = ( g / G )(det F) 2 = J 2 ,
∂J ∂J 1 ∂J 2 1 ∂(det C) =2 = = ∂E AB ∂C AB J ∂C AB J ∂C AB = JC
7
−1 AB
Additionally, from (2.120),
= JF
−1 A .a
ab
g F
−1B .b
(2.160)
= JX g X . A ., a
ab
B .,b
∂F.Ba ∂F −1.Ab = − F. Aa F.Bb and = − F −1.Aa F −1.Bb . −1 A ∂F .b ∂F.Ba
2.5 The Deformation Gradient
47
2.5.3 Linearization
It is instructive to consider the small deformation, i.e., geometrically linear or infinitesimal, kinematic description often applied in engineering practice. In the usual linear theory, displacements and displacement gradients are assumed small so that configurations B0 and B nearly coincide, and the same coordinate system is used in both configurations. Thus the shifter degenerates to g.aA = δ .aA , and partial coordinate differentiation with respect to either configuration is nearly the same operation, e.g., ∂ a (.) ≈ δ .aA ∂ A (.) . Since there is only one coordinate system, lower case indices are used in this book for representation of mathematical objects the linear theory, by default. Covariant differentiation with respect to the LeviCivita connecg
g
tion is represented by ∇ , Christoffel symbols by Γ ..bca ( x) , and metric by g ab ( x) . In Euclidean space, spatial and reference coordinates are related in the linear theory by the vector addition rule x= X+u, (2.161) where u is the displacement vector. Components of the right CauchyGreen strain tensor E( X , t ) of (2.156) are related to spatial covariant derivatives of u( x, t ) as (Eringen 1962) 2 F.a−1 A E AB F.b−1B = ua ;b + ub ;a − u;ca uc ;b . (2.162) Components of the infinitesimal strain tensor ε( x, t ) (also called the linear or small strain tensor) are defined as 1 ε ab = u( a ;b ) = (ua ;b + ub;a ) , (2.163) 2 and clearly differ from those of finite strain tensor E by terms of order two in displacement gradients. Such terms are assumed negligibly small with respect to the displacement gradient itself in the linear theory. Volume changes in the linear theory are computed after omitting terms of orders two and higher in displacement gradients in (2.147) as g
g
J ≈ 1 + u;aa = 1 + tr( ∇ u) , J −1 ≈ 1 − u;aa = 1 − tr( ∇ u) . (2.164) The skew rotation tensor Ω is also introduced in the linear theory: g
Ωab = u[ a ;b] = u[ a ,b] − Γ
..c
[ba ]uc
= u[ a ,b] ,
(2.165)
which itself can be reduced to a vector w via the axial transformation 1 1 wa = − ε abc Ωbc = − ε abc u[b ,c] , Ω ab = −ε abc wc . (2.166) 2 2
48
2 Mathematical Foundations
Tensor Ω , when acting on differential element dx, produces the relative displacement Ωdx = w × dx , where (w × dx) a = ε abc wb dx c . When all components of Ω are small compared to one radian, this relative displacement represents a true rotation, and in Cartesian coordinates, R = 1 + Ω is the corresponding rotation tensor appearing in (2.149).
2.6 Velocities and Time Differentiation Material velocity V ( X , t ) and spatial velocity v ( x, t ) satisfy the following definitions in direct and indicial notation, respectively: ∂x ∂ϕ a ∂ g a , V a ( X , t ) = ϕ a ( X , t ) = v a (ϕ ( X , t ), t ) ; (2.167) V= = ∂t ∂t X ∂t v t = Vt ϕt−1 , v a ( x, t ) = V a (ϕ −1 ( x, t ), t ) .
(2.168)
Recall the notation x = ϕ ( X , t ) and X = ϕ ( x, t ) from Sections 2.1.2 and 2.5.1. Subscript t in the first of (2.168) denotes a spatial field quantity at a particular (fixed) time t. Notice that components of both velocity fields are referred to spatial coordinates. In each definition, the material particle at X is held constant during time differentiation, meaning that velocity is the time rate of change of position of a given material particle. The composition operation in (2.168) is often implicitly assumed rather than written explicitly, and is omitted later in the text when no confusion arises. −1
2.6.1 The Material Time Derivative
The material time derivative measures the rate of change of a quantity associated with given a material particle at X. Because spatial position x of a given particle may change with time, the material time derivative and the partial time derivative of a function expressed in terms of spatial position x can differ. The material time derivative of a differentiable scalar function f of time t and spatial position x is defined as df ∂f δf f ( x, t ) = = + dt ∂t x δ t = =
∂f ∂t ∂f ∂t
+ x
∂f ∂x a ∂x a t ∂t
+ f;a v a , x
(2.169) X
2.6 Velocities and Time Differentiation
49
where the partial time derivative is taken with spatial coordinates x (i.e., position x) held constant, and the intrinsic derivative that accounts for convective changes of scalar function f resulting from the velocity field is δf g = ∇ v f = f;a v a = ( fv a );a − fv;aa = f ,a v a . (2.170) δt It follows that for differentiable functions f and g, d ( f + g ) / dt = f + g and d ( fg ) / dt = fg + fg . The material time derivative is applied in an analogous way to vectors and tensors of higher order as, for example, ∂f da......fc ∂f a f a ( x, t ) = + f ;ba v b , f da......fc ( x, t ) = + f da......fc; k v k . (2.171) ∂t x ∂t x The material time derivative of a timedependent function of position in the reference configuration, with all indices referred to reference coordinates8, by definition equals its partial time derivative: ∂f A...C ∂f ∂f A f ( X ,t ) = , f A ( X ,t ) = , f DA......FC ( X , t ) = D... F . (2.172) ∂t X ∂t X ∂t X
One application of (2.171) for a spatial vector is the spatial acceleration: g ∂v + ∇v v a ( x, t ) = a a g a = v = ∂t x =
∂v a g a + ( v ,b g b ) v ∂t x
=
∂v a g a + [(v c g c ),b g b )][v d g d ] ∂t x
=
g ∂v a ⎛ ⎞ g a + ⎜ v.,cb g c + v c Γ ..bca g a ⎟ vb ∂t x ⎝ ⎠
⎡ ∂v a =⎢ ⎣⎢ ∂t
x
g ⎛ + ⎜ v.,ab + Γ ⎝
(2.173)
⎞ ⎤ v ⎟ vb ⎥ g a . ⎠ ⎦⎥
.. a c bc
8 For a function f of reference position with one or more indices referred to spatial coordinates, letting D / Dt denote the partial derivative with both X and g constant, the material time derivative is defined by (Truesdell and Toupin 1960) g Df DA......FC da......cf ⎛ g ..a A...C k ...c ⎞ f DA......FC da......cf ( X , t ) = + ⎜ Γ bk f D...F d ... f + ... − Γ ..bdk f DA......FC ka......cf − ... ⎟ V b . Dt ⎝ ⎠
50
2 Mathematical Foundations
On the other hand, the material acceleration, i.e., the material time derivative of material velocity (2.167) referred to spatial coordinates, satisfies ∂ (V a g a ) ∂V = A ( X , t ) = Aa g a = ∂t X ∂t X =
∂V a ∂t
∂V = ∂t
ga + V a X
a
∂x g a + V g c,b ∂t c
X
X
b
(2.174)
X
⎛ ∂V ⎞ =⎜ + Γ ..bcaV cV b ⎟ g a , ⎜ ∂t ⎟ X ⎝ ⎠ = (∂v a / ∂t ) x + v.,ab v b from (2.167). Expressed as a
noting that (∂V a / ∂t ) X
∂g a ( x) ∂t
g
material time derivatives, contravariant velocity components are written as V a ( X , t ) = v a ( x, t ) = x a ( X , t ) and contravariant acceleration components are written as Aa ( X , t ) = a a ( x, t ) = x a ( X , t ) . Using (2.118) and (2.171), the material time derivative of the deformation gradient F = F. Aa g a ⊗ G A = x.,aAg a ⊗ G A of (2.112), an example of a twopoint tensor, is calculated in components as follows (Eringen 1962): ∂F a δ F a ∂F a F. Aa = . A + . A = . A + F. Aa ;b vb ∂t x δt ∂t x =
g ∂F. Aa ⎛ + ⎜ F. Aa ,b + Γ ∂t x ⎝
..a bc
⎞ F. Ac ⎟ vb ⎠
(2.175) g DF. Aa g ..a c b = + Γ bc F. AV = V.,aA + Γ ..bca F. AcV b Dt g ⎛ ⎞ = ⎜ v.,ac + Γ ..cba vb ⎟ F. Ac = v;ac F. Ac . ⎝ ⎠ The spatial velocity gradient tensor L(x,t), i.e., the covariant spatial derivative of the velocity vector v(x,t), is L = v ,b ⊗ g b = v;ab g a ⊗ g b = FF −1 , (2.176) L.ab = v;ab = ( x a );b = F. Aa F −1.Ab . Noting that d ( F. Aa F −1.Ab ) / dt = d (δ.ba ) / dt = 0 , the material time derivative of the inverse deformation gradient satisfies ( F −1 ).Aa = − F −1.Ab Lb.a = − X .,Ab ( xb );a .
2.6 Velocities and Time Differentiation
51
The covariant derivative of a metric tensor with respect to its LeviCivita connection always vanishes identically; thus the material time derivative of spatial metric tensor with components g ab ( x ) vanishes: g ab ( x) =
∂g ab ∂g ab + g ab;c v c = 0 , g ab ( x) = ∂t ∂t x
+ g;abc v c = 0 .
(2.177)
x
Furthermore, GAB ( X ) = (∂GAB / ∂t ) X = 0 . Thus, raising or lowering of indices commutes with material time differentiation in either configuration. 2.6.2 The Lie Derivative
The Lie derivative of a differentiable but otherwise arbitrary function f ( x, t ) on spatial manifold B taken with respect to the velocity field v( x, t ) of (2.168) is computed by ⎡d ⎤ (2.178) L v f = ϕ* ⎢ (ϕ * f ) ⎥ , ⎣ dt ⎦ where ϕ* and ϕ* denote pullback and pushforward operations with respect to the motion. The notation d / dt denotes a material time derivative, as implied already by (2.169). In this text, particular Lie derivative (2.178) is considered exclusively. However, more general definitions of Lie derivatives taken with respect to timedependent vector fields, e.g., fields other than velocity v, exist (Schouten 1954; Marsden and Hughes 1983). Lie derivatives are useful for positing constitutive equations in rate form because objective rates of secondrank tensors have objective Lie derivatives. The component representation of Lie derivative (2.178) for a scalar function f equals its material time derivative: ∂f ∂f ∂f Lv f = f = = + v a f;a = + (fv a );a − fv;aa . (2.179) ∂t X ∂t x ∂t x For vectors and tensors of higher order, the Lie derivative in components is
52
2 Mathematical Foundations
Lv f a ...h i ...r =
∂f a...h i...r ∂t
+ v s f a ...h i ...r ; s x
− v;as f s...h i...r − ... − v;hs f a ...s i ...r + v;ti f s ...h t ...r + ... + v;tr f a ...s i ...t ∂f a...h i ...r = ∂t
+v f s
(2.180)
a ...h i ... r , s
x
− v.,as f s...h i...r − ... − v.,hs f a...s i...r + v.,t i f s...ht ...r + ... + v.,t r f a...s i ...t since terms involving Christoffel symbols in the covariant derivatives cancel by the symmetry of the LeviCivita connection on B. For the scalar J ( X , t ) , a direct calculation with the chain rule, (2.144), and (2.176) gives ∂J a Lv J ( F. Aa ( X , t ), g ( x), G ( X )) = J = F. A = JF −1.Aa F. Aa ∂F. Aa (2.181) = JLa.a = JD.aa = Jv;aa = J ( x a );a . In components, the Lie derivative of the spatial metric tensor g ab ( x) is ( Lv g ) ab = ∂g ab / ∂t x + v c g ab;c + v;ca g cb + v;cb g ac = 2 L( ab ) = 2 Dab ,
(2.182)
=0
where Dab are components of the symmetric deformation rate tensor. 2.6.3 Rate Kinematics
Velocity gradient L provides, to first order, the difference dv in spatial velocities of two particles in the spatial frame separated by a small vector dx. The material time derivative applied to (2.115) results in dv = Ldx , dv a = dx a = F. Aa dX A = F. Aa F −1.Ab dx b = v;ab dx b = La.b dx b . (2.183) Deformation rate tensor D provides the material time derivative of the squared length of a differential line element dx: d ( dxidx ) / dt = 2dxidv = 2 Lab dx a dxb (2.184) = 2 L( ab ) dx a dxb = 2 Dab dx a dxb because dx a dx b = dx ( a dx b ) . Since from (2.115), d ( dxidx ) / dt = d ( F. Aa dX A g ab F. Bb dX B ) / dt = C AB dX A dX B , (2.185) time rates of right CauchyGreen strain and deformation tensors satisfy
2.7 Theorems of Gauss and Stokes
53
1 E AB = C AB = F. Aa Dab F.Bb , (2.186) 2 relationships that can also be derived directly from (2.153), (2.156), (2.176), and (2.182), without resorting to use of firstorder approximation (2.115). The skew covariant part of L, called the spin tensor or vorticity tensor and labeled W, provides the time rate of rotation of a differential line element dx. In components, Wab = L[ ab] = Lab − Dab = va ;b − v( a ;b ) = v[a ;b] = v[a ,b] , (2.187) with the final equality following from the symmetry of the connection coefficients. Appealing to the polar decomposition in the first of (2.149) and (2.176), the velocity gradient can be written L = RR T + RUU −1R T . (2.188) From time differentiation of (2.150), the covariant version of the first term on the right of (2.188) is always skew: g ac R.cA RT .Ab = − g bc R.cA RT .Aa , (2.189) meaning that the spatial deformation rate is comprised of the symmetric part of the second term on the right of (2.188): (2.190) 2 Dab = g ac R.cAU .ABU −1.BC RT .Cb + g bc R.cAU .ABU −1.BC RT .Ca . Noting that u = v , in the context of the geometrically linear theory of Section 2.5.3, the deformation rate is equivalent to the time rate of the small strain tensor, and the spin is equivalent to the rate of rotation: Dab = v( a ;b ) = u( a ;b ) = ε ab , (2.191) Wab = u[a ;b] = u[ a ,b] = Ωab = −ε abc wc .
2.7 Theorems of Gauss and Stokes Two fundamental theorems of vector calculus associated with integration are used frequently later in the text. The first, known as Gauss’s theorem or Green’s theorem, relates volume and surface integrals. A particular case is the wellknown divergence theorem. The second is Stokes’s theorem, and it relates surface and line integrals. 2.7.1 Gauss’s Theorem
The generalized Gauss’s theorem exhibits the form (Malvern 1969) (2.192) ∫ A ∗ ∇ dV = ∫ A ∗ N dS , V
S
54
2 Mathematical Foundations
where A is a scalar, vector, or tensor of arbitrary order that has continuous first derivatives with respect to local coordinates, ∇ is the covariant derivative operator with respect to the LeviCivita connection of these coordinates, and N is the outward unit normal covariant vector to differential surface area element dS. Surface S, which encloses volume V, is required to be piecewise smooth and exhibit a topological outside and inside, such that N may be clearly assigned to point from the inside to the outside of V for each surface element dS. Volume V must be simply connected for a single continuous surface S to suffice9; otherwise, (2.192) may be applied over the union of disjoint surfaces completely enclosing a volume that is not simply connected. The ∗ operator—not to be confused with the pushforward ϕ∗ or pullback ϕ * introduced in Section 2.5.1 that feature asterisks written in respective subscript or superscript positions—represents a general product that exhibits the distributive property. Examples include the dual product , , the dot product i , the vector cross product × , and the tensor (outer) product ⊗ . The familiar divergence theorem of vector calculus is obtained from (2.192) when ∗ is the dual or dot product, e.g., for a spatial vector field aˆ ( x, t ) ,
∫ aˆ
a ;a
v
dv = ∫ aˆ a na ds .
(2.193)
s
As a second example (Hill 1972, 1984; Clayton and McDowell 2003a), consider cases wherein the body is simply connected, enclosed by a single continuous surface. In (2.192), let A → x( X , t ) and let V be the volume of the body in the reference configuration enclosed by surface S, with local outward normal N. The ∗ operator is chosen to be the outer product ⊗ , giving a a (2.194) ∫ x; A dV = ∫ x N A dS . V
S
Since (2.194) involves integration of a twopoint tensor field, for the integrals to represent valid quantities at any location in Euclidean space10, basis vectors g a ( x ) and G A ( X ) should be chosen as constant with respect to changes in position. This requirement leads to vanishing of the Christoffel In many texts, integration over a closed surface in (2.192) or closed curve in (2.197) is delineated by the explicit notation ∫ . Throughout this text, domains of 9
integration are simply defined as they appear. 10 Alternatively, the integral of a vector or tensor field can be defined in a valid manner at a single point in space by parallel transporting all positiondependent quantities within the integrand to that point using a shifter (Toupin 1956). This approach is pursued explicitly in Chapter 3 in the context of the Burgers circuit.
2.7 Theorems of Gauss and Stokes
55
symbols in each configuration. This restriction does not require that basis vectors in the two configurations must coincide, nor does it require that basis vectors in each configuration must be orthogonal. In other words, (2.194) requires g ab,c = 0 and GAB ,C = 0 , but one can still have g ab ≠ δ ab , GAB ≠ δ AB , and g.aA ≠ δ .aA , as considered by Sedov (1966). Thus, (2.194) reduces to a a a (2.195) ∫ x., AdV = ∫ F. A dV = ∫ x N A dS . V
V
S
Dividing (2.195) by V gives the volume average of the deformation gradient in terms of spatial position and reference orientation of surface S: V −1 ∫ FdV = V −1 ∫ x ⊗ NdS . (2.196) V
S
1
Strict application of (2.196) requires C continuity of x( X , t ) . 2.7.2 Stokes’s Theorem
The generalized Stokes’s theorem is written (Malvern 1969) ∫ (N × ∇) ∗ A dS = ∫ dX ∗ A , S
(2.197)
C
where quantities introduced already in (2.192) have the same definitions, and where C is a closed curve with coordinates X encircling an oriented surface S with normal N. Again, A must have continuous first derivatives with respect to coordinates corresponding to covariant derivative with gradient operator ∇. Surface S must be simply connected for a single curve C to suffice; otherwise the line integration must proceed over the collection of bounding curves interior and exterior to S. When path C of the line integral is taken in a counterclockwise sense, the positive direction of normal N is defined according to the usual righthand rule of vector calculus. Stokes’s theorem, like Gauss’s theorem, can be applied in either configuration of the body. For example, when A → v( x, t ) (the spatial velocity field) and ∗ → . , . x , the following equality applies:
∫ε s
abc
g
g
nb ∇ c va ds = ∫ ε abc va ;c nb ds = ∫ ε abc (va ,c − Γ s
..d ca d
v )nb ds
s
= − ∫ ε abc va ,b nc ds = − ∫ va ,b dx a ∧ dx b = ∫ va dx a , s
s
(2.198)
c
where s and c denote, respectively, surfaces and bounding curves on a body in the spatial description. When the curl or skew gradient of v van
56
2 Mathematical Foundations
ishes, i.e., when v[ a ;c] = v[ a ,c] = Wac = 0 , the integrand in (2.198) is identically zero, and the velocity field is said to be irrotational. Consider now the deformation gradient in the context of Stokes’s theorem. Let S and C denote, respectively, surfaces and bounding curves on a body in the reference description, let A → F ( X , t ) , and let ∗ → . , . X . Then in indicial notation, ABC a ABC a ∫ ε F. A;C N B dS = −∫ ε F. A, B NC dS S
S
(2.199)
= − ∫ F. Aa , B dX A ∧ dX B = ∫ F. Aa dX A . S
C
G
where symmetry properties of the Christoffel symbols Γ
.. A BC
been exploited. Likewise, in the spatial description, abc −1 A abc −1 A ∫ ε F .a;c nb ds = −∫ ε F .a,b nc ds s
s
= − ∫ F −1.Aa ,b dx a ∧ dx b = ∫ F −1.Aa dx a . s
G
=Γ
.. A ( BC )
have
(2.200)
c
Restrictions on coordinate systems may apply since (2.199) and (2.200) involve integration of vector fields. Specifically, basis vectors g a must be constant for all points x in the domain of integration in global equation (2.199), while basis vectors G A must be constant for all points X in the domain of integration of (2.200). Otherwise, integrands in (2.199) and (2.200) must be parallel transported to a single point (x or X) using the appropriate shifter, and the integral then evaluated at that point (Toupin 1956). Furthermore, F ( X , t ) and F −1 ( x, t ) must have continuous first derivatives with respect to reference and spatial coordinates, respectively. From (2.115), since the line integral of position about a closed loop on the surface of or within a simply connected body vanishes, 0 = ∫ dx a = ∫ F. Aa dX A = − ∫ ε ABC F. Aa , B N C dS , (2.201) c
C
S
0 = ∫ dX A = ∫ F −1.Aa dx a = − ∫ ε abc F −1.Aa ,b nc ds . C
c
(2.202)
s
Since (2.201) and (2.202) must hold for any path within the body, F.[aA, B ] = F.[aA; B] = F.[aA:B] = 0 , F −1.A[a ,b] = F −1.A[a ;b] = F −1.A[a:b] = 0 . (2.203) As discussed further in Section 2.8, (2.203) can be interpreted as local compatibility conditions for the deformation gradient and its inverse.
2.8 Anholonomic Spaces and Compatibility
57
2.8 Anholonomic Spaces and Compatibility The following topics associated with compatibility, or lack thereof, of arbitrary tangent maps and linear connections are discussed in Section 2.8: anholonomic deformations and anholonomic configurations, strain compatibility, connection compatibility, and the Jacobian determinant. 2.8.1 Anholonomicity
Consider a field of covariant basis vectors gα (α = 1, 2 ,3) , spanning a tangent bundle TB associated with arbitrary configuration B . By introducing the twopoint map F (X ,t ) = F α.A gα ⊗ G A that is assumed to be differentiable and invertible, generic vectors V ∈ TX B0 are pushed forward to Tx B :
FV = F α. A g α ⊗ G A (V B G B ) = F α. AV B gα G A , G B = F α. AV Bδ . BA gα = F α. AV Agα ∈ Tx B.
(2.204)
Basis vectors are tangent to globally continuous coordinate curves x α (i.e., gα = ∂ / ∂xα for some coordinate parameterization xα (X ,t ) ) if and only if the following integrability conditions hold for F (Schouten 1954): ∂ 2 xα ∂ 2 xα F. Aα, B = F .αB , A ⇔ = . (2.205) A B ∂X ∂X ∂X B ∂X A If conditions (2.205) are not satisfied, then gα is called an anholonomic basis vector, the tangent map F is called an incompatible map, and B is called an incompatible configuration or an anholonomic space11. In such a case, anholonomic coordinates xα , sometimes called nonholonomic coordinates (Stojanovitch 1969), are available as onetoone functions of location X only over local patches of B , if at all. Anholonomic spaces can be interpreted as containing regions where coordinates xα may be multivalued (overlaps) or undefined (holes) functions of X (Kondo 1964). From another perspective, when anholonomic, B can be considered a ninedimensional space (nine independent components of F α.A ) in contrast to When F does not have continuous first partial derivatives, (2.205) does not apply. For example, a piecewise linear field of coordinates xα ( X ) can result in a 11
piecewise constant deformation gradient x.,αA ( X ) with discontinuities, as can occur physically in crystals in the context of deformation twinning (James 1981).
58
2 Mathematical Foundations
holonomic configuration B0 parameterized by three independent coordinates X A . Since the deformation gradient and its inverse are integrable, F.[aA, B] = 0 and F.[−a1,bA] = 0 , as indicated in (2.203) in the context of Stokes’s theorem. Because conventional differentiation with respect to anholonomic coordinates does not apply, partial differentiation with respect to anholonomic x α is defined in a special manner: ∂ ( . ) ∂ ( . ) −1 A ∂α ( . ) = ( . ),α = α = F .α ∂x ∂X A (2.206) a −1 A −1 A = ∂ A ( . )F .α = ∂ a ( . ) F. A F .α . The anholonomic object κ is introduced (Schouten 1954; Kondo 1964): α κ ..βχα = F −.β1 A F −. 1χB ∂[ A F .αB] = F −.β1 A F −.1χB F .α[ B , A] = κ ..[ βχ (2.207) ], a geometric construct whose components vanish if and only if F is integrable. Consider the transformation law for the connection coefficients given by (2.28), but now applied with respect to a change from holonomic to anholonomic coordinates X A → xα , where (2.206) is used to define partial differentiation with respect to xα . Arbitrary connection coeffi..A ..α on B0 then transform to coefficients Γ βχ on B as cients Γ BC ..α .. A Γ βχ = F −. 1βB F −. 1χC F .αA Γ BC + F −. χ1C, β F .αC .. A = F −. 1βB F −. 1χC F .αAΓ BC − F −. 1βB F −. 1χC F .αC , B .
(2.208)
Torsion tensor T of (2.33) pushed forward to B becomes, in components .. A α ..α Tβχ..α = F −. 1βB F −. 1χC F .αATBC = Γ [..βχ (2.209) ] + κ βχ , α ..A implying that Γ [..βχ ] need not vanish for covariant components of Γ BC to
be symmetric. Partial derivatives of basis vectors with respect to an arbitrary connection on B are defined as analogs of (2.56): ..α χ .. χ (2.210) gα, β = −Γ βχ g , gα , β = Γ βα gχ . Relations (2.210) are treated here as general postulates, applicable regardless of whether or not (2.208) is used to define connection coefficients on B . However, when (2.208) does specifically apply, skew partial derivatives of covariant basis vectors in (2.210) need not always vanish even if Tβχ..α = 0 , since .. χ .. χ g[α , β ] = Γ [..βαχ ] g χ = (Tβα − κ βα )g χ .
(2.211)
2.8 Anholonomic Spaces and Compatibility
59
The expression for the RiemannChristoffel curvature tensor of a linear ...A connection, defined with respect to holonomic coordinates in B0 as RBCD in (2.34) and pushed forward to anholonomic coordinates xα , is (Schouten 1954; Kondo 1964) ...α ... A Rβχδ = F −. 1βB F −. 1χC F −.δ1D F .αA RBCD ..α ∂Γ χδ
..α ∂Γ βδ
..α ..ε ..α ..ε ..ε + Γ βε − Γ χε + 2κ βχ Γ χδ Γ βδ Γ εδ..α ∂x β ∂x χ ε ..α = 2∂[ β Γ χ..α]δ + 2Γ [..βαε Γ χ..ε]δ + 2κ [..βχ ]Γ εδ ,
=
−
(2.212)
which, upon comparison with the holonomic representation in (2.34), differs only by the rightmost term that includes the anholonomic object. 2.8.2 Strain Compatibility
A second interpretation of compatibility follows from consideration of the RiemannChristoffel curvature tensor. From (2.43), Christoffel symbols of the second kind in the context of Riemannian geometry formed from the symmetric right CauchyGreen deformation tensor C( X , t ) are C C 1 Γ ..BCA = C −1 AD (CBD,C + CCD, B − CBC , D ) = Γ ..CBA . (2.213) 2 C
C
A curvature tensor R can be constructed by substituting components Γ C
..A BC
g
into (2.34). Since C = ϕ * (g) , R = φ* (R ) follows from properties of the connection and curvature (Marsden and Hughes 1983). Thus, if the deformation tensor field C is derivable from a motion ϕ (X ,t ) , and since g
C
R = 0 , it follows that R = φ* (0) = 0 and C is compatible. Section D.3 of Appendix D contains an alternative derivation worked out in convected coordinates, demonstrating vanishing of the curvature tensor formed from C AB = F. Aa g ab F. Bb noting that conditions F. Aa = x.,aA and F. Aa , B = F.Ba , A apply. Notice that Ccompatibility does not require specification of a unique spatial configuration, since C is independent of the rotation tensor associated with the right polar decomposition in (2.149). Furthermore, even if C is compatible, integrability of an arbitrary field F generating the field C = FT F may be precluded by rotations R that do not arise from rigidbody transformations of ϕ . For example, consider the field F. Aa = R.aA with R.aA RT .Ab = δ .ba , such that C AB = F. Aa g ab F.Bb = R.CAGCD R.DB = GAB . Integrability of
60
2 Mathematical Foundations
F is violated by a rotation field for which R.[aA, B] ≠ 0 , even though the curvature tensor constructed from C AB = GAB vanishes identically in this case. A material in such a condition is said to be in a state of contorted aleotropy (Noll 1967). The converse of the previous theorem has also been proven, albeit only locally (Eisenhart 1926). In other words, given a positive definite, symmetric, secondorder tensor C whose curvature vanishes (i.e., C
R = 0 ) then at any point X ∈ B0 there exists a neighborhood U 0 of X endowed with a mapping ϕ : B0 ⊃ U 0 → U ⊂ B whose deformation tensor is C. A more extensive discussion of compatibility in terms of C is given by Fosdick (1966), who notes that vanishing of the Ricci tensor or the EinC
stein tensor constructed from R is sufficient to ensure compatibility of C. One can consider Ccompatibility an outcome of deformation gradient compatibility (i.e., Fcompatibility): if F. Aa ( X , t ) is compatible, then it follows that C AB ( X , t ) = F. Aa g ab F.Bb is also compatible, as demonstrated in Section D.3 of Appendix D. It is emphasized that a LeviCivita connection—a connection both torsionfree and metric with respect to g , where the metric has components gαβ = gα ig β —on anholonomic space B may not exist, since the field of vectors gα may not be sufficiently smooth over all of B to admit coordinate differentiation with respect to coordinates that may in fact be discontinuous or multivalued, i.e., anholonomic coordinates. However, in anholonomic (e.g., intermediate or natural) configurations of elastoplasticity theory, each local volume element of material is often referred to an external system of coordinates with Euclidean metric tensor, typically taken as Kronecker’s delta for convenience (Teodosiu 1967a, b; Simo and Ortiz 1985), though the assumption gαβ = δαβ is not always necessary (Maugin 1995; Clayton et al. 2004a). This issue is discussed in more detail in Section 3.2.2. Notice also that the RiemannChristoffel curvature tensor formed from the generally incompatible covariant deformation measure C AB = F α.A gαβ F .Bβ does not necessarily vanish unless xα are holonomic, in contrast to the vanishing curvature tensor derived from connection (2.213) formed from the compatible deformation tensor C. Compatibility equations for the small strain tensor of (2.163) are typically expressed somewhat differently than those for C (Malvern 1969; Mura 1982; Teodosiu 1982). The former are derived from differentiation
2.8 Anholonomic Spaces and Compatibility
61
of the right side of (2.163) and a sequence of indicial manipulations, leading to vanishing of the incompatibility tensor with components s cf : cf s cf = s ( ) = g −1e abc e def ε bd ;ae = − g −1ecab e fed ε bd ;ae = 0 . (2.214) The six independent equations in (2.214) ensure that symmetric tensor ε(x,t ) with continuous second derivatives with respect to holonomic coordinates x a is integrable; i.e., (2.214) ensures that a continuously differentiable displacement field u( x, t ) exists such that (2.163) applies. Analogously to (2.203), ua ,[bc] = 0 from the commutative property the of the mixed second partial derivative with respect to holonomic coordinates, and vanishing of the curvature and torsion of the LeviCivita connection results in ua ;[bc ] = 0 , as concluded from (2.40). 2.8.3 Connection Compatibility
Consider coefficients of a special linear connection formed by spatial differentiation of a smooth, possibly anholonomic tangent map with inverse F −1 (x,t ): Tx B → Tx B , defined as follows:
Γ cb..a = F.αa ∂ c F .−b1α = F.αa F .−b1,αc = − F.αa ,c F .−b1α = − F.αa , β F .−b1α F .−c1β ,
(2.215)
where the third of (2.215) follows from (F.αa F .−b1α ),c = δ .ba ,c = 0 and the final equality follows from (2.206). Connections of the form (2.215) have special meaning in field theories of lattice defects (Bilby et al. 1955; Kroner 1960) and are said to exhibit the property of teleparallelism or absolute parallelism (Einstein 1928; Schouten 1954). Partial differentiation of (2.215) yields (2.216) ( F −.a1α Γ bc..a ) , d = F −.c1α,bd , the left side of which is expanded as F −.a1α, d Γ bc..a + F −.a1α Γ bc..a,d = F −.a1α (Γ de..a Γ bc..e + Γ bc..a, d ) .
(2.217)
Since the order of partial differentiation on the right side of (2.216) is arbitrary (Schouten 1954; Le and Stumpf 1996a), 0 = 2∂ [b ∂ d ] F −.c1α = F −.a1α (Γ dc..a,b − Γ bc..a, d + Γ be..a Γ dc..e − Γ de..a Γ bc..e ) (2.218) ...a = F −.a1α Rbdc , ...a are components of the RiemannChristoffel curvature tensor where Rbdc
derived from Γ cb..a of (2.215) using definition (2.34). Upon multiplication
62
2 Mathematical Foundations
...a of (2.218) through by F , it is evident that Rcdb = 0 are conditions ensuring satisfaction of (2.215). In that case (i.e., null curvature), the connection with coefficients Γ cb..a is said to be integrable (Schouten 1954). Secondarily, if the connection with coefficients in (2.215) is symmetric, then its torsion vanishes by definition, and it follows from arguments analogous to those accompanying (2.205) that F −1 (x,t ) is itself integrable:
Tcb..a = Γ [..cba ] = F.αa F .−[b1α,c ] = 0 ⇔ F .−a1α = x.,αa = ∂ a x α .
(2.219)
When (2.219) applies, 1 Γ bc..a = C −1ad (Cbd ,c + Ccd ,b − Cbc , d ) , ∇ a Cbc = 0 , (2.220) 2 meaning that Γ cb..a are LeviCivita coefficients formed from a metric tensor with components Cab (x,t ) = F −.a1α gαβ F −.b1β , and the set { B,Γ cb..a ,Cab } consti
...a tutes a Euclidean space since Rbdc = 0 . Components of a second metric
tensor on B are denoted by gαβ and can be chosen as gαβ = δαβ for convenience. The first equality in (2.220) follows from direct calculation and (2.219) as 2Γ bc..a = C −1ad (Cbd ,c + Ccd ,b − Cbc ,d )
= 2 F.αa F .−( 1cα,b ) + 2 F.αa g αβ F.βd ⎡ F −.b1χ F −.[1dδ,c] + F −.c1χ F −.[1dδ,b] ⎤ g χδ ⎣ ⎦ a −1α = 2 F.α F .( c ,b ) ,
(2.221)
and the second of (2.220) is verified by substituting the first of (2.220) into .. d ∇ a Cbc = Cbc , a − Γ ab Cdc − Γ ac..d Cbd = 0 . (2.222) 2.8.4 The Jacobian Determinant for Anholonomic Mappings
The Jacobian determinant of anholonomic mapping F introduced in (2.204) provides, by definition, the relationship between a differential reference volume element dV ⊂ B0 and its deformed counterpart in the anholonomic space, dV ⊂ B :
JdV = dV . (2.223) Analogously to (2.142), the function J ( X , t ) , regarded as a true scalar under coordinate transformations, is calculated in coordinates as
2.8 Anholonomic Spaces and Compatibility
63
1 1 J = ε αβχ ε ABC F.αA F.βB F.Cχ = g / Geαβχ e ABC F.αA F.βB F.Cχ 6 6 (2.224) 1 1 α = detF g / G = det( F. A ) det( gαβ ) / det(G AB ), 6 6 where g = det( gαβ ) = det(gα ig β ) ≥ 0 . Requiring that the volume of any element must remain positive and finite implies bounds ∞ > J > 0 . Differentiation of (2.224) produces an identity like (2.144): ∂J 1 (2.225) = ε αβχ ε ABC F.βB F.Cχ = JF.α−1 A . α ∂F. A 2 Taking the total covariant derivative of the first of (2.225) then gives 2( JF.α−1 A ): A = ε αβχ ε ABC ( F.βB: A F.Cχ + F.βB F.Cχ : A ) (2.226) = ε αβχ ε ABC ( F.[βB: A] F.Cχ + F.βB F.[χC: A] ). When (2.205) is not satisfied, meaning anholonomic object κ in (2.207) does not vanish, the right side of (2.226) may be nonzero and Piola identities such as those in (2.145) and (2.146) for holonomic mapping F and its inverse do not always hold for anholonomic mappings. Let oriented differential area elements referred to configurations B0 and B be labeled NdS and nds , respectively. Analogously to (2.148), these elements are related by Nanson’s formula or a Piola transformation: nds = JF −* NdS , nα ds = JF α−*. A N A dS = JF .−α1 A N A dS . (2.227) β χ In terms of the wedge product, nα ds = ε αβχ dx[ dx ] = ε αβχ dx β ∧ dx χ / 2 and
dx a ∧ dx b = ε αβχ nχ ds , with dx a and dx b components of two different infinitesimal vectors so their tensor product is not identically symmetric. Relation (2.227) can be obtained directly from (2.224), noting that 6 = (ε αβχ )( J −1ε ABC F.αA F.βB F.Cχ ) = ( geαβχ )( J −1 −1 Ge ABC F.αA F.βB F.Cχ ) = ε αβχ ε αβχ = ε ABC ε ABC
(2.228)
= ( J −1 geαβχ F.αA F.βB F.Cχ )(−1 Ge ABC ). Therefore, permutation tensors referred to configurations B and B0 satisfy
ε αβχ = J −1ε ABC F.αA F.βB F.Cχ , ε ABC = J −1ε αβχ F.αA F.βB F.Cχ . α
α
(2.229)
Letting dx = F. A dX , it follows that an oriented area element in B0 is A
64
2 Mathematical Foundations
N A dS = ε ABC dX B dX C = ε ABC F .−ε1B F .−φ1C dxε dxφ = J −1 F.αAε αβχ dx β dx χ = J −1 F.αA nα ds ,
(2.230)
the inverse of which yields the final result in (2.227). The same approach can be used to derive (2.148) directly from (2.142), as demonstrated in Section D.2 of Appendix D.
3 Kinematics of Crystalline Solids
Chapter 3 provides descriptions of kinematics of crystalline materials undergoing various deformation mechanisms at the microscopic scale. Specifically, such deformation mechanisms can include recoverable and residual elasticity, thermal expansion or contraction, plasticity manifesting from dislocation glide, and volume changes resulting from point defects and voids. A description of kinematics of deformation twinning is postponed until Chapter 8. The treatment of kinematics is developed in the context of geometric nonlinearity; i.e., finite strains and rotations are addressed. Finite deformation theory is considered more applicable than linear or infinitesimal deformation theory for a number of reasons. From a physical standpoint, a nonlinear theory permits consideration of the sequence of deformation mechanisms occurring in a crystalline solid in terms of a multiplicative series of tangent maps. Such a description is naturally associated with a series of configurations or manifolds corresponding to real or virtual states of the deforming body. For example, application of the inverse elastic tangent map to a deformed crystal leads to a stressfree, unloaded state. Such configurations are possibly incompatible, or anholonomic in the terminology of Chapter 2, and their geometric description can be directly related to physical features such as defect content in a crystal. In addition to the increased generality and physical insight afforded by a finite deformation description, a nonlinear theory is essential for obtaining accurate depictions of material behavior in applications of solid mechanics wherein strains are inevitably large, for example in ballistic impact, crashworthiness scenarios, metal forming, and high pressure phenomena, with the latter encountered, for example, in geologic settings and shock physics experiments. Such nonlinear problems often require numerical solutions because of their complexity. Even when average deformations remain small, large deformations may still arise locally in many micromechanical problems of interest, for example studies of defect core structures, crack tip mechanics, and strain localization phenomena. Furthermore, since nearly all natural single crystals are anisotropic, large rotations of the lattice may be of importance even when strains are small. Finally, reduction of the finite deformation description to the infinitesimal deformation the
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_3, © Springer Science+Business Media B.V. 2011
65
66
3 Kinematics of Crystalline Solids
ory via linearization is usually straightforward (though it is noted that methods of linearization are often not unique), while extension of a linear description to the nonlinear regime is often not. For completeness, occasional comparisons are drawn in Chapter 3 with complementary geometrically linear theories. Chapter 3 begins with an introductory description of crystal structures. The usual fourteen Bravais lattices comprising the seven crystal systems are introduced. The CauchyBorn hypothesis (Born and Huang 1954; Ericksen 1984)—a fundamental postulate stating that primitive Bravais lattice vectors of a crystal structure deform according to the action of a spatially constant deformation gradient acting over a homogeneously deforming volume element of crystal—is then discussed. Deformations of the solid induced explicitly by changes in temperature are described. Multiplicative inelasticity (Bilby et al. 1957; Kroner 1960; Lee and Liu 1967) is presented next. Characterizations of plastic deformation in the context of dislocation flux (i.e., discrete dislocation dynamics), slip system activity in single crystals (i.e., crystal plasticity), and flow in polycrystals (i.e., macroscopic plasticity) are presented in turn. While plasticity manifesting from dislocation glide is volumepreserving, inelastic deformation attributed to the generation and motion of point defects, including vacancies associated with dislocation climb, is generally not (Teodosiu and Sidoroff 1976; Kroner 1990). At a somewhat larger length scale, damage mechanisms such as porosity evolution (e.g., void growth or pore compaction) can engender inelastic volume changes. Such phenomena are all addressed in the kinematic descriptions of Chapter 3. Coarsegraining principles (Clayton and McDowell 2003a) enabling quantification of heterogeneous local elastic and plastic deformations within a volume element of crystalline material are also presented. Defect densities, typically tensorvalued quantities (Nye 1953), are considered next, from a differentialgeometric viewpoint. In Chapter 3, defects are frequently treated as continuous distributions rather than as discrete entities with singularities in displacement gradients, and elastic and plastic tangent maps are assumed suitably smooth; specifically, these maps are assumed at least twice differentiable with respect to local coordinates. The multiplicative decomposition of elastoplasticity is used to describe the possibly large deformation of a volume element of crystalline material, and a complementary linear connection is introduced to describe spatial gradients of stretch and rotation of a field of lattice director vectors at a finer scale of resolution. Geometric properties of the connection enable characterization of dislocations (Bilby et al. 1955; Kroner 1960; Kondo 1963; Noll 1967), disclinations (Lardner 1973, 1974; Minagawa 1979, 1981; Clayton et al. 2005, 2006), point defects (Minagawa 1979; Kroner 1981,
3.1 Crystals and Lattice Deformation
67
1990; Clayton et al. 2008a), and physical origins of incompatibility of a more generic nature (Clayton et al. 2005).
3.1 Crystals and Lattice Deformation Section 3.1 begins with an introductory description of crystal structures and related terminology. This is followed by discussion of homogeneous deformation of an element of the crystal, i.e., the CauchyBorn hypothesis, under isothermal conditions and in the absence of defects in the crystal. The description is then generalized to account for effects of temperature change, for example expansion of the lattice with increasing temperature. 3.1.1 Crystal Structures In this book, a crystal is defined as a material whose majority of atoms occupies a periodically repeating arrangement called a lattice. A crystal structure consists of a Bravais lattice and a basis for atoms decorating that lattice. A Bravais lattice is an infinite array of points generated by repeated translation of a set of vectors called primitive lattice vectors. A point on a threedimensional Bravais lattice can be identified by its position in threedimensional vector space via the vector summation 3
R (l ) = ∑ l i A i = l1A1 + l 2 A 2 + l 3 A3 , ( l1 , l 2 , l 3 ∈ ),
(3.1)
i =1
where R (l ) denotes the Bravais lattice vector directed from the origin of a global Cartesian coordinate system to the lattice point corresponding to primitive unit cell l, A i are the primitive Bravais lattice vectors, and l i are integers. By convention, a lattice point is placed at the origin of the global coordinate system. Each primitive unit cell contains exactly one lattice point, and each primitive unit cell occupies volume Ω P = A1 i( A 2 × A 3 ) . An entire perfect lattice, i.e., one free of defects, can be reconstructed by stacking the primitive unit cells. In three spatial dimensions, crystals are assigned to one of fourteen distinct kinds of Bravais lattices. Symmetry considerations enable each of the fourteen Bravais lattices to be grouped into one of seven crystal systems. Similarities among different Bravais lattices comprising a single crystal system become evident upon examination of conventional unit cells. Conventional unit cells may be nonprimitive, i.e., they may contain more than one lattice point per cell; equivalently, the volume of a conventional cell is an integer number of primitive cell volumes. Conventional unit cells may,
68
3 Kinematics of Crystalline Solids
like primitive unit cells, be translated to exactly reconstruct an entire (infinite) lattice. The location of a corner point of any conventional unit cell in the lattice can be described by a linear combination of three vectors labeled a, b, and c. In a nonprimitive cell, however, all points of the Bravais lattice are not necessarily included in the set of corner points. For example, lattice points may be centered inside a conventional cell or on its faces, in addition to those points at the corners. Conventional lattice parameters consist of the magnitudes of conventional cell vectors: a = (aia)1/ 2 , b = (bib)1/ 2 , c = (cic)1/ 2 , (3.2) and of the three angles describing their relative orientations, denoted by α, β, and γ. Vectors a, b, and c and angles α, β, and γ are shown in Fig. 3.1 for a conventional unit cell. The volume of the conventional unit cell is ΩC = ai(b × c) = N Ω P , with N the number of lattice points per conventional unit cell.
Fig. 3.1 Conventional lattice parameters
In a crystal structure, each Bravais lattice point, i.e., the lattice point of each primitive unit cell, is decorated by an identical basis of one or more atoms. A basis is a set of one or more atoms with the same stoichiometry (i.e., chemical composition) as the overall material. When each lattice point corresponds to a single atom, the basis is said to be monatomic. On the other hand, a polyatomic basis consists of multiple atoms per point on the Bravais lattice. These atoms may or may not be of different elemental species. The simplest example of a polyatomic structure is a diatomic crystal, which consists of two monatomic lattices, one differing from the other by a uniform translation (Ericksen 1970). The position of each atom k of a polyatomic basis relative to the Bravais lattice point centered at the origin of a local coordinate system for each primitive unit cell is specified by the basis vector for atom k, labeled as R (0k ) . Since each atom is located within its own unit cell, its basis vector can be expressed in terms of fractional components of the primitive Bravais lattice vectors: 3
R ( 0k ) = ∑ mi Ai = m1 A1 + m 2 A 2 + m3 A 3 , ( 0 ≤ mi < 1 ), i =1
(3.3)
3.1 Crystals and Lattice Deformation
69
The position of any atom (e.g., any one atom’s nuclear coordinates) in Cartesian space in a perfect lattice is then the sum of the basis vector for that atom and the Bravais lattice vector for that atom’s primitive unit cell: 3
R ( lk ) = R ( 0k ) + R ( l ) = ∑ (mi + l i ) Ai ,
(3.4)
i =1
where R (lk ) denotes the global position of atom k within primitive unit cell l. When the structure is monatomic, basis vector R ( 0k ) is redundant and the location of the an atom is simply R (l ) , since the number of primitive unit cells and number of atoms then coincide. A measure of atomic volume in an infinitely extended lattice is Ω0 = Ω P / K = ΩC /( NK ) , where K is the number of atoms in the basis (i.e., the number of atoms per primitive cell). The total number of atoms per conventional unit cell is the product NK. Note that a polyatomic basis—and hence a primitive unit cell in a polyatomic structure—can contain more than one formula unit. The fourteen Bravais lattices are organized into crystal systems in Table 3.1 and Fig. 3.2, following the notational scheme of Rohrer (2001). Conventional unit cells are drawn in Fig. 3.2; those labeled with a P are also primitive (one lattice point per cell), while those labeled with an I, F, or C are not. Specifically, I refers to an inner centered lattice, F refers to a face centered lattice, and C refers to a lattice with a lattice point centered only on faces normal to conventional unit cell vector c. Lattice points of primitive unit cells are represented by spheres in Fig. 3.2; when the basis is monatomic, each sphere corresponds to (the nucleus of) an atom in the crystal. Table 3.1 Crystal systems and symmetry restrictions (Rohrer 2001) Crystal system Cubic Tetragonal Orthorhombic Monoclinic Triclinic Rhombohedral Hexagonal
Number of lattices 3 2 4 2 1 1 1
Conventional cell parameters a = b = c ; α = β = γ = 90° a = b ≠c; a ≠ b ≠ c; a ≠ b ≠ c; a ≠ b ≠ c; a =b=c;
α = β = γ = 90° α = β = γ = 90° α = γ = 90° ≠ β α≠β≠γ
α = β = γ < 120°, ≠ 90° a = b ≠ c ; α = β = 90°, γ = 120°
70
3 Kinematics of Crystalline Solids
Fig. 3.2 Bravais lattices
3.1 Crystals and Lattice Deformation
71
When a monatomic basis is added to each site of a lattice, a common crystal structure is often recovered. For example, a cubic P lattice with a monatomic basis forms a simple cubic (SC) structure. A cubic I lattice with a monatomic basis produces a body centered cubic (BCC) structure. A cubic F lattice with a monatomic basis produces a face centered cubic (FCC) structure. On the other hand, the hexagonal close packed (HCP) structure consists of a basis of two atoms at each point on a hexagonal Bravais lattice, the first located, for example, at a corner point of the conventional cell and the second in a plane spaced midway between two faces of the cell perpendicular to c (i.e., perpendicular to the caxis). Table 3.2 lists several geometric parameters for each of the SC, BCC, FCC, and HCP structures wherein all atoms are of identical size (e.g., of the same species). Radius r is used to denote the size of an atom in the structure when that atom is idealized as a rigid sphere in exact (i.e., nonpenetrating) contact with its nearest neighbors. The coordination number is the number of nearest neighbors, i.e., the number of sphere centers located at a distance 2r from the center of a given sphere. The packing factor P is defined as the volume occupied by the spheres contained in a conventional unit cell divided by the total volume of the conventional unit cell: P = 4π r 3 NK / (3ΩC ) = 4π r 3 K / (3Ω P )=4π r 3 / (3Ω0 ) . It follows that the volume of each hard sphere is the product of the atomic volume and the packing factor. Often the c/a ratio in a material classified as HCP differs from the ideal value of 1.633 because of effects of atomic bonding. Table 3.2 Geometric characteristics of several common crystal structures
Structure SC BCC FCC HCP
Atomic radius r r = a/2 r = 3a / 4 r = 2a / 4 r = a / 2 = 0.306c
No. atoms NK 1 2 4 2
Coord. no. 6 8 12 12
Packing P 0.52 0.68 0.74 0.74
Locations of atoms within a unit cell are written, in terms of fractional components of primitive Bravais lattice vectors in (3.4), by the notational convention (m1 , m 2 , m3 ) ⇔ ( x, y , z ) . Directions in the unit cell are written in terms of coefficients of the primitive Bravais lattice vectors by the notational convention [l 1l 2l 3 ] ⇔ [uvw] , with overbars denoting negative values. Families of directions, i.e., directions that are indistinguishable because of particular values of the indices [uvw] and symmetry of the lattice,
are denoted by uvw . Planes are denoted by Miller indices (hkl ) , with
72
3 Kinematics of Crystalline Solids
families of crystallographically equivalent planes denoted by {hkl} . Miller indices of planes are reciprocals of intercepts of directional axes intersecting those planes. A zero is assigned to a Miller index when a plane does not intersect that axis. In cubic crystals, Miller indices of a plane are the same as the indices of the direction normal to that plane. It is common for one to denote corner points on the lattice of conventional unit cells by the position vector R (c) = c1a + c 2 b + c3c , ( c1 , c 2 , c 3 ∈ ). (3.5) In terms of conventional unit cell vectors, directions in Miller’s notation then obey the correspondence [c1c 2 c3 ] ⇔ [uvw] . Miller indices of planes in the conventional unit cell description are defined as reciprocals of intercepts of the [c1c 2 c3 ] directions. For nonprimitive unit cells, R (c) does not describe every point on the Bravais lattice. MillerBravais indices of type [uvtw] are conventionally used for directions in hexagonal crystal systems, subject to the constraint u + v + t = 0 . This fourindex notational scheme is also often used for crystals of the rhombohedral or trigonal system (Kronberg 1957). Indices u, v, and t correspond to directions in the basal plane spaced 120° apart, while w corresponds to translation along the caxis. Families of directions are denoted by uvtw . Individual planes and families of planes are denoted, respectively, by the notation (hkil ) and {hkil} , with the constraint h + k + i = 0 . The reciprocal lattice concept is often useful, especially for study of lattice vibrations. Coordinates of a point in the primitive reciprocal lattice are R ′hkl (l ) = hA1 + kA 2 + lA 3 , ( h, k , l ∈ ), (3.6) where reciprocal primitive Bravais lattice vectors are expressed in terms of primitive Bravais lattice vectors by (Maradudin et al. 1971) 2π ( A 2 × A 3 ) 2π ( A3 × A1 ) 2π ( A1 × A 2 ) , A2 = , A3 = , (3.7) A1 = ΩP ΩP ΩP or more succinctly in Cartesian space, AAi Ω P = π eABC eijk ABj AkC , (3.8) where upper case indices denote components of each vector referred to the reference coordinate system and lower case indices are placeholders. Notice that the primitive Bravais lattice vectors are contravariant (indices in upper positions), while the primitive reciprocal lattice vectors are covariant (indices in lower positions). The primitive lattice vectors and their reciprocals satisfy the orthogonality conditions
3.1 Crystals and Lattice Deformation
A i , A j , = 2πδ .ij ,
73
(3.9)
and locations of points on the primitive Bravais lattice and the primitive reciprocal lattice satisfy (3.10) R (l ), R ′hkl (l ) = 2π ( l 1h + l 2 k + l 3l ) = 2π n , ( n ∈ ).
For each set of parallel planes in the primitive Bravais lattice specified by Miller indices h, k, and l, there exists a point on the primitive reciprocal lattice. The direction of the reciprocal vector R ′hkl (l ) of (3.6) is normal to the plane with Miller indices (hkl ) . The factor of 2π in (3.7) is omitted in alternative definitions by some authors (Born and Huang 1954). Conventional unit cell vectors can also be used to define a reciprocal lattice. In that case, analogs of (3.6), (3.7), and (3.10) are R ′hkl (c) = ha′ + kb′ + lc′ , ( h, k , l ∈ ), (3.11) 2π (b × c) 2π (c × a) 2π (a × b) a′ = , b′ = , c′ = ; (3.12) ΩC ΩC ΩC R (c), R ′hkl (c) = 2π ( c1h + c 2 k + c3l ) = 2π n , ( n ∈ ).
(3.13)
The direction of R ′hkl (c) of (3.11) is normal to the plane with Miller indices (hkl ) , though some values of h, k, and l will produce reciprocal lattice vectors that do not correspond to points on the reciprocal lattice, and not all points on the primitive reciprocal lattice are described by R ′hkl (c) . For cubic, tetragonal, and orthorhombic Bravais lattices, conventional unit cell vectors and their reciprocals are parallel: a′ a , b′ b , and c′ c . Table 3.3 lists formulae for metric tensors, unit cell volumes, and interplanar spacings for each of the seven crystal systems, all in terms of conventional unit cell parameters. The metric tensor G in Table 3.3 is used to determine lengths of vectors R (c ) in (3.5): R ( c ) i R (c ) =
3
∑cG c
i , j =1
i
ij
j
,
(3.14)
where components of the metric are denoted by Gij = G ji and satisfy ⎡ G11 G12 ⎢G ⎢ 21 G22 ⎢⎣G31 G32
G13 ⎤ ⎡ aia aib aic ⎤ G23 ⎥⎥ = ⎢⎢bia bib bic ⎥⎥ . G33 ⎥⎦ ⎢⎣ cia cib cic ⎥⎦
(3.15)
74
3 Kinematics of Crystalline Solids
Table 3.3 Metrics, unit cell volumes, and interplanar spacings (Rohrer 2001) System
Cubic
Tetragonal
Orthorhombic
Monoclinic
Triclinic
Metric G
Unit cell volume Ω C
Spacing 1/ d hkl 2
0⎤ ⎥ 0⎥ 2⎥ a ⎦
a3
h2 + k 2 + l 2 a2
a 2c
h2 + k 2 l 2 + 2 a2 c
abc
h2 k 2 l 2 + + a 2 b2 c2
abc sin β
1 ⎡ h2 ⎢ + sin 2 β ⎣ a 2
⎡a 2 ⎢ ⎢0 ⎢0 ⎣
0 a2
⎡a 2 ⎢ ⎢0 ⎢0 ⎣
0 a2 0
0⎤ ⎥ 0⎥ 2⎥ c ⎦
⎡a 2 ⎢ ⎢0 ⎢0 ⎣
0 b2 0
0⎤ ⎥ 0⎥ 2⎥ c ⎦
0
⎡ a2 0 ⎢ b2 ⎢ 0 ⎢ ac cos β 0 ⎣
ac cos β ⎤ ⎥ 0 ⎥ c2 ⎥⎦
⎡ a2 ab cos γ ac cos β ⎤ ⎢ ⎥ b2 bc cos α ⎥ ⎢ab cos γ 2 ⎢ ac cos β bc cos α ⎥ c ⎣ ⎦
k 2 sin 2 β l 2 + 2 b2 c 2hl cos β ⎤ − ac ⎥⎦
1 ⎡ h 2 b 2 c2 sin 2 α ΩC 2 ⎣
abc ⎡⎣1 − cos 2 α − cos 2 β − cos 2 γ + 2 cos α cos β cos γ ]
1/ 2
+k 2 a 2 c2 sin 2 β +l 2 a 2 b 2 sin 2 γ +2hkabc2 × (cos α cos β − cos γ ) +2kla 2 bc × (cos β cos γ − cos α) +2lhab2 c × (cos γ cos α − cos β) ]
Rhombohedral
⎡ a2 a 2 cos α a 2 cos α ⎤ ⎢ 2 ⎥ a2 a 2 cos α ⎥ ⎢a cos α 2 ⎢a 2 cos α a 2 cos α ⎥ a ⎣ ⎦
a 3 ⎣⎡1 − 3cos 2 α − 1/ 2
+ 2 cos3 α ⎤⎦
a4 × ΩC 2 ⎡⎣(h 2 + k 2 + l 2 ) × sin 2 α +2(hk + kl + hl ) ×(cos 2 α − cos α) ⎤⎦
Hexagonal
⎡ a2 −a 2 / 2 0 ⎤ ⎢ 2 ⎥ − a / 2 a2 0⎥ ⎢ 2 ⎢ 0 0 c ⎥⎦ ⎣
3 2 a c 2
4(h 2 + hk + k 2 ) l 2 + 2 3a 2 c
3.1 Crystals and Lattice Deformation
75
The conventional unit cell volume is ΩC = ai(b × c) , as noted following (3.2). Magnitudes of reciprocal lattice vectors R ′hkl (c) are inversely proportional to separation distances between planes (hkl ) , written as d hkl : ⎡ a′ia′ a′ib′ a′ic′ ⎤ ⎡ h ⎤ R ′hkl iR ′hkl 1 1 = = 2 [ hkl ] ⎢⎢b′ia′ b′ib′ b′ic′⎥⎥ ⎢⎢ k ⎥⎥ , (3.16) d hkl 2 4π 2 4π ⎢⎣ c′ia′ c′ib′ c′ic′ ⎥⎦ ⎢⎣ l ⎥⎦ where the 3×3 matrix in (3.16) is the metric of the reciprocal space. Analogous formulae apply when primitive Bravais lattice vectors of the primitive unit cell are used. For a more comprehensive treatment of crystallographic terminology, structures of various crystalline substances, and lattice orientation characterization, the reader is referred to books dealing with topics in crystallography (Schmid and Boas 1950; Wyckoff 1963; Buerger 1965; Senechal 1990; Rohrer 2001) and texture analysis (Bunge 1982; Randle and Engler 2000). 3.1.2 The CauchyBorn Hypothesis
The CauchyBorn hypothesis (Born and Huang 1954), also often called the CauchyBorn rule or CauchyBorn approximation, states that under a homogeneous deformation, the primitive Bravais lattice vectors of a crystal in the reference configuration, Ai ∈ TB0 of (3.1), deform in an affine manner via a 3 × 3 matrix F to spatial vectors ai ∈ TB : ai = FA i , aia = F.Aa AiA , (i = 1, 2,3) . (3.17) Accordingly, coordinates of points on the Bravais lattice in (3.1) are updated under a homogeneous deformation as 3
3
i =1
i =1
r(l ) = ∑ l i ai = ∑ l i FA i = FR (l ) .
(3.18)
In an elastic body, F of (3.17) is often identified with the deformation gradient of (2.112). By the polar decomposition (2.149), stretch and rotation of the primitive Bravais lattice vectors are included in (3.17). Stretch U or V induces a change in the lattice parameters of the primitive unit cell, and thus a (probable) change in interatomic forces sustained by the crystal. A homogeneous deformation for a crystal with a polyatomic basis, in the sense of Born and Huang (1954), is r ( lk ) = q ( 0k ) + FR ( lk ) . (3.19)
76
3 Kinematics of Crystalline Solids
Vector q(0k ) represents a uniform displacement (translation) of all atoms of type k, as might occur for example when an ionic crystal becomes polarized under an electric field. Substituting from (3.4) and (3.18), r ( lk ) = q ( 0k ) + FR ( lk ) = q ( 0k ) + F ⎡⎣ R ( 0k ) + R ( l ) ⎤⎦ 3
3
i =1
i =1
= ∑ ∆mi ( 0k ) ai + FR ( 0k ) + r ( l ) = ∑ [∆mi ( 0k ) + mi + l i ]ai
(3.20)
= F ⎣⎡ F −1q ( 0k ) + R ( 0k ) + R ( l ) ⎦⎤ = F ⎣⎡Q ( 0k ) + R ( lk )⎦⎤ , with ∆mi (0k ) a scalar translation parameter for all atoms of type k in the crystal structure. In the context of coincident Cartesian coordinate systems in reference and deformed crystal lattices, Born and Huang (1954) call q(0k ) the internal displacement and F − 10 the external strain. The former, i.e., the inner displacement or internal displacement, can arise in complex crystal structures subject to external deformation F via relative displacements of sublattices, even in the absence of electric polarization (Ericksen 1970; Wallace 1972; Cousins 1978). A rotationally invariant version of inner displacement of basis atom k is represented by vector Q(0k ) = F −1q (k0 ) (Tadmor et al. 1999). Vector Q(0k ) generally depends on the applied (i.e., farfield) deformation; in practice the set of particular values of all internal displacement vectors k for a given applied deformation gradient F tend to minimize the energy of the crystal. Inner displacements also arise in the context of optical vibrations (Chen and Lee 2005). Rigid translation of the entire structure is omitted in (3.19) and (3.20); such motion can be included by adding a translation vector, independent of position, to r (lk ) . Now consider the reciprocal lattice. Assuming that in the deformed configuration, primitive Bravais lattice vectors and their reciprocals a j remain orthogonal: ai , a j = aai a aj = 2πδ .ij , (3.21) reciprocal Bravais lattice vectors transform like dual vectors according to ai = F −* Ai , aai = F −1.aA AAi , (i = 1, 2,3) . (3.22) A point on the primitive reciprocal lattice has spatial coordinates ′ (l ) = ha1 + ka 2 + la3 = F −* R ′hkl (l ) , rhkl (3.23) from which it follows that, analogously to (3.10), in a homogeneously deformed primitive Bravais lattice, ′ (l ) = 2π ( l1h + l 2 k + l 3l ) = 2π n , ( n ∈ ). r (l ), rhkl (3.24)
3.1 Crystals and Lattice Deformation
77
Quantities introduced in (3.17)(3.20) are depicted in Fig. 3.3 for primitive unit cell l of a triclinic Bravais lattice with diatomic basis ( k = 0,1 ). In Fig. 3.3, parallel Cartesian coordinate systems are used for reference ( X A ) and deformed ( x a ) configurations of the crystal structure, and ξ is a vector directed from the origin of the reference frame to the origin of the spatial frame.
Fig. 3.3 Homogeneous deformation in the sense of Born and Huang (1954)
In an elastic crystal, the following notation is used in this book to indicate that the local deformation gradient of the material in the continuum sense, F of (2.112), and the local deformation of the lattice F L , coincide: F(X ,t ) = F L (X ,t ) , (3.25) where dependence on position and time indicates that the deformation gradient need not be homogeneous in space or static in time. For example, with this notation (3.18) becomes 3
3
i =1
i =1
r (l ) = ∑ l i a i = ∑ l i F L A i = F L R (l ) .
(3.26)
On the other hand, as will be demonstrated later in Chapter 3, when a crystalline substance deforms inelastically, for example via dislocation plasticity, F and F L do not coincide. In the remainder of this book, F L is referred to as the lattice deformation. Substituting (3.25) into (3.17)(3.20), F L (X ,t ) stretches and rotates the primitive Bravais lattice vectors and ba
78
3 Kinematics of Crystalline Solids
sis vectors of a primitive unit cell or a collection of primitive unit cells assigned to “material point” X. When a differential volume element in the reference configuration dV ( X ) is assumed to consist of multiple primitive cells, then lattice vectors and basis vectors of each cell of that volume element deform homogeneously according to the value of F L (X ,t ) for that material point centered at X. Lattice vectors and basis vectors of unit cells assigned to different locations X deform heterogeneously when F L (X ,t ) varies with position. Further exposition on the CauchyBorn rule, its extensions, and related applications in crystal mechanics and multiscale modeling can be found in a number of references (Ericksen 1970, 1984, 2005, 2008; Zanzotto 1992, 1996; Tadmor et al. 1996, 1999; Knap and Ortiz 2001; Arroyo and Belytschko 2002; Chung and Namburu 2003; Curtin and Miller 2003; Sunyk and Steinmann 2003; Clayton and Chung 2006). 3.1.3 Elastic Deformation and Thermal Deformation
In crystalline solids, lattice deformations may be introduced by forces of purely mechanical origin (e.g., elasticity due to bond stretching1), temperature changes, and applied electromagnetic fields (e.g., piezoelectricity, electrostriction, piezomagnetism, or magnetostriction). Consider a crystalline solid subjected to mechanical loading and temperature variations. With increasing temperature, the equilibrium spacing of atomic nuclei tends to increase as a result of increasing vibrational energy that accompanies local thermal oscillations. This leads to thermal expansion, specifically stretching of the Bravais lattice vectors and basis vectors, even when no mechanical forces are applied from external agents. Thorough discussion of atomic and quantum mechanical origins of thermal expansion in solids can be found in treatments of condensed matter physics (Slater 1939; Brillouin 1964). Cooling will usually lead to the opposite effect, i.e., thermal contraction. However, at a given pressure, contraction with increasing temperature is not impossible (Hanson et al. 1974), even in the absence of phase transformations. In continuum thermoelasticity, contributions from temperature change and those from mechanical stress are not usually explicitly delineated within lattice deformation F L (Thurston 1974; Marsden and Hughes 1983; Rosakis et al. 2000), as described in de1 At the scale of electronic and nuclear resolution, even “mechanical” forces associated with atomic bonds result from Coulombtype electrostatic interactions among electrons and nuclei. Dynamic exchange forces associated with phonons, photons, protons, and electrons can also contribute to mechanical stiffness (Gilman 2003).
3.1 Crystals and Lattice Deformation
79
tail later in Chapter 5. However, in some cases it is useful to make the distinction (Stojanovitch 1969; Lu and Pister 1975; Imam and Johnson 1998; Clayton 2005a, b, 2006a) F L = F E F θ , F La. A = F E .aB F θ .BA , (3.27) where F E is associated with mechanical loading and possible rigid body rotation of the lattice, and where F θ is attributed to stressfree thermal expansion or contraction. For simplicity, both indices of the thermal deformation are referred to the reference coordinate system in (3.27). Introducing the absolute temperature θ and its material time derivative θ , a rate expression for thermal deformation can be written as2 (3.28) F θ F θ −1 = α Tθ , F θ.CA F θ −1.CB = α T .ABθ , where α T ( X , t ) is a secondorder tensor of thermal expansion that is generally symmetric (Nye 1957), since thermal expansion does not induce any spin of the lattice. The coefficient of thermal expansion α T can be treated as a polar tensor of rank two in the terminology of Thurston (1974), with independent components listed for crystal classes in Table A.4 of Appendix A. For cubic crystals and isotropic materials, thermal deformation is isotropic: α T = α T 10 , where αT is a scalar coefficient of thermal expansion. In that case, and when thermal expansion/contraction is the only deformation mode, (3.29) J θ J θ −1 = d ( −1 G det Fθ ) / dt G det Fθ −1 = dv / dv = 3α T θ ,
(
)(
)
with dv = J θ dV the volume of a material element after thermal deformation. In the geometrically linear theory (i.e., the small deformation theory of Section 2.5.3), an analog of (3.27) is ε L = ε E + ε θ = ε E + α T ∆θ , (3.30) where ε L is a symmetric total lattice strain, ε E is the mechanical elastic strain, the coefficient of thermal expansion α T is symmetric with the same meaning as in (3.28), and ∆θ is the change in temperature from a reference state at which thermal strain εθ vanishes.
Kinematic prescription (3.28) is not unique. Another reasonable possibility consistent with (3.30) is F θ .AB ( X , t ) = δ .BA + α T .AB ∆θ , where α T has a similar meaning and ∆θ is the change in temperature from an undeformed reference state. 2
80
3 Kinematics of Crystalline Solids
3.2 Multiplicative Inelasticity Finite deformation inelasticity theory is predicated on the existence of a relaxed configuration of the body free of internal and/or external forces at some length scale of observation. For example, a crystal may attain a globally unloaded state upon removal of traction along its external surfaces. However, a heterogeneous crystalline solid supporting residual stresses such as those arising from defects may simultaneously be globally relaxed and locally or microscopically stressed. In such cases the body must be cut into small pieces, or in geometric terminology mapped to an anholonomic state as defined in Section 2.8, in order to relieve such internal stress fields. From an atomic perspective, it may be physically impossible to define a configuration of a defective lattice free of all internal forces without breaking stretched or distorted bonds in the vicinity of defects. 3.2.1 Background
The concept of a locally relaxed, generally anholonomic state was posited by Eckart (1948), who introduced a metric tensor describing lengths of material elements in such an unloaded state and used this construction in a thermodynamic theory of anelasticity. Kondo (1949) invoked the concept of a metric with nonvanishing curvature tensor to describe plastic yielding. Bilby et al. (1955) forwarded the idea of using a generally incompatible, twopoint lattice deformation map to describe the Bravais lattice vectors of a crystal containing dislocations, purely from the perspective of crystallography and independent of the notion of stress relaxation or removal of mechanical forces. The multiplicative decomposition of the deformation gradient (formally introduced in (3.31)) is perhaps the most popular postulate used to describe the deformation kinematics of elasticplastic crystals subjected to large strains and rotations. Bilby et al. (1957) are often credited with first explicitly proposing the twoterm multiplicative decomposition for elasticplastic crystals, using the terminology “shape deformation”, “lattice deformation”, and “dislocation deformation” to describe the total deformation gradient, its elastic part, and its plastic or latticepreserving (i.e., “lattice invariant” in their terminology) part, respectively (see also Bilby and Smith (1956)). Kroner (1960) posited a similar model for kinematics of elasticplastic crystals. Teodosiu (1967a, 1968) developed a generalized continuum theory of elastoplasticity incorporating a multiplicative decomposition of the deformation gradient into a product of two incompati
3.2 Multiplicative Inelasticity
81
ble maps, generalizing Toupin’s theory of hyperelastic materials of grade two (Toupin 1964). Fox (1968), Lardner (1969), and Teodosiu (1970) postulated continuum theories of finite deformation plasticity from consideration of dynamics of mobile dislocation lines or loops. The abovementioned studies were generally conducted in the context of continuously distributed dislocations, whereby internal stress fields resulting from defects were of primary interest in practical applications of the theory involving solutions of boundary value problems (Kroner and Seeger 1959; Teodosiu 1967b; Willis 1967). The multiplicative decomposition emerged somewhat independently in the context of macroscopic continuum plasticity theory of engineering and structural mechanics, a context wherein evolution of mechanical stresses and macroscopic state variables of solid bodies, usually polycrystalline, subjected to large external forces is of primary concern. Acknowledging prior work by Eckart, Bilby, and Sedov, Lee and Liu (1967) introduced a twoterm multiplicative decomposition to describe deformations of metals subjected to large pressures occurring in impact problems. This early study of kinematics and thermodynamics was extended to general deformation histories by Lee (1969), popularizing the multiplicative decomposition among the engineering mechanics community. Shock waves in elasticplastic solids were studied using finite strain approaches by Lee and Wierzbicki (1967), Foltz and Grace (1969), and Germain and Lee (1973). In decades since, the multiplicative decomposition is the standard prescription used for the nonlinear kinematics of crystal plasticity (Rice 1971; Teodosiu and Sidoroff 1976; Asaro 1983), wherein the generally anisotropic mechanical response of single crystals is modeled via consideration of dislocation glide along preferred directions in the crystal lattice on a number of discrete slip planes. The decomposition has also become popular for describing macroscopic plasticity (Kratochvil 1971; Simo and Ortiz 1985; Bammann and Aifantis 1987; Moran et al. 1990; Scheidler and Wright 2001; Wright 2002), whereby at each volume element centered at a point X within a body, the response of a large number of grains, typically metallic, is modeled in an average sense. Issues regarding material symmetries and multiple, evolving natural configurations have been addressed by Rajagopal and Srinivasa (1998) and Epstein and Elzanowski (2007). 3.2.2 The Multiplicative Decomposition
The twoterm multiplicative decomposition of the deformation gradient for elasticplastic solids is written F = F L F P , F.Aa = F La.α F Pα.A , (3.31)
82
3 Kinematics of Crystalline Solids
where F L is the lattice deformation first mentioned in (3.25) and F P is the plastic deformation. Accompanying (3.31) are the following requirements: det F P > 0 , det F L > 0 , and inverses F L −1 and F P −1 exist that satisfy F La.α F L −1α.b = δ .ba , F L −1α.a F La.β = δ.αβ , (3.32) F P −1.Aα F Pα.B = δ . BA , F Pα. A F P −1.Aβ = δ .αβ . Decomposition (3.31) suggests existence of an additional configuration of the body, called the intermediate configuration and labeled B in Fig. 3.3, such that globally, F P :TB0 → TB and F L :TB → TB . Although F L and
F P are referred to as elastic and plastic “deformation gradients”, these two tangent maps need not be integrable; i.e., elastic and plastic deformation gradients and their inverses need not be true gradients of vector fields taken with respect to any spatial or material coordinates.
Fig. 3.4 Tangent maps and configurations
Plastic deformation F P as defined here is engendered by cumulative motions of defects that are said to be latticepreserving or lattice invariant
3.2 Multiplicative Inelasticity
83
(Bilby et al. 1957), in other words phenomena that do not significantly alter the crystal structure from the length scale of resolution of the external observer. In crystalline solids, F P is most often attributed to collective motion of dislocations when the solid is observed at a length scale coarse enough that local microscopic stretch and rotation fields associated with individual defects may be neglected. Such typically omitted fields may encompass, for example, stretch and rotation of primitive Bravais lattice vectors and basis vectors of the crystal structure in the immediate vicinity of cores of individual dislocation lines. From an atomistic perspective, reference configuration B0 can be related to intermediate configuration B as follows (Clayton and Chung 2006) when mapping F P represents the cumulative deformation of the material, but not the lattice, attributed to dislocation glide through a local volume element of a crystalline body. Consider a fixed control volume (i.e., a Eulerian representation centered at spatial point x) and initially containing of a large number of atoms, for example the number of atoms occupying a basis decorating at least 103 primitive unit cells. Once atoms have passed through this control volume as a result of dislocation glide, B0 and B appear identical in terms of atomic coordinates if no defects remain within the volume element and if elastic fields of dislocations that have passed through this element are excluded in configuration B . Yet deformation of the material will have taken place because of dislocation motion. For a purely plastic process with F L = 1 , new atoms would enter the control volume in identical locations as the old, to replace those that exited due to plastic flow, and the mass of material contained within the control volume element would be conserved. The concept is illustrated in Fig. 3.5 for a cubic lattice, in which atoms that exit the volume are denoted by filled circles, and those that enter the cell by open circles, with the underlying material undergoing pure “plastic” shear. Boundaries of the fixed control volume through which atoms may pass are denoted by dashed lines, and boundaries of a Lagrangian material element (e.g., centered at X) and associated with a fixed set of atoms are denoted by solid lines. The mass of the Lagrangian element remains fixed because dislocation glide does not involve mass transport, and the volume occupied by the Lagrangian element remains fixed because dislocation glide is isochoric. The magnitude of the plastic shear shown in Fig. 3.5, upon prescription of parallel rectangular coordinate frames in each configuration, is F P1.2 = (2 / 5)(b / d ) .
84
3 Kinematics of Crystalline Solids
Fig. 3.5 Plastic deformation from atomic perspective
The lattice deformation F L in turn encompasses all remaining physical mechanisms that do affect the underlying crystal structure. This includes rigid rotations of the entire solid body, as well as local rotations and local stretching of the Bravais lattice vectors associated with mechanical stresses and thermal expansion or contraction. The majority of theoretical developments in finite deformation inelasticity seem to address plasticity in crystalline metals, perhaps since historically, inelastic behavior of these materials has garnered utmost interest in structural mechanics and manufacturing sciences. However, multiplicative kinematics of (3.31) have been extended to describe deformations of a variety of nonmetallic (poly)crystalline solids, whereby F L accounts for stretch and rotation of some aspect of the microstructure of the particular material under consideration. Decomposition (3.31), or variations of it, has been used to describe finite inelasticity in brittle crystalline solids such as geological materials (Krajcinovic 1996; Barton and Wenk 2007; Clayton 2010a) and dielectric and piezoelectric ceramics (Clayton 2009a, b, 2010b), granular media such as soils (Ortiz and Pandolfi 2004), heterogeneous structural solids such as concrete (Clayton 2008), energetic crystals (Barton et al. 2009), and crystalline and semicrystalline polymers (Shepherd et al. 2006). Multiplicative kinematics have also been used to model amorphous solids (Anand and Gurtin 2003). However, rotation of the microstructure within an element of isotropic amorphous material, relative to the total rotation of that element, is of presumably less consequence to the mechanical response than would be expected for an anisotropic crystalline solid wherein the directions of the lattice vectors of the structure dictate thermomechanical properties such as elastic constants and thermal expansion coefficients. The polar decomposition (2.149) applied to each of F L and F P yields F = V L R L R P UP = R L UL V P R P , (3.33) L where V is the left lattice stretch, R L is the lattice rotation that includes rigid body rotations of the entire body, R P is the plastic rotation, and U P
3.2 Multiplicative Inelasticity
85
is the right plastic stretch. In the second of (3.33), U L is the right lattice stretch and V P is the left plastic stretch. In many interpretations, deformation mapping F L , rather than being linked explicitly to the deformation of Bravais lattice vectors and basis vectors (Born and Huang 1954), is defined in terms of a reversible or elastic unloading from a stressed configuration to an unstressed configuration. In other words, unloading via V L −1 maps the solid body from the stressed current configuration to an unloaded intermediate configuration. In continuum plasticity models, depending on the constitutive formulation used to specify the evolution of plastic deformation, this operation may leave the unloaded state indeterminate by a rotation, as discussed more in Section 3.2.7. Reverse decompositions, i.e., F = F P F L , have also been forwarded (Bilby et al. 1957; Clifton 1972; Lubarda 1999). While such a reverse decomposition may pose no formal difficulties from a mathematical standpoint, an apparent benefit of original decomposition (3.31) is that unloading occurs most realistically from the actual (current) configuration of the body, as opposed to unloading from a stressed intermediate configuration as in the case of the reverse decomposition. In the former case, from (3.33) and for a compatible stretch field V L , an entire stressed crystalline body could conceivably be unloaded to an intermediate configuration in one piece, simply by removal of traction along its external boundaries. However, since F L and F P and their inverses are generally not compatible or integrable, configuration B is generally anholonomic or nonholonomic. As demonstrated later in Section 3.3.2, the mathematical anholonomicity conditions imply, physically, the presence of geometrically necessary dislocations in the crystal, induced by the incompatible nature of F L −1 or F P . These defects differ from those dislocations that pass through the crystal in a relatively homogenous manner, contributing to the compatible or integrable part of F P . From the perspective of local mechanical unloading, the incompatibility of V L −1 implies that the body must be cut into pieces to relieve internal stresses associated with heterogeneous local elastic deformations (Eckart 1948). As depicted in Fig. 3.4, tangent mappings from the material body B to the reference or current configuration, κ t :T B → TBt (t ≥ 0) , need not be integrable, implying that χ t (t ≥ 0) of Fig. 2.2 could be an anholonomic function of reference coordinates (t = 0) or spatial coordinates (t > 0) , and that natural configuration B , like B , could be anholonomic. Incompatibility of κ 0 implies that the defect content differs between the actual mate
86
3 Kinematics of Crystalline Solids
rial body B and its initial representation in Euclidean space B0 . For example, it often becomes convenient to treat the body at t = 0 as a perfect crystal. If the real body B contains defects, then κ 0 may be used to remove the effects of defects from the mathematical representation of the body at t = 0 , or viceversa. While some authors simultaneously introduce both κ t and F P (Teodosiu 1970; Rice 1971; Tigoiu and Soos 1990; Le and Stumpf 1996a; Clayton et al. 2004a) in an independent manner similar to Fig. 3.4 (with possible differences in notation), in practice the distinction between reference configuration B0 and natural configuration B is usually omitted. In this way, contributions of all defects towards the deformation gradient kinematics are embedded in F L and F P , even though the crystal may be imperfect at t = 0 . For the most part, henceforward in this book, this practical viewpoint will be used, meaning that mappings κ 0 and κ t and material manifold B will not be considered explicitly. Returning now to decomposition (3.31), lattice and plastic deformations are written fully in component form as, respectively, β F L = F La.α g a ⊗ gα , F P = F P .A gβ ⊗ G A , (3.34) where the anholonomic basis vectors gα and their reciprocals gα obey
gα ,g β = δ .αβ .
(3.35)
Unless noted otherwise, it is assumed that F L ( X , t ) and F P ( X , t ) are at least twice differentiable with respect to reference coordinates X A , and that their inverses F L −1 ( x, t ) and F P −1 ( x, t ) are at least twice differentiable with respect to spatial coordinates x a . Applying definition (2.206) for anholonomic partial differentiation with respect to lattice and plastic deformations, along with definition (2.112) and identity (3.31), leads to ∂ ( . ) P −1 A ∂ ( . ) a P −1 A ∂ ( . ) La F .α = x., A F .α = F .α . (3.36) ∂ α ( . ) = ( . ) ,α = ∂X A ∂x a ∂x a Partial coordinate derivatives of anholonomic basis vectors and reciprocal basis vectors, following verbatim from postulates (2.210), are ..α χ .. χ (3.37) gα, β = −Γ βχ g , gα , β = Γ βα gχ ,
where from (2.208), either of the following definitions, not necessarily equivalent or exclusive3, can be used for connection coefficients on B :
3 Symbols in (3.38) and (3.39) are derived in Appendix D (Section D.4) via use of convected anholonomic basis vectors. Others are possible (e.g., (3.51) later).
3.2 Multiplicative Inelasticity G
..α Γ βχ = F P −1B. β F P −1C. χ F Pα. A Γ G
= F P −1B. β F P −1C. χ F Pα. A Γ
.. A BC
+ F P −1C. χ , β F Pα.C
.. A BC
− F P −1B. β F P −1C. χ F Pα.C , B ,
87
(3.38)
g
..α Γ βχ = F Lb. β F Lc. χ F L −1α.a Γ ..bca + F Lc. χ , β F L −1α.c
=F
Lb .β
F
Lc .χ
F
L −1α .a
g
Γ −F .. a bc
Lb .β
F
Lc .χ
F
L −1α .c , b
(3.39) . G
Since LeviCivita connections with Christoffel symbols Γ
..A BC
g
and Γ
..a bc
are
.. χ
symmetric, Tβα = 0 in (2.209) and the skew part of the second of (3.37) is .. χ g[α , β ] = Γ [..βαχ ] g χ = −κ βα gχ ,
(3.40)
where anholonomic objects (2.207) obtained from (3.38) and (3.39) are identical4: κ ..βχα = F La.β F Lb. χ F L −1α.[b,a] = F P −1 A.β F P −1B. χ F Pα.[ B ,A] . (3.41) On the other hand, only when B is holonomic, meaning that coordinates xα exist that are continuously (twice) differentiable functions of x a or X A , are all of the following conditions satisfied simultaneously: ∂xα ∂xα ∂ F L −1α.a = a , F Pα.A = , gα = α , κ ..βχα = 0 , g[α ,β ] = 0 . (3.42) A ∂x ∂x ∂X
3.2.3 The Metric Tensor in the Intermediate Configuration
A generic metric tensor on anholonomic space B is expressed as g = gαβ gα ⊗ g β and is positive definite and symmetric by definition. Components of this metric tensor satisfy gαβ = gα ig β = g β i gα = g βα ,
(3.43)
where i denotes the scalar product of vectors akin to (2.9). The scalar product of two arbitrary vectors a ,b ∈ TB then becomes aib = aα gα ib β g β = aα b β gα ig β = aα gαβ b β .
4
(3.44)
A different anholonomic object defined as κ ..βχα = F L a.β F Lb. χ F L −1α.[ a ,b] was used
in previous work (Clayton et al. 2004a), but implications regarding the vanishing or nonvanishing of the RiemannChristoffel curvature tensor introduced in anholonomic coordinates in (36) of that paper remain the same.
88
3 Kinematics of Crystalline Solids
Components of metric tensor g are also used to lower indices in the conventional manner, for example a contravariant vector is converted to a dual or covariant vector via aα = gαβ a β . (3.45) Transposes (see e.g., (2.125) and (2.126)) of lattice and plastic deformations are given, respectively, by F LT α.a = g αβ F Lb.β g ab = g αβ F L* .bβ gba , (3.46)
F PT .Aα = gαβ F P .Bβ G AB = gαβ F P*.Bβ G BA , where g
αβ
(3.47) −1
are components of the inverse intermediate metric g . Jaco
bian invariants of deformation mappings F L and F P providing relationships among volume elements dv ⊂ B , dV ⊂ B , and dV ⊂ B0 also depend upon g , as in (2.141), (2.142), (2.223), and (2.224). Letting z a , z α , and Z A denote coordinates referred to local Cartesian axes associated with material elements in B, B , and B0 , respectively, Jacobian determinants are found as (Teodosiu 1967b; Clayton et al. 2004a) ⎛ ∂z a ∂x β ⎞ dv = det ⎜ b F Lb.β α ⎟ = det( F Lb.β ) det( g ab ) / det( gαβ ) , (3.48) JL = ∂z ⎠ dV ⎝ ∂x ⎛ ∂z α ∂X B ⎞ dV = det ⎜ β F P .βB = det( F P .βB ) det( gαβ ) / det(GAB ) , (3.49) A ⎟ ∂ ∂ dV x Z ⎝ ⎠ where det( gαβ ) = [det(∂zα / ∂x β )]2 has been used. Introducing permutation JP =
tensors ε αβχ = geαβχ and ε αβχ = −1 geαβχ and setting g = det( gαβ ) ,
1 1 J L = ε αβχ ε abc F La.α F Lb. β F Lc. χ , J P = ε αβχ ε ABC F Pα. A F P β.B F P χ.C , (3.50) 6 6 a form consistent with (2.224). Since F L and F P are required to have positive determinants as mentioned following (3.31), and since g is positive definite, J L > 0 , J P > 0 , and dV > 0 . Conceivable choices for metric tensor g and basis vectors gα in (3.43) are now discussed (Clayton et al. 2004a). The simplest and most prevalent option from the literature is (Teodosiu 1967a, b; Simo and Ortiz 1985) ..δ ..δ g = δ αβ eα ⊗ e β , eα , A = eα , β F P.βA = Γ βα eδ F P.βA = 0 , Γ βα =0. (3.51) where intermediate metric tensor components are gαβ = δαβ . Intermediate Kronecker delta symbols δαβ = 1∀α = β and δαβ = 0∀α ≠ β , and gα = eα
3.2 Multiplicative Inelasticity
89
are constant orthonormal (Cartesian) basis vectors5. The last of (3.51) applies in the present context, instead of alternatives (3.38) or (3.39). Prescription (3.51) indicates that contravariant vectors defined on B are referred to a single global Cartesian frame, or equivalently, a parallel Cartesian frame attached to each local relaxed volume dV ⊂ B . This implies either that (i) B is a Euclidean space or that (ii) the gα are not actually tangent to any coordinate lines inscribed on base manifold B since such coordinates do not exist, but instead correspond to some external reference frame. Statement (i) is ruled out in general by a nonvanishing anholonomic object in (3.40), physically indicating the presence of crystal defects such as dislocations that render B anholonomic. This leaves statement (ii): indices of vectors on TB are not referred to the actual tangent spaces of any deformed material manifold but are instead referred to the fixed external Cartesian frame. The intermediate metric δ αβ (or equivalently, the external Cartesian frame) is introduced somewhat artificially as an additional modeling assumption, accompanying introduction of kinematic variables F L and F P . Along similar lines, Simo (1988) posited an intermediate configuration metric gαβ = δ A.α G ABδ B.β , implying a Cartesian metric for B when B0 is described using Cartesian coordinates, and requiring introduction of the twopoint Kronecker delta (i.e., shifter) δ .Aα . Several alternatives have been proposed (Moran et al. 1990; Maugin 1994, 1995; Le and Stumpf 1998; Miehe 1998; Clayton et al. 2004a) that, in contrast to (3.51), do not embed nonEuclidean space B within a global Cartesian space equipped with a Euclidean metric tensor δ αβ . It should be noted, however, that (3.48) and (3.49), wherein Cartesian zα are assigned to each volume element dV ⊂ B , do rely on the pointwise assumption that transformation formulae to intermediate Cartesian coordinates z α are available. One such alternative is specification of an alternative kind of intermediate metric tensor g′ as the covariant lattice deformation tensor CL (Moran et al. 1990; Maugin 1994; Clayton et al. 2004a): 5
Conditions gαβ = gα ig β = δαβ can still be imposed without requiring gα ( X )
remain parallel for all X. For example, basis vectors gα ( X ) of unit length could ..δ differ by a (jump in) rotation at distinct points; conditions gα , A = 0 and Γ βα =0
would not hold everywhere in that case, and the second of (3.51) would not apply.
90
3 Kinematics of Crystalline Solids L ′ ( x, t ) = C αβ gαβ = F La.α g ab F Lb.β = F La.α g a i F Lb.β g b = gα′ ig ′β ,
(3.52)
implying that an alternative set of anholonomic basis vectors can be defined by gα′ ( x, t ) = F La.α ( x, t )g a ( x) . (3.53) Requiring that g ′α ,g′β = δ .αβ leads to the corresponding reciprocal vectors g′α ( x, t ) = F L −1α.a ( x, t )g a ( x) . Since components F
La .α
(3.54)
L
and C αβ evolve with time along with changes in
crystal structure (i.e., stretch and/or rotation of Bravais lattice vectors), basis vectors in (3.53) and (3.54) represent a kind of convected coordinates. Most generally, gα′ ≠ gα meaning that basis vectors in (3.43) and (3.52) 6
do not coincide . However, letting gα ( x) = g.aα g a , the first of (3.34) becomes F L ( x, t ) = F L.aα g a ⊗ gα (3.55) = F L.aα g a ⊗ g.αb g b = g.αa ( x )gα′ ( x, t ) ⊗ g a ( x ), and is analogous to the convected coordinate representation of the deformation gradient (2.128) when coordinate systems are chosen such that the shifter is g .aα = gα ,g a = δ .aα . Maugin (1995) suggested an analogous form
of (3.52) as a metric tensor on possibly anholonomic material manifold B . The covariant plastic deformation CP can likewise be employed as a metric on B (Miehe 1998): P ′ ( X , t ) = C αβ gαβ = F P −1 A.α GAB F P −1.Bβ (3.56) = F P −1 A.α G A i F P −1.Bβ G B = gα′ ig′β , implying anholonomic basis vectors obey gα′ ( X , t ) = F P −1 A.α ( X , t )G A ( X ) . In (3.52) and (3.56), respectively, the standard Euclidean relations g ab = g a ig b and GAB = G A iG B are used.
In a previous paper (Clayton et al. 2004a), the same notation was used for gα′ and gα in different sections, an ambiguity that could cause confusion. In that paper, the intended implication was that anholonomic basis vectors used in definitions of elastic and plastic deformation gradients differ from those used in metric tensors (3.52) and (3.56). Otherwise, setting g′α = gα in (3.34) results, recur6
sively, in null lattice deformation: F L = F L.aα g a ⊗ F L −1α.b g b = δ .ba g a ⊗ g b .
3.2 Multiplicative Inelasticity
91
The gα′ in (3.52) or (3.56) are not tangent to any global coordinate curves xα since such coordinates are precluded by the anholonomicity of B , but they do exist in a onetoone manner with the set g a ( x) and the map F La.α ( x, t ) or with the set G A ( X ) and the map F P −1.Aα ( X , t ) , respectively. In this sense, CL and CP are welldefined, but timedependent, geometric quantities referred to space B , in contrast to δ αβ of (3.51) that cannot be derived from components of lattice or plastic deformation maps and holonomic basis vectors on B0 or B . Regardless, basis vectors gα and their reciprocals gα must always be prescribed by the modeler in the context of (3.34) so that components of F L.aα and F Pα. A can be defined. In later parts of this book (e.g., (3.64), (3.65), and thermodynamic treatments in Chapters 6, 8, and 9), to avoid unnecessary complexity, timeindependent (extrinsic) basis vectors gα with metric tensor components gαβ = gα i g β are prescribed. Practical sets of timeindependent intermediate {basis vectors, metric tensor components} include, but are not limited to, the following: { gα = eα , gαβ = δ αβ } , { gα = δ .αA G A , gαβ = δ .Aα GABδ B.β } , and { gα = δ .αa g a , gαβ = δ a.α g abδ b.β } . Twopoint Kronecker delta symbols obey δ .Aα = 1 for α = A and δ .Aα = 0 for α ≠ A , where α , A = 1, 2,3 . Analogous relationships apply for Kronecker delta symbols δ a.α . Consider now the rank four RiemannChristoffel curvature tensor formed from connection coefficients (3.38) on anholonomic space B , with components found from (2.212): g
...α ...a Rβχδ = F Lb.β F Lc. χ F L d.δ F L −1α.a R bcd
ε ..α = 2∂[ β Γ χ..α]δ + 2Γ [..βαε Γ χ..ε]δ + 2κ [..βχ ]Γ εδ .
(3.57)
g
...a Recall that R bcd = 0 identically since B is a Euclidean space; hence,
...α Rβχδ = 0 regardless of the vanishing of F L −1α.[a ,b] . However, integrability ...α ..ε conditions Rβχδ = 0 and κ βχ = 0 hold identically and simultaneously when
F L −1.αa (x, t ) = x.,αa , i.e., when B is homeomorphic to Euclidean space B and xα = xα ( x, t ) are holonomic coordinates with respect to which partial coordinate differentiation can be defined as usual. Under such conditions, the anholonomic object in the first of (3.41) reduces to
92
3 Kinematics of Crystalline Solids
κ ..βχα = x a., β xb., χ xα.,[ba ] = 0 . When F La.α (x, t ) = x.,aα , the curvature tensor formed from the symmetric Riemannian connection with metric coefficients L L L C L −1αδ (C βδ , χ + C χδ , β − C βχ ,δ ) / 2 vanishes identically since this curvature tensor is the pullback by a continuously differentiable motion xα , to the g
...a formed from components of the intermediate configuration, of R bcd Euclidean spatial metric g ab , analogously to the situation discussed in Section 2.8.2. Similar statements apply for (3.39): the RiemannChristoffel curvature tensor from coefficients in (3.39) vanishes identically; anholonomic object following the second equality of (3.41) vanishes if
G
F Pα. A ( X , t ) = x.,αA , giving κ ..βχα = X A., β X B., χ xα.,[ BA] = 0 ; and since R ...A BCD = 0 , the RiemannChristoffel curvature tensor constructed from coefficients P P P Pα α C P −1αδ (C βδ , χ + C χδ , β − C βχ ,δ ) / 2 vanishes identically when F . A = x., A . 3.2.4 Kinematics, Rates, and Kinematic Approximations
Taking the material time derivative7 of (3.31), applying the product rule, and postmultiplying the result by the inverse of deformation gradient F leads to L = FF −1 = F L F L −1 + F L F P F P −1F L −1 = LL + F L LP F L −1 , (3.58) where L is the spatial velocity gradient of (2.176) with mixedvariant components La.b = v;ab . The quantity LL = F L F L −1 is a mixedvariant tensor with components referred to spatial configuration B and is called the lattice velocity gradient, and LP = F P F P −1 is a mixedvariant tensor referred to intermediate configuration B and is called the plastic velocity gradient. Using (3.33), the following definitions are introduced, where subscripts skew and symm refer to antisymmetric and symmetric parts of covariant ingredients in (3.58), i.e., skew and symmetric parts of Lab = g ac F. Ac F.b−1 A : FF −1 = W L + DL + F L ( W P + DP ) F L −1 ,
W L = ( LL )
skew
= R L R LT + ( R L U L U L −1R LT )
DL = ( LL )
7
symm
From Section 2.6.1, F .PAα ( X , t ) =
= ( R L UL U
∂F Pα. A ∂t
L −1
R LT )
symm
skew
,
(3.60)
,
and F .Lαa ( x, t ) = X
(3.59)
(3.61)
∂F La.α ∂t
+ F L.aα ;b vb . x
3.2 Multiplicative Inelasticity
W P = ( LP )
skew
= R P R PT + ( R P U P U P −1R PT )
DP = ( LP )
= ( R P U P U P −1R PT )
symm
symm
skew
,
93
(3.62)
.
(3.63)
Above, W L is the lattice spin, DL is the lattice deformation rate, W P is the plastic spin, and DP is the plastic deformation rate. Another strain rate relation analogous to (2.186) that will become useful later is L EL = F L* DL F L , Eαβ = F L .aα DabL F Lb.β ,
(3.64) L
where lattice strain referred to the intermediate configuration, E , is defined analogously to the right CauchyGreen strain introduced in (2.156): 1 1 L L EL = (CL − g) , Eαβ = (Cαβ − gαβ ) = E(Lαβ ) , (3.65) 2 2 L with symmetric lattice deformation tensor C αβ = F La.α g ab F Lb.β as first introduced in (3.52). Conditions gαβ = 0 are assumed in (3.64). Analogously to (2.114), lattice and plastic deformation gradients provide firstorder approximations of the length and direction of a differential line element dx ∈ TB mapped to the intermediate configuration. For example, for the plastic deformation: dxα = xα ( X ′) − xα ( X ) 1 = F Pα. A dX A + F Pα. A:B dX A dX B (3.66) X X 2! 1 + F Pα. A:BC dX A dX B dX C + ..., X 3! A A A where dX = X ′ − X is the infinitesimal vector between two reference points X and X ′ , and the total covariant derivative, similar to (2.116), is G
F Pα. A:B = F Pα. A, B − Γ
..C BA
..α F Pα.C + Γ βχ F P .χA F P .βB ,
(3.67)
..α where Γ βχ are connection coefficients associated with basis vectors on B .
Noting dX A dX B = dX B dX A , skew terms F Pα.[ A:B] , while generally nonzero, will not contribute to (3.66). Similarly for the lattice deformation, dxα = xα ( x′) − xα ( x) 1 L −1α F .a:b dx a dxb x 2! 1 + F L −1α.a:bc dx a dxb dx c + ..., x 3!
= F L −1α.a dx a + x
(3.68)
94
3 Kinematics of Crystalline Solids
where dx a = x′a − x a is the infinitesimal vector between two spatial points x and x′ , and analogously to (2.116), the total covariant derivative g
F L −1α.a:b = F L −1α.a ,b − Γ
..c ba
..α F L −1α.c + Γ βχ F L −1.χa F L −1.βb .
(3.69)
Skew terms F L −1α.[a:b] are nonzero when F L −1 is not integrable, but will not affect the quadratic term in (3.68). From (3.66) and (3.68), to first order, dx = F P dX = F L −1dx , dxα = F Pα. A dX A = F L −1α.a dx a . (3.70) Because lattice and plastic deformation gradients are generally not integrable, dx is generally not an exact differential and is sometimes referred to as a Pfaffian (Stojanovitch 1969). The role of the lattice deformation and lattice strain tensors in the context of firstorder deformed lengths of differential line elements is thus
dx = F L dx =
dx, CL dx ,
dxidx − dxidx = 2 dx, EL dx .
(3.71) (3.72)
Two approximations are commonly encountered pertaining to relative magnitudes of lattice and plastic deformations. The first is the small lattice strain assumption: V L = 1 + ε L , ε L = (ε L : ε L )1/ 2 1 , (3.73) where terms of the symmetric tensor g acε Lc.b are small relative to unity as indicated. This assumption is often deemed relevant for ductile metallic crystals that deform by dislocation motion before large elastic strains are attained (Bammann and Johnson 1987). The contribution of the plastic velocity gradient in (3.58) is then often approximated as F L LP F L −1 = (1 + ε L )R L LP R LT (1 + ε L )−1 ≈ R L LP R LT . (3.74) Neither W L nor DL necessarily vanishes according to approximation (3.73), since lattice rotation and stretch rates may still be arbitrarily large. The second approximation is the small deformation assumption, as introduced in Section 2.5.3, with rate kinematics listed in (2.191). The analog of (3.31) in the geometrically linear theory is F ≈ 1 + β L + β P , F. Aa ≈ g abδ .cA ( gbc + β bcL + β bcP ) , (3.75) where the lattice displacement gradient is denoted by β L and the plastic displacement gradient is denoted by β P , such that an additive decomposition of the total covariant displacement gradient applies: (3.76) ua ;b = β abL + β abP .
3.2 Multiplicative Inelasticity
95
Displacement gradients in (3.76) are sometimes called distortions (Mura 1982). Like the lattice and plastic deformation maps of (3.31), the lattice and plastic distortions of (3.75) are generally incompatible, i.e. β aL[b ,c] ≠ 0 , β aP[b ,c] ≠ 0 , (3.77) even though the total distortion, since it is a true covariant derivative of a continuous displacement field, must satisfy ua ,[bc] = ua;[bc] = 0 . Distortions are separated into skew rotational and symmetric strain tensors as follows: ε ab = u( a ;b ) = ε abL + ε abP , Ωab = u[a ,b] = ΩabL + ΩabP ; (3.78)
β abL = ε abL + ΩabL , ε abL = β (Lab ) , ΩabL = β[Lab] ;
(3.79)
β abP = ε abP + ΩabP , ε abP = β (Pab ) , ΩabP = β[Pab] .
(3.80)
Upon taking time derivatives of (3.78)(3.80), linearized lattice and plastic rotation and strain rates are obtained: (3.81) ua ;b = ΩabL + ε abL + ΩabP + ε abP ;
Ω abL = β[Lab] ≈ WabL , ε abL = β (Lab ) ≈ DabL ;
(3.82)
Ω =β
(3.83)
P ab
P [ ab]
≈W , ε = β P ab
P ab
P ( ab )
≈D ; P ab
where approximations in (3.82) and (3.83) hold when both lattice and plastic distortions are small so that, in Cartesian coordinates, W L ≈ R L , DL ≈ U L , W P ≈ R P , DP ≈ U P , R L ≈ 1 + Ω L , U L ≈ 1 + ε L , R P ≈ 1 + Ω P , U P ≈ 1 + ε P , and F = F L F P ≈ 1 + Ω L + ε L + Ω P + ε P , consistent with (3.75). 3.2.5 Dislocation Plasticity
Dislocations are elementary line defects in crystalline solids, and their motion is often the primary source of plastic deformation in crystalline materials. Dislocations are characterized by a tangent line and Burgers vector (Burgers 1939; Frank 1951). The dimensionless tangent line ξ ( X , t ) ∈ TB , which may be straight or curved, indicates the direction of the defect and is typically assigned a unit magnitude. At any point along the dislocation line L, the tangent line defines the normal to a plane perpendicular to the defect. Dislocation lines may intersect with other defects or free surfaces of the crystal, and may form loops, but do not end abruptly within an otherwise perfect crystal lattice. The Burgers vector b( X , t ) ∈ TB (dimensions of length) indicates the magnitude and direction of the closure failure, or step in the lattice, induced by mapping a closed loop in a defective crystal to a perfect crystal or viceversa (Hirth and Lothe 1982; Teodosiu
96
3 Kinematics of Crystalline Solids
1982; Hull and Bacon 1984). The corresponding closed loop is called a Burgers circuit. Straight dislocation lines may be of screw, edge, or mixed character. Screw dislocations have parallel tangent lines and Burgers vectors, while edge dislocations have perpendicular tangent lines and Burgers vectors. Mixed dislocations are neither parallel nor perpendicular to their tangent lines. Partial dislocations, dislocation loops, helical dislocations, disclinations (Frank 1958; De Wit 1973), and other more general defect structures such as Somigliana dislocations (Eshelby 1956; Asaro 1976) are also observed in some kinds of crystals. Dislocationlike defects can also emerge in geologic solids (Eshelby 1973) and porous media (Pan 1991). The magnitude of the Burgers vector of a full (complete) dislocation is equal to the distance between two atoms in a perfect crystal in the direction of the atomic displacement, e.g., a lattice parameter in a primitive unit cell. In contrast, the magnitude of a partial dislocation may differ from the distance between two atoms in a perfect crystal. The movement of an isolated partial dislocation through a region of crystal leaves behind a stacking fault in that region, but a perfect lattice can be restored by collective movement of partial dislocations (e.g., leading and trailing partial dislocations separated by a stacking fault). Mechanical twinning can also involve coordinated motion of partial dislocations (Christian and Mahajan 1995; Bernstein and Tadmor 2004). Full dislocations tend to dissociate into partial dislocations if the energy of the full dislocation exceeds the sum of energies of the partial dislocations (including their core and elastic interaction energies) and the energy of the stacking fault between the partials (Hull and Bacon 1984).
3.2 Multiplicative Inelasticity
97
Fig. 3.6 Burgers circuit surrounding single edge dislocation in cubic crystal
The Burgers circuit concept is illustrated explicitly in Fig. 3.6 for a cubic crystal containing a single edge dislocation. The tangent line of the dislocation is directed in a positive sense out of the plane of the figure, i.e., ξ G 3 . Two kinds of Burgers circuits are typically considered. In the first, shown in Fig. 3.6(a), a closed circuit about the defect line in the current configuration on the right, beginning and ending at point x0 , is mapped to an open circuit by counting the same steps in a perfect lattice in the intermediate configuration on the left. By convention the circuit is taken in a clockwise sense from an observer viewing in the direction of the tangent line, or equivalently, via the usual righthand rule of vector calculus. In the perfect lattice, the circuit does not close. The Burgers vector in Fig. 3.6(a) is then the vector b = x0 − x directed from the point x at the end of the circuit to the point x0 at the start. In the second kind of Burgers circuit shown in Fig. 3.6(b), a closed circuit about the defect line in the in
98
3 Kinematics of Crystalline Solids
termediate configuration on the left, beginning and ending at point x0 , is mapped to an open circuit by counting the same steps in the defective lattice in the current configuration on the right. By convention, the circuit is again taken in the righthanded sense. In the dislocated lattice, the circuit does not close. The Burgers vector in Fig. 3.6(b) is b = x − x0 , directed from point x0 at the start of the circuit to point x at the end. Kondo (1963) calls the circuit of Fig. 3.6(a) “Frank’s disturbance”, and the circuit of 3.6(b) “Read’s disturbance”. Using a nonlinear elastic model based on Volterra’s construction (Volterra 1907) in which F = F L , Teodosiu (1982) demonstrates that after neglecting terms on the order of the square of b , the two Burgers vectors are related by b( X , t ) = F L ( X , t )b( X , t ) , b a = F La.α b α . (3.84) Willis (1967) and Teodosiu (1982) note that b does not depend upon the choice of starting point x0 , while b does depend upon choice of starting point x0 as a result of the local lattice deformation F L ( X = x0 ) . Different conventions exist for algebraic signs of Burgers vectors and tangent lines and for the positive sense of circulation about the Burgers circuit; those used here follow from Willis (1967) and Hull and Bacon (1984). Volterratype elasticity models of discrete dislocation lines and disclination lines are provided in Appendix C, Section C.1. Linear elastic models of dislocation and disclination loops are discussed in Section C.2 of Appendix C. The Burgers circuit concept can be used for dislocation lines of screw and mixed character, and can be extended to describe the total summed Burgers vector of a number of dislocation lines passing through an oriented surface in the crystal enclosed by a circuit. Mobile dislocations engender plastic stretch and rotation. When acted on by external forces, dislocations tend to move directions normal to their tangent vectors. For a single mobile dislocation, the direction of movement of atoms is in the same direction as the Burgers vector. For an edge dislocation, atoms move in the same direction as the motion (i.e., the velocity) of the dislocation line and perpendicular to the tangent vector. For a screw dislocation, atoms move parallel to the tangent line but normal to the velocity vector of the dislocation line. Dislocation motion may proceed by glide or climb. Dislocations that undergo glide are often labeled glissile, while dislocations that are immobile, or locked in place due to constraints imposed by other defects for example, are often labeled sessile. Glide is dislocation motion whereby the movement of the dislocation is restricted to a surface called the glide plane that contains both the Burgers vector and tangent line. Glide is often referred to as slip, and terms glide
3.2 Multiplicative Inelasticity
99
and slip are used interchangeably in this book. Dislocation glide is an example of conservative motion, meaning that the local volume of the crystal is unaffected by the process. The surface on which the dislocation glides is called the slip plane or glide plane. Unlike edge dislocations, screw dislocations do not exhibit a mathematically unique slip plane since the latter’s Burgers vector and tangent line are parallel. However, in crystals a finite set of discrete planes upon which screw dislocations usually move is often dictated by the crystal structure. Cross slip, or a change of slip planes, may occur during the course of plastic deformation as screw dislocations seek paths of least resistance (Hirth and Lothe 1982). The usual thermodynamic driving force for dislocation glide is a shear stress component acting on the slip plane in the direction of the Burgers vector, as demonstrated in explicit detail in Sections 6.2 and 6.3 of Chapter 6. The combination of Burgers vector or its orientation—with the latter denoting the slip direction—and the slip plane constitute a slip system. Typical slip systems for cubic and hexagonal crystal structures are illustrated in Fig. 3.7 and are listed in Table 3.4. The direction of the Burgers vector is always parallel to the slip direction. Dislocations tend to move in closepacked directions on closepacked planes, though exceptions exist among certain kinds of materials. Depending on the particular material (e.g., element or compound), its purity, and environmental conditions (e.g., temperature), the most common slip system, or that with the least resistance to slip, may vary. More extensive lists of slip systems in different materials—including for example secondary systems activated at higher temperatures as well as slip systems for other crystal structures not listed in Table 3.4—can be found in books by Schmid and Boas (1950) and Hirth and Lothe (1982). Exceptions to the slip systems in Fig. 3.7 are common among polyatomic structures and nonmetals, especially ionic solids wherein electrostatic interactions (e.g., charge imbalances) among ions strongly affect defect structures and mobilities (Sprackling 1976). For example, primary slip systems in alkali halide crystals (rock salt structure) are of type 110 {1 10} . Pure ionic crystals are often very ductile, with high dislocation mobilities (Gilman 2003). For hexagonal structures, direction X 1 is often chosen parallel to 2 1 10 rather than 12 10 as shown in Fig. 3.7, though in the present context the choice is arbitrary.
100
3 Kinematics of Crystalline Solids
Fig. 3.7 Slip systems for cubic and hexagonal crystal structures
3.2 Multiplicative Inelasticity
101
Table 3.4 Slip systems and Burgers vectors for several crystal structures Structure
SC
Primary slip systems 100 {010}
Burgers vector, magnitude 100 , a
BCC
111 {1 10} , 111 {112} , 111 {123}
1/ 2 111 , a 3 / 2
FCC
110 {1 11}
1/ 2 110 , a 2 / 2
HCP
1120 {0001} , 1120 {1 100} , 1120 {1 101}
1/ 3 1120 , a
Climb occurs when an edge dislocation moves out of the surface containing its Burgers vector and tangent line, and is a generally nonconservative motion since the volume of the solid is changed locally by the process. Dislocation climb often involves the motion of point defects such as vacancies or interstitials to accommodate volume changes. Conservative climb of prismatic dislocation loops is possible, however (Hull and Bacon 1984). In engineering metals deformed at low temperatures or high strain rates, glide tends to prevail over climb, since diffusion mechanisms often require higher temperatures and longer time scales to contribute substantially to inelastic deformation. The intermediate configuration B in Fig. 3.4 differs from B0 due to the influence of cumulative motion of lattice defects through the volume element under consideration and perturbations of atomic positions resulting from defects contained within that volume. Defects considered in what follows next in the present Section are displacement discontinuities tangential to an internal surface (i.e., crystallographic plane) in the material. These include gliding straight or curved dislocation lines, dislocation loops, and partial dislocations. Configuration B is considered free of external traction and free of all internal stresses, and hence is fictitious in the sense that local stress fields of defects are absent. In the context of continuum elasticity, one could view the volume element in configuration B at the stage of the Volterra process (see e.g., Appendix C) after discontinuities in displacement have been introduced, but prior to the stage of resealing the body and introduction of selfstresses (Eshelby 1956; Toupin and Rivlin 1960; De Wit 1973; Mura 1982). For a crystal containing a single dislocation, a singular plastic deformation map can be defined in the vicinity of the defect in Cartesian coordinates as follows (Teodosiu 1970; Rice 1971; Ortiz and Repetto 1999): F P = 1 + b ⊗ M δ ( X, M ) χ , (3.85) where 1 is the unit tensor, M is the normal to the slip plane in the reference configuration, δ (.) is Dirac’s delta function, and χ is a characteristic
102
3 Kinematics of Crystalline Solids
function equal to unity at reference coordinates X on a slipped surface (i.e., surface of singularity) Σ and zero elsewhere. The coordinate system for X is chosen with its origin in the slip plane so that along the surface of displacement discontinuity X A M A = 0 . Plastic deformation (3.85) is singular on Σ and vanishes elsewhere. A dislocation density tensor corresponding to the discrete dislocation line described by (3.85) is (Teodosiu 1970) α 0 = b ⊗ ξ 0δ ( L ) , (3.86) where ξ 0 ∈ TB0 is tangent to dislocation line L in the reference configuration. From (3.85) and (3.86), X−
b = − ∫ + F P dX = ∫ α 0 NdA . X
(3.87)
A
Line integration in the first of (3.87) takes place between limiting coordinates immediately above ( X + ) and below ( X − ) the slipped singular surface Σ ( X + ≅ X − ). Area integration in the second of (3.87) proceeds over the union of oriented reference elements NdA pierced once by the dislocation line, and ξ 0 , N dA = dA by definition at the intersection of L and A. Now consider the average plastic deformation gradient for a volume element containing multiple dislocation lines. If the dislocations are introduced into the volume element sequentially, a logical nonsingular extension of (3.85) is n
(
)
n
(
)
F P = ∏ 1 + V −1 ∫ b ⊗ Mδ ( Σ ) dV = ∏ 1 + V −1b ⊗ MΣ , m =1
m =1
(3.88)
where the product is taken over n dislocations, each with a possibly different Burgers vector b and constant normal vector M to an assumed flat slipped surface (i.e., glide plane) of reference area Σ . The volume of the element in the reference configuration is denoted by V. Note that (3.88) depends upon the sequence in which each dislocation is introduced ( m = 1 corresponds to the most recently generated dislocation) and hence cannot be used effectively if dislocations with different Burgers vectors or slip surfaces are generated simultaneously. Since b ⊥ M from the definition of a glide plane, (3.88) consists of a product of simple shears and volume is conserved, i.e., J P = 1 . For a collection of i = 1, 2,... j straight dislocation line populations of density ρ 0i = lim( Li / V ) = dLi / dV ≥ 0 , Burgers V →0
i
i 0
vector b , reference tangent ξ , and plane normal M i , dislocation density in (3.86) and Burgers integral in (3.87) can be extended as j
α 0 = V −1 ∫ b ⊗ ξ 0 dL = ∑ ρ0i bi ⊗ ξ i0 , L
i =1
(3.89)
3.2 Multiplicative Inelasticity
103
j
B = ∫ α 0 , N dA = ∫ ∑ ρ0i bi ξ i0 , NdA ,
(3.90)
A i =1
A
with B the summed projection of all local Burgers vectors of dislocation lines passing through area A contributing to the closure failure of the Burgers circuit corresponding to the boundary of A. Line integration in (3.89) proceeds over all dislocations of total length L. The second equation in (3.90) pertains to j discrete dislocation populations with the same tangent line and local Burgers vector for each value of i. Using a version of Nanson’s formula (2.227), a differential Burgers vector from (3.90) can be defined completely in terms of quantities in the intermediate configuration as follows: j
dBα = α 0α A N A dA = ∑ ρ 0i b iα ξ 0i A N A dA i =1
j
j
i =1
i =1
(3.91)
= ∑ ρ 0i b iα ξ 0i A J P −1 F P.βA nβ da = ∑ ρ i b iα ξ i β nβ da = α αβ nβ da, where the intermediate tangent line, number of dislocations per unit volume in B , and intermediate dislocation density tensor, are respectively, ξ iα = F Pα. Aξ0i A , ρ i J P = ρ0i , α αβ = J P −1α 0α A F P.βA , (3.92) and the differential area element maps from reference to intermediate configuration according to (see e.g., Cermelli and Gurtin (2001) and (2.227)) nα da = J P F P −1.Aα N A dA . (3.93) Integration of (3.91) then gives Bα = ∫ dBα = ∫ α αβ nβ da . (3.94) a
a
From the first of (3.92), the intermediate tangent vector with components ξ iα need not be of unit length when ξ 0i Aξ 0i A = 1 . As discussed in Section 3.2.3, the assignment of Cartesian basis vectors to intermediate configuration B is not always necessary, and is not geometrically natural when the plastic deformation gradient is not integrable. However, (3.87), (3.89), (3.90), and (3.94) are integrals of vector fields whose components are referred to TB . Thus, these integral equations are valid globally, in component form, only when basis vectors gα are independent of position within the domains of integration, e.g., when these basis vectors are spatially constant, but not necessarily orthonormal. On the other hand, following Toupin (1956), such integrals can be evaluated numerically at a single point X by parallel transporting the integrands to that point using a shifter g.αA ( X , X ′) that is assumed to exist everywhere within the domain of integration. For example, (3.94) evaluated at X is
104
3 Kinematics of Crystalline Solids
B A ( X ) = ∫ g.αA ( X , X ′)dBα ( X ′) = ∫ g.αA ( X , X ′)α αβ ( X ′) nβ ( X ′) da . (3.95) a
a
The resultant can then be transported back to any point X ′ via B β ( X ′) = g.βA ( X ′, X ) B A ( X ) = g.βA ( X ′, X ) ∫ g.αA ( X , X ′)dBα ( X ′) .
(3.96)
a
Steps such as (3.95) and (3.96) are implied henceforth in this book for integrals of vector and tensor fields when curvilinear coordinates are involved, and are usually not written out explicitly. A more general definition of the average plastic deformation of a volume element accounts for the time history of generation and motion of mobile defects within it, in which case F P is defined as the solution of the following differential equation with initial conditions: (3.97) F P = LP F P , F P = 1. t =0
The average plastic velocity gradient LP in (3.58) for the volume element, including both rate of deformation and spin, is dictated by the flux ς of mobile dislocations (Mura 1968; Lardner 1969; Lempriere 1970; Zbib et al. 2002; Clayton et al. 2006): LP = ς : ε , LPα.β = ς αχδ ε χδβ ; (3.98) j
ς = V −1 ∫ bi ⊗ ξ i ⊗ vi dL = ∑ ρ i bi ⊗ ξ i ⊗ v i ,
(3.99)
i =1
L
where ε χδβ are covariant permutation tensor components first introduced in (2.224) and ξ i = ξ α i / ξ α i gα and vi are respectively the normalized unit tangent vector and velocity of dislocation population i, all referred to configuration B . Since dislocation segments exhibit perpendicular velocities and tangent lines, ξ i ⊥ v i and bi ⊥ (ξ i × vi ) , J P = J P trLP = 0 and J P = 1 , meaning volume is conserved by (3.98). Relation (3.99) applies for straight dislocation lines; similar expressions can be formulated for dislocation loops (Kroupa 1962; Teodosiu 1970), or curved lines can simply be discretized into a number of smaller straight segments (Zbib et al. 1998; Arsenlis and Parks 2002; Zbib and De La Rubia 2002). Introducing the notation ξ i × v i = mi v i , v i = vi  , b i = b i si , and b i = bi  , where m i is the unit normal to the slip plane in configuration B and si is a unit vector in the direction of slip, the plastic velocity gradient of (3.98) reduces to the form most often encountered in crystal plasticity (Rice 1971; Asaro 1983): (3.100) LP = ∑ ρ i b i v i s i ⊗ mi = ∑ γ i s i ⊗ m i , γ i = ρ i b i v i . i
i
3.2 Multiplicative Inelasticity
105
The definition of the slip rate γ i in (3.100) is often attributed to Orowan (1934, 1940), Polanyi (1934), and Taylor (1934). Implicit in (3.100) is the idea that only mobile dislocations ( v i ≠ 0 ) contribute. Since the product γ i s i ⊗ m i does not depend upon the orientation of the Burgers vector relative to the tangent line, summation in (3.100) can be reduced to a sum over i slip systems identified by slip direction and slip plane normal, and γ i then accounts for all mobile screw, edge, partial, and mixed dislocations, including loops, with an effective scalar Burgers vector b i , average velocity v i , and total mobile density ρ i on that slip system. Since s i ⊥ m i , again J P = J P trLP = 0 and J P = 1 . Thus the scalar line densities are equal in intermediate and reference configurations: ρ i = ρ 0i . Some authors switch positions of the tangent line and dislocation velocity in the dislocation flux; in that case, (3.100) can still be recovered by defining the slip plane as the negative of that used in (3.100), i.e., m i = ( v i × ξ i ) / v i . Regardless, the contravariant index of LP always corresponds to the direction of atomic motion, i.e., the Burgers vector or the slip direction. Kinematic relationship (3.100) is considered again in Section 3.2.6 dealing with continuum crystal plasticity theory. Consideration of kinematics of mechanical twinning resulting from the collective motion of partial dislocations and atomic shuffling (Christian and Mahajan 1995; Zanzotto 1996; Clayton 2009a, 2010c) is deferred until Chapter 8.
Fig. 3.8 Plastic shear resulting from a single edge dislocation
Slip rate equation γ i = ρ i b i v i in (3.100) can be derived intuitively as follows. First consider the glide of a single edge dislocation with Burgers vector of magnitude b , as shown in Fig. 3.8, where the volume of the element of crystal prior to plastic deformation is dV = dX 1dX 2 dX 3 . The velocity of the dislocation line is v = δ , where δ is the distance the dislo
106
3 Kinematics of Crystalline Solids
cation moves during the course of plastic deformation. The plastic shear experienced by the volume element is ∆ bδ γ= . (3.101) = 3 dX dX 1dX 3 When n parallel edge dislocations of the same configuration shown in Fig. 3.8 are superposed, the plastic shear becomes n n ∆m bδm n (3.102) γ = ∑ 3 = ∑ 1 3 = 1 3 b δ = ρ 0b δ = ρ b δ , dX dX dX dX dX m =1 m =1 where δ is an average distance moved by the dislocations, ρ = J P −1 ρ 0 is the scalar mobile dislocation density, and J P = 1 . Since b is a constant, time differentiation of (3.102) leads to γ = ρ bv + ρ bδ . (3.103) Typically the second term on the right side, which can be attributed to dislocation generation or annihilation, is not treated explicitly. However, in some constitutive models for plasticity (see e.g., Zerilli and Armstrong (1987)) the contribution of dislocation generation to the total inelastic strain rate is considered substantial. When the second term on the right of (3.103) is omitted, Orowan’s slip rate equation written in the second of (3.100) is recovered for the case of a single set of parallel edge dislocations. Relation (3.103) was modified to account for the motion of disclinations, or rotational dislocations, by Li and Gilman (1970): γ = κη Rωv , (3.104) where κ is a scalar geometry factor, η is the line density of mobile disclination loops per unit reference or intermediate volume of the material, ω is the magnitude of the Frank vector representing the strength of the disclination, R is an effective scalar disclination radius, and v is again the mean line velocity of the defects. Das et al. (1973) and Kossecka and De Wit (1977) considered kinematics of mobile disclinations in the setting of geometric linearity. Disclinations are further examined in the context of geometric theories of continuous defect distributions in Section 3.3.3, and elastic solutions for disclination lines and loops are given in Appendix C. Returning now to the plastic velocity gradient resulting only from the dislocation flux, (3.98) can be written as (Werne and Kelly 1978) ⎛ j ⎞ LP = ⎜ ∑ α iT ⊗ v i+ ⎟ : ε , (3.105) ⎝ i =1 ⎠ with summation applied over j populations of straight dislocation lines, each with velocity vector v +j . The total dislocation density tensor α iT is
3.2 Multiplicative Inelasticity
α iT = ( ρ+i + ρ−i ) bi+ ⊗ ξ i ,
107
(3.106)
with ρ+i and ρ−i the densities (line length per unit volume in B ) of positively and negatively signed dislocations, where, for each value of i, positive and negative dislocations share the same tangent ξ i but oppositely oriented Burgers vectors bi+ = −bi− and velocities v i+ = − v i− . Using (3.104), Clayton et al. (2006) generalized (3.105) to account for contributions of total densities of mobile dislocation and disclination lines to the plastic velocity gradient. Deformations of primitive Bravais lattice vectors and basis vectors of crystal structures are now considered in the context of decomposition (3.31) and (3.26). Let a volume element of crystalline material of sufficient size as discussed in Section 3.2.2 deform via F = F L F P , where the plastic deformation from dislocation flux F P results from time integration of (3.98)(3.99) or (3.100). Let ai denote primitive Bravais lattice vectors of (3.1) mapped to B : α aiα = g .A AiA , (i = 1, 2,3) . Basis vectors in (3.3) likewise map only via the shifter 3
R ( 0k ) = ∑ mi g.αA AiA , ( 0 ≤ mi < 1 ). α
(3.107) (3.108)
i =1
Relations (3.107) and (3.108) imply that primitive lattice vectors and the basis vectors of the crystal structure are not affected by F P , in accordance with continuous dislocation theory (Bilby et al. 1957; Kroner 1960). However, primitive Bravais lattice vectors deform from configuration B to configuration B according to α ai = F L ai , aia = F La.α aiα = F La.α g .A AiA , (3.109) and correspondingly, in the absence of inner displacements q(0k ) a and ∆mi of the sort described in (3.19) and (3.20), deformed basis vectors satisfy 3
r ( 0k ) = F La.α g.αA R ( 0k ) = F La.α ∑ mi g.αA AiA . a
A
(3.110)
i =1
However, because of plastic deformation, (3.26) cannot be used to specify absolute spatial coordinates of (the nucleus of) a particular atom occupying a point on the Bravais lattice with reference position R (l ) . This is because atoms are translated in space by moving dislocations, even though primitive Bravais lattice vectors and basis vectors remain fixed in magnitude and direction while the material undergoes plastic flow. Reference Bravais lattice vectors A i are uniform in a perfect homogeneous lattice. However, when defects are contained within the volume, the
108
3 Kinematics of Crystalline Solids
deformed primitive lattice vectors ai represent suitable averages (Naghdi and Srinivasa 1993) of local primitive lattice vectors a′i that may not be spatially constant within the deformed element of material: ai = V −1 ∫ a′i dV . (3.111) V
The lattice deformation and lattice strain tensors in (3.65) thus provide firstorder deformed lengths of primitive Bravais lattice vectors and basis vectors of the crystal structure: ai = F L ai =
1/ 2
L ai , CL ai = ⎡⎣ AiA g.αACαβ g.βB AiB ⎤⎦
⎡⎛ 3 ⎞ L ⎛ 3 i β B ⎞⎤ r ( 0k ) = ⎢⎜ ∑ mi g.αA AiA ⎟ Cαβ ⎜ ∑ m g.B Ai ⎟ ⎥ ⎠ ⎝ i =1 ⎠⎦ ⎣⎝ i =1
,
1/ 2
,
L L ai iai − A i i A i = g.αA AiA (Cαβ − gαβ ) AiB g.βB = 2 Eαβ g.αA AiA AiB g.βB .
L
(3.112) (3.113) (3.114)
L
From (3.112)(3.114), it is evident that C and E provide a firstorder accurate measure of the stretch of the interatomic bond vectors in a crystal structure. 3.2.6 Crystal Plasticity
In what is referred to in this book as crystal plasticity theory, plastic deformation of single crystals is represented by slip on a finite number of glide planes, but lengths and directions of individual dislocation lines are not resolved explicitly. Early studies, in this context, of potentially finite distortions of cubic metallic crystals were conducted by Taylor and coworkers in the first half of the 20th century (Taylor and Elam 1923; Taylor 1927; Taylor 1938). A detailed account of these studies is given by Havner (1992). More modern treatments of finite deformation crystal plasticity that follow a notational scheme similar to that used here include those of Rice (1971), Hill and Rice (1972), Teodosiu and Sidoroff (1976), Peirce et al. (1982), and Asaro (1983).
3.2 Multiplicative Inelasticity
109
Fig. 3.9 Crystal plasticity kinematics
Fundamental variables entering the kinematic description of crystal plasticity theory are shown in Fig. 3.9. Multiplicative decomposition (3.31) applies, with the same general premise of Fig. 3.5 implied: plastic deformation resulting from dislocation glide is latticepreserving (Bilby et al. 1957). Slip director unit vectors si0 ( X ) ∈ TX B0 give the direction of dislocation motion on glide planes with unit normal covectors mi0 ( X ) ∈ TX* B0 . Index i refers to a slip system comprised of si0 and m i0 for a particular value of i, where i = 1, 2,...n , with n the total number of slip systems. Upon designation of a coordinate system, numerical values of si0 and m i0 can be assigned for particular crystal structures; for example, slip systems for cubic and hexagonal structures are listed in Table 3.4 and illustrated in Fig. 3.7. In FCC metals, slip systems are usually of type 110 {1 11} , in which case n = 12 if positive and negative slip are both allowed on a single system8. By definition, si0 and m i0 are orthonormal for each value of i: si0 , mi0 = s0i A m0i A = 0 .
(3.115)
P
From Fig. 3.9, since F is latticepreserving, slip vectors and slip plane covectors have parallel representations in intermediate configuration B : s iα = g.αA s0i A , m.iα = g.αA m0i A ; (3.116) si , mi = s i α mαi = g.αA s0i A g.Bα m0i B = s0i Aδ. BA m0i B = 0 .
(3.117)
8 If on the other hand positive and negative slip are described by mathematically distinct slip systems, n = 24 in FCC crystals.
110
3 Kinematics of Crystalline Solids
However, these quantities are pushed forward to the current configuration via the lattice deformation gradient: si ( x, t ) = F L s i ∈ Tx B , m i ( x, t ) = F L −*m i = m i F L −1 ∈ Tx* B . (3.118) The transformation law for a slip direction is analogous to that of a primitive Bravais lattice vector in (3.109), and the transformation law for a slip plane normal is analogous to that of a reciprocal Bravais lattice vector in (3.22) with F replaced by the lattice deformation. For a particular slip system i, si and m i are orthogonal: si , mi = F La.α s iα F L −1.βa mβi = s iα δ .αβ mβi = 0 .
(3.119)
However, neither si nor m i is necessarily of unit length. Scalar slip rates or shearing rates γ i are introduced on each system so that the plastic velocity gradient entering (3.58) is written as in (3.100): (3.120) LP = ∑ γ i s i ⊗ m i , i
though Orowan’s relation in (3.100) need not be formally enforced. Scalar γ i need not be a material time derivative of the cumulative slip on a particular glide system i. From (3.117), plastic deformation is isochoric: (3.121) J P = J P LPα.α = J P ∑ γ i si , m i = 0 , i
in agreement with the microscopic observation that dislocation glide is volumeconservative. From (3.118) and (3.120), the contribution from slip to the spatial velocity gradient of (3.58) is simply (3.122) F L LP F L −1 = ∑ γ i si ⊗ mi , i
P
and plastic spin W and plastic deformation rate DP tensors are computed in covariant form as 2 W P = ∑ γ i ⎡⎣(gsi ) ⊗ mi − mi ⊗ (gs i ) ⎤⎦ , (3.123) i
2D = ∑ γ i ⎡⎣ (gsi ) ⊗ m i + mi ⊗ (gs i ) ⎤⎦ . P
(3.124)
i
In the geometrically linear theory, stretch and rotation of the slip vectors are typically omitted, i.e., si and mi are assumed of constant (unit) length and orthonormal for all t ≥ 0 . In such a linear theory, using g to denote the metric tensor of the coordinate system, time rates of plastic distortion, rotation, and strain (refer to (3.81)(3.83)) are computed, respectively, as (3.125) β P = ∑ γ i si ⊗ m i , i
2Ω = ∑ γ ⎡⎣ (gsi ) ⊗ m i − m i ⊗ (gsi ) ⎤⎦ , i
P
i
(3.126)
3.2 Multiplicative Inelasticity
2ε P = ∑ γ i ⎡⎣(gsi ) ⊗ mi + mi ⊗ (gs i ) ⎤⎦ .
111
(3.127)
i
3.2.7 Macroscopic Plasticity In what is labeled in this book as macroscopic plasticity, a volume element of material undergoing inelastic deformation is assumed to contain a large number of single crystals or grains. Deformation map F P thus depicts the net contribution of local plastic responses of individual grains to that of the aggregate. In this representation of macroscopic plasticity, evolution of plastic deformation is prescribed without explicit consideration of individual grains and hence, without explicit consideration of individual glide systems or discrete defects corresponding to those systems. Macroscopic plasticity is distinguishable from what is termed typically as polycrystal plasticity. In polycrystal plasticity, various averaging or homogenization schemes are used to construct the response of the aggregate from that of its constituent single crystals (Taylor 1938; Bishop and Hill 1951; Kocks 1970). Consider the polar decompositions entering (3.33). Often the following requirements are stipulated for individual terms entering this kinematic description, in the context of macroscopic plasticity: plastic deformation F P is latticepreserving (i) and hence is volumepreserving (ii). Some measure of applied stress is work conjugate to V L (iii), such that a relaxed intermediate configuration B can be achieved via local unloading of the volume element by V L −1 (iv). This unloading scenario (iv) is in agreement with lattice preservation requirement (i), since mechanical stresses are associated with stretch of the interatomic bond vectors (primitive Bravais lattice vectors and basis vectors) at the atomistic level, as discussed at the end of Section 3.2.5. Requirement (ii) that J P = 1 is in agreement with the microscopic observation that dislocation glide is a conservative motion. Regarding the first equality of (3.33), if total deformation F is applied, and if symmetric plastic stretch U P is known from a constitutive or kinetic relation, then since FU P −1 = V L R L R P , it follows that R L and R P are not known uniquely (Bammann and Johnson 1987), but their product R L R P is. In such circumstances, elastically unloaded intermediate configuration B is nonunique up to a rotation. Uniqueness of B can only be ensured by prescription of skew rotation rate R P R PT for all t ≥ 0 or plastic spin W P of (3.62), in addition to the symmetric plastic deformation rate DP of
112
3 Kinematics of Crystalline Solids
(3.63)9. However, in implementations of macroscopic plasticity wherein the stressstrain response of the material of interest is isotropic, plastic spin is often not prescribed explicitly since the stress state can be deduced from knowledge of elastic and plastic stretch tensors and/or their time derivatives. This is in contrast to single crystal plasticity, wherein the plastic spin is prescribed explicitly by (3.123) and the intermediate configuration B is always defined uniquely. In particular, the choice of orientation of intermediate configuration and corresponding plastic rotation is usually thought unimportant for isotropic polycrystals, e.g., large numbers of randomly oriented grains whose individual anisotropies have no net effect on the mechanical response of the polycrystal. Kratochvil (1971) and Mandel (1973) suggested the intermediate configuration be associated with the substructure or a representative lattice in the polycrystalline material; Mandel (1973) labeled one such relaxed intermediate configuration an isoclinic space. Proper choices of constitutive functions or kinetic relationships for the plastic spin have been addressed by a number of researchers (Bammann and Aifantis 1987; Dafalias 1998; Scheidler and Wright 2003). 3.2.8 Inelastic Volumetric Deformation While dislocation glide is volumepreserving, in general the contribution of other kinds of lattice defects to the deformation gradient need not be. Consider a volume element of solid material containing a uniformly distributed collection of spherical defects, which could include isotropic point defects of local dimensions on the order of the lattice spacing: vacancies, interstitial atoms, or substitutional atoms. At a coarser scale of resolution, spherical defects could also include voids, defined as holes in the material of volume much greater than the atomic volume, or inclusions, defined as embedded inhomogeneities of dimensions much greater than the atomic volume. These defects can induce an isotropic, i.e. spherical or purely volumetric, deformation in the crystal, as modeled in what follows, though in general the deformation resulting from point defects, voids, or inclusions of arbitrary shape will be anisotropic. Finite deformation kinematics of crystalline solids with point defects was modeled by Teodosiu and Sidoroff (1976) and Kroner (1990), while large deformation kinematics of void growth in metallic crystals was adAlternatively, one could prescribe a separate constitutive equation for skew lattice spin tensors R L R LT or W L in order to specify a unique intermediate configuration, but this approach seems rarely used since R L is usually presumed to include rigid body rotations of the entire solid. 9
3.2 Multiplicative Inelasticity
113
dressed by Bammann and Aifantis (1989). Nunziato and Cowin (1979) formulated a geometrically nonlinear model of elastic solids with voids incorporating a multiplicative decomposition of the mass density. In solids of geologic origin such as many crystalline rocks, pore compaction (i.e., void shrinkage and collapse accompanying pressure loading) and dilatancy (i.e., inelastic volumetric expansion accompanying shear loading) are frequently observed (Brace et al. 1966; Rudnicki and Rice 1976; Goodman 1989). The pore compaction mechanism occurring in crushable brittle solids has been modeled with finite multiplicative kinematics (Clayton 2008). Unlike latticepreserving dislocation glide, the deformation induced by volumetric mechanisms generally does affect the lattice spacing in the (poly)crystal and hence is embedded in lattice deformation gradient F L : FL = FEFV , (3.128) E E E where F = V R is the elastic deformation associated with mechanical loading introduced in (3.27) and F V ( X , t ) accounts for volume changes from the reference configuration that remain in an element of the solid after mechanical loads are removed. Stresses applied to the volume element are associated with the stretch V E , so that unloading by V E −1 maps the element to a new stressfree intermediate configuration B . Proper orthogonal tensor R E includes rigid body rotation of the entire body. Deformation F V is not reversed when mechanical loads are removed from the volume element, e.g., when traction on the surface of the element is relaxed. The contribution of defects to mechanically irreversible volume changes of the solid may be written as (Bammann and Aifantis 1989; Clayton et al. 2005; Clayton 2009b) (3.129) F V = υδ α.β gα ⊗ g β , with the scalar υ ( X , t ) given by
υ = (1 − φ ) −1/ 3 ,
(3.130)
where φ ( X , t ) will be defined shortly. Requiring 0 < υ < ∞ leads to the limits −∞ < φ < 1 . Consider differential volume elements dV ⊂ B and
dV ⊂ B , where the generally anholonomic tangent map F V : TB → TB . The relationship between volume elements is det g 1 dV = J V dV = dV , (3.131) det F V dV = det g 1−φ
114
3 Kinematics of Crystalline Solids
upon assuming coincident coordinate systems and equivalent metric tensors g and g in B and B , respectively, as implied by g.αβ = δ α.β in (3.129). Thus the scalar φ is defined by
dV − dV . (3.132) dV When defects are introduced into a volume element of fixed mass within the body, φ is interpreted as a fraction of defects in the intermediate con
φ =
figuration B , per unit intermediate configuration volume: φ dV = dV − dV = (αξ dV + dV ) − dV = αξ dV ,
(3.133)
where ξ ( X , t ) and α ( X , t ) are the number of defects per unit volume and the volume change induced by each defect, respectively, contained within dV . When volume increases as a result of defects, for example from nucleation and growth of voids, then α > 0 . This condition is not required, however. For example, for an isotropic distribution of interstitial atoms, there could result a net decrease in volume due to F V , since the volume occupied per atom can decrease with increasing number density of interstitial atoms if the mass of the volume element is held fixed. Volume could also decrease if voids present in the reference configuration are compacted irreversibly as a result of applied pressure. In such cases α < 0 . Thus by (3.133), defects decrease the mass density of the solid when α > 0 , while defects increase the mass density when α < 0 . A different interpretation of deformation induced by vacancies or interstitials is possible if the mass of the volume element is not required to remain constant when such defects are introduced (Kroner 1990; Clayton et al. 2005). In such instances, introduction of a vacancy by removal of an atom from the crystal structure will typically cause contraction of the remaining atoms towards the defect as a result of attractive interatomic forces among atoms surrounding the vacancy, and the introduction of an interstitial atom into an otherwise perfect crystal will typically engender expansion of the remaining atoms away from the defect as a result of repulsive interatomic forces between the interstitial atom and its neighbors.
3.2 Multiplicative Inelasticity
115
Fig. 3.10 Kinematics of crystal element of fixed mass containing vacancies
Models of discrete point defects based on continuum linear elasticity are described in Section C.3 of Appendix C. A general expression for the total volume change per vacancy defect, when modeled as a rigid sphere in an isotropic elastic medium, is α = Ω0 + (1 + Γ)∆v , (vacancy), (3.134) where Ω0 > 0 is the atomic volume introduced in Section 3.1.1, ∆v ≤ 0 is the relaxation volume introduced in (C.188) or (C.195), and Γ( X , t ) is a scalar correction factor, ordinarily satisfying  Γ < 1 , accounting for elastic nonlinearity (Eshelby 1954; Holder and Granato 1969) formally derived later in Section 7.4 of Chapter 7. Often for vacancies, −0.1 ≤ ∆v / Ω0 ≤ 0 (Hull and Bacon 1984), though in materials with strong interatomic forces α < 0 is possible, leading to a net increase in mass density (Garikipati et al. 2006). For insertion of an interstitial atom of the same species as the surrounding medium, (3.134) is replaced with α = −Ω0 + (1 + Γ) ∆v , (interstitial), (3.135) where typically 0.1 ≤ ∆v / Ω 0 ≤ 1.0 (Hull and Bacon 1984). Decomposition (3.128) is illustrated in Fig. 3.10 for a cubic crystal with vacancies. Dark circles represent atoms and open circles represent vacancies. Mass is conserved since the volume element in each configuration contains the same number of atoms. Atoms neighboring each vacancy exhibit attraction towards the defect, leading to negative relaxation ∆v < 0 in (3.134). For a substitutional atom, the net volume change is simply α = (1 + Γ) ∆v , with ∆v positive in algebraic sign when the volume of the substitutional atom exceeds the atomic volume of the atom it replaces and negative when the
116
3 Kinematics of Crystalline Solids
volume of the substitutional atom is less than that of the atom it replaces. Insertion of a substitutional atom almost always involves a mass change. The preceding discussion applies primarily towards monatomic structures. In polyatomic crystals, distinct volumes are associated with defects (e.g., missing or extra atoms) of each species. In ionic crystals, defects often carry an electric charge that can significantly affect the imparted volume change (Mott and Littleton 1938; Sprackling 1976). For example, it is possible that a charged vacancy can induce local expansion ( ∆v > 0 ) as a result of repulsive Coulomb interactions among surrounding ions. Vacancies can arise in several ways that involve multiple atoms (Mott and Gurney 1948). Consider a simple monatomic lattice. A Frenkel defect consists of an interstitial atom together with a vacant lattice site, with these two individual defects spaced far enough apart so that their interaction is negligible. A Schottky defect consists of a vacancy and corresponding missing atom placed at a normal lattice site on a free surface of the crystal. The total volume of a crystal with Schottky defects will be greater than that of a perfect crystal with the same number of atoms provided that contraction of neighboring atoms towards each vacancy is not too large. From (3.129) and (3.130), the contribution to the time rate of deformation from inelastic volumetric deformation is also spherical:
F V F V −1 =
φ 3(1 − φ )
1 , F V.χα F V −1.χβ =
φ 3(1 − φ )
δ .αβ .
(3.136)
Since F V is generally incompatible, conditions δ .[αβ φ, χ ] ≠ 0 may apply. 3.2.9 Residual Deformation and a Multiscale Description As introduced in (3.26) and (3.31), lattice deformation F L accounts for all mechanisms that affect the primitive Bravais lattice vectors. When applied to an element of finite volume of a single crystalline or polycrystalline solid, deformation of the lattice may consist of contributions from multiple sources. Following Kratochvil (1972) and Clayton and McDowell (2003a), (3.31) may be expanded as a sequence of three terms: F = F E F I F P , FL = FE FI = V E R E FI , (3.137) where intermediate deformation map F I ( X , t ) accounts in some way for residual lattice deformation, distinct from the recoverable elastic stretch V E associated with mechanical loading, and also distinct from the average rigid body rotation of the element embedded within elastic rotation R E . Mapping F I is attributed to deformation induced by defects or microscopic heterogeneities within the element of crystal distinct from lattice
3.2 Multiplicative Inelasticity
117
preserving plastic flow associated with F P . These defects may include deformation twins, dislocation substructures and subgrain boundaries, and point defect or void distributions of the sort described already by (3.128) and (3.129). Thermal deformation can be distinguished from mechanical elastic deformation via a similar decomposition, as discussed in Section 3.1.3. Even a single dislocation, in isolation, will contribute to the local positions of atoms, as indicated in Fig. 3.11, which depicts the physics behind (3.137) in the context of a simple cubic lattice.
Fig. 3.11 Volume element of cubic crystal containing a single edge dislocation
In Fig. 3.11, traction applied to the volume in B is denoted by vector t ( x, t ) , formally defined later in (4.2) of Chapter 4. The displacement discontinuity in the wake of the dislocation is sealed by residual lattice deformation F I . Prior to the application of F I , for the body labeled B , elastic strain fields are absent, and plastic deformation F P is associated with relative rigid motion of the two halves of the lattice on opposite sides of the slip plane (dotted line). Note also that B is anholonomic in the vicinity of the slip plane: lattice vectors are discontinuous across this plane. The element in this configuration contains displacement (slip) discontinuities but no lattice strains, and is considered free of internal residual stress fields. This is in contrast to B , which may contain residual stress and strain fields but includes no discontinuities in displacements or displacement gradients except for those in the immediate vicinity of the individual defect line (i.e., the dislocation core) contained within the volume. Though not necessary, some authors make the additional assumption that F E , but not F L , be integrable at some scale of observation, or physically that its stretch be associated with external loads applied to solid body at that scale (Bilby and Smith 1956). Similar ideas have been forwarded in more recent strain gradient plasticity formulations (Bammann 2001; Regueiro et al. 2002). In that case, the contribution to the anholonomicity of F L −1 ( x, t ) arises strictly from skew gradients of F I −1 ( x, t ) (Clayton et al. 2004b):
118
3 Kinematics of Crystalline Solids
2 F L −1α.[ a ,b] = ( F I −1α. β F E −1.βa ),b − ( F I −1α.β F E −1.βb ), a = 2 F E −1.[βa F I −1α. β ,b ] ,
(3.138)
since F E −1.β[a ,b] = 0 are compatibility conditions for F E−1 . Other authors have suggested that F I be limited to a rotation R I = R I −T , for example accounting for irreversible rotations of Bravais lattice vectors attributed to disclination defects (Lardner 1973, 1974; Pecherski 1983, 1985), as discussed in greater depth in Section 3.3.3. An explicit expression for F I can be derived in terms of volume averages—over an element of crystalline material of finite size—of microscopic residual lattice and plastic deformations, following multiscale analysis (Clayton and McDowell 2003a; Clayton et al. 2004b). In such a multiscale interpretation of (3.137), continuous elastic and plastic deformation mappings describe the motion of the material at two length scales: a larger scale corresponding to the average or coarsegrained behavior of the volume element, and a smaller scale corresponding to subvolumes within this larger volume element. Continuum elements serving as domains for volume integration are shown in Fig. 3.12. Symbols V , V , and v describe respective crystalline volume elements in reference, unloaded intermediate, and current configurations. The lineal size of V is denoted by l, the latter presumed to far exceed the lattice parameters. However, the upper bound of l is left unspecified, such that V may encompass a region within a single crystal or numerous grains within a polycrystal. Corresponding reference, intermediate, and current configurations of the element are labeled B0 , B , and B , respectively. All of these configurations are described in more detail later in the text. Local, scalar differential volume elements within reference, intermediate, and current configurations are labeled dV , dV , and dv , respectively. These socalled differential elements are required to be smaller than their associated volume elements and should consist of no more than one grain of a polycrystalline aggregate, but should still be of dimensions larger than the atomic spacing in a perfect crystal.
3.2 Multiplicative Inelasticity
119
Fig. 3.12 Configurations, local volumes, and coordinate systems in reference configuration B0 , intermediate configuration B , and current configuration B
The motion of material points within element V from reference to current configurations is written x a = ϕ a (X ,t ) , where ϕ : B0 → B is continuously differentiable within V . Local intermediate configuration coordinates x α = x α (X ,t ) are also assumed to be continuously differentiable within V . Additional remarks on availability of continuously differentiable coordinates x α follow later. In what follows, basis vectors, basis covectors, and metric tensors are restricted to be constant, but not necessarily Cartesian, within each element in each configuration, such that covariant and partial differentiation are equivalent operations. However, these objects are permitted to vary smoothly across neighboring macroscopic volume elements V , V , and v if curvilinear coordinates are useful at the macroscale, and also from configuration to configuration. Configurations shown in Fig. 3.12 are now defined precisely. The referential volume V consists of the crystal structure as it existed prior to application of external forces, i.e., at initial time t = 0 , such that it is free of traction along its external boundary S . It may or may not contain dislocations, internal residual elastic strains, or residual plastic deformation. The current configuration volume element, v , is the elastically and plastically deformed single crystal or polycrystal, supporting possibly nonvanishing traction vector t on its external boundary s . The local or nested microscopic deformation gradient f for material points with coordinates X A within volume element V is defined as the tangent mapping ∂ϕ a f = Tϕ X = ga ⊗ G A . (3.139) ∂X A The volume averaged deformation gradient F for the macroscopic element of volume V is then defined by the motion of its external boundary,
120
3 Kinematics of Crystalline Solids
equivalent to the volume averaged local deformation gradient upon use of Gauss’s theorem as in (2.194)(2.196), with a slight change in notation: F .aA = V −1 ∫ x a N A dS = V −1 ∫ x.,aA dV = V −1 ∫ f .aA dV . (3.140) S
V
V
In (3.140), N A dS is an oriented differential surface element of S , with N an outward unit covector normal to the surface, as shown in Fig. 3.12. An elastic stretch tensor V E is associated with the traction or stress applied to s . A new intermediate configuration Bˆ is reached upon hypothetical instantaneous unloading via the inverse of the elastic stretch V E −1 , corresponding to null traction conditions on the external boundary of the element Vˆ (i.e., the traction ˆt = 0 along ˆs ), as shown in Fig. 3.13. The left elastic stretch tensor V E is determined explicitly from −1
⎛ ⎞⎛ ⎞ V = ⎜ ∫ x ⊗ NdS ⎟⎜ ∫ ˆx ⊗ NdS ⎟ , (3.141) ⎝S ⎠⎝ S ⎠ where ˆx are local coordinates of the external boundary of the element in configuration Bˆ . Thus, configuration Bˆ arises from instantaneous removal of traction along the boundary of Vˆ , constrained in such a way that global rotation of the volume element, R E −1 , does not occur upon stress relaxation. Furthermore, during unloading by V E−1 , plastic rearrangements of the solid are idealized as rate independent and inertial effects are excluded. Elastic rotation tensor R E is determined from solution of the following integrodifferential equation arising purely from local lattice rotations along with the following initial conditions: R E R E −1 = V −1 ∫ r Er E −1dV , R E = rE = 1 . (3.142) E
V
t =0
t =0
Denoted by r E is the local elastic and rigid body rotation exhibited by microscopic element of volume dV as it is deformed to its current representation dv . Note that R ET = R E−1 and r ET = r E−1 , since the antisymmetric property of the spin is preserved by volume averaging.
3.2 Multiplicative Inelasticity
121
Fig. 3.13 Configurations of macroscopic material element in context of multiscale threeterm decomposition of macroscopic deformation gradient
Intermediate configuration Bˆ is achieved by the net unloading procedure F E−1 = R ET V E−1 , i.e., unloading of the macroscopic element in the current configuration by removal of external forces then and subsequent rotation by the inverse (equivalently, the transpose) of the elastic rotation. After this unloading procedure, local coordinates x α describe positions of material particles within volume element V . The microscopic residual deformation gradient f is the tangent mapping ∂ϕ α f = Tϕ X = g ⊗ GA , (3.143) A α ∂X with x α = ϕ α (X ,t ): B0 → B the local motion for differential volume elements between reference and intermediate configurations. The volume averaged residual deformation F for the macroscopic crystal element is deduced from intermediate configuration coordinates of its external boundary. This definition of F is equivalent to the volumeaveraged residual local deformation gradient upon invocation of Gauss’s theorem, analogously to (3.140): F α. A = V −1 ∫ x α N A dS = V −1 ∫ x.,αA dV = V −1 ∫ f .αA dV . (3.144) S
V
V
Two additional assumptions, following kinematics of single crystalline elastoplasticity in Section 3.2.6, are made on a pointwise basis, for each differential volume element (Bilby et al. 1957): f = f Ef P , f = f E f P . (3.145)
122
3 Kinematics of Crystalline Solids
Denoted by f E = v Er E is the total lattice stretch ( v E ) and rotation ( r E ) for a differential volume element deformed to the current configuration, and f P is the remaining plastic deformation attributed to the history of motion of dislocations within or traversing that local element. Local elastic rotation r E was first introduced in (3.142). In the second equality listed in (3.145), f E embodies residual elastic stretch and rotation for a subvolume dV contained within externally unloaded volume V , and f P is the residual plastic deformation arising from dislocation motion. Microscopic volumes dV ⊂ V , dV ⊂ V , and dv ⊂ v are shown in Fig. 3.14, each visually enlarged relative to its surrounding macroscopic volume element for clarity. Local deformations of (3.145) then are interpreted as mappings between tangent spaces of local configurations associated with each microscopic element. Of the six tangent mappings entering (3.145), only f and f are necessarily compatible deformation gradient fields, as is clear from the integrands in (3.140) and (3.144). Furthermore, these six mappings are each regarded as constant (e.g., spatial averages) over their corresponding microscopic or differential volumes. Volumes whose boundary coordinates are generally anholonomic are denoted by dashed curves in Fig. 3.14, while holonomic coordinates are presumed available over external boundaries of elements depicted by solid curves in Fig. 3.14. Macroscopic plastic deformation F P emerges in the present multiscale context from the following integrodifferential equation written in terms of the volume averaged local plastic velocity gradient (Clayton et al. 2004b): F P F P −1 = V −1 ∫ f P f P −1dV , F P t = 0 = f P t = 0 = 1 . (3.146) V
Initial conditions in (3.146) presume that plastic deformation vanishes at the initial time. Notice that if the local plastic flow is isochoric such that Pα P1 A f .A f .α = 0 , then the volume averaged plastic flow of (3.146) is volumePα F P1.Aα = 0 then follows automaticonserving as well, since J P = J P F .A cally from (3.146). In an earlier work (Clayton and McDowell 2003a), alternative definition F P = V −1 ∫ f P dV was suggested; however, according to
that definition, F P is isochoric only to first order in terms of local plastic distortions if f P is isochoric but heterogeneous because volume averaging and the determinant operation do not generally commute.
3.2 Multiplicative Inelasticity
123
Fig. 3.14 Volumes, tangent maps, and configurations at two length scales
Upon assuming a threeterm multiplicative decomposition along the lines of (3.137) for total macroscopic deformation gradient F: F = FEFI F P = FEF , (3.147) net residual deformation gradient F enters the decomposition in accordance with (3.140), (3.141), and (3.144). Combining (3.144), (3.145), and (3.147) then leads to a representation of F I (Clayton and McDowell 2003a; Clayton et al. 2004b): ⎛ ⎞ F I = FF P −1 = V −1 ⎜ ∫ f E f P dV ⎟ F P −1 . (3.148) ⎝V ⎠ Deformation map F I can be interpreted as an indicator of residual elasticity in configuration B , along with corresponding residual stresses and stored elastic strain energy in the solid (Clayton et al. 2004b). Twopoint deformation tensor F I defined according to (3.148) contains both residual elastic ( f E ) and plastic ( f P , F P −1 ) contributions. It is clear from (3.148) that F I → 1 as f E → 1 and f P → F P , as would be the case for homogeneous deformation of the entire macroscopic (poly)crystalline element, such that external unloading by V E −1 relieves all local internal stresses and plastic rearrangements do not occur upon instantaneous unloading. On the other hand, if elastic and plastic deformation fields are heterogeneous throughout the macroscopic volume element, F I and commensurate residual stresses may not vanish. This is the usual circumstance when V encompasses a polycrystalline sample whose grains are
124
3 Kinematics of Crystalline Solids
misoriented by a nonnegligible amount (Clayton and McDowell 2003a). Such heterogeneity may arise within single crystals when cellular or laminar dislocation substructures misoriented from one other by finite lattice rotations, embodied here by the orthogonal part r E of f E , evolve and refine for example in FCC metals (Hughes et al. 1997; KuhlmannWilsdorf 1999; Ortiz and Repetto 1999; Ortiz et al. 2000) and BCC metals (Valiev et al. 2002) deformed to very large strains. Thus, when volume element V encompasses an entire single crystal, F I can represent the contribution of grain subdivision processes to the total deformation gradient F, as proposed by Butler and McDowell (1998). Additionally, if heterogeneity of local deformation and stresses (e.g., increased slip system activity and stress concentrations) are intensified in the vicinity of misoriented grain and subgrain boundaries—see for example experimental and numerical results for polycrystalline copper subjected to finite strains (Clayton et al. 2002; Clayton and McDowell 2003a)—then the largest contributions to F I would presumably emerge from these regions. Deformation tensor F I represents, in an average sense, the incompatibility of local microelastic deformation f E−1 within an element of reference volume V. If local elastic unloading f E−1 is uniform and hence integrable throughout spatial volume v , then f E = F E , f E = 1 , and if plasticity is locally homogeneous so that F = f = f P = f P = F P , then F I = 1 (refer to Fig. 3.14). However, F I reveals nothing about the compatibility, or lack thereof, of the average recoverable elastic deformation F E −1 ( x, t ) from macroscopic volume element to neighboring macroscopic volume element. If each macroscopic volume element V is regarded as an entire single crystal, then the incompatibility of F E−1 measures intergranular incompatibility among neighboring grains, while if each V is regarded as a subgrain, then incompatibility of F E −1 is an intragranular measure. Here incompatibility of F E−1 refers to a lack of continuous, single valued coordinates x α ( x, t ) spanning the union of i intermediate configuration volume elements ∪V ( ) . Thus, while the x α are assumed to be available i and differentiable within each volume element V ( ) , they may not be so over global configuration B . If in fact x α are multivalued or discontinuous over this global configuration, they are anholonomic in the sense of Section 2.8.1. An alternative definition of residual lattice deformation tensor F I is derived in Chapter 7. In the approach of Chapter 7, F I is defined in covariant Cartesian indices as the sum of the unit tensor and the average taken i
3.2 Multiplicative Inelasticity
125
over a reference volume element of material displacement gradients associated with residual stress fields of defects. Selfequilibrium conditions provide analytical expressions for the symmetric part of F I in the context of continuum nonlinear elasticity or anharmonic lattice statics. The nonlinear elastic approach of Chapter 7 builds on previous work of a number of authors (Zener 1942; Seeger and Haasen 1958; Toupin and Rivlin 1960). A detailed discussion of the approach is deferred until later (Chapter 7) because the derivation requires elements of thermomechanics and nonlinear elasticity developed in Chapters 4 and 5, respectively. This is in contrast to the derivation of F I in (3.148) that is purely kinematical. 3.2.10 Multiplicative Atomistic Plasticity
An alternative perspective of finite crystal kinematics is achieved upon consideration of motions of individual atoms (Clayton and Chung 2006; Chung and Clayton 2007). Assume that in reference configuration B0 , the representative Lagrangian volume element under consideration consists of a majority of atoms arranged on a lattice, but perhaps imperfectly due to the presence of defects within that volume element. Furthermore, assume that in configuration B of Fig. 3.4, the same mass and number of atoms exist in this representative volume, for example after propagation of dislocations across the volume. Atomic coordinates in B0 and B may not coincide, even though the crystal structure may look the same to an external observer in each of these two configurations because of the latticepreserving nature of dislocation glide. For simplicity, considered in the present Section are monatomic crystal structures for which basis vectors of the crystal structure vanish. Generalization of the present approach to polyatomic lattices is straightforward but requires introduction of additional mathematical machinery and notation. Furthermore, the treatment of Section 3.2.10 is restricted to coincident Cartesian coordinates in all configurations. Generalization to curvilinear coordinates is possible but requires additional cumbersome notation, e.g., shifter tensors. The position vector for arbitrary atom i in evolving intermediate configuration B is denoted by r i , where angled brackets are reserved for atomic labels, and i = 1, 2,...n , with n the total number of atoms contained within the volume element. Spatial positions of atoms (e.g., nuclear coordinates) in current configuration B , written as r i , are then found as r ai = δ.αa Rαi + q ai ,
(3.149)
126
3 Kinematics of Crystalline Solids
with q i the Cartesian displacement vector between intermediate and current locations of atom i. Vectors separating atoms i and j in respective configurations B and B are denoted by R i\ j = R j − R i , r i\ j = r j − r i . (3.150) Let the spatial position of atom i be updated according to n
r ai = ∑ F ijL aα Rαj + ∆r ai .
(3.151)
j =1
The first term on the right side of (3.151) accounts for the projection, over the volume element of atoms, of the macroscopic lattice deformation field to each atom within. Assuming that the CauchyBorn approximation of (3.26) applies only for the first term on the right side of (3.151), operator F ijL aα can be decomposed multiplicatively into the product of a continuum tangent map F.αL a ( X , t ) akin to that in (3.31) and a discrete Kronecker delta operator δ ij , with the latter satisfying δ ij = 1 for i = j and δ ij = 0 otherwise: F ijL aα = F.αL aδ ij .
(3.152)
The second term on the right side of (3.151), ∆r i , is the atomic scale perturbation in displacement attributed to microscopic heterogeneity in the vicinity of lattice defects, written here for atom i. This perturbation measures discrepancies in local atomic coordinates from those that would be predicted under homogeneous deformation of a monatomic crystal structure under the CauchyBorn hypothesis such as given in (3.109) for the primitive Bravais lattice vectors. From (3.151) and (3.152), spatial separation vectors introduced in (3.150) are updated according to (3.153) r i \ j = F L R i \ j + ∆r j − ∆r i . The perturbation in atomic displacement from an atom’s position in the intermediate configuration B is measured by ∆r i . However, if F P , the plastic deformation gradient of (3.31), is assumed to leave the geometry of the lattice unaltered as illustrated in the periodic domain of Fig. 3.5, then displacement perturbation ∆r i may be considered equivalent, from the standpoint of mechanical properties of the crystal, to a displacement perturbation measured from reference configuration B0 . The perturbation in this case would correspond to that of a different atom that may have entered a corresponding Eulerian control volume (dotted boundary in Fig. 3.5) during the course of plastic slip. Immobile defects such as pinned dis
3.3 A Linear Connection for Lattice Defects
127
locations, grain or subgrain boundaries, and fixed point defects may also be present in configurations B0 and B ; such defects are represented mathematically by perturbed atomic coordinates in the reference configuration. The description afforded by (3.149)(3.153) has been used to study effects of point, line, and surface defects upon stored energy and tangent elastic stiffness of the lattice in BCC crystals in the context of single slip (Clayton and Chung 2006) and to facilitate comparisons between predictions of molecular statics calculations (see Section B.2 of Appendix B) and continuum theories of lattice defects (Chung and Clayton 2007). The atomistic description follows from earlier work (Chung and Namburu 2003; Chung 2004) that considered perturbations in atomic displacements from their predicted positions under the CauchyBorn approximation in elastic solids—for example perturbations attributed to point defects—without recourse to introduction of an evolving intermediate configuration B needed to describe dislocationbased plasticity at finite deformations.
3.3 A Linear Connection for Lattice Defects The twoterm multiplicative decomposition of the deformation gradient of (3.31), F = F L F P , was proposed by Bilby et al. (1957) and Kroner (1960) for modeling the deformation of single crystals within the framework of continuously distributed dislocations. Here in Section 3.3, the description afforded by (3.31) is enhanced via consideration of a special class of linear connection (Section 2.2) describing physics of crystalline solids at a length scale more refined than that associated with (3.31). Such connections enable description of higherorder gradients of stretch and rotation in the lattice, or equivalently, enable more accurate approximation of atomic positions at microscopic spatial locations between two representative volume elements of crystal, each of whose average set of deformed, primitive Bravais lattice vectors is encapsulated by the nine degrees of freedom corresponding to a particular value of F L ( X , t ) according to (3.109)(3.114). Discovery of the relationship between the density of continuously distributed dislocations and Cartan’s torsion tensor of the crystal connection is usually credited to Kondo (1953, 1963), Bilby et al. (1955), and Kroner (1960). The crystal connection is defined in terms of a spatial gradient of the lattice deformation. Specifically, Γ cb..a = F La.α F L −1α.b ,c = − F La.α ,c F L −1α.b are coefficients of the crystal connection, integrable according to (2.218) as will be later demonstrated explicitly. The nonRiemannian geometric
128
3 Kinematics of Crystalline Solids
space associated with the crystal connection is said to possess a distant parallelism or a teleparallelism (Einstein 1928; Schouten 1954), and exhibits the special property that covariant derivatives of vectors taken with respect to this connection vanish if these vectors comprise a spatially constant vector field when pulled back to the intermediate configuration. The null curvature property of the crystal connection, together with knowledge of its torsion and a certain covariant plastic or elastic strain tensor is sufficient to uniquely specify the relaxed intermediate configuration (Le and Stumpf 1996a). Berdichevski and Sedov (1967), Noll (1967), Teodosiu (1967a), De Wit (1968), Toupin (1968), and Steinmann (1996) provided detailed viewpoints of dislocation kinematics using linear connections and geometric ideas. Since dislocations associated with the crystal connection are required to sustain compatibility of the total deformation, they are often labeled geometrically necessary dislocations in the sense of Ashby (1970). This is in contrast to absolute dislocations (Lardner 1969; Werne and Kelly 1978) that, when mobile, enable a nonzero dislocation flux and hence a nonzero rate of plastic deformation in (3.105). Nye (1953) associated a dislocation density tensor with the gradient of lattice rotation, i.e., the stressfree lattice curvature. Lardner (1969) showed that vanishing of the torsion tensor of the crystal connection corresponds to vanishing of excess dislocations of the same sign. Grain boundary, surface, and interface dislocations have been investigated from the standpoint of differential geometry and/or compatibility conditions (Bullough and Bilby 1956; Marcinkowski and Sadananda 1975; Hartley and Blachon 1978; Cermelli and Gurtin 1994; Dluzewski 1996; Gupta et al. 2007). Experimental techniques for measuring lattice curvature, redundant defect populations associated with geometrically necessary dislocations, and statistically stored dislocations have emerged and advanced in recent years (ElDasher et al. 2003; Hughes et al. 2003; Taheri et al. 2006) Kondo (1949, 1953, 1963, 1964) proposed general frameworks for yielding and plastic deformation allowing nonzero RiemannChristoffel curvature associated with a connection different from the crystal connection. Kondo’s frameworks admit different nonunique anholonomic (i.e., incompatible) intermediate configurations, or “tearings” in his terminology, for the same crystal. These configurations differ from the unique intermediate configuration favored by Bilby et al. (1955), for which the curvature tensor of the associated crystal connection vanishes and teleparallelism is enforced. Kondo (1964) associated nonzero curvature with the presence of rotational anomalies in the lattice, which can be interpreted as disclinations (Nabarro 1967; De Wit 1971, 1973). Connections admitting nonvanishing curvature tensors have since been used by many
3.3 A Linear Connection for Lattice Defects
129
for modeling disclinations in Bravais lattices (Anthony 1970; Lardner 1973, 1974; Minagawa 1979, 1981; Amari 1981; De Wit 1981). Rotational defects falling under the general category of Somigliana dislocations (Eshelby 1951, 1956; Asaro 1976; Teodosiu 1981) were addressed in terms of a pathdependent integral of a nonvanishing curvature tensor by Pecherski (1983; 1985). Nonmetric connections admitting extramatter defects (e.g., interstitial atoms, vacancies, or other point defects) were introduced in continuum theories by Kroner (1960, 1980, 1983), Minagawa (1979), and De Wit (1981). A brief early history of generalized continuum theories—for example theories with kinematic descriptions addressing orientations in addition to positions of material particles—was given by Eringen (1968). The remainder of Section 3.3 is organized as follows. First, a general linear connection is introduced in Section 3.3.1, capable of describing a variety of defects in the crystal in its deformed configuration. Particular forms of this connection, corresponding to various classes of admitted defects, are then examined in detail. The crystal connection and geometrically necessary dislocations are described in Section 3.3.2. The representation of distributions of disclinations in terms of a linear connection is developed in Section 3.3.3. Isotropic defects are considered in a differentialgeometric context in Section 3.3.4. Finally, the geometric description of kinematics of crystals with defects is summarized in Section 3.3.5. The remaining content of Section 3.3 parallels, refines, and substantially extends earlier work for modeling lattice defects (Clayton et al. 2005, 2006, 2008a). 3.3.1 General Form and Properties of the Connection
Consider a volume element of a crystalline solid whose average deformation gradient F follows decomposition F = F L F P of (3.31). As was the case in Section 3.2, this volume element is required to be of lineal dimensions much larger than the lattice parameters of the unit cell of the crystal structure, so that many dislocations or other defects may be contained within it. However, in Section 3.3, the volume element is restricted to either be embedded within a single crystal, or to consist of an entire single crystal. This restriction implies that when defects are absent, the orientation of each of the primitive Bravais lattice vectors in (3.1) does not vary with position within the element in its undistorted reference configuration. Recall from Section 3.2.2 that intermediate configuration B is generally anholonomic, with associated anholonomic coordinates xα , while refer
130
3 Kinematics of Crystalline Solids
ence and spatial configurations B0 and B are holonomic, spanned by continuously differentiable coordinates X A ( x, t ) and x a ( X , t ) , respectively. Note that (3.137) also applies here in general, though in Section 3.3 no decomposition of the total lattice deformation into recoverable and residual parts is necessary. Introduced next are continuously differentiable vector fields of director triads (Fox 1966) referred to tangent spaces of each configuration: d A ∈ TB0 , dα ∈ TB , d a ( x, t ) ∈ TB , ( A,α ,a = 1, 2,3 ). (3.154) Vectors of each triad in (3.154) are all dimensionless. From the last of (3.154), within a single crystal only the deformed directors referred to the spatial configuration are assumed to vary with position and time. Directors are mapped across configurations via the relations (3.155) dα = δ .Αα d Α , d a = F L −1 α.a ( x, t )dα = F L −1 α.aδ .Αα d Α , with summation implied over repeated indices. Plastic deformation F P is assumed latticepreserving as discussed in Section 3.2.1 such that the directors are physically the same in reference and intermediate configurations, as is clear from the first of (3.155). According to the second of (3.155), each director vector dα is pushed forward to the current configuration by the lattice deformation as the individual component of a covariant vector, analogously to (2.133). Reciprocal directors to (3.154) are introduced, satisfying d A ∈ T * B0 , dα ∈ T * B , d a ( x, t ) ∈ T * B , ( A,α ,a = 1, 2,3 ); (3.156)
d A , d B = δ .BA , dα , d β = δ.αβ , d a , db = δ.ba .
(3.157)
It follows that transformation formulae for the reciprocal directors are dα = δ α. Ad A , d a = F La.α ( x, t )dα = F La.α δ α. Ad A . (3.158) Thus, each reciprocal director is pushed forward by the lattice deformation like the component of a contravariant vector analogously to (2.131). By analogy with basis vectors of coordinate systems in (2.2) and (2.3), director vectors with indices in lower positions (3.154) are referred to as covariant director vectors or covariant lattice directors, while those with indices in upper positions (3.158) are referred to as contravariant director vectors or contravariant lattice directors. It is assumed that director vectors in configuration B are of unit length and are orthogonal: dα id β = dαχ g χδ d βδ = δαβ , (3.159) with δαβ emerging as a natural Euclidean metric on B . A generally nonEuclidean metric CL ( x, t ) with components referred to spatial configura
3.3 A Linear Connection for Lattice Defects
131
tion B and associated with the director strain is obtained from (3.155) and (3.156) as CabL = d a id b = F L −1α.a dα id β F L −1.bβ = F L −1α.aδ αβ F L −1.bβ . (3.160) The contravariant version of (3.160) provides the inverse metric: C L −1ab = d a id b = F La.α dα id β F Lb.β = F L .aα δ αβ F Lb.β ,
(3.161)
where the following orthonormality conditions have been applied: (3.162) dα id β = d χα g χδ dδβ = δ αβ . It follows that covariant and contravariant lattice directors are related by (3.163) d A = δ AB d B , dα = δαβ d β , d a = CabL db , d a = C L −1ab d b . In crystals with cubic, orthorhombic, or tetragonal structures (refer to Table 3.1 and Fig. 3.2), it is instructive to assign each reference director parallel to a reciprocal lattice vector, e.g., d Α δ Ai Ai , and to assign a coincident Cartesian coordinate system in each configuration with axes aligned with the referential reciprocal lattice vectors. In that case,
d a = F L −1 α.aδ .Αα d Α = F L −1 α.aδα i A i A i = F L −1 α.aδ .αB ABi A i
−1
g a = ai A i
−1
−1
(3.164) .
From (3.164), director vectors in the current configuration d a are equivalent to reciprocal basis vectors ai in the current configuration, normalized by their original lengths. In crystal structures wherein primitive reciprocal vectors are not necessarily orthogonal, directors of (3.154) are not necessarily parallel to the primitive translation vectors of the unit cell, but are instead an external construct. In that case, directors d a and strain metric (3.160) still provide a measure of the lattice deformation. Components of lattice deformation and its inverse can be recovered directly from the scalar products F La.α = F La.β d β , dα = d a idα , F L −1α.a = F L −1α.b db , d a = dα id a , (3.165) implying that knowledge of the vector fields in (3.155) and (3.156) is sufficient to characterize the firstorder deformation of the lattice. At a microscopic scale of resolution, absolute changes in lattice directors d a are described in terms of a covariant derivative executed with respect to a linear connection with coefficients Γˆ ..a ( x, t ) . The absolute bc
change of director vector d a with spatial position is defined in terms of the ˆ , treating the index of the corresponding covariant derivative operation ∇ director as that of a component of a covector in (2.30): ˆ d = d − Γˆ ..c d = ∂ d − Γˆ ..c d , ∇ (3.166) b a a ,b ba c b a ba c
132
3 Kinematics of Crystalline Solids
with the subscripted comma denoting partial differentiation with respect to spatial coordinates x a ( X , t ) . Similarly, for a contravariant director d a , ˆ d a = d a + Γˆ ..a d c = ∂ d a + Γˆ ..a d c . ∇ (3.167) b
., b
bc
b
bc
Coefficients of the connection in (3.166) and (3.167) are defined by (Minagawa 1979, 1981; Clayton et al. 2005, 2006, 2008a) Γˆ cb..a = F La.α F L −1α.b ,c + Qcb..a = Γ cb..a + Qcb..a , (3.168) where Γ cb..a = F La.α F L −1α.b ,c = − F La.α ,c F L −1α.b are coefficients of the crystal connection of nonRiemannian dislocation theories (Bilby et al. 1955; Noll 1967; Le and Stumpf 1996a), and Qcb..a are micromorphic degrees of freedom representing additional contributions of defects to spatial gradients of ˆ d = 0 (Minagawa 1981; the lattice director fields. Upon assuming ∇ b a Clayton et al. 2006), the connection of (3.166)(3.168) enables one to interpolate for directions and magnitudes of lattice directors at spatial locations between centroids of neighboring volume elements within a crystalline solid. In the trivial situation when Γˆ cb..a = 0 , lattice directors are spatially constant since in that case d a ,b = 0 . The crystal connection ( Γ cb..a ) component of (3.168) accounts for effects of firstorder spatial gradients of (the inverse of) F L , while micromorphic variable Q of (3.168) accounts for additional spatial variations of lattice directors not captured by the firstorder gradient of F L −1 . The deformation of a representative set of director vectors located at spatial position x corresponding to the volume element’s centroid is determined by F L , as indicated by (3.155). Stretch and rotation gradients of the lattice at spatial position x, for example at the scale of subgrain cells and cell blocks within a severely deformed single crystal (Seefeldt 2001; Hughes et al. 2003), are represented by coefficients of (3.168). Covariant components of Q are defined via lowering by the metric CL : Qcba = Qcb..d CdaL . (3.169) The covariant derivative of CL with respect to the connection coefficients in (3.168) is found by direct invocation of (2.30) as ˆ C L = C L − Γ ..d C L − Γ ..d C L − Q..d C L − Q..d C L ∇ c ab ab ,c ca db cb ad ca db cb ad = −2Qc ( ab ) + δαβ ⎣⎡ F L −1α.a F L −1.βb ,c + F L −1α.a ,c F L −1.βb − F L .dχ F L −1aχ,c F L −1α.d F L −1.βb − F L .dχ F L −1bχ,c F L −1α.a F L −1.βd ⎤⎦
(3.170)
= −2Qc ( ab ) . Components of the torsion tensor of the connection are obtained from application of (2.33):
3.3 A Linear Connection for Lattice Defects
Tˆcb..a = Γˆ [..acb] = Tcb..a + Q[..acb] ,
133
(3.171)
where Tcb..a = Γ [..a are components of the torsion of the crystal connection. cb ] Mixedvariant components of the RiemannChristoffel curvature tensor, ...a Rˆ bcd , formed from connection coefficients Γˆ cb..a are computed from (2.34): ... a Rˆbcd = Γˆ cd..a,b − Γˆ bd..a, c + Γˆ be..a Γˆ cd..e − Γˆ ce..a Γˆ bd..e (3.172) = 2∂[b Γˆ c..]ad + 2Γˆ [..bae Γˆ c..]ed , which, because of additive decomposition (3.168), can be expressed as the following sum (Schouten 1954): ...a ...a Rˆbcd = Rbcd + 2∇ˆ [b Qc..]ad + 2Tˆbc..e Qed..a − 2Q[..bed Qc..]ae ˆ Q..a + 2Tˆ ..e Q..a − 2Q..e Q..a = 2 F La.α ∂[b ∂ c] F L −1α.d + 2∇ bc ed [b c ] d [b d c ]e
(3.173)
ˆ Q..a + 2Tˆ ..e Q..a + Q..e Q..a − Q..e Q..a . = 2∇ bc ed cd be bd ce [b c] d ...a In (3.173), the curvature from the crystal connection, Rbcd , vanishes identically since the crystal connection is integrable, as follows from the generic derivation in (2.215)(2.218). The fully covariant curvature tensor corresponding to (3.173) is obtained directly using (3.170) and the product rule as follows: ˆ Q ..e C L + 2Tˆ ..e Q − 2Q ..e Q .. f C L Rˆ bcda = 2∇ bc eda [b c]d ae [b d c]e af
ˆ Q + 2Tˆ ..e Q − 2Q ..e ∇ ˆ C L − 2Q ..e Q = 2∇ bc eda b] ae ⎡c d [b d c]ea [b c] da ⎣
ˆ Q + 2Tˆ Q + 4Q = 2∇ eda [ b c] da ..e bc
..e ⎡⎣b d
Qc]( ae) − 2Q[..eb d Qc]ea
(3.174)
ˆ Q + 2Tˆ ..eQ + 2Q ..e Q . = 2∇ bc eda [ b c] da [b d c ]ae ˆ vanishes identically when From (3.173) and (3.174), curvature tensor R the supplementary degrees of freedom vanish, i.e., when Q = 0 . Decomposing (3.174) into an antisymmetric part over the final two indices gives L −1ef ⎡ ˆ Q ˆ ..e Rˆ[bc][ da] = 2∇ Q Q − Q[b af Qc]de ⎤ [b c][ da] + 2Tbc Qe[ da] + C ⎣ [b df c]ae ⎦ e L ef .. 1 − ˆ Q ˆ ⎡Q b de Qc af − Q b af Qc de ⎤ = 2∇ [b c][ da] + 2Tbc Qe[ da] + C ] [ ] ⎦ ⎣ [ (3.175) L −1 fe ˆ Q ˆ ..eQ ⎡ ⎤ T C Q Q Q Q = 2∇ + − − 2 bc e[ da ] [ c af b]de ⎦ [b c][ da] ⎣ [c af b]de .. e ˆ Q = 2∇ + 2Tˆ Q . [b
c ][ da]
bc
e[ da ]
The symmetric part of (3.174) over the final two covariant indices is obtained from identity (2.49) and (3.170):
134
3 Kinematics of Crystalline Solids L ˆ ∇ ˆ ˆ ..e ˆ L ˆ ˆ ..e Rˆ [bc]( da ) = −∇ [b c]Cda − Tbc ∇ e Cda = 2∇[b Qc]( da ) + 2Tbc Qe( da ) .
(3.176)
The notion of a Cartan displacement (Schouten 1954; Brillouin 1964; Wang and Truesdell 1973; Minagawa 1979) is often used to provide a geometric interpretation of nonintegrability of a space or manifold with possibly nonvanishing torsion and curvature. Cartan’s displacement about a curve c encircling area a with differential element dx a ∧ dxb = ε abc nc da is derived using Stokes’s theorem of Section 2.7.2. While the general treatment of Section 3.3 permits arbitrary curvilinear coordinates in the spatial configuration, the derivation given immediately below in (3.177) in indicial notation is restricted to spatial coordinates x a wherein corresponding g
Christoffel symbols Γ ..bca = 0 by definition (e.g., Cartesian coordinates), since integration of a vector field is involved. Cartan’s displacement is defined as the following line integral: Bˆ a = − ∫ (δ .ae + x.,ae )dx e = − ∫ δ .ae dx e − ∫ x.,ae dx e c
c
c
= ∫ δ dx ∧ dx + ∫ Γˆ ec..a x c dx e a .e , b
e
b
a
c
= ∫ δ dx ∧ dx − ∫ (Γˆ ec..a x c ),b dx e ∧ dxb a .e ,b
e
a
b
a
= − ∫ Γˆ eb..a dx e ∧ dx b + ∫ (Γˆ ec..a x c ),b dx e ∧ dx b a
a
= − ∫ Tˆeb..a dx e ∧ dx b + ∫ (Γˆ ec..a,b x c + Γˆ ec..a x.,cb )dx e ∧ dxb a
(3.177)
a
= − ∫ Tˆeb..a dx e ∧ dx b + ∫ (Γˆ ec..a,b x c − Γˆ ec..a Γˆ bd..c x d )dx e ∧ dxb a
a
= − ∫ Tˆeb..a dx e ∧ dx b + ∫ (∂ [b Γˆ e..]ad + Γˆ [..bac Γˆ e..]cd ) x d dx e ∧ dx b a
a
1 ...a d 1 ˆ ...a d Rbed x )dx b ∧ dx e = −ε bec ∫ (Tˆbe.. a + Rˆbed x ) nc da. 2 2 a a The following special definitions10 that presume a kind of modified parallel transport of Kronecker’s delta δ .ae and spatial position x d with respect to (3.168) are also used to compute the Cartan displacement in (3.177): ˆ ′ δ a = δ a − Γˆ ..aδ c = δ a − Γˆ ..a = 0 , ∇ ˆ ′ x c = x c + Γˆ ..c x d = 0 . (3.178) ∇ .e , b .e , b .,b b .e bc .e be b bd Using (3.174)(3.177), the Cartan displacement can be written as the sum = − ∫ (Tˆbe..a +
10
ˆ ′ as defined in (3.178) does not obey (2.30); i.e., ∇ ˆ′ ≠∇ ˆ . Notice that ∇ a a a
3.3 A Linear Connection for Lattice Defects
135
1 ⎡ ⎤ Bˆ a = − ∫ ⎢Tˆbc..a + C L −1ae ( Rˆbc[de] + Rˆbc ( de ) ) x d ⎥ dx b ∧ dx c . (3.179) 2 ⎦ a⎣ Cartan displacement Bˆ a will be associated later in Sections 3.3.2, 3.3.3, and 3.3.4 with a total Burgers vector (i.e., incompatibility measure) resulting from effects of all defects (e.g., dislocations, disclinations, and point defects) threading or situated on oriented area a encircled by circuit c. Application of Stokes’s theorem in (3.177) requires that connection coefficients have continuous first derivatives with respect to spatial coordinates, implying that lattice deformation and its inverse must have continuous second derivatives with respect to spatial coordinates. It is often instructive to consider a linearized theory. In that case, the distinction between intermediate and spatial coordinate systems is omitted, and the lattice deformation gradient and lattice distortion are related by (3.180) F La.b = δ.ba + β La.b , F L −1.ab = δ .ba − β La.b . Clayton et al. (2008a) considered a partially nonlinear regime wherein approximation (3.180) applies for lattice deformation, but wherein gradients of lattice directors may be arbitrarily large, thus retaining fully nonlinear forms of connection (3.168), torsion (3.171), and curvature (3.172). On the other hand, a fully linear description omits all secondorder terms in the connection coefficients, torsion, and curvature. In the context of such a fully linear theory, the connection (3.168) becomes Γˆ cb..a = −(δ .ad + β La.d ) β Ld.b ,c + Qcb..a ≈ − β La.b ,c + Qcb..a = Γ cb..a + Qcb..a , (3.181) where the linearized crystal connection and its torsion are, respectively, Γ cb..a = − β La.b ,c , Tcb..a = − β La.[b,c ] . (3.182) The linearized metric of (3.160) is CabL = F L −1α.aδαβ F L −1.βb = (δ .da − β Ld.a )δ de (δ .eb − β Le.b ) = (δ ab − β abL − β baL + β eaL β Le.b ) ≈ δ ab − 2β (Lab ) . Similarly, the linearized inverse metric of (3.161) is C L −1ab = F La.α δ αβ F Lb.β = (δ .ad + β La.d )δ de (δ .be + β Lb.e )
(3.183)
(3.184) = (δ ab + β Lab + β Lba + β Lae β Lb.e ) ≈ δ ab + 2β L ( ab ) . Covariant components of connection (3.181) are then approximated as Γˆ cba ≈ (− β Ld.b,c + Qcb..d )CdaL ≈ (− β Ld.b,c + Qcb..d )(δ da − 2 β (Lda ) ) (3.185) ≈ −∂ c β L ab + Qcb..d δ da . Connection coefficients in (3.185) can then be partitioned as 1 Γˆ c( ba ) ≈ ∂ c C L ( ba ) + Qc ( ba ) , Γˆ c[ba ] ≈ ∂ c β L[ba ] + Qc[ba ] . (3.186) 2
136
3 Kinematics of Crystalline Solids
The torsion tensor of (3.181) is simply Τˆcb..a ≈ β L.a[c ,b] + Q[..cba ] .
(3.187)
The curvature tensor of (3.172) is approximated successively as follows by neglecting products of two and higher in the connection coefficients: ...a Rˆbcd ≈ 2∂[b Γˆ c..]ad = 2∂[c ∂ b] β La.e + 2∂[b Qc..]ad = 2∂[b Qc..]ad . (3.188) Fully covariant approximations of the curvature tensor are then Rˆ bcda ≈ 2∂[b Qc]da , Rˆ bc[da ] ≈ 2∂[b Qc ][da ] , Rˆ bc ( da ) ≈ 2∂ [b Qc ]( da ) .
(3.189)
The Cartan displacement in (3.177) can then be obtained in the linear approximation via use of (3.187) and (3.188). Association of the mathematical framework of Section 3.3.1 is made with the physics of continuous distributions of lattice defects in what follows in the remainder of Section 3.3. This association is accomplished by considering three limiting cases: traditional (geometrically necessary) dislocation theory in Section 3.3.2, characterized by Qcba = 0 ; disclination theory in Section 3.3.3, characterized by Qcba = Qc[ba ] ; and a theory for isotropically distributed point defects in Section 3.3.4, characterized by Qcba = ϒ c CbaL . Superposition of ideas set forth in each of the three cases then enables description of crystals containing dislocations, disclinations, and point defects. 3.3.2 Dislocations and the Crystal Connection The description of Section 3.3.1 encompasses only traditional, translational dislocations if Qcba = 0 , for which (3.168) reduces to the crystal connection (Bilby et al. 1955; Kroner 1960; Noll 1967): Γˆ cb..a = Γ cb..a = F La.α F L −1α.b,c (3.190) = − F La.α ,c F L −1α.b = − F La.α , β F L −1.βc F L −1α.b , where the third equality follows from ( F La.α F L −1α.b ) ,c = δ .ba ,c = 0 . The torsion tensor obtained from connection coefficients in (3.190) is then Tˆcb..a = Tcb..a = F La.α F L −1α.[b,c ] = F La.α ∂ [c F L −1α.b] , (3.191) The torsion in (3.191) vanishes by (2.219) when the lattice deformation is integrable: Tcb..a = 0 ↔ F L −1α.[b,c] = 0 ⇔ F L −1α.a = x.,αa , (3.192)
3.3 A Linear Connection for Lattice Defects
137
in which case xα = xα ( x, t ) . Recall from (3.170) that the connection is metric, ∇ a CbcL = 0 , and from (3.173) that the connection is integrable, ... a Rbcd = 0 , both following from prescription Qcba = 0 in (3.190). Consider partial derivatives of the lattice director vectors and their reciprocals obtained following (3.155) and (3.158): d a ,b = F L −1α.a ,b dα = F L −1α.a ,b F Lc.α d c = Γ ba..c d c , (3.193)
d.,ab = F La.α ,b dα = F La.α ,b F L −1α.c d c = − F L.aα F L −1α.c ,bd c = −Γ bc..a d c ,
(3.194)
α
since by definition, dα ,b = 0 and d.,b = 0 . Relations (3.193) and (3.194) denote parallel transport of the lattice directors with respect to the crystal connection: (3.195) ∇ bd a = d a ,b − Γ ba..c d c = 0 , ∇b d a = d.,ab + Γ bc..a d c = 0 , and are analogous to relationships for partial coordinate derivatives of holonomic basis vectors in (2.59).
Fig. 3.15 Defective cubic lattice as described by the crystal connection
A twodimensional visual interpretation of the crystal connection is given in Fig. 3.15 for a simple cubic lattice. Inscribed on the image of the body on the left side of Fig. 3.15 are two orthogonal fields of constant contravariant vectors in configuration B —denoted by u and v —that form a rectilinear grid representative of the field of primitive Bravais lattice vectors. More specifically, each vector u or v is parallel to a primitive Bravais lattice vector of (3.1), but is of magnitude of a Bravais lattice vector multiplied by a factor of eight. In a simple cubic lattice, u and v are also parallel to slip directions and perpendicular to slip planes, as deduced from Table 3.4. The representation of a perfect lattice in B is in agreement with dislocationbased plasticity theory (Section 3.2.5) and crystal plastic
138
3 Kinematics of Crystalline Solids
ity theory (Section 3.2.6), for example, wherein F P : TB0 → TB is assumed to leave the slip directions and slip planes unperturbed. Notice that the crystal may have undergone slip with respect to its position relative to reference configuration B0 , as indicated by the dotted unit cell boundaries on the left side of Fig. 3.15. For clarity, these slip steps are not shown on the right side of Fig. 3.15, though they do exist in configuration B. Since vectors u and v are independent of position in the intermediate configuration, u( A) = u( B) , v( A) = v( B ) , (3.196) where A and B are two points on the lattice in the relaxed configuration separated by a small distance dx = x( B ) − x( A) when their positions are mapped onto the deformed image of the crystal. Focusing for the moment on the field u , both sides of the first of (3.196) are premultiplied by F L ( B) , the value of the deformation at the location corresponding to point B on the lattice, to obtain F La.α ( B)uα ( A) = F La.α ( B)uα ( B) . (3.197) Expanding F L ( B ) with a firstorder (i.e., linear) approximation in x gives
F La.α ( B) ≈ F La.α ( A) + F La.α ,b ( A)dxb ,
(3.198)
which is then substituted into (3.197) to yield u a ( B ) = u a ( A) + F La.α ,b ( A) F L −1α.c ( A)u c ( A)dx b ,
(3.199)
where vectors u are pushed forward via u a ( A) = F La.α ( A)u α ( A) , u a ( B ) = F La.α ( B)uα ( B) .
(3.200)
Using the identity ( F
La .α
F
L −1α .c
) , b = 0 , (3.199) is rewritten as
0 = u ( B) − u ( A) + F La.α ( A) F L −1α.c ,b ( A) dxb u c ( A) . a
a
Making the linear approximation u a ( B) − u a ( A) ≈ ∂ b u a ( A) ⎡⎣ x b ( B) − x b ( A) ⎤⎦ = u.,ab ( A) dx b ,
(3.201) (3.202)
and dropping notation signaling localization to point A, (3.201) becomes 0 = u a.,b dx b + F La.α F L −1α.c ,b dx b u c . (3.203) This is the structure of a null covariant derivative, i.e., parallel transport with respect to the crystal connection of (3.190): (3.204) ∇b u a = u a.,b + Γ bc..a u c = 0 , because dx b is now arbitrary. Since connection coefficients corresponding to ∇ in (3.204) are equivalent to those given in (3.190), parallel transport of vectors u with respect to the crystal connection physically corresponds
3.3 A Linear Connection for Lattice Defects
139
to a reconstruction of the deformed lattice from a rectilinear grid in relaxed configuration B . Analogously, field v in Fig. 3.15 obeys (3.205) ∇b v a = v a.,b + Γ bc..a v c = 0 , i.e., the vector field v = F L v ∈ TB constructed by pushing forward from the uniform reference grid v ∈ TB obeys the rule of parallel transport with respect to the connection in (3.190). It is now clear why the crystal connection is said to possess the property of teleparallelism in the context of geometric field theories (Einstein 1928; Schouten 1954). The closure failure or Cartan displacement Bˆ of the area a shown in Fig. 3.15—i.e., the area of the parallelogram enclosed by u( A) , u( B) , v ( A) , and v (C ) , with C a third location in the deformed crystal—is equivalent to the integral of a field of local Burgers vectors b( x, t ) (Kroner 1980). Consider first the vector addition relation that follows from visual inspection of Fig. 3.15: Bˆ a = u a ( A) − u a ( B ) + v a (C ) − v a ( A) . (3.206) ˆ Comparison with Fig. 3.6(b) demonstrates that B represents the sum of local Burgers vectors of dislocations traversing area a, when the tangent lines of dislocations are defined in a righthanded sense when the Burgers circuit is taken as counterclockwise. In configuration B in Fig. 3.15, xb ( B ) − xb ( A) = vb ( A) , xb (C ) − xb ( A) = u b ( A) . (3.207) Upon making the linear approximations u a ( B ) − u a ( A) ≈ u.,ab ( A)vb ( A) , v a (C ) − v a ( A) ≈ v.,ab ( A)u ( A) b , (3.208) and invoking (3.204) and (3.205), the closure failure of (3.206) becomes (3.209) Bˆ a = −u.,ab ( A)v b ( A) + v.,ab ( A)u b ( A) = Γ bc..a v b u c − Γ bc..a u b v c , which can be written as c b (3.210) Bˆ a = 2Γ [..a vb u c = 2Tbc..a u [ v ] . bc ] Making the identification
1 1 c b u [ v ] = (u c v b − u b v c ) = ∫ dx c ∧ dxb 2 2a
(3.211) 1 cbd 1 cbd = ε ∫ nd da = ε nd a , 2 2 a equality (3.210) is then rewritten as Bˆ a = −ε bcd Tbc..a nd a , (3.212) which is identical to the Cartan displacement in (3.177) when the curvature ... a = 0 is always true for the integrable crystensor vanishes (recall that Rbcd
140
3 Kinematics of Crystalline Solids
tal connection) and when the normal to the area enclosed by the Burgers circuit is constant, as is the case in the twodimensional scenario shown in Fig. 3.15. More generally, the Cartan displacement or total Burgers vector in (3.177) is written as Bˆ a = ∫ b a da = − ∫ T cd..a dx c ∧ dx d a
a
= −∫ T ε ..a cd
a
bcd
nb da = ∫ α ab nb da ,
(3.213)
a
with the geometrically necessary dislocation density tensor11 referred to B: α ab = ε bcd Tdc..a = F La.α ε bcd F L −1α.c ,d , 2Tdc..a = ε cdbα ab . (3.214) Formally, field b a ( x, t ) is assumed continuous and differentiable, in the context of theories of continuously distributed dislocations (Bilby et al. 1955; Willis 1967; Teodosiu 1982). On the other hand, Burgers vectors in real crystals measure discrete steps in the lattice. In continuum field theories (Bilby et al. 1955; Willis 1967; Teodosiu 1982), one often considers a volume element of a body in which the number of discrete dislocations tends towards infinity while the Burgers vector of each tends to zero such that their product remains finite. In this limiting process, the radius of each dislocation core, and the total volume occupied by core regions is also assumed to approach zero (Willis 1967). In terms of straight defect lines, analogously to (3.89), the dislocation density tensor in the spatial configuration is written (Lardner 1974) j
j
i=1
i =1
α = ∑ ρ i bi ⊗ ξ i , α ab = ∑ ρ i biaξ ib ,
(3.215)
with ρ i , bi , and ξ i the nonnegative line length per unit current volume, Burgers vector, and tangent line in the spatial configuration for dislocation population i. Complete and partial dislocations may contribute to (3.214) and (3.215). Nye (1953) is credited with equating the dislocation density tensor of (3.215) with that of (3.214) when the lattice deformation reduces to a small rotation:
Depending on the sign convention used to define the Burgers circuit, positive line direction of dislocations, and positive orientation of the area enclosed by the circuit, the algebraic sign of the total Burgers vector and dislocation density tensor may vary (Minagawa 1979; Teodosiu 1982; Clayton et al. 2005). The relationship between the dislocation density tensor and torsion may differ by a factor of two depending on the definition used for the torsion tensor. The transpose of (3.214) is often used as a definition of the dislocation density tensor (Minagawa 1979). 11
3.3 A Linear Connection for Lattice Defects
α ab = −(δ .ae + β La.e )ε bcd β Le.c ,d ≈ −ε bcd β La.c ,d ≈ − g aeε bcd Ω[Lec],d = g aeε cdb ε cfe wL.,fd = g ab wLd.,d − g ad wLb.,d ,
141
(3.216)
where w La = −ε abc Ω bcL / 2 is a lattice rotation vector obtained via an axial transformation such as (2.166). Now consider relaxed intermediate configuration B , which is generally anholonomic as discussed in Section 3.2.2. The anholonomicity of B may be represented in terms of the nonintegrability of either of tangent maps F L −1 or F P via a nonvanishing anholonomic object in (3.41), or equivalently, with a net Burgers vector B ∈ TB , defined in terms of closure failure of the line integral of pseudodifferential vector element (i.e., Pfaffian) dx = F L −1dx = F P dX over a loop c in B (Bilby et al. 1955; Kroner 1960): B = − ∫ dx = − ∫ F L −1dx = − ∫ F P dX , (3.217) c
c
C
where c and C are closed images of Burgers circuit c mapped to current and reference configurations, respectively12. The opposite sign convention for B is used by some authors (Teodosiu 1970, 1982; Clayton et al. 2004a). Comments regarding integration of vector fields over TB in the context of (3.95) and (3.96) and general curvilinear coordinates apply here as well. Using the generalized Stokes’s theorem of Section 2.7.2, and replacing F with F P in (2.199) and F −1 with F L −1 in (2.200), leads to − ∫ F Pα. A dX A = ∫ F Pα.[ A; B ] dX A ∧ dX B = ∫ ε CAB F Pα. A, B N C dA , (3.218) C
A
−∫ F c
L −1α .a
A
dx = ∫ F a
L −1α .[ a ;b ]
a
dx ∧ dx = ∫ ε cab F L −1α.a ,b nc da . a
b
(3.219)
a
Similarity of (3.219) with the geometric interpretation (3.213) is evident: Bα = ∫ ε dab F L −1α.[ a ,b] nd da a
..c nd da = ∫ F L −1α.cα cd nd da. = ∫ ε dab F L −1α.cT ba a
(3.220)
a
Twopoint dislocation density tensors α 0 and α L are introduced as B = ∫ α 0 NdA = A
∫α
L
nda ;
(3.221)
a
α 0α A = ε ABC F Pα.B ;C = ε ABC F Pα. B ,C , α Lα a = ε abc F L −1α.b;c = ε abc F L −1α.b ,c . (3.222)
12 Designation of c as “closed” is somewhat abstract since configuration B is anholonomic. The first equality in (3.217) can be omitted without consequence.
142
3 Kinematics of Crystalline Solids
Symmetries of LeviCivita connections are exercised in (3.218), (3.219), and (3.222). The first of (3.222) exhibits a discrete version (3.89), analogously to (3.215). Using Nanson’s formula (2.227), surface integrals in (3.221) are mapped to integrals over area a in configuration B : β Bα = ∫ α 0α A J P −1 F P .A nβ da = ∫ α Lα a J L F L −1.aβ nβ da = ∫ α αβ nβ da , (3.223) a
a
a
where J L and J P are defined in (3.48) and (3.49), and where components of the dislocation density tensor referred to the intermediate configuration α αβ = J P −1α 0α A F P .Aβ = J Lα Lα a F L −1.aβ . (3.224) The first of (3.224) is consistent with the last of (3.92). The second equality in (3.224) can be derived directly from (2.142) and (3.31) as follows: J P −1 F P.βAε ABC F Pα. B ,C = J −1 J L F L −1.βa F. Aa ε ABC ( F L −1α.b F. Bb ),C = J L F L −1.βa ⎡⎣ J −1 F. Aa ε ABC F L −1α.b ,C F. Bb ⎤⎦ = J L F L −1.βa ⎡⎣( J −1ε ABC F. Aa F. Bb F.Cc ) F L −1α.b,c ⎤⎦
(3.225)
= J L F L −1.βa ε abc F L −1α.b ,c . In terms of discrete lines, terms entering various intermediate and spatial dislocation densities are related by j
dBα = α Lα a na da = ∑ ρ i b iα ξ i a na da i =1 j
= α αβ nβ da = ∑ ρ i b iα ξ i β nβ da
(3.226)
i =1 j
= α ba na da = ∑ ρ i b ibξ i a na da, i =1
where tangent lines, scalar numbers of dislocations per unit volume, and local Burgers vectors are mapped across configurations as ξ i a = F La.α ξ iα = F. Aaξ0i A , ρ i = J L −1 ρ i = J −1 ρ 0i , bib = F Lb.α b iα . (3.227) From the first of (3.227), the tangent vector is generally only of unit length in one configuration. From the second of (3.227), since J P = 1 when slip is latticepreserving, the scalar densities satisfy ρ i J L = ρ i = ρ 0i . The third of (3.227) is consistent with the relationship between intermediate and spatial Burgers vectors in (3.84). In the context of the geometrically linear theory, all line and surface integrals effectively take place in the same (e.g., spatial) configuration; a total Burgers vector B in this configuration is found in terms of plastic distortion β P = F P − 1 as
3.3 A Linear Connection for Lattice Defects
143
B a = − ∫ (δ.ba + β P.ab )dx b = ∫ β Pa.b;c dx b ∧ dx c c
c
g
= ∫ ( β P.ab, c + Γ
.. a ( cd )
g
β P.db − Γ
.. d ( cb )
β P.ad )ε bcd nd da .
(3.228)
c
= ∫ ε bcd β P.ab, c nd da = ∫ α ad nd da. c
c
Similarly, the total Burgers vector in terms of the elastic distortion is B a = − ∫ (δ .ba − β L.ab )dx b = − ∫ β L.ab ;c dx b ∧ dx c c
= −∫ ε
c
bcd
β
c
(3.229)
n da = ∫ α ad nd da.
La .b , c d
c
Comparing (3.228) and (3.229), the linearized dislocation density tensor satisfies (3.230) α ad = ε bcd β Pa.b ,c = −ε bcd β La.b ,c . The dislocation density in terms of the skew gradient of the elastic distortion is consistent with derivation (3.216). Analogously to (3.225), the second of (3.230) can be derived directly from the compatibility conditions: ε bcd β P.ab ,c = ε bcd β P.ab;c = ε bcd ( β.ba;c − β La.b;c ) = ε bcd (u;abc − β La.b;c ) (3.231) = ε bcd (u;a( bc ) − β La.b;c ) = −ε bcd β La.b;c = −ε bcd β L.ab ,c . Returning to the nonlinear description, continuity equations for the twopoint dislocation densities defined in (3.221) are deduced by integrating the fields of local Burgers vectors over closed oriented surfaces with area elements N A dS and na ds enclosing volume elements dV and dv in B0 and B , respectively: αA αA αa αa (3.232) ∫ α 0 N A dS = ∫ α 0; A dV , ∫ α L na ds = ∫ α L;a dv , S
V
s
v
where Gauss’s theorem of Section 2.7.1 has been used to convert from surface to volume integration. Considering definitions (3.222), localized continuity equations become α 0;α AA = ε ABC F Pα.B ;(CA) = 0 , α Lα;aa = ε abc F L −1α.b;( ca ) = 0 , (3.233) G
g
where symmetries of torsionfree Christoffel symbols Γ ..BCA and Γ ..bca have been exploited. Since dislocation density tensors are divergencefree, (3.233) implies that dislocation lines cannot terminate abruptly inside the crystal (De Wit 1971, 1981), but instead must terminate at other defects or at free surfaces (Teodosiu 1982; Hull and Bacon 1984). Linearized global and local continuity equations are, respectively,
144
3 Kinematics of Crystalline Solids
∫α s
ad
nd ds = ∫ α ;add dv = ∫ ε bcd β Pa.b;( cd ) ds = 0 , α ;add = 0 . v
(3.234)
s
Following Lardner (1969, 1974) the fully intermediate dislocation density tensor α is readily decomposed into contributions from positively signed dislocations ( α + ) and negatively signed dislocations ( α − ): j
α = α + + α − = ∑ ( ρ +i − ρ −i ) b i+ ⊗ ξ i ,
(3.235)
i =1
j
j
i =1
i =1
α + = ∑ ρ +i b i+ ⊗ ξ i , α − = ∑ ρ −i b i− ⊗ ξ i ,
(3.236)
with ρ+i and ρ−i the densities (line length per unit volume in B ) of positively and negatively signed dislocations, where, for each value of i, positive and negative dislocations share the same unit tangent ξ i (defined following (3.99)) but opposite Burgers vectors bi+ = −b i− and line velocities v i+ = − v i− . Recall also from Section 3.2.5 that edge dislocations are char
acterized by b ⊥ ξ , while screw dislocations are characterized by b ξ . Thus when a set of dislocations all sharing the same tangent line ξ i (but different Burgers vectors bi ) is considered, and when orthogonal coordinate axes are introduced in B with one axis aligned along ξ i , screw dislocations comprise the diagonal components of α and edge dislocations comprise the offdiagonal components of α . Werne and Kelly (1978) call α the net dislocation density tensor. In contrast, the absolute or total dislocation density tensor α T is defined as j
j
i =1
i =1
α T = α + − α − = ∑ ( ρ+i + ρ−i ) b i+ ⊗ ξ i = ∑ α iT ,
(3.237)
where α iT , the absolute dislocation density for straight dislocation line population i, is defined in (3.106). Notice from (3.105) the explicit dependence of the plastic velocity gradient LP = F P F P −1 on the summation of contributions from mobile dislocations comprising absolute dislocation density tensors α iT . Net and absolute dislocation density tensors can be further decomposed into contributions from mobile and immobile dislocations (Lardner 1969), with the latter characterized by v i+ / − = 0 and thus not affecting dislocation flux (3.99) or plastic velocity gradient (3.105). When the conditions α = α + + α − = 0 , then α T = 2α + = −2α − . When such conditions hold for all t > 0 , then the dislocation flux of (3.99) and plastic velocity gradient of (3.105) may be nonzero, but the geometrically necessary
3.3 A Linear Connection for Lattice Defects
145
dislocation density vanishes. In such cases, dislocation content of the crystal is limited to statistically stored dislocations (Ashby 1970; Arsenlis and Parks 1999). Statistically stored dislocations, also called redundant dislocations (Arsenlis and Parks 1999), consist of closed loops, dislocation dipoles, and other selfterminating dislocation structures that give no contribution to the total Burgers vector of (3.217) or the dislocation density tensor (3.235). A formal definition extending that given in a linear framework by Arsenlis and Parks (1999) is ρ Si = ρTi − ρ i , ρ Si = ρTi − ρ i = J L −1 ρ Si = J L −1 ( ρTi − ρ i ) , (3.238) where ρ Si is the scalar statistically stored dislocation density per unit intermediate volume for dislocation population i, and the total scalar density of segments of orientation i and length Li is 1 dLi ρTi = lim ∫ dLi = ≥ 0. (3.239) V →0 V dV L Summation over all populations leads to the following definitions: j j j 1 ρT = ∑ ρTi = lim ∫ dL = ρ + ρ S , ρ = ∑ ρ i , ρ S = ∑ ρ Si . (3.240) V →0 V i =1 i =1 i =1 L The scalar ρT measures the total line density of all dislocations per unit volume in the intermediate configuration. Returning to the crystal connection of (3.190), note that by (2.218), ...a L −1α Rbdc F .a = −2 F L −1α.c ,[bd ] = 0 , (3.241) ...a are the components of the RiemannChristoffel curvature tenwhere Rbdc ...a sor derived from Γ bc..a . Conditions Rbdc = 0 ensure satisfaction of (3.241), meaning that the crystal connection is integrable (Schouten 1954). Since the crystal connection is also metric (Section 2.1.3) with respect to CL from (3.170) with Qbca = 0 , and since its curvature tensor vanishes identi
cally, the set { B , Γ cd..a , CabL } constitutes a metric, nonRiemannian space. From (2.221), 2CabL Γ (..cda ) = CcbL , d + CdbL ,c − CdcL ,b . (3.242) In the particular instance wherein the torsion vanishes, i.e., Tcd..a = 0 such that Γ cd..a = Γ (..acd ) , the following statements apply: the crystal connection is symmetric (i.e., { B , Γ cd..a , CabL } becomes a nonCartan space), geometrically necessary dislocations are absent, (3.242) defines a set of LeviCivita connection coefficients akin to (2.58) on the current configuration with associated metric tensor CL , and the set { B , Γ cd..a , CabL } constitutes a Euclid
146
3 Kinematics of Crystalline Solids
ean space. In that case, (3.192) applies, meaning F L −1α.a = x.,αa . The lattice director vectors then satisfy d a ,b = Γ (..bac )d c = d b , a and d[ a ,b] = 0 , and are tangents to holonomic curves λ a ( x, t ) : d a = x.,αa dα = x.,αa ∂ / ∂λ α = ∂ / ∂λ a . 3.3.3 Disclinations
The disclination concept is used to describe rotational defects in crystals. In a general sense, such defects may encompass lowangle, highangle, and twin boundaries. Disclinations can be interpreted as equivalent arrays of dislocations with net Burgers vectors that collectively can be used to represent grain and phase boundaries. Limiting these boundaries to finite strain energy necessitates that they be composed of disclinations of finite size, i.e., partial disclinations compensated by disclination dipoles, termed disclination structural units by Nazarov et al. (2000). Finite elastoplasticity theory has been extended (Clayton et al. 2006) to incorporate continuous distributions of disclinations since such defects can describe size effects and selforganization of dislocation substructure, physical phenomena becoming increasingly evident in experimental characterization of ductile metallic crystals at finer length scales (Pantleon 1996; Hughes et al. 1998; Valiev et al. 2002). By including both dislocations and disclinations in a geometric modeling framework, distinctions naturally emerge among different classes of geometrically necessary defect densities reflecting incompatible deformation modes at multiple length scales. For example, Hughes and coworkers (Hughes et al. 1997, 1998) observed, within deforming ductile FCC metals, the formation of cells of relatively small misorientation organized collectively into larger cell blocks, with average misorientations between blocks usually greater in magnitude than those between cells. With increasing applied strain, cell block sizes generally decrease at a faster rate than do cell sizes (Hughes et al. 1997). In the context of the present geometric theory, the disclination concept can be used to capture gradients of lattice rotation (or alternatively, smoothed variations in orientations of Bravais lattice vectors) in the vicinity of cell block boundaries that arise from organization and superposition of relatively small misorientations between cells. Lattice curvature (i.e., rotation gradients) resulting from the latter (small) misorientations are reflected by geometrically necessary dislocations (Nye 1953). The disclination concept has also been used (Clayton et al. 2008a) to describe misorientations across domain walls in polarized dielectric solids such as ferroelectric ceramic crystals wherein gradients of the polarization field may reflect domain wall energies (Maugin 1988; Shu and Bhattacharya 2001; Xiao et al. 2005).
3.3 A Linear Connection for Lattice Defects
147
In the early 20th century, Volterra (1907) introduced six fundamental types of defects in elastic bodies: three types of translational displacement discontinuities, known as edge and screw dislocations, and three types of rotational incompatibilities, later termed disclinations by Frank (1958) and further classified as either wedge or twist disclinations. A detailed treatment of Volterra models of straight dislocation and disclination lines is given in Section C.1 of Appendix C, including linear elastic solutions for isolated line defects embedded in isotropic bodies of infinite extent. Disclination theory has been applied to numerous problems of interest. These include descriptions of micropolar rotations in liquid crystals (Frank 1958; Cermelli and Fried 2002), rotational defect substructures and strain hardening in metal forming (Romanov 1993; Valiev et al. 2002), grain boundary structure in crystalline solids (Li 1972; Gertsman et al. 1989), deformation twins (Mullner and Romanov 1994; Christian and Mahajan 1995), and polycrystalline triple junctions (Bollmann 1991). Disclinations have also been recognized as characteristic defects in polymers (Li and Gilman 1970) and nanocrystals (Nazarov et al. 1993; Konstantinidis and Aifantis 1998). Molecular dynamics simulations incorporating disclination concepts (Shenderova and Brenner 1999; Nazarov et al. 2000) have been undertaken to characterize grain boundary energy distributions over a range of intergranular misorientations. Spearot et al. (2005) proposed a partial disclination dipole model of distorted lattices in the vicinity of metallic grain boundaries undergoing dislocation emission. Continuum theories of distributed disclinations can be found in geometrically oriented works of Anthony (1970), Lardner (1973), Kossecka and De Wit (1977), Minagawa (1979, 1981), Amari (1981), and De Wit (1981). In a series of three papers, De Wit (1973) provides a comprehensive account of linear elastic solutions for discrete disclination lines and loops in isotropic and anisotropic solids. Texts of Nabarro (1967), Lardner (1974), Mura (1982), Maugin (1993), and Zubov (1997) also include mathematical descriptions or elastic solutions. Lazar and Maugin (2004) describe the stress field of a wedge disclination using higher gradient elasticity theory. Pecherski (1983, 1985) employs disclination concepts in continuum formulations describing finite elasticplastic kinematics, strain hardening, dislocation substructure development, and geometrical softening, the latter resulting from local lattice rotations and acting as a potential precursor to shear localization. An extensive review of disclination theory focusing upon kinetics and contributions to plastic strain hardening is provided by Seefeldt (2001), who suggests partial disclination dipoles be used to describe the collective effects of dislocations comprising misoriented subgranular interfaces (i.e., cell block boundaries) manifesting with dislocation substructure refinement in advanced stages of plastic deformation.
148
3 Kinematics of Crystalline Solids
Seefeldt et al. (2001) use dislocationdisclination models to predict texture diffusion and cellular refinement commensurate with grain subdivision. Panin (1998) and Makarov et al. (2000) emphasize the role of disclination structures accompanying finite rotations of the microstructure in metals often occurring in conjunction with shear localization triggered by microscopic heterogeneity. Classification of disclinations as fundamental defects in Bravais crystals has been an occasional subject of debate in the literature (Kroner 1983; Marcinkowski 1990; Kroner and Lagoudas 1992). This argument arises because one generally must consider a larger length scale of observation— e.g., in a discrete disclination model the distance R from the axis of rotation to the point where the discontinuity in displacement is measured—to define the displacement jump associated with a single disclination in a solid crystal than is required for an isolated dislocation, whose effects manifest at a scale on the order of the lattice parameter (i.e., the Burgers vector of a single dislocation). In fact, one may construct a nearly equivalent lattice configuration by replacing disclinations with organized arrays of translational dislocations (Li 1972; De Wit 1981; Seefeldt 2001). While such a reconstruction in terms of dislocations may be capable of capturing the stress fields associated with the original distribution of disclinations, the lattice curvature may not always be identically reproduced (De Wit 1981). Figure 3.16 shows how a simple tilt boundary may be represented either in terms of edge dislocations (Li 1960; Hull and Bacon 1984) or partial disclination dipoles (Li 1972). In Fig. 3.16, θ is the angle of misorientation, b is the magnitude of the Burgers vector, ω is the magnitude of the Frank vector (i.e., the strength of the individual disclination), h is the spacing between edge dislocations, l is the spacing between disclination dipoles, and 2R is the characteristic spacing between partial wedge disclinations comprising each disclination dipole. The tangent line of each defect, directed out of the plane of the figure, is denoted by ξ . Pure twist boundaries may be constructed from either screw dislocations or partial twist disclination dipoles in an analogous fashion (Seefeldt 2001), and general grain boundaries—including all types of coincidentsite interfaces such as deformation twins—can be built up from a mixture of dislocation or disclination types.
3.3 A Linear Connection for Lattice Defects
149
Fig. 3.16 Tilt boundary (left) comprised of edge dislocations (center) or partial disclination dipoles (right)
Partial disclinations are needed to describe lattice misorientations of strength less than 90° in cubic crystal structures and of strength less than 60° in hexagonal crystal structures. Full wedge disclinations ( ω = π / 3 ) with tangent lines normal to basal planes have been observed experimentally in hexagonal structures (Anthony et al. 1968). In Fig. 3.17, director vector d a is parallel transported about a closed loop to a new vector d′a that differs from d a by a finite rotation (Lardner 1974). The Cartan displacement about a Burgers circuit corresponding to the dashed line in Fig. 3.17 measures incompatibility induced by the disclination. The disclinated crystal structure exhibits a characteristic pentagonal shape for both (i) a negative wedge disclination with tangent line normal to a {001} plane in a cubic lattice (shown in Fig. 3.17), corresponding to insertion of a 90° wedge of material and (ii) a positive wedge disclination with tangent line normal to a basal {0001} plane in a hexagonal lattice (not shown), corresponding to removal of a 60° wedge of material (De Wit 1971; Clayton et al. 2006). Atomic coordinates differ in these two cases, however, as do elastic stress and strain fields induced by the de
150
3 Kinematics of Crystalline Solids
fect since the algebraic sign and magnitude of ω are different in each case (as are anisotropic elastic constants). Disclination dipole descriptions are generally required to allow termination of misoriented interfaces over finite distances, providing for bounded elastic energies (Li 1972; Seefeldt 2001). Since the strain energy of a disclination line or loop is proportional to ( Rω ) 2 —see, e.g., the linear elastic isotropic solutions (C.149), (C.167), and (C.170) in Sections C.1 and C.2 of Appendix C—disclinations tend to organize into dipoles to minimize (i.e., screen) the contribution of R to this energy, and tend to disocciate into partials (De Wit 1981) to minimize the contribution of ω to this energy. Partial disclinations have an associated surface energy (Li 1972), analogous to the stacking fault energy associated with partial dislocations.
Fig. 3.17 Full negative (90°) wedge disclination in cubic lattice (Lardner 1974)
A differentialgeometric description of crystalline solids containing both dislocations and disclinations, based on general concepts introduced in Section 3.3.1, is given in what follows. The linear connection coefficients Γˆ cb..a in the dislocationdisclination version of the present framework are given by (3.168), with the covariant components of Q restricted to be antisymmetric (Minagawa 1979, 1981; Clayton et al. 2006): Qcba = Qcb..d CdaL = −Qcab = Qc[ba ] , Qc( ba ) = 0 . (3.243) Kinematic variable Q, termed here a microrotation or micropolar rotation, describes spatial gradients of lattice rotation within a crystalline volume element arising from distributed disclinations. The absolute change of director vector d a is then expressed in terms of the corresponding covariant ˆ as in (3.166): derivative ∇ ˆ d = ∂ d − F Lc ∂ F L −1α d − Q d c , ∇ (3.244) b
a
b
a
.α
b
.a
c
b[ ac ]
where (3.163) has been used. Similarly, for contravariant field d a ( x, t ) ,
3.3 A Linear Connection for Lattice Defects
ˆ d a = ∂ d a + F La ∂ F L −1α d c + C L −1ad Q d c . ∇ b b .α b .c b[ cd ]
151
(3.245)
Although (3.154) and (3.155) apply for representative sets of director vectors at the centroid of the volume element under consideration, differential equations (3.193) and (3.194) do not apply when Q is nonzero. Instead, micropolar rotation Q augments the description of spatial gradients of the director vectors obtained from direct differentiation of (3.154) and (3.155). Consider parallel transport of a covariant lattice director d a , over small oriented distance dx to a new orientation d′a , conducted with respect to covariant derivative (3.244). For illustrative purposes, attention is temporarily restricted to the special case when F L ≈ 1 and spatial gradients of lattice deformation tensor F L are negligible. In that case, ∂ b d a = Qb[ac ]d c , and d′a = d a + d a ,b dx b = d a + Qb[ac] dx b d c = (δ ac + dx bQb[ac] )d c = Φac d c , (3.246) where rotation matrix Φac satisfies ΦT ≈ Φ−1 and det Φ ≈ 1 for small magnitudes of dx b Qb[ac] , i.e., small relative lattice rotations such as those occurring across lowangle grain or subgrain boundaries (Brandon 1966). Notice from (3.246) that Qbac acts in effect as a gradient of rotation in the direction of xb . However, since Q is not required to satisfy the following compatibility conditions, it is not a true gradient: Qb[ac ], d − Qd [ac],b ≠ 0 → Qb[ac ] ≠ ψ [ac ],b , (3.247) where ψ [ ac] is a skew matrix that exists only when Qb[ ac],d = Qd [ ac],b . In general situations, components of F L and its spatial gradient may be arbitrarily large. From (3.170), connection (3.168) restricted by conditions (3.243) is metric, since the covariant derivative of CL vanishes: ˆ C L = −2Q ∇ =0. (3.248) c ab c ( ab ) Components of the torsion tensor of connection Γˆ bc..a are given by Tˆbc..a = Tbc..a + Q[..bca ] = F La.α F L −1α.[c ,b] + Q[..bca ] , (3.249) where Tcb..a is the torsion of the crystal connection discussed in Section 3.3.2. Covariant components of the RiemannChristoffel curvature tensor are, from (3.175) and (3.176), ˆ Q ˆ ..e Rˆ ab[cd ] = 2∇ [ a b][cd ] + 2Tab Qe[cd ] , (3.250) ˆ Q ˆ ..e Rˆ ab( cd ) = 2∇ [a b]( cd ) + 2Tab Qe( cd ) = 0.
152
3 Kinematics of Crystalline Solids
Thus, from the second of (3.250), the curvature tensor of the connection with micropolar rotations consists of up to nine independent components: Rˆ abcd = Rˆ [ab][cd ] . Consider a Burgers circuit c in the current configuration, enclosing area a comprised of oriented differential elements ε bcf n f da = dx b ∧ dx c . A total Burgers vector accounting for incompatibility induced by torsion and curvature may be identified with the Cartan displacement of (3.179) (Kondo 1964; Lardner 1973; Minagawa 1979): 1 Bˆ a = − ∫ Tˆbc..a dxb ∧ dx c − ∫ C L −1ae Rˆbc[ de] x d dx b ∧ dx c 2a a (3.251) 1 bcf ..a bcf L −1ae ˆ d ˆ . = −ε ∫ Tbc n f da − ε ∫ C Rbc[de] x n f da 2 a a Total Burgers vector (3.251) reduces to that of (3.213) when disclinations ...a are absent (i.e., when Tˆbc..a = Tbc..a , Qbc..a = 0 , and Rˆ bcd = 0 ) . One can rewrite (3.251) in terms of the secondorder geometrically necessary dislocation tensor α and secondorder geometrically necessary disclination tensor θ , each referred to spatial configuration B: Bˆ a = ∫ (α af + C L −1aeε ehd θ hf x d )n f da , (3.252) a
where components of the defect density tensors are, in indicial notation13, 1 α af = ε fbcTˆcb..a , θ gf = ε gdeε fbc Rˆ cbde . (3.253) 4 The disclination density tensor of the second of (3.253) becomes equivalent to the negative transpose of Einstein’s tensor of (2.38) when ε cab ⇒ ecab (det CL ) −1/ 2 . Rank two defect density tensors α and θ of ˆ and rank (3.253) enable full reconstruction of rank three torsion tensor T ˆ : four curvature tensor R 1 ..a ad fe ˆ ˆ Tˆcb..a = Tˆ[cb (3.254) ] = ε bcd α , Rabcd = R[ ab][ cd ] = ε baeε cdf θ . 2 The tensors of (3.252) are related to summed contributions of discrete defects as j
l
i =1
k =1
α = ∑ ρ i bi ⊗ ξ i , θ = ∑η k ω k ⊗ ξ k .
(3.255)
13 As with the dislocation density, the algebraic sign and placement of indices used to define the disclination density tensor vary among authors (Minagawa 1979, 1981; De Wit 1981; Clayton et al. 2005, 2006, 2008).
3.3 A Linear Connection for Lattice Defects
153
In (3.255), ρ i , bi , and ξ i are the scalar dislocation line density, Burgers vector, and tangent line, respectively, for dislocation population i = 1, 2,... j , while η k , ω k , and ξ k are the scalar disclination line density, Frank vector, and tangent line, respectively, for disclination population k = 1, 2,...l . Complete and partial disclinations may contribute to θ . The physical definition of the dislocation density tensor α in the first of (3.255) is identical to (3.215), but the mathematical definition in the first of (3.253) differs from that in (3.214) when Q[..acb] ≠ 0 . For an element of crystal containing a single dislocation population with uniform Burgers vector and tangent line, and a single disclination population with uniform Frank vector and tangent line, substitution of (3.255) into (3.252) gives Bˆ a = ∫ b a ( ρξ f n f ) da + ∫ ε ehd ω h x d (C L −1aeηξ f n f )da , (3.256) a
a
which in turn is the nonlinear analog of displacement jump relation (C.5) for a single Volterra line defect given in Section C.1 of Appendix C. Complete pullbacks of α and θ to the intermediate configuration B are written α αβ = J L F L −1α.aα ab F L −1.βb (3.257) = J Lε bcd F L −1α.c ,d F L −1.βb + J L F L −1α.aε bcd Q[..dca ] F L −1.βb , 1 (3.258) 4 with J L the Jacobian determinant of F L found from (3.48). Notice that (3.257) is consistent with (3.224), and hence (3.226) and (3.227) apply as transformation formulae for dislocation tangent lines, scalar numbers of dislocations per unit volume, and local Burgers vectors. Analogous transformation formulae can be assigned to disclination tangent lines, scalar numbers of disclinations per unit volume, and local Frank vectors in (3.255): ξ k a = F L .aα ξ k α = F. Aaξ 0k A , η k = J L −1η k = J −1η0k , ω k b = F Lb.α ω k α , (3.259)
θ αβ = J L F L −1α.aθ ab F L −1.bβ = J L F L −1α.aε adg ε bce Rˆ [ce][ gd ] F L −1.bβ ,
where tilded quantities are defined on B , and quantities with zero subscripts are defined in reference configuration B0 . The analog of (3.226) is then l
l
k =1
k =1
θ ba na da = ∑η k ω k bξ k a na da = ∑η k ω k β ξ k α nα da = θ βα nα da .
(3.260)
Kinematic variables α and θ may be regarded as “elastic” in the sense that they are derived completely from lattice kinematic quantities F L and
154
3 Kinematics of Crystalline Solids
Q and/or spatial gradients of F L and Q, and not from plastic deformation F P or its higherorder gradients. As discussed in Section 3.3.2, α does not account for curved defect segments and combinations of defect lines that do not contribute to the total Burgers vector. Hence, the same definitions introduced in (3.235)(3.240) can be used to define total dislocation density tensors, scalar total dislocation densities, and scalar statistically stored dislocation densities. The same statements apply to the geometrically necessary disclination density tensor θ : this tensor does not account for combinations of defect lines and loops whose local Frank vectors cancel and hence do not contribute to the total Burgers vector (3.252). The disclination density can be decomposed into contributions from positively signed disclinations ( θ + ) and negatively
signed disclinations ( θ − ): l
θ = θ + + θ − = ∑ (η +k − η −k ) ω +k ⊗ ξ k ,
(3.261)
k =1
where l
l
k =1
k =1
θ + = ∑η +k ω +k ⊗ ξ k , θ − = ∑η −k ω −k ⊗ ξ k ,
(3.262)
with η+k and η −k the densities (line length per unit volume in B ) of positively and negatively signed disclinations, where, for each value of k, positive and negative disclinations share the same tangent ξ k but opposite Frank vectors ω k+ = −ω −k and if mobile, line velocities v k+ = − v −k . As explained in Section C.1 of Appendix C, twist disclinations are characterized by ω ⊥ ξ , while wedge disclinations are characterized by ω ξ . Thus when a set of disclinations all sharing the same tangent line ξ k (but different Frank vectors ω k ) is considered, and when orthogonal coordinate axes are introduced in B with one axis aligned along ξ k , wedge disclinations comprise the diagonal components of θ and twist disclinations comprise the offdiagonal components of θ . In contrast to (3.261), an absolute or total disclination density tensor θT is defined as (Clayton et al. 2006) l
θT = θ + − θ − = ∑ (η+k + η−k )ω +k ⊗ ξ k .
(3.263)
k =1
When the conditions θ = θ + + θ − = 0 apply, then θ T = 2θ + = −2θ − . When such conditions hold, then the total disclination line length L in the crystal
3.3 A Linear Connection for Lattice Defects
155
may be nonzero, but the geometrically necessary disclination density vanishes. In such cases, the disclination content of the crystal is limited to statistically stored disclinations, analogous to statistically stored dislocations (Ashby 1970; Arsenlis and Parks 1999) discussed in Section 3.3.2. Statistically stored disclinations give no contribution to the total Burgers vector of (3.252) or the disclination density tensor (3.261). A formal definition for the scalar density η Sk of statistically stored disclinations of population k per unit intermediate volume is η Sk = ηTk − η k , η Sk = ηTk − η k = J L −1η Sk = J L −1 (ηTk − η k ) , (3.264) where the total scalar density of segments of orientation k and length Lk is 1 dLk ηTk = lim ∫ dLk = ≥0. (3.265) V →0 V dV L Summation over all l populations leads to the following definitions analogous to those given for scalar dislocation densities in (3.240): l l l 1 ηT = ∑ηTk = lim ∫ dL = η + η S , η = ∑η k , η S = ∑η Sk . (3.266) V →0 V k =1 k =1 k =1 L Notice that disclination dipoles, when summed over a finite volume, give no contribution to the value of θ or θ for that volume, and hence no contribution to the total Burgers vector. In order to measure the misorientation attributed to a wall of disclination dipoles as in Fig. 3.16, one must consider in (3.252) the local field θ( x) consisting of contributions of infinitesimal Frank vectors ω( x) with tangent lines ζ( x) piercing area a enclosed by the Burgers circuit. Even though the average Frank vector of the disclination density tensor may vanish over the entire area, e.g., ab ∫ θ nb da = 0 , the distribution of disclinations within the area can still produce a nonzero total Burgers vector because of the presence of coordinates x d in (3.252). Alternatively, by treating each dipole as a single disclination with terminated radius of influence and effective Frank vector of magnitude 2 Rω / l (refer to Fig. 3.16), one can use an average value of (3.261) to compute the nonzero contribution of an array of disclination dipoles to the total Burgers vector or to the lattice misorientation across a boundary, as discussed at the conclusion of Section 3.3.3. The stress field and strain energy of such an array of dipoles would differ from that of a distribution of disclinations of the same sign producing the same total Burgers vector. Continuity equations for dislocation and disclination density tensors in the current configuration follow from Schouten’s identity (2.48) and Bianchi’s identity (2.50):
156
3 Kinematics of Crystalline Solids
ˆ Tˆ ..a − 4Tˆ ..eTˆ ..a , ∇ ˆ Rˆ ...a = 2Tˆ .. f Rˆ ...a . Rˆ[...bcda ] = 2∇ [b cd ] [bc d ]e [e bc ]d [eb c ] fd
(3.267)
Substitution of (3.254) gives for the first of (3.267): ˆ α aeε + ε C L −1aeε [bc g ε d ]ef θ fg = ∇ ε α agα ef , cd ]e [b ⎡bc f d ]eg
(3.268)
and for the second of (3.267): ˆ (C L −1ag ε ε θ fh ) = ε α fk C L −1ag ε ε θ mh . ∇ cb] h dgf c ] hf dgm [e [be k
(3.269)
⎣
The geometrically linear dislocationdisclination theory is now formally considered. From (3.181), (3.186), (3.187), and (3.189), using (3.243): Γˆ cb..a ≈ − β La.b ,c + Qcb..a ; (3.270) 1 Γˆ c( ba ) ≈ ∂ c C L ( ba ) , Γˆ c[ba] ≈ ∂ c β L[ba] + Qc[ba] ;
(3.271)
Τˆcb..a ≈ β La.[c ,b] + Q[..cba ] ;
(3.272)
Rˆ bc[da ] ≈ 2∂ [b Qc ][da ] , Rˆ bc ( da ) = 0 .
(3.273)
2
The second of (3.271) can be written as Γˆ c.[ba] ≈ ∂ c Ω L[ba] + Qc.[ba] = ε abd κ dcL ,
(3.274)
where elastic bendtwist κ and micropolar rotation ϕ are defined by 1 1 κ abL = − ε acd Ω..,Lb[cd ] − ϕab , ϕ ab = ε acd Qb.[cd ] . (3.275) 2 2 The dislocation density tensor of (3.253) becomes α af = ε fbc ( β La.c ,b + Qcb..a ) = ε fbc ( β La.c,b + δ bd ε daeϕec ) , (3.276) while the disclination density tensor in (3.253) can be expressed as 1 1 θ gf = ε gdeε fbc ∂[c Qb][de] = ε gdeε fbcε deh ∂[cϕ.hb] = ε fbcϕ.gb ,c . (3.277) 2 2 Continuity equations in the linearized case can then be obtained by direct substitution into (3.268) and (3.269), replacing covariant derivatives with partial derivatives and omitting higherorder terms: δ aeε [bc g ε d ]ef θ fg = ∂ [b α aeε cd ]e , (3.278) L
ε daf ∂ [eθ fhε bc ]h = 0 .
(3.279)
In the context of a geometrically linear formulation, De Wit (1981) inferred from equations analogous to (3.279) that disclination lines cannot end abruptly within a crystalline body, and from equations analogous to (3.278) that disclinations may act as sources or sinks for dislocations. Consider now the threeterm decomposition of (3.137), wherein the lattice deformation is decomposed as F L = F E F I = V E R E R I U I . Following Lardner (1973, 1974), the rotational part R I of F I , when the former is at
3.3 A Linear Connection for Lattice Defects
157
tributed solely to disclinations within a volume element of crystal, can be associated with the change in orientation of a vector with unit components ( x d → 1 in (3.251)) upon parallel transport around a closed circuit of area a containing a nonvanishing disclination density θ (Clayton et al. 2006): ⎛ ⎞ 1 ...a b R I α.β = g.αa ⎜ δ .ad − ∫ Rˆbcd dx ∧ dx c ⎟ g.dβ 2a ⎝ ⎠ = δ .αβ + g.αa g.dβ ∫ C L −1aeε ehdθ hf n f da a
≈δ
α .β
+ g.a g C L −1aeε ehd ∫ θ hf n f da α
d .β
(3.280)
a
= δ .αβ + g.αa g.dβ C L −1aeε deh Ωˆ h ≈ g α e g.dβ (δ de + ε deh Ωˆ h ), and where in the third equality of (3.280), a constant lattice stretch has been assumed over a, such that the net Frank vector Ωˆ h = ∫ θ hf n f da acts in Cartesian coordinates as the axial vector of R I − 1 , meaning that R I is truly orthogonal only in the limit of small lattice stretch and small rotations as implied in the final expression. Notice that (3.280) is nonunique in the sense that R I depends on choice of oriented area element nda . In a crystal plasticity framework (Section 3.2.6), one possible means of addressing this integral involves a discrete sum over area elements on representative set of crystallographic planes (e.g., lowindex or slip planes) (Clayton et al. 2006). A more general approach advocated here, accounting for all possible orientations n, is prescription of the domain of integration in (3.280) as a spherical halfshell (in orientation space) of radius l : R I α.β = δ .αβ + l 2 g.αa g.dβ
π π
∫ ∫C
L −1ae
ε ehdθ hf n f (sin φ )(dφ )( dϕ ) ,
(3.281)
0 0
where θ hf is expressed in rectangular coordinates, unit normal components are n1 = sin 2φ cos 2ϕ , n2 = sin 2φ sin 2ϕ , and n3 = cos 2φ , and l 2 corresponds to the effective area over which the disclinations act. In the limit that the crystal volume element shrinks to infinitesimal size (see Fig. 3.12), l → 0 , and effects of disclinations cannot be resolved by the multiplicative decomposition of the deformation gradient (3.137). Dislocationdisclination theory may be applied to describe evolution of cellular defect substructures observed in ductile metallic crystals deformed at low homologous temperatures to relatively large total strains (Stout and Rollett 1990; Pantleon 1996; Hughes et al. 1997, 1998; Valiev et al. 2002).
158
3 Kinematics of Crystalline Solids
As shown in the left part of Fig. 3.18, this substructure consists of nearly equiaxed cells with interiors of relatively low defect density, separated by incidental dislocation boundaries (IDBs) across which lattice misorientations are generally of the lowangle variety, for example, limited to less than 10° in aluminum and nickel coldrolled to 100% effective strain (Hughes et al. 2003). With increasing applied strain, the cells tend to organize collectively into bands or cell blocks, often elongated in shape in a direction depending upon the initial texture and loading conditions. The cell blocks are separated by dislocation walls termed geometrically necessary boundaries (GNBs), across which misorientations can reach highangle magnitudes, i.e., in excess of 15°. Both GNBs and IDBs are thought to contain mixed populations of statistically stored and geometrically necessary dislocations (Hughes et al. 2003).
Fig. 3.18 Dislocation substructure (left) and lattice director vectors (right) in a severely plastically deformed (SPD) single crystal
In the context of the present geometric framework, kinematics of defect substructure can be described as follows. Redundant dislocations and disclinations that contribute no net misorientation are grouped collectively into statistically stored dislocation and disclination scalars: line lengths per unit spatial volume ρ S and ηS , respectively, as introduced following (3.238) and (3.264), respectively. Geometrically necessary dislocations comprising α represent nonredundant defects corresponding to fluctuations in lattice orientation in the vicinity of the cell boundaries, i.e., IDBs. Micropolar rotation variable Q (in conjunction with associated net disclination density tensor θ ) measures the nonredundant defect content of the cell block boundaries, i.e., GNBs. Fractions of dislocations and disclinations that are nonredundant or geometrically necessary as opposed to redundant or statistically stored may differ since they represent different features of the microstructure.
3.3 A Linear Connection for Lattice Defects
159
The general theory developed in Section 3.3.3 places no restriction on characteristic spacing or strength (i.e., magnitude of angle) of the misoriented boundary to which is attributed a particular type of defect density. For example, dislocations could alternatively comprise GNBs and disclinations could comprise IDBs, or a mixture of defect types could comprise each kind of boundary. The decision to model GNBs with the disclination density and IDBs with the dislocation density stems from both convenience and from physical considerations in agreement with models set forth in prior literature (Panin 1998; Seefeldt 2001). Thus, the rotational units that serve to accommodate inelastic deformation and subgranular incompatibility seen at comparatively large strains are associated with disclinations (GNBs), with geometrically necessary dislocations capturing the local misorientations across IDBs arising at a smaller length scale. From this standpoint, with inelastic straining, dislocations accumulate first, and then later organize into disclination structures at larger applied deformations (Seefeldt 2001; Valiev et al. 2002). The microrotation concept in the context of GNBs and IDBs is illustrated on the right side of Fig. 3.18. Let x and x′ be spatial coordinates of material points in neighboring cell blocks, with corresponding lattice director vectors d a and d′a . Recall that by definition, in configuration B director vector triads are parallel, leading to dα = dα′ . (3.282) Let F L and F L′ denote the local lattice deformations at x and x′ , respectively. Premultiplying both sides of (3.282) by F L′−1 results in
⎡ ⎤ F L′−1α.a − F L −1α.a c d′a = ⎢ F L −1α.a + (3.283) ( x′ − x c ) ⎥ F Lb.α db . c c x′ − x ⎢⎣ ⎥⎦ ˆ d = 0 ), From (3.166), (3.168), and assertion of parallel transport (i.e., ∇ b a L −1α L −1α c L −1α ..d c Lb d′a = ( F .a + F .a ,c dx + F .d Qca dx ) F .α db , (3.284) where dx c = x′c − x c and d′a − d a ≈ d a ,b dx b .
Comparing (3.283) and
(3.284), Q reflects the possible inability of the first spatial gradient of F L −1 to capture the change in the directors over small distance dx c : ⎛ F L′−1α − F L −1α ⎞ L −1α .a .a − (3.285) Qca..d = F L.dα ⎜ F .a , c ⎟ . ⎜ ⎟ dx c ⎝ ⎠ One can think of Q as implicitly representative of cumulative effects of all higher than firstorder gradients of the (inverse) lattice deformation F L −1 on the spatial variation of the lattice directors. In many higherorder gra
160
3 Kinematics of Crystalline Solids
dient crystal plasticity theories from the more recent literature (Naghdi and Srinivasa 1993; Le and Stumpf 1996a, b, c; Shizawa and Zbib 1999; Acharya 2001; Bammann 2001; Regueiro et al. 2002; Garikipati 2003; Clayton et al. 2004b), the firstorder gradient of the elastic or plastic deformation influences the material response, for example through its manifestation in the dislocation density tensor. However, by including the microrotation variable Q, potentially nonlinear spatial variations in lattice directors between neighboring material points are captured. This nonlinearity arises in the dislocation density α and in the disclination density θ through variable Q and its spatial gradient, respectively. It is noted that Qbc..a is not an explicit function of higherorder lattice deformation gradients F L −1α.a ,bc , F L −1α.a ,bcd ,... ; rather, Q is an independent kinematic variable. The disclination concept has been extended to describe domain boundaries in spontaneously polar perovskite crystals (Clayton et al. 2008a). Consider a finite wedge disclination density—e.g., a set of partial wedge disclination dipoles (Li 1972)—with net nonzero component θ 11 = ηω , meaning both the axis of rotation ( ζ ) and the effective rotation vector ( ω ) are aligned along the x1direction in the sample. An effective disclination density tensor in this case can be used to represent a tilt boundary with misorientation vector aligned along the x1direction. In this construction, each dipole is replaced with a single disclination line of strength ω whose Frank vector terminates at a distance R from the core of the defect, i.e., at the position of the other disclination line comprising the dipole in Fig. 3.16. To represent domain walls in barium strontium titanate (BST), for example, let η ∝ 1/ l D2 where l D is the typical domain or grain size, on the order of 50 nm in representative BST thin films (Cole et al. 2003). Referring to Fig. 3.16, for a standard lowangle boundary, θ ≤ π /12 (Brandon 1966), while θ = π / 2 and θ = π are energetically favorable misorientations across domain walls in noncubic phases of some kinds of ferroelectric crystals (Shu and Bhattacharya 2001). For closely packed disclination dipoles, 2 R = l and θ = ω in Fig. 3.16. 3.3.4 Point Defects
Attention is now focused on a geometric representation of uniformly distributed point defects within a volume element of a crystal structure. Recall that the contribution F V of such defects to the lattice deformation F L of the total deformation gradient F for such an element is described in Section 3.2.8, specifically in (3.128)(3.136). The corresponding micro
3.3 A Linear Connection for Lattice Defects
161
scopic description, at a more refined length scale of explicitly resolved gradients in the lattice directors, is given in what follows. The same connection coefficients Γˆ ..a ( x, t ) listed in (3.168) are used, but the form of Q bc
is restricted as (Minagawa 1979, 1981; Clayton et al. 2005, 2008a) Γˆ cb..a = F La.α F L −1α.b ,c + Qcb..a = Γ cb..a + ϒ cδ .ba , Qcb..a = ϒ cδ .ba , (3.286) while the covariant version of Q is Qcba = ϒ c CbaL = ϒ c C(Lba ) . From (3.166),
ˆ d dx c = d dx c − Γ ..b dx c d − ϒ dx c d , ∇ c a a,c ca b c a
(3.287)
ˆ d is an implying that the contribution from point defects to derivative ∇ c a isotropic stretch of magnitude  ϒ c dx c  . Considering for the moment the case when the crystal connection coefficients vanish and the directors undergo parallel transport, and letting dx c = x′c − x c , (3.287) results in (3.288) d′a = d a + d a ,c dx c = (1 + ϒ c dx c )d a , ∂ c d a = ϒ c d a . The connection in (3.286) is nonmetric, since by (3.170), ˆ C L = −2ϒ C L , (3.289) ∇ c ab c ab meaning physically that vacancies, interstitials, or voids alter the counting of atomic steps in the crystal (Kroner 1981, 1990). The torsion tensor is, upon substitution of (3.286) into (3.171), Tˆcb..a = Tcb..a + ϒ [cδ .ba] , (3.290) From (3.174) or (3.175), skew components of the covariant RiemannChristoffel curvature tensor vanish identically since CabL is symmetric: ˆ ϒ C L + 2Tˆ ..eϒ C L = 0 . Rˆ = 2∇ (3.291) [bc ][ da ]
[b
c]
[ da ]
bc
[ da]
e
From (3.176), symmetric components of the curvature tensor are ˆ ϒ + Tˆ ..eϒ )C L = 2(∂ ϒ − Γˆ ..e ϒ + Tˆ ..eϒ )C L Rˆ = 2(∇ [bc]( da )
[b
c]
bc
e
da
[b
c]
[bc]
e
bc
e
= 2∂[bϒ c]C . L da
da
(3.292)
The total Burgers vector resulting from Cartan displacement (3.179) is 1 ⎡ ⎤ Bˆ a = − ∫ ⎢Tˆbc..a + C L −1ae Rˆbc ( de ) x d ⎥ dxb ∧ dx c 2 ⎦ a ⎣ = − ∫ (Tbc..a + ϒ [bδ .ca] ) dx b ∧ dx c + ∫ϒ [b ,c ] x a dx b ∧ dx c a
= −ε
a
bce
∫ (T
..a bc
a
+ ϒ δ ) ne da + ε bce ∫ϒ [b ,c ] x a ne da a [b .c ]
a
= ∫ α ae ne da + ∫ x aϑ e ne da, a
a
(3.293)
162
3 Kinematics of Crystalline Solids
where the dislocation density tensor α is defined in terms of the torsion in the same way as in (3.253) and (3.254): (3.294) α ae = ε cbeTˆbc..a = ε cbe F La.α F L −1α.c ,b − ε cbeϒ cδ .ba , 2Tˆbc..a = ε cbeα ae , and components of the point defect vector (Clayton et al. 2008a) satisfy14 ϑ e = ε ebcϒ b,c = ε ecb (∇ˆ [bϒ c] + Tˆbc..eϒ e )
1 ˆ ϒ + Tˆ ..eϒ ) = δ .aaε ecb (∇ bc e [b c ] 3 (3.295) 1 ˆ ϒ + 2Tˆ ..eϒ )C L = C L −1ad ε ecb (2∇ bc e ( da ) [b c ] 6 1 = C L −1ad ε ecb Rˆ[bc]( ad ) . 6 When (3.291) applies, the disclination density of (3.253) and (3.254) vanishes. Dislocation density α has the same physical interpretation as that given in (3.215) of Section 3.3.2, but differs mathematically from (3.214) by the term ε bceϒ [cδ.ba] . From (3.295), it follows that 2ϒ [b ,c] = ε bcdϑ d . A local differential Burgers vector induced by the point defect vector is ⎡ δχ e ⎤ a dBˆ a = x aϒ b ,c dxb ∧ dx c = x aϑ e ne da = x a ⎢ b ⎥ ne da = x δχ , (3.296) dx dx b ⎦ ⎣ where the following definitions apply:
δχ e = neδχ = ϑ e da = ϑ e dxb dxb , δχ = δχ eδχ e , da = dxb dxb . (3.297) From (3.296) and (3.297), one then may write x a + dBˆ a = (1 + δχ ) x a = (1 + ϑ e ne da ) x a , (3.298) where δχ represents a microscopic isotropic expansion ( δχ > 0 ) or contraction ( δχ < 0 ). Consider the case when the point defects correspond to atomic vacancies in the lattice. Analogous to the situation for continuous distributions of dislocations discussed in Section 3.3.2, let the radius of each vacancy shrink to zero and the number of vacancies in each volume element tend to infinity, such that their product remains finite. Let δχ represent a constant spherical stretch of the lattice produced by a concentration of vacancies at the origin x a = 0 . Coordinates of a nearby point x′ after application of this microstretch are then (1 + δχ ) x′a . A ,simple physically motivated assumption is that δχ is equivalent to the vacancy concen14 A factor of 1/6 was unintentionally omitted in (23) of Clayton et al. (2008a). 1 That misprint is corrected here in (3.295). The opposite sign convention was used in that work for the Cartan displacement.
3.3 A Linear Connection for Lattice Defects
163
tration at x minus that at x′ (Clayton et al. 2008a). Bianchi’s identity in the second of (3.267) becomes for the present case ˆ ϒ = Tˆ .. f ∂ ϒ ⇔ ∇ ˆ ϑ aε = ε α fa ∂ ϒ , ∇ (3.299) cb ]a c] f [e c ,b ] [eb c ] f [e ⎡be a ⎣
providing a continuity equation for the point defect vector. The geometrically linear theory is now reconsidered for crystals with dislocations and point defects. From (3.181), (3.186), (3.187), and (3.189), using (3.286): Γˆ cb..a ≈ − β La.b,c + ϒ c δ .ba ; (3.300) 1 2
Γˆ c( ba ) ≈ ∂ c C L ( ba ) + ϒ c C L ( ba ) , Γˆ c[ba] ≈ ∂ c β L[ba] ;
(3.301)
Τˆcb..a ≈ β La.[c ,b] + ϒ [cδ .ba] ;
(3.302)
Rˆ bc[ da] = 0 , Rˆbc ( da ) ≈ 2∂[bϒ c]δ da .
(3.303)
The dislocation density tensor of (3.294) and point defect vector of (3.295) are α af ≈ ε fbc ( β L.ac ,b + ϒ [cδ .ba] ) , ϑ e = ε ebcϒ [b,c] , (3.304) where the latter evidently is the same in both linear and nonlinear descriptions. The linear disclination density tensor in (3.277) vanishes. The continuity equation (3.299) in linearized form is ∂ [eϒ c ,b] = 0 ⇔ ∂ [eϑ aε cb]a = 0 . (3.305) Consider now a linear connection formed by superposition of components of the crystal connection with skew and symmetric components of Q introduced, respectively, in (3.243) and (3.286): Γˆ cb..a = Γ cb..a + C L −1ad Qc[bd ] + ϒ cδ .ba , (3.306) where C L −1ad Qc[bd ] accounts for disclinations according to Section 3.3.3 and ϒ cδ .ba accounts for point defects as discussed above. In this case, ˆ C L = −2ϒ C L , ∇ (3.307) c
ab
c
ab
1 Tˆcb..a = Tcb..a + C L −1ae (Qcbe − Qbce − Qceb + Qbec ) + ϒ [cδ .ba] . (3.308) 4 Skew components of the covariant RiemannChristoffel curvature tensor are identical to the first of (3.250): L ˆ Q ˆ ..e Rˆ[bc][ da] = 2∇ [b c][ da ] + 2Tbc Qe[ da ] + ϒ [bϒ c ] C[ da ] (3.309) ˆ Q ˆ ..e Q . = 2∇ + T 2 bc e[ da ] [b c][ da ] From (3.176), symmetric components of the curvature tensor are identical to (3.292):
164
3 Kinematics of Crystalline Solids
ˆ ϒ + Tˆ ..eϒ )C L = 2∂ ϒ C L . Rˆ[bc]( da ) = 2(∇ bc e da [b c ] [b c ] da
(3.310)
The total Burgers vector resulting from Cartan displacement (3.179) is 1 1 ⎡ ⎤ Bˆ a = − ∫ ⎢Tˆbc..a + C L −1ae Rˆbc[de] x d + C L −1ae Rˆbc ( de ) x d ⎥ dxb ∧ dxc 2 2 ⎦ a ⎣ 1 = − ∫ Tˆbc..a dxb ∧ dxc − ∫ C L −1ae Rˆbc[de] x d dxb ∧ dxc + ∫ϒ [b ,c ] x a dxb ∧ dxc 2a a a (3.311) 1 bcf bcf L −1ae ˆ d bcf a ..a ˆ Rbc [de ] x n f da + ε ∫ϒ [b ,c ] x n f da = −ε ∫ Tbc n f da − ε ∫ C 2 a a a
= ∫ α af n f da + ∫ C L −1aeε ehdθ hf x d n f da + ∫ x aϑ f n f da, a
a
a
where spatial components of the defect density tensors are, in indicial notation, 1 α af = ε fbcTˆcb..a , θ gf = ε gdeε fbc Rˆ cbde ; (3.312) 4 1 ϑ f = ε bcf ϒ b ,c = C L −1deε fbc Rˆ[cb]( de ) . (3.313) 6 Definitions (3.312) and (3.313) agree with (3.253) and (3.295), and can be inverted to reconstruct the torsion and curvature tensors: 2Tˆcb..a = ε bcf α af , Rˆ cb[ de] = ε fbcε gdeθ gf , Rˆcb( de) = ε bcf ϑ f CdeL . (3.314) Substitution of (3.314) into identities (3.267) then provides continuity equations relating dislocation and disclination density tensors, the point defect vector, and their covariant derivatives: ˆ α aeε + ε C L −1aeε [bc g ε d ]ef θ fg + δ .[ad ε bc] f ϑ f = ∇ ε α agα ef , (3.315) cd ]e ⎡ bc f d ]eg [b ⎣
ˆ (C L −1ag ε ε θ fh ) + ∇ ˆ ϑ fε δ a ∇ cb ]h dgf cb ] f . d [e [e 1 = ε [be k α fk C L −1ag ε c]hf ε dgmθ mh + ε [be k α fk ε c] gf ϑ g δ .ad . 2
(3.316)
3.3.5 Summary
The theory presented in Section 3.3 is founded upon two major assumptions, the first being multiplicative decomposition (3.31), F = F L F P , of the average deformation gradient F for a volume element of a crystalline solid, where plastic deformation attributed to the flux of mobile crystal defects, F P , is latticepreserving or lattice invariant, and where F L accounts for stretch and rotation of the lattice. Lattice deformation F L can be further
3.3 A Linear Connection for Lattice Defects
165
decomposed into recoverable and residual parts according to (3.137), but such an enhanced description is not necessary in the context of Section 3.3. The second major assumption is an additive decomposition of a linear connection describing spatial gradients of lattice director vectors between neighboring crystalline elements, i.e., a microscopic description. Coefficients of this connection, introduced in (3.168), may be written as Γˆ cb..a = F La.α ∂ c F L −1α.b + C L −1ad Qc[bd ] + δ .baϒ c + C L −1ad (Qc( bd ) − ϒ c CbdL ) (3.317) crystal connection (dislocations)
microrotation (disclinations)
microdilatancy (point defects)
microstrain (Somigliana dislocations)
where the first term on the right side of (3.317) describes gradients of the director vectors attributed to firstorder spatial gradients of the average lattice deformation tensor F L at the centroid of the volume element, following Bilby et al. (1955), as discussed in Section 3.3.2. Micromorphic variable Q (Minagawa 1979; De Wit 1981; Clayton et al. 2005, 2008a) participates in the remaining three terms on the right of (3.317): a microrotation associated with disclinations as discussed in Section 3.3.3, a spherical micromorphic expansion or contraction associated with point defects as discussed in Section 3.3.4, and a general micromorphic strain that may be used to represent arbitrary lattice director deformations when combined with the other terms in (3.317). Defect densities then follow from contributions of the torsion and curvature of the connection to the Cartan displacement defined generically in (3.177). When the rightmost term is absent in (3.317) and Qc(bd ) = ϒ c CbdL , then suitable definitions for defect densities are given in (3.312)(3.313). On the other hand, when Qc( bd ) ≠ ϒ c CbdL , alternative definitions of defect densities are possible. Table 3.5 provides classifications of the affine geometries corresponding to various crystal defects (Clayton et al. 2005), following the geometric terminology of Section 2.1.1 and motivated by Steinmann (1996). The present framework has been developed with the primary intent of describing crystalline solids that deform plastically by dislocation glide, most typically exhibiting a Bravais lattice structure and most often realized in engineering metals in a face centered cubic, body centered cubic, or hexagonal close packed arrangement (Tables 3.2 and 3.4). Concepts that have been forwarded here are most naturally applied to cubic lattices, wherein the director vectors of (3.155) may be assigned parallel to primitive translation vectors of the Bravais lattice as in (3.164) (recall from Section 3.1.1 that primitive Bravais lattice vectors and their reciprocals are parallel in cubic crystals). The framework is valid for crystal structures of lower symmetry (e.g., hexagonal Bravais lattices) so long as the CauchyBorn rule (Section 3.1.2) applies for deformation of the interatomic bond vec
166
3 Kinematics of Crystalline Solids
tors. In such cases, while the covariant directors of relations (3.155) assigned to each crystalline volume element are not parallel to physical edges of primitive or conventional unit cells of the Bravais lattice, they are assumed to fully characterize the stretch and rotation of interatomic vectors comprising the primitive cells contained in that volume element, as is clear from (3.165). On the other hand, for more complex structures wherein recoverable (i.e., elastic) deformation is nonuniform within the unit cell, e.g., polyatomic structures such as noncentrosymmetric crystals with a basis undergoing inner displacements among sublattices (Cousins 1978; Garikipati 2003), additional degrees of freedom not included in Section 3.3 may prove useful for characterizing certain kinds of defects that affect the geometry of each sublattice differently. Table 3.5 Geometric classifications, kinematic quantities, and lattice defects Geometry
Torsion
Metric
Defects
ˆ =0 T
Curvature ˆ =0 R
Euclidean ( B holonomic) Cartan and nonRiemannian Riemannian and symmetric Metric, Cartan, and Riemannian Nonmetric, Cartan, and Riemannian
ˆ CL = 0 ∇
Statistically stored defects 15
ˆ ≠0 T
ˆ =0 R
ˆ CL = 0 ∇
ˆ =0 T
ˆ ≠0 R
ˆ CL = 0 ∇
ˆ ≠0 T
ˆ ≠0 R
ˆ CL = 0 ∇
Geometrically necessary dislocations Geometrically necessary disclinations Dislocations and disclinations
ˆ ≠0 T
ˆ ≠0 R
ˆ CL ≠ 0 ∇
Any point and line defects
Admissible for all geometries in Table 3.5. All straight nonterminating dislocations are geometrically necessary when considered in isolation; collections of SSDs produce no net Burgers vector and no contribution to the torsion tensor. 15
4 Thermomechanics of Crystalline Solids
Chapter 4 addresses fundamental thermomechanical relationships necessary for describing physical behavior of crystalline materials. Meant by the term thermomechanics are the balance principles from continuum mechanics and thermodynamics that dictate the response of the solid when subjected to mechanical forces, temperature variations, or other physical stimuli. Accordingly, the state of the material, for example equilibrium positions of atoms within a crystal and local vibrations of atoms about these positions, may change reversibly or irreversibly during a thermomechanical process. Complementary to the geometrically nonlinear description of kinematics in Chapter 3, the content of Chapter 4 focuses on descriptions of solid bodies subjected to finite deformations. Reductions of the nonlinear theory to the case of geometric linearity are included in many instances. The behavior of crystalline solids generally consists of a combination of a (thermo)elastic response corresponding to recoverable deformation and the inelastic response corresponding to plastic deformation such as that resulting from the generation and motion of defects. Elastic materials with viscosity and heat conduction were examined from a continuum thermodynamic viewpoint by Coleman and Noll (1963), who developed a method for exploiting the entropy production inequality to deduce thermodynamic relationships among field variables and restrictions on constitutive laws. Coleman (1964) extended this approach to materials with memory. In earlier work, Eckart applied similar, but apparently less mathematically formal, approaches towards deducing thermodynamic restrictions on behaviors of simple fluids (Eckart 1940) and elasticanelastic bodies undergoing potentially large deformations (Eckart 1948). Anelasticity in a general sense refers to any thermodynamically irreversible deformation and encompasses viscoelasticity and plasticity, for example. Viscoelastic media, both solid and fluid, were a primary focus of the study of Coleman and Noll (1963). The internal state variable concept is used in continuum theories to represent features of the material distinct from those addressed by conventional field variables (i.e., external variables) such as deformation and temperature. Internal state variables for crystalline solids often represent
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_4, © Springer Science+Business Media B.V. 2011
167
168
4 Thermomechanics of Crystalline Solids
microscopic features of the crystal structure that may evolve with strain or temperature. For example, internal state variables can often include scalaror tensorvalued measures of defect densities such as the number of point defects per unit volume in (3.133) or the dislocation density tensor of (3.224). Evolution refers to a change of a variable with time. Coleman and Gurtin (1967) developed a formal procedure using the balance of energy and dissipation inequality to impose restrictions on evolution of internal state variables. Internal state variable concepts were applied by Rice (1971) in an examination of inelastic constitutive relationships for crystalline solids. A critical comparison of competing theories of thermodynamics of irreversible processes is outside the scope of this text; a concise overview is given by Maugin (1988, pp. 99115). Other relevant works that feature treatments of continuum thermodynamics include those of Gurtin (1965), Truesdell and Noll (1965), Malvern (1969), Germain et al. (1983), Ericksen (1991), Grinfeld (1991), and Maugin and Muschik (1994a, b). Chapter 4 is organized as follows. Continuum concepts of mass density, traction, and stress referred to reference and current configurations are introduced. Thermodynamic potentials are defined. Classical balance equations of thermomechanics in continuous media undergoing potentially large deformations are reviewed: conservation of mass, momentum, and energy. A brief introduction to internal state variable theory is provided, including discussion of possible choices of internal variables for crystalline solids, followed by presentation of the dissipation inequality. Chapter 4 concludes with a short treatment of general kinetic relationships for irreversible processes, including dissipation potentials for inelastic rates. Much of the material presented in Chapter 4 applies to any continuous body in the framework of continuum mechanics; i.e., much of the forthcoming treatment in Chapter 4 is not restricted to crystalline solids and also applies to amorphous solids and fluids, for example. Developments in Chapter 4 are, however, restricted to classical continua as opposed to generalized continua. Generalized continua do not always obey standard balance laws of momentum and energy presented in Chapter 4. Generalized continua include materials supporting couple stresses (Cosserat and Cosserat 1909; Toupin 1962, 1964; Malvern 1969). Because balance laws of generalized continua differ among various theories, balance laws for generalized continua are addressed in this book on a casebycase basis. Specifically, governing equations for generalized elasticity (Toupin 1964) are discussed in Section 5.7 of Chapter 5, for generalized elasticity with an evolving intermediate configuration (Teodosiu 1967a, 1968) in Section 6.7 of Chapter 6, and for micropolar elastoplasticity (Clayton et al. 2006) in Section 9.4 of Chapter 9.
4.1 Classical Balance Laws and Definitions
169
Possible electromagnetic contributions to governing equations are omitted from the presentation of Chapter 4 and are deferred until Chapter 10. In continuum electromechanical theories (Stratton 1941; Toupin 1956, 1963; Eringen 1963; Tiersten 1971; Maugin 1988), electromagnetic forces may influence balances of momentum and energy and the reduced entropy inequality.
4.1 Classical Balance Laws and Definitions The present Section discusses what are termed classical balance laws of continuum mechanics: mass conservation, linear and angular momentum conservation, and the balance of energy. Though applicable to continuous bodies of an arbitrary nature, these relationships are used in later Chapters to enable rigorous descriptions of physical phenomena in crystalline solids deforming by one or more physical mechanisms (e.g., elasticity, dislocationbased plasticity, void growth, fracture, and so forth). Definitions of thermomechanical variables are presented first, followed by the aforementioned conservation and balance laws. Introduction of the dissipation inequality, i.e., the Second Law of Thermodynamics, follows later in Section 4.2.2. For additional insight, the reader is referred to other books dealing with nonlinear continuum mechanics (Truesdell and Toupin 1960; Eringen 1962; Truesdell and Noll 1965; Malvern 1969; Gurtin 1981; Marsden and Hughes 1983). Omitted from the discussion is treatment of surfaces of discontinuity1 occurring in the context of shock waves (e.g., discontinuous particle velocity, deformation gradient, and stress) or acceleration waves (e.g., discontinuous particle acceleration, velocity gradient, and secondorder position gradient). In other words, sufficient differentiability of field variables is presumed unless noted otherwise. 4.1.1 Definitions Definitions are provided for fundamental local quantities associated with mass, force, energy, and entropy. When forces or energies are measured on a per unit area or per unit volume basis, multiple definitions are needed to represent such quantities corresponding to each configuration of a deformable body. At a minimum, two definitions are needed for completeness: one referred to reference configuration B0 and another referred to 1 Surfaces of discontinuity are formally addressed by Truesdell and Toupin (1960).
170
4 Thermomechanics of Crystalline Solids
spatial configuration B. For tensorvalued entities such as stress, the number of possible definitions increases because of the possibility of twopoint tensors. Reference mass density ρ 0 (X ) and current mass density ρ (x, t ) of an element of mass m ≥ 0 are defined by m dm m dm ρ 0 = lim = , ρ = lim = , (4.1) V →0 V v→0 v dV dv with V and v that element’s volume in configurations B0 and B, respectively. Mass m (or dm) of a particular material particle, or of a fixed set of atoms, is assumed the same in (4.1) for corresponding reference and deformed volume elements. In continuum mechanics, mass density is subject to the constraints 0 ≤ ρ 0 < ∞ and 0 ≤ ρ < ∞ . Traction vectors measure directed forces per unit area acting on oriented surfaces, either external or internal, to the body. The reference traction t 0 (X , t ) and current traction (or simply the traction vector) t (x, t ) satisfy
t 0 dS = tds = dP ∈ Tx B , t0a dS = t a ds = dP a , (4.2) where dS and ds are differential area elements in configurations B0 and B, respectively, and dP is the force acting on the surface element. The reference traction t 0 is thus the force per unit reference area, while the traction vector t measures the force per unit spatial area. In either case, the index on the vector is referred to the current configuration. Thus indices of both traction vectors in (4.2) are referred to basis vectors g a ( x) of spatial tangent bundle TB.
Fig. 4.1 Deforming material element
Stress tensors relate traction vectors of (4.2) and unit normal covectors N and n (Fig. 4.1) associated with differential area elements dS and ds, respectively. Cauchy stress tensor σ (x, t ) ∈ Tx B × Tx B and first PiolaKirchhoff stress tensor P(X , t ) ∈ Tx B × TX B0 satisfy
t = σn , t a = σ ab nb ;
(4.3)
t 0 = PN , t = P N A .
(4.4)
a 0
aA
4.1 Classical Balance Laws and Definitions
171
Relations (4.3) and (4.4) are often referred to either as versions or outcomes of Cauchy’s theorem (Truesdell and Toupin 1960; Eringen 1962; Marsden and Hughes 1983). The linear function relating traction and the unit normal is the stress tensor. From (4.2)(4.4) and Piola transform (2.148), (4.5) t a ds = σ ab nb ds = JF −1.Abσ ab N A dS = P aA N A dS = t0a dS , implying that the two stress tensors in (4.3) and (4.4) are related by (4.6) P = JσF −* , P aA = J σ ab F.b−1 A . Second PiolaKirchhoff stress tensor Σ(X , t ) ∈ TX B0 × TX B0 and nominal stress tensor S(X , t ) ∈ TX B0 × Tx B are defined by pulling back and transposing P, respectively, while Kirchhoff stress tensor τ (x, t ) ∈ Tx B × Tx B is simply the Cauchy stress normalized by the Jacobian determinant as an energy per unit reference volume: Σ = F −1P , S = PT , τ = Jσ . (4.7) Relationships among contravariant components of the five stress tensors introduced in (4.3)(4.7) are listed in Table 4.1 for ease of reference2. In the geometrically linear theory of continuum mechanics (i.e., infinitesimal strain theory of Section 2.5.3), distinctions between first PiolaKirchhoff stress P aA and Kirchhoff stress τ ab = P aA F. Ab = P aA (δ .bA + u;bA ) ≈ P aAδ .bA are conventionally omitted (Malvern 1969), as explained in more detail in the context of the balance of linear momentum in Section 4.1.3. Table 4.1 Relationships among stress tensors Stress Cauch. σ
σ
Kirch. τ
Jσ
st
1 PK P nd
σ
τ J −1τ ab
ab
τ
ab
Jσ ab F.b−1 A
2 PK Σ
JF
Nom. S
JF.b−1 Aσ ab
ab
−1 B .b
aA
aA
b .A
b .A
P aA
τ F
F.b−1 Aτ ab
−1 B .b
F
−1 A .a
P aA
P
Σ J −1F.Ba Σ BA F. Ab
S
F Σ F
S Aa F. Ab
F. BaΣ BA
S Aa
Σ
S Ba F −1.Aa
a .B
P F
−1 A ab .a
F
−1
J P F
ab
τ ab F.b−1 A
σ F
−1 A .a
P
aB
BA
AB
Σ BA F. Ba
b .A
J −1S Aa F. Ab
S Aa
2 Placement of indices in stress tensors varies among authors. For example, Eringen (1962) and Malvern (1969) use the transpose of the definition used in this book for the Cauchy stress, expressing (4.3) as t a = nbσ ba . In such cases, the summation convention used for stress divergence in momentum balance (4.17) is modified accordingly. The distinction is irrelevant when the Cauchy stress is symmetric as occurs in classical continuum mechanics, but is important in generalized continuum theories (e.g., Sections 5.7 and 6.7) and nonlinear electromechanical theories (Chapter 10) wherein the Cauchy stress is not always symmetric.
172
4 Thermomechanics of Crystalline Solids
Absolute temperature θ (X , t ) ≥ 0 and entropy per unit mass η (X , t ) are introduced. Temperature θ traditionally is associated with local vibrations of atomic nuclei about their equilibrium positions, though the total (e.g., free) energy of an unstrained solid will also contain electronic contributions. Entropy in a qualitative sense measures the disorder of the substance or the ability of a system to perform work; more formal interpretations following from statistical mechanics principles and atomic systems are possible (Slater 1939; Phillips 2001) but are not included here. As will be demonstrated later in Sections 4.2.2 and 4.3, entropy production is associated with dissipative or irreversible thermodynamic processes. Also introduced are the following thermodynamic potentials, defined on a per unit mass basis: internal energy e(X , t ) , enthalpy h(X , t ) , Helmholtz free energy ψ (X , t ) , and Gibbs function g (X , t ) . Interrelationships among thermodynamic potentials for elastic bodies are listed in Table 4.2, following the scheme of Thurston (1974). Definitions of enthalpy and the Gibbs function depend upon the appropriate workconjugate thermodynamic tension or stress (e.g., the secondPiola Kirchhoff stress Σ of (4.7)) and deformation (e.g., the right CauchyGreen strain E of (2.156)) measures. By allowing each of the thermodynamic potentials to depend on a particular set of independent variables—for example deformation gradient (2.112) and temperature, or stress (4.6) and entropy—additional relationships among thermodynamic quantities can be deduced from partial crossderivatives of the potentials. In later Chapters dealing with constitutive theory, Helmholtz free energy ψ , often simply called the free energy, is featured prominently since it is conventionally assumed a function of the deformation gradient and temperature in the Gibbs formalism, and since deformation gradient and temperature are variables that are conveniently controllable in solid mechanics experiments, as opposed to entropy and enthalpy, for example (though in certain dynamic experiments, such as those involving wave propagation, that can be idealized as adiabatic, use of internal energy is often more convenient). Different definitions of the various thermodynamic potentials, particularly h and g, are possible for general states of stress (Malvern 1969), and traditional thermodynamic potentials of thermoelasticity (Thurston 1974) may require modification to account for inelastic deformation (Scheidler and Wright 2001; Wright 2002) as well as electromechanical effects (Devonshire 1954; Thurston 1974; McMeeking et al. 2007).
4.1 Classical Balance Laws and Definitions
173
Table 4.2 Thermodynamic potentials for elastic solids Potential [energy per unit mass] Internal energy e Enthalpy h
Relationship to internal energy e e h = e − ρ 0−1Σ AB E AB
Helmholtz free energy ψ Gibbs function g
ψ = e − θη g = e − ρ 0−1Σ AB E AB − θη
It sometimes becomes useful to define thermodynamic potentials and entropy on a per unit volume basis: Ν = ρη , E = ρ e , H = ρ h , Ψ = ρψ , G = ρ g ; (4.8) Ν 0 = ρ0η , E0 = ρ0 e , H 0 = ρ0 h , Ψ 0 = ρ 0ψ , G0 = ρ0 g . (4.9) In (4.8), capitalization denotes a quantity defined on a per unit current volume basis in spatial configuration B. The zero subscript introduced in (4.9) is used in conjunction with capitalization for an energetic or entropic quantity measured per unit volume in reference configuration B0 . 4.1.2 Mass Conservation Mass m of an element of material is said to be conserved when that element’s mass does not vary with time, i.e., when m is the same in referential and spatial descriptions. Eliminating dm from (4.1) and using (2.141), mass densities in spatial and reference configurations are related by ρ0 = ρ J . (4.10) Since volume elements are nonnegative and of finite size in both configurations, 0 < J < ∞ as noted already following (2.141), and 0 < J −1 < ∞ . Thus ρ = 0 if and only if ρ0 = 0 and the mass of the corresponding element vanishes. The continuity equation expresses the time rate of change of current mass density ρ . This equation can be derived in a number of ways, for example integration over a control volume supporting fluxes of mass across its external surfaces followed by localization, or direct time differentiation of local conservation law (4.10). Taking the latter approach and using (2.181), ρ 0 = 0 = ρ J + ρ J = ρ J + ρ Lv J = J ( ρ + ρ v;aa ) , (4.11) where the first equality follows from the assertion that mass density in the reference configuration is timeindependent. From the definition of the material time derivative in (2.169), continuity equation (4.11) can be written in either of two forms upon division by J as
174
4 Thermomechanics of Crystalline Solids
∂ρ + ( ρ v a ); a = 0 . (4.12) ∂t x A material for which ρ ( x( X , t ), t ) = ρ0 ( X ) at all material points X, and hence for which J ( X , t ) = 1 for all X and for all t > 0 , is called incompressible. In the geometrically linear theory, use of (2.164) in (4.10) and (4.11) produces the following firstorder approximations for mass density and its time rate of change: ρ 0 ≈ ρ (1 + u;aa ) and ρ + ρ u;aa = 0 . Reynolds transport theorem accounts for the time rate of change of a given quantity carried by a deformable mass of material occupying an evolving volume v in configuration B. The rate of change of generic quantity aˆ , which may be any differentiable scalar, vector, or tensor of higher order, is computed as follows: ∂ d ˆ − ∫ ρ aˆ v, n ds , (4.13) ∫v ∂t ( ρ aˆ ) dv = dt ∫v ρ adv s where s is the external surface of v with oriented unit normal covector n( x, t ) . Applying the divergence theorem of (2.193) in conjunction with (4.12), Reynolds transport theorem is written more compactly as d ∂ ∂ ˆ = ∫ ( ρ aˆ ) dv + ∫ ρ av ˆ a na ds = ∫ ( ρ aˆ ) dv + ∫ ( ρ av ˆ a ) dv ρ adv ;a dt ∫v ∂ t ∂ t v s v v (4.14) ⎡ ∂ρ ⎤ ⎡ ∂aˆ a a⎤ ˆ + ∫ ρ ⎢ + aˆ;a v ⎥ dv = ∫ ρ adv ˆ . = ∫ ⎢ + ( ρ v ) ⎥ adv ;a ∂t ⎦ ⎣ ∂t ⎦ v ⎣ v v
ρ + ρ v;aa = 0 ,
Recall from Section 2.6.1 that d / dt denotes the material time derivative (i.e., reference particle at X held fixed during time differentiation), and ∂ / ∂t denotes the partial time derivative taken with spatial position x held fixed. 4.1.3 Momentum Conservation
Traditional conservation laws of momentum consist of balances of linear and angular momentum. The global spatial balance of linear momentum is d ρ vdv = ∫ bdv + ∫ tds , (4.15) dt ∫v v s where v ( x, t ) is the spatial velocity of (2.168), b ( x, t ) is the body force vector (measured here as a force per unit spatial volume), and integration proceeds over the body in current configuration B with volume v enclosed
4.1 Classical Balance Laws and Definitions
175
by surface s. From (4.3), (4.14), and application of the divergence theorem, (4.15) can be written as a ab a (4.16) ∫ ρ v dv = ∫ (σ ;b + b )dv . v
v
Localization of (4.16) and use of (4.12) then provides a spatial balance of linear momentum that can be expressed in two forms: ∂ σ ;abb + b a = ρ a a ⇔ (σ ab − ρ v a vb );b + b a = ( ρ v a ) , (4.17) ∂t with a a ( x, t ) = v a the spatial acceleration of (2.173). The global material balance of linear momentum is written as follows: d ρ 0 VdV = ∫ BdV + ∫ t 0 dS , (4.18) dt V∫ V S
where V ( X , t ) is the material velocity of (2.167) and B( X , t ) is the body force per unit reference volume. Application of (4.4) and the divergence theorem gives (Eringen 1962; Malvern 1969; Marsden and Hughes 1983) a a aA (4.19) ∫ ρ0V dV = ∫ B dV + ∫ P: A dV , V
V
V
with the total covariant derivative (more specifically, divergence) of the first PiolaKirchhoff stress P found via application of (2.73), (2.117), and inclusion of only the referential partial derivative of P aA ( X , t ) : G
P: AaA = P..,aAA + Γ
.. A AB
g
P aB + Γ
..a bc
P cA F. Ab g
= P..,aAA + (ln G ), A P aA + Γ = ( JF = Jσ
σ ): A = ( JF
−1 A .b
ab :b
ab
..a bc
P cA F. Ab
) σ
−1 A .b : A
ab
+ JF
(4.20)
σ
−1 A .b
ab :A
= Jσ . ab ;b
Application of Piola’s identity (2.146), i.e., ( JF −1.Ab ): A = 0 , to the stress divergence, and use of properties of the total covariant derivative in (2.117), enable derivation of the final three equalities in (4.20). The local material balance of linear momentum following from (4.19) is P: AaA + B a = ρ0 Aa , (4.21) where Aa ( X , t ) is the material acceleration of (2.174). It follows from (4.10), (4.20), and B a = Jb a that the local material momentum balance can be obtained from local spatial momentum balance (4.17) via multiplication of the latter by J (Truesdell and Toupin 1960). While local forms of the balance of linear momentum in (4.17) and (4.21) apply for any choice of spatial coordinates, global coordinate forms (4.16) and (4.19) in
176
4 Thermomechanics of Crystalline Solids
volve integrals of vector fields over the spatial manifold with current tangent bundle TB. Thus the latter are valid only for coordinate systems wherein spatial basis vectors g a are independent of position x, e.g., Cartesian coordinates. Alternatively, following Toupin (1956) and discussion in Section 3.2.5, resultant forces and total linear momentum can be evaluated at a particular point x via parallel transport of integrands to that point using appropriate shifter tensors. Table 4.3 Spatial momentum balance in physical cylindrical coordinates Quantity Momentum
Rcomponent
θ−component
Zcomponent
σ RR ,R + R −1σ Rθ ,θ
σ θ R ,R + R −1σ θθ ,θ
σ ZR ,R + R −1σ Zθ ,θ
+σ RZ ,Z + R (σ RR − σ θθ )
+σ θ Z ,Z + 2 R σ θ R
+σ ZZ ,Z + R −1σ ZR
−1
Acceleration
Velocity
−1
= ρ aR − bR
= ρ aθ − bθ
= ρ aZ − bZ
aR = ∂vR / ∂t
aθ = ∂vθ / ∂t
aZ = ∂vZ / ∂t
+ vR vR ,R + R −1vθ vR ,θ
+ vR vθ , R + R −1vθ vθ ,θ
+vR vZ ,R + R −1vθ vZ ,θ
−1
+ vZ vR ,Z − R −1 (vθ ) 2
+ vZ vθ ,Z + R vR vθ
+ vZ vZ ,Z
vR = R
vθ = Rθ
vZ = Z
Table 4.4 Spatial momentum balance in physical spherical coordinates Quantity Momentum
Acceleration
Rcomponent
θ−component
σ RR ,R + R −1σ Rθ ,θ
σ θ R ,R + R −1σ θθ ,θ
ϕcomponent σ ϕ R , R + R −1σ ϕθ ,θ
+( R sin θ ) −1σ Rϕ ,ϕ
+( R sin θ ) −1σ θϕ ,ϕ
+( R sin θ )−1σ ϕϕ ,ϕ
+ R −1 (2σ RR − σ θθ
+ R −1[3σ θ R + (σ θθ
+ R −1 (3σ ϕ R
−σ ϕϕ + σ Rθ cot θ )
−σ ϕϕ ) cot θ ]
+2σ ϕθ cot θ )
= ρ aR − bR
= ρ aθ − bθ
= ρ aϕ − bϕ
aR = ∂vR / ∂t
aθ = ∂vθ / ∂t
aϕ = ∂vϕ / ∂t
+ vR vR ,R + R −1vθ vR ,θ
+ vR vθ ,R + R −1vθ vθ ,θ
+vR vϕ ,R + R −1vθ vϕ ,θ
+ ( R sin θ ) −1 vϕ vR ,ϕ
+( R sin ϕ ) −1 vϕ vθ ,ϕ
+( R sin ϕ ) −1 vϕ vϕ ,ϕ
− R [(vθ ) + (vϕ ) ]
+ R [vR vθ − (vϕ ) cot θ ]
+ R −1vϕ [vR + vθ cot θ ]
vR = R
vθ = Rθ
vϕ = ϕ R sin θ
−1
Velocity
2
2
−1
2
Procedures for deriving the balance of linear momentum in terms of physical components of vectors and tensors are given by Eringen (1962) and Malvern (1969). Tables 4.3 and 4.4 provide spatial balances of linear momentum in cylindrical coordinates of Section 2.4.2 and spherical coordinates of Section 2.4.3. Components of velocity (2.168) and acceleration (2.173) in corresponding physical components are also listed in Tables 4.3 and 4.4. In Table 4.5, components of velocity gradient (2.176) that enter
4.1 Classical Balance Laws and Definitions
177
the convective part of the spatial acceleration are listed, following Malvern (1969). In contrast to Section 2.4 in which physical components correspond to the reference configuration, indices of cylindrical and spherical coordinates are referred to the spatial configuration B in Tables 4.34.5. The summation convention does not apply over repeated indices in Tables 4.34.5. Table 4.5 Velocity gradient components in cylindrical and spherical coordinates Coordinate system Cylindrical
Spherical
g
Velocity gradient L = ∇ v
LRR = vR, R Lθ R = vθ , R LZR = vZ ,R
LRθ = R −1 (vR ,θ − vθ ) Lθθ = R −1 (vθ ,θ + vR ) LZθ = R −1vZ ,θ
LRZ = vR , Z Lθ Z = vθ , Z LZZ = vZ ,Z
LRR = vR ,R Lθ R = vθ ,R
LRθ = R −1 (vR ,θ − vθ ) Lθθ = R −1 (vθ ,θ + vR )
LRϕ = ( R sin θ ) −1 vR ,ϕ − R −1vϕ Lθϕ = ( R sin θ )−1 vθ ,ϕ − R −1vϕ cot ϕ
Lϕ R = vϕ ,R
Lϕθ = R −1vϕ ,θ
Lϕϕ = ( R sin θ ) −1 vϕ ,ϕ + R−1 (vθ cot θ + vR )
The global balance of angular momentum referred to the spatial configuration is d x × ρ vdv = ∫ x × bdv + ∫ x × tds , (4.22) dt ∫v v s where × is the vector cross product. In indicial notation, (4.22) is written d (4.23) ε abc xb ρ v c dv = ∫ ε abc x b b c dv + ∫ ε abc xb t c ds . dt ∫v v s Using divergence theorem (2.193), Cauchy’s theorem (4.3), and Reynolds transport theorem (4.14), (4.23) becomes b c b c b c b cd ∫ ε abc ( ρ v v + ρ x v − x b )dv = ∫ ε abc x σ nd ds v
s
= ∫ ε abc ( x σ );d dv = ∫ ε abc (σ cb + x bσ ;cdd ) dv. b
v
cd
v
Collecting terms gives b c c cd cb b c ∫ ε abc x ( ρ v − b − σ ;d )dv = ∫ ε abc (σ − ρ v v )dv . v
(4.24)
(4.25)
v
The left side of (4.25) vanishes by (4.17), and the last term in the integrand b c on the right of (4.25) vanishes from symmetry of the dyad vb v c = v ( v ) . This leaves the local requirement ε abcσ cb = 0 ⇔ σ ab = σ ( ab ) , σ [ ab] = 0 , (4.26)
178
4 Thermomechanics of Crystalline Solids
i.e., the Cauchy stress tensor is symmetric in classical continuum mechanics. From (4.6) and (4.7), the local balance of angular momentum can also be expressed in any of the following forms as F. Aa P bA = P aA F. Ab , Σ AB = Σ BA , S Ab F. Aa = F. Ab S Aa , τ ab = τ ba . (4.27) In geometrically linear theories of continuum mechanics, with the assumption P aA ≈ τ abδ.bA (Malvern 1969), the balance of linear momentum a a (4.21) in terms of force per unit reference volume is τ ;ab b + B = ρ0u . a a Similarly, σ ;ab b + b = ρ u in terms of force per unit current volume (4.17).
−1 ab ab );b = τ ;ab ≈ τ ;ab is implied if both moTogether, J σ ;ab b = J (J τ b − J ;bσ b mentum balances are assumed to apply simultaneously in the linear theory. Thus, formally, two linear momentum balances would seem necessary in the linear theory even though the distinction between reference and spatial coordinates is not enforced explicitly. This issue arises when mass density is permitted to change with deformation in the linear theory, as noted following (4.12). In the geometrically linear theory, angular momentum balances (4.26) and (4.27) remain unchanged from those of the nonlinear theory: σ ab = σ ba and τ ab = τ ba . Like the coordinate form of the global balance of linear momentum, the indicial expression of the global balance of angular momentum is restricted to spatial coordinate systems for which holonomic basis vectors are independent of position. Local forms (4.26) and (4.27), however, apply for any choice of coordinate system, e.g., curvilinear coordinates. Local forms of conservation of mass (4.12), balance of linear momentum (4.17), and balance of angular momentum (4.26) can be obtained without resorting to the global (i.e., integral) forms via prescription of an energy balance that is presumed invariant under rigid body motions (Green and Rivlin 1964a). This alternative approach towards derivation of local balance laws, which does not require assignment of particular kinds of coordinate systems, is formally discussed by Marsden and Hughes (1983).
4.1.4 Energy Conservation
The global form of the balance of energy or First Law of Thermodynamics for a continuous body is written d (4.28) (E + K ) = P + Q , dt where E is the global internal energy, K is the global kinetic energy, P is the mechanical rate of working, and Q is the rate of work of nonmechanical sources. These quantities are defined as follows for a body in
4.1 Classical Balance Laws and Definitions
179
spatial configuration B occupying volume v and enclosed by surface s, with the latter’s orientation defined by outward unit normal covector n: E = ∫ ρ edv , (4.29) v
K = ∫ ( ρ / 2) v i vdv ,
(4.30)
P = ∫ bi vdv + ∫ t i vds ,
(4.31)
Q = ∫ ρ rdv − ∫ q, n ds .
(4.32)
v
v
s
v
s
In (4.32), r ( x, t ) is the scalar heat source per unit mass that may arise from nonmechanical phenomena (e.g., a radiation field), and q( x, t ) ∈ Tx B is the heat flux vector associated with heat conduction. Source r vanishes identically in most typical boundary value problems. The sign convention for q is specified such that when q, n = q a na > 0 , energy flows out of the body so that the contribution from heat flux to energy rate Q is negative. The local version of (4.28) is derived as follows. Using (4.14) and the divergence theorem to convert surface integrals in (4.31) and (4.32) to volume integrals, b b ba a ∫ ρ (e + v vb )dv = ∫ b vb dv + ∫ (σ vb − q ) ;a dv + ∫ ρ rdv v
v
v
v
= ∫ vb (b + σ )dv + ∫ (σ vb;a − q;aa )dv + ∫ ρ rdv. b
ba ;a
ba
v
v
(4.33)
v
Then from (4.17), terms associated with stress divergence, linear momentum, and body forces cancel. Localizing, the remaining terms comprise the spatial balance of energy: ρ e = σ ab va ;b − q;aa + ρ r , (4.34) or in direct notation g
ρ e = σ , D − ∇, q + ρ r ,
(4.35)
where (4.26) has been used and D = (1/ 2) L v g is the deformation rate tensor of (2.182). The skew part of the velocity gradient, i.e., the spin tensor W of (2.187), does not contribute to balance of energy (4.35) because of the symmetry of the Cauchy stress tensor. The local balance of energy is expressed in material form as follows. Heat flux q is mapped to Q( X , t ) ∈ TX B0 via Nanson’s formula (2.148): Q A N A dS = Q A J −1 F. Aa na ds = q a na ds → Q A = JF.a−1 A q a . (4.36) Using Piola’s identity (2.145), the divergence of the heat flux satisfies
180
4 Thermomechanics of Crystalline Solids
q;aa = ( J −1 F. Aa Q A );a = ( J −1 F. Aa ):a Q A + J −1 F. Aa Q:aA = J −1Q;AA . (4.37) Scalars e and r are defined on a per unit mass basis and hence remain stationary with respect to changes in configuration, while the mass density changes according to (4.10). From (2.186), (4.6), and (4.7), the stress power per unit current volume can be written σ ab Dab = σ ab F.a−1 A E AB F.b−1B = J −1Σ AB E AB , (4.38) where the right CauchyGreen strain tensor E is defined in (2.156). Multiplying (4.35) by J and using (4.10), (4.37), and (4.38) gives the local material balance of energy: ρ 0 e = Σ AB E AB − Q;AA + ρ 0 r . (4.39) In the context of the geometrically linear theory of (2.191), deformation rate and strain rate are equivalent, and the local balance of energy of (4.34) reduces to ρ e = σ abε ab − q;aa + ρ r . (4.40) When body forces are conservative, global energy balance (4.28) can be expressed in an illustrative form (Eringen 1962). Conservative forces are derivable from a local potential energy function Φ ( x ) that depends only on position, and not explicitly on time: ρ ba ⇒ ba ( x) = −Φ , a ( x) , Φ = ∫ ρΦ dv . (4.41) v
In the first of (4.41), b is a body force per unit mass, and the dimensions of the local potential energy Φ ( x) are energy per unit mass. The second of (4.41) defines a global potential energy. From (4.41) the latter’s rate is ⎛ ∂Φ ⎞ + Φ , a v a ⎟ dv = ∫ ρΦ ,a v a dv = − ∫ ρ ba v a dv . (4.42) Φ = ∫ ρΦ dv = ∫ ρ ⎜ ⎝ ∂t x ⎠ v v v v The global rate of mechanical working in (4.31) becomes P = ∫ ρ ba v a dv + ∫ t a va ds = ∫ t a va ds − Φ . v
s
(4.43)
s
Global energy balance (4.28) then becomes E + K + Φ = ∫ t a va ds + Q .
(4.44)
s
When the right side of (4.44) vanishes, E + K + Φ = constant , meaning that the sum of internal, kinetic, and potential energies is conserved. Specific scenarios for which this holds are conditions in which the body is insulated (i.e., adiabatic or vanishing heat flux q with no heat sources r) and when either velocities or tractions vanish on boundary surface s. The analogous situation for conservative discrete particle systems is derived in
4.2 Internal State Variables and the Dissipation Inequality
181
Section B.1, specifically relations (B.13) and (B.15), in the context of the Hamiltonian representation of governing equations of molecular dynamics.
4.2 Internal State Variables and the Dissipation Inequality A number of formal philosophical interpretations exist regarding consideration of thermodynamic quantities, balance equations, and fundamental inequalities in the context of modern continuum mechanics (Germain et al. 1983; Maugin and Muschik 1994a). What is often called classical thermodynamics deals with equilibrium states of materials. A system is said to be in thermodynamic equilibrium if it is isolated, does not evolve with time, and hence contains no unbalanced internal forces. Classical thermodynamics is thus sometimes referred to as thermostatics (Thurston 1974). In thermostatics, temperature and entropy of a material and thermodynamic potentials introduced in Section 4.1.1 have clear origins in statistical mechanics (Slater 1939; Malvern 1969). On the other hand, in many physical problems of interest the situation is more complex, and one often seeks descriptions of the condition of the material as it attains various nonequilibrated states, i.e., descriptions afforded by nonequilibrium thermodynamics. In such circumstances, traditional thermostatic definitions do not readily apply, and the system cannot be adequately described by a finite collection of state variables. To overcome this difficulty, the notion of local accompanying equilibrium states or constrained equilibrium states is often introduced (De Groot and Mazur 1962; Lubliner 1990; Kestin 1992). In this context, the material is treated as if it were in local equilibrium at any given instant, even when undergoing an irreversible process, and thus can be described by the thermodynamic temperature, thermodynamic potentials, and a finite set of state variables. This is often deemed an appropriate assumption when time scales for irreversible processes are fast relative to those for incremental changes in driving forces such as mechanical stresses or temperature gradients (Rice 1971; McDowell 2005). The concept is also appropriate when such driving forces change rapidly enough that changes in internal variables associated with irreversibility do not have time to occur. Though the formal definition of constrained equilibrium states does not apply in situations wherein time scales associated with internal variables and their driving forces are similar, the state variable concept is still used regularly in modern applications of continuum thermomechanics, albeit in the context of nonequilibrium thermodynamics, to describe various behaviors of deformable continuous bodies (Maugin and Muschik 1994a, b).
182
4 Thermomechanics of Crystalline Solids
The condition or state of the material, for example its energy content and constitutive response, is assumed from a mathematical perspective to depend upon a number of independent state variables. These may include kinematic variables such as volume or strain, intrinsic field variables such as temperature or entropy, and any number of internal state variables. An internal state variable refers to an intrinsic quantity that is required to fully characterize the state of the material and that can be varied, albeit often irreversibly, without changing the other independent state variables. In crystalline solids, such variables are typically used to reflect influences of the microstructure on the state of the system, for example energies attributed to lattice defects, or phenomena at a finer length scale not represented by strain or temperature fields at the coarser scale of immediate consideration. For example, dislocation densities were treated as internal state variables in an early continuum plasticity theory of Kroner (1963a). The transition of the material from one state (i.e., one particular set of values of state variables) to another is called a thermodynamic process. If application of the inverse of the external stimuli invoked during a given thermodynamic process returns the material to its original state, such a process is said to be reversible. On the other hand, if the inverted stimuli do not return the material to its original condition, the material is said to have undergone an irreversible process. Irreversible processes involve dissipation of energy and production of entropy. The reversibility of a thermodynamic process, or lack thereof, may depend upon the scale at which the observer views the process (Germain et al. 1983). For example, a crystal structure undergoing small, slow deformations may appear reversible (i.e., elastic) at the macroscale, but could be irreversible at the scale of the motion of some individual atoms, particularly those in the vicinity of imperfections (i.e., defects) in the material. The ClausiusDuhem inequality and various renditions of it are alternatively referred to as the Second Law of Thermodynamics, the entropy production inequality, or the dissipation inequality. This relationship reduces to an equality for thermodynamically reversible processes. In solids undergoing irreversible processes, a local version of this inequality, in combination with the local balance of energy, provides an indication of contributions of various mechanisms to energy stored in the material and to energy dissipated by the material. Constitutive equalities and thermodynamic restrictions on constitutive and kinetic relationships can be derived by appealing to the First and Second Laws of Thermodynamics, as formally demonstrated for heat conducting media with viscosity by Coleman and Noll (1963) and continua with generic internal state variables by Coleman and Gurtin (1967). Such methods of thermodynamic analysis have become commonplace for constructing nonlinear theories of elasto
4.2 Internal State Variables and the Dissipation Inequality
183
plasticity of crystalline solids (Scheidler and Wright 2001), including those incorporating internal variables associated with higherorder deformation gradients reflecting dislocation content (Teodosiu 1970; Steinmann 1996; Bammann 2001; Regueiro et al. 2002; Clayton et al. 2004b, 2006). Section 4.2.1 describes considerations for selection of constitutive variables (including both dependent and independent variables) and internal state variables that together describe the thermodynamic state of a body. Particular attention is paid to variables appropriate for crystalline solids undergoing potentially large deformations. 4.2.1 Constitutive and Internal Variables for Crystalline Solids
Constitutive laws are mathematical relationships that describe properties of particular materials or particular classes of materials. Such relationships emerge from the constitution of the material, e.g., its composition and structure, hence the term “constitutive law”. In the context of continuum thermomechanics, constitutive laws describe relationships between independent and dependent state variables and/or their rates of change. A number of possibilities exist with regards to selection of which variables should be used as independent quantities and which should be dependent quantities. For example, various formulations treating temperature, entropy, or internal energy as either independent or dependent variables exist (Eringen 1962; Coleman and Noll 1963; Coleman and Gurtin 1967; Malvern 1969; Thurston 1974; Wright 2002), all of which are mathematically and physically valid. Selections of independent and dependent variables in thermodynamic processes are labeled in this book as constitutive assumptions. Though more general assumptions are possible, for crystalline solids under consideration in this text the following forms are perhaps most common3: g ⎛ ⎞ ψ = ψ ⎜ F L , α ,θ , ∇ θ , X , G A ⎟ , ψ = ψ ( F La.α ,α ,θ ,θ , a , X , G A ) ; (4.45) ⎝ ⎠ g ⎛ ⎞ η = η ⎜ F L ,α ,θ , ∇θ , X , G A ⎟ , η = η ( F La.α ,α ,θ ,θ,a , X , G A ) ; (4.46) ⎝ ⎠
Not included in (4.45)(4.49) is a dependence on higherorder deformation gradients, e.g., F. Aa:B = x:aAB of (2.116). A material is often said to be of grade N, where N is the highest order of deformation gradient present in the list of dependent state variables (Toupin 1964). Thus, when F La.α = x.,aA g.αA such as in an elastic 3
solid described by (3.25), relations (4.45)(4.49) describe a material of grade 1.
184
4 Thermomechanics of Crystalline Solids
g ⎛ ⎞ (4.47) σ = σ ⎜ F L ,α ,θ , ∇ θ , X , G A ⎟ , σ ab = σ ab ( F L.aα ,α ,θ ,θ , a , X , G A ) ; ⎝ ⎠ g ⎛ ⎞ (4.48) q = q ⎜ F L , α ,θ , ∇ θ , X , G A ⎟ , q a = q a ( F La.α ,α ,θ ,θ ,a , X , G A ) ; ⎝ ⎠ g ⎛ ⎞ (4.49) α = α ⎜ F L ,α ,θ , ∇ θ , X , G A ⎟ , α = α ( F La.α ,α ,θ ,θ ,a , X , G A ) . ⎝ ⎠ Dependent variables in (4.45)(4.49) are Helmholtz free energy per unit mass ψ , entropy per unit mass η , Cauchy stress σ , heat flux vector q, and the material time derivative of a generic scalar internal state variable α ( X , t ) . Extension of the treatment to multiple state variables of scalar, vector, or tensor character is straightforward, and is pursued by example later in Chapters 8 and 9. Independent variables are lattice deformation gradient F L of (3.31), absolute temperature θ and its spatial gradient θ,a , and internal state variable α . Additionally, dependence on position of material particle X is included, as is dependence on basis vectors G A ( X ) in the reference configuration. Dependence on X is required to describe variations, with changes in position, of properties in a heterogeneous material, while dependence on G A is required to describe anisotropy, or dependence of the response on orientation of a body with certain symmetries (see Appendix A) relative to the chosen system of coordinates4. As discussed in Section 3.1.2, in defectfree elastic crystals F L corresponds to deformation gradient F. More generally, as indicated in (3.31), for a crystal featuring inelastic deformation, F L = FF P −1 ≠ F . The rationale for dependence of free energy and stress upon lattice deformation follows from (3.109)(3.114): lattice deformation provides a firstorder accurate measure of stretch and rotation of interatomic bond vectors in a crystal structure. In dielectric solids, the list of independent variables may be supplemented with a measure of the electric polarization (e.g., measuring relative translations among charged nuclei in a polyatomic ionic crystal), and dependent variables then may include the electric field or electric displacement, as described in detail in Chapter 10. It is possible to write (4.45)(4.49) in terms of variables defined partially or entirely with respect to coordinate charts of different configurations
Often dependence on X and G A is not written out explicitly, but rather is included implicitly in the material coefficients (e.g., thermoelastic moduli) entering series expansions of the thermodynamic potentials. This will become clear in Chapter 5 in the context of thermoelastic crystalline solids. 4
4.2 Internal State Variables and the Dissipation Inequality
185
(e.g., spatial configuration B or reference configuration B0 ), and with dependent energetic and entropic variables measured on a perunitvolume basis following (4.8) or (4.9), as opposed to a perunitmass basis. Certain choices of configuration may result in different constitutive laws or different predicted behaviors, and some choices may be more physically motivated than others, as considered later for elasticplastic crystals in Chapters 6, 8, and 9. Response functions (4.45)(4.49) are often presumed to adhere to a collection of formal, fundamental principles or postulates. These include the principle of equipresence (Truesdell 1951) that suggests that all independent variables should be present in each constitutive equation unless contradicted by physical laws or symmetry properties of the material. The latter requirement is often delineated as a separate principle, that is functions (4.45)(4.49) should respect symmetry properties of the substance, as addressed explicitly here by presence of basis vectors G A (Eringen 1962). The response should also satisfy an objectivity, frameindifference, or covariance principle, versions of which have been considered for a number of years in the mathematical mechanics literature (Noll 1958; Coleman and Noll 1963; Coleman and Gurtin 1967; Marsden and Hughes 1983; Yavari et al. 2006). Objectivity as defined here implies that physical behavior is independent of the reference frame of the observer. Specifically, the physical behavior of an event should not change under a change of spatial coordinate system (Coleman and Noll 1963; Coleman and Gurtin 1967). Objective constitutive functions can be formulated in a number of ways. Perhaps the easiest way involves replacing the list of independent variables by constructs of these variables that are invariant under appropriate rigid body motions (i.e., rigid rotations and translations) of the spatial coordinate system, and by choosing complementary forms of dependent variables that are likewise spatially invariant. Consider the choice of lattice deformation gradient F L as an independent variable entering functions (4.45)(4.49). Under a change of spatial ˆ (t ) = Q ˆ −T (t ) is a spatially constant, proper orˆ + c , where Q frame x → Qx thogonal rotation matrix and c(t ) is a spatially constant translation vector, ˆ L. ˆ and the lattice deformation F L → QF the deformation gradient F → QF More general kinds of spacetime transformations involving time shifts and additional translations are possible (Malvern 1969; Gurtin 1981; ˆ + c is sufficient for the preMaugin 1988), but consideration of x → Qx sent discussion. Often, a number of possible sets of reduced constitutive equations exist that fulfill the objectivity requirement. For example, re
186
4 Thermomechanics of Crystalline Solids
placing dependent variable F L ( X , t ) with CL ( X , t ) of (3.52) satisfies the objectivity requirement that is not unequivocally satisfied by use of independent variable F L , since under a change of frame, L Cαβ = F L.aα g ab F Lb.β = F La.α F LTβ a → (Qˆ.ac F Lc.α )(Qˆ T.ad F LTβ d ) (4.50) L = Qˆ T.ad Qˆ.ac F Lc.α F L d β = δ .dc F Lc.α F L d β = F Ld.α F L d β = Cαβ . Spatial metric tensor g(x) is unaffected by such an orthogonal transformation since g ab → Qˆ.ca g cd Qˆ.db = Qˆ .ca Qˆ cb = Qˆ bcT Qˆ .ca = gba = g ab . Similarly, spatial temperature gradient θ, a ( X , t ) is not frame indifferent. One of several possible substitutions that fulfills the objectivity requirement is the reference gradient θ , A = θ ,a x.,aA (Coleman and Noll 1963):
θ, A = θ,a x.,aA = θ ,a FAaT → Qˆ.acθ ,c FAdT Qˆ T.ad
(4.51) T = Qˆ .Tad Qˆ.acθ ,c FAd = θ ,c FAcT = θ,c x.,cA = θ, A . In classical continuum mechanics, response functions (4.45)(4.49) are also required to satisfy a principle of locality, meaning that dependent variables corresponding to a particular material particle at X are functions of independent variables at point X and not values of independent variables at other material points X ′ . However, in many generalized continuum theories, the assertion of locality is relaxed (Eringen 1972; Bazant 1991). As an example, consider a material that exhibits time evolution of internal state variable α . Classes of nonlocal internal variable theories include those with evolution equations of the general type α ( X , t ) = f ( F La.α ,α ,θ ,θ , a , G A , X , X ′ ) , (4.52) where the value of α at X is affected by the values of state quantities at different points X ′ ∈ B0 entering function f. Integral formulations, inherently nonlocal, are also possible, e.g. α ( X , t ) = V −1 ∫ f ′ ( F L.aα ,α ,θ ,θ, a , G A , X , X ′ )dV , (4.53) V
where the domain of integration may encompass some local region (e.g., volume V) in the vicinity of point X in the body (Hall and Hayhurst 1991), or may engulf the entire solid. Finally, theories of the highergradient type are often labeled nonlocal in character (Voyiadjis and Deliktas 2009). For example, consider an evolution equation of the form α ( X , t ) = f ( F La.α ,α ,α , A ,θ ,θ, a , G A , X ) . (4.54) Expanding α in a Taylor series approximation about point X gives
4.2 Internal State Variables and the Dissipation Inequality
α
X′
=α
X
+ α, A
X
dX A +
1 α ; AB 2!
X
187
dX A dX B
(4.55) 1 A B C + α ; ABC X dX dX dX + ..., 3! where dX A = X ′ A − X A . Omitting second and higherorder terms in dX, the material gradient of α is expressed via local and nonlocal values of α: α , A ( X , t )dX A = α ( X ′, t ) − α ( X , t ) , (4.56) implying that (4.54) exhibits a particular form encompassed by nonlocal equation (4.52). Constitutive functions depending on firstorder, but not higherorder, spatial gradients of position and temperature are considered to describe materials categorized as classical rather than generalized continua. Elastic solids of grade 2 (see Section 5.7), as a matter of semantics, can be labeled local (Epstein and Elzanowski 2007) or nonlocal. Particular choices of internal state variables should satisfy physical and practical considerations. Internal state variables may be directly measurable or observable to allow straightforward construction of evolution laws such as (4.49) from experimental data, or they can be “hidden” variables that influence the response in a measurable way but lack a precise microscopic interpretation. Examples of the former include measures of dislocation density in plastically deforming crystals (Kroner 1963a; Teodosiu 1970) and direct measures of porosity or crack density in damaged media (Bammann and Aifantis 1989; Kachanov 1992; NematNasser and Horii 1998). Examples of the latter include generic variables representing strain hardening in plastic crystals (e.g., thermodynamic conjugate variables to a yield stress or back stress) and generic scalar or tensor damage measures that reflect mechanical stiffness reduction, for example (Germain et al. 1983; Lemaitre 1985). However, while an internal variable or its effects should be measurable, its value should not be controllable simply by immediate application of external boundary conditions (e.g., mechanical traction and heat flux), since in that case it would be an external as opposed to internal variable. In such a case, the socalled internal variable would not be independent of other state variables such as stress, strain, and temperature, and would be redundant for characterizing the state of the material. Instead, instantaneous values of internal state variables tend to depend on initial conditions and the cumulative history of boundary conditions applied to the body. Internal state variables should be chosen to adhere to underlying physics of the microstructure of the material, and their evolution should reflect corresponding changes in forces or energies supported in the substance. For example, accumulating dislocations tend to increase the energy stored in
188
4 Thermomechanics of Crystalline Solids
the crystal as a result of their local stress and strain fields, and damage mechanisms such as voids or cracks tend to affect the energy of a strained crystal via a reduction in the effective elastic stiffness. On the other hand, noncumulative measures of plastic flow such as plastic deformation gradient F P of (3.31) or plastic strain tensor ε P of (3.80) are not always realistic choices for internal state variables. From a microscopic perspective (Sections 3.2.1, 3.2.2, and 3.2.53.2.7), plastic deformation is regarded as latticepreserving or lattice invariant (Bilby et al. 1957), and dislocations may pass completely through a volume element of the crystal, engendering significant plastic deformation without leaving behind any defects that would render the energetic state of the crystal different from that of an initially perfect lattice. From a macroscopic perspective, prescription of F P (or, for example, ε P in the linear case) as a state variable fails in applications wherein external loading is not monotonic. For example, a crystalline specimen can be deformed plastically and then deformed plastically again to its original shape. Under such a sequence, the material in its final state will often contain larger internal residual stresses, more defects, and greater energy of cold work (Farren and Taylor 1925; Taylor and Quinney 1934; Rosakis et al. 2000) than the specimen in its initial state, yet such changes will not be reflected by F P or ε P , since these variables are negligible both at the start and the end of the cyclic experiment. Finally, particular forms of constitutive assumptions (4.45)(4.49) should not lead to violations of the fundamental balance principles of continuum thermomechanics: balances of mass, momentum, and energy. In addition, thermodynamic processes should be thermodynamically admissible, meaning they should satisfy the ClausiusDuhem inequality. 4.2.2 The ClausiusDuhem Inequality
The ClausiusDuhem inequality, alternatively referred to as the entropy production inequality or dissipation inequality, is the particular form of the Second Law of Thermodynamics usually considered in continuum mechanics. The global form of the ClausiusDuhem inequality is written for a continuous body in spatial configuration B as q, n d ρr ρη dv ≥ ∫ dv − ∫ ds , (4.57) ∫ dt v θ θ v s where heat flux vector q( x, t ) and heat source scalar r ( x, t ) were introduced in (4.32). Applying the divergence theorem to the rightmost term,
4.2 Internal State Variables and the Dissipation Inequality
∫
q, n
θ
s
g
ds = ∫ ∇, v
q
θ
dv = ∫ v
1
θ
g
∇, q dv − ∫ v
1
θ
2
g
∇θ , q dv ,
or in indicial notation, −1 a −1 a −1 a −2 a ∫ θ q na ds = ∫ (θ q );a dv = ∫ θ q;a dv − ∫ θ θ,a q dv . s
v
v
189
(4.58) (4.59)
v
The local form of (4.57) becomes, upon using Reynolds transport theorem (4.14) and (4.59), (4.60) Γ = ρη + θ −1 (q;aa − ρ r − θ −1q aθ , a ) ≥ 0 . Above, Γ is the total entropy production rate per unit spatial volume that, according to the Second Law of Thermodynamics, must be nonnegative. The entropy production rate is often written on a per unit mass basis by dividing (4.60) by mass density ρ ( x, t ) > 0 (Malvern 1969). When Γ = 0 , the corresponding thermodynamic process is said to be thermodynamically reversible or conservative; when Γ > 0 , the process is said to be irreversible or dissipative. Entropy production law (4.60) is often partitioned into two separate, more restrictive inequalities (Truesdell and Noll 1965): Γ L = ρη + θ −1 ( q;aa − ρ r ) ≥ 0 , Γ C = −θ −2 q aθ ,a ≥ 0 , (4.61) where Γ L is the rate of local entropy production and Γ C is the rate of entropy production attributed to heat conduction. The first inequality in (4.61) is often referred to as the strong form of the ClausiusDuhem inequality, and it requires that the specific entropy rate η be nonnegative in the absence of heat supply r and heat conduction q. The second inequality of (4.61) prevents heat from spontaneously flowing from regions of low temperature to high temperature. Though more general constitutive equations for heat flux are possible (Truesdell and Noll 1965), the following constitutive assumption in the spatial frame is standard for many solids: g
q = −k ∇θ , q a = − k abθ ,b , Γ C = θ −2θ , a k abθ,b ≥ 0 ,
(4.62)
where k ( x, t ) ∈ Tx B × Tx B is the contravariant tensor of thermal conductivity, assumed symmetric and positive semidefinite. Conductivity k may generally depend on temperature, deformation, other state variables, position, and orientation of the material element. When all entries of k ab are constants, (4.62) is often referred to as Fourier’s law of heat conduction. From differentiation of the free energy in Table 4.2, θη = e − ψ − θη , so that after multiplying by θ , (4.60) can be written
190
4 Thermomechanics of Crystalline Solids
ρθη + (q;aa − ρ r − θ −1q aθ , a )
(4.63) = ρ (e −ψ − θη − r ) + q;aa − θ −1q aθ , a ≥ 0. For classical continua, substitution of energy balance (4.35) into (4.63) then gives (4.64) σ ab Dab − ρψ − ρθη − θ −1q aθ ,a ≥ 0 . Expanding the rate of free energy ψ of (4.45) using the chain rule (Coleman and Noll 1963) gives ∂ψ ∂ψ ∂ψ ∂ψ (4.65) ψ = La F .La θ+ γa + α, α + ∂F .α ∂θ ∂θ, a ∂α where as noted following (2.129), G A ( X ) = 0 since convected reference coordinates are not considered. The rate of temperature gradient is γ a = d (θ,a ) / dt = d (θ, A F −1.Aa ) / dt = θ,a + θ ,b FAb F .−a1 A (4.66) = θ,a − θ ,b FAb F −1.Aa = θ ,a − θ ,b v;ba = θ ,a − θ ,b Lb.a . Substitution of (4.65) into (4.64) then results in a local form of the ClausiusDuhem inequality that accounts for constitutive dependencies allotted in (4.45): ⎡ ∂ψ ∂ψ ⎞ ∂ψ ∂ψ ⎤ ⎛ σ ab Dab − ρ ⎢ La F .La γa + α ⎥ ≥ θ −1q aθ ,a . (4.67) α + ⎜η + ⎟θ + ∂θ ⎠ ∂θ , a ∂α ⎥⎦ ⎝ ⎢⎣ ∂F .α Quantity − ρ∂ψ / ∂α is often referred to as a conjugate thermodynamic force or conjugate driving force to thermodynamic flux α . Thermodynamic processes for which θ = 0 are called isothermal processes. Processes for which η = 0 are labeled isentropic processes. Processes for which q a = 0 are referred to as adiabatic processes. The ClausiusDuhem inequality exhibits an analogous representation in reference configuration B0 . The referential representation can be derived starting from a global principle like (4.57), but couched in the reference frame, or by converting local quantities using appropriate pullback and Piola transform operations. The latter approach is pursued here. Local dissipation inequality (4.60) becomes, upon multiplying by J ( X , t ) > 0 ,
Γ 0 = J Γ = ρ 0η + θ −1 ( Jq;aa − ρ 0 r − θ −1 Jq aθ , a ) = ρ 0η + θ −1 (Q;AA − ρ 0 r − θ −1Q Aθ , A ) ≥ 0,
(4.68)
where mass density ρ 0 = ρ J by (4.10), heat flux Q A = JF.a−1 A q a by (4.36), and Jq;aa = Q;AA by (4.37). A heat conduction law of the following form in
4.3 Kinetics and Inelastic Rates
191
the reference configuration can be prescribed, so that the rightmost term in (4.68) associated with conduction is always nonnegative: G
Q = −K ∇ θ , Q A = − K ABθ , B , −θ −2Q Aθ , A = θ −2θ , A K ABθ , B ≥ 0 ,
(4.69)
where K ( X , t ) ∈ TX B0 × TX B0 is a symmetric and positive semidefinite matrix of thermal conductivity. Similarly to k of (4.62), K of (4.69) may depend on temperature as is often the case in crystalline solids, strain, location and orientation of the material element (heterogeneity and anisotropy), as well as internal state variables. Consistency with (4.62) implies that spatial and referential matrices of thermal conductivity are related by k ab = J −1 F. Aa K AB F.Bb . From (4.68) and ψ = e − θη , an analog of (4.63) measured as an energy rate per unit reference volume is ρ 0 (e − ψ − θη − r ) + Q;AA − θ −1Q Aθ , A ≥ 0 . (4.70) Substituting referential energy balance (4.39) into (4.70) gives (4.71) Σ AB E AB − ρ 0ψ − ρ 0θη − θ −1Q Aθ, A ≥ 0 . Then upon expanding the rate of free energy per unit mass ψ using (4.65), the referential form of (4.67) is ⎡ ∂ψ ∂ψ ⎞ ⎛ Σ AB E AB − ρ 0 ⎢ La F .La α + ⎜η + ⎟θ ∂θ ⎠ ⎝ ⎣ ∂F .α (4.72) ∂ψ ∂ψ ⎤ −1 A + γa + α ⎥ ≥ θ Q θ, A . ∂θ , a ∂α ⎥⎦ In the case of geometric linearity, i.e., small deformations with (4.40), dissipation inequality (4.67) is simply ⎡ ∂ψ ∂ψ ⎞ ∂ψ ∂ψ ⎤ ⎛ σ abε ab − ρ ⎢ L β abL + ⎜η + γa + α ⎥ ≥ θ −1q aθ ,a , (4.73) ⎟θ + ∂ ∂ ∂ ∂ β θ θ α ⎝ ⎠ ,a ⎣⎢ ab ⎦⎥ where dependence of free energy ψ on lattice distortion β abL of (3.75) replaces dependence of free energy on lattice deformation gradient F La.α in constitutive assumption (4.45).
4.3 Kinetics and Inelastic Rates The term kinetics is used generically in this book to denote thermodynamically irreversible processes involving rates or fluxes of matter or energy. For example, kinetic processes in crystals include defect generation and
192
4 Thermomechanics of Crystalline Solids
motion, such as dislocation nucleation and glide or vacancy production and diffusion. Other irreversible processes include damage evolution in the form of microcracking in brittle solids or pore collapse in crushable solids. Kinetic processes are contrasted to reversible processes in crystalline solids such as mechanically elastic deformation in the absence of viscosity or internal friction. Kinetic processes involve dissipation of energy, for example heat produced by the conjugate pair of dislocation velocity and lattice friction (Kocks et al. 1975), or the rate of work of crack sliding conjugate to frictional forces along fracture surfaces in contact. In the context of (4.67) or (4.72), dissipation may result from three physical mechanisms: heat conduction, mechanical deformation, and time rates of internal state variables. As noted in Section 4.2.1, internal state variables typically account for irreversible structural rearrangements within crystalline solids, often at a microscopic scale of resolution. Regardless of mechanism or physical origin, dissipative energy changes in the solid can often be written in the generic form k
d = ∑ λ i Zi ,J i ,
(4.74)
i =1
where d is the time rate of energy change or dissipation, J i is a generalized rate or flux, Zi is a generalized conjugate force to J i , and λ i ≥ 0 is a scalar multiplier, each for fluxforce pair i. Summation in (4.74) runs over i = 1, 2,...k generalized fluxforce pairs that may be scalars, vectors, or tensors of higher order. To ensure that energetic changes associated with (4.74) are always dissipative, or always contribute positively to the rate of entropy production Γ in (4.60) for example, the dissipation potential concept is often invoked (Ziegler 1963; Germain et al. 1983): ∂Θ ∂Ω Zi = i , J i = i , (4.75) ∂J ∂Z where scalar potentials Θ and Ω are constructed such that d ≥ 0 in (4.74). A straightforward way to guarantee positive dissipation is prescription of the quadratic forms 1 k 1 k Θ = ∑ J i ,Oij J j , Ω = ∑ Zi ,oij Z j , (4.76) 2 i , j =1 2 i , j =1 where operators O and o are symmetric with respect to i and j and are positive definite. Potentials (4.76) lead to linear relationships between fluxes and forces known as Onsager’s relations (Onsager 1931a, b): k
k
j =1
j =1
Zi = ∑ Oij J j , J i = ∑ oij Z j . The rate of dissipated energy of (4.74) in these cases is
(4.77)
4.3 Kinetics and Inelastic Rates k
k
i , j =1
i , j =1
d = ∑ λ i J i ,Oij J j = ∑ λ i Zi ,oij Z j ≥ 0 .
193
(4.78)
Kinetic relations of the form (4.77) are convenient and physically realistic in some, but not all, circumstances (Onsager 1931a, b). Ziegler (1963) demonstrated that Onsager’s relations correspond to a principle of maximum entropy production or maximum dissipated energy, an appealing concept if one follows the viewpoint that kinetic processes in materials take place in such a way that stored energy in the substance tends to evolve towards a minimum value. However, linear relations of the form (4.77) are not the most general kinetic laws that simply ensure positive entropy production, and in many cases more physically realistic alternatives exist. Energetic changes attributed to heat conduction often follow the scheme outlined in (4.74)(4.78). From (4.61), dissipation from conduction is 1 (4.79) d = θΓ C = − q aθ, a .
θ
In the scheme of (4.74), λ = θ −1 > 0 , heat flux J a = q a , and Z a = −θ, a is a conjugate thermodynamic force. A dissipation potential can be defined: 1 Ω = θ, a k abθ,b , (4.80) 2 where in the context of (4.76), o = k is the symmetric thermal conductivity. Using (4.75), this potential leads to Fourier conduction: ∂Ω ∂Ω (4.81) qa = =− = − k abθ,b , ∂ (−θ ,a ) ∂θ ,a and to unconditionally nonnegative dissipation in (4.78): 1 (4.82) d = θ, a k abθ,b ≥ 0 .
θ
Next consider energetic changes associated with evolution of internal state variables. Following (4.67), the time rate of change of a single internal state variable α produces a rate of change in free energy ∂ψ (4.83) d = −ρ α, ∂α where in the notation of (4.74), λ = 1 , the flux is the rate of the internal variable J = α , and the conjugate force is the negative free energy derivative Z = − ρ∂ψ / ∂α . In this context, d > 0 implies that the material dissipates energy as a result of structural rearrangements associated with rates of internal variables, leading to a decrease in Helmholtz free energy ψ . Structural rearrangements need not always be dissipative, however, and in many cases lead to an increase in free energy of the solid, such that d < 0 .
194
4 Thermomechanics of Crystalline Solids
An example of such an energetic storage process in a crystal is an increase in defect density and corresponding increase in residual elastic energy associated with stress fields of individual defects. However, to ensure positive dissipation when physically appropriate, a dissipation potential can still be used along the lines of (4.74)(4.78) to dictate rates of internal variables or their conjugate thermodynamic forces. Finally, consider energetic changes stemming from rates of inelastic deformation. For illustrative purposes, consider specifically the time rate of plastic deformation gradient F P of multiplicative decomposition (3.31), and its work conjugate stress measure labeled here as Z P . More precise definitions of appropriate inelastic rates and conjugate stress measures are derived in Chapter 6 dealing with elastoplasticity, but a generic description suffices for now. The dissipation associated with this stressdeformation rate pair is Pα d = Z P ,F P = Z P .Aα F .A , (4.84) or in the terminology of (4.74), λ = 1 , flux J = F P , and the driving force Z = Z P . A dissipation potential can be constructed to ensure positive dissipation, i.e., 2Ω = Z P , λ P : Z P
N
PB N N = ( Z P.Aα λ Pαβ AB Z . β ) = Z ,
(4.85)
where λ P is a positive semidefinite operator of order four and is clearly a twopoint tensor. Exponent N (subject to constraint N > 0 ), when given a value other than unity, accounts for situations when a linear dependence of the dissipation potential on scalar product Z is physically inappropriate. The rate of plastic deformation becomes, from the second of (4.75), ∂Ω ∂Ω Pα PB F P = P = NZ N −1λ P : Z P , F .A = P A = NZ N −1λ Pαβ (4.86) AB Z .β , ∂Z .α ∂Z and the dissipation of (4.78) is always nonnegative: d = NZ N −1 Z P ,λ P : Z P = NZ N ≥ 0 . (4.87) P αβ When the matrix λ P is isotropic, i.e., λ Pαβ AB = λ g G AB , the rate of plastic
deformation gradient is coaxial with driving stress Z P : Pα F P = NZ N −1λ P Z P , F .A = NZ N −1λ P g αβ GAB Z P .Bβ ,
(4.88)
and λ P is the plastic multiplier found by squaring both sides of (4.88): λ P = N −2 Z 1− 2 N F P : F P = N −2 Z 1− 2 N F .APα gαβ G AB F .BP β , (4.89) As demonstrated by example in Section 6.4 of Chapter 6, a description similar to (4.88) is often used in macroscopic plasticity theories for ductile metals, such that the time rate of plastic deformation and its driving force
4.3 Kinetics and Inelastic Rates
195
always share the same direction. A distinct kinetic relation, or a constitutive assumption such as the consistency condition of associative plasticity (see Section 6.4), specifies the magnitude of the plastic deformation gradient rate via the instantaneous value of λ P ( X , t ) . In plasticity theory, the explicit prescription of the rate of plastic deformation is often labeled a flow rule. When derived from the gradient of a plastic potential, e.g., Ω of (4.86), plastic deformation is said to obey a normality principle. When each rate α of an internal variable representing a microscopic structural rearrangement—for example dislocation position or cumulative slip—is dictated solely by its conjugate driving force − ρ∂ψ / ∂α , the temperature θ , and the current values of the set of such structural variables, a generalized normality structure similar to that depicted in (4.86) emerges for increments of plastic strain (Rice 1971). However, derivation of such a normality structure seems to require that the increment of plastic deformation gradient (or plastic strain) be characterized by a kinematic equation of the form δ F P = Σ(∂F P / ∂α )δα , with summation applied over all structural α
variables α, an equation which may not always be physically realistic if α are interpreted as internal state variables in the usual energetic sense of continuum thermomechanics. Recall that plastic slip is often not a valid internal state variable associated with energetic changes in the crystal, as explained in Section 4.2.1, so a direct correspondence between F P and usual internal state variable(s) may not always exist5.
5 More precisely, Rice (1971) defines an increment in a symmetric plastic strain tensor as the change in total strain resulting from changes in microscopic structural variable(s) with macroscopic stress and temperature held constant. The number of such structural variables may thus far exceed the number of internal state variables of the averaging type (i.e., α) needed to characterize the average free energy of a volume element of the solid.
5 Thermoelasticity
Deformation of a crystalline solid is labeled, in this book, as purely elastic in the absence of defect motion and temperature changes. In an elastic material of grade one, the mechanical stress supported by a material particle located at a particular point in space and the deformation gradient or strain in the material at that point are related by a constitutive law, e.g., a local tensorvalued version of Hooke’s law relating force and stretch. A hyperelastic material of grade one can be defined as a material possessing a strain energy density function depending on the firstorder deformation gradient, or on a symmetric deformation tensor or strain tensor constructed from this deformation gradient (Truesdell and Noll 1965). In such a material, the partial derivative of strain energy density with respect to a deformation gradient component produces a corresponding stress component, more precisely a component of the first PiolaKirchhoff stress tensor. Thermoelasticity by definition addresses recoverable mechanical deformation (i.e., elastic deformation from body and surface forces) and thermal effects (e.g., temperature rates, temperature gradients, heat sources, and heat flux) as well as their couplings (e.g., thermal expansion or contraction). Two alternative formulations of finite deformation thermoelasticity of grade one are presented in Chapter 5. In both cases, following the theme of this book, the focus is geared towards crystalline solids, though many aspects of these theories apply for arbitrary solid bodies, regardless of crystallinity. Both formulations rely on balance laws for classical continua presented in Section 4.1 and the general treatment of dissipation in Section 4.2. Viscoelasticity, a ratedependent elastic response that may involve local entropy production (i.e., entropy production even in the absence of heat conduction), is not addressed in this book. Discussion of electromechanical coupling effects present in elastic dielectric crystals is deferred until later in Chapter 10. In the first formulation—which can best be labeled traditional nonlinear thermoelasticity—presented in Sections 5.15.4, the contribution to the deformation gradient arising from temperature changes is not explicitly delineated in the kinematic description, and independent, timedependent variables entering constitutive response functions consist of the total deformation gradient and temperature. Dependence of strain energy of the
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_5, © Springer Science+Business Media B.V. 2011
197
198
5 Thermoelasticity
material upon the firstorder deformation gradient, and not higherorder gradients of position or strain, indicates a hyperelastic response of grade one, as noted in Section 4.2.1. As explained in Section 4.2.1 and discussed explicitly later in Chapter 5, objectivity requirements reduce dependence of thermodynamic potentials and response functions on deformation gradient to a dependence on a stretch tensor (or a symmetric deformation or strain tensor) derived from the deformation gradient. This formulation follows classical treatments of hyperelasticity with temperature changes (Truesdell and Noll 1965; Thurston 1974; Marsden and Hughes 1983; Rosakis et al. 2000). Materially nonlinear and materially linear constitutive models are discussed. Relationships among material coefficients derived from thermodynamic potentials are presented in Section 5.2 for general threedimensional stress states (Section 5.2.1) as well as hydrostatic stress states (Section 5.2.2), following earlier work of Thurston (1974). Symmetry properties of material coefficients are discussed, with a brief focus on isotropic behavior representative of nontextured polycrystals; the reader is directed to Appendix A for an extensive treatment of symmetry properties of all thirtytwo crystal classes. In Section 5.3, a free energy function accounting for large thermoelastic volume changes but small elastic shape changes, applicable for example at large hydrostatic pressures observed in some shock physics experiments, is described. In Section 5.4, reduction of the finite strain theory to the geometrically linear case is considered for completeness. In a second, alternative or nontraditional formulation of nonlinear thermoelasticity presented in Section 5.5, purely thermal deformation induced by temperature changes is explicitly delineated in the kinematic description from the mechanical deformation associated with applied stresses. Independent state variables in thermodynamic potentials consist of mechanical elastic deformation and temperature. The deformation gradient is decomposed multiplicatively into an elastic part associated with mechanical loading and a thermal part associated with temperature changes, following the qualitative discussion of Section 3.2.2. Such a formulation, while not following what may be termed classical thermoelasticity, offers a more detailed depiction of the kinematics and provides different thermodynamic relationships among independent and dependent state variables (Stojanovitch 1969; Lu and Pister 1975; Imam and Johnson 1998; Clayton 2005a, b, 2006a). Thermal strain can be expressed via an evolution equation associated with the temperature rate (Lee et al. 1997), and additional thermoelastic couplings emerge via higherorder thermal stress coefficients, e.g., those reflecting dependence of elastic moduli on temperature. Dissipative effects are omitted in the final two Sections of Chapter 5. Section 5.6 presents the Lagrangian field theory of elasticity, wherein the
5.1 Nonlinear Elasticity and Thermoelasticity
199
linear momentum balance and constitutive laws of hyperelasticity of grade one are deduced from EulerLagrange equations of the appropriate action integral. Section 5.7 discusses hyperelastic bodies of grade two, following the variational approach of Toupin (1964). Such materials may support hyperstresses (including couple stresses) and do not obey the classical balance laws of continuum mechanics presented in Chapter 4 apart from the conservation of mass of Section 4.1.2 which is presumed identical for elastic materials of grades one and two. This Chapter, while providing detailed descriptions of selected topics in thermoelasticity, does not provide a comprehensive account of the whole subject of elasticity to which numerous books have been entirely devoted. For completeness, a few other relevant references include Love (1927), Landau and Lifshitz (1959), Marsden and Hughes (1983), and Ogden (1997). References specifically dealing with nonlinear elasticity of anisotropic crystals include Thurston (1974) and Teodosiu (1982).
5.1 Nonlinear Elasticity and Thermoelasticity In a thermoelastic crystalline material not containing mobile defects, or in which contributions from defects to deformation are negligible, the deformation gradient is asserted to follow (3.25): F ( X , t ) = T ϕ X (t ) = F L ( X , t ), (5.1) F. Aa = x.,aA = F L.aα g.αA = F La. B g.Bα g.αA = F L.aA .
In this context, there is no need for introduction of an evolving intermediate configuration, since the lattice deformation serves as the local tangent map F L ( X , t ) : TX B0 → Tx B . Recall that superscript L indicates deformation of the lattice (e.g., deformation of primitive Bravais lattice vectors and basis vectors in (3.109)(3.110)) in the volume element of crystal associated, symbolically, with material point X, under the CauchyBorn hypothesis. From (5.1), this superscript is dropped from the notation for the lattice or total deformation gradient F in the remainder of Chapter 5 without consequence. 5.1.1 Constitutive Assumptions Applying (5.1), and prior to consideration of objectivity requirements, appropriate versions of functional dependencies of dependent state variables (4.45)(4.48) for a hyperelastic material of grade one are
200
5 Thermoelasticity
g ⎛ ⎞ (5.2) ⎝ ⎠ g ⎛ ⎞ (5.3) η = η ⎜ F,θ , ∇ θ , X , G A ⎟ , η = η ( F. Aa ,θ ,θ, a , X , G A ) ; ⎝ ⎠ g ⎛ ⎞ σ = σ ⎜ F,θ , ∇ θ , X , G A ⎟ , σ ab = σ ab ( F. Aa ,θ ,θ,a , X , G A ) ; (5.4) ⎝ ⎠ g ⎛ ⎞ (5.5) q = q ⎜ F,θ , ∇ θ , X , G A ⎟ , q a = q a ( F. Aa ,θ ,θ , a , X , G A ) . ⎝ ⎠ Independent quantities (in parentheses) are deformation gradient, temperature, spatial temperature gradient, position or choice of material particle at X, and reference basis vectors. The present definition of a hyperelastic material includes no internal state variables, meaning that (4.49) is not needed. Dependence on deformation gradient follows arguments given in Section 4.2 and relations (3.109)(3.114) of Chapter 3. Specifically, F reflects, to first order, the stretch of interatomic bonds since primitive Bravais lattice and basis vectors in a volume element of a crystal structure at point X deform according to the value of F ( X , t ) at that point at time t. Since changes in interatomic bond distances and angles result in mechanical stresses and corresponding changes in energy stored in the crystal, as explained in detail in Appendix B in the context of discrete lattice statics, dependence of Cauchy stress and free energy on F is appropriate1. De
ψ = ψ ⎜ F,θ , ∇ θ , X , G A ⎟ , ψ = ψ ( F. Aa ,θ ,θ , a , X , G A ) ;
1 In polyatomic structures, internal (i.e., inner) displacements discussed in Section 3.1.2 also affect bond distances and angles, and hence free energy and other response functions. Recall from (3.20) that Q(0k ) denotes the inner displacement vector for basis atom k, with K the total number of atoms in the basis. Without loss of generality, let the primitive Bravais lattice and k = 0 coincide, so Q(00 ) = 0 . Since Q(0k ) can be determined if the other independent state variables (e.g., deformation gradient and temperature) are known, internal displacement(s) need not be included in the list of independent state variables entering (5.2)(5.5). For example, the free energy of a homogeneous material in the athermal case can be written as ψ ( F ) = ψˆ ( F, Q(0k )(F ) ) . Inner displacement vector(s) at a given de
formation gradient F can then obtained as the solution of (Tadmor et al. 1999) ∂ψˆ ∂ 2ψˆ = 0 ( ∀ k = 1,... K − 1) ; positive definite . ∂Q(0k ) F ∂Q(0k )∂Q(l0 ) It follows that at the equilibrium conditions corresponding to this solution, K −1 ∂Q(0k ) ∂ψˆ ∂ψ ∂ψˆ ∂ψˆ . = +∑ = 0 ∂F ∂F Q (0k ) k =1 ∂Q( k ) F ∂F ∂F Q (0k )
5.1 Nonlinear Elasticity and Thermoelasticity
201
pendence of entropy and heat flux on deformation gradient is written out following the equipresence principle. Dependence of free energy and entropy on temperature depicts wellknown phenomena, e.g., from physical chemistry, of the specific heat capacity of the material to account for changes in energy and entropy that accompany local thermal vibrations of atoms as well as possibly significant electronic contributions. Dependence of stress on temperature enables a description of thermal expansion, while dependence of heat flux on temperature enables a description of temperaturedependent conductivity. Dependence of heat flux on temperature gradient enables, for example, use of Fourier’s law of (4.62). Dependence of the other state variables on temperature gradient is written out in (5.2)(5.4) for completeness, but will be eliminated following thermodynamic considerations in Section 5.1.2. As discussed in Section 4.2.1, dependence of response functions on X is included to permit description of a heterogeneous body, that is a body whose properties such as elastic stiffness, mass density, or thermal conductivity vary with position in the undeformed state. Dependence on basis vectors G A ( X ) , often implied rather than written out explicitly in other presentations of elasticity theory, is used to describe solids exhibiting an anisotropic response, as explained more in Section 5.1.5. ˆ +c, Under superposed rigid body motions of the spatial frame x → Qx ˆ =Q ˆ −T is a spatially constant rotation matrix and c is a spatially where Q
constant translation vector, vector and tensorvalued variables entering (5.2)(5.5) transform as F. Aa → Qˆ .ab F. Ab , σ ab → Qˆ.acσ cd Qˆ.bd , q a → Qˆ.ab q b , θ ,a → Qˆ.abθ ,b . (5.6) Scalars (i.e., free energy, entropy, and temperature) associated with a given material particle X, as well as reference basis vectors G A ( X ) , are all invariant under such spatial coordinate transformations. From (5.6), it is clear that constitutive assumptions of the general form (5.2)(5.5) are not always objective, since independent and dependent variables transform differently under a change of spatial basis. To conform to objectivity requirements, constitutive assumptions for thermoelastic solids should satisfy the following requirements (Coleman and Noll 1963; Coleman and Gurtin 1967), where the spatial temperature gradient is expressed in contravariant vector form following the last of (5.6): g g ⎛ ⎞ ⎛ˆ ˆ ∇θ , X , G ⎞ , (5.7) ψ ⎜ F,θ , ∇ θ , X , G A ⎟ = ψ ⎜ QF ,θ , Q A⎟ ⎝ ⎠ ⎝ ⎠ g g ⎛ ⎞ ⎛ˆ ˆ ∇θ , X , G ⎞ , (5.8) η ⎜ F,θ , ∇ θ , X , G A ⎟ = η ⎜ QF ,θ , Q A⎟ ⎝ ⎠ ⎝ ⎠
202
5 Thermoelasticity
g g ˆ ⎛ F,θ ∇ θ , X , G ⎞ Q ˆ T = σ ⎛ QF ˆ ,θ , Q ˆ ∇θ , X , G ⎞ , (5.9) Qσ A⎟ A⎟ ⎜ ⎜ ⎝ ⎠ ⎝ ⎠ g g ˆ ⎛ F,θ , ∇ θ , X , G ⎞ = q ⎛ QF ˆ ,θ , Q ˆ ∇θ , X , G ⎞ . (5.10) Qq A⎟ A⎟ ⎜ ⎜ ⎝ ⎠ ⎝ ⎠ A number of possible variations of (5.2)(5.5) satisfy (5.7)(5.10). The forms suggested below are straightforward and are frequently encountered: G ψ = ψ ⎛⎜ C,θ , ∇θ , X , G A ⎞⎟ , ψ = ψ ( C AB ,θ ,θ, A , X , G A ) ; (5.11) ⎝ ⎠ G (5.12) η = η ⎛⎜ C,θ , ∇ θ , X , G A ⎞⎟ , η = η ( C AB ,θ ,θ , A , X , G A ) ; ⎝ ⎠ G ⎛ ⎞ (5.13) Σ = Σ ⎜ C,θ , ∇ θ , X , G A ⎟ , Σ AB = Σ AB ( C AB ,θ ,θ, A , X , G A ) ; ⎝ ⎠ G ⎛ ⎞ (5.14) Q = Q ⎜ C,θ , ∇ θ , X , G A ⎟ , Q A = Q A ( C AB ,θ ,θ, A , X , G A ) . ⎝ ⎠ where symmetric deformation tensor C AB = F. Aa g ab F. Bb by (2.153), symmet
ric second PiolaKirchhoff stress tensor Σ AB = JF.a−1 Aσ ab F.b−1B according to (4.6)(4.7) and the identities listed in Table 4.1, referential heat flux vector Q A = JF.a−1 A q a by (4.36), and referential temperature gradient θ , A = F. Aaθ , a as in (4.51). All variables of order one or greater in (5.11)(5.14) exhibit indicial components referred to reference configuration B0 and are invariant under spatial coordinate transformations (see e.g., (4.50)(4.51)). For purposes of constructing strain energy functions in constitutive models of thermoelastic response, the following versions of (5.11)(5.14) are often useful, and will be invoked frequently in Chapter 5: G ψ = ψ ⎛⎜ E,θ , ∇θ , X , G A ⎞⎟ , ψ = ψ ( E AB ,θ ,θ, A , X , G A ) ; (5.15) ⎝ ⎠ G η = η ⎛⎜ E,θ , ∇ θ , X , G A ⎞⎟ , η = η ( E AB ,θ ,θ , A , X , G A ) ; (5.16) ⎝ ⎠ G ⎛ ⎞ Σ = Σ ⎜ E,θ , ∇ θ , X , G A ⎟ , Σ AB = Σ AB ( E AB ,θ ,θ , A , X , G A ) ; (5.17) ⎝ ⎠ G ⎛ ⎞ Q = Q ⎜ E,θ , ∇ θ , X , G A ⎟ , Q A = Q A ( E AB ,θ ,θ, A , X , G A ) ; (5.18) ⎝ ⎠ where symmetric right CauchyGreen strain tensor 2 E AB = C AB − GAB by (2.156) and is also invariant under rigid body transformations of the spatial coordinate system, since
5.1 Nonlinear Elasticity and Thermoelasticity
203
T T ˆTb ˆ a c 2 E AB = FAa F. Ba − G AB → FAb Q.a Q.c F. B − G AB
(5.19) T = FAb F. Bb − GAB = 2 E AB . Dependence of response functions on strain tensor E rather than on deformation tensor C is useful for linearization of the energy density about a strainfree reference state, since E = 0 at a reference state in which F = 1 and C = 1 . 5.1.2 Thermodynamics
Using kinematic assumption (5.1) and constitutive assumptions (5.2)(5.5), dissipation inequality (4.67) referred to spatial configuration B becomes ⎡ ∂ψ ∂ψ ⎞ ∂ψ ⎤ ⎛ σ ab Dab − ρ ⎢ a F. Aa + ⎜η + γ a ⎥ − θ −1q aθ , a ≥ 0 . (5.20) ⎟θ + ∂θ ⎠ ∂θ, a ⎥⎦ ⎝ ⎢⎣ ∂F. A The stress power per unit current volume can be written as follows: σ ab Dab = σ ab Lab = σ ab FaA F −1.Ab = J −1 Pa. A F. Aa , (5.21) with P the first PiolaKirchhoff stress of (4.6). Substituting into (5.20), ⎛ ∂ψ ⎞ ⎛ −1 . A ∂ψ ⎞ a ∂ψ ⎞ ⎛ −1 a ⎟ γ a − θ q θ, a ≥ 0 . (5.22) ⎜ J Pa − ρ a ⎟ F. A − ρ ⎜η + ⎟θ − ρ ⎜⎜ ⎟ F ∂ ∂ ∂ θ θ ⎝ ⎠ .A ⎠ ⎝ ⎝ ,a ⎠ Presuming that rates of deformation gradient, temperature, and temperature gradient (i.e., F , θ , and γ ) can be prescribed arbitrarily—i.e., independently of each other and of their coefficients in a thermodynamic process—such coefficients (in parentheses in (5.22)) should vanish identically (Coleman and Noll 1963). Presumably, judicious application of body force b a of (4.17) and heat source r of (4.34) enables this arbitrary prescriptions of rates F , θ , and γ . Such reasoning leads to the constitutive relations ∂ψ ∂ψ ∂ψ (5.23) Pa. A = ρ0 , η =− , = 0. a ∂F. A ∂θ ∂θ, a Notice from (5.2)(5.4) that free energy, entropy, and stress do not depend on F , θ , or γ . If, on the other hand, the dependent state variables were permitted to depend on rates of deformation gradient, temperature, or temperature gradient, it would not be possible to vary such rates independently of their coefficients in (5.22), and hence (5.23) would not necessarily follow. Because the heat flux vector and temperature gradient are explicitly related through (5.5), neither can be varied arbitrarily in (5.22), and neither
204
5 Thermoelasticity
must vanish in a generic heat conductor. From (4.6), the Cauchy stress tensor satisfies ∂ψ b (5.24) F. A . σ ab = J −1 g ac Pc. A F. Ab = ρ ∂FaA It follows from (5.23) that free energy, entropy, and stress do not depend explicitly on the spatial temperature gradient: ψ = ψ ( F,θ , X , G A ) , η = η ( F,θ , X , G A ) , σ = σ ( F,θ , X , G A ) . (5.25) Since θ > 0 , the local entropy production inequality reduces to the conduction inequality in the second of (4.61). θΓ = θΓ C = −θ −1θ ,a q a ≥ 0 . (5.26) The rate of local entropy production vanishes in a hyperelastic material: θΓ L = ρθη + q;aa − ρ r = σ ab Dab − ρψ − ρθη = 0 . (5.27) A similar procedure can be followed with the entropy inequality (4.72) referred to the reference configuration taken as a starting point, which becomes, using (5.1) and (5.11)(5.14), ⎛ Σ AB ∂ψ ⎞ ∂ψ ⎞ ⎛ − ρ0 ⎜ ⎟ C AB − ρ 0 ⎜η + ⎟θ ∂ ∂θ ⎠ 2 C ⎝ AB ⎠ ⎝ (5.28) ∂ψ A −1 − ρ0 γ 0 A − θ θ, AQ ≥ 0, ∂θ , A where 2 E AB = C AB . The reference rate of temperature gradient satisfies ∂ψ ∂ψ ∂θ, A ∂ψ a ∂ψ γa = γa = F. Aγ a = γ 0 A ⇔ γ 0 A = F. Aa γ a . (5.29) ∂θ, a ∂θ, A ∂θ, a ∂θ, A ∂θ, A The following stressstrain and temperatureentropy relations are then deduced for hyperelastic materials, using (2.158): ∂ψ ∂ψ ∂ψ ∂ψ ∂ψ Σ AB = 2 ρ0 = ρ0 = ρ0 = Σ BA , η = − , = 0 . (5.30) ∂C AB ∂E AB ∂EBA ∂θ ∂θ , A It follows that in addition to the free energy, the entropy and stress do not depend explicitly on the referential temperature gradient: ψ = ψ ( C,θ , X , G A ) , η = η ( C,θ , X , G A ) , Σ = Σ ( C,θ , X , G A ) . (5.31) Since θ > 0 , the entropy production inequality reduces to the conduction inequality: JθΓ = JθΓ C = −θ −1θ , AQ A ≥ 0 . (5.32) The rate of local entropy production vanishes: (5.33) JθΓ L = ρ0θη + Q;AA − ρ0 r = Σ AB E AB − ρ0ψ − ρ0θη = 0 .
5.1 Nonlinear Elasticity and Thermoelasticity
205
Writing the free energy as ψ = ψ ( C(F ( X , t ), g ( x)),θ , X , G A ) and using (2.158) with (5.23) and (5.30), the following relationships emerge: ∂ψ ∂ψ ∂ECD ∂ψ P aA = F.Ba Σ BA = 2 ρ0 F.Ba = 2 ρ 0 F.Ba = ρ 0 F.Ba , (5.34) ∂CAB ∂ECD ∂CAB ∂EBA ∂ψ ∂ψ ∂C AB ∂ψ b ∂ψ ∂ψ −1B = = F. Aa = F −1.Aa (5.35) F. B ⇔ F .b , ∂g ab ∂C AB ∂g ab ∂C AB ∂C AB ∂g ab ∂ψ b ∂ψ ∂ψ σ ab = J −1 F. Aa Σ AB F.Bb = 2 ρ F. Aa F. B = 2 ρ = 2ρ = σ ba . (5.36) ∂C AB ∂g ab ∂gba Notice from (5.30) and (5.36) that angular momentum balances (4.26) and (4.27) are satisfied identically: Σ = ΣT and σ = σT . The first of (5.30) provides the relationship between the reference second PiolaKirchhoff stress Σ and a pullback of the spatial metric g, while (5.36) provides the relationship between a pushforward of the reference stress Σ and the spatial metric g. Relation (5.36) is often called the DoyleEricksen formula (Doyle and Ericksen 1956; Yavari et al. 2006). From (2.182) and (5.36), in a hyperelastic material the spatial stress power can be expressed compactly in terms of the scalar product of the derivative of the free energy with respect to metric g and its Lie derivative with respect to the velocity field: ∂ψ σ, D = ρ , Lv g . (5.37) ∂g Relation (5.34) can also be deduced directly from (2.158) and (5.23): ∂ψ ∂CBC ∂ψ ∂ψ Pa. A = ρ 0 g abδ .BA F.Cb = 2 ρ0 g ab F. Bb . (5.38) = 2 ρ0 a ∂CBC ∂F. A ∂CBC ∂C AB As noted in Section 4.2, alternative choices of independent and dependent state variables are possible. One typical prescription regards the entropy as an independent variable and temperature as a dependent variable, with the internal energy e used as the primary thermodynamic potential: e = e ( F,η , X , G A ) , θ = θ ( F,η , X , G A ) , σ = σ ( F,η , X , G A ) , (5.39) where the partial Legendre transform (Marsden and Hughes 1983) e = θ ( F,η , X , G A )η + ψ ( F,θ , X , G A ) . (5.40) From the second of (5.30) and the chain rule, ∂e ∂ψ ∂ψ ∂θ ∂θ = + + η ∂F. Aa ∂F. Aa ∂θ ∂F. Aa ∂F. Aa (5.41) ∂ψ ∂θ ⎛ ∂ψ ⎞ ∂ψ , = + +η ⎟ = ⎜ a ∂F. Aa ∂F. Aa ⎝ ∂θ ⎠ ∂F. A
206
5 Thermoelasticity
so that constitutive relationships for the first PiolaKirchhoff stress, second PiolaKirchhoff stress, and Cauchy stress in terms of internal energy are ∂e ∂e ∂e ∂e , Σ AB = 2 ρ 0 , σ ab = 2 ρ . (5.42) Pa. A = ρ0 = ρ0 a ∂g ab ∂F. A ∂C AB ∂E AB The thermodynamic analysis of (5.20)(5.42) is often labeled the ColemanNoll procedure, after Coleman and Noll (1963). In the present Section, this procedure is applied to hyperelastic crystalline solids, following Teodosiu (1982) for example, though formal analytical methods of Coleman and coworkers have been applied to numerous classes of materials (Coleman and Noll 1963; Coleman 1964; Coleman and Mizel 1964; Coleman and Gurtin 1967; Maugin 1988). It is also noted that constitutive relations among stress, deformation gradient, free or internal energy, temperature, and entropy need not be derived for hyperelastic bodies using the Second Law of thermodynamics or the ColemanNoll procedure. For example, Marsden and Hughes (1983) obtain (5.30) by applying principles of locality, the balance of energy, and covariance. Other approaches can be found in Eringen (1962) and Truesdell and Noll (1965). Alternatively, stress and entropy can simply be assigned in hyperelastic solids as derivatives of thermodynamic potentials, taking (5.30) as basic definitions (Thurston 1974). When temperature rates and temperature gradients are omitted from the description, the body is said to be elastic as opposed to thermoelastic. In such a description, let θ = constant such that θ = 0 and θ , A = 0 , and let the heat flux q and heat source r vanish. Conduction inequality (5.32) is identically zero, and the entropy production (5.27) becomes θΓ L = ρθη = 0 . (5.43) Since temperature and entropy are treated as constants, there is no need to include them explicitly in the thermodynamic description. General expressions (5.31) for free energy and stress become ψ = ψ ( C, X , G A ) , Σ = Σ ( C, X , G A ) , (5.44) and the resulting constitutive equations are ∂ψ ∂ψ ∂ψ ∂ψ , Σ AB = 2 ρ 0 = ρ0 , σ ab = 2 ρ Pa. A = ρ 0 . (5.45) a ∂F. A ∂C AB ∂E AB ∂g ab The temperatureindependent thermodynamic potential ψ = ψ (C, X , G A ) is called the strain energy density. Relations (5.45) along with the balance of linear momentum and boundary conditions can also be obtained from Hamilton’s principle of stationary action, as demonstrated later in Section 5.6.
5.1 Nonlinear Elasticity and Thermoelasticity
207
The specific heat capacity at constant deformation gradient F (i.e., at constant strain E) is introduced as ∂e ∂e ∂η ∂e ∂ ⎛ ∂ψ ⎞ ∂ 2ψ , (5.46) c= = =− = − θ ⎜ ⎟ ∂θ ∂η ∂θ ∂η ∂θ ⎝ ∂θ ⎠ ∂θ 2 since from the second of (5.23) and (5.40), ∂e ∂ ∂ ∂θ ⎛ ∂ψ ⎞ (5.47) = (θη ) + ψ = θ + ⎜η + ⎟ =θ . ∂η ∂η ∂η ∂η ⎝ ∂θ ⎠ Also often used for thermoelastic solids is Fourier’s Law of conduction, as first introduced in (4.69), leading to nonnegative dissipation from conduction: Q A = − K ABθ , B , −θ , AQ A = θ , A K ABθ , B ≥ 0 . (5.48) From (5.33) and (5.48), the local energy balance can be expressed as d ⎛ ∂ψ ⎞ AB (5.49) −θ ⎜ ρ0 ⎟ = ( K θ, B ) ; A + ρ0 r . dt ⎝ ∂θ ⎠ Note that, by the chain rule, ∂ ⎛ ∂ψ ∂ψ ⎞ d ⎛ ∂ψ ⎞ −θ ⎜ ρ 0 θ⎟ E AB + ⎜ ⎟ = −θρ 0 ∂θ ⎝ ∂E AB ∂θ ⎠ dt ⎝ ∂θ ⎠ (5.50)
= θβ AB E AB + ρ 0 cθ , where (5.15) has been used and where the symmetric contravariant tensor β = −∂Σ / ∂θ = − ρ 0 ∂ 2ψ / ∂θ∂E accounts for thermoelastic coupling. Equating (5.49) and (5.50) results in a rate equation for the temperature: ρ 0 cθ = ( K ABθ, B ) ; A − θβ AB E AB + ρ0 r . (5.51) In the absence of strain rate E (e.g., a rigid body) and heat sources r, and when K AB = KG AB with K a constant (e.g., an isotropic homogeneous conductor), (5.51) becomes the transient heat equation K G2 K K −1 G GG ABθ, A , B , θ= ∇ θ= (G ABθ, A ) ; B = (5.52) ρ0c ρ0 c ρ0 c where the Laplacian is given by (2.77).
(
)
5.1.3 Materially Nonlinear Hyperelasticity
Differentiation of (5.23) and (5.30) results in definitions of secondorder elastic stiffness coefficients: ∂P. A ∂ 2ψ A.aA.b. B (F,θ , X , G A ) = a b = ρ0 , (5.53) ∂F.B ∂F. Aa ∂F. Bb
208
5 Thermoelasticity
∂Σ AB ∂ 2ψ = ρ0 . (5.54) ∂ECD ∂E AB ∂ECD Coefficients in (5.53) and (5.54) are generally not constants and are labeled as tangent moduli when evaluated at particular values of the state variables. Thirdorder coefficients are defined via further differentiation: ∂ 2 P. A ∂ 3ψ A.aA.b.B.c.C (F,θ , X , G A ) = b a c = ρ0 , (5.55) a ∂F. B ∂F.C ∂F. A ∂F. Bb ∂F.Cc ABCD
(E,θ , X , G A ) =
∂ 2 Σ AB ∂ 3ψ . (5.56) = ρ0 ∂ECD ∂EEF ∂E AB ∂ECD ∂EEF Tangent moduli of orders four and higher can be defined by straightforward extension, i.e., additional differentiation with respect to deformation gradient or strain. The following symmetries follow automatically from definitions (5.53)(5.54) and symmetry of E AB = E( AB ) : ABCDEF
(E,θ , X , G A ) =
A.aA.b.B = A.bB.a. A , Tensor A
. A. B a .b
ABCD
=
( AB )( CD )
=
CDAB
.
(5.57)
consists of 45 independent entries before consideration of
material symmetry, while ABCD consists of up to 21 independent entries. Similarly, A.aA.b.B.c.C = A.bB.a. A.c.C = A.aA.c.C.b. B , (5.58) ABCDEF = ( AB )( CD )( EF ) = CDABEF = ABEFCD . In particular, thirdorder tangent stiffness ABCDEF consists of up to 56 independent entries. Transformation formulae among elastic coefficients are deduced as follows. Since from (2.158), ∂P. A ∂F ∂Σ EA ∂ECD A.aA.b.B = a b = aEb Σ EA + FaE ∂F. B ∂F. B ∂ECD ∂F. Bb (5.59) = g ab Σ AB + FaC ACBD FbD , it follows from (5.57) that ACBD = F −1.Aa A aCbD F −1.Bb − Σ AB F −1.Ca g ab F −1.Db . (5.60) Similarly, the relationship between thirdorder tangent elasticity coefficients is, using (5.58), AEBDCG = (A aAbBcC − ABCF g ab F.Fc (5.61) − ACBF g ac F.Fb − AFBC g bc F. Fa ) F −1.Ea F −1.Db F −1.Gc . Expressing free energy (5.31) of a hyperelastic material with thermal effects in a Taylor series of multiple variables (cf. Hoffman (1992)) about a reference state wherein F. Aa = g.aA , C AB = GAB , E AB = 0 , and θ = θ 0 > 0
5.1 Nonlinear Elasticity and Thermoelasticity
209
produces the following result per unit reference volume, where free energy per unit reference volume Ψ 0 is introduced in (4.9):
Ψ 0 = ρ0ψ ( E AB ,θ , X , G A ) = Ψ0 +
AB
E AB +
1 2!
ABCD
E AB ECD +
1 3!
ABCDEF
E AB ECD EEF
1 ABCDEFGH E AB ECD EEF EGH + ... − β AB E AB ∆θ 4! (5.62) 1 1 − β ABCD E AB ECD ∆θ − β ABCDEF E AB ECD EEF ∆θ − ... 2! 8 1 1 AB − β ′ E AB (∆θ ) 2 − β ′′ AB E AB (∆θ )3 − ... 8 2! 1 ABCD E AB ECD (∆θ )2 ... + Y0 (θ , X ) . − β′ 4 Temperature change from the reference state ∆θ = θ − θ 0 can be positive, zero, or negative. Presuming sufficient differentiability of Ψ 0 with respect to independent state variables, quantities in (5.62) are defined as follows: (5.63) Ψ 0 ( 0,θ 0 , X , G A ) =Ψ 0 ( X ) + Y0 (θ 0 , X ) = 0 , +
AB
ABCD
ABCDEF
ABCDEFGH
( X ,G A ) =
( X ,G A ) =
∂Ψ 0 ∂E AB
=0,
(5.64)
E=0
θ =θ0
∂ 2Ψ 0 ∂E AB ∂ECD
,
(5.65)
E=0 θ =θ0
( X ,G A ) =
∂ 3Ψ 0 ∂E AB ∂ECD ∂EEF
( X ,G A ) =
∂ 4Ψ 0 ∂E AB ∂ECD ∂EEF ∂EGH
β AB ( X , G A ) = − β ABCD ( X , G A ) = −
∂ 2Ψ 0 ∂θ∂E AB
∂ 3Ψ 0 ∂θ∂E AB ∂ECD
E=0
(5.66)
,
(5.67)
E =0 θ =θ0
,
(5.68)
E=0 θ =θ 0
=− θ =θ0
, E=0 θ =θ0
∂
ABCD
∂θ
, E= 0
θ =θ0
(5.69)
210
5 Thermoelasticity
β ABCDEF ( X , G A ) = −
∂ 4Ψ 0 ∂θ∂E AB ∂ECD ∂EEF
=− E =0 θ =θ 0
β ′ AB ( X , G A ) = −
∂ 3Ψ 0 ∂θ 2 ∂E AB
β ′′ AB ( X , G A ) = −
∂ 4Ψ 0 ∂θ 3∂E AB
β ′ ABCD ( X , G A ) = −
∂ 4Ψ 0 ∂θ 2 ∂E AB ∂ECD
∂
∂θ
, (5.70) E =0 θ =θ0
,
(5.71)
,
(5.72)
E=0 θ =θ0
E= 0 θ =θ0
=− E=0 θ =θ 0
ABCDEF
∂2
ABCD
∂θ 2
.
(5.73)
E=0 θ =θ0
The total free energy at the reference state is chosen as a zero datum in (5.63) for convenience (Ψ 0 ( X ) = −Y0 (θ 0 , X ) ), since from inspection of the derivations in Section 5.1.2, the dependent variables stress, entropy, and heat flux only depend on derivatives of the free energy and not its absolute value. Firstorder elastic constants AB are zero by definition in (5.64) so that by (5.30) and (5.34), stress vanishes in the reference state. Coefficients in (5.65)(5.67) are referred to, respectively, as isothermal secondorder elastic constants, isothermal thirdorder elastic constants, and isothermal fourthorder elastic constants. Stresstemperature coefficients of various orders are defined in (5.68)(5.73); some of these can be interpreted as temperature derivatives of the elastic moduli at the reference state as indicated. All constants in (5.65)(5.73) can depend on position X in a heterogeneous body as well as orientation G A ( X ) , but have fixed values at each point X. Stressstrain and entropytemperature relations become 1 ABCDEF 1 ABCDEFGH Σ AB = ABCD ECD + ECD EEF + ECD EEF EGH + ... 2 6 3 − β AB ∆θ − β ABCD ECD ∆θ − β ABCDEF ECD EEF ∆θ − ... (5.74) 8 1 1 1 − β ′ AB (∆θ ) 2 − β ′′ AB (∆θ )3 − ... − β ′ ABCD ECD (∆θ ) 2 ..., 2 8 2
5.1 Nonlinear Elasticity and Thermoelasticity
N 0 = ρ0η = −
211
∂Ψ 0 ∂θ
∂Y0 1 1 + β AB E AB + β ABCD E AB ECD + β ABCDEF E AB ECD EEF + ... (5.75) ∂θ 2 8 3 1 2 +β ′ AB E AB ∆θ − β ′′ AB E AB (∆θ ) − ... − β ′ ABCD E AB ECD ∆θ .... 8 2 The thermal energy Y0 is not expanded in a polynomial series in (5.62) since such an expansion is usually deemed more appropriate for internal energy rather than free energy. Two early models for thermal energy of solids include Einstein’s model (Einstein 1907) and Debye’s model (Debye 1912). A thermal internal energy is defined as ∂Y U 0 (θ , X ) = Y0 − θ 0 . (5.76) ∂θ According to Einstein’s model (Born and Huang 1954), ⎡ ξ 2 eξ ⎤ ∂U 0 ξ ⎞ ⎛ξ , (5.77) = 3nk B ⎢ ξ U 0 = 3nk Bθ ⎜ + ξ ⎟ , C0 = 2 ⎥ ∂θ ⎝ 2 e −1⎠ ⎣ (e − 1) ⎦ =−
where C0 (θ ) is a specific heat per unit reference volume and ξ = Θ E / θ , Θ E = hν E / k B , (5.78) with Einstein’s temperature ΘE presently assumed constant for a given substance with characteristic vibrational frequency ν E , measured here in units of cycles per second. Planck’s constant and Boltzmann’s constant are written as h = 2π and k B , respectively. The number of degrees of freedom per unit reference volume is 3n. For a monatomic crystal 3n = 3/ Ω0 , with Ω0 the atomic volume introduced in Section 3.1.1. According to Debye’s model, considered more accurate for many crystalline solids (Born and Huang 1954; Brillouin 1964), thermal internal energy and specific heat are given by ⎡⎛ θ ⎞3 ΘD / θ ⎛ 1 1 ⎞ 3 ⎤ (5.79) U 0 = 9nk Bθ ⎢⎜ ⎟ ∫ ⎜ + ξ ⎟ ξ dξ ⎥ , ⎢⎣⎝ Θ D ⎠ 0 ⎝ 2 e − 1 ⎠ ⎥⎦ ⎡⎛ θ ⎞3 ΘD / θ eξ ξ 4 ⎤ ∂U 0 = = C0 9nk B ⎢⎜ dξ ⎥ , (5.80) ⎟ ∫ ξ 2 ∂θ ⎢⎣⎝ Θ D ⎠ 0 (e − 1) ⎥⎦
212
5 Thermoelasticity
where Debye’s temperature ΘD is here assumed constant2 for a substance with characteristic maximum frequency ν D of vibrational modes: Θ D = hν D / k B . (5.81) At relatively high temperatures θ ΘD , the energy U 0 in (5.79) is linear in temperature, and the specific heat in (5.80) is constant: ⎡⎛ θ ⎞3 ΘD / θ ⎤ 2 U 0 ≈ 9nk Bθ ⎢⎜ (5.82) ⎟ ∫ ξ d ξ ⎥ = 3nk Bθ , C0 ≈ 3nk B . ⎢⎣⎝ ΘD ⎠ 0 ⎥⎦ At relatively low temperatures θ θ D , (5.79) and (5.80) become (Brillouin 1964) ⎛ 3π 4 ⎞ ⎛ 12π 4 ⎞ (5.83) U0 = ⎜ nk B ⎟θ 4 + C , C0 = ⎜ nk B ⎟ θ 3 , 3 3 ⎝ 5ΘD ⎠ ⎝ 5Θ D ⎠ with C a material constant reflecting the cohesive or total ground state internal energy of the undeformed material at θ = 0 . Methods of derivation of elastic coefficients in (5.53)(5.61), and elastic constants in (5.65) and (5.66), using atomistic models (i.e., lattice statics) are provided in Sections B.2.4B.2.6 of Appendix B. Derivations of thermoelastic and thermal properties of matter (e.g., stresstemperature coefficients, thermal conductivity, and caloric equations of state), apart from the brief treatment in (5.76)(5.83), from atomistic or quantum mechanical models fall outside the scope of this book. Such derivations can instead be found in books by Slater (1939), Born and Huang (1954) and Brillouin (1964), while Slater (1955) gives a historical account of quantum theories of specific heats of condensed matter. Methods of extending or combining Debye and Einstein models for specific heats of polyatomic substances wherein effects of intramolecular vibrations are significant are also discussed by Slater (1939).
Debye’s temperature Θ D is constant for a given substance according to the model of (5.79) that omits coupling between vibrational energy and specific volume. Frequency ν D can be related to sound speeds and hence elastic constants (Hearmon 1956). More generally, Θ D = Θ D ( J , θ ) , where dependence on absolute temperature is most evident at very low temperatures (Born and Huang 1954; Bian et al. 2008). Volumetric (i.e., J) dependence of Debye and Einstein temperatures is considered explicitly in Section 5.2.2 in the context of Gruneisen’s parameter. 2
5.1 Nonlinear Elasticity and Thermoelasticity
213
5.1.4 Materially Linear Hyperelasticity Material coefficients of orders three and higher (e.g., third and fourthorder elastic constants) can be of importance for crystalline solids in high pressure events such as shock physics experiments wherein elastic deformations can be large, or high temperature events wherein nonlinear thermal expansion can be significant (Thurston 1974; Hiki 1981; Graham 1992). Higherorder elastic constants also affect elastic wave speeds in pressurized media, and provide insight into anharmonic atomic interactions (Appendix B, Section B.2.5). On the other hand, in many practical applications, higherorder coefficients can be omitted from the series expansion of the free energy while still maintaining a reasonably accurate depiction of thermoelastic behavior. In such cases, (5.62) becomes 1 ABCD θ Ψ0 = E AB ECD − β AB E AB ∆θ − ρ 0 cθ ln , (5.84) θ0 2 where elastic constants ABCD , stresstemperature coefficients β AB , and specific heat c are defined as second derivatives of the free energy at null strain and reference temperature: ⎛ ∂ 2ψ ⎞ ∂ 2Ψ 0 ∂ 2Ψ 0 ABCD = , β AB = − , c = − ⎜θ 2 ⎟ . (5.85) ∂E AB ∂ECD E =0 ∂θ∂E AB E= 0 ⎝ ∂θ ⎠ E =0 θ =θ0
θ =θ0
θ =θ 0
At a particular material point X, parameters in (5.85) are all constants. The thermal energy comprising the rightmost term in (5.84) depends only on temperature. This term (Abeyaratne and Knowles 1993) is consistent with a thermal internal energy U 0 measured per unit reference volume depending linearly on temperature: 1 ∂U 0 . (5.86) U 0 = ρ0 cθ ⇔ c = ρ0 ∂θ Stress and entropy measured in the reference configuration are Σ AB = ABCD ECD − β AB ∆θ , (5.87) ⎛ θ ⎞ N 0 = ρ0η = β AB E AB + ρ0 c ⎜ ln + 1⎟ . (5.88) ⎝ θ0 ⎠ In (5.87), the first term on the right accounts for stress due to strain and the second accounts for changes in stress resulting from changes in temperature ∆θ = θ − θ 0 . This is a geometrically nonlinear but materially linear constitutive relationship; i.e., second PiolaKirchhoff stress is linearly related to (finite) right CauchyGreen strain and the temperature change.
214
5 Thermoelasticity
At a fixed reference temperature θ = θ 0 , the requirement that the free energy Ψ 0 be positive for all nonzero strains E implies that the fourthrank tensor ABCD should be positive definite. From the first of (5.85), it follows that at θ = θ0 , in the material linear case addressed in (5.84), Ψ 0 is a strictly convex function3 of E. Stress equation (5.87) applies for any choice of reference configuration coordinate system, including Cartesian coordinates and general curvilinear coordinates. In physical components of orthogonal curvilinear coordinates (Section 2.4), the stressstrain law exhibits the same general form (Malvern 1969):
Σ
AB
=
3
∑
C , D =1
ABCD
E CD − β
AB
∆θ ,
(5.89)
where indices in angled brackets are referred to physical components of orthogonal curvilinear coordinates such as cylindrical coordinates of Section 2.4.2 and Table 4.3 or spherical coordinates of Section 2.4.3 and Table 4.4. Transformation formulae relating quantities in (5.89) to their counterparts in Cartesian coordinates are lengthy and are given by Malvern (1969). 5.1.5 Symmetry Following from (5.65) and (5.68), matrices of secondorder elastic constants ABCD and thermal stress constants β AB exhibit the following symmetries: ABCD = CDAB = BACD = ABDC , β AB = β BA , (5.90) meaning that ABCD contains up to 21, as opposed to 34 = 81 , independent entries, and β AB contains up to 6 as opposed to 32 = 9 independent entries. Appealing to such symmetry considerations, (5.87) is often written in reduced matrix form as (Nye 1957; Hirth and Lothe 1982)
3 In nonlinear elasticity in three spatial dimensions, convexity is not always necessary, and may be overly restrictive for addressing certain physical phenomena such as buckling associated with nonuniqueness of solutions (Marsden and Hughes 1983). Less restrictive assumptions such as polyconvexity and quasiconvexity may be more appropriate for strain energy functions of some kinds of materials. Also not addressed in Chapter 5 are nonconvex, multiwell strain energy potentials that may emerge in continuum theories of phase transformations (Ericksen 1975; Ball and James 1987; Abeyaratne and Knowles 1993).
5.1 Nonlinear Elasticity and Thermoelasticity ⎡ Σ 11 ⎤ ⎡ ⎢ 22 ⎥ ⎢ ⎢Σ ⎥ ⎢ ⎢ Σ 33 ⎥ ⎢ ⎢ 23 ⎥ = ⎢ ⎢Σ ⎥ ⎢ ⎢ Σ 31 ⎥ ⎢ ⎢ 12 ⎥ ⎢ ⎣⎢ Σ ⎦⎥ ⎣⎢
⎤ ⎡ E11 ⎤ ⎡ β 11 ⎤ ⎥⎢ ⎥ ⎢ 22 ⎥ ⎥ ⎢ E22 ⎥ ⎢ β ⎥ 36 ⎥ ⎢ E33 ⎥ ⎢ β 33 ⎥ ⎥ ⎢ ⎥ − ⎢ 23 ⎥ ∆θ 46 ⎥ ⎢ 2 E23 ⎥ ⎢ β ⎥ 56 ⎥ ⎢ 2 E ⎥ ⎢ β 31 ⎥ ⎥ ⎢ 31 ⎥ ⎢ ⎥ 66 12 ⎦⎥ ⎢⎣ 2 E12 ⎦⎥ ⎣⎢ β ⎦⎥
11
12
13
14
15
16
12
22
23
24
25
26
13
23
33
34
35
14
24
34
44
45
15
25
35
45
55
16
26
36
46
56
,
215
(5.91)
where components of the symmetric 6×6 matrix of elastic constants are ⎡ ⎢ ⎢ ⎢ ⎢ ⎢ ⎢ ⎢ ⎢⎣
11
=
1111
12
= = = = =
1122
22
1133
23
1123
24
13 14 15 16
−
1113
25
1112
26
= = = = =
− 2222 2233
33
2223
34
2213
35
2212
36
− = = = =
3333 3323
44
3313
45
3312
46
−
−
−
− − = = =
− − − = =
− − − − =
2323 2313
55
2312
56
1313 1312
66
⎤ ⎥ ⎥ ⎥ ⎥. ⎥ ⎥ ⎥ 1212 ⎥⎦
(5.92)
The indicial form of (5.92) is often referred to as Voigt’s notation (Voigt 1928). Nine components of symmetric secondorder tensors reduce to six according to the correspondence 11 ~ 1, 22 ~ 2, 33 ~ 3, (5.93) 23 = 32 ~ 4, 31 = 13 ~ 5, 12 = 21 ~ 6. In the compact notation of Brugger (1964), Thurston (1974), and Teodosiu (1982), components of the stress and thermoelastic moduli are rewritten to take advantage of these symmetries: Σ ( AB ) ~ Σ A , ( AB )(CD ) ~ AB , β AB ∼ β A . (5.94) Barred single indices span 1,2,…6 and correspond to unbarred pairs of indices as indicated in (5.93). Consistent with (5.91) and (5.94), strains are 2 E( AB ) = (1 + δ AB ) E A . (5.95)
As a consequence of hyperelasticity, secondorder elastic constants have the remaining symmetries
(5.96) = ( ). Using (5.94), Helmholtz free energy per unit reference volume in the materially linear case, (5.84), is expressed as 1 AB θ (5.97) Ψ0 = E A EB − β A E A ∆θ − ρ 0 c θ ln , θ0 2 and the second PiolaKirchhoff stress of (5.87) is written compactly as (5.98) Σ A = AB EB − β A ∆θ . AB
AB
Voigt’s notation can also be used for tangent moduli ABCD of (5.54) in the materially nonlinear regime, since tangent moduli exhibit the same symmetries as the constants in (5.90). Voigt’s notation is likewise often ap
216
5 Thermoelasticity
plied to thirdorder elastic constants, as described in Section A.3 of Appendix A. In many practical applications, the material axes (e.g., the conventional unit cell (lattice) vectors in a cubic crystal) and the reference coordinate axes do not coincide. In such cases, a rotation or reflection operation is required to represent the matrix of elastic constants in the reference coordinate system as opposed to the crystallographic frame. Let X ′ A denote coordinates in the crystallographic frame, and let X A denote coordinates in the reference configuration. The transformation X A = Q.AB X ′B (5.99) describes the relationship between coordinate systems, with orthogonal −1 A matrix Q satisfying Q.TA and  det Q.AB = 1 . When det Q.AB = +1 , the B = Q. B rotation is said to be proper orthogonal; otherwise, when det Q.AB = −1 , the operation is said to be improper orthogonal, i.e., a reflection. The elasticity tensor then transforms from its representation ′ ABCD in the crystal coordinate system to its representation ABCD in the reference coordinate system as a fourthorder tensor, while the thermal stress coefficients transform from β ′ AB to β AB as components of a rank two tensor: (5.100) = Q.AE Q.BF Q.CG Q.DH ′EFGH , β AB = Q.CA Q.BD β ′CD . Analogous formulae apply for tangent moduli in (5.54) and higherorder material coefficients in (5.62). In practice, the 6 × 6 square matrix of elastic moduli in crystallographic coordinates must often be converted to fourth rank ( 3 × 3 × 3 × 3 ) form by appealing to (5.92), and then the first of (5.100) can be applied. Finally, the resulting fourthorder elasticity tensor, now based in reference coordinates X A , can be converted back to 6 × 6 form by again using (5.92). In fields of crystallography and texture analysis, the three independent components of the matrix Q are often represented in terms of Euler angles describing successive angular rotations about particular directions in the sample (Bunge 1982; Kocks et al. 1998; Randle and Engler 2000; Cermelli and Gurtin 2001). One particular representation is (Cermelli and Gurtin 2001) Q = ⎡⎣exp ( −ϕ1εk ) ⎦⎤ ⎣⎡exp ( −ψεi ) ⎦⎤ ⎣⎡exp ( −ϕ2 εk ) ⎦⎤ , (5.101) ABCD
where the Euler angles in Bunge’s notation are limited to the range ϕ1 , ϕ2 ∈ [0, 2π ) , ψ ∈ [0, π ] , (5.102) A and (i, j, k ) form an orthonormal basis for the X ′ coordinate system. Arguments of matrix exponentials in (5.101) are skew, e.g.
5.1 Nonlinear Elasticity and Thermoelasticity
( −ϕ1εk ) AB = −ϕ1ε ABC k C .
217
(5.103)
The matrix exponential of a secondorder tensor A is ∞ 1 A2 exp A = ∑ A k = 1 + A + + .... (5.104) 2 k =0 k ! If A is skew (i.e., if AAB = − ABA ), then its matrix exponential exp A is a (proper) orthogonal tensor, i.e., a rotation. In that case, to first order in A, the difference exp A − 1 is also skew. Recall from (5.7)(5.18) and (5.31) that the thermodynamic potentials and response functions generally depend on reference basis vectors G A ( X ) , following the notational convention of Eringen (1962). Such dependence can be made explicit by considering effects of orthogonal transformations of reference coordinates along the lines of (5.99). Under such rotations or reflections Q , basis vector G A and metric tensor G(X) transform as D C G A → G B Q.BA , GAB → Q.CAGCD Q.DB = G AC Q.TC D Q. B = G AC δ . B = G AB . (5.105) Dependence of response functions on basis vectors is conventionally assumed to result only from dependence of independent state variables on the basis vectors, so that (5.31) can be written ψ = ψ ( C( X , G A ),θ , X ) , η = η ( C( X , G A ),θ , X ) , (5.106) Σ = Σ ( C( X , G A ),θ , X ) . Similarly, heat flux equation (5.14) becomes G ⎛ ⎞ Q = Q ⎜ C( X , G A ),θ , ∇ θ ( X , G A ), X ⎟ . (5.107) ⎝ ⎠ Deformation gradient F, right CauchyGreen deformation tensor C and Lagrangian strain tensor E transform as T T F. Aa → Q.BA F. Ba , C AB → QAC C.CD Q.DB , E AB → QAC E.CD Q.DB . (5.108) Heat flux Q and reference temperature gradient transform as T Q A → Q.AB Q B , θ, A → θ, B Q.BA = QAB (5.109) θ ,B . It follows that for all rotations and reflections Q ∈ within symmetry group of the considered material, the following identities apply:
ψ ( C,θ , X ) = ψ ( QT CQ,θ , X ) , η ( C,θ , X ) = η ( QT CQ,θ , X ) ,
(
(5.110) (5.111)
)
QΣ ( C,θ , X ) QT = Σ QT CQ,θ , X ,
(5.112)
218
5 Thermoelasticity
G G ⎛ ⎞ ⎛ ⎞ (5.113) QQ ⎜ C,θ , ∇ θ , X ⎟ = Q ⎜ QT CQ,θ , QT ∇ θ , X ⎟ . ⎝ ⎠ ⎝ ⎠ Regarding the heat flux vector, when Fourier’s law (5.48) applies, Q A = − K ABθ , B → −Q.CA ( K CBθ , B ) = −(Q.CA K CD Q.ED )(θ , B Q.BE ) . (5.114) Relations (5.110)(5.113) may result in a reduction of the number of independent components of material coefficients that can be defined as derivatives of thermodynamic potentials with respect to independent state variables couched in the reference configuration and listed as arguments of these potentials. Without loss of generality, C can be replaced by E in (5.110)(5.113). Such material coefficients include tangent elastic moduli (5.54) and (5.56), thermal stress coefficients, and elastic and thermal stress constants of all orders in (5.62)(5.73). Symmetric conductivity matrix K, while not the derivative of a thermodynamic potential, transforms in (5.114) as a secondorder tensor under changes of reference coordinates and thus should exhibit the same symmetries as material tensors that are secondorder derivatives of thermodynamic potentials (e.g., β AB of (5.100)). Specifically, when consists only of the identity map and the inversion, there is no reduction in the number of independent elasticity coefficients due to material symmetry; in this case, the crystalline material is said to be triclinic. The crystal class of a given crystal structure determines symmetry properties of thermoelastic material coefficients for that structure. Recall from Section 3.1, Table 3.1, and Fig. 3.2 that the seven crystal systems encompass fourteen different kinds of Bravais lattices. The symmetry of a crystal is further described by its crystal class or point group of symmetry operations comprising . Thirtytwo crystal classes exist for natural crystal structures, each falling into one of eleven Laue groups. Mechanical elastic properties such as second and thirdorder elastic constants depend only on the Laue group of the crystal, while other material coefficients such as vectors and tensors of odd rank (e.g., pyroelectric and piezoelectric coefficients emerging in electromechanical theories, as discussed in Chapter 10) can depend on the particular crystal class within a Laue group. A detailed discussion of symmetry of crystals in the context of material coefficients is provided in Appendix A. In particular, Tables A.3A.7 list the independent material coefficients for tensors of ranks one, two, three, and four, while Tables A.8 and A.9 list second and thirdorder elastic constants for all Laue groups. of the material contains all orthogonal When the symmetry group transformations, the response is independent of the choice of G A , and the material is said to be isotropic. Isotropy is extremely rare among single
5.1 Nonlinear Elasticity and Thermoelasticity
219
crystalline solids. However, the macroscopic response of polycrystals containing a large number of randomly oriented grains can often be accurately represented as isotropic, so that isotropic behavior is of keen interest in the general study of crystalline solids. In an isotropic solid, (5.52) applies for heat conduction in the context of Fourier’s law, and (5.106) reduces to ψ = ψ ( I1 , I 2 , I 3 ,θ , X ) , η = η ( I1 , I 2 , I 3 ,θ , X ) , (5.115) Σ = Σ ( I1 , I 2 , I 3 ,θ , X ) . Three scalar invariants of C are defined as 1 I1 = C.AA , I 2 = (det C)tr(C−1 ) = ⎡⎣C.AAC.BB − C.AB C.BA ⎤⎦ , I 3 = det C . (5.116) 2 For isotropic materials, it follows from (5.30) and (5.115)(5.116) that the second PiolaKirchhoff stress can be written 3 ∂ψ ∂ψ ∂I λ Σ AB = 2 ρ 0 = 2ρ0 ∑ ∂C AB (5.117) λ =1 ∂I λ ∂C AB = α 0G AB + α1C AB + α 2C AD CD.B . where the scalar functions α λ generally depend on the invariants of C, the temperature, and location in the material (Marsden and Hughes 1983): (5.118) α λ = α λ ( I1 , I 2 , I 3 ,θ , X ) , (λ = 0,1, 2) . The tangent elastic stiffness of (5.54) becomes, for an isotropic material, ∂ 2ψ ∂ 2ψ ABCD = ρ0 = 4ρ0 ∂E AB ∂ECD ∂C AB ∂CCD = γ 1G AB G CD + γ 2 (C AB G CD + G AB C CD ) + γ 3 (C 2 AB G CD + G AB C 2CD ) + γ 4C AB C CD + γ 5 (C
CD
+C C
+ γ 7 (G G
BD
+ γ 8 (G C
BD
2 AB
C
AC
AC
AB
2 CD
) + γ 6C
2 AB
C
+G G
AD
)
+G C
AD
+ G AD C BC + G BD C AC ),
BC
BC
(5.119)
2 CD
where the notation (C2 ) AB = C 2 AB = C AC CC. B and coefficients are scalar functions of the following form: γ χ = γ χ ( I1 , I 2 , I 3 ,θ , X ) , ( χ = 1, 2,...8) . (5.120) Thus the maximum number of independent components of ABCD at material point X is reduced from 21 to 8 in a nonlinear isotropic thermoelastic solid. Now consider a materially linear, isotropic hyperelastic solid. In that case, the secondorder elastic constants in (5.85) become
220
5 Thermoelasticity
ABCD
= ρ0
∂ 2ψ ∂E AB ∂ECD
E =0
= 4 ρ0
θ =θ0
∂ 2ψ ∂C AB ∂CCD
C=G
θ =θ0
(5.121)
= µ (G AC G BD + G AD G BC ) + λ G AB G CD , with µ ( X ) = γ 7 the shear modulus and λ ( X ) = γ 1 Lamé’s constant, both evaluated at the reference state. The remaining parameters γ χ in (5.119) are redundant in the materially linear theory and can be set to zero. Thus, the elasticity tensor consists of two independent components, and in 6×6 matrix form is written as ⎡ 2µ + λ ⎢ λ ⎢ ⎢ λ ⎡⎣ ⎤⎦ = ⎢ ⎢ 0 ⎢ 0 ⎢ ⎢⎣ 0
λ λ
λ λ 2µ + λ
0 0 0
0
0
µ
0 0
0 0
0 0
2µ + λ
0⎤ 0 ⎥⎥ 0⎥ ⎥. 0⎥ 0⎥ ⎥ µ ⎥⎦
0 0 0 0
µ 0
(5.122)
Secondorder thermal stress coefficients for an isotropic material exhibit the form ∂ 2ψ ∂ 2ψ β AB = − ρ0 = −2 ρ 0 = β G AB , (5.123) ∂θ∂E AB E= 0 ∂θ∂C AB C= G θ =θ 0
θ =θ 0
with β a constant. For isotropic solids, transformation formulae are not needed among orthogonal reference coordinate frames since (5.100) degenerates to ABCD = ′ ABCD and β AB = β ′ AB . Stressstraintemperature relations exhibit the form Σ AB = 2µ E AB + (λ E.CC − β ∆θ )G AB . (5.124) Defining the bulk modulus for a materially linear, isotropic elastic solid as K = 2 µ / 3 + λ , (5.124) can be inverted to give
Σ β 1 1 ⎛ ⎞ (5.125) 2 µ ⎜ E AB − E.CC G AB ⎟ = Σ AB − Σ .CC GAB , E.AA = . A + ∆θ . 3 K K 3 3 ⎝ ⎠ The first of equality of (5.125) is recognizable as a relationship between ′ and deviatoric strain E AB ′ : the deviatoric (i.e., traceless) stress Σ AB 1 1 ′ = 2µ E AB ′ , Σ AB ′ = Σ AB − Σ .CC G AB , E AB ′ = E AB − E.CC GAB . (5.126) Σ AB 3 3 The second of (5.125) relates traces of strains and stresses and temperature change. When deformations are small, E.AA ≈ J − 1 ≈ u;aa accurately reflects volume changes in the material, as is clear from (2.162)(2.164). From inA
5.2 Thermostatic Relationships
221
version of the second of (5.125) and assuming stressfree strain from isotropic thermal expansion of the form E.AA = αT ∆θδ . AA = 3αT ∆θ with
Σ . AA = 0 , the relationship between the coefficient of thermal expansion α T and β is obtained: β = 3K α T . (5.127) Elastic isotropy is discussed in more detail in Section A.3.3 of Appendix A, including representations of thirdorder elastic constants and a complete table of algebraic relationships among various secondorder elastic constants (Table A.10).
5.2 Thermostatic Relationships A number of material coefficients, and relationships among these coefficients, can be derived from thermodynamic potentials of Table 4.2 and results of the analysis of Section 5.1.2. Such derivations are given in Section 5.2, primarily following from the presentation of Thurston (1974). Wallace (1972) offers a similar account. The general situation involving threedimensional states of stress is considered first in Section 5.2.1, while the special scenario of a spherical state of Cauchy stress (i.e., hydrostatic pressure without deviatoric or shear stresses) is considered in Section 5.2.2. 5.2.1 Threedimensional Stress States
Consider thermostatic potentials, measured as energy per unit reference volume as in (4.9), of the following functional forms: E0 = E0 ( EAB , N 0 , X , G A ) , H 0 = H 0 ( Σ AB , N 0 , X , G A ) , (5.128)
Ψ 0 = ( E AB ,θ , X , G A ) , G0 = G0 ( Σ AB ,θ , X , G A ) ,
(5.129)
where the entropy per unit reference volume is of the functional form N 0 = N 0 ( E AB , E0 , X , G A ) . (5.130) In the remainder of Section 5.2, dependence of potentials on material symmetry (e.g., via G A ) and position of material particle X is implied and not written out explicitly, and partial derivatives of functions are assumed to take place with G A and X fixed. With this reduction in notation, and using Voigt’s notation (5.93)(5.95) with barred indices spanning 1, 2,...6 ,
(
)
E0 = E0 ( E A , N 0 ) , H 0 = H 0 Σ A , N 0 ,
(5.131)
222
5 Thermoelasticity
(
)
Ψ 0 =Ψ 0 ( E A ,θ ) , G0 = G0 Σ A ,θ , N 0 = N 0 ( E A , E0 ) .
(5.132) (5.133)
Multiplying the relationships in Table 4.2 by ρ 0 ( X ) produces
H 0 = E0 − Σ AB E AB = E0 − Σ A E A ,
(5.134)
Ψ 0 = E0 − θ N 0 , G0 = H 0 − θ N 0 .
(5.135) (5.136)
Differentials of the potentials are found from (5.131)(5.136): dE0 = Σ A dE A + θ dN 0 , dH 0 = − E A d Σ A + θ dN 0 ,
(5.137)
dΨ 0 = Σ dE A − N 0 dθ , dG0 = − E A d Σ − N 0 dθ . (5.138) First derivatives then provide the following thermostatic relationships: ∂Ψ 0 ∂G ∂E ∂H 0 , (5.139) N0 = − =− 0 , θ = 0 = ∂θ E ∂θ Σ ∂N 0 E ∂N 0 Σ A
ΣA =
∂E0 ∂E A
A
∂Ψ 0 ∂H 0 , EA = − ∂E A θ ∂Σ A
N0
∂N 0 ∂N 0 , Σ A = −θ ∂E0 E ∂E A
E0
= N0
1
θ
=
=−
∂G0 , ∂Σ A θ
(5.140)
.
(5.141)
Specific heats per unit reference volume at constant strain, CE , and constant stress, CΣ are defined respectively as CE =
CΣ =
∂E0 ∂θ
∂H 0 ∂θ
=θ E
=θ Σ
∂N 0 ∂θ
= −θ E
∂N 0 ∂θ
= −θ Σ
∂ 2Ψ 0 ∂θ 2
E
∂ 2G0 ∂θ 2
Σ
,
(5.142)
.
(5.143)
From (5.46), CE is related to specific heat per unit mass c via CE = ρ 0 c . Subscripts on specific heat coefficients in (5.142) and (5.143) are labels of scalar quantities and are not subject to the Einstein summation convention. Second derivatives provide isothermal and isentropic elastic stiffness coefficients (i.e., tangent moduli) of second order: ∂ 2Ψ 0 ∂ 2Ψ 0 ∂Σ A ∂Σ AB AB , ABCD = ; (5.144) = = = ∂EB θ ∂E A ∂EB θ ∂ECD θ ∂E AB ∂ECD θ AB
=
∂Σ A ∂EB
= N0
∂ 2 E0 ∂E A ∂EB
, N0
ABCD
=
∂Σ AB ∂ECD
= N0
∂ 2 E0 ∂E AB ∂ECD
. (5.145) N0
5.2 Thermostatic Relationships
223
Isothermal secondorder coefficients are identical to those introduced in Section 5.1.3. Isentropic coefficients are denoted by an underscore and are sometimes referred to as adiabatic coefficients (e.g., adiabatic elastic moduli) in applications wherein heat conduction and (radiative) heat supply do not arise, since in that case, (5.27) results in N 0 = ρ0η = J ρη = 0. Notice the symmetry conditions AB = BA and AB = BA follow identically from the assumption of hyperelasticity. Isothermal coefficients are typically used for elastostatic problems, while isentropic coefficients are typically deemed appropriate for studies of wave propagation (Thurston 1974). Isothermal and isentropic elastic compliances are defined, respectively, as ∂E A ∂ 2 G0 ∂ 2G0 ∂E AB S AB = , S ; (5.146) = − = = − ABCD ∂Σ CD θ ∂Σ AB ∂Σ CD θ ∂Σ B θ ∂Σ A ∂Σ B θ
SAB =
∂E A ∂Σ B
=− N0
∂2 H0 ∂Σ A ∂Σ B
, SABCD = N0
∂E AB ∂Σ CD
=− N0
∂2 H0 ∂Σ AB ∂Σ CD
. (5.147) N0
Symmetry relations S AB = SBA and SAB = SBA apply. Secondorder elastic stiffness and compliance tensors are related by ∂EB ∂Σ A ∂Σ A ∂EB AB A AB SBC = δ = , S = = δ.CA ; (5.148) .C BC C ∂EB θ ∂Σ θ ∂EB N ∂Σ C N0 0
2 ABCD SCDEF = δ . EAδ .BF + δ .FA δ .BE , 2 ABCD SCDEF = δ . EAδ .BF + δ .FA δ .BE . (5.149) Thirdorder elastic stiffness coefficients are defined via further differentiation of (5.144)(5.145) with respect to strain: ∂ 3Ψ 0 ∂ 3Ψ 0 ∂ 2Σ A ABC , ABCDEF = ; (5.150) = = ∂E AB ∂ECD ∂EEF θ ∂EB EC θ ∂E A ∂EB EC θ ABC
=
∂2Σ A ∂EB ∂EC
= N0
∂ 3 E0 ∂E A ∂EB ∂EC
, N0
ABCDEF
=
∂ 3 E0 ∂E AB ∂ECD ∂EEF
. (5.151) N0
Isothermal thirdorder elastic stiffness coefficients are identical to those of Section 5.1.3. Notice the symmetry conditions ABC = BAC = ACB and ABC = BAC = ACB . Isothermal and isentropic thirdorder compliances are, respectively, ∂ 3G0 ∂ 3G0 S ABC = − , S ; (5.152) = − ABCDEF ∂Σ AB ∂Σ CD ∂Σ EF θ ∂Σ A ∂Σ B ∂Σ C θ
224
5 Thermoelasticity
SABC = −
∂3 H 0 ∂Σ A ∂Σ B ∂Σ C
, SABCDEF = − N0
∂3 H 0 ∂Σ AB ∂Σ CD ∂Σ EF
.
(5.153)
N0
Symmetry relations S ABC = SBAC = S ACB and SABC = SBAC = SACB apply. Relationships among thirdorder stiffness and compliance coefficients can be derived as follows. Differentiation of the first of (5.148) by the strain tensor leads to ∂S ∂Σ E ∂ ( AB SBC ) = ABDSBC + AB BCE ∂ED ∂Σ ∂ED (5.154)
=
ABD
SBC +
AB
ED
SBCE = 0.
Multiplying (5.154) by CF and using (5.148) and symmetry properties of the elastic coefficients gives ABC (5.155) = − AD BE CF SDEF , ABC = − AD BE CF SDEF , where the second of (5.155) applies analogously for the isentropic coefficients. Analogous differentiation of (5.148) by the stress leads to S ABC = −S ADSBE SCF DEF , SABC = −SAD SBE SCF DEF . (5.156) Secondorder thermal expansion coefficients are defined as ∂E ∂ 2G0 ∂ 2G0 ∂E AB ( α ) = = − αT A = A = − , , (5.157) T AB ∂θ Σ ∂θ∂Σ AB ∂θ Σ ∂θ∂Σ A and secondorder thermal stress coefficients are defined as ∂ 2Ψ 0 ∂ 2Ψ 0 ∂Σ AB ∂Σ A βA =− , β AB = − . =− =− ∂θ E ∂θ∂E AB ∂θ E ∂θ∂E A
(5.158)
Thermal stress coefficients in (5.158) are identical to those introduced in (5.50). The T subscript on thermal expansion coefficients in (5.157) is used as a label and is not subject to the Einstein summation convention. Maxwell equations provide additional relationships among thermostatic coefficients. For example, using (5.143) and (5.157), ∂E A ∂E α θ ∂θ (5.159) = A = TA . ∂N 0 Σ ∂θ Σ ∂N 0 Σ CΣ Similarly, from (5.142) and (5.158), ∂Σ A ∂N 0
= E
∂Σ A ∂θ
∂θ ∂ N0 E
=− E
β Aθ CE
.
(5.160)
From the chain rule, thermal stress coefficients and thermal expansion coefficients are related by the following identity that incorporates isothermal secondorder elastic coefficients:
5.2 Thermostatic Relationships
βA =−
∂Σ A ∂θ
= E
∂N 0 ∂E A
= θ
∂N 0 ∂Σ B
θ
∂Σ B ∂E A
= θ
∂EB ∂θ
∂Σ B A Σ ∂E
= αT B
BA
225
. (5.161)
θ
Multiplying (5.159) by the secondorder isentropic elastic stiffness coefficients gives α θ ∂Σ B ∂E A ∂Σ A ∂θ − BA T A = = CΣ ∂E A N ∂N 0 Σ ∂EB N ∂Σ A N0 0 0 (5.162) B B ∂θ ∂Σ β θ . = = =− CE ∂EB N ∂N 0 E 0
Relation (5.162) can be written as C αT A AB = Σ β A = CR β A , (5.163) CE where the ratio of specific heats satisfies, from (5.161), CRα T A AB = α T A AB . (5.164) It can be shown (Thurston 1974) from Maxwell relations that the difference between specific heats at constant stress and constant strain is CΣ − CE = θβ Aα T A = θα T Aα T B
=
AB
θ
α T Aα T B
AB
. (5.165) CR Isentropic and isothermal secondorder elastic stiffnesses are related by ∂Σ A ∂Σ A ∂Σ A ∂θ θ A B AB β β . (5.166) = = + = AB + CE ∂EB N ∂EB θ ∂θ E ∂EB N 0
0
Similarly, for isentropic and isothermal secondorder elastic compliances, ∂E A ∂E A ∂E θ ∂θ SAB = αT αT . (5.167) = + A = S AB − B B B CΣ A B ∂Σ N0 ∂Σ θ ∂θ Σ ∂Σ N0
Thus, differences between isentropic and isothermal secondorder elastic coefficients result from the dyadic (tensor) product of thermal expansion or thermal stress coefficients. Such differences are often overlooked in practical applications at low to moderate temperatures, since differences between isentropic and isothermal constants can typically be of the same order of magnitude as uncertainties in experimental measurements of the elastic coefficients. Gruneisen numbers (i.e., Gruneisen’s tensor components) are dimensionless quantities written in full as 1 ∂θ 1 ∂θ ∂N 0 1 ∂Σ AB β AB = =− = Γ AB = − , (5.168) CE ∂θ E CE θ ∂E AB N θ ∂N 0 E ∂E AB θ 0
226
5 Thermoelasticity
or in reduced Voigt notation, using (5.161)(5.164), β A αT B BA αT B 1 ∂θ Γ A =− = = = CE CΣ θ ∂E A N C E
BA
.
(5.169)
0
It follows from Maxwell’s relations that Gruneisen parameters satisfy the following equalities: 1 ∂Σ A 1 ∂θ 1 ∂Σ A 1 ∂N 0 Γ A =− , (5.170) =− =− = θ ∂N 0 E θ ∂E A N CE ∂θ E CE ∂E A θ 0
and the ratio of specific heats at constant strain to constant stress can be expressed in terms of absolute temperature, thermal expansion coefficients, and Gruneisen numbers as C θ CR = Σ = 1 + αT αT AB CE CΣ A B (5.171) = 1 + θΓ Aα T A = 1 + θΓ AB (α T ) AB , where (5.165) and (5.169) have been used. The number of independent components of all tensorvalued material coefficients, defined specifically as derivatives with respect to thermodynamic potentials evaluated at some undistorted reference state (i.e., polar tensors in the terminology of Thurston (1974)), can be reduced as a result of material symmetries of the particular crystal class (i.e., the point group) to which the substance under consideration belongs, as discussed in Appendix A. Forms of symmetric secondrank polar tensors such as thermal stress constants, thermal expansion constants, and Gruneisen’s constants for all eleven Laue groups encompassing the 32 crystal classes are provided in Table A.5. Forms of secondorder elastic constants (which include isothermal and isentropic moduli and compliances) are listed in Table A.8. Forms of thirdorder elastic stiffness constants (which include isothermal and adiabatic moduli only) are listed in Table A.9. 5.2.2 Hydrostatic Stress States
In certain applications, the pressurevolume response of a material may be of great importance while deviatoric (i.e., shear) stresses may not be. Such situations occur in some fluids that cannot support significant shear stresses, for example. Furthermore, in many high pressure applications, the deviatoric stress response may be insignificant compared to the hydrostatic stress response. The Cauchy pressure p ( x, t ) , which will often be called the hydrostatic pressure or simply the pressure, is defined as
5.2 Thermostatic Relationships
227
1 1 p = − trσ = − σ .aa . (5.172) 3 3 The relationship between pressure and PiolaKirchhoff stresses is 1 1 p = − P aA FaA = − F.Ba Σ BA FaA . (5.173) 3J 3J Using kinematic identity (2.144) and constitutive relationship (5.42), for a hyperelastic material, holding the deviatoric part of F constant, ∂J −1 1 ∂E0 −1 1 ∂E0 p=− J FaA = − J FaA 3 ∂FaA 3 ∂J J −1/ 3F ∂FaA (5.174) ∂E0 1 ∂E0 1 ∂E0 A −1 Aa −1 =− JF J FaA = − δ. A = − . ∂J J −1/ 3F 3 ∂J J −1/ 3F 3 ∂J J −1/ 3F Similarly from (5.23), in terms of Helmholtz free energy per unit reference volume, the pressure satisfies ∂Ψ 0 p=− . (5.175) ∂J J −1/ 3F Relations (5.172)(5.175) hold regardless of dimensionality of the stress state. In the remainder of Section 5.2.2, the focus is on hydrostatic stress states for which the Cauchy stress tensor satisfies, by definition, 1 σ ab = − pg ab , σ ′ab = σ ab − σ .cc g ab = σ ab + pg ab = 0 , (5.176) 3 where σ′ is the deviatoric part of the Cauchy stress. PiolaKirchhoff stresses are generally not spherical under conditions (5.176): P aA = − JpF −1.Ab g ab , Σ AB = − JpF −1.Aa g ab F −1.Bb = − JpC −1 AB . (5.177) Using (5.176), the stress power per unit reference volume becomes J σ ab Dab = − JpLa.a = − pJv;aa = − pJ . (5.178) In general anisotropic materials, no particular strain components E AB need vanish when the Cauchy stress state is hydrostatic; only in elastic materials with isotropic or cubic symmetry does a spherical deformation gradient F. Aa = J 1/ 3 g.aA with C AB = J 2 / 3G AB always result in a hydrostatic state of stress. For example, for an isotropic, nonlinear hyperelastic material, (5.117) results in σ ab = J −1/ 3 g.aAΣ AB g.bB = (α 0 J −1/ 3 + α1 J 1/ 3 + α 2 J ) g ab when the deformation gradient is spherical. Thermostatic potentials of Section 5.2.1 are redefined for spherical stress states with − p replacing Σ and J replacing E. In this context, all independent and dependent state variables in the thermostatic framework are scalars, and (5.131)(5.133) are replaced with
228
5 Thermoelasticity
E0 = E0 ( J , N 0 ) , H 0 = H 0 ( p, N 0 ) ,
(5.179)
Ψ 0 =Ψ 0 ( J ,θ ) , G0 = G0 ( p,θ ) ,
(5.180)
(5.181) N 0 = N 0 ( J , E0 ) . The relationships in Table 4.2 are redefined as H 0 = E0 + pJ , Ψ 0 = E0 − θ N 0 , G0 = H 0 − θ N 0 , (5.182) where in general, enthalpies in (5.134) and (5.182) do not coincide since pJ ≠ −Σ AB E AB . Differentials of the potentials are dE0 = − pdJ + θ dN 0 , dH 0 = Jdp + θ dN 0 , (5.183) dΨ 0 = − pdJ − N 0 dθ , dG0 = Jdp − N 0 dθ . (5.184) First derivatives then provide the following thermostatic relationships: ∂E ∂H 0 ∂Ψ 0 ∂G , (5.185) N0 = − =− 0 , θ = 0 = ∂N 0 J ∂N 0 p ∂θ J ∂θ p p=−
∂E0 ∂J
=− N0
1
θ
=
∂H 0 ∂Ψ 0 , J= ∂p ∂J θ
∂N 0 ∂N , p =θ 0 ∂E0 J ∂J
= N0
∂G0 . ∂p θ
(5.186)
.
(5.187)
E0
Isothermal (B) and isentropic ( B ) bulk moduli are defined as follows: B = −J
∂ 2Ψ 0 ∂p ∂p =J , B = −J 2 ∂ J ∂J θ ∂J θ
=J N0
∂ 2 E0 ∂J 2
,
(5.188)
N0
Isothermal and isentropic compressibilities are defined, respectively, as 1 1 ∂J 1 1 ∂J χ = =− , χ = =− . (5.189) B J ∂p N0 B J ∂p θ Recalling from the conservation of mass (4.10) that ρ 0 = ρ J , partial derivatives with respect to Jacobian determinant J can be expressed as ∂ (.) ∂ (.) ∂ρ ∂ (.) ∂J −1 ∂ (.) ∂ (.) . (5.190) J =J = ρ0 J = − ρ 0 J −1 = −ρ ∂J ∂ρ ∂J ∂ρ ∂J ∂ρ ∂ρ Defining specific volume as υ = ρ −1 = J ρ 0−1 , derivatives can also be written ∂ (.) 1 ∂ (.) ∂υ 1 ∂ (.) ∂ρ −1 1 −2 ∂(.) ∂ (.) J . (5.191) =− =− = ρ =υ υ ∂υ ∂ρ υ ∂υ ∂ρ υ ∂J ∂υ ∂υ The absolute spatial volume v can be substituted for the specific volume:
5.2 Thermostatic Relationships
229
∂ (.) dv ∂ (.) v ∂ (.) ∂ (.) = = =v . (5.192) ∂J dV ∂ (dv / dV ) V ∂v / V ∂v Thus isothermal and isentropic bulk moduli in (5.188) can be written ∂p ∂p ∂p ∂p ∂p ∂p . (5.193) B=ρ = −υ = −v , B=ρ = −υ = −v ∂ρ θ ∂υ θ ∂v θ ∂ρ N0 ∂υ N0 ∂v N0 J
A volumetric expansion coefficient at constant pressure, i.e., an isotropic coefficient of thermal expansion, is defined as 1 ∂J 1 ∂ 2G0 A= = . (5.194) J ∂θ p J ∂θ∂p It follows from mass conservation that 1 ∂J ∂ρ −1 1 ∂ρ A= =ρ =− J ∂θ p ∂θ p ρ ∂θ
=− p
∂ ln ρ . ∂θ p
(5.195)
From (5.193) and (5.195) and noting that p = p[ ρ ( p,θ ),θ ] , 0=
∂p ∂θ
= p
∂p ∂θ
+ ρ
∂p ∂ρ ∂ρ θ ∂θ
= p
∂p ∂θ
− AB ⇒ ρ
∂p ∂θ
= AB = ρ
∂p . (5.196) ∂θ J
Definitions at a reference state of null strain and zero stress are instructive and useful for formulating constitutive models in terms of measured thermoelastic properties. In this state, the deformation gradient, strain, and Jacobian determinant are F. Aa = g.aA , C AB = GAB , E AB = 0 , J = 1 , (5.197) and the stress state is, by definition, Σ AB = 0 , P aB = 0 , σ ab = 0 , p = 0 . (5.198) Let the temperature at the reference state be θ0 , which can be of arbitrary positive value. From the second of (5.177), ∂Σ AB = − JC −1 AB p =0 = −G AB . (5.199) ∂p p = 0 θ =θ 0 θ =θ0
Also from (2.160), in the reference state ∂J ∂J =2 = JC −1 AB p =0 = G AB . ∂E AB p = 0 ∂C AB p = 0 θ =θ 0 θ =θ 0
(5.200)
θ =θ 0
Tensors of thermal expansion coefficients (5.157) and thermal stress coefficients (5.158) evaluated at the reference state are then ∂E ∂E ∂Σ AB ∂Σ AB (αT 0 ) AB = AB , β 0AB = − . (5.201) = AB =− ∂θ Σ = 0 ∂θ p = 0 ∂θ E =0 ∂θ J =1 θ =θ 0
θ =θ 0
θ =θ0
θ =θ0
230
5 Thermoelasticity
From (5.194) and (5.200), the scalar expansion coefficient at null pressure and reference temperature is the trace of the corresponding tensor coefficient of thermal expansion: ⎛ 1 ∂J ⎛ 1 ∂J ⎞ ∂E AB ⎞ ⎟ A0 = ⎜ =⎜ = G ABαT 0 AB = αT 0.AA . (5.202) ⎜ J ∂θ p ⎟⎟ ⎜ ⎟ θ J E ∂ ∂ Σ ⎠ p =0 AB p ⎝ ⎠ θp==θ0 ⎝ θ =θ 0 0
For the isothermal compressibility of the first of (5.189) at the reference state, from (5.199) and (5.200), ⎛ 1 ∂J ⎞ ⎛ 1 ∂J ∂E AB ∂Σ CD ⎞ 1 χ0 = = −⎜ = −⎜ ⎟ ⎟ CD ⎜ J ∂p ⎟ B0 ∂p ⎠ p = 0 ⎝ J ∂E AB ∂Σ θ ⎠ p=0 ⎝ θ =θ0 θ =θ 0 (5.203) = G AB ⎛⎜ S ABCD p = 0 ⎞⎟ G CD = G AB G CD SABCD . θ =θ 0 ⎠ ⎝ An analogous relationship applies for the isentropic compressibility and isentropic elastic compliance coefficients: ⎛ 1 ∂J ⎞ 1 ⎟ (5.204) = −⎜ = G AB G CD SABCD p = 0 . χ0 = ⎜ J ∂p N ⎟ θ =θ0 B0 0 ⎠ p =0 ⎝ θ =θ 0
Relations (5.202)(5.204) apply regardless of material symmetry. For an isotropic materially linear thermoelastic solid, in the context of (5.127) and holding shear strains fixed, the isothermal bulk modulus satisfies ⎛ ∂p ⎞ K⎡ ∂ ⎤ B0 = − ⎜ J C.AA E.BB ) ⎥ = ⎢J ( ⎟ J J 3 ∂ ∂ ⎣ ⎦ p =0 θ ⎠ p =0 ⎝ θ =θ 0
θ =θ 0
⎡ ∂ A B A B ⎤ ⎢ J ∂J ( C. AC. B − C. Aδ . B ) ⎥ p =0 ⎣ ⎦ θ =θ
=
K 6
=
∂C ⎤ K⎡ K ∂ (3J ) B = ⎢ J ( 2C. B − 3) ⎥ ∂J ⎦ p = 0 ∂J 6⎣ 2 p =0 θ =θ θ =θ
(5.205)
0
A .A
2/3
0
=KJ
−1/ 3
p =0
θ =θ 0
0
= K.
Thus, from (5.127) and (5.205), isothermal thermoelastic coupling coefficients are related in isotropic solids by the relationships (α T 0 ).AB = (α T )δ . BA , A0 = 3α T = β / K , and K = B0 = 1/ χ 0 . Similar relationships hold for crystals with cubic symmetry, but not for general anisotropic bodies.
5.2 Thermostatic Relationships
231
Definitions of specific heats per unit reference volume at constant volume Cv and constant pressure C p , i.e., isochoric and isobaric specific heats, are, respectively, Cv = Cp =
∂E0 ∂θ ∂H 0 ∂θ
=θ J
∂N 0 ∂θ
=θ p
∂N 0 ∂θ
= −θ
∂ 2Ψ 0 , ∂θ 2 J
(5.206)
= −θ
∂ 2G0 . ∂θ 2 p
(5.207)
J
p
At the reference state, since both pressure and stress vanish by (5.198), ∂H 0 ∂H 0 C p0 = = = CΣ 0 . (5.208) ∂θ p =0 ∂θ Σ =0 θ =θ 0
θ =θ 0
Noting that ∂N 0 ∂θ
= p
∂N 0 ∂θ
+ J
∂N 0 ∂J
θ
∂J , ∂θ p
(5.209)
specific heats at constant pressure and constant volume are related at any equilibrium state by ∂N 0 ∂N 0 ∂J ∂N Cp = θ +θ = Cv + θ JA 0 ∂θ J ∂J θ ∂θ p ∂J θ = Cv + θ JA = Cv + ABθ
∂N 0 ∂p
θ
∂p ∂J θ
= Cv − θ AB
∂ 2 G0 ∂J = Cv + ABθ ∂p∂θ ∂θ
∂N 0 ∂p
(5.210) θ
= Cv + JA2 Bθ . p
From (5.165) and (5.210), C p − CΣ − Cv + CE = θ ( JA2 B − αT ABαT CD
ABCD
).
(5.211)
At the reference state, from (5.208), this reduces to CE 0 − Cv 0 = θ ( A02 B0 − α T 0 ABα T 0CD ABCD ) . (5.212) Thurston (1974) noted that the difference in (5.212) vanishes identically in isotropic materials and crystals of cubic symmetry, but that CE 0 ≠ Cv 0 in general for materials of greater anisotropy. As explained by Thurston (1974), thermostatic potentials can be redefined at an alternative state of nonzero constant hydrostatic pressure, and relationships among their derivatives can be calculated at this alternative reference state. Choice of zero pressure for the reference state is not necessary, but is convenient if one assigns for the physical environment (e.g., laboratory) a datum of zero gauge pressure.
232
5 Thermoelasticity
The following relationships can be derived from the thermostatic potentials: ∂J J θ A ∂p θ AB = , = . (5.213) Cv ∂N 0 p C p ∂N 0 J Noting that p = p[ J ,θ ( J , N 0 )] , ∂p ∂J
= N0
∂p ∂p + ∂J θ ∂θ
J
∂θ ∂J
.
(5.214)
N0
Dividing both sides of (5.214) by isothermal bulk modulus B and using (5.196), isentropic and isothermal bulk moduli are related by ⎛ −∂p ⎞ ∂J ∂p ∂θ B JA2 Bθ ⎛ −J ⎞ . (5.215) =1+ =1+ ⎜ = + 1 AB ⎜ ⎟ ( ) ⎟ ⎜ ∂N 0 ⎟ ∂p θ ∂θ J ∂J N0 B Cv ⎝ B ⎠ J ⎠ ⎝ Comparing (5.210) and (5.215), (5.216) B / B = C p / Cv . The Gruneisen parameter (scalar) is defined as J ∂θ ∂ ln θ Γ =− =− . θ ∂J N0 ∂ ln J N0
(5.217)
It follows from (5.216) and the thermostatic potentials that the Gruneisen “gamma” satisfies the following identities: J ∂N 0 J ∂p ∂p JAB JAB Γ = = =J = = . (5.218) Cv ∂J θ Cv ∂θ J ∂E0 J Cv Cp Furthermore from (5.189), (5.210), and (5.216), B Cp χ = = = 1 + AΓθ . B Cv χ
(5.219)
From (5.168) and (5.217), threedimensional Gruneisen numbers are related to scalar Gruneisen parameter by ∂E J ∂N 0 ∂E AB J ∂N 0 = θ Γ = Γ AB AB Cv ∂E AB θ ∂J θ Cv ∂θ E ∂J θ (5.220) JCE AB ∂E AB = . Γ Cv ∂J θ Under a hydrostatic stress state, the following identity holds: ∂E AB ∂E AB ∂Σ CD ∂p B ∂Σ CD = = − , (5.221) S ABCD J ∂J θ ∂Σ CD θ ∂p θ ∂J θ ∂p θ which, when substituted into (5.220), leads to the relationship
5.2 Thermostatic Relationships
Γ =−
BCE Γ Cv
AB
S ABCD
∂Σ CD , ∂p θ
233
(5.222)
and at the stressfree undeformed reference state, from (5.199), BC Γ 0 = 0 E 0 Γ 0AB SABCD G CD . (5.223) Cv 0 Recall from discussion following (5.212) that CE 0 = Cv 0 for isotropic solids and for crystals with cubic symmetry, in which case (5.223) yields Γ 0AB = Γ 0G AB and 3Γ 0 = Γ 0.AA . A number of theoretical models for the Gruneisen parameter have been developed using macroscopic arguments or atomic treatments of lattice vibrations. According to Einstein’s model (Einstein 1907; Born and Huang 1954), when the internal energy of (5.77) is extended to include effects of volume change, ξ ⎞ ⎛ξ (5.224) E0 ( J ,θ ) = U S ( J ) + UV ( J ,θ ) = U S ( J ) + 3nk Bθ ⎜ + ξ ⎟, −1⎠ 2 e ⎝ where ξ ( J ,θ ) = ΘE ( J ) / θ , ΘE = hν E ( J ) / k B . (5.225) Einstein’s temperature Θ E and characteristic frequency ν E are not constant as was the case in (5.78), but are instead here assumed to depend on volume via J, but not on absolute temperature θ. Static internal energy per unit reference volume is written U S , and UV is the vibrational energy. The free energy per unit reference volume corresponding to (5.224) is ⎡ξ ⎤ Ψ 0 = E0 − N 0θ = U S ( J ) + 3nk Bθ ⎢ + ln (1 − e−ξ ) ⎥ . (5.226) ⎣2 ⎦ Similarly, for Debye’s model (Debye 1912), the total internal energy can be expressed as (Born and Huang 1954) E0 ( J ,θ ) = U S ( J ) + UV ( J ,θ ) ⎡⎛ θ ⎞ 3 Θ D / θ ⎛ 1 (5.227) 1 ⎞ 3 ⎤ = U S ( J ) + 9nk Bθ ⎢⎜ ⎟ ∫ ⎜ + ξ ⎟ ξ dξ ⎥ , ⎢⎣⎝ Θ D ⎠ 0 ⎝ 2 e − 1 ⎠ ⎥⎦ with the corresponding definitions ξ ( J ,θ ) = Θ D ( J ) / θ , ΘD ( J ) = hν D ( J ) / k B . (5.228) The free energy per unit reference volume in Debye’s theory is (Born and Huang 1954)
234
5 Thermoelasticity
Ψ 0 = E0 − N 0θ ⎧⎪⎛ θ ⎞ ΘD / θ ⎡ 1 ⎫⎪ (5.229) −ξ ⎤ 2 = U S ( J ) + 9nk Bθ ⎨⎜ ⎟ ∫ ⎢ ξ + ln (1 − e ) ⎥ ξ d ξ ⎬ . ⎦ ⎪⎩⎝ ΘD ⎠ 0 ⎣ 2 ⎪⎭ Writing Θ to describe either the Einstein temperature or the Debye temperature, it can be shown (Born and Huang 1954) ∂ξ ∂ξ v d Θ ∂ξ d ln Θ ∂ξ ∂ξ J =v = = = −Γ , (5.230) ∂J θ ∂v θ Θ dv ∂ ln Θ θ d ln v ∂ ln Θ θ ∂ ln Θ θ so that for Einstein’s model, d ln Θ Ε d ln Θ Ε J d ΘΕ J dν E v dν E ΓE = − =− =− =− =− , (5.231) d ln v ΘΕ dJ d ln J ν E dJ ν E dv and for Debye’s model, d ln Θ D d ln ΘD J d ΘD J dν D v dν D =− =− =− =− . (5.232) ΓD = − Θ D dJ ν D dJ ν D dv d ln v d ln J Using (5.224) or (5.227), ∂Ψ 0 dU S −J +J = Γ UV , (5.233) ∂J θ dJ from which dividing by J and using (5.186) gives a functional form for the equation of state of Mie and Gruneisen (1926): dU S p ( J ,θ ) = − + Γ J −1UV . (5.234) dJ Consider now the pressure derivative of the isothermal bulk modulus B at constant temperature: J ∂B J ∂ ⎛ ∂p ⎞ J ⎛ −B ∂B ∂J ∂B ∂2 p ⎞ = =− = +J 2 ⎟ ⎜J ⎟ = ⎜⎜ B ∂J θ B ∂J ⎝ ∂J ⎠ θ B ⎝ J ∂p θ ∂p θ ∂J θ ∂J θ ⎟⎠ (5.235) J (∂ 2 p / ∂J 2 ) v (∂ 2 p / ∂v 2 ) J 2 ∂2 p θ θ . = −1 + = −1 − = −1 − (∂ p / ∂ J ) θ (∂ p / ∂v ) θ B ∂J 2 θ One may also write ∂B J ∂B ∂ ln B v ∂B ∂ ln B . =− =− =− =− ∂p θ B ∂J θ ∂ ln J θ B ∂v θ ∂ ln v θ
(5.236)
The relationship between Gruneisen’s coefficient and the isothermal pressure derivatives in (5.235) and (5.236) is often expressed as 2 2 v (∂ p / ∂v ) θ 1 ∂B 1 (5.237) = + − CΓ , Γ = −CΓ − 2 (∂p / ∂v) θ 2 ∂p θ 2
5.3 Finite Elastic Volume Changes
235
where CΓ is a constant. Slater (1939) suggested CΓ = 2 / 3 following a Debyetype analysis in which Poisson’s ratio is assumed independent of volume. Dugdale and MacDonald (1953) suggested CΓ = 1 for isothermal conditions based on analysis of plane wave velocities in a monatomic lattice, leading to vanishing of Γ when interatomic forces are harmonic. Value CΓ = 7 / 6 has also been widely suggested (Slater 1940; Eshelby 1954). Notice that the reference Gruneisen parameter Γ 0 can be determined from (5.237) when the pressure derivative of the isothermal bulk modulus is evaluated at the reference state. A number of other functional forms of Gruneisen’s parameter have been suggested. Segletes and Walters (1998) developed a powerlaw model for Gruneisen’s parameter that encompasses several historical models (Slater 1940; Dugdale and MacDonald 1953). Murnaghan (1944) developed a simple model in which the bulk modulus varies linearly with pressure. Birch (1978) developed a popular nonlinear equation of state for crystalline solids undergoing potentially large volume changes. Vinet et al. (1989) developed a universal form for equations of state of covalent and metallic solids. Zhou (2005) postulated a free energy function similar to (5.229) by additively decomposing atomic velocities into high frequency terms associated with thermal oscillations and low frequency terms associated with bulk structural motion.
5.3 Finite Elastic Volume Changes Consider applications wherein large elastic volume changes are of interest, but large elastic deviatoric deformations are not. In many ductile crystalline solids such as engineering metals, large deviatoric deformations are sustained by dislocation glide which is assumed to be latticepreserving (i.e., inelastic), as explained in Sections 3.2.2 and 3.2.5. In more brittle solids such as many ceramic crystals at low to moderate temperatures, driving forces necessary for dislocation motion exceed those for fracture, and large deviatoric deformations are sustained by damage mechanisms (e.g., microcracking) when mechanical stresses exceed some threshold. Inelastic tensile volumetric deformations are accommodated by damage mechanisms such as voids in ductile materials and mode I cracks in brittle materials. On the other hand, large compressive volumetric deformations are accommodated in fully dense (i.e., nonporous) crystalline solids by elastic contraction of the lattice. Tensile damage mechanisms of void growth and mode I fracture are impeded by large compressive pressures.
236
5 Thermoelasticity
Such confining pressures are attained in shock physics experiments, for example, under dynamic impact situations (Graham and Brooks 1971; Graham 1992; Vogler and Clayton 2008), as well as in more general scenarios of ballistic impact or high pressure/blast loading, or geological activity involving significant confinement. The model framework that follows is appropriate for thermoelastic behavior of isotropic solids (e.g., polycrystals with random grain orientations) undergoing large volume changes but small shape changes. The framework is a reduction of the more general one of Section 5.1.3, but is based on a series expansion of the internal energy rather than the free energy. Specifically, internal energy per unit reference volume is written E0 ( E,θ , X ) = ES ( E′, X ) + EV (ζ ( J ),θ , X ) , (5.238) where the deviatoric right CauchyGreen strain and measure of volumetric deformation are, respectively, 1 ρ ′ = E AB − E.CC G AB , ζ = E AB − 1 = J −1 − 1 . (5.239) 3 ρ0 Kinematic variable ζ ( X , t ) contains the same information as J so that volume changes are measured exactly to the extent permitted by the deformation gradient itself. From the second of (5.239), ζ = 0 at the reference state with J = 1 , ζ > 0 when the material is spherically compressed, and ζ < 0 when the material is spherically expanded. The deviatoric energy is usually taken as a quadratic function of E′ , while the term EV is generally a nonlinear function of ζ and θ , accounting for the equation of state of the material, a generally nonlinear pressurevolumetemperature relationship. Using (5.238) in (5.42), the second PiolaKirchhoff stress satisfies, from (2.160), ′ ∂E0 ∂ES ∂ECD ∂E ∂ζ ∂J = + V Σ AB = ′ ∂E AB ∂ECD ∂E AB ∂ζ ∂J ∂E AB (5.240) ∂ES ⎛ A B 1 AB ⎞ 1 ∂EV −1 AB = − − δ δ G G C . CD ⎟ ′ ⎝⎜ .C . D 3 ∂ECD ⎠ J ∂ζ Cauchy stress and Cauchy pressure are computed, respectively, as 1 ∂ES ⎛ a b 1 a b AB ⎞ 1 ∂E σ ab = F.C F. D − F. A F. B G GCD ⎟ − 2 V g ab , (5.241) ⎜ ′ ⎝ 3 J ∂ECD ⎠ J ∂ζ 1 ∂ES ⎛ 1 ⎞ 1 ∂EV . (5.242) C − C AG + ′ ⎝⎜ CD 3 . A CD ⎠⎟ J 2 ∂ζ 3 J ∂ECD For illustrative purposes, let the internal energy (5.238) be written at material point X as p=−
5.3 Finite Elastic Volume Changes
237
1 1 ′ + ⎛⎜ B0ζ 2 + B1ζ 3 + ... ⎞⎟ + A0 B0ζ∆θ + C ∆θ . (5.243) E0 = µ E ′ AB E AB 3 ⎝2 ⎠ The first term on the right of (5.243) accounts for the deviatoric response, with µ a constant shear modulus. Terms in parentheses account for the nonlinear pressurevolume response at constant temperature, with B0 and B1 material constants. The next term accounts for thermoelastic coupling, with A0 a constant. The final term accounts for the purely thermal energy, with C a constant specific heat per unit reference volume and ∆θ = θ − θ 0 , with θ0 a reference temperature at which this thermal energy vanishes. Material constants satisfy ∂ 2 EV 1 ∂ 2 ES 1 ∂ 3 EV µ= B = B = , , , (5.244) 0 1 ′ E=0 ∂ζ 2 E = 0 2 ∂E ′ AB ∂E AB 2 ∂ζ 3 E=0 θ =θ0
1 ∂ 2 E0 A0 = B0 ∂θ∂ζ
θ =θ0
E= 0 θ =θ 0
∂E , C= 0 ∂θ
θ =θ0
E=0 θ =θ 0
.
(5.245)
From (5.240)(5.242), stress components and Cauchy pressure are 1 (5.246) Σ AB = 2µ E ′ AB − C −1 AB ⎡⎣( B0ζ + B1ζ 2 + ...) + A0 B0 ∆θ ⎤⎦ , J 2 1 σ ab = µ E ′ AB F. Aa F. Bb − 2 ⎡⎣( B0ζ + B1ζ 2 + ...) + A0 B0 ∆θ ⎤⎦ g ab , (5.247) J J 2 1 p = − µ E ′ AB C AB + 2 ⎡⎣( B0ζ + B1ζ 2 + ...) + A0 B0 ∆θ ⎤⎦ . (5.248) 3J J Consider the volume derivative of the pressure at the reference state when the contribution from the first term on the right side of (5.248) vanishes (e.g., null shear stress): ⎛ 1 ∂p ⎞ ⎛ ∂p ⎞ ⎡1 ⎤ −⎜ J =⎜ = ⎢ ( B0 + 2 B1ζ + ...) ⎥ = B0 . (5.249) ⎟ ⎟ ⎝ ∂J ⎠ E = 0 ⎝ J ∂ζ ⎠ E= 0 ⎣ J ⎦ ζ =0 θ =θ 0
θ =θ 0
θ =θ 0
Thus B0 is equivalent to isothermal bulk modulus at the reference state in the context of hydrostatic stress conditions, as introduced in (5.203). Now consider the relationship ∂p ⎡⎛ 1 ∂J ⎞⎛ ∂p ⎞ ⎤ = ⎜ = ( AB) E = 0 = A0 B0 , (5.250) ⎟⎜ − J ⎟ θ =θ 0 ∂θ E = 0 ⎢⎣⎝ J ∂θ ⎠⎝ ∂J ⎠ ⎥⎦ E = 0 θ =θ 0
θ =θ 0
implying that A0 is equivalent to the spherical thermal expansion coefficient of (5.202) at the reference state for hydrostatic stress conditions:
238
5 Thermoelasticity
⎛ 1 ∂J ⎞ . A0 = ⎜ ⎟ ⎝ J ∂θ ⎠ θE==θ0
(5.251)
0
For isotropic solids, the right side of (5.212) vanishes (Thurston 1974). Thus the specific heat at constant volume or constant strain at the reference state satisfies CE 0 = Cv 0 = C , and the product A0 B0 ∆θ = J −1Γ C ∆θ = J −1Γ U 0 ,
(5.252)
where Γ = JA0 B0C is Gruneisen’s parameter of (5.218), and U 0 = C ∆θ is the thermal energy in (5.243). For negligible shape changes, note that C AB ≈ J 2 / 3GAB and the first term on the right of (5.248) vanishes, leaving the following equation of state for the hydrostatic pressure: 1 (5.253) p ( J ,θ ) = 2 ⎡⎣( B0ζ + B1ζ 2 + ...) + Γ J −1U 0 ⎤⎦ , J which is similar in appearance to the MieGruneisen form given in (5.234). −1
5.4 Geometrically Linear Elasticity In geometrically linear elasticity theory, the distinction between reference and current configurations is not made explicit, and the displacement gradient (i.e., distortion) of (3.76) is used as the fundamental kinematic descriptor as opposed to the deformation gradient. In the geometrically linear theory, the analog of (5.1) is ua ;b = β abL , (5.254) with u ( x, t ) the displacement and β L ( x, t ) the lattice distortion. Strains and rotations are, respectively, the symmetric and skew parts of (5.254): u( a;b ) = ε ab = β (Lab ) = ε abL , (5.255) u[a ;b] = u[a ,b] = β[Lab] = Ω abL = Ω ab = −ε abc wc , with w ( x, t ) the rotation vector of (2.166). 5.4.1 Constitutive Assumptions Applying (5.254), and prior to consideration of objectivity requirements, appropriate versions of functional dependencies of dependent state variables (4.45)(4.48) for a hyperelastic material of grade one are ψ = ψ ( ua ;b ,θ ,θ , a , x , g a ) , (5.256)
5.4 Geometrically Linear Elasticity
η = η ( u a ;b , θ , θ , a , x , g a ) ,
σ ab = σ ab ( ua ;b ,θ ,θ,a , x, g a ) , q a = q a ( u a ;b , θ , θ , a , x , g a ) .
239
(5.257) (5.258) (5.259)
Independent variables are displacement gradient, temperature, temperature gradient, position or choice of material particle at x, and basis vectors. The dependence on displacement gradient replaces that of the deformation gradient in Section 5.1.1. Dependence of response functions other than heat flux q on temperature gradient is written out in (5.256)(5.259) for completeness, but will be eliminated following thermodynamic considerations in Section 5.4.2. Dependence of response functions on position x (analogous to dependence on X in the nonlinear case) is included to permit description of a heterogeneous body. Dependence on basis vectors g a ( x) enables description of solids exhibiting an anisotropic response, as explained in Section 5.4.5. ˆ )x + c , where Under superposed small rigid body motions, x → (1 + Ω ˆ (t ) = −Ω ˆ T is a skew rotation matrix and c(t ) is a spatially constant Ω translation vector, to first order the displacement gradient and its skew and symmetric parts transform as ua ;b → ua ;b + Ωˆ ab , u[ a ,b] → u[ a ,b] + Ωˆ ab , ε ab = u( a ;b ) → u( a ;b ) . (5.260) Thus, the skew part of the displacement gradient (2.254) should not enter the list of independent variables since the response (e.g., thermodynamic potentials) should not be affected by rigid body motions of the frame of observation. The temperature gradient transforms under small rigid body rotations as θ, a → (δ.ba + Ωˆ .ba )θ,b = θ,a + Ωˆ .baθ,b ≈ θ, a , (5.261) so that dependence of response functions on θ,a is not considered a violation of objectivity, in contrast to the nonlinear theory of Section 5.1.1. Similarly to (5.261), heat flux q and stress σ remain approximately unchanged when rigid rotations are small. Thus, appropriate analogs of (5.15)(5.18) in the geometrically linear regime are ψ = ψ (ε ab ,θ ,θ , a , x, g a ) , (5.262)
η = η (ε ab ,θ ,θ ,a , x, g a ) ,
σ
ab
=σ
ab
(ε
ab
, θ , θ , a , x, g a ) ,
q a = q a (ε ab ,θ ,θ, a , x, g a ) .
(5.263) (5.264) (5.265)
240
5 Thermoelasticity
5.4.2 Thermodynamics Using kinematic assumption (5.254) and constitutive assumptions (5.262)(5.265), dissipation inequality (4.73) becomes ⎛ ab ∂ψ ⎞ ∂ψ ⎞ ∂ψ ⎛ γ a − θ −1q aθ ,a ≥ 0 . (5.266) ⎜σ − ρ ⎟ ε ab − ρ ⎜η + ⎟θ − ρ ∂ ∂ ∂ ε θ θ ⎝ ⎠ ,a ab ⎠ ⎝ To ensure thermodynamic admissibility, coefficients of ε , θ , and γ must vanish identically in (5.266). This leads to the constitutive relationships ∂ψ ∂ψ ∂ψ σ ab = ρ , η =− , = 0. (5.267) ∂ε ab ∂θ ∂θ ,a It follows that free energy, entropy, and stress do not depend explicitly on the spatial temperature gradient: ψ = ψ ( ε,θ , x, g a ) , η = η ( ε,θ , x, g a ) , σ = σ ( ε,θ , x, g a ) . (5.268) The entropy production inequality reduces to the conduction inequality in (4.60): (5.269) θΓ = θΓ C = −θ −1θ ,a q a ≥ 0 . The rate of local entropy production vanishes: θΓ L = ρθη + q;aa − ρ r = σ abε ab − ρψ − ρθη = 0 . (5.270) Treating the entropy as an independent variable and temperature as a dependent variable, with the internal energy e used as the primary thermodynamic potential gives e = e ( ε,η , x, g a ) , θ = θ ( ε,η , x, g a ) , σ = σ ( ε,η , x, g a ) , (5.271) where the partial Legendre transform e = θ ( ε,η , x, g a )η + ψ ( ε,θ , x, g a ) . (5.272) From the second of (5.267) and the chain rule, ⎛ ∂ψ ∂ψ ∂θ ∂e ∂θ ⎞ ∂ψ ρ η⎟= ρ = ρ⎜ + + = σ ab . (5.273) ε θ ε ε ε ∂ε ab ∂ ∂ ∂ ∂ ∂ ab ab ab ⎝ ab ⎠ When temperature and temperature gradients are held fixed or are omitted from the description, the body is said to be elastic as opposed to thermoelastic. In such a description, let θ = constant such that θ = 0 and θ ,a = 0 , and let heat flux q and heat sources r vanish. The conduction inequality (5.269) is identically zero, and the rate of entropy production becomes θΓ = ρθη = 0 . (5.274)
5.4 Geometrically Linear Elasticity
241
Since temperature and entropy are treated constants, there is no need to include them explicitly in the description. Expressions (5.268) for free energy and stress become (5.275) ψ = ψ ( ε , x , g a ) , σ = σ ( ε , x, g a ) , and the constitutive equations are given by (5.273). Temperatureindependent thermodynamic potential ψ = ψ (ε, x, g a ) is then referred to as the strain energy density. The specific heat capacity per unit mass at constant strain ε is ∂e ∂e ∂η ∂e ∂ ⎛ ∂ψ ⎞ ∂ 2ψ . (5.276) c= = =− = − θ ⎜ ⎟ ∂θ ∂η ∂θ ∂η ∂θ ⎝ ∂θ ⎠ ∂θ 2 Fourier’s Law of conduction, as introduced in (4.62), leads to nonnegative dissipation: (5.277) q a = −k abθ,b , −θ, a q a = θ, a k abθ,b ≥ 0 . From (5.270) and (5.277), the local energy balance can be expressed as d ⎛ ∂ψ ⎞ ab (5.278) − ρθ ⎜ ⎟ = ( k θ ,b ) ;a + ρ r . dt ⎝ ∂θ ⎠ Note that, by the chain rule, d ⎛ ∂ψ ⎞ ∂ ⎛ ∂ψ ∂ψ ⎞ ε ab + θ ⎟ = θβ abε ab + ρ cθ , (5.279) − ρθ ⎜ ⎜ ⎟ = − ρθ dt ⎝ ∂θ ⎠ ∂θ ⎝ ∂ε ab ∂θ ⎠ where β ab = − ρ∂ 2ψ / ∂θ∂ε ab accounts for thermoelastic coupling. Equating (5.278) and (5.279) results in (5.280) ρ cθ = ( k abθ,b ) ;a − θβ abε ab + ρ r . In the absence of heat sources, in a homogeneous isotropic rigid conductor with k ab = kg ab , (5.280) becomes the transient heat equation k g k k −1 θ = ∇ 2θ = ( g abθ, a ) ;b = (5.281) g g g abθ , a ,b . ρc ρc ρc
(
)
5.4.3 Materially Nonlinear Hyperelasticity Differentiation of (5.267) with respect to strain results in the following definition of secondorder elastic stiffness coefficients: ∂σ ab ∂ 2ψ abcd (ε,θ , x, g a ) = =ρ . (5.282) ∂ε cd ∂ε ab ∂ε cd From (2.162), finite Lagrangian strain E and linear strain ε are related by 1 E AB = u( a ;b ) (δ .aA + u.,aA )(δ .bB + u.,bB ) − u;ca uc ;b (δ .aA + u.,aA )(δ .bB + u.,bB ) . (5.283) 2
242
5 Thermoelasticity
It follows that
⎡⎛ ∂E AB 1 ⎞ ∂ = δ .(( dAδ .eB)) + ⎢⎜ u( a ;b ) − u;ca uc ;b ⎟ (δ.aAu.,bB + δ.bB u.,aA + u.,aAu.,bB ) 2 ∂u( d ;e ) ⎠ ∂u( d ;e ) ⎢⎣⎝
(5.284) c ⎤ ∂uc ;b c ⎞ a 1 ⎛ ∂u;a a b b − ⎜ u c ;b + u;a ⎟ ( δ. A + u., A )( δ. B + u., B ) ⎥ . 2 ⎜⎝ ∂u( d ;e ) ∂u( d ;e ) ⎟⎠ ⎥⎦ Thus, tangent moduli in (5.54) and (5.282) are related, at the same temperature and material point, by ∂ ⎛ ∂ψ ⎞ ∂ ⎛ ∂ψ ⎞ ∂ECD ∂E AB abcd −1 =ρ ⎜ ⎟ = J ρ0 ⎜ ⎟ ∂ε ab ⎝ ∂ε cd ⎠ ∂E AB ⎝ ∂ECD ⎠ ∂ε cd ∂ε ab (5.285) =
ABCD
{
}
δ.(( aAδ .bB))δ.((Cc δ .dD)) 1 + ⎡⎣o(ua;b ) + o(ua;b )2 + o(ua;b )3 + ...⎤⎦ ,
where terms in square braces correspond to products of those of orders one and higher in displacement gradients in (5.284). The following natural symmetries apply for the linear coefficients: abcd = ( ab )( cd ) = ( cd )( ab ) , (5.286) meaning that the tangent elastic stiffness contains up to 21 independent entries. Thirdorder coefficients can be defined in a similar manner: ∂ 2σ ab ∂ 3ψ abcdef (ε,θ , x, g a ) = . (5.287) =ρ ∂ε cd ∂ε ef ∂ε ab ∂ε cd ∂ε ef From (5.287), symmetry conditions limit the number of independent thirdorder coefficients in abcdef to 56. Analogously to (5.62), expanding free energy of the first of (5.268) for a hyperelastic material with thermal effects in a Taylor series about a reference state wherein ua ;b = ε ab = 0 and θ = θ 0 > 0 produces the following result per unit reference volume, where temperature variation ∆θ = θ − θ 0 : 1 abcd 1 abcdef ρ 0ψ ( ε ab ,θ , x, g a ) = Ψ 0 + abε ab + ε abε cd + ε abε cd ε ef 2! 3! 1 abcdefgh + ε abε cd ε ef ε gh + ... − β abε ab ∆θ 4! 1 1 (5.288) − β abcd ε abε cd ∆θ − β abcdef ε abε cd ε ef ∆θ − ... 2! 8 1 1 − β ′abε ab (∆θ )2 − β ′′abε ab (∆θ )3 − ... 2! 8 1 abcd − β ′ ε abε cd (∆θ )2 ... + Y0 (θ , x ) . 4
5.4 Geometrically Linear Elasticity
Quantities in (5.288) are defined as ρ 0ψ ( 0,θ 0 , x, g a ) =Ψ 0 ( x ) + Y0 (θ 0 , x ) = 0 , ab
( x, g a ) = ρ 0
∂ψ ∂ε ab
( x, g a ) = ρ 0
∂ 2ψ ∂ε ab ∂ε cd
abcd
abcdef
abcdefgh
( x, g a ) = ρ 0 ( x, g a ) = ρ 0
β abcd ( x, g a ) = − ρ 0 β abcdef ( x, g a ) = − ρ 0
=0,
∂ 2ψ ∂θ∂ε ab
,
(5.291)
ε =0 θ =θ 0
,
β ′ab ( x, g a ) = − ρ 0
(5.293)
(5.294)
∂
abcd
=−
∂
(5.295)
ε=0 θ =θ0 abcdef
∂θ
ε=0 θ =θ 0
, (5.296) ε=0 θ =θ 0
,
(5.297)
ε =0 θ =θ0
∂ 4ψ ∂θ 3∂Eab
,
(5.298)
ε =0 θ =θ 0
=− ε =0 θ =θ0
,
∂θ
ε=0 θ =θ 0
∂ 4ψ ∂θ 2 ∂ε ab ∂ε cd
, ε =0 θ =θ0
,
∂ 3ψ ∂θ 2 ∂ε ab
β ′′ab ( x, g a ) = − ρ 0
(5.292)
ε=0 θ =θ0
ε =0 θ =θ 0
=−
∂ 4ψ ∂θ∂ε ab ∂ε cd ∂ε ef
β ′abcd ( x, g a ) = − ρ0
(5.290)
∂ 4ψ ∂ε ab ∂ε cd ∂ε ef ∂ε gh
∂ 3ψ ∂θ∂ε ab ∂ε cd
(5.289)
ε =0 θ =θ 0
∂ 3ψ ∂ε ab ∂ε cd ∂ε ef
β ab ( x, g a ) = − ρ0
243
∂ 2 abcd ∂θ 2
.
(5.299)
ε=0 θ =θ0
Thermal free energy Y0 (θ , x) can be defined in the same way as Y0 (θ , X ) in Section 5.1.3, noting that x and X refer to the same material particle in the linear theory of the present Section. Definitions (5.289) and (5.290) provide for zero free energy and stress at the reference state. Isothermal elastic constants of orders two, three, and four are defined in (5.291)
244
5 Thermoelasticity
(5.293). Stresstemperature coefficients of various orders are listed in (5.294)(5.299). Stressstraintemperature relations become, from (5.267), ∂ψ ∂ψ σ ab = ρ = J −1 ρ 0 ∂ε ab ∂ε ab ⎡ = J −1 ⎢ ⎣
abcd
ε cd +
1 2
abcdef
ε cd ε ef +
1 6
abcdefgh
ε cd ε ef ε gh + ...
(5.300) 3 abcdef ε cd ε ef ∆θ − ... − β ∆θ − β ε cd ∆θ − β 8 1 1 1 ⎤ − β ′ab ( ∆θ ) 2 − β ′′ab ( ∆θ )3 − ... − β ′abcd ε cd (∆θ )2 ...⎥ . 2 8 2 ⎦ In the geometrically linear theory, terms of orders two and higher in the strain ε are typically omitted from (5.300) since displacement gradients are assumed small. Such an omission is consistent with the use of infinitesimal strain measure ε as opposed to finite strain measure E as a state variable, since ε differs from E by terms quadratic in displacement gradients in (2.162). Furthermore, if the distinction between the Kirchhoff stress and Cauchy stress is omitted, then τ ab = J σ ab ≈ σ ab , with σ ab thus used as the exclusive measure of stress in the linear theory, then (5.300) becomes 1 σ ab = abcd ε cd − β ab ∆θ − β abcd ε cd ∆θ − β ′ab (∆θ ) 2 2 (5.301) 1 1 − β ′′ab (∆θ ) 3 − ... − β ′abcd ε cd (∆θ ) 2 .... 8 2 Notice also that at the reference state, from (5.65) and (5.285), secondorder elastic constants of nonlinear and linear theories are equal since terms of orders one and higher in displacement gradients vanish from (5.284) and (5.285) at the reference state: ⎛ ∂ 2ψ ⎞ ∂ 2ψ abcd δ .(( aAδ .bB))δ.((Cc δ .dD)) =⎜Jρ = ρ0 ⎟ E E ε ε ∂ ∂ ∂ ∂ E = 0 ε = 0 ab cd ⎠ AB CD ⎝ (5.302) ab
abcd
θ =θ0
θ =θ0
=
ABCD
δ .(( aAδ.bB))δ .(( Cc δ.dD)) .
Similarly, thermal stress coefficients in (5.68) and (5.294) are equal at the reference state: ⎛ ∂ 2ψ ⎞ ∂ 2ψ = − ρ0 β ab = − ⎜ J ρ δ .(( aAδ .bB)) = β ABδ .(( aAδ .bB)) . (5.303) ⎟ ∂ ∂ ∂ ∂ θ ε θ E 0 E = 0 ε = ab ⎠ AB ⎝ θ =θ0
θ =θ 0
5.4 Geometrically Linear Elasticity
245
5.4.4 Materially Linear Hyperelasticity
Omitting terms of orders two and higher in strains and temperature variations, (5.288) becomes 1 abcd θ ρ0ψ = ε abε cd − β abε ab ∆θ − ρ 0 cθ ln , (5.304) θ0 2 where elastic coefficients abcd , stresstemperature coefficients β ab , and specific heat c are defined as second derivatives of the free energy at null strain and reference temperature: ⎛ ∂ 2ψ ⎞ ∂ 2ψ ∂ 2ψ abcd , β ab = − ρ 0 , c = − ⎜θ 2 ⎟ .(5.305) = ρ0 ∂ε ab ∂ε cd ε = 0 ∂θ∂ε ab ε = 0 ⎝ ∂θ ⎠ ε =0 θ =θ0
θ =θ0
θ =θ 0
At a particular material point x, parameters in (5.305) are all constants. The thermal energy comprising the rightmost term in (5.304) depends only on temperature. This term is consistent with a thermal internal energy U 0 measured per unit reference volume depending linearly on temperature: 1 ∂U 0 . (5.306) U 0 = ρ0 cθ ⇔ c = ρ0 ∂θ Stress and entropy are, from (5.304) and (5.267) σ ab ≈ τ ab = abcd ε cd − β ab ∆θ , (5.307) ⎛
⎞ θ (5.308) + 1⎟ . ⎝ θ0 ⎠ At a fixed reference temperature θ = θ 0 , the requirement that the free energy be positive for all nonnegligible strains ε ab ≠ 0 implies that the
ρ 0η = β abε ab + ρ 0 c ⎜ ln
fourthorder tensor abcd should be positive definite. From (5.304), it follows that at θ = θ 0 , ρ 0ψ is a strictly convex function of ε. Stress equation (5.307) applies for any choice of coordinate system, including Cartesian coordinates and general curvilinear coordinates. In physical components of orthogonal curvilinear coordinates (Section 2.4), the stressstrain law exhibits the same form (Malvern 1969):
σ
ab
=
3
∑
c , d =1
abcd
ε cd − β ab ∆θ ,
(5.309)
where indices in angled brackets are referred to physical components of orthogonal curvilinear coordinates such as cylindrical coordinates of Section 2.4.2 and Table 4.3 or spherical coordinates of Section 2.4.3 and Table 4.4. Transformation formulae relating quantities in (5.309) to their counterparts in Cartesian coordinates are listed by Malvern (1969).
246
5 Thermoelasticity
5.4.5 Symmetry
Analogously to (5.90), matrices of secondorder elastic constants and thermal stress constants exhibit the following symmetries: abcd (5.310) = cdab = bacd = abdc , β ab = β ba , meaning that abcd contains up to 21 independent entries and β ab contains up to 6 independent entries. Thus (5.307) is often written in reduced matrix form as ⎡ σ 11 ⎤ ⎡ ⎢ 22 ⎥ ⎢ ⎢σ ⎥ ⎢ ⎢σ 33 ⎥ ⎢ ⎢ 23 ⎥ = ⎢ ⎢σ ⎥ ⎢ ⎢ σ 31 ⎥ ⎢ ⎢ 12 ⎥ ⎢ ⎢⎣ σ ⎥⎦ ⎢⎣
11
12
13
14
12
22
23
24
25
13
23
33
34
35
14
24
34
44
45
⎤ ⎡ ε11 ⎤ ⎡ β 11 ⎤ ⎥ ⎥ ⎢ 22 ⎥ 26 ⎢ ⎥ ⎢ ε 22 ⎥ ⎢ β ⎥ 36 ⎥ ⎢ ε 33 ⎥ ⎢ β 33 ⎥ ⎥ ⎥ − ⎢ 23 ⎥ ∆θ 46 ⎢ ⎥ ⎢ 2ε 23 ⎥ ⎢ β ⎥ 56 ⎥ ⎢ 2ε ⎥ ⎢ β 31 ⎥ ⎥ ⎢ 31 ⎥ ⎢ 12 ⎥ 66 ⎥⎦ ⎢⎣ 2ε 12 ⎦⎥ ⎢⎣ β ⎥⎦
15
15
25
35
45
55
16
26
36
46
56
16
,
(5.311)
where components of the symmetric 6×6 matrix of secondorder elastic constants are identical to those in (5.92): ⎡ ⎢ ⎢ ⎢ ⎢ ⎢ ⎢ ⎢ ⎢⎣
11
=
1111
12
= = = = =
1122
13 14 15 16
− 22
1133
23
1123
24
1113
25
1112
26
= = = = =
2222 2233
33
2223
34
2213
35
2212
36
−
−
−
−
− = = = =
− − = = =
− − − = =
− − − − =
3333 3323
44
3313
45
3312
46
2323 2313
55
2312
56
1313 1312
66
⎤ ⎥ ⎥ ⎥ ⎥ . (5.312) ⎥ ⎥ ⎥ 1212 ⎥⎦
Voigt’s notation in (5.93)(5.98) applies. Components of the stress and moduli are written in reduced form to take advantage of symmetries: (5.313) σ ( ab) ~ σ a , ( ab)( cd ) ~ ab , β ab ~ β a . Barred indices span 1,2,…6 and correspond to unbarred pairs of indices as noted in (5.93). Consistent with (5.311) and (5.313), strains in Voigt’s notation satisfy 2ε ( ab ) = (1 + δ ab )ε a . (5.314) As a consequence of hyperelasticity, secondorder elastic constants exhibit the remaining symmetries ( ab )
= . Free energy in the materially linear case, (5.304), is 1 ab θ ρ 0ψ = ε a ε b − β a ε a ∆θ − ρ 0 cθ ln , θ0 2 and the stress of (5.307) is written compactly as σ a = ab ε b − β a ∆θ . ab
(5.315) (5.316) (5.317)
5.4 Geometrically Linear Elasticity
247
Arguments pertaining to transformations of material coefficients under rotations of the coordinate system in (5.99)(5.104) apply likewise in the geometrically linear theory. Furthermore, since (5.302) and (5.303) indicate that elastic constants and thermal stress coefficients measured at the reference state in linear and nonlinear theories are equal, these particular material coefficients share the same symmetries in linear and nonlinear theories. Since in a rigid heat conductor, the reference and current configurations coincide, it follows that conductivity coefficients in the linear theory, k ab of (5.277), are related to those of the nonlinear theory, K AB in (5.48), at material point X in the undeformed reference state by k ab ε = 0 = δ .aAδ .bB K AB E = 0 . (5.318) θ =θ 0
θ =θ 0
Thus, thermal conductivities in linear and nonlinear descriptions should exhibit the same symmetries when evaluated at the same reference state. Now consider a geometrically linear and materially linear, isotropic hyperelastic solid. Secondorder elastic constants in (5.310) become abcd (5.319) = µ ( g ac g bd + g ad g cb ) + λ g ab g cd , with µ ( x) the shear modulus and λ ( x ) Lamé’s constant. Thus, the elasticity tensor in 6×6 matrix form is identical to that of (5.122). Thermal stress coefficients for an isotropic material are β ab = β g ab . (5.320) Stressstraintemperature relations then exhibit the form (5.321) σ ab = 2 µε ab + (λε .cc − β ∆θ ) g ab . Local balance of linear momentum (4.17), per unit spatial volume, is σ ;abb = (2 µε ab );b + (λε .cc − β ∆θ );b g ab = ρ u a − b a . (5.322) Under isothermal conditions ( ∆θ = 0 ) and when elastic constants are independent of position (i.e., a homogeneous body), (5.322) reduces to c ab 2 µε ;ab = ρu a − b a . (5.323) b + λε .c ;b g In rectangular Cartesian coordinates, the covariant derivatives become partial derivatives. In general curvilinear coordinates, (5.323) is cumbersome. Tables 5.1 and 5.2 list (5.323) in physical components of cylindrical coordinates (see Section 2.4.2 and Table 4.3) and spherical coordinates (see Section 2.4.3 and Table 4.4), following Malvern (1969).
248
5 Thermoelasticity
Table 5.1 Momentum balance of linear isotropic elasticity: cylindrical coordinates Quantity Momentum
Rotation Dilatation
Rcomponent
θ−component
Zcomponent
(2 µ + λ )e, R − 2 µ R −1wZ ,θ
(2 µ + λ ) R −1e,θ − 2 µ wR ,Z
(2 µ + λ )e,Z − 2 µ R −1 ( rwθ ) ,R
+2 µ wθ ,Z = ρ aR − bR
+2 µ wZ , R = ρ aθ − bθ
+2 µ R −1wR ,θ = ρ aZ − bZ
2 wR = R −1u Z ,θ − uθ ,Z
2 wθ = u R ,Z − uZ ,R
2 wZ = R −1[( Ruθ ) ,R − u R ,θ ]
−1
e = R [( Ru R ), R + uθ ,θ ] + u Z ,Z
Table 5.2 Momentum balance of linear isotropic elasticity: spherical coordinates Quantity Momentum
Rcomponent (2 µ + λ )e,R
Dilatation
ϕcomponent
+2 µ R sin θ ×
−2 µ R −1[( Rwθ ), R − wR ,θ ]
−2 µ R sin θ × [( wϕ sin θ ),θ − wθ ,ϕ ]
[( Rwϕ sin θ ),R − wR ,ϕ ]
= ρ aR − bR
= ρ aθ − bθ
2 wR = R −1 sin −1 θ
2 wθ = R −1[uR ,ϕ sin −1 θ
×[(uϕ sin θ ),θ − uθ ,ϕ ]
−( Ruϕ ),R ]
−1
Rotation
θ−component (2µ + λ ) R −1e,θ
−1
−1
−1
(2µ + λ )e,ϕ R −1 sin −1 θ = ρ aϕ − bϕ 2 wϕ = R −1[( Ruθ ), R − u R ,θ ]
e = R −2 sin −1 θ [( R 2u R sin θ ),R + ( Ruθ sin θ ),θ + ( Ruϕ ),ϕ ]
5.5 Explicitly Resolved Thermal Deformation An alternative formulation of finite hyperelasticity with temperature changes addresses the kinematics of deformation in a more refined or explicit manner (Stojanovitch 1969; Lu and Pister 1975; Imam and Johnson 1998; Clayton 2005a, b, 2006a) that proves useful in certain experimental and computational settings. Extending (5.1), the total deformation gradient and lattice deformation gradient remain equivalent, but each is further decomposed into mechanically recoverable elastic and thermal parts, following (3.27): F = FL = FEFθ , (5.324) α θB θα a a La Ea Ea B θα Ea F. A = x., A = F .α g. A = F . B F . A = F .B g.α F . A = F .α F . A , (5.325) where F E is associated with purely mechanical loads, and where Fθ is the deformation attributed solely to temperature changes in the absence of mechanical forces. The form after the final equality in (5.325) is introduced for convenience in keeping track of indices during manipulation of the thermodynamic relations later in Section 5.5.2, even though all indices of F θ are referred to reference coordinates, meaning g.αA = δ .αA . Though alternative prescriptions are possible (see the footnote in Section 3.1.3), evolution of F θ is assumed to follow (3.28):
5.5 Explicitly Resolved Thermal Deformation
F θ F θ −1 = α Tθ , F θ. Aα F θ −1.Aβ = αT α.β θ = α T .AB g.αA g.Bβ θ ,
249
(5.326)
where α T (θ , X , G A ) is a symmetric secondorder tensor of thermal expansion coefficients that, by definition, may depend on temperature θ , location X of material particle (for a heterogeneous solid), and material symmetry via dependence on reference basis vectors G A ( X ) . Thermal expansion coefficients in (5.326) are assumed to possess material symmetries of generic symmetric rank two polar tensors listed in Table A.5. The form of (5.325) applicable for cubic crystals, i.e., αT α.β = αT δ .αβ , has been used for computational modeling of thermoelasticplastic behavior of cubic metals deformed at high strain rates (Lee et al. 1997; Clayton 2005a, b, 2006a; Vogler and Clayton 2008). 5.5.1 Constitutive Assumptions
In the context of (5.324), constitutive assumptions (5.2)(5.5) are replaced by the following, meaning that the state of the material at point X is determined by the elastic deformation, temperature, and temperature gradient: g ⎛ ⎞ (5.327) ψ = ψ ⎜ F E ,θ , ∇ θ , X , G A ⎟ , ψ = ψ ( F E .aα ,θ ,θ ,a , X , G A ) ; ⎝ ⎠ g ⎛ ⎞ η = η ⎜ F E ,θ , ∇ θ , X , G A ⎟ , η = η ( F E .aα ,θ ,θ, a , X , G A ) ; (5.328) ⎝ ⎠ g ⎛ ⎞ σ = σ ⎜ F E ,θ , ∇ θ , X , G A ⎟ , σ ab = σ ab ( F E .aα ,θ ,θ, a , X , G A ) ; (5.329) ⎝ ⎠ g ⎛ ⎞ q = q ⎜ F E ,θ , ∇ θ , X , G A ⎟ , q a = q a ( F E .aα ,θ ,θ, a , X , G A ) . (5.330) ⎝ ⎠ Like (5.2)(5.5), relations (5.327)(5.330) are not always objective under a rigid body transformation of spatial coordinates. Let such a transformation ˆ + c , where Q ˆ =Q ˆ −T . Then the elastic deformabe described by x → Qx tion is assumed to transform in the same manner as the total deformation ˆ E . The recoverable (symmetric) elastic deformagradient, i.e., F E → QF tion tensor CE and strain tensor EE , defined in covariant form by 1 E E E Cαβ = F E .aα g ab F E .bβ , Eαβ = (Cαβ − gαβ ) , (5.331) 2 thus remain invariant under such rigid body motions, following the same analysis procedure considered in (4.50). Hence, a possible set of objective constitutive assumptions is
250
5 Thermoelasticity E ,θ , θ , A , X , G A ) ; ψ = ψ ⎛⎜ EE ,θ , ∇ θ , X , G A ⎞⎟ , ψ = ψ ( Eαβ
G
(5.332) ⎝ ⎠ G E (5.333) η = η ⎛⎜ EE ,θ , ∇θ , X , G A ⎞⎟ , η = η ( Eαβ , θ ,θ , A , X , G A ) ; ⎝ ⎠ G ⎛ ⎞ E Σ = Σ ⎜ EE ,θ , ∇ θ , X , G A ⎟ , Σ αβ = Σ αβ ( Eαβ ,θ ,θ , A , X , G A ) ; (5.334) ⎝ ⎠ G ⎛ ⎞ E , θ ,θ , A , X , G A ) ; (5.335) Q = Q ⎜ EE ,θ , ∇ θ , X , G A ⎟ , Q A = Q A ( Eαβ ⎝ ⎠ immediately recognizable as (5.15)(5.18) with the total strain E replaced by the elastic strain EE and the second PiolaKirchhoff stress replaced by Σ αβ = J E F E −1α.aσ ab F E −1.βb , (5.336) where J E = g / g det F E . The stress in (5.336), referred to as an elastic second PiolaKirchhoff stress or simply an elastic stress, is symmetric and is invariant under rigid body motions of the spatial coordinate frame: Σ αβ → J E −1 F E −1α.a Qˆ .−c1a Qˆ .ceσ ef Qˆ .df Qˆ .−d1b F E −1.βb = J E −1 F E −1α.eσ ef F E −1.βf . (5.337) As a result of different constitutive assumptions used in (5.332)(5.335), thermodynamic and thermostatic relationships derived in Sections 5.15.4 generally do not apply when thermal deformation is nonnegligible. 5.5.2 Thermodynamics
From (5.324) and (5.326), spatial velocity gradient L of (2.176) is (5.338) La.b = v;ab = F. Aa F −1.Ab = F .Eαa F E −1α.b + F E .aα αT α.β F E −1.βbθ . The material time derivative of the elastic strain tensor is computed directly from (5.331), leading to a relationship similar to (3.64): E 2 Eαβ = F .Eαa g ab F E .bβ + F E .aα g ab F .Eβb = 2 F E .aα DabE F E .bβ , (5.339) with the symmetric rate of elastic deformation referred to the spatial frame 2 DabE = g ac F .Eαc F E −1α.b + gbc F .Eαc F E .−a1α = 2 D(Eab ) . (5.340) Stress power per unit reference volume entering (4.39) can then be written as follows, using symmetry of the Cauchy stress: Σ AB E AB = J σ ab Lab = J σ ab ( DabE + g ac F E .cα α T α.β F E −1.βbθ ) (5.341) E = J σ ab ( F E −1α.a Eαβ F E −1.βb + g ac F E .cα α T α.β F E −1.βbθ ). Using constitutive assumption (5.332) along with (5.339), the appropriate version of dissipation inequality (4.72) is
5.5 Explicitly Resolved Thermal Deformation
⎛ E −1α ab E −1β ∂ψ ⎞ E ⎜⎜ JF .aσ F .b − ρ 0 E ⎟⎟ Eαβ ∂Eαβ ⎠ ⎝ ∂ψ ⎛ ⎞ − ρ 0 ⎜η + − J ρ 0−1σ ab g ac F E .cα α T α.β F E −1.βb ⎟θ ∂θ ⎝ ⎠ ∂ψ − ρ0 γ 0 A − θ −1θ, AQ A ≥ 0, ∂θ , A
251
(5.342)
where the referential rate of temperature gradient γ 0 A is defined in (5.29). Appealing to arguments analogous to those immediately following (5.22) regarding thermodynamic admissibility, the following constitutive equations for the Cauchy stress tensor, the elastic stress measure (5.336), and the specific entropy emerge: ∂ψ σ ab = ρ F E .aα E F Eb.β , (5.343) ∂Eαβ
Σ αβ = J E ρ
∂ψ , E ∂Eαβ
∂ψ + ρ 0−1 J σ ab g ac F E .cα αT α.β F E −1.βb ∂θ ∂ψ ∂ψ ∂ψ E =− + Cαχ + ς. αT α.β E = − ∂θ ∂Eχβ ∂θ
(5.344)
η =−
(5.345)
Scalar quantity ς (EE ,θ , X ) , with dimensions of entropy per unit mass, does not emerge in the classical theory of thermoelasticity of Section 5.1. For the case of isotropic thermal expansion αT α.β = αT δ .αβ , this term reduces to ς = −3αT p / ρ , where p is the Cauchy pressure (Clayton 2005a). From (5.340)(5.342), ∂ψ / ∂θ , A = 0 , and the response functions reduce to
ψ = ψ ( EE ,θ , X , G A ) , η = η ( EE ,θ , X , G A ) , Σ = Σ ( EE ,θ , X , G A ) . (5.346)
The conduction inequality remains identical to that of (5.32): −θ −1θ , AQ A ≥ 0 , (5.347) and the local rate of entropy production vanishes as in (5.33). The specific heat capacity per unit mass at constant elastic strain is defined similarly, but not identically, to that in (5.46): ∂e ∂η ∂ ⎛ ∂ψ ∂ 2ψ ∂ς ⎞ c= = −θ − = − +θ , (5.348) ς θ ⎜ ⎟ 2 ∂η ς = 0 ∂θ ∂θ ⎝ ∂θ ∂θ ∂θ ⎠
252
5 Thermoelasticity
following the definition of the free energy ψ = e − θη in Table 4.2 which still applies in the present context. Using Fourier’s law (5.48), energy balance (4.39) reduces to ρ 0θη = ( K ABθ, B ) ; A + ρ0 r . (5.349) By the chain rule, (5.332), and (5.348), d⎛ ∂ψ ⎞ ρ0θη = ρ0θ ⎜ ς − ⎟ dt ⎝ ∂θ ⎠ = ρ 0θς − ρ 0θ
∂ ⎛ ∂ψ E ∂ψ ⎞ θ⎟ ⎜ E Eαβ + ∂θ ⎜⎝ ∂Eαβ ∂θ ⎟⎠
∂ 2ψ (5.350) θ ∂θ 2 ∂ς E = ρ 0 cθ + θβ αβ Eαβ − ρ 0θ θ + ρ 0θς ∂θ ⎛ ∂ς ⎞ E = ρ 0 cθ + θ ⎜ β αβ + ρ 0 E ⎟ Eαβ , ⎜ ∂Eαβ ⎟⎠ ⎝ E where symmetric contravariant tensor β αβ = − ρ0 ∂ 2ψ / ∂θ∂Eαβ accounts for E = ρ 0θς + θβ αβ Eαβ − ρ 0θ
thermoelastic coupling. Equating (5.349) and (5.350) results in a rate equation for the temperature analogous to (5.51): E ρ 0 cθ = ( K ABθ, B ) ; A − θβˆ αβ Eαβ + ρ0 r , (5.351) where the modified thermal stress coefficients4 are defined according to ⎛ ∂ς ∂ς ∂ 2ψ ⎞ . (5.352) βˆ αβ = ρ0 E + β αβ = ρ0 ⎜⎜ E − E ⎟ ⎟ ∂Eαβ ⎝ ∂Eαβ ∂θ∂Eαβ ⎠ 5.5.3 Representative Free Energy
An apparent advantage of the present formulation (Section 5.5) over classical nonlinear thermoelasticity (Section 5.1) is that in the former, deformations and deformation rates attributed to temperature rise can easily be delineated from those due to mechanical stresses. The free energy in the first of (5.346) is expanded in a Taylor series about a reference state charE acterized by the conditions F E .aα = g.aα , Eαβ = 0 , θ = θ 0 > 0 as follows: 4
In prior work (Clayton 2005a, b; Vogler and Clayton 2008) the distinction be
tween thermal stress coefficients was omitted, i.e., it was assumed β αβ = βˆ αβ .
5.5 Explicitly Resolved Thermal Deformation
253
E Ψ 0 = ρ 0ψ ( Eαβ ,θ , X , G A )
= Ψ0 +
αβ
E + Eαβ
1 2!
αβχδ
E E + Eαβ Eχδ
1 3!
αβχδεφ
E E Eαβ Eχδ EεφE
1 αβχδεφϕγ E E E E E Eαβ Eχδ Eεφ Eϕγ + ... − β αβ Eαβ ∆θ 4! (5.353) 1 1 E E E E − β αβχδ Eαβ Eχδ ∆θ − β αβχδεφ Eαβ Eχδ EεφE ∆θ − ... 2! 8 1 1 E E (∆θ ) 2 − β ′′αβ Eαβ (∆θ )3 − ... − β ′αβ Eαβ 2! 8 1 E E (∆θ ) 2 ... + Y0 (θ , X ). − β ′αβχδ Eαβ E χδ 4 The temperature change from the reference state is ∆θ = θ − θ0 . Material properties in (5.353) are defined as follows: Ψ 0 ( 0,θ 0 , X , G A ) =Ψ 0 ( X ) + Y0 (θ 0 , X ) = 0 , (5.354) +
αβ
αβχδ
αβχδεφ
αβχδεφϕγ
( X ,G A ) = ( X ,GA ) =
( X ,G A ) = ( X ,G A ) =
∂Ψ 0 E ∂Eαβ
∂ 2Ψ 0 E E ∂Eαβ ∂Eχδ
β αβχδεφ ( X , G A ) = −
,
(5.356)
,
∂ 2Ψ 0 E ∂θ∂Eαβ
,
(5.358)
EE = 0 θ =θ 0
,
(5.359)
EE = 0 θ =θ 0
=−
=− EE = 0 θ =θ0
αβχδ
∂
EE = 0 θ =θ 0
∂ 4Ψ 0 E ∂θ∂Eαβ ∂Eχδ ∂EεφE
(5.357)
EE = 0 θ =θ 0
∂ 4Ψ 0 E E ∂Eαβ ∂Eχδ ∂EεφE ∂EϕγE
∂ 3Ψ 0 E E ∂θ∂Eαβ ∂Eχδ
E
(5.355)
EE = 0 θ =θ 0
∂ 3Ψ 0 E E ∂Eαβ ∂Eχδ ∂EεφE
β αβ ( X , G A ) = − β αβχδ ( X , G A ) = −
= 0, EE = 0 θ =θ 0
∂θ ∂
,
(5.360)
EE = 0 θ =θ 0
αβχδεφ
∂θ
, (5.361) EE = 0 θ =θ 0
254
5 Thermoelasticity
β ′αβ ( X , G A ) = −
∂ 3Ψ 0 E ∂θ 2 ∂Eαβ
β ′′αβ ( X , G A ) = − β ′αβχδ ( X , G A ) = −
,
∂ 4Ψ 0 E ∂θ 3∂Eαβ
∂ 4Ψ 0 E E ∂θ 2 ∂Eαβ ∂Eχδ
(5.362)
EE = 0 θ =θ 0
,
(5.363)
EE = 0 θ =θ 0
=− EE = 0 θ =θ0
∂ 2 αβχδ ∂θ 2
.
(5.364)
EE = 0 θ =θ 0
Definitions (5.354) and (5.355) result in null free energy and null stress at the reference state. Isothermal elastic constants of orders two, three, and four are defined in (5.356)(5.358). Isothermal stresstemperature coefficients of various orders are listed in (5.359)(5.364). Since coefficients in (5.356)(5.364) are all derivatives of thermodynamic potentials, these coefficients exhibit the same material symmetries as polar tensors of the same orders in (5.65)(5.73) and Section 5.1.5. If the reference state is chosen as one in which F θ α. A = g.αA (i.e., thermal deformation vanishes at θ = θ 0 ), then reference states in (5.62) and (5.353) coincide. From (5.344) and (5.353), the elastic second PiolaKirchhoff stress is ∂ψ ∂ψ ∂ψ Σ αβ = J E ρ E = J E J −1 ρ 0 E = J θ −1 ρ 0 E ∂Eαβ ∂Eαβ ∂Eαβ
⎡ = J θ −1 ⎢ ⎣
αβχδ
E Eχδ +
1 2
αβχδεφ
E Eχδ EεφE +
1 6
αβχδεφϕγ
E Eχδ EεφE EϕγE + ...
3 E Eχδ ∆θ − β αβχδεφ Eχδ EεφE ∆θ − ... − β ∆θ − β 8 1 1 1 ⎤ E − β ′αβ (∆θ ) 2 − β ′′αβ (∆θ )3 − ... − β ′αβχδ Eχδ ( ∆θ ) 2 ⎥ . 2 8 2 ⎦ αβ
αβχδ
(5.365)
E
The Jacobian determinant of thermal deformation is J θ = g / G det F θ . Recall that stressfree thermal expansion to first order in strain is included in kinematic description (5.324)(5.326), since α T = α T (θ , X , G A ) . Rank two stresstemperature coefficients β αβ , β ′αβ , β ′′αβ , … will also induce thermal expansion of the same physical origin. Thus, experimental delineation of secondorder stresstemperature coefficients in (5.365) from secondorder temperaturedependent thermal expansion coefficients in (5.326) becomes problematic. This ambiguity can be eliminated by assuming that β αβ , β ′αβ , β ′′αβ , … vanish by definition:
5.6 Lagrangian Field Theory of Elasticity
β αβ = −
β ′αβ = −
β ′′αβ = −
∂ 2Ψ 0 E ∂θ∂Eαβ ∂ 3Ψ 0 E ∂θ 2 ∂Eαβ ∂ 4Ψ 0 E ∂θ 3∂Eαβ
=0,
255
(5.366)
EE = 0 θ =θ 0
=0,
(5.367)
=0.
(5.368)
EE = 0 θ =θ0
EE = 0 θ =θ 0
Thermal stress coefficients of orders four and higher are retained since α T is, by definition, independent of elastic strain. The stress becomes 1 αβχδεφ E 1 αβχδεφϕγ E E E ⎡ Σ αβ = J θ −1 ⎢ αβχδ EχδE + Eχδ + Eχδ Eεφ Eϕγ + ... 2 6 ⎣ (5.369) 3 αβχδεφ E E 1 αβχδ E αβχδ E 2⎤ −β Eχδ ∆θ − β Eχδ Eεφ ∆θ − ... − β ′ Eχδ ( ∆θ ) ⎥ . 8 2 ⎦ Thermal free energy Y0 (θ , X ) in (5.353) can be defined in the same way as in Section 5.1.3. In the materially linear, but geometrically nonlinear, regime the appropriate reduction of (5.353), using (5.366), is 1 αβχδ E E θ Ψ0 = Eαβ Eχδ − ρ0 c θ ln , (5.370) 2 θ0 where a constant specific heat capacity is defined as in the last of (5.85): ⎛ ∂ 2ψ ⎞ . (5.371) c = − ⎜θ 2 ⎟ ⎝ ∂θ ⎠ EE = 0 θ =θ0
The elastic second PiolaKirchhoff stress and Cauchy stress then become, respectively, Σ αβ = J θ −1 αβχδ EχδE , σ ab = J −1 F E .aα αβχδ EχδE F E .bβ . (5.372)
5.6 Lagrangian Field Theory of Elasticity Hamilton’s principle applied to the appropriate action integral for hyperelastic bodies can be used to obtain a local form of the balance of linear momentum as well as constitutive equations relating stress, deformation gradient, and strain energy. The treatment of Section 5.6 is restricted to the athermal case with no dissipation, meaning heat flux, heat sources,
256
5 Thermoelasticity
temperature gradients, and temperature rates are not addressed. Prior to presentation of Hamilton’s principle in the context of nonlinear elasticity of grade one, the variational derivative is introduced. 5.6.1 The Variational Derivative A family of deformations is denoted by x a = x a ( X A , Λ ) , where Λ is a scalar parameter. At a reference state characterized by conditions Λ = 0 and x a = g.aA X A , field x a = x a ( X A ,0) is known. The first variation of x is then defined by (Toupin 1956, 1962; Eringen 1962): ∂x a δ xa = dΛ , (5.373) ∂Λ X Λ=0
A
where reference coordinates X of material particle at X are held fixed during the variation. For a scalar function f = f ( x a , x.,aA , x:aAB ,...) depending on spatial position, deformation gradient, and higherorder total covariant derivatives of position (see e.g., (2.116)), the first variation of f is ∂f δf = dΛ . (5.374) ∂Λ X Λ =0
Since reference coordinates are held fixed in the variation, partial differentiation of a scalar with respect to reference coordinates commutes with the variational derivative: δ ( f , A ) = (δ f ), A = δ f, A . (5.375) The first variation does not commute with partial differentiation in the spatial frame ∂ a = ∂ / ∂x a . Similarities between the variational derivative and the material time derivative of Section 2.6.1 are evident (Eringen 1962). In particular, δ x a is analogous to v a dt , and δ f is analogous to fdt . The following formulae for variations of kinematic quantities are often useful (Toupin 1956; Eringen 1962): δ F. Aa = δ ( x.,aA ) = (δ x a ), A + F. Aa ;bδ xb (5.376) = (δ x a );b F. Ab = (δ x a );b x.,bA = (δ x a ); A ,
δ F −1.Aa = δ ( X .,Aa ) = − F −1.Ab F −1.Ba (δ xb ); B = − F −1.Ab (δ xb );a ,
δ J = J (δ F. Aa ) F −1.Aa = J (δ x a );a .
(5.377)
(5.378) Notice that (5.376) is analogous to (2.175), and (5.378) is analogous to (2.181). It follows from (5.375), (5.377), and the chain rule that
5.6 Lagrangian Field Theory of Elasticity
δ ( f , a ) = δ ( f, A F −1.Aa ) = F −1.Aaδ ( f, A ) + f, Aδ F −1.Aa = F −1.Aa (δ f ), A − f,b F −1.Aa (δ xb ); A = (δ f ), a − f,b (δ xb ); a .
257
(5.379)
5.6.2 Hamilton’s Principle in Nonlinear Elasticity A general version of Hamilton’s principle incorporating boundary conditions and external forces can be written as (Toupin 1964) t2
⎡
t1
⎣V
(
)
⎤
t2
⎡
⎤
⎦
t1
⎣S
⎦
(
)
t2
δ A + ∫ ⎢ ∫ ρ0bˆ iδ x dV ⎥ dt + ∫ ⎢ ∫ ( tˆiδ x ) dS ⎥ dt = ∫ Pˆ iδ x dV , V
(5.380)
t1
where bˆ ( X , t ) is a vector of generalized body forces per unit mass, tˆ( X , t ) is a generalized traction vector prescribed per unit reference area, Pˆ is a vector of generalized momenta, and the action integral is t2
A = ∫ L dt .
(5.381)
t1
The Lagrangian functional L is given by the volume integral L = ∫ L0 dV ,
(5.382)
V
where L0 is the Lagrangian energy density per unit reference volume of the following functional form for hyperelastic solids of grade one (Yavari et al. 2006): (5.383) L0 = L0 ( x a , x a , x.,aA , g ab , X A , G A ) . Computation of the variation in (5.380) leads to t2 t2 ⎛ ⎞ δ A = δ ∫ L dt = δ ∫ ⎜ ∫ L0 dV ⎟ dt = t1 t1 ⎝ V ⎠ t
2 ∂L ∂L ∂L ⎛ ∂L = ∫ ∫ ⎜ a0 δ x a + a0 δ x a + 0a δ F. Aa + 0 δ g ab ∂x ∂x ∂F. A ∂g ab t1 V ⎝
⎞ ∂L ∂L + 0A δ X A + 0 iδ G A + L0δ (dV ) ⎟ dVdt ∂X ∂G A ⎠ t
(5.384)
2 ⎛ ∂L ⎞ ∂L ∂L ∂L = ∫ ∫ ⎜ a0 δ x a + a0 δ x a + 0a δ F. Aa + 0 δ g ab ⎟ dVdt , ∂x ∂F. A ∂g ab ⎠ t1 V ⎝ ∂x since L0 does not depend explicitly on time and since, by the definition of the variational derivative used here,
258
5 Thermoelasticity
δ X A = 0 , δ G A ( X ) = 0 , δV ( X ) = 0 , δ t = 0 ,
(5.385) thereby enabling the variational operator to be brought inside the integration over time and reference volume. Integrating the remaining terms by parts, noting that d (δ x a ) / dt = δ ( dx a / dt ) = δ x a , and applying the divergence theorem of (2.193) of Section 2.7.1 in material coordinates results in t2 t2 ⎡ d ⎛ ∂L0 a ⎞ d ⎡ ∂L0 ⎤ a ⎤ ∂L0 a δ x dVdt = ∫t V∫ ∂x a ∫t V∫ ⎢⎣ dt ⎜⎝ ∂x a δ x ⎟⎠ − dt ⎢⎣ ∂x a ⎥⎦ δ x ⎥⎦dVdt 1 1 (5.386) t2 t2 ⎡ ⎛ ∂L0 a ⎞ ⎤ d ⎡ ∂L0 ⎤ a = ⎢ ∫ ⎜ a δ x ⎟ dV ⎥ − ∫ ∫ ⎢ a ⎥ δ x dVdt , ⎠ ⎦ t t1 V dt ⎣ ∂x ⎦ ⎣V ⎝ ∂x 1
t2
∂L0
∫ ∫ ∂F t1 V
a .A
⎡ ∂L0 ⎤ (δ x a ); A dV ⎥ dt a ∂F. A t1 ⎣ V ⎦
t2
δ F. Aa dVdt = ∫ ⎢ ∫
t2 ⎡ ⎤ ⎛ ∂L ⎞ ⎛ ∂L ⎞ = ∫ ∫ ⎢⎜ 0a δ x a ⎟ − ⎜ 0a ⎟ δ x a ⎥dVdt ⎥⎦ ⎠; A ⎝ ∂F. A ⎠; A t1 V ⎢ ⎣⎝ ∂F. A t
(5.387)
t
2 2 ⎛ ∂L ⎞ ⎛ ∂L ⎞ = ∫ ∫ ⎜ 0a N Aδ x a ⎟dSdt − ∫ ∫ ⎜ 0a ⎟ δ x a dVdt , ∂F. A ⎠ t1 V ⎝ ∂F. A ⎠; A t1 S ⎝
t2
t
2 ∂L0 ∂L0 c δ g dVdt = ∫t V∫ ∂g ab ab ∫t V∫ ∂gab gab,cδ x dVdt 1 1
(5.388) ⎞ c g ad ⎟ δ x dVdt , ⎠ appealing to symmetry properties of the spatial Christoffel symbols and their spatial derivatives from (2.60): g ⎛g ⎞ (5.389) δ g ab ( x) = g ab,cδ x c = ⎜ Γ ..cbd g ad + Γ ..cad gbd ⎟ δ x c . ⎝ ⎠ Collecting terms, the first variation of the action integral in (5.384) is t2 ⎡ ∂L ∂L ⎛ g d ⎛ ∂L ⎞ ⎛ ∂L ⎞ ⎞⎤ δ A = ∫ ∫ ⎢ a0 − ⎜ a0 ⎟ − ⎜ 0a ⎟ + 2 0 ⎜ Γ ..abd g cd ⎟ ⎥δ x a dVdt ∂g cb ⎝ dt ⎝ ∂x ⎠ ⎝ ∂F. A ⎠; A ⎠ ⎦⎥ ⎢ ∂x t1 V ⎣ (5.390) t2 t2 ⎡ ⎛ ∂L0 ⎞ a ⎤ ⎛ ∂L0 ⎞ a + ∫ ∫ ⎜ a N A ⎟δ x dSdt + ⎢ ∫ ⎜ a ⎟ δ x dV ⎥ . ∂ ⎠ t1 S ⎝ F. A ⎣V ⎝ ∂x ⎠ ⎦ t1 t2
∂L ⎛ g = ∫∫2 0 ⎜Γ ∂g ab ⎝ t1 V
..d cb
Substitution of (5.390) into (5.380), localizing the result, and requiring that Hamilton’s principle be satisfied for arbitrary variations δ x a gives the
5.6 Lagrangian Field Theory of Elasticity
259
field equations within reference domain V, also called EulerLagrange equations: ⎛ ∂L ⎞ ∂L ∂L ⎛ g d ⎛ ∂L ⎞ ⎞ − ⎜ 0a ⎟ + ρ0 bˆa + a0 = ⎜ a0 ⎟ − 2 0 ⎜ Γ ..abd gcd ⎟ , (5.391) ∂ ∂ ∂ ∂ F x dt x g ⎝ ⎠ ⎝ ⎠ cb ⎝ . A ⎠; A traction boundary conditions on reference surface S: ∂L − 0a N A = tˆa , (5.392) ∂F. A with N the outward unit normal to S, and endpoint conditions on linear momentum per unit reference volume: ∂L0 ˆ = Pa , (at t = t1 , t2 ). (5.393) ∂x a For a hyperelastic solid of grade one, the following Lagrangian is assumed to apply: ⎛1 ⎞ L = K − E − Φ = ∫ ρ ⎜ v a va − e − Φ ⎟ dv 2 ⎝ ⎠ v (5.394) ⎛ ρ0 a ⎞ = ∫ ⎜ x xa − E0 − Φ 0 ⎟ dV , ⎠ V⎝ 2 where kinetic energy K and global internal energy E are introduced in (4.28)(4.30) and global potential energy Φ is given by (4.41), with local potential energy per unit reference volume Φ 0 ( x) = ρ 0 ( X )Φ ( x) . Since in the present Section, entropy production and temperature rates are assumed to vanish, internal energy per unit reference volume E0 and free energy per unit reference volume Ψ 0 = E0 − θ N 0 differ by an arbitrary additive constant. Letting this constant vanish for convenience, and denoting the strain energy density by ρ0ψ =Ψ 0 = E0 , the Lagrangian density becomes
L0 =
ρ0
x a xa −Ψ 0 ( F. Aa , X , G A ) − Φ 0 ( x ) ,
(5.395) 2 where the dependence on F temporarily replaces that on C in (5.44). Notice that (5.395) is a particular form of (5.383). The partial covariant derivative in the first term on the left side of (5.391), using (5.395), becomes ⎛ ∂L ⎞ ⎛ ∂Ψ 0 ⎞ ⎛ ∂Ψ 0 ⎞ ⎛ ∂Ψ 0 ⎞ c − ⎜ 0a ⎟ = ⎜ =⎜ −⎜ F. A a ⎟ a ⎟ a ⎟ ⎝ ∂F. A ⎠; A ⎝ ∂F. A ⎠; A ⎝ ∂F. A ⎠: A ⎝ ∂F. A ⎠;c (5.396) g ⎛ ∂Ψ 0 ⎞ c ..b ⎛ ∂Ψ 0 ⎞ =⎜ + Γ ca ⎜ F , a ⎟ b ⎟ .A ⎝ ∂F. A ⎠: A ⎝ ∂F. A ⎠
260
5 Thermoelasticity
where the total covariant derivative of two point tensor ∂Ψ 0 / ∂F. Aa is defined similarly to (2.116)(2.118) and (4.20). The third term on the left side of (5.391) becomes ∂L0 ∂Φ = − a0 = − ρ0Φ , a = − J ρΦ , a = J ρ ba = ρ0 ba , (5.397) a ∂x ∂x where the conservative body force per unit mass with covariant components ba is introduced in (4.41). The first term on the right of (5.391) becomes (Yavari et al. 2006) d ⎛ ∂L0 ⎞ ρ 0 d ⎡ ∂ = ( xb gbc xc )⎤⎥⎦ dt ⎜⎝ ∂x a ⎟⎠ 2 dt ⎢⎣ ∂x a ρ d ⎡ ∂ d ⎡ ∂ ⎤ ρ ⎤ = 0 g bc ⎢ a ( x b x c ) ⎥ + 0 x b x c ⎢ a g bc ⎥ 2 dt ⎣ ∂x dt ⎣ ∂x ⎦ 2 ⎦ ρ ρ d = 0 g bc ⎡⎣ x bδ .ca + x cδ .ba ⎤⎦ + 0 x b x c g bc , a (5.398) 2 2 dt g ρ ρ ⎛g ⎞ = 0 gbc ( Abδ .ca + Acδ .ba ) + 0 xb x c ⎜ Γ ..acd gbd + Γ ..abd gcd ⎟ 2 2 ⎝ ⎠ g ⎛ ⎞ = ρ 0 ⎜ g ab Ab + xb x c Γ ..abd gcd ⎟ , ⎝ ⎠ with Ab ( X , t ) contravariant components of the material acceleration of (2.174). The rightmost term of (5.391) is ⎤g ∂L ⎛ g ∂ ⎞ ⎡ ∂Ψ 0 −2 0 ⎜ Γ ..abd g cd ⎟ = ⎢ 2 − ρ0 ( x e g ef x f ) ⎥ Γ ..abd g cd ∂g cb ⎝ ∂g cb ⎠ ⎣ ∂g cb ⎦ (5.399) g ⎡ ∂Ψ 0 ..d c b⎤ = ⎢2 − ρ 0 x x ⎥ Γ ab gcd . ⎣ ∂g cb ⎦
Substituting (5.396)(5.399) into (5.391) and collecting terms results in the following reduced set of EulerLagrange equations: ⎛ ∂Ψ 0 ⎞ ⎛ ∂Ψ 0 ∂Ψ 0 b ⎞ g ..d gcd − F. A ⎟ Γ ba . (5.400) + ρ0 (bˆa + ba ) − ρ0 g ab Ab = ⎜ 2 ⎜ a ⎟ ∂F. Ad ⎝ ∂F. A ⎠: A ⎝ ∂gcb ⎠ The first PiolaKirchhoff stress tensor and total body force per unit reference volume are defined respectively as ∂Ψ 0 Pa. A = , Ba = ρ 0 (bˆa + ba ) . (5.401) ∂F. Aa Now following invariance arguments of (5.34)(5.36), let the strain energy density depend on the deformation gradient F and spatial metric g only through the symmetric deformation tensor C:
5.6 Lagrangian Field Theory of Elasticity
Ψ 0 ( F. Aa , G A , X ) =Ψ 0 ( C AB ( F. Aa , g ab ), G A , X ) , where C AB = F. Aa g ab F. Bb . It follows that ∂Ψ 0 ∂Ψ 0 ∂CBC ∂Ψ 0 c F.C , = = F. Bb ∂g bc ∂C BC ∂g bc ∂C BC ∂Ψ 0 ∂Ψ 0 ∂CBC ∂Ψ 0 b A = = (δ .d δ . B gbc F.Cc + δ .cd δ .CA g bc F. Bb ) ∂F. Ad ∂C BC ∂F. Ad ∂C BC ∂Ψ 0 A ∂Ψ 0 = δ .B g dc F.Cc + δ .CA g bd F. Bb ) = 2 g ad F.Ba , ( ∂C BC ∂C AB from which the right side of (5.400) vanishes: ∂Ψ 0 ∂Ψ 0 c 2 g cd = 2 F. Bb F.C g cd ∂g cb ∂CBC
261
(5.402)
(5.403)
(5.404)
(5.405) ⎛ ∂Ψ 0 −1C ae ⎞ c b ∂Ψ 0 F .a g ⎟ F.C g cd = F. B . =F ⎜ e ∂F. Bd ⎝ ∂F. B ⎠ Substituting from (5.401), the left side of (5.400) is identical to the material balance of linear momentum of (4.21): (5.406) P: AaA + B a = ρ0 Aa . Traction boundary conditions (5.392) are identical to those entering Cauchy’s theorem in (4.4): ∂L ∂Ψ 0 tˆa = − 0a N A = N A = Pa. A N A = t0 a , (5.407) ∂F. A ∂F. Aa where by definition tˆa = t0 a is the traction per unit reference area. The b .B
conditions (5.393) on initial and final momentum density are ∂L ρ ⎡ ∂ ⎤ Pˆa = a0 = 0 gbc ⎢ a ( x b x c ) ⎥ = ρ0 g ab x b , (at t = t1 , t2 ). (5.408) 2 ∂x ⎣ ∂x ⎦ Invariance of free energy density under rigid rotations of the spatial frame provides the local balance of angular momentum. Consider a finite rotation F. Aa → Qˆ .ab F. Ab as discussed in Section 4.2.1. An infinitesimal rotaac tion can be expressed in the form Qˆ a ≈ δ a + g Ωˆ ac , where Ωˆ ac = Ωˆ [ ] . .b
.b
bc
According to Toupin (1964), invariance of the free energy density under infinitesimal rotations is sufficient to ensure invariance under finite rotations. Let the differential change of free energy under such small rotations be (Eringen 1962)
262
5 Thermoelasticity
dΨ 0 =
∂Ψ 0 ∂ (Qˆ.ab F. Ab ) ˆ c ∂Ψ 0 dQ.d = F. Ab dQˆ.ab ∂ (Qˆ.ae F. Ae ) ∂Qˆ.cd ∂ (Qˆ.ae F. Ae )
∂Ψ 0 b = F. A g bc d Ωˆ [ac ] = Pa. A FcA d Ωˆ [ ac] . ∂F. Aa
(5.409)
ac Requiring that (5.409) vanish under arbitrary rotations d Ωˆ [ ] leads to a local balance of angular momentum identical to the first of (4.27): dΨ 0 = 0 ⇒ P[.aA Fc] A = 0 ⇔ P aA F. Ac = F. Aa P cA . (5.410)
Notice that no global balance of linear or angular momentum has been posited in Section 5.6.2, and that the derivations apply for any choice of generalized spatial or referential coordinates, including curvilinear coordinates. The procedure followed in (5.380)(5.406) is somewhat analogous to that sketched in Section B.1.2 of Appendix B dealing with dynamic particle systems.
5.7 Elasticity of Grade Two Recall from kinematic relations (2.114) and (2.115) that deformation gradient F provides a firstorder accurate approximation of the length and direction of a differential line element mapped to the current configuration: dx = FdX . This approximation can be interpreted as exact for the case of homogeneous deformations. On the other hand, a secondorder accurate approximation is obtained by retaining the secondorder term in (2.114), leading to 1 dx a ( X ) = F. Aa dX A + FAa:B dX A dX B , (5.411) X X 2 where the total covariant derivative of F with components FAa:B = x:aAB satisfies, from (2.57), (2.59), and (2.116), F, B ⊗ G B = ( F. Aa g a ⊗ G A ), B ⊗ G B = F. Aa:B g a ⊗ G A ⊗ G B (5.412) g G = ( F. Aa , B + Γ ..bca F. Ac F.Bb − Γ ..BAC F.Ca )g a ⊗ G A ⊗ G B .
It follows from local compatibility conditions (2.203) and symmetries of spatial and referential Christoffel symbols that FAa:B = FBa: A , meaning that
5.7 Elasticity of Grade Two
263
the total covariant derivative of F consists of at most 3 × 6 = 18 independent entries. Eringen (1962) shows that5 g
FAa:B = F. Aa , B + Γ
.. a bc
g
F. Ac F. Bb = ( F. Aa ,b + Γ
.. a bc
F. Ac ) F. Bb = FAa;b F. Bb ;
(5.413)
FAa:B = FAa;b F. Bb ⇔ x:aAB = ( x.,aA );b x.,bB ,
from which it follows that for the inverse of the deformation gradient, (5.414) 0 = ( F. Aa F −1.Ac );b ⇒ F −1.Bc ;b = − F −1.Ac F −1.Ba F −1.Cb FAa:C . The first variation of F. Aa:B is found using (5.376), (5.377), and (5.413) as
δ ( F. Aa:B ) = δ ( F. Aa;b F. Bb ) = F. Bbδ ( F. Aa;b ) + F. Aa;bδ ( F.Bb ) = F.Bb ⎡⎣δ ( FAa;C F −1.Cb ) ⎤⎦ + F. Aa ;b (δ xb ); B = F.Bb ⎡⎣δ ( F. Aa ;C ) F −1.Cb + F. Aa ;C (δ F −1.Cb ) ⎤⎦ + F. Aa ;b (δ xb ); B
(5.415)
= F ⎡⎣δ ( F ) F − F F (δ x );b ⎤⎦ + F (δ x ); B = δ ( F. Aa ); B . In what follows in Section 5.7, concepts of surface gradient and normal derivative of a differentiable function at a surface are used. For a differentiable function f ( x, t ) defined on spatial surface s, the covariant derivative, normal derivative, and surface gradient are related by (Toupin 1962): f;a = na D ( f ) + Da ( f ) , D( f ) = f;a n a , Da ( f ) = (δ a.b − na nb ) f;b , (5.416) b .B
a . A ;C
−1C .b
a A ;C
−1C .c
c
a . A; c
c
where na ( x, t ) is the unit outward normal to s, the first term on the right accounts for the normal derivative Df ( x, t ) , and the second accounts for the tangential derivative Da f ( x, t ) . The following integral identity applies for the tangential derivative of f over surface s bounded by closed curve c: c c d (5.417) ∫ Da ( f )nb ds = ∫ (κ.c na nb − κ ab ) fds − ∫ f ε acd n nb dx , s
s
c
where boundary s is assumed sufficiently smooth (i.e., no sharp edges or corners) and f ( x, t ) is assumed to have continuous first partial derivatives with respect to x a . The second fundamental form of a smooth surface is defined as (Toupin 1962) κ ab ( x) = − Da nb = − Db na = κ ba . (5.418) Consider a hyperelastic material of grade two, in which stress and strain energy depend on the total covariant derivative of F in addition to the deformation gradient, reference position of a material particle (in the case of 5
It is assumed in (5.413) and in the remainder of Section 5.7 that a coordinate G
system is chosen such that referential Christoffel symbols vanish, i.e., Γ
..C BA
= 0.
264
5 Thermoelasticity
heterogeneity) and reference basis vectors (in the case of anisotropy). The strain energy density is written in functional form as ρ 0ψ =Ψ 0 =Ψ 0 ( F. Aa , F. Aa:B , X , G A ) . (5.419) By assertion, the balance of mass in (4.10)(4.12) still applies for materials of grade two: ρ0 = ρ J with J = dv / dV = g / G det F from (2.141)(2.142), despite (5.411). On the other hand, stress and traction definitions in Section 4.1.1, linear and angular momentum balances in Section 4.1.3, and the treatment of thermodynamics in Sections 4.1.4 and 4.2 do not generally apply for the theory of elasticity of grade two presented in what follows in the present Section. As was assumed in Section 5.6, in the present Section entropy production and temperature rates are assumed to vanish, and free energy and internal energy are equivalent to the strain energy. Heat conduction, heat sources, and temperature gradients are not considered in the present Section. Furthermore, considered for simplicity in what follows is the quasistatic case, in which velocities and accelerations are omitted. Potential energies from conservative body forces are also omitted for simplicity of presentation, but these forces could be incorporated easily by subtracting the appropriate term from the Lagrangian. Thus, the Lagrangian density function and the Lagrangian functional of (5.394) simply become, respectively, L0 = −Ψ 0 , L = ∫ L0 dV = −E = − ∫Ψ 0 dV = − ∫ ρ 0ψ dV = − ∫ ρψ dv , (5.420) V
V
V
v
since kinetic energy K = 0 and global potential energy Φ = 0 by definition in the present simplified case. The appropriate generalization of Hamilton’s principle (5.380) for elastic materials of grade two (Toupin 1962, 1964) with vanishing inertia is written as follows in the spatial configuration: t2 t2 ⎡ ⎤ ⎡ ⎤ δ A + ∫ ⎢ ∫ ( biδ x ) dv ⎥ dt + ∫ ⎢ ∫ ( t iδ x + hi Dδ x ) ds ⎥ dt = 0 , (5.421) t1 ⎣ v t1 ⎣ s ⎦ ⎦ with h( x, t ) a generalized surface traction introduced as a work conjugate to the normal derivative of the variation of spatial motion at the surface, Dδ x = (δ x a );b nb g a = (δ x a );b nb g a . Body force per unit current volume is written as b ( x, t ) , and t ( x, t ) is a surface traction, i.e., a force vector per unit spatial area. Substituting from (5.420),
5.7 Elasticity of Grade Two t2
t2
⎛
t1
t1
⎝V
265
⎞
δ A = δ ∫ L dt = δ ∫ ⎜ ∫ L0 dV ⎟ dt ⎠
⎛ ⎞ ⎛ ⎞ = − ∫ ⎜ ∫ δΨ 0 dV ⎟ dt = − ∫ ⎜ ∫ δΨ 0 ( J −1dv) ⎟ dt. t1 ⎝ V t1 ⎝ v ⎠ ⎠ t2
t2
Thus the equality − ∫ J −1δΨ 0 dv + ∫ baδ x a dv + ∫ ⎡⎣taδ x a + ha D (δ x a ) ⎤⎦ ds = 0 v
v
(5.422)
(5.423)
s
should hold at any time in (arbitrary) interval t1 ≤ t ≤ t2 . The first integral on the left side of (5.423) can be written using (5.419) as ⎡ ∂Ψ ⎤ ∂Ψ 0 − ∫ J −1δΨ 0 dv = − ∫ J −1 ⎢ a0 δ F. Aa + δ ( F. Aa:B ) ⎥ dv , (5.424) a ∂F. A:B ⎣ ∂F. A ⎦ v v where from (5.376), (5.415), and the product rule, ∂Ψ 0 ∂Ψ J −1 δ F. Aa + J −1 a 0 δ ( F. Aa:B ) ∂F. Aa ∂F. A:B ⎡ ⎡ ⎤ ∂Ψ 0 ⎛ −1 ∂Ψ 0 b ⎞ ⎤ ∂Ψ F. B ⎟ ⎥ δ F. Aa + ⎢ J −1 a 0 F. Bb δ F. Aa ⎥ = ⎢ J −1 −⎜J a a ∂F. A ⎝ ∂F. A:B ∂F. A:B ⎠;b ⎥⎦ ⎣ ⎦ ;b ⎣⎢ ⎡ ∂Ψ 0 ⎛ −1 ∂Ψ 0 b ⎞ ⎤ c = ⎢ J −1 −⎜J F.B ⎟ ⎥ F. A (δ x a );c a a ∂F. A ⎝ ∂F. A:B ⎢⎣ ⎠;b ⎥⎦
(5.425)
⎡ ⎤ ∂Ψ + ⎢ J −1 a 0 F. Bb F. Ac (δ x a );c ⎥ , ∂F. A:B ⎣ ⎦ ;b since by (5.413) and (5.415), ⎡ −1 ∂Ψ 0 b a ⎤ ⎡ ⎤ ∂Ψ ∂Ψ F. Bδ F. A ⎥ = ⎢ J −1 a 0 F.Bb ⎥ δ F. Aa + J −1 a 0 δ ( F. Aa:B ). (5.426) ⎢J a F F F. A:B ∂ ∂ ∂ . A:B . A:B ⎣ ⎦ ;b ⎣ ⎦ ;b G
Noting from (2.145) that ( J −1 F. Aa );a = 0 when Γ
.. B BA
= 0 , the rank two stress
tensor σ ( x, t ) and rank three hyperstress tensor H bdc ( x, t ) are defined, respectively, as ⎡ ⎛ ⎞ ⎤ ∂Ψ ∂Ψ σ dc = g daσ a.c = g da ⎢ J −1 a0 − ⎜ J −1 a 0 F.Bb ⎟ ⎥ F. Ac ∂F. A ⎝ ∂F. A:B ⎢⎣ ⎠;b ⎥⎦ (5.427) ⎡ ⎤ c da −1 ∂Ψ 0 b ⎛ ∂Ψ 0 ⎞ = g J ⎢ a − F.B ⎜ a ⎟ ⎥ F. A , ⎢⎣ ∂F. A ⎝ ∂F. A:B ⎠;b ⎥⎦ dc
266
5 Thermoelasticity
∂Ψ 0 b c ∂Ψ 0 c b F.B F. A = J −1 g da F.B F. A = H cdb . (5.428) a a ∂F. A:B ∂F.B: A In physical components, the stress in (5.427) exhibits dimensions of force per unit spatial area or energy per unit spatial volume, while the hyperstress in (5.428) exhibits dimensions of force per unit spatial length or energy per unit spatial area. The hyperstress consists of up to 18, as opposed to 27, independent entries as a consequence of compatibility conditions F.[aA:B ] = 0 . The stress tensor of (5.427) consists of up to 9 independent enH bdc = g da H ab.c = J −1 g da
tries, and is generally not symmetric, in contrast to the Cauchy stress tensor of classical continuum mechanics defined in Chapter 4. Substituting these stress definitions into (5.425), J −1δΨ 0 = σ a.c (δ x a );c + ⎡⎣ H ab.c (δ x a );c ⎤⎦ ;b (5.429) .c a .c a = (σ a δ x );c − (σ a );c δ x + ⎡⎣ H ab.c (δ x a );c ⎤⎦ . ;b Applying the divergence theorem of (2.193) in spatial coordinates to (5.424) gives
{
}
− ∫ J −1δΨ 0 dv = − ∫ (σ a.cδ x a );c − σ a.c;cδ x a + ⎡⎣ H ab.c (δ x a );c ⎤⎦ dv ;b v
v
= ∫ σ a.c;cδ x a dv − ∫ ⎡⎣σ a.cδ x a + H ab.c (δ x a );b ⎤⎦ nc ds. v
(5.430)
s
Using (5.416)(5.418), Stokes’s theorem (2.198), and integration by parts, the rightmost term in the surface integral in (5.430) can be expressed as follows (Teodosiu 1967a), appealing to the symmetry of H ab.c = H ac.b :
∫H s
b .c a
(δ x a );b nc ds = ∫ H ab.c [ D(δ x a ) nb + Db (δ x a )]nc ds s
= ∫ H n n D(δ x a )ds + ∫ H ab.c (κ .dd nb nc − κ bc )δ x a ds b .c a b c
s
s
− ∫ H ε n ncδ x a dxe b .c a bde
d
c
= ∫ H n n D(δ x a )ds + ∫ H ab.c (κ .dd nb nc − κ bc )δ x a ds b .c a b c
s
s
− ∫ ( H ab.cε bde n d ncδ x a ); g n f ε efg s
= ∫ H n n D(δ x a )ds − ∫ H ab.c (κ .dd nb nc − κ bc )δ x a ds b .c a b c
s
s
− ∫ Db ( H )ncδ x a ds, b .c a
s
(5.431)
5.7 Elasticity of Grade Two
267
where Db ( H ab.c ) = H ab.;.cb − D( H ab.c ) nb = H ab.;.cb − H ab.c ;d nd nb is the surface gradient of the hyperstress, with normal derivative D ( H ab.c ) = H ab;.dc n d . Finally, substituting (5.430) and (5.431) into (5.423) and collecting terms, .c a b .c a ∫ (σ a;c + ba )δ x dv = ∫ ⎡⎣ H a nb nc − ha ⎤⎦ D(δ x )ds v
S
+ ∫ ⎡⎣σ n − H ab.c (κ.dd nb nc − κ bc ) − Db ( H ab.c )nc − ta ⎤⎦ δ x a ds. .c a c
(5.432)
s
Presuming (5.432) must hold for arbitrary variations δ x a and normal surface variations D(δ x a ) , the following equilibrium equations and boundary conditions are obtained: σ a.c;c + ba = 0 , (5.433) ta = σ a.c nc − H ab.c (κ .dd nb nc − κ bc ) − Db ( H ab.c )nc ,
(5.434)
ha = H n n . (5.435) Relation (5.433) is the static balance of linear momentum. Relation (5.434) is the boundary condition for the traction. Relation (5.435) is the boundary condition for the hypertraction. Spatial relations (5.433)(5.435) were first derived by Toupin (1962) using the virtual work procedure outlined above, and were presented later in material coordinates by Toupin (1964). For the particular case when free energy (5.419) does not depend on secondorder position gradient F. Aa:B , i.e., when Ψ 0 =Ψ 0 ( F. Aa , X , G A ) , b .c a b c
stress σ dc becomes identical to the Cauchy stress of classical nonlinear elasticity (e.g., (5.24) and (5.427) become equivalent), and the hyperstress H bdc = 0 in (5.428). Thus, in that particular case, (5.433) becomes equivalent to linear momentum balance (4.17) in the absence of spatial acceleration, boundary condition (5.434) becomes equivalent to Cauchy’s relation (4.3), and the right side of (5.435) vanishes identically. In the general theory, however, i.e., when the free energy depends on F. Aa:B , the stress in (5.427) depends, in part, on the derivative of the free energy with respect to F. Aa:B . Such dependence can be interpreted from (5.411) as resulting from secondorder effects on stretch of interatomic bond vectors (e.g., possibly interpreted as anharmonic or nonlinear effects), thereby influencing interatomic forces and the resulting stress tensor of (5.427), and giving rise to the hyperstress tensor of (5.428). As was the case in Section 5.6, a local balance of angular momentum can be obtained by restricting the strain energy density to be invariant under rigid body rotations of the spatial frame. Consider a finite rotation
268
5 Thermoelasticity
F. Aa → Qˆ .ab F. Ab as discussed in Sections 4.2.1 and 5.6.2. The total covariant derivative transforms in this situation as F. Aa:B → Qˆ.ab F. Ab:B . An infinitesimal rotation is then written in the form Qˆ a = δ a + g Ωˆ ac , where the skew ma.b
.b
bc
ac trix Ωˆ ac = Ωˆ [ ] . According to Toupin (1964), invariance of the strain energy density under infinitesimal rotations is sufficient to ensure invariance under finite rotations. Extending (5.409), the variational change of strain energy under such small rotations is ⎡ ∂Ψ 0 ⎤ ∂Ψ 0 J −1dΨ 0 = J −1 ⎢ F. Ab + F. Ab:B ⎥ dQˆ .ab a e a e ˆ ˆ ∂ (Q.e F. A:B ) ⎢⎣ ∂ (Q.e F. A ) ⎥⎦
⎡ ∂Ψ ⎤ ∂Ψ = J −1 ⎢ a0 F. Ab + a 0 F. Ab:B ⎥ d Ωˆ .ab ∂F. A:B ⎣ ∂F. A ⎦
(5.436)
⎡ ∂Ψ ⎤ ∂Ψ = J −1 ⎢ a0 FbA + a 0 FbA:B ⎥ d Ωˆ ab . ∂F. A:B ⎣ ∂F. A ⎦ Requiring that (5.436) vanish under small but otherwise arbitrary rotations ab d Ωˆ [ ] leads to the local balance of angular momentum for elastic materials of grade two: ⎡ ∂Ψ ⎤ ∂Ψ (5.437) dΨ 0 = 0 → J −1 ⎢ [a0 Fb] A + [a0 Fb] A:B ⎥ = 0 . ∂F. A:B ⎣⎢ ∂F. A ⎦⎥ Components of the secondorder stress tensor in (5.427) can be expressed as (Toupin 1964) ⎡ ∂Ψ ⎛ ∂Ψ ⎞ ⎤ σ a.b = J −1 ⎢ a0 − F.Bc ⎜ a 0 ⎟ ⎥ F. Ab ⎢⎣ ∂F. A ⎝ ∂F. A:B ⎠;c ⎥⎦ = J −1
∂Ψ 0 b ⎛ −1 c ∂Ψ 0 ⎞ b F. A − ⎜ J F.B ⎟ F. A ∂F. Aa ∂F. Aa:B ⎠;c ⎝
= J −1
∂Ψ 0 b ∂Ψ 0 b F. A + J −1 F. Bc F. A;c ∂F. Aa ∂F. Aa:B
⎛ ∂Ψ 0 b ⎞ − ⎜ J −1 F.Bc F. A ⎟ ∂F. Aa:B ⎝ ⎠ ;c
⎡ ∂Ψ ∂Ψ 0 b ⎤ = J −1 ⎢ a0 F. Ab + F. A:B ⎥ − H .ba.;cc . a ∂ F ∂ F . A:B ⎣ .A ⎦ Substituting the antisymmetric part from (5.437) into (5.438), ⎛ ∂Ψ ⎞ ∂Ψ 0 b b [ba ]c [ ab]c abc 0 σ [ab] = J −1 ⎜ F. A] + F. A:]B ⎟ − H ...; c = H ...;c = M ...;c , ⎜ ∂F[ a A ⎟ ∂F[a A:B ⎝ ⎠
(5.438)
(5.439)
5.7 Elasticity of Grade Two
269
where rank three tensor (i.e., thirdorder tensor) of couple stresses M abc and rank two couple stress tensor md.c are constructed from the antisymmetric part of the hyperstress6: 1 ab c M abc = ε abd md.c = H [ ] , md.c = ε dab M abc = ε dab H abc . (5.440) 2 Local angular momentum balance (5.439) becomes 1 σ [ab ] − M ...;abcc = σ [ab] − ε abd md.c;c = 0 ⇔ ε abcσ ab − mc.d;d = 0 . (5.441) 2 The symmetric part of the hyperstress H ( ab )c = H abc − M abc , while not affecting the angular momentum balance (5.441), does not always vanish identically and has been interpreted as resulting from a distribution of selfequilibrating forces (Toupin 1964). A frame indifferent version of strain energy function (5.419) is Ψ 0 =Ψ 0 ( E AB , BABC , X , G A ) , (5.442) where the right CauchyGreen strain 2 E AB = F. Aa g ab F.Bb − GAB as in (2.156), and the covariant strain gradient referred to the reference configuration satisfies 1 BABC = FaA F. Ba:C = (C AB ;C + C AC ; B − CCB ; A ) (5.443) 2 = E AB ;C + E AC ; B − ECB ; A . Clearly, the strain gradient tensor BABC = BA( BC ) , like
F.Bb:C = F.Cb :B , con
tains 18 independent entries. Contravariant hyperstress and stress tensors are then computed, respectively, from the chain rule as follows: ∂Ψ 0 ∂ ( FeC FDe:E ) b c ∂Ψ 0 b d c H bdc = J −1 g da F.B F. A = J −1 F.B F.C F. A , (5.444) ∂BCDE ∂F. Aa:B ∂BCAB
6 The secondorder couple stress defined in (5.440) is consistent with the definition of Toupin (1964) but is the negative transpose of the couple stress defined by Malvern (1969).
270
5 Thermoelasticity
⎡ ∂Ψ
⎛ ∂Ψ ⎞ ⎤ − F.Bb ⎜ a 0 ⎟ ⎥ F. Ac ⎢⎣ ∂F ⎝ ∂F. A:B ⎠;b ⎥⎦ ⎡ ∂Ψ ∂E ⎛ ∂Ψ 0 ∂BCDE ⎞ ⎤ ∂Ψ 0 ∂BCDE CD 0 = g da J −1 F. Ac ⎢ + − F. Bb ⎜ ⎟ ⎥ a a a ⎢⎣ ∂ECD ∂F. A ∂BCDE ∂F. A ⎝ ∂BCDE ∂F. A:B ⎠;b ⎥⎦ (5.445) ⎡ ⎤ ⎛ ⎞ Ψ Ψ Ψ ∂ ∂ ∂ 0 0 0 = g da J −1 F. Ac ⎢ FaC + FaC :B − F.Bb ⎜ FaC ⎟ ⎥ ∂BACB ∂ B ⎢⎣ ∂E AC ⎝ CAB ⎠;b ⎥⎦
σ dc = g da J −1 ⎢
0 a .A
⎡ ∂Ψ ⎛ ∂Ψ 0 ⎞ d ⎛ ∂Ψ 0 ⎞ d ⎤ 0 ⎟ F.C:B ⎥ . = J −1 F. Ac ⎢ F.Cd − F.Bb ⎜ ⎟ F.C + ⎜⎜ ⎟ ∂B ⎢⎣ ∂E AC ⎥⎦ ⎝ ∂BCAB ⎠;b ⎝ [ AC ]B ⎠ Expanding strain energy density (5.442) in a Taylor expansion to second order in strains and strain gradients about a reference state at which F. Aa = g.aA and F. Aa:B = 0 gives 1 ABCD Ψ 0 =Ψ 0 + AB E AB + D ABC BABC + E AB ECD 2 (5.446) 1 + D ABCDEF BABC BDEF + K ABCDE E AB BCDE , 2 where Ψ 0 =Ψ 0 (0,0, X , G A ) is the strain energy density at the reference state, and where constant material coefficients at a material point X are defined as follows: ∂Ψ 0 ∂Ψ 0 ∂ 2Ψ 0 AB = , D ABC = , ABCD = , (5.447) ∂E AB E= 0 ∂BABC E= 0 ∂E AB ∂ECD E = 0 B =0
D ABCDEF =
B =0
∂Ψ0 ∂BABC ∂BDEF 2
, K ABCDE = E=0 B=0
B =0
∂Ψ0 ∂E AB ∂BCDE 2
.
(5.448)
E=0 B=0
As noted by Toupin (1964), a natural state in which both the stress and hyperstress vanish everywhere may not exist for a given material, and such a state may be an exceptional case rather than the norm. None of the constants in (5.447) and (5.448) need vanish in general for an arbitrary (i.e., fully anisotropic) material of grade two. Since choice (5.442) is invariant under spatial rotations, (5.437) and hence angular momentum balance (5.441), are satisfied identically. Linear momentum balance (5.433) provides three equations in three unknowns x a ( X ) , (a = 1, 2,3) , subject to boundary conditions (5.434) and (5.435). The theory of hyperelastic materials of grade two presented heretofore in Section 5.7 is a particular kind of generalized continuum theory with
5.7 Elasticity of Grade Two
271
higherorder stresses (i.e., hyperstresses). More general theories have been formulated accounting for dynamics and deformations of microstructures (i.e., director vectors), as summarized by Toupin (1964). Elastic materials of grade two are a particular class of director theory in which a set of directors at X is constrained to deform in conjunction with material particles (i.e., first and higherorder deformation gradients) at X. More general theories of oriented (micropolar) or micromorphic elastic solids were developed by Cosserat and Cosserat (1909), Ericksen and Truesdell (1958), Toupin (1962, 1964), Mindlin (1964), Eringen and Suhubi (1964), and Eringen (1968), among others. Mindlin (1965) considered elastic bodies whose strain energy density depends on strain and first and second gradients of strain (corresponding to elasticity of grade three in the terminology used in this Chapter), while Green and Rivlin (1964b) considered bodies supporting higherorder stresses work conjugate to velocity gradients of first and arbitrarily higher order. Cosserat and Cosserat (1909) developed a theory of elasticity for a continuum embedded with a triad of rigid directors that may rotate independently of the macroscopic displacement field of material particles, and angular momentum balance (5.441) is often credited to these authors. Eringen (1968) provided some historical references and remarks on early generalized continuum theories. Truesdell and Noll (1965) offered an indepth analysis of director theories and secondgrade elasticity. Green and Naghdi (1995) developed a general procedure for obtaining balance laws for generalized continua using an energy balance, invariance arguments, and thermodynamic principles. Yavari and Marsden (2009) obtained balance laws and constitutive relations for generalized continua (e.g., elastic materials with microstructure) using covariance principles. Recall that in the case of elasticity, (5.1) applies ( F ( X , t ) = F L ( X , t ) ), implying that the (total) covariant derivative of F reflects material gradients of stretch and rotation of interatomic bond vectors among atoms in a crystal structure. The hyperstress—or its antisymmetric part, the couple stress of (5.440)—reflects moments induced by distributions of interatomic forces and interatomic moments corresponding to these gradients of interatomic bond vectors. Physical origins of higherorder stresses in the context of atomistic force or moment interactions were suggested by Kroner (1963b), Mindlin (1964, 1968a, 1972), Zhou and McDowell (2002), and Sunyk and Steinmann (2003). Kroner (1963b) and Bammann (2001) gave arguments supporting the presence of couple stresses resulting from the stress fields of dislocations in crystals. If the viewpoint in (5.411) is adopted, elasticity of grade two can be interpreted as providing additional accuracy over elasticity of grade one in
272
5 Thermoelasticity
terms of description of the kinematics of deformation. This does not imply that the total covariant derivative of F vanishes in elasticity of grade one; rather, this quantity simply does not explicitly enter the thermodynamic potentials in the classical theory. It is noted, however, that series expansion (5.411) is written only to provide physical interpretation of the total covariant derivative of the deformation gradient and does not explicitly enter the subsequent constitutive theory in Section 5.7. Elasticity of grade two also provides a number of other possible advantages over classical nonlinear elasticity. Strain gradient theories enable numerical solution of certain kinds of boundary value problems without mesh sensitivity that may emerge in classical theories (Menzel and Steinmann 2000; Abu AlRub and Voyiadjis 2005). Second and highergrade elasticity provides analytical solutions for stress and strain fields produced by dislocation or disclination lines without singularities in these fields near defect cores (Lazar and Maugin 2004, 2005; Deng et al. 2007). Such singularities inevitably arise in solutions obtained from the classical theory of elasticity of grade one, as exemplified by linear elastic solutions for straight line defects listed in Section C.1 of Appendix C. Drawbacks of secondgrade elasticity, relative to classical elasticity of grade one, are complex hyperelastic constitutive relations (5.427)(5.428) and traction boundary conditions (5.434), boundary conditions for the hyperstress (5.435) that may be difficult to interpret physically, and the large number of material constants arising even in the lowest order (quadratic) approximation of the strain energy in (5.446). The latter point is in contrast to classical nonlinear elasticity of grade one, wherein for the lowest degree of symmetry (e.g., a triclinic crystal structure) only 21 distinct secondorder elastic constants are required. As a counterexample, Mindlin’s geometrically linear theory of elastic materials of grade two with unconstrained microdeformations (Mindlin 1964) requires 903 independent material coefficients to describe a material of maximum anisotropy, following a Taylor series expansion of the strain energy of quadratic accuracy akin to (5.446).
6 Elastoplasticity
Plasticity attributed to dislocation motion in crystals is considered in detail in Chapter 6. In many crystalline solids, large deformations are not sustainable by thermomechanically recoverable deformation alone. Deviatoric elastic deformations generate shear stresses, which, when large enough, facilitate generation and motion of lattice defects. More specifically, ductile crystals tend to exhibit plastic deformation arising from generation and glide of dislocations (e.g., dislocation lines and loops) when subjected to deviatoric stresses exceeding some mechanical threshold, elastic limit, or yield point. Thermally activated dislocation motion (e.g., kink migration) is possible even when resistance in isolated locations (e.g., in the vicinity of obstacles such as heterogeneities) to glide exceeds the magnitude of average resolved stress acting on a glide plane in the slip direction. Thermodynamics and kinetics of dislocationbased plasticity have been studied since the early twentieth century. Fundamental restrictions on plastic work or plastic dissipation in the context of the entropy inequality were posited by Drucker (1951) and Ilyushin (1961). These restrictions were generalized to the case of finite deformations, i.e., geometric nonlinearity, by Lee (1969) and Kratochvil (1971). In the context of crystal plasticity theory, Bishop and Hill (1951) suggested a maximum plastic work postulate for determining active slip systems in crystals subjected to small deformations, while Rice (1971), Hill and Rice (1972, 1973), and Havner (1986) studied aspects of the normality structure of finite deformation inelasticity. Kocks et al. (1975) developed a systematic framework for describing thermodynamics and kinetics of slip across a range of length scales spanning from behaviors of individual dislocation segments to large groups of dislocations represented in slip rate variables of continuum crystal plasticity. Changes in microstructure of crystalline materials occur as lattice defects are generated and propagated, manifesting in changes in the thermodynamic state of the solid. For example, stored energy associated with residual, selfequilibrated stress fields attributed to defects in crystals, often referred to as stored energy of cold working, has been investigated for some time (Farren and Taylor 1925; Taylor and Quinney 1934; Zener
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_6, © Springer Science+Business Media B.V. 2011
273
274
6 Elastoplasticity
1942; Toupin and Rivlin 1960; Wright 1982; Rosakis et al. 2000; Longere and Dragon 2008). This energy is properly reflected in the thermodynamic potentials via prescription of dependence of such potentials on evolving internal state variables representing densities of defects in the solid. In geometrically nonlinear elastoplasticity, a naturally arising conjugate thermodynamic force to the plastic velocity gradient is a variant of the socalled Eshelby stress tensor (Maugin 1994; Svendsen 2001; Clayton et al. 2004b). The divergence of the Eshelby stress is a material force, i.e., an energy gradient, associated with explicit changes in position of heterogeneities, as demonstrated in the context of linear elasticity (Eshelby 1951) and nonlinear elasticity (Eshelby 1975; Epstein and Maugin 1990; Maugin 1994, 1995). Tensors of similar nature but often not identical mathematical form, often referred to as energymomentum tensors or chemical potential tensors depending on context, have been used to describe a number of phenomena in continuum physics (Bowen 1967; Grinfeld 1981, 1991; Hill 1986; Maugin and Epstein 1991; Gurtin 1995; Maugin 1994, 1995; Cermelli and Fried 1997). Chapter 6 is organized as follows. A general formulation of finite deformation elastoplasticity is presented in Section 6.1, following the formalism of the internal state variable framework described in Section 4.2, and in the context of balance laws for classical continua given in Section 4.1. Most aspects of the kinematic and thermodynamic description are now standard in the finite deformation plasticity literature (Lee 1969; Bammann and Aifantis 1987; Lubliner 1990; Scheidler and Wright 2001), with the deformation gradient decomposed into lattice and plastic parts according to (3.31), F = F L F P , and the Helmholtz free energy density dependent upon the stretch associated with the lattice deformation F L , the temperature, and one or more internal state variables accounting for stored energy associated with lattice defects. The formulation presented here differs from many others, however, via its consideration of thermodynamic potentials measured per unit volume in an unstressed intermediate configuration, as opposed to thermodynamic potentials measured per unit mass. This difference turns out to be inconsequential, however, when inelastic deformation is isochoric, as is the case with pure slip as defined by (3.97)(3.100) and demonstrated in (3.121) in the context of crystal plasticity. Specialization of the general formulation to discrete dislocationbased plasticity of Section 3.2.5 and crystal plasticity of Section 3.2.6 then follow in Sections 6.2 and 6.3, respectively. In the former, a vector measure of force per unit length analogous to the PeachKoehler force (Peach and Koehler 1950) emerges as the conjugate force to the velocity of mobile line defects, i.e., glissile dislocation segments. In the latter, the dissipative
6.1 Twoterm Multiplicative Elastoplasticity
275
part of the stress power can be decomposed into a sum of products of slip rates and conjugate shear stresses acting on each glide system. Kinetic equations for inelastic deformation rates (i.e., dislocation velocities and slip rates), both thermodynamically admissible and physically motivated, are discussed, primarily following the scheme of Kocks et al. (1975). A concise summary of general kinetic relations encountered in classical macroscopic plasticity theory is then presented in Section 6.4, wherein the notion of a dissipation potential first introduced in Section 4.3 proves useful. Reduction of the nonlinear theory of elastoplasticity to the geometrically linear case is given in Section 6.5. In the thermodynamic analysis of Section 6.1, a stress tensor similar in appearance to several proposed by Eshelby (Eshelby 1951, 1975) is found to act as a conjugate driving force to the time rate of plastic deformation. This stress quantity is considered in Section 6.6 from the perspective of material forces in continuum elasticity theory. Chapter 6 concludes, in Section 6.7, with an extension of elasticity of grade two of Section 5.7 to the context of multiplicative elastoplasticity. The presentation of Section 6.7 focuses on large elastic deformations from a stationary, but possibly anholonomic, intermediate configuration in the athermal case. Dissipative processes associated with evolution of the intermediate configuration are not explicitly considered, nor are temperature effects. Governing equations and boundary conditions are derived using a variational principle, following Teodosiu (1967a, b). The content of Chapter 6 by no means constitutes a complete treatment of the field of plasticity; entire texts have been devoted to subdisciplines addressed in individual Sections of Chapter 6. A few relevant general references on plasticity theory include books of Hill (1950), Nadai (1950), Schmid and Boas (1950), Lubliner (1990), Khan and Huang (1995), and NematNasser (2004). Texts including treatments of dislocation kinetics and single crystal slip include those of Friedel (1964), Nabarro (1967), Hirth and Lothe (1982), and Havner (1992), and the extensive article of Kocks, Argon, and Ashby (1975).
6.1 Twoterm Multiplicative Elastoplasticity Early investigations (Lee 1969; Teodosiu 1970; Kratochvil 1971) of thermomechanics of crystalline bodies in the context of the twoterm multiplicative decomposition followed a scheme similar to that posited here, apart from the distinction that the present analysis is conducted with energetic
276
6 Elastoplasticity
quantities measured on a perunitvolume basis as opposed to a perunitmass basis. According to (3.31), let F = F L F P , F. Aa = F La.α F Pα. A , (6.1) whereby total deformation gradient F is decomposed multiplicatively into lattice deformation F L and plastic deformation F P , neither of which necessarily satisfies integrability conditions (3.42). Recall from Fig. 3.4 that (6.1) implies the existence of a number of configurations for each material element: reference configuration B0 , intermediate configuration B , and current or spatial configuration B. The intermediate configuration is anholonomic unless conditions (3.42) are satisfied. Terms entering decomposition (6.1) act as mappings between tangent bundles on each configuration, i.e., F : TB0 → TB , F P :TB0 → TB , and F L :TB → TB . The lattice
deformation F L encompasses both mechanical elastic deformation and thermal deformation following the theory of traditional thermoelasticity outlined in Sections 5.15.4; mechanical and thermal origins of lattice deformation are not explicitly delineated in the kinematic description of Chapter 6, in contrast to the treatment of Section 5.5. As illustrated in Fig. 3.5 and discussed at length in Sections 3.2.2, 3.2.5, 3.2.6, and 3.2.7, plastic deformation F P is by definition latticepreserving, meaning that F P does not alter the arrangement of the lattice, such as distances between atoms and angles between atomic bonds; i.e., lattice parameters and bond vectors are not changed by plastic deformation. For example, when F P is attributed to glide of full (as opposed to partial) dislocations and loops, relative tangential displacements of planes of atoms occur in discrete steps corresponding to scalar multiples of the Burgers vector. After the crystal has been affected by F P alone, its shape may have changed (e.g., steps may exist on the surface of a crystal with initially flat faces), but the structure of its interior is assumed to remain unchanged presuming no dislocations remain within its volume. Of course, in real crystals, plastic deformation does not occur in isolation without some accompanying deformation of the lattice F L , so that consideration of F P in isolation is a hypothetical exercise conducted only to lend physical interpretation to (6.1). Because of the latticepreserving property of F P , the kinematic state (i.e., orientation and stretch) of the bulk lattice in intermediate configuration B appears identical to the kinematic state of the bulk lattice in reference configuration B0 . Inverse lattice tangent map
F L −1 :TB → TB returns the crystal from its possibly stretched and rotated condition to the unstressed intermediate configuration. The thermal constituent of F L −1 corresponds to deformation of the crystal from its current
6.1 Twoterm Multiplicative Elastoplasticity
277
temperature to a reference temperature at which the contribution to stress from thermoelastic coupling (i.e., thermal expansion or contraction) vanishes. Viceversa, action of the lattice deformation F L takes the crystal from its evolving unloaded state at a reference temperature to its current stressed and rotated state at the current temperature. Thus, intermediate configuration B serves as an updated reference configuration for the instantaneous thermoelastic response. Hence, a thermodynamic analysis analogous to that performed for elastic bodies in Chapter 5 with reference configuration B0 serving as the reference state for thermoelastic response is conducted in what follows in Chapter 6 for elasticplastic bodies with evolving intermediate configuration B serving as the reference state for thermoelastic response. Following the formulation of Section 5.1 of Chapter 5, the elastic response addressed in Section 6.1 is treated as hyperelastic of grade one, with full account of geometric and material nonlinearities and material anisotropy appropriate to the particular crystal class under consideration. Viscoelastic phenomena are not addressed. 6.1.1 Constitutive Assumptions
A number of variables defined with respect to intermediate configuration B are introduced: ρ = ρ 0 J P −1 = ρ J L , (6.2)
Ψ = ρψ , E = ρ e , N = ρη , 2 Eαβ = Cαβ − gαβ = F L
Σ
αβ
L
Pα .A
Pβ .B
La .α
g ab F
Lb .β
L −1α .a
− gαβ ,
Σ F =J F σ F θ,α = θ , A F P −1.Aα = θ ,a F La.α = ∇αθ ,
=J
P −1
F
AB
L
(6.3)
ab
L −1β .b
(6.4) ,
(6.5) (6.6)
qα = J P −1 F Pα. AQ A = J L F L −1α.a q a . (6.7) Mass density per unit intermediate volume ρ in (6.2) follows from (3.48),
(3.49), and (4.10), noting that J = J L J P . While plastic deformation is usually assumed to be isochoric following arguments that dislocation glide is latticepreserving and hence volume conservative (Sections 3.2.2 and 3.2.5), for illustrative purposes the requirement J P = 1 is not enforced in the present mathematical developments. The Helmholtz free energy Ψ , internal energy E , and specific entropy N are defined on a per unit intermediate configuration volume basis in (6.3). Definitions in (6.4) of symmetric covariant lattice deformation and symmetric lattice strain, both with indices referred to the span of cotangent spaces T * B × T * B , follow
278
6 Elastoplasticity
from (3.52) and (3.65). Relationships among contravariant lattice stress Σ ∈ TB × TB (symmetric automatically by (4.26), (4.27), and (6.5)), second PiolaKirchhoff stress Σ of (4.7), and Cauchy stress σ of (4.3) and (4.6) are analogous to those between the latter two in Table 4.1, but with coordinate transformations conducted here only with respect to either plastic or lattice parts of the total deformation gradient F. The intermediate temperature gradient in (6.6) follows from the definition of the anholonomic partial derivative given in (3.36). The covariant derivative in intermediate coordinates in the last of (6.6) is valid only for a scalar function. In contrast, the covariant derivative of a vector or tensor will depend on the particular definition used for the anholonomic covariant derivative (e.g., see later (6.38)) and may depend on the choice of coordinate basis gα and co..α introduced for configuration B . These coefficients could efficients Γ βχ
be defined as anholonomic transformations from reference or spatial Christoffel symbols, using (3.38) or (3.39), respectively. However, in practice, following discussion in Section 3.2.3 and (3.51), an external Cartesian coordinate frame is usually assigned to B , leading to gαβ = δαβ in ..α = 0 . In the first of (6.7), the heat flux vector Q transforms (6.4) and Γ βχ
from reference to intermediate configuration in a similar manner as in (4.36), and the second of (6.7) then follows automatically from the first of (6.7) and (6.1). ˆ +c, Under rigid body motions of the spatial frame of the form x → Qx ˆ =Q ˆ −T is a rotation matrix and c is a translation vector independwhere Q ent of position, the following transformation laws are assumed to hold, with intermediate and reference configurations held fixed (Bammann and Johnson 1987): ˆ , F L → QF ˆ L , FP → FP , F → QF (6.8) L L P P ˆ and since det Q = 1 , it follows that scalars J → J and J → J . Following from (6.8), variables defined with respect to the intermediate configuration in (6.2)(6.7) all remain invariant under such rigid rotation and translation. Invariance of scalar quantities in (6.2) and (6.3) follows trivially from conservation of mass (i.e., invariance of the reference mass density ρ0 ) and invariance of J P . Invariance of CL and EL follows from direct calculation using the second of (6.8). Invariance of Σ , ∇θ , and q follow, respectively, from invariance of reference quantities Σ , θ, A , and Q entering (6.5)(6.7) (see (4.50)(4.51)) and from invariance of F P in the last of (6.8).
6.1 Twoterm Multiplicative Elastoplasticity
279
Objective forms of constitutive assumptions (4.45)(4.49) are specified as follows for elasticplastic solids: L Ψ =Ψ EL ,α ,θ , ∇θ , X , gα , Ψ =Ψ Eαβ , α , θ , ∇ α θ , X , gα ; (6.9)
( ) ( ) N = N ( E ,α ,θ , ∇θ , X , g ) , N = N ( E ,α ,θ , ∇ θ , X , g ) ; Σ = Σ ( E , α , θ , ∇θ , X , g ) , Σ = Σ ( E , α , θ , ∇ θ , X , g ) ; q = q ( E , α , θ , ∇ θ , X , g ) , q = q ( E , α ,θ , ∇ θ , X , g ) ; α = α ( E , α , θ , ∇ θ , X , g ) , α = α ( E , α ,θ , ∇ θ , X , g ) ; L
L
α
α
L
αβ
αβ
α
L
L
α
α
αβ
α
α
L
αβ
L
αβ L
αβ
α
α
α
(6.10) (6.11)
α
α
(6.12)
α
α
(6.13)
where α ( X , t ) denotes a scalar internal state variable of the sort discussed in Section 4.2.1, accounting for changes in the thermodynamic potentials or response functions of the crystalline solid attributed to sources other than changes in the lattice strain, temperature, and temperature gradient. For simplicity of presentation, only a single scalar internal state variable is considered here, though multiple internal state variables, including scalars and/or vector or tensorvalued internal variables of higher order, can be included without conceptual difficulty, as demonstrated by example later in Chapters 8 and 9. Constitutive assumptions (6.9)(6.12) are analogous to those of thermoelasticity theory in (5.15)(5.18). Dependence of response functions on lattice strain accounts for changes in energy and stress associated with stretching of atomic bonds, for example. The same arguments given in Section 5.1.1 apply here (and in subsequent Chapters 8, 9, and 10) with regards to possible inner displacements that may implicitly affect strain energy in polyatomic crystals: such inner displacements are presumed obtainable (e.g., via energy minimization) when other state variables are prescribed, and hence are not independent state variables (though conceivably, inner displacements could be addressed via internal state variables (Garikipati 2003)). Dependence of response functions on temperature and temperature gradient follows the same arguments given in Section 5.1.1. Dependence of response functions on reference position X of a material particle accounts for heterogeneity (e.g., variations in material properties with position), while dependence on intermediate basis vectors gα is written out explicitly to account for elastic anisotropy that exists in almost all single crystals, following the notational schemes of Chapter 5 and Eringen (1962). Though not explicitly listed in (6.9)(6.13), an additional relationship is usually required to dictate evolution of plastic deformation F P , e.g., a kinetic equation for dislocation velocity, slip system shearing, or deviatoric plastic flow, as discussed in more detail in Sections 6.2, 6.3, and 6.4.
280
6 Elastoplasticity
Notice that no dependence of free energy, entropy, stress, or other response functions upon plastic deformation is prescribed explicitly, i.e., the mapping F P ( X , t ) is not included in the list of independent variables entering (6.9)(6.13). Recall from Chapter 3 that plastic deformation F P represents the shape change of an element of the crystal that has undergone plastic slip. Because F P is latticepreserving, energetic or stress changes directly associated with changes in atomic arrangement (e.g., bond stretching, bond angle changes, and lattice vibrations) by definition are not reflected by F P . Defects such as pinned dislocations may naturally be associated with residual strain energy of the solid and may accumulate with plastic deformation; in such cases, the corresponding change in the local thermodynamic state of the solid is reflected by a change in the local value of internal variable α . For example, consider a ductile crystalline sample that is deformed plastically by F P , and then returned via F P −1 to its original shape. After this cyclic deformation process, the material may have accumulated defects and stored energy (e.g., energy of cold working), but will exhibit null net plastic strain, i.e., F P = 1 at the conclusion of the experiment. In this case, the (null) change in plastic deformation is unable to indicate energetic changes in the crystal, and hence an internal state variable is needed to reflect such changes associated with null net, but nonzero cumulative, plastic strain. In ductile metallic crystals, a typical physically motivated choice of internal variable is the line length per unit volume of dislocations, either scalar or tensor in rank (Kroner 1963a; Teodosiu 1970), though a complete set of internal state variables should logically also include other relevant anomalies in the crystal structure that affect the thermodynamic response functions (Kratochvil 1971, 1972), e.g., densities of point defects, grain and subgrain boundaries, deformation twins, inclusions, voids, microcracks, and so forth. 6.1.2 Thermodynamics
According to (4.71), the entropy production inequality can be written as Σ AB E AB − ρ0 (ψ + ηθ ) − θ −1Q Aθ, A ≥ 0 . (6.14) The stress power per unit reference volume can be written Σ AB E AB = J σ a.b La.b = J P ( J L F L −1.βbσ a.b F La.α )( F L −1α.e Le.d F Ld.β ) (6.15) = J P M α.β Lα.β ,
6.1 Twoterm Multiplicative Elastoplasticity
281
where quantity M , often called the Mandel stress (Mandel 1974), and the velocity gradient pulled back to intermediate configuration B are defined, respectively, by L M α.β = J L F La.α σ a.b F L −1.βb = Cαδ Σ δβ , Lα.β = F L −1α.a La.b F Lb.β , (6.16) L acts as a natural inwhere (6.4) and (6.5) have been used. Notice that Cαδ termediate metric (see Section 3.2.3) for lowering the index of the lattice stress Σ δβ in the definition of the Mandel stress. The quantity M χ.β g αχ is
generally not symmetric in contravariant indices. The total velocity gradient of (3.58) is g
L = ∇ v = FF −1 = F L F L −1 + F L F P F P −1F L −1 ,
(6.17)
leading to (6.18) L = F L −1F L + F P F P −1 . The material time derivative of the free energy per unit intermediate volume is, from (6.2) and (6.3), d Ψ = ( ρψ ) = ρψ + ρψ = J P −1 ρ0ψ − J P J P − 2 ρ0ψ (6.19) dt = ρ (ψ − F .PAα F P −1.Aαψ ) = ρψ −Ψ LPα.α = ρψ −Ψ D Pα.α , via a relation akin to (2.181)1. Substituting (6.2), (6.3), (6.6), (6.7), (6.15), (6.18), and (6.19) into (6.14) and multiplying by J P −1 gives the local entropy production inequality referred to intermediate configuration B :
M α.β Lα.β −Ψ LPα.β δ .αβ −Ψ − Nθ − θ −1qαθ ,α ≥ 0 ,
(6.20)
P −1
is the plastic velocity gradient introduced in (3.58). where L = F F Using (6.16) and (6.18), .β Pα M α.β Lα.β = M α.β F L −1α.a F .La β + M α L .β P
P
.β Pα = ( F L −1δ a F L −1α.a M α.β )( F L bδ F .Lb β ) + M α L .β
(6.21)
L Σ βχ EδβL + M α.β LPα.β = Σ βδ EδβL + M α.β LPα.β , = C L −1δα Cαχ
where gαβ = d (gα ig β ) / dt = 0 has been assumed. From (6.9) with gα = 0 ,
∂Ψ L ∂Ψ ∂Ψ ∂Ψ Eαβ + θ+ γα + α, L ∂θ ∂θ,α ∂α ∂Eαβ where the intermediate rate of temperature gradient satisfies
Ψ =
1
From (2.225),
(6.22)
d (ln J P ) J P 1 ∂J P Pα = P = P F . A = F P −1.Aα F .PAα = LPα.α = D Pα.α . dt J J ∂F P.αA
282
6 Elastoplasticity
dθ,α
d (θ, A F P −1.Aα )
= θ,α + θ, β F P.βA F .Pα−1 A = θ,α − θ, β LP.βα . (6.23) dt dt Using (6.21) and (6.22) in (6.20), the local dissipation inequality becomes ⎛ αβ ∂Ψ ⎞ L ⎛ ∂Ψ ⎞ ∂Ψ Σ − L ⎟ Eαβ − ⎜ N + γα ⎟θ − ⎜⎜ ⎟ ∂θ ⎠ ∂θ ,α ∂Eαβ ⎠ ⎝ ⎝ (6.24) ∂Ψ + M α.β −Ψδ .αβ LPα.β − α − θ −1qαθ,α ≥ 0. ∂α
γα =
=
(
)
Extending the logic of Section 5.1.2, coefficients of rates E L , θ , and γ should vanish identically to ensure thermodynamic admissibility, presuming such rates can be prescribed independently of each other and their coefficients in a thermodynamic process. Constitutive relations ∂Ψ ∂Ψ ∂Ψ (6.25) Σ = L = ΣT , N = − =0 , ∂E ∂θ ∂(∇θ ) are then deduced immediately from (6.24). Hence, it follows that free energy, entropy, and stress do not depend explicitly on temperature gradient: Ψ = Ψ E L , α , θ , X , g α , N = N E L , α ,θ , X , gα , (6.26) Σ = Σ EL ,α ,θ , X , gα .
(
(
)
(
)
)
Cauchy stress and specific entropy per unit mass are found, respectively, from (6.5) and (6.3): ∂Ψ ∂Ψ 1 ∂Ψ σ ab = J L −1 F L.aα L F Lb.β = J L −1 F Lb.β L F La.α = σ ba , η = − . (6.27) ρ ∂θ ∂Eαβ ∂Eβα L L identically by definition (6.4), Σ αβ = Σ βα as in (6.25), Since Eαβ = Eβα
and σ ab = σ ba as indicated in (6.27). Thus the Cauchy stress is consistently symmetric, and angular momentum balance (4.26) holds identically. L L Using the chain rule and the functional dependency Cαβ = Cαβ ( F La.α , g ab ) ,
∂Ψ ∂Ψ ∂Cαβ ∂Ψ Lb =2 L = F La.α (6.28) F .β , L ∂g ab ∂Eαβ ∂Cαβ ∂g ab a relationship similar to DoyleEricksen formula (5.36) of nonlinear hyperelasticity emerges: L
2
6.1 Twoterm Multiplicative Elastoplasticity
283
⎡ ∂ ( J −1Ψ 0 ) ⎤ ⎡ ∂ ( J L −1 ) ⎤ ∂Ψ 2 = 2⎢ − ⎥ ⎢Ψ ⎥ ∂g ab ∂g ab ⎦ ⎣ ∂g ab ⎦ ⎣ ⎡ ⎡ ∂ ( J L −1 ) ⎤ ∂Ψ 0 ∂J −1 ⎤ = 2 ⎢ J −1 +Ψ 0 ⎥ − 2 ⎢Ψ ⎥ ∂g ab ∂g ab ⎦ ∂g ab ⎦ ⎣ ⎣
σ ab = 2 J L −1
= 2 J −1
∂Ψ 0 ∂g −Ψ 0 J −2 −1 gG det( F. Aa ) ∂g ab ∂g ab +Ψ J L − 2 −1 gg det( F L.aα )
= 2 J −1
∂g ∂g ab
(6.29)
∂Ψ 0 −Ψ 0 J −2 g / G det( F. Aa ) g ab ∂g ab +Ψ J L − 2 g / g det( F La.α ) g ab
= 2 J −1
∂Ψ 0 − J −1Ψ 0 g ab + J L −1Ψ g ab ∂g ab
∂ψ ∂ψ = 2ρ , ∂g ab ∂g ab where (2.142)(2.144), (3.48), (4.8), (4.9), and (6.3) have been used. A particular version of (6.29) with det( g ab ) = g = constant was derived by Clayton et al. (2004b). A number of other relations for stresses can be derived using the chain rule in a similar manner2. Table 4.1 provides some requisite identities. = 2 J −1 ρ 0
Because F L = FF P −1 , Ψ (EL , α ,θ , X , gα ) = J P −1Ψ 0 (F L (F, F P , g ), α ,θ , X , gα ) . Holding (α ,θ , X , g ab , gα ) fixed, first PiolaKirchhoff and Mandel stresses satisfy 2
∂Ψ 0 ∂F. Aa
= FP
L Lb ∂( J PΨ ) ∂Eαβ ∂F . χ L ∂F Lb. χ ∂F. Aa ∂Eαβ
=J Σ P
αχ
= FaB Σ ∂Ψ 0 ∂F Pα. A
= F
=
L bα
F F
BA
∂Ψ 0 ∂F Pα. A
P −1B .χ
= FP
∂ ( F.Bb F P −1.Bχ ) 1 P αβ χ L J Σ (δ .β Fbα + δ .αχ FbLβ ) 2 ∂F. Aa
δ δ = J F (J b A .a . B
P
L aα
P −1
F
Pα .B
Σ
BC
F
Pχ .C
)F
FP
P −1 A .χ
=P , .A a
+ FL
∂Ψ 0 ∂F La.β
∂F L.aβ FP
∂F Pα. A
= JP F
L La ∂Ψ ∂Eχδ ∂F .β L ∂F La.β ∂F Pα. A ∂Eχδ
P −1B .β Pα .A
∂F 1 P χδ β L J Σ (δ .δ Faχ + δ .βχ FaLδ ) F.Ba 2 ∂F
L = − J P Cαχ Σ χβ F P −1.Aβ = − J P M α.β F P −1.Aβ .
F
= − J P FaLχ Σ χβ F.Ba F P −1.Bα F P −1.Aβ
284
6 Elastoplasticity
Dissipation associated with conduction can be made nonnegative upon assuming a Fouriertype conduction law analogous to (5.48), but couched here in the intermediate configuration: q = −K∇θ , qα = − K αβ θ , β = − K αβ θ,b F Lb.β = − K αβ θ, B F P.Bβ , (6.30) with K a symmetric positive semidefinite matrix of thermal conductivity that, like K of (5.48), may generally depend on temperature and other state variables: (6.31) −θ −1 ∇θ , q = θ −1 ∇θ , K∇θ ≥ 0 . The dissipation inequality consists of the remaining terms in (6.24): ∂Ψ α + θ −1 ∇θ , K∇θ ≥ 0 , Π : LP − (6.32) ∂α where (6.33) Π = M −Ψ 1 , Π α.β = M α.β −Ψδα.β . Stress measure Π , as discussed in detail in Section 6.6, is closely related to a quantity introduced by Eshelby (1951, 1975) whose divergence represents a kind of force on arbitrary heterogeneities in elastic solids3. The quantity W P = Π : LP = Π α.β LPα.β is often referred to as the plastic dissipation or the rate of plastic work. When the material is plastically incompressible—which is always true for latticepreserving plastic deformation manifesting only from dislocation glide—conditions J P = 1 and tr(LP ) = 0 hold and the plastic dissipation reduces to W P = M : LP . Variants of stress Π have been used by a number of authors as a conjugate thermodynamic force to plastic velocity gradient LP (Maugin 1994; Le and Stumpf 1996b, c; Clayton et al. 2004b, 2006; Clayton 2009a). Use of Mandel stress M in a similar capacity is also widespread (Moran et al. 1990; Maugin and Epstein 1998; Regueiro et al. 2002). Since Σ is symmetric, from (6.16), L Pα W P = Π α.β LPα.β = M α.β LPα.β −Ψ LPα.α = Σ βδ Cαδ L .β −Ψ LPα.α (6.34) L L = Σ βδ Cαδ D Pα.β + Σ βδ Cαδ W Pα.β −Ψ J P J P −1 , P P P where plastic spin WαβP = W[αβ ] and plastic deformation rate Dαβ = D(αβ ) re
ferred to the intermediate configuration are introduced in (3.62) and (3.63). 3 Precisely, Π is a negative pushforward to configuration B of one of several socalled energymomentum tensors introduced by Eshelby (1975). The sign convention used in (6.33) enables both the stress and plastic velocity gradient to share the same (positive) algebraic sign in (6.32) and follows the convention of Epstein and Maugin (1990) and Clayton et al. (2004b, 2006).
6.1 Twoterm Multiplicative Elastoplasticity
285
As is evident from (6.34), only the symmetric part of CL LP contributes to W P , but both plastic deformation rate DP and plastic spin W P can contribute to W P . In particular, CL W P is not generally antisymmetric. Inequality (6.32) indicates that, in the absence of heat conduction, plastic dissipation should exceed the rate of increase in free energy associated with time rate(s) of internal state variable(s). In crystalline solids such as metals and ceramics, free energy changes attributed to internal state variables are often associated with changes in cumulative defect densities, e.g., energetic changes associated with local residual stresses in the vicinity of dislocation lines and internal boundaries such as grain, subgrain, and twin boundaries (Kocks et al. 1975). The specific heat at constant elastic strain and constant internal variable α , measured as energy per degree per unit intermediate volume, is introduced as ⎡ ∂E ⎤ ⎡ ∂N ⎤ ⎡ ∂E ∂θ ⎛ ∂Ψ ⎞ ⎤ ⎡ ∂ 2Ψ ⎤ ∂ 2Ψ , (6.35) θ C= N = ⎢ ⎥ ⎢ ⎥ = ⎢θ + + − = − ⎜ ⎟⎥ ⎢ ⎥ ∂θ EL ⎣ ∂N ⎦ ⎣ ∂θ ⎦ ⎣ ∂θ ⎠ ⎦ ⎣ ∂θ 2 ⎦ ∂θ 2 ∂N ⎝ α
where (6.3) and (6.25) have been used. Multiplying (4.39) by J P −1 , the energy balance in configuration B is
ρ e = E − ρ e = E − J P −1 ρ0 e = E + J P J P −1 E = M α.β Lα.β − J P −1Q;AA + ρ r . (6.36) Substituting from the second of (6.25) leads to
E =Ψ + θ N + θ N =
∂Ψ L ∂Ψ α + θ N = M α.β Lα.β − LP.αα E − ∇α qα + ρ r , Eαβ + L ∂α ∂Eαβ
(6.37)
where, for the heat conduction term, the anholonomic covariant derivative is defined by (Clayton 2009a) ∇α ( . ) = ( . ): A F P −1.Aα + J P −1 ( . )( J P F P −1.Aα ) : A , (6.38) such that J P −1Q;AA = J P −1 ( J P F P −1.Aα qα ); A (6.39) = ( qα ): A F P −1.Aα + J P −1qα ( J P F P −1.Aα ): A = ∇α qα . The term ( J P F P −1.Aα ): A = 0 by Piola’s identity akin to (2.146) in general only when the plastic deformation gradient satisfies compatibility conditions F Pα.[ A:B ] = 0 . Rearranging (6.37) for the rate of entropy production and using (6.25),
286
6 Elastoplasticity
θ N = M α.β Lα.β −
( = (M
∂Ψ L ∂Ψ α − LP.αα E − ∇α qα + ρ r Eαβ − L ∂α ∂Eαβ
)
(
)
= M α. β − Eδ .αβ LPα. β − ∂Ψ / ∂α α − ∇α qα + ρ r .β α
)
(
)
−Ψδ .αβ − θ N δ .αβ LP α. β − ∂Ψ / ∂α α − ∇α qα + ρ r
⎛ = ⎜ Π α. β + δ .αβ θ ⎝ Analogously to (5.50), d ⎛ ∂Ψ θ N = −θ ⎜ dt ⎝ ∂θ
(6.40)
∂Ψ ⎞ P α ∂Ψ α − ∇ α qα + ρ r . ⎟ L .β − ∂θ ⎠ ∂α
⎛ ∂ 2Ψ ⎞ ∂ 2Ψ ∂ 2Ψ ⎞ L θ θ α⎟ E = − + + ⎜ ⎟ αβ L ⎜ ∂θ 2 ∂θ∂α ⎟⎠ ∂θ∂Eαβ ⎠ ⎝ (6.41) 2 Ψ ∂ L α, = Cθ + θβ αβ Eαβ −θ ∂θ∂α with stresstemperature coefficients referred to intermediate configuration ∂ 2Ψ β=− . (6.42) ∂θ∂EL α Equating (6.40) and (6.41) and using (6.30), the temperature rate becomes ⎛ ∂Ψ ⎞ Pα ⎛ ∂Ψ ∂ 2Ψ ⎞ Cθ = ⎜ Π α.β + δ .αβ θ ⎟ L .β − ⎜ −θ ⎟α ∂θ ⎠ ∂θ∂α ⎠ (6.43) ⎝ ⎝ ∂α L − θβ αβ Eαβ + ∇α ( K αβ θ, β ) + ρ r.
The first term on the right side of (6.43) represents the effect of the plastic velocity gradient on the rate of temperature increase. It can be written ⎛ .β ⎞ ⎛ ∂Ψ ⎞ Pα β ∂Ψ θ ⎟ LPα.β = Σ βδ CαδL LPα.β − ⎜Ψ + θ ⎜ Π α + δ .α ⎟ L .α ∂θ ⎠ ∂θ ⎠ ⎝ ⎝ (6.44) P θ Ψ Ψ J ∂ ∂ . J P =W P + P =W P + P J ∂θ J ∂ ln θ From the symmetry of Σ , again only the symmetric part of the covariant product CL LP contributes to plastic dissipation W P and hence the temperature change. From (6.32)(6.34) and (6.43), when plastic deformation is not isochoric, the absolute value of free energy Ψ enters the entropy inequality and energy balance. Thus, the zero datum used to define free energy and other thermodynamic potentials is not inconsequential; e.g., the free energy in this case is not arbitrary to within an additive constant. Notice that when the plastic deformation is isochoric, J P = 0 and the temperature rate equation becomes
6.1 Twoterm Multiplicative Elastoplasticity
287
⎛ ∂Ψ ∂ 2Ψ ⎞ αβ L αβ Cθ = W P − ⎜ (6.45) −θ ⎟ α − θβ Eαβ + ∇α ( K θ , β ) + ρ r. α θ α ∂ ∂ ∂ ⎝ ⎠ The first term on the right of (6.45), i.e., the rate of plastic work, accounts for dissipation from moving dislocations such as that resulting from lattice friction. The second term on the right of (6.45) represents energetic changes attributed to the rate of change of the internal state variable, for example residual elastic energy accumulation with increases in defect density. The third term represents effects of thermoelastic coupling. The final two terms on the right of (6.45) account for heat conduction (i.e., temperature gradients) and nonmechanical heat sources such as a radiation field, respectively. Energy balance (6.45) is often written as follows for ductile crystalline metals: L Cθ = β ′W P − θβ αβ Eαβ + ∇α ( K αβ θ, β ) + ρ r ,
(6.46)
where
⎛ ∂Ψ ∂ 2Ψ ⎞ −θ ⎟α . ∂θ∂α ⎠ ⎝ ∂α
β ′W P = W P − ⎜
(6.47)
Scalar β ′ is often called the TaylorQuinney parameter. The product (1 − β ′)W P measures the rate of energy accumulation in the solid associated with irreversible changes in its internal structure, for example stored energy of cold working. Following measurements of β ′ on several engineering metals subjected to large deformations (Farren and Taylor 1925; Taylor and Quinney 1934; Havner 1992), analysts often assume a constant value of β ′ in the range 0.8 ≤ β ′ ≤ 1.0 (Bammann et al. 1993; Zhou et al. 1994), though more recent experiments (Rosakis et al. 2000) indicate that for some metallic materials β ′ may fall outside this range and may change significantly with history of plastic deformation. When ∂ 2Ψ /(∂θ∂α ) = 0 , (6.32) requires β ′ ≥ 0 in the absence of heat conduction, i.e., for an adiabatic process. However, if the energetic change associated with the rate of an internal state variable is dissipative, for example if condition ∂Ψ / ∂α < 0 holds over some regime in which α > 0 , thermodynamic admissibility does not preclude β ′ > 1 .
288
6 Elastoplasticity
6.1.3 Representative Free Energy
A specific form of the Helmholtz free energy potential of (6.9) and (6.26) for finite elastoplasticity is now considered. For describing crystalline materials in structural applications, the free energy density is often decomposed additively into a thermoelastic part Ψ E associated with reversible deformations and temperature changes and a residual part Ψ R associated with the internal state variable: (6.48) Ψ =Ψ E EL ,θ , X , gα +Ψ R (α ,θ , X , gα ) .
(
)
The additive decoupling of reversible thermoelastic and residual free energies as depicted in (6.48) is common (Bammann 2001; Regueiro et al. 2002; McDowell 2005), though may not always be a physically realistic assumption if free energies associated with the internal state variable (i.e., defect energies) are amplified by external stress fields (Gibeling and Nix 1980; Clayton et al. 2004a; Chung and Clayton 2007), or if elastic moduli are strongly affected by the evolving defect density represented by the internal state variable (Smith 1953; Clayton and Chung 2006). A more general formulation for elasticplastic crystals with residual elastic strains and residual stresses, posited in Section 9.4.6 of Chapter 9, addresses these issues. Furthermore, as demonstrated in Section 9.2 of Chapter 9, when defects such as interstitials, vacancies, pores, voids, or microcracks affect the instantaneous thermoelestic response, internal variables associated with defects should reflect elastic stiffness variations, and hence cannot be decoupled from the lattice strain in the free energy (Mackenzie 1950; Dienes 1952; Grinfeld and Wright 2004; Clayton 2008; Clayton et al. 2008a). The thermoelastic part of the free energy, Ψ E , is often defined in a similar manner to the corresponding potential Ψ 0 in classical thermoelasticity of Sections 5.1.3 and 5.1.4, but with quantities defined in the intermediate as opposed to the reference configuration, with total strain E replaced by lattice strain E L , and with second PiolaKirchhoff stress Σ replaced by symmetric lattice stress Σ . For example, consider a series expansion of the thermoelastic part free energy density of up to third order in lattice strains (Havner 1973) about a possibly evolving intermediate state—a state that serves as an updated reference configuration for the thermoelastic response—but otherwise analogous to materially linear thermoelasticity of (5.84):
6.1 Twoterm Multiplicative Elastoplasticity
ΨE=
1 2
αβχδ
L L Eαβ Eχδ +
1 6
αβχδεφ
L L Eαβ Eχδ EεφL
(6.49)
θ − β Eαβ ∆θ − Cθ ln . θ0 αβ
289
L
The state about which (6.49) is expanded is characterized by conditions L L F La.α = g.aα , Cαβ = gαβ , Eαβ = 0 , and θ = θ 0 > 0 . Temperature change from this reference state ∆θ = θ − θ 0 can be positive, zero, or negative. Material constants referred to configuration B are defined at a material point X with stationary basis gα ( X ) by αβχδ
=
∂ 2Ψ E L L ∂Eαβ ∂Eχδ
β αβ = −
αβχδεφ
,
=
EL = 0 θ =θ 0
∂ 2Ψ E L ∂θ∂Eαβ
∂ 3Ψ E L L ∂Eαβ ∂Eχδ ∂EεφL
,
(6.50)
EL = 0 θ =θ0
⎛ ∂ 2Ψ E ⎞ . , C = − ⎜θ 2 ⎟ ⎝ ∂θ ⎠ EL =0 EL = 0
(6.51)
θ =θ 0
θ =θ0
In (6.51), the thermal stress coefficients and specific heat are constant versions of quantities first introduced in (6.42) and (6.35), respectively. Isothermal second and thirdorder elastic constants are introduced in (6.50), the latter important in structural or shock physics applications wherein confining pressures and elastic strains can be large, especially in certain kinds of crystals (e.g., those with covalent and ionic bonding such as ceramics) wherein resistance to dislocationmediated plastic slip can be high. Material coefficients in (6.50) and (6.51) are related to those of (5.66) and (5.85) at the same material point X as follows: αβχδ = J P −1 ABCD g.αA g.βB g.χC g.δD , (6.52) αβχδεφ
= J P −1
β
αβ
ABCDEF
β
=J
P −1
C = ρc = J
P −1
g.αA g.βB g.χC g.δD g.εE g.φF , AB
α
β
g. A g. B ,
ρ0 c = J
P −1
C0 .
(6.53) (6.54) (6.55)
Since gα = 0 and G A = 0 (e.g., see discussion in Section 2.5.1), the shifter
g.αA = gα , G A at X does not depend on time. When plastic deformation is isochoric ( J P = 1 ) and when coincident coordinate systems are used in reference and intermediate configurations so that g.αA = δ .αA , numerical values of material coefficients on left and right sides of each of (6.52)(6.55)
290
6 Elastoplasticity
are equal4. Hence, all considerations regarding symmetry of reference material coefficients discussed in Section 5.1.5 and Appendix A apply for intermediate elasticity tensors in (6.52) and (6.53) and thermal stress coefficients in (6.54). To convert symmetry relations in Section 5.1.5 and Appendix A to the present context, reference indices in capital Roman font are merely replaced with intermediate indices in Greek font. The thermostatic formalism of Section 5.2 can be applied as well, wherein partial derivatives are taken with respect to lattice strains as opposed to total strains. This enables definitions of isentropic material coefficients, Gruneisen parameters, and Maxwell relations among thermostatic variables. Details of such an approach are given by Scheidler and Wright (2001) and Wright (2002). Like the elastic constants, thermal stress coefficients and specific heat in (6.51) are assumed constant and not dependent upon internal variables representing defect densities, for example. This assumption is standard in plasticity theories, but may not always be physically appropriate since dislocations can affect the specific heat capacity (Gottstein 1973). Stressstraintemperature relations following from (6.25) and (6.49) exhibit the form 1 αβχδεφ L L Σ αβ = αβχδ EχδL + Eχδ Eεφ − β αβ ∆θ . (6.56) 2 L Consider a stressfree thermal strain of the form Eαβ = ααβ ∆θ , where ααβ
may generally depend on the thermodynamic state. Setting the left side of (6.56) to zero gives, analogously to (5.161), β αβ = αβχδ α χδ + αβχδεφ α χδ α εφ ∆θ / 2 = αβχδ α χδ θ , (6.57)
(
)
θ0
0
with ααβ a symmetric rank two tensor of thermal expansion coefficients. For the case of thermoelastic isotropy, secondorder thermoelastic constants become αβχδ (6.58) = µ ( g αχ g βδ + g αδ g χβ ) + λ g αβ g χδ , β αβ = β g αβ , with µ the shear modulus, λ Lamé’s constant, and β a thermal stress constant, identical to those entering (5.124) when J P = 1 . Stressstraintemperature relations for thermoelastically isotropic solids are, when thirdorder elastic constants are omitted, When J P ( X , t ) ≠ 0 , then coefficients on both sides of (6.52)(6.55) cannot all be constant. If the left sides are taken as constant in time, then the elastic coefficients and specific heat per unit reference volume on the right sides increase with increases in plastic volume change. This issue is taken up again in Chapter 8 wherein residual volume changes are incorporated explicitly in the constitutive model framework. 4
6.1 Twoterm Multiplicative Elastoplasticity
Σ αβ = 2 µ E Lαβ + (λ E .Lχχ − β∆θ ) g αβ .
291
(6.59)
The form of the residual free energy Ψ R introduced in (6.48) depends upon the specific choice of internal state variable, and is thus materialspecific. A quadratic function akin to the first term in the thermoelastic potential Ψ E is simple and logical in many instances: 1 Ψ R = κα 2 , (6.60) 2 where material coefficient κ may generally depend on temperature, reference position, and orientation of the material element: ∂ 2Ψ R κ (θ , X , gα ) = . (6.61) ∂α 2 α = 0
Relations (6.32) and (6.60) yield a thermodynamic force linear in the internal state variable conjugate to the time rate of the internal state variable, i.e., −∂Ψ / ∂α = −κα . When κ > 0 , residual free energy (6.60) is a convex function of internal state variable α . However, for a material whose total free energy consists of contributions from multiple sources—e.g., lattice strains, temperature, and one or more internal state variables representing irreversible lattice rearrangements—the global free energy may not be convex with regards to distributions of field variables (Carstensen et al. 2002; Clayton et al. 2006). In such cases, even when a crystal with uniform initial properties is subjected to affine farfield boundary conditions, heterogeneous distributions of field variables such as localized deformation gradients can emerge as the thermodynamic state of the deforming crystal evolves towards a condition of minimum global energy (Ball and James 1987; Bhattacharya 1991; Ortiz and Repetto 1999). Formation of heterogeneous deformation patterns is expected in anisotropic crystals that favor single slip as a result of strong latent hardening (Conti and Ortiz 2005), i.e., strong hardening on slip systems that are noncoplanar with an active system (see Section 6.3 and (6.110)). The theoretical description of material behavior is completed via prescription of kinetic laws for evolution of inelastic deformation, i.e., F P , and rate of internal state variable, i.e., α . Ideally, such kinetic relations should be formulated in such a way that (6.32) is satisfied unequivocally. Such kinetic equations, along with physically descriptive choices of internal state variables, are described in Sections 6.2, 6.3, and 6.4 in the context of discrete dislocation plasticity, crystal plasticity, and macroscopic plasticity, respectively.
292
6 Elastoplasticity
6.2 Dislocation Plasticity Consider a kinematic description further refined to account for motion of discrete dislocation lines as developed in Section 3.2.5. Plastic velocity gradient LP can in this case be expressed by combining (3.98) and the last of (3.99): j
LPα.β = F .PAα F P −1.Aβ = ς αχδ ε χδβ = ∑ ρ i b iα ξ i χ v iδ ε χδβ .
(6.62)
i =1
Summation proceeds over i = 1, 2,... j populations of dislocations with the same tangent line, Burgers vector, and velocity for each value of i; nomenclature entering (6.62) is explained more thoroughly in Section 3.2.5. The plastic dissipation per unit intermediate volume, W P = Π : LP of (6.34), is j
j
i =1
i =1
Π α.β LPα.β = ∑ ρ i v iδ ε χδβ ξ iχ M αβ.b iα − ∑ ρ iΨ b iβ ε βχδ ξ iχ v iδ j
= ∑ ρ i v iδ ε χδβ ξ i χ ( J L F L −1.βbσ a.b F La.α ) F L −1α.c bic i =1 j
= ∑ ρ v ε χδβ ξ ( J F i iδ
i =1
iχ
L
j
(6.63)
σ )b = ∑ ρ v ε χδβ ξ S.a b
L −1β .b
.b a
ia
i iδ
iχ
β
ia
i =1
j
j
i =1
i =1
= −∑ ρ i (ε δχβ ξ iχ S.βa bia )v iδ = ∑ ρ i fδi v iδ , where since the Burgers vector and normal to the glide plane are always orthogonal, b i β ε βχδ ξ i χ v iδ = 0 . The thermodynamic force, with dimensions of force per unit length, acting on dislocation population i is f i = −ξ i × Sbi , β
where the twopoint nominal lattice stress S.a = J F L
(6.64)
σ . Force f i
L −1β .b
.b a
conjugate to dislocation line velocity v i is similar in nature to the force acting on a single dislocation line by an external, as opposed to selfinduced, stress field in a linear elastic body: i fPK = −ξ i × σb i , (6.65) i is known as the PeachKoehler force (Peach and Koehler The vector fPK 1950; Mura 1968; Zorski 1981; Bammann and Aifantis 1982) acting on dislocation type i with unit tangent ξ i and Burgers vector bi . The PeachKoehler force is the force conjugate entering the expression for the negative energy gradient −∂W / ∂s attributed to rigidly translating the dislocation line along trajectory λds = ds (Peach and Koehler 1950):
6.2 Dislocation Plasticity
293
∂W = − ∫ baσ abε bcd λ c dξ d = − ∫ ε dbcξ d σ ba ba λ c dL = ∫ ( f PK )c λ c dL , (6.66) ∂s L L L where dξ = ξdL is a segment of the dislocation line. In the limit of small −
i elastic deformations, S.βa ≈ g.βb σ a.b , ξ i χ ≈ g.χa ξ ia , and ( f i )α ≈ g.aα ( f PK )a . In physical descriptions of dislocation kinetics, use of Orowan’s (1940) relation in (3.100) is often preferred over (6.62): (6.67) LPα.β = ∑ ρ i b i v i s iα mβi , i
where for each slip system i, the magnitude of Burgers vector, direction of atomic motion, dislocation line velocity, and normal to the glide plane, are respectively b i = bi  , s i = b i / b i , v i = v i  , m i = ξ i × v i / v i . (6.68) Using (6.67) in (6.34), the rate of plastic work per intermediate volume is Π α.β LPα.β = ∑ ρ i b i v i s iα M αβ.mβi − ∑ ρ i b i v iΨ ( s iα δαβ. mβi ) i
i
= ∑ ρ b v s (J F i
i i iα
L
La .α
σ F L −1.βb )mβi .b a
(6.69)
i
= ∑ ρ i b i v i ( J L sai σ ab mbi ) = ∑ ρ i b i v iτ i , i
i
where the resolved shear stress (more precisely, a resolved lattice Kirchhoff stress) is τ i = J L sai σ ab mbi = J L sai σ ba mbi = J Lσ ab s(ia mbi ) , (6.70) the latter two relations following from the symmetry of the Cauchy stress. The kinetic relationship between the velocity of a dislocation v i and its driving stress τ i depends upon the thermodynamic state of the crystal, as represented here by lattice strain, temperature, and internal state variable α reflecting contributions from internal structure such as defects or obstacles to dislocation motion. In the remainder of Section 6.2, index i is often dropped, with a focus on kinetic relations for the velocity magnitude v of a representative dislocation or set of dislocations on that system subjected to shear stress magnitude τ . Both v and τ are assumed to exhibit the same (positive) algebraic sign in this context. Though supersonic dislocation motion has been posited (Hirth and Lothe 1982) and may be sustainable if a dislocation is nucleated supersonically at a stress concentration in a crystal subjected to very high applied shear stress (Gumbsch and Gao 1999), conventionally the dislocation velocity is assumed to be bounded from above by the speed of transverse elastic waves in the crystal (Eshelby 1949a; Johnston and Gilman 1959). In anisotropic crystals, elastic plane waves can propagate in a given direc
294
6 Elastoplasticity
tion in three distinct, mutually orthogonal modes when no degeneracy occurs (Brugger 1965); these modes are in general neither longitudinal nor transverse. Special directions exist in crystals allowing for propagation of one longitudinal and two transverse modes. These directions, and speeds of propagation of plane waves, depend upon secondorder elastic constants in initially unstressed crystals, as listed by Brugger (1965). In the isotropic approximation, the elastic shear wave speed cS is
cS = µ / ρ0 ,
(6.71)
with µ the isentropic shear modulus and ρ0 the reference mass density. The maximum sustainable shear stress is the theoretical strength τ T of the crystal of Section C.4.1 (Frenkel 1926); when subjected to stresses of this magnitude, all atomic bonds spanning two crystallographic planes undergoing relative shear are broken simultaneously. In an isotropic linear elastic body, the theoretical strength is approximated by (C.209) as τ T ≈ µ /10 . Thus, upper bounds on dislocation velocity and resolved shear stress are v ≤ cS = µ / ρ0 , τ ≤ τ T ≈ µ /10 . (6.72) Denote the resistance to motion of dislocation population i by the shear stress (6.73) τˆi = τˆi EL ,α ,θ , X , gα ,
(
)
with τˆ ≥ 0 denoting a characteristic magnitude of dislocation line resistance to motion, sometimes called a mechanical threshold stress. Steady state dislocation glide can be achieved when the resolved shear stress τ greatly exceeds threshold stress τˆ , but when the dislocation velocity remains appreciably lower than cS . In this case, the following kinetic relation applies (Kocks et al. 1975): (6.74) (τ − τˆ)b = Β v , where Β is the drag coefficient that depends on lattice friction (e.g., the Peierls mechanism of Section C.4.3), phonon drag, and at very low temperatures, electron drag (Kocks et al. 1975). Kocks et al. (1975) define an atomic frequency ω A = cS / b , (6.75) and the drag coefficient as k θ k θ b k θ b ρ0 , (6.76) Β= B = B = B Ω0 ω AΩ0 cS Ω0 µ where k B is Boltzmann’s constant and Ω0 is the atomic volume introduced in Section 3.1.1. The drag coefficient increases with temperature
6.2 Dislocation Plasticity
295
because phonon mechanisms become stronger as the temperature rises. The dragcontrolled steady state velocity is then, from (6.74) and (6.76), (τ − τˆ)b Ω 0 (τ − τˆ) v= cS . (6.77) = k Bθ Β The rate of plastic work is always nonnegative since τ v = [ Ω 0τ (τ − τˆ) /(k Bθ )] cS ≥ 0 . (6.78) Conditions for which (6.74) applies are τˆ τ k Bθ / Ω0 . (6.79) When applied stresses vary rapidly, or when obstacles to glide are closely spaced, inertial effects can become important. Such effects are omitted in (6.74), corresponding to a regime in which the dislocation motion is said to be overdamped. As the dislocation velocity approaches the sound speed, say v > 0.7cS , drag forces increase with increasing velocity and (6.74) no longer applies. Because additional dissipation occurs from dislocationphonon interactions and other radiative mechanisms, the stressvelocity relationship becomes nonlinear in this socalled radiationcontrolled regime (Kocks et al. 1975). When the resistance τˆ exceeds the applied stress τ at some locations in the slip plane, thermal oscillations may supply enough energy to enable dislocations to move in a jerky fashion (Kocks et al. 1975). Such jerky glide often involves kink migration between obstacles. The dislocation velocity in this regime can be written (Hull and Bacon 1984) ⎛ −∆G ⎞ (6.80) v = yωG exp ⎜ ⎟, ⎝ k Bθ ⎠ where 0 ≤ ωG ≤ ω A is the vibrational frequency of the dislocation, y is the distance the dislocation moves for each obstacle overcome, and ∆G is the activation energy that may generally depend on stress, temperature, and structure variable α . A phenomenological relation for the activation energy, deemed most appropriate when τˆ stems from short range obstacles, is (Kocks et al. 1975; Hull and Bacon 1984) q
∆G = F0 ⎡⎣1 − (τ / τˆ) p ⎤⎦ ,
(6.81)
where F0 is the activation free energy and p and q are empirical constants limited to the range 0 < p ≤ 1 and 1 ≤ q ≤ 2 , with p = 1/ 2 and q = 3/ 2 typical. Relations (6.80) and (6.81) are valid when ∆G k Bθ , 0 < τ < τˆ . (6.82) ˆ When τ ≈ τ , superposition of effects of drag and thermal activation becomes necessary. In the absence of drag, dislocation velocity would in
296
6 Elastoplasticity
∼
v/cS
0.6 0.4
ly on ag
0.8
radiation
dr
1.0
obstacles only
crease rapidly towards its limiting value (i.e., the shear wave speed) as applied shear stress τ approaches threshold stress τˆ . When τ = 0 , (6.80) does not apply since the net dislocation velocity in a particular direction should not be nonzero in an unstressed body. Figure 6.1 summarizes regimes of dislocation velocity versus applied stress, following Kocks et al. (1975). The solid line corresponds to physically realistic behavior over the entire range of shear stress up to the theoretical strength. Dashed and dotted lines correspond to responses associated with individual mechanisms. In particular, drag control corresponds to (6.74), while thermal activation, or obstacle control, corresponds to (6.80). Plastic velocity gradient (6.63) or (6.67) depends on the mobile dislocation density ρ i . Since the mobile dislocation density decreases as a result of dislocations exiting the crystal at free surfaces, maintenance of a constant mobile density, and hence a constant plastic velocity gradient under conditions of steady state dislocation velocities, requires generation and multiplication of dislocations to offset those that exit the crystal or that are pinned or annihilated via interactions with other defects.
drag control
0.2
superposition
0.0
thermal activation
τ^
τ∼
τΤ
Fig. 6.1 Dislocation velocityshear stress diagram (Kocks et al. 1975)
A number of functional relationships between dislocation velocities and conjugate driving stresses have been observed or posited (Johnston and Gilman 1959; Lardner 1969; Teodosiu 1970; Bammann and Aifantis 1982), as have evolution equations for mobile and/or immobile dislocation line densities (Bammann and Aifantis 1982; Aifantis 1987; Zikry and Kao 1996; Rezvanian et al. 2007). Dislocation densities, both glissile and sessile, can be viewed as internal state variables, with their evolution equations expressed in the general form of (6.13).
6.3 Crystal Plasticity
297
Partial dislocations can be addressed using the same formalism as outlined in (6.62)(6.82) when the partials move collectively, with a total Burgers vector b = ∑ b P , with b P the Burgers vector of an individual partial. In some cases, mobility of the leading partial may exceed that of the trailing partial, in which case only the Burgers vectors, line densities, and velocities of mobile partials contribute to the plastic velocity gradient. Separation of a full dislocation into partial dislocations in the absence of slip barriers is energetically favorable when the energy of the full dislocation with total Burgers vector exceeds the sum of the energies of the partial dislocations, their interaction energy, and the stacking fault energy of the faulted region between the partials. Dissociation at slip barriers can occur when (Kocks et al. 1975) τˆ > WSF / b , (6.83) where WSF is the stacking fault energy per unit intermediate area. The shear stress required to move only the leading partial of a dissociated dislocation with partial Burgers vector of magnitude bP is often estimated as
τˆ = WSF / bP (Maeda et al. 1988).
6.3 Crystal Plasticity Consider the description of kinematics of slip on one or more distinct systems i afforded by crystal plasticity theory of Section 3.2.6. The plastic velocity gradient is given by (3.120): LP = F P F P −1 = ∑ γ i s i ⊗ m i , (6.84) i
and the plastic work rate per unit intermediate volume is, from (3.117), W P = Π α.β LPα.β = ∑ γ i s iα M αβ.mβi − ∑ γ iΨ ( s iα δαβ. mβi ) i
i
= ∑γ s (J F i iα
L
La .α
σ F L −1.βb ) mβi .b a
(6.85)
i
= ∑ γ i ( J L sai σ ab mbi ) = ∑ γ iτ i , i
i
where the resolved lattice Kirchhoff shear stress is τ i = J L sai σ ab mbi = J L sai σ ba mbi = J Lσ ab s(ia mbi ) .
(6.86)
Symmetrized dyad s( a m = ( s m + s m ) / 2 is sometimes called a Schmid i
i b)
i a
i b
i b
i a
tensor. As explained below, the resolved shear stress τ i plays a prominent role in kinetic relations for the slip rates, following Schmid’s law that
298
6 Elastoplasticity
states that plastic flow initiates in a single crystal at a given temperature and orientation when the applied stress is such that τ i reaches a critical magnitude. In uniaxial stress experiments, (6.86) reduces to Schmid’s relation τ i = J L −1τ i = σ cos(λ i ) cos(φ i ) , where σ is the applied true stress,
λ i is the angle between the loading axis and the slip direction, and φ i is the angle between the loading axis and the normal to slip plane i. The product cos(λ i ) cos(φ i ) is known as the Schmid factor. Before addressing slip on multiple systems and their interactions, consider kinetics of slip on a single system, extending the treatment of Section 6.2. In the dragcontrolled regime of (6.79), (6.77) gives ρ i (b i ) 2 (τ i − τˆi ) ρ i b i Ω 0 (τ i − τˆi ) (6.87) γ i = ρ ibi vi = = cS . Β k Bθ In the thermally activated regime of (6.82), (6.80) leads to ⎛ −∆G ⎞ τ i ⎛ −∆G ⎞ τ i i (6.88) γ i = ρ i b i v i = ρ i b i yωG exp ⎜ ⎟ i = γ 0 exp ⎜ ⎟ i , ⎝ k Bθ ⎠  τ  ⎝ k Bθ ⎠  τ  with γ 0i = ρ i b i yωG ≥ 0 . Term τ i /  τ i  ensures that the applied shear stress and dislocation velocity share the same algebraic sign when the convention of Section 3.2.6 adopted. According to that convention, γ i may be positive, negative, or zero in algebraic sign. Since γ i = ρ i b i v i , this implies dislocation velocities v i may likewise be positive, negative, or zero. A number of operational parameters are often introduced in the context of thermally activated slip (Kocks et al. 1975). Considering single slip with γ i ⇒ γ , activation energy parameter Q is defined by Q=
∂ ln γ ∂ ln γ = k Bθ ∂[−1/(k Bθ )] τ ∂ ln θ
= kB τ
θ 2 ∂γ . γ ∂θ τ
(6.89)
Rate sensitivity m is defined by m=
∂ ln γ ∂ ln τ
= θ
τ ∂γ . γ ∂τ θ
(6.90)
Since
∂ ln τ ∂ ln θ
=0= τ
∂ ln τ ∂ ln θ
+ γ
∂ ln τ ∂ ln γ
θ
∂ ln γ , ∂ ln θ τ
it follows from (6.89) and (6.90) that (Kocks et al. 1975) ∂ ln τ ∂ ln γ ∂ ln τ Q . =− =− ∂ ln θ γ ∂ ln θ τ ∂ ln γ θ mk Bθ
(6.91)
(6.92)
6.3 Crystal Plasticity
An activation volume can be described by k θ ∂ ln γ ∂ ln γ = B V * = k Bθ τ ∂ ln τ ∂τ θ
= θ
mk Bθ
τ
.
299
(6.93)
If γ 0i and ∆G are treated as independent of temperature in (6.88), then ∂[ −∆G /(k Bθ )] ∂ ln γ (6.94) = = ∆G . ∂[ −1/(k Bθ )] τ ∂[ −1/(k Bθ )] τ A simple and common prescription for activation energy in crystal plasticity theory, used at applied stress levels τ both above and below the mechanical threshold τˆ , is (6.81) with p = q = 1 : Q=
Q = ∆G = F0 [1 − (τ / τˆ)] ,
(6.95)
where F0 and τˆ are treated as parameters independent of stress and temperature, but possibly dependent on internal state variable α . It follows that m ⎡ F ⎛τ ⎞⎤ ⎛τ ⎞ (6.96) γ = γ 0 exp ⎢ 0 ⎜ − 1⎟ ⎥ ≈ γ 0 ⎜ ⎟ , ⎝ τˆ ⎠ ⎣ k Bθ ⎝ τˆ ⎠ ⎦ where m=
F ∂ ln[(τ / τˆ) m ] = 0 . k ∂ ln τ Bθ θ
(6.97)
Activation volume V * of (6.93) then becomes V * = F0 / τ . (6.98) The resistance to dislocation motion, τˆ , consists of shortrange barriers associated with lattice friction and longrange barriers associated with interactions between mobile dislocations and other defects, for example (Hull and Bacon 1984; Beltz et al. 1996). A simple way of superposing effects of these barriers at a particular location X in the crystal with particular orientation and elastic constants is the sum (Hull and Bacon 1984) τˆ(α ,θ , p) = τ P (θ , p ) + τ D (α ,θ , p) , (6.99) where τ P accounts for shortrange barriers such as the Peierls stress of (C.237), (C.246), or (C.248) of Section C.4.3, and τ D is the resisting stress from defects that depends on internal state variable α . Shortrange barriers, by definition, manifest approximately at scales on the order of the lattice spacing or smaller. Longrange barriers account for sources of glide resistance separated by distances larger than the lattice spacing, for example forest dislocations or point defects separated by tens of nanometers or more. When other dislocations are the primary longrange obstacle, the following dimensionless internal state variable is often appropriate:
300
6 Elastoplasticity
α = b ρT ,
(6.100)
where ρT ( X , t ) is the total line density of dislocations, both immobile and mobile, per unit volume in the intermediate configuration, as defined in (3.240). At room temperature in many engineering metals, τ D τ P , and the shortrange barriers can be overcome by thermal activation (Hull and Bacon 1984), though exceptions exist. At very low temperatures, or in stiff crystals with high concentrations of valence electrons such as ceramics, Peierls stress τ P can comprise a significant part of the total slip resistance (Friedel 1964; Clayton 2009a, 2010c, d). The slip resistance arising from other dislocations is often expressible in a functional form called Taylor’s law (Taylor 1934; Beltz et al. 1996; Clayton 2005a): aˆ µ b τ D = aˆ µα = aˆ µ b ρT = , 0.05 < aˆ < 1.0 , (6.101) l with paramter aˆ depending on the type of material and l = ρT −1/ 2 a mean dislocation spacing. Possible temperature and pressuredependencies of τ D arise only from temperature and pressuredependencies of effective (tangent) shear modulus µ (θ , p) , and are often omitted. In particular, dependence of τ P and τ D on hydrostatic pressure p can result from dependence of shear modulus on pressure, since both terms in (6.99) are proportional to the shear modulus. Such pressure effects can be important in shock physics applications (Steinberg et al. 1980; Becker 2004). By definition, τˆ ≥ 0 , τ P ≥ 0 , and τ D ≥ 0 . When various dislocation types move simultaneously (e.g., screw, edge, and mixed dislocations and dislocation loops of various orientations), resistances of those types with the largest impedance to motion contribute most strongly to (6.99). Now consider activity of multiple slip systems in the context of crystal plasticity theory. Phenomenological kinetic laws for slip fall into two categories: rate independent and rate dependent. In the former class of models (Kocks 1970; Hill and Rice 1972; Peirce et al. 1982; Asaro 1983), rate independence occurs when m → ∞ in (6.96), leading to the yield conditions τ i = τˆi ⇔ γ i ≥ 0, (6.102) τ i < τˆi ⇔ γ i = 0. In the context of rate independent plasticity, the total number of slip systems n is typically chosen such that slip rates and driving stresses are always nonnegative (Peirce et al. 1982). Such a prescription requires distinct assignment of positive and negative directions on a slip plane, as per
6.3 Crystal Plasticity
301
the special convention noted in the footnote of Section 3.2.6. Plastic flow occurs on slip system i when the driving stress τ i attains a critical value τˆi . Systems for which γ i > 0 are called active slip systems. Shear stresses obey the following hardening laws: n
τˆi = ∑ hij γ j .
(6.103)
j =1
In (6.103), hij (α ,θ , p, X ) is an interaction matrix that accounts for hardening (or softening) and possible interactions among slip systems. Instantaneous values of entries of hij will generally depend upon defects (e.g., immobile dislocation networks and forest dislocations) that accumulate with inelastic straining, represented by internal state variable α in the present framework, as well as temperature θ . Diagonal entries hii account for self hardening, and offdiagonal entries hij (i ≠ j ) account for latent hardening. In many metals, latent hardening coefficients exceed those for self hardening (Kocks 1970; Conti and Ortiz 2005) in part since dislocations moving and accumulating on the same system do not provide as much obstruction as those on intersecting slip planes. The latter (noncoplanar) defects include forest dislocations, for example. Explicit representations of hij follow later in the context of rate dependent plasticity. For actively hardening slip systems, consistency conditions following from (6.102) are n
τ i = τˆi = ∑ hij γ j > 0 ⇔ γ i > 0 .
(6.104)
j =1
When the rate of resolved shear stress falls below the critical shear stress rate, a formerly active system becomes inactive: n
τ i < τˆi = ∑ hij γ j ⇔ γ i = 0 ,
(6.105)
j =1
Clearly, dissipation of (6.85) is always nonnegative in the context of rate independent crystal plasticity since slip rates are always nonnegative in the present description and since γ i ≥ 0 only when τ i = τˆ i ≥ 0 . Rate dependent, i.e., viscoplastic, kinetic relations for crystallographic slip are more general and perhaps more commonly encountered (Hutchinson 1976; Teodosiu and Sidoroff 1976; Asaro and Needleman 1985; NematNasser and Obata 1986; Schoenfeld et al. 1995; Schoenfeld 1998; Horstemeyer et al. 1999; Clayton 2005a, b). The usual sign convention of Section 3.2.6 is prescribed, whereby slip may proceed in either direction on a given system, such that γ i may be positive or negative in algebraic sign. A typical functional form for a viscoplastic flow rule is
302
6 Elastoplasticity m
τ i − χˆ i τ i − χˆ i γ = γ0 , τ i − χˆ i  τˆ i i
(6.106)
where parameter γ 0 does not depend on stress and exhibits the same value for all slip systems. Typically γ 0 is imposed as constant (Hutchinson 1976) or a function of temperature alone (Balasubramanian and Anand 2002) for a particular type of crystal. As often prescribed for nonproportional or cyclic loading scenarios, χˆ i is an evolving backstress capturing directional hardening effects (McDowell and Moosebrugger 1992; Horstemeyer and McDowell 1998; Horstemeyer et al. 1999; Xie et al. 2004). Backstress χˆ i = 0 by definition in many traditional models (Asaro 1983; Asaro and Needleman 1985). By inverting and time differentiating (6.106), it is evident that as m → ∞ , the limiting case of rate independent behavior is approached. Notice that so long as τ i ≥ χˆ i , (6.106) results in unconditionally nonnegative dissipation W P in (6.85). When χˆ i = 0 , (6.106) corresponds to a dissipation potential Ω in the context of the second of (4.75):
γ τˆi τ i Ω =∑ 0 i i =1 1 + m τˆ n
1+ m
, τi
∂Ω ≥0, ∂τ i
(6.107)
with ⎧∂Ω / ∂τ i ∀τ i ≠ 0, ∀τ i = 0. ⎩ 0 Hardening evolution laws typically exhibit the form
γi =⎨
(6.108)
n
τˆi = ∑ hij γ j ,
(6.109)
j =1
where matrix hij is defined in the same manner as in (6.103). A standard assumption for many metallic solids is (Hutchinson 1976; Peirce et al. 1982; Asaro 1983) hij = qh + (1 − q )hδ ij , 1.0 < q < 1.4 , (6.110) where q is the latent hardening ratio that is treated as a constant for a given material. When q = 1 , all systems harden equally, an assumption used by and often credited to Taylor (1934). Strong latent hardening with q ≈ 1.4 of noncoplanar systems has been suggested as a typical rule for ductile metallic crystals (Asaro and Needleman 1985). Parameter h in (6.110) is an internal variable that evolves with cumulative plastic shear γ and possibly temperature, e.g.,
6.3 Crystal Plasticity
h = h (γ ,θ , p ) , γ = ∑ ∫ γ i dt .
303
(6.111)
i
Two different slip system hardening models suggested by Peirce et al. (1982) include ⎛ hγ ⎞ (6.112) h = h0 sech 2 ⎜ 0 ⎟ , ⎝ τˆS − τˆ0 ⎠ and nˆ −1
⎛hγ ⎞ (6.113) h = h0 ⎜ 0 + 1⎟ , ⎝ nˆτˆ0 ⎠ where h0 is a hardening modulus with dimensions of stress, τˆ0 is an initial value of τˆ , τˆS is a saturation value of τˆ , and nˆ is a hardening exponent. An alternative hardening relation to (6.109) given by Horstemeyer et al. (1999) is n
n
j =1
j =1
τˆi = h0 ∑ ⎡⎣ q + (1 − q)δ ij ⎤⎦ γ j − r0τˆi ∑ γ j ,
(6.114)
where h0 is a hardening modulus and r0 is a dimensionless parameter that accounts for dynamic recovery, leading to eventual saturation of slip resistance τˆi . Both h0 and r0 may depend on temperature; for example reflecting increased dislocation mobility at observed at higher temperatures in the thermally activated regime of Fig. 6.1. The backstress on a given slip system in (6.106) typically evolves only as a result of slip on that system (Horstemeyer et al. 1999; Clayton and McDowell 2003a): χˆ i = h1γ i − r1 χˆ i γ i , (6.115) where h1 and r1 may in general depend on temperature. Regardless of particular formulation, when τˆ i and χˆ i evolve with changes in deformation and temperature, each can be interpreted as a kind of internal state variable, though τˆ i and χˆ i do not explicitly enter the thermodynamic potentials and response functions of (6.9)(6.13). When dislocations are the primary source of stored energy in the lattice—for example energy of cold working attributed to selfequilibrating stress fields supported by dislocations—the simplest natural choice for a scalar internal state variable is a dimensionless function of the total dislocation density ρT , as in (6.100). Scalar ρT defined in (3.240), with physical dimensions of length of dislocation line per unit intermediate volume, is assumed to encompass energetic effects of both geometrically necessary and statistically stored dislocations (Ashby 1970), or net disloca
304
6 Elastoplasticity
tions and absolute dislocations (Werne and Kelly 1978), as described in Section 3.3.2. More detailed, tensorbased internal variable descriptions delineating energies of geometrically necessary and statistically stored dislocation densities are deferred until Chapters 8 and 9. Using (6.100), residual free energy (6.60) becomes (Clayton 2005a, b; 2009a) 1 Ψ R = κ b 2 ρT . (6.116) 2 The linear dependence of stored energy on dislocation density indicated by (6.117) has been used in thermodynamic components of a number of finite deformation plasticity models, particularly with regards to statistically stored dislocations (Bammann 2001; Regueiro et al. 2002; Svendsen 2002). Coefficient κ can be assigned a more explicit definition when details regarding the dislocation distribution, such as dislocation orientations and median separation distances, are known. In the simplest approximation, in which all dislocations are treated as noninteracting straight lines of the same type in an infinite elastic medium, the energy per unit length E of dislocation line is given by linear elastic solution (C.152): b2 ⎛ R ⎞ (6.117) ln ⎜ E = Kˆ ⎟, 4π ⎝ RC ⎠ where, as explained in Section C.1.6 of Appendix C, the energy factor Kˆ depends on the type (i.e., screw, edge, or mixed) and orientation of the dislocation as well as the secondorder elastic coefficients that may depend on temperature. For a pure screw dislocation in the isotropic elastic approximation, energy factor Kˆ = µ , the elastic shear modulus. Combining (6.116) and (6.117), a typical approximation is (Kocks et al. 1975; Hull and Bacon 1984; Clayton 2009a, 2010c, d) ˆ 2 ρ , 0.5 < Λ < 1.0 , Ψ R = E ρT = Λ Kb (6.118) T leading to
Ψ
R
= 2Λ Kˆ . (6.119) b ρT Using (6.85), (6.100), (6.116), and (6.118), TaylorQuinney parameter of (6.47) becomes, in the context of crystal plasticity with the (square root of) total scalar dislocation density as an internal variable as in (6.100),
κ =2
2
⎛ ∂κ ⎞ ⎞ ⎛ ⎛ i i ⎞ β ′ = ⎜ ∑τ i γ i − α ⎜ κ − θ ⎟α ⎟ ⎜ ∑τ γ ⎟ ∂θ ⎠ ⎠ ⎝ i ⎝ ⎠ ⎝ i −1 ⎛ ∂Kˆ ⎞ ⎛ ⎞ = 1 − Λb 2 ρT ⎜⎜ Kˆ − θ τ iγ i ⎟ . ⎟⎟ ⎜⎝ ∑ ∂ θ ⎠ ⎝ ⎠ i
−1
(6.120)
6.4 Macroscopic Plasticity
305
When the dependence of Kˆ on temperature is negligible, as the rate of dislocation accumulation increases, residual energy storage increases, β ′ decreases, and the fraction of plastic work converted to temperature rise via (6.46) decreases. A typical, but not universal, trend is that the fraction of plastic work converted to heat energy can be significantly less than unity as a metallic crystal or polycrystal strain hardens, and then later increases towards unity as the material ceases to harden and the strain energy contribution from defect densities saturates (Taylor and Quinney 1934; Foltz and Grace 1969; Lee 1969; Aravas et al. 1990; Wright 2002; Clayton 2005a, 2009c). The conjugate thermodynamic force associated with (6.60), (6.100), and (6.116)(6.119) is −∂Ψ R / ∂α = −2Λ Kˆ α ≈ − µ b ρT , which is notably proportional to (the negative of) resistance τ D to dislocation glide from dislocation interactions in Taylor’s hardening rule (6.101). An evolution equation for ρT of the general form (6.13) is required to complete the thermodynamic description. Such an equation should be formulated so that relationships between defect content and strain hardening, e.g., (6.99)(6.101) when applicable, as well as experimentally observed trends for β ′ for the particular crystalline solid under consideration, are all captured simultaneously (Clayton 2005a, b, 2009a).
6.4 Macroscopic Plasticity Recall from Section 3.2.7 that macroscopic plasticity refers to a description in which each volume element of material to which kinematic and constitutive models are assigned contains a large number of grains in a polycrystal. A convenient way of ensuring that the rate of working from plastic deformation is nonnegative5 in the context of macroscopic plasticity is specification of a plastic dissipation potential along the lines of that described in a general way in Section 4.3. In the present context, from (6.32), the appropriate thermodynamic flux is the plastic velocity gradient LP , and the conjugate driving force is the Eshelby stress measure Π . Recall that both of these quantities are couched in intermediate configuration B. 5 Restricting the rate of plastic working associated with dislocation glide to be dissipative is often a physically realistic assumption. However, in arbitrary solids, the rate of inelastic working need not always dissipate energy if rates of internal variables and heat conduction provide enough dissipation so that the net entropy production (left side of (6.32)) always remains nonnegative (Lubliner 1990).
306
6 Elastoplasticity
Specifically as an illustrative example, let ∂Ω , (6.121) LP = λ P ∂Π′ where the scalar plastic multiplier λ P ≥ 0 will be determined later, and the flow potential Ω is constructed such that the generalized scalar product Π : ∂Ω / ∂Π′ ≥ 0 . The deviatoric part of the intermediate Eshelby stress is equivalent to the deviatoric part of the Mandel stress: 1 Π α′.β = M α.β −Ψδα.β − ( M χ.χ −Ψδ χ.χ )δα.β 3 (6.122) 1 = M α.β − M χ.χ δα.β = M α′.β . 3 A simple illustrative example of dissipation potential is ′ )1/ 2 ≥ 0 . (6.123) Ω = (Π α′.β Π .′βα )1/ 2 = (Π ′αβ Π αβ From (6.121) and (6.123), the plastic velocity gradient becomes LPα.β =
λP α Π .′β , Ω
(6.124)
and is clearly coaxial (i.e., of the same direction in TB × T * B ) as the driving stress Π′ . Squaring both sides of (6.124) leads to the consistent definition λ P = ( LPαβ LPαβ )1/ 2 . (6.125) The resulting plastic dissipation is always nonnegative since ∂Ω λ P αβ ′ = λ PΩ ≥ 0 . Π α.β LPα.β = λ P Π α.β = Π ′ Π αβ ∂Π α′β. Ω
(6.126)
Relations (6.121)(6.126) parallel (4.84)(4.89), with LP used here as the thermodynamic flux rather than F P used in Section 4.3. Another subtle difference is that in (4.85) and (4.86) of Section 4.3, the plastic multiplier is absorbed into the dissipation potential, whereas λ P is written distinctly from the dissipation potential in (6.121). Since Π α′.α = 0 , J P = J P LPα.α = 0 from (6.124), ensuring that macroscopic plastic deformation is isochoric. A constitutive relationship between λ P and the state variables (e.g., stress or strain, temperature, and internal state variable(s)) then dictates the magnitude of plastic flow. Typically in engineering practice, as opposed to (6.121), a kinetic equaˆ P mapped to the current tion is specified for the plastic velocity gradient L configuration B, i.e., ˆ P = ( F L LP F L −1 ) , (6.127) ˆ P = ( F L LP F L −1 ) Lˆ P = F L LP F L −1 , D , W symm
skew
6.4 Macroscopic Plasticity
307
ˆ P is a symmetric plastic strain rate and W ˆ P is a skew plastic spin. where D With these definitions, the spatial velocity gradient of (3.58) becomes La.b = v;ab = F. Aa F −1.Ab = F .Lαa F L −1α.b + LˆP.ba (6.128) = LLa.b + Wˆ .Pb a + Dˆ .Pb a . Kinetic equations for the plastic strain rate and plastic spin of (6.127) are usually prescribed separately. The latter is often omitted (i.e., Wˆ .Pb a = 0 by definition) for solids that remain isotropic throughout their deformation history, e.g., polycrystalline metals with randomly oriented grains that do not develop significant texture or anisotropic hardening during plastic flow. In plastically anisotropic polycrystals, anisotropic hardening can be represented by a traceless, symmetric secondorder tensor (i.e., a tensor inˆ often labeled a backstress. In such anisotropic maternal state variable) α terials, the plastic spin can be assigned as (Aifantis 1987; Bammann and Aifantis 1989; Bammann et al. 1993; Regueiro et al. 2002) ˆ P = λˆW (αD ˆ P αˆ ) , αˆ = αˆ T , tr(αˆ ) = 0 , ˆ ˆP −D W (6.129) W ˆ with scalar λ related to dislocation interactions (Bammann and Aifantis 1989) or dominant slip system orientations (Regueiro et al. 2002). The plastic strain rate of the second of (6.127) can be assigned a kinetic law in a number of physically meaningful and mathematically convenient ways, and an immense literature exists on the subject (Hill 1950; Perzyna 1963; Follansbee and Kocks 1988; Lubliner 1990; Bammann et al. 1993; Marin and McDowell 1996; Simo and Hughes 1998; Scheidler and Wright 2001, 2003; Wright 2002; NematNasser 2004). For example, for nonporous viscoplastic solids, a direct flow rule applicable over a range of strain rates and temperatures can be prescribed as (Bammann et al. 1993) ⎧ ⎡ ˆ ˆ ˆ ⎤ ˆ ˆ (θ ) sinh ⎢  ξ  − k − Y (θ ) ⎥ ξ for  ξˆ = (ξˆ : ξˆ )1/ 2 ≥ kˆ + Yˆ , ⎪ f ⎪ P ˆ ˆ ˆ V (θ ) (6.130) D =⎨ ⎣⎢ ⎦⎥  ξ  ⎪ for  ξˆ = (ξˆ : ξˆ )1/ 2 < kˆ + Yˆ , ⎪⎩ 0 where the stress difference 2 (6.131) ξˆ = σ ′ − αˆ , 3 and the deviatoric Cauchy stress is 1 σ ′ab = σ ab − σ .cc g ab = σ ab + pg ab , (6.132) 3 with p the Cauchy pressure. In (6.130), fˆ , Yˆ , and Vˆ are scalar functions of temperature, kˆ reflects isotropic hardening (or softening) and may in
308
6 Elastoplasticity
crease (or decrease) during the deformation history. Similarly, backstress αˆ evolves with the deformation history. Evolution equations for kˆ and αˆ often follow a hardeningdynamic recovery format similar to (6.114) and (6.115) and are available in the literature (Bammann et al. 1993; McDowell et al. 1993; Marin and McDowell 1996). Described in what follows in (6.133)(6.143) is the standard engineering approach towards kinetics of macroscopic plasticity based on principles of normality, associativity, and a Von Mises–type yield function. Often, for isotropic and plastically incompressible solids, the normality conditions ˆ ⎧ ˆP ˆ ′ ˆ P = ⎪⎨ λ (∂Ω / ∂σ ) for F = 0, D (6.133) 0 for Fˆ < 0, ⎩⎪ are assigned, where values of Ωˆ = constant represent a set of flow isosurfaces in deviatoric stress space, λˆ P ≥ 0 is a plastic multiplier, and Fˆ is the yield function . Though many other possible flow functions exist, according to the most prevalent assumption for ductile metals, Ωˆ is defined in terms of the second invariant of the deviatoric stress: 1/ 2
⎛1
⎞
′ ⎟ Ωˆ = J 2 = ⎜ σ ′abσ ab ⎝2 ⎠
=
σ 3
3 τ , 2
=
(6.134)
1 ′ , J 2 = σ ′abσ ab 2 1/ 2 2 ⎛2 ⎞ τ = ⎜ J2 ⎟ = σ, 3 ⎝3 ⎠
(6.135) (6.136)
σ = −1 2 {(σ 11 − σ 22 ) 2 + (σ 22 − σ 33 ) 2 + (σ 33 − σ 11 ) 2
}
+ 6 ⎡⎣ (σ 12 ) 2 + (σ 23 ) 2 + (σ 31 ) 2 ⎤⎦ = ⎡⎣(3/ 2)σ abσ ab − (1/ 2)σ .aaσ .bb ⎤⎦
1/ 2
′ ⎤⎦ = ⎡⎣(3/ 2)σ ′abσ ab
1/ 2
1/ 2
(6.137) = [3 J 2 ] . 1/ 2
Above, σ is called the Von Mises stress (Von Mises 1913) or effective stress, and τ is called the octahedral shear stress. For a uniaxial normal stress state with nonzero Cauchy stress component σ 11 , the following conditions apply: σ = σ 11 , J 2 = 2(σ 11 ) 2 / 9 , and τ = 2σ 11 / 3 . For a shear stress state with nonzero component σ 12 = σ 21 , the following conditions hold: J 2 = (σ 12 )2 , σ = 3σ 12 , and τ = 2 / 3σ 12 . The spatial plastic deformation rate following from (6.133) and (6.134) is
6.4 Macroscopic Plasticity
ˆP ˆP ˆP ˆ P = λ σ′ = λ σ ′ = 3λ σ′ , (for Fˆ = 0 ), D 2σ 2Ωˆ 2 J2
309
(6.138)
clearly traceless and symmetric. From a rudimentary physical standpoint, (6.138) is realistic: the material deforms inelastically in the direction of the applied stress, in agreement with experimental observations. Squaring both sides of (6.133) or (6.138), the plastic multiplier satisfies −1/ 2 ˆ P :D ˆ P )1/ 2 ⎡(∂Ωˆ / ∂σ ′) : (∂Ωˆ / ∂σ′) ⎤ ˆ P :D ˆ P )1/ 2 . (6.139) λˆ P = (D = (2D ⎣ ⎦ Kinetic equations for plastic deformation are often labeled either as associative or nonassociative. In an associative flow rule, with a plastic potential of the form (6.134), the yield function is (6.140) Fˆ = Ωˆ − kˆ = J 2 − kˆ , where scalar function kˆ({ς }, X ) demarcates elastic and plastic domains and {ς } is a set of scalars that may include temperature, internal state variable α , and other field variables (e.g., pressure). When the yield and flow functions do not depend upon the time rate of plastic deformation, plastic behavior is said to be rate independent, while in the converse situation, the plastic deformation is said to be rate dependent or viscoplastic. In many engineering applications, plastic deformation is idealized as rate independent. In such cases, the magnitude of the plastic strain rate for a given thermodynamic state (e.g., state of stress, temperature, and internal variables) is prescribed as follows. KuhnTucker conditions are (Lubliner 1990) λˆ P Fˆ = 0 , λˆ P ≥ 0 , Fˆ ≤ 0 , (6.141) with the plastic multiplier ⎧⎪ Hˆ −1 (∂Fˆ / ∂σ ab )σ ab for Fˆ = 0 and Hˆ ≠ 0, (6.142) λˆ P = ⎨ ⎪⎩ 0 for Fˆ < 0. Macaulay brackets in (6.142) satisfy A = 0∀A ≤ 0 and A = A∀A > 0 for scalar function A, and are not to be confused with the dual product operator of (2.4) and (2.80)(2.82) which acts only on vector and tensor objects of higher order. Hardening modulus Hˆ satisfies the consistency conditions ∂Fˆ ab (when Fˆ = 0) σ Fˆ = 0 = Fˆ + ∂σ ab σ (6.143) ∂Fˆ ∂kˆ P ˆ ˆ ˆ ⇒ F = −λ H = ∑ ς = −∑ ς, ∂ς σ ∂ς σ σ
310
6 Elastoplasticity
where summation applies over all variables of the set {ς } . During plastic deformation, the yield surface in stress space represented by Fˆ = 0 and the stress state coincide. During elastic unloading, Fˆ < 0 , and one says that the stress state is contained within the yield surface. Typically (6.138) and (6.142) are combined with (3.58) and an objective rate form of (6.29) to provide a relationship between the time derivative of Cauchy stress and the total deformation rate Dab = L( ab ) . The constitutive description is complete upon prescription of evolution equation(s) for internal state variable(s) α and a functional relationship for kˆ in terms of {ς } at each location X. When kˆ is a constant, Hˆ = 0 in (6.143), and the corresponding mechanical behavior is labeled perfectly plastic. When Hˆ = 0 , λˆ P is indeterminate in (6.142), but the plastic deformation rate is still dictated by Fˆ = 0 and Fˆ = 0 (Lubliner 1990). In the case of nonassociative plasticity, the yield function and flow function need not be related, i.e., Fˆ ≠ Ωˆ − kˆ . More generally, for the nonassociative case, the direction of plastic deformation and its magnitude can be prescribed independently of any dissipation potential, as in (6.130). Bammann et al. (1993) showed that nonzero function Vˆ renders direct flow rule (6.130) rate dependent. The theoretical framework of (6.133)(6.143) is used frequently in engineering practice for isotropic ductile metals; when the material is plastically incompressible, this framework always provides for unconditionally nonnegative dissipation from plastic working in (6.32). From (6.16), (6.34), and (6.127), when J P = 0 the plastic work rate per unit intermediate volume is W P = Π α.β LPα.β = M α.β LPα.β = J Lσ ab LˆPab = J Lσ ab Dˆ abP . (6.144) Substituting (6.138) then gives
′ σ ′ σ ab = J L λˆ P Ωˆ = J L λˆ P J 2 ≥ 0 . (6.145) W P = J Lσ ab Dˆ abP = J L λˆ P 2Ωˆ ˆ P of (6.127), Since the plastic spin referred to the current configuration, W is skew by definition, this quantity does no mechanical work in (6.144) and does not contribute to the energy balance or dissipation inequality. It is emphasized that (6.133)(6.143) and (6.145) apply only for isotropic (poly)crystalline solids. When inelastic behavior is anisotropic, typically the notion of backstress is introduced to reflect differences in diˆ P and the deviatoric Cauchy stress σ′ (Lubliner 1990; Bamrections of D ab
6.5 Geometrically Linear Elastoplasticity
311
mann et al. 1993; Marin and McDowell 1996; Voyiadjis and Abu AlRub 2003), as indicated for example in (6.130). Furthermore, the lattice spin, and hence the total and plastic spins, require delineation in anisotropic solids, since the representation of the Cauchy stress in a hyperelastic solid depends on the rotational part of the lattice deformation, R L = V L −1F L , via the second of (6.5), even when lattice stretch V L is small. From (6.138) the spatial plastic velocity gradient Lˆ P = F L LP F L −1 is always traceless, though the true plastic volume change J P = J P LPα.α ≠ 0 in general, meaning that (6.144) is not ensured by (6.138). However, in the limit of small lattice strains, (3.73) and (3.74) lead to (6.146) LPα.α ≈ R LT α.a LˆP.ba R Lb.α = LˆP.baδ .ba = Dˆ .Paa = 0 .
6.5 Geometrically Linear Elastoplasticity Linearization of finite deformation kinematics of twoterm multiplicative elastoplasticity follows from (3.78)(3.83). Recall that displacement gradient ∇u , strain ε , and rotation Ω are each decomposed additively as (6.147) ua ;b = β abL + β abP ,
ε ab = u( a;b ) = β (Lab ) + β (Pab ) = ε abL + ε abP ,
(6.148)
Ωab = u[a ,b] = β[Lab] + β[Pab] = ΩabL + ΩabP ,
(6.149)
where superscripts L and P denote latticechanging and plastic (i.e., latticepreserving) parts, and the remaining notation is explained in Section 3.2.4. When plastic deformation is isochoric, the resulting kinematic implications are tr(ε P ) = 0 and tr(ε P ) = 0 , though throughout the forthcoming developments of Section 6.5, plastic deformation is not constrained to be volumepreserving unless noted otherwise. 6.5.1 Constitutive Assumptions In the geometrically linear theory of elasticplastic solids, (6.9)(6.13) are replaced by the following constitutive assumptions: ψ = ψ ( ε L ,α ,θ , ∇θ , x, g a ) , ψ = ψ ( ε abL , α ,θ ,θ, a , x, g a ) ; (6.150)
η = η ( ε L ,α ,θ , ∇θ , x, g a ) , η = η ( ε abL ,α ,θ ,θ,a , x, g a ) ;
σ = σ ( ε L , α ,θ , ∇θ , X , g a ) , σ ab = σ ab ( ε abL ,α ,θ ,θ ,a , x, g a ) ;
(6.151) (6.152)
312
6 Elastoplasticity
q = q ( ε L ,α ,θ , ∇θ , x, g a ) , q a = q a ( ε abL ,α ,θ ,θ , a , x, g a ) ;
α = α ( ε L , α ,θ , ∇θ , x, g a ) , α = α ( ε abL ,α ,θ ,θ ,a , x, g a ) ;
(6.153) (6.154)
Because all volume changes are assumed small in the present linear analysis, thermodynamic potentials are defined, for convenience, on a per unit mass basis as opposed to a per unit (intermediate configuration) volume basis as was considered in Section 6.1. Analogously to those of the nonlinear theory, thermodynamic potentials and response functions in (6.150)(6.154) do not depend explicitly upon the plastic distortion or plastic strain. Notice that objectivity with respect to small rigid body rotations precludes the use of the lattice rotation Ω L of (6.149) as a dependent variable entering (6.150)(6.154), via the same arguments used in Section 5.4.1 following (5.260). 6.5.2 Thermodynamics Substituting (6.150) into linearized dissipation inequality (4.73) gives ⎡ ∂ψ ∂ψ ⎞ ∂ψ ∂ψ ⎤ ⎛ σ abε ab − ρ ⎢ L ε abL + ⎜η + γa + α ⎥ ≥ θ −1q aθ ,a . (6.155) ⎟θ + ∂θ ⎠ ∂θ ,a ∂α ⎥⎦ ⎝ ⎢⎣ ∂ε ab From the time derivative of (6.148), ε ab = ε abL + ε abP , so (6.155) becomes
⎛ ∂ψ ⎞ ⎛ ab ∂ψ ⎞ L ∂ψ ⎞ ⎛ ⎟⎟ γ a ⎜ σ − ρ L ⎟ ε ab − ρ ⎜η + ⎟θ − ρ ⎜⎜ ∂ε ab ⎠ ∂θ ⎠ ⎝ ⎝ ⎝ ∂θ, a ⎠ (6.156) ψ ∂ α − θ −1q aθ,a ≥ 0. + σ abε abP − ρ ∂α Following arguments akin to those of Section 5.1.2, coefficients of ε abL , θ , and γ a = d (θ , a ) / dt should vanish identically, leading to the equalities ∂ψ ∂ψ ∂ψ , η=− , =0, L ∂ε ∂θ ∂∇θ and the reduced constitutive forms ψ = ψ ( ε L , α , θ , x , g a ) , η = η ( ε L , α ,θ , x , g a ) ,
σ=ρ
σ = σ ( ε L , α ,θ , x , g a ) .
(6.157)
(6.158)
Assuming Fourier conduction of the kind suggested in (4.62) and (5.277): q a = −k abθ,b , (6.159)
6.5 Geometrically Linear Elastoplasticity
313
where k is symmetric and positive semidefinite, local entropy production from heat conduction −θ −2 q aθ, a is always nonnegative. The entropy inequality then consists of the remaining terms in (6.156): ∂ψ 1 σ : εP − ρ (6.160) α + ∇θ , k∇θ ≥ 0 , ∂α θ demonstrating that in the absence of temperature gradients, the rate of plastic work W P = σ : ε P must exceed the rate of free energy accumulation associated with the time derivative of internal state variable α . When plastic deformation is isochoric, the plastic dissipation can be expressed as W P = σ : ε P = (σ − ρψ 1) : ε P = πˆ : ε P , (6.161) ˆ with π = σ −Ψ 1 a symmetric, small deformation analog of the Eshelbytype stress Π of the nonlinear theory first defined in (6.33). An equation for the temperature rise, analogous to (6.45), in terms of the plastic work rate, thermoelastic coupling, the rate of the internal variable, heat conduction, and heat sources can be derived immediately in the context of geometric linearity. Plastic rotation rate Ω abP = β[Pab] does not contribute to (6.160) or W P . 6.5.3 Representative Free Energy
A version of free energy function (6.48) describing a geometrically linear thermoelastic response additively decoupled from effects of internal variables, is ψ = ψ E ( ε L , θ , x , g a ) + ψ R (α , θ , x , g a ) . (6.162) The thermoelastic part of (6.162), assuming a linear response analogous to (5.304) about a reference state wherein ε L = 0 and ∆θ = θ − θ 0 = 0 , is 1 abcd L L θ ρ0ψ = ε abε cd − β abε abL ∆θ − ρ 0 cθ ln , (6.163) θ0 2 where the thermoelastic constants at a point x with basis g a ( x) are abcd
= ρ0
∂ 2ψ E ∂ε abL ∂ε cdL
εL = 0 θ =θ0
, β ab = − ρ0
⎛ ∂ 2ψ E ⎞ c = − ⎜θ . 2 ⎟ ⎝ ∂θ ⎠ εL = 0 θ =θ 0
∂ 2ψ E ∂θ∂ε abL
,
(6.164)
εL = 0 θ =θ0
(6.165)
314
6 Elastoplasticity
Thermoelastic constants in (6.164) depend on the symmetry of the material (via g a ( x) ) and are identical to those of (5.305) so long as the former are measured in a loading regime for which the material undergoes only lattice (thermoelastic) and not plastic deformation. Specific heat per unit mass in (6.165) likewise is identical to that of Section 5.1.4. All considerations regarding symmetry of material coefficients discussed in Section 5.4.5 and Appendix A apply for the elasticity tensor and the thermal stress coefficients in (6.164). Possible effects of evolving densities of defects (i.e., nonstationary internal variables) on material coefficients are omitted in (6.162)(6.165). From (6.148), (6.157), and (6.163), linearized stressstraintemperature relations are σ ab = J −1τ ab ≈ τ ab = abcd ε cdL − β ab ∆θ (6.166) = abcd (ε cd − ε cdP ) − β ab ∆θ . The residual part of the free energy, ψ R in (6.162), can be constructed in a manner completely analogous to (6.60) if, for example, a simple quadratic form is used for the energetic contribution from internal state variable α . 6.5.4 Linearized Dislocation Plasticity
In the geometrically linear theory, the rate of plastic distortion can be expressed by linearizing (3.98) and the last of (3.99), leading to (Mura 1968) j
β abP = ς a.cd ε cdb = ∑ ρ i bai ξ ic vid ε bcd .
(6.167)
i =1
Summation proceeds over i = 1, 2,... j populations of dislocations with the same tangent line, Burgers vector, and velocity for each value of i. The spatial dislocation flux, a thirdorder tensor, is ς ( x, t ) . The length per unit volume, Burgers vector, unit tangent line, and velocity of dislocation population i are, respectively, ρ i , b i , ξ i , and v i . Plastic dissipation per unit volume, W P = σ : ε P of (6.161), is then computed as follows, using the symmetry of the Cauchy stress: j
W P = σ abε abP = σ ab β abP = ∑ ρ i (ε cdbξ icσ ab bai )vid i =1
j
j
(6.168)
= ∑ ρ ( −ε dcbξ σ b )v = ∑ ρ ( f ) v , i =1
i
ic
ba i a
id
i =1
i
i PK d
id
where the PeachKoehler force (Peach and Koehler 1950; Mura 1968; Bammann and Aifantis 1982) is i fPK = −ξ i × σbi . (6.169)
6.5 Geometrically Linear Elastoplasticity
Use of Orowan’s (1940) relation instead of (6.167) gives β abP = ∑ ρ i bi vi sai mbi ,
315
(6.170)
i
where in the geometrically linear theory, for each slip system i, the magnitude of Burgers vector, slip direction, dislocation line velocity, and unit normal to the glide plane, are respectively (6.171) bi = bi  , si = bi / bi , vi = v i  , mi = ξ i × vi / v i . Using (6.171) in (6.161), the rate of plastic work per unit spatial volume is W P = σ abε abP = σ ab β abP = ∑ ρ i bi vi ( sai σ ab mbi ) = ∑ ρ i bi viτ i , (6.172) i
i
where the resolved shear stress is τ i = sai σ ab mbi = s(iaσ ab mbi ) .
(6.173)
Kinetic relationships between dislocation velocity and resolved shear stress in the geometrically linear case are posited in the same manner as outlined in Section 6.2, simply by replacing v i of the nonlinear theory with vi in the second of (6.171), and τ i of the nonlinear theory with τ i of (6.173). 6.5.5 Linearized Crystal Plasticity
In the linearized description of kinematics of slip in crystal plasticity theory of Section 3.2.6, the plastic rate of distortion is given by (3.125): (6.174) β P = ∑ γ i si ⊗ m i , i
and the plastic work rate per unit volume is, just as in (6.172), W P = σ abε abP = σ ab β abP = ∑ γ i (sai σ ab mbi ) = ∑ γ iτ i , i
(6.175)
i
where the resolved shear stress τ i is defined in (6.173). Kinetic relationships between slip rate γ i and resolved shear stress τ i in the geometrically linear case are prescribed in the same way as demonstrated in Section 6.3 for the nonlinear case, simply by replacing the resolved Kirchhoff stress τ i of the nonlinear theory with τ i of (6.173). The quadratic form used as an estimate of the residual free energy in (6.116) can be replaced by 1 1 ρψ R = κα 2 = κ b 2 ρT , α = b ρT , κ = 2Λ Kˆ , 0.5 < Λ < 1.0 , (6.176) 2 2 with ρT the total dislocation line length per unit spatial volume and Kˆ , as defined in (C.152), the energy factor for a dislocation line in an anisotropic
316
6 Elastoplasticity
elastic body. For a pure screw dislocation in an isotropic solid, the energy factor is equivalent to the temperaturedependent shear modulus. 6.5.6 Linearized Macroscopic Plasticity
Macroscopic plasticity as outlined in the geometrically nonlinear context in Section 6.4 can be described analogously in the linear theory, replacing ˆ P of (6.127) with plastic Lˆ P of (6.127) with plastic distortion rate β P , D ˆ P of (6.127) with plastic rotation rate Ω P . For exstrain rate ε P , and W ample, relations (6.133)(6.143) for a plastically incompressible and plastically isotropic material based on concepts of normality, associated flow, and a Von Misestype (i.e., J 2 ) yield and flow function are linearized as follows. The flow rule, assuming normality, is ⎧⎪ λˆ P (∂Ωˆ / ∂σ′) for Fˆ = 0, (6.177) εP = ⎨ 0 for Fˆ < 0, ⎪⎩ with flow function 1/ 2 Ωˆ = J = (σ ′abσ ′ / 2 ) = σ / 3 = 3/ 2τ , (6.178) 2
ab
where the second invariant of the deviatoric stress, the octahedral shear stress, and the Von Mises effective stress are defined identically as in Section 6.4: ′ /2, J 2 = σ ′abσ ab (6.179)
τ = 2 J 2 / 3 = 2σ / 3 ,
(6.180)
σ = 3J 2 .
(6.181)
The plastic strain rate then follows as λˆ P λˆ P 3λˆ P εP = σ′ = σ′ = σ′ , ( Fˆ = 0 ), 2σ 2Ωˆ 2 J2 and the plastic multiplier satisfies −1/ 2 λˆ P = (ε P : ε P )1/ 2 ⎡⎣(∂Ωˆ / ∂σ′) : (∂Ωˆ / ∂σ′) ⎤⎦ = (2ε P : ε P )1/ 2 . The yield function is Fˆ = Ωˆ − kˆ = J 2 − kˆ , with kˆ = kˆ({ς }, X ) and the constraints
λˆ P Fˆ = 0, λˆ P ≥ 0, Fˆ ≤ 0 .
(6.182)
(6.183) (6.184)
(6.185) In rate independent plasticity, the plastic multiplier can be expressed as (Lubliner 1990)
6.6 The Eshelby Stress
⎧⎪ Hˆ −1 (∂Fˆ / ∂σ ab )σ ab for Fˆ = 0 and Hˆ ≠ 0, ⎪⎩ 0 for Fˆ < 0,
λˆ P = ⎨
317
(6.186)
where hardening modulus Hˆ is obtained from the consistency condition ∂Fˆ ∂kˆ (6.187) Fˆ = −λˆ P Hˆ = ∑ ς = −∑ ς , (for Fˆ = 0 ). ∂ς σ ∂ς σ σ When Hˆ = 0 , as occurs in a perfectly plastic material, λˆ P is indeterminate (Lubliner 1990), but the magnitude of the plastic strain rate is still dictated by the constraint that the stress state remain on the yield surface during plastic loading. The rate of plastic work and plastic volume change are respectively ′ /(2Ωˆ ) = λˆ P Ωˆ = λˆ P J 2 ≥ 0 , (6.188) W P = σ ab β abP = σ abε abP = λˆ Pσ ′abσ ab ˆ )σ ′a = 0 . (6.189) ε P a = (λˆ P / Ω .a
.a
From (6.188) and (6.189), respectively, it follows that plastic dissipation is always nonnegative and the plastic strain rate is always isochoric.
6.6 The Eshelby Stress The stress tensor Π , work conjugate to the plastic velocity gradient in (6.32) in the setting of twoterm multiplicative elastoplasticity, can be related to several quantities introduced by Eshelby (1951, 1975) in the context of continuum elasticity theory. This stress measure can be written, using (4.6), (4.7), or Table 4.1, along with (6.1)(6.5), (6.16), and (6.33), as follows: (6.190) Π = M −Ψ 1 = − J L F L −1 π*F L = − J P −1F P Π*F P −1 , where the superposed asterisk denotes the dual of a mixed variant tensor akin to (2.119). Expressed in indicial notation, (6.190) is Π α.β = M α.β −Ψδα.β = − J L F L −1.βbπ a.b F La.α = − J P −1 F P.βB Π A.B F P −1.Aα , (6.191) with π a.b = − J L −1 F Lb.β ( M α.β −Ψδα.β ) F L −1α.a (6.192) =Ψδ a.b − J L −1 F Lb.β M α.β F L −1α.a =Ψδ a.b − σ a.b , and
Π A.B = JF −1.Bb (Ψδ a.b − σ a.b ) F. Aa =Ψ 0δ A. B − F. Aa Pa. B = Ψ 0δ A. B − C AC Σ CB .
(6.193)
318
6 Elastoplasticity
According to (6.161), quantity πˆ = − π serves as the conjugate stress to the plastic strain rate in geometrically linear elastoplasticity, but only when the plastic strain rate is traceless. Tensors π , Π , or variations of them, exhibit interesting characteristics in the context of elastic bodies containing defects and are often referred to as elastic energymomentum tensors (Eshelby 1951, 1975). Following Maugin (1995), local stress measures π ∈ Tx* B × Tx B and Π ∈ TX* B0 × TX B0 in (6.192) and (6.193) are labeled spatial and referential Eshelby stresses, respectively. It is noted as a point of clarification that a number of other tensors often differing in mathematical form and/or physical origin from those of Eshelby enter descriptions of thermodynamics of heterogeneous systems (Bowen 1967; Grinfeld 1991) and configurational (Gurtin 1995) or material forces (Maugin 1995). For example, chemical potential tensors (Grinfeld 1981) can emerge in theories of phase transformations. Consider a nonlinear elastic body in the context of elastostatics (no inertia) and in the absence of body forces and thermal effects. Local balances of linear and angular momentum are, from (4.21) and (4.27), P: AaA = 0 , F. Aa P bA = P aA F. Ab , (6.194) and the constitutive equations of elasticity theory are given by (5.44)(5.45), written here in terms of the deformation gradient F( X , t ) as independent state variable: ∂Ψ 0 Pa. A = , Ψ 0 =Ψ 0 ( F, G A ( X ), X ) . (6.195) ∂F. Aa Strain energy density per unit reference volume can be expressed as a series expansion along the lines of (5.62): 1 ABCD 1 ABCDEF Ψ0 = E AB ECD + E AB ECD EEF + ... , (6.196) 2 6 where elastic constants ABCD and ABCDEF are defined in (5.65) and (5.66) and may depend on orientation (via G A ) in anisotropic crystals as well as choice of material particle X in heterogeneous bodies. Consider the material gradient of the strain energy density: ∂Ψ 0 ∂Ψ 0 a ∂Ψ 0 ∂Ψ 0 Ψ 0, A = F. B: A + G B; A + = A a ∂X ∂F. B ∂G B ∂X A exp (6.197) ∂Ψ 0 a ∂Ψ 0 F. B: A + , = ∂F. Ba ∂X A exp where the explicit material gradient is defined by (Eshelby 1975)
6.6 The Eshelby Stress
∂Ψ 0 ∂X A
= exp
∂Ψ 0 ∂X A
=Ψ 0, A −
F. aA = const. B
X = const. (A≠ B )
∂Ψ 0 a F. B: A . ∂F. Ba
319
(6.198)
From (6.193)(6.197), the divergence of the referential Eshelby stress is Π A.B; B =Ψ 0, Bδ A. B − ( F. Aa Pa.B ); B =Ψ 0, A − Pa. B F. Aa; B − F. Aa Pa.;BB g
=Ψ 0, A − Pa. B ( F. Aa; B + Γ
..a bc
g
F. Ac F. Bb ) − F. Ac ( Pc.;BB − Γ
=Ψ 0, A − Pa. B F. Aa:B − F. Ac Pc.:BB =Ψ 0, A − Pa. B F. Aa:B =Ψ 0, A −
∂Ψ 0 ∂Ψ 0 a F. A:B = a ∂X A ∂F. B
.. a . B bc a
P F. Bb ) (6.199)
exp
1 BCDE 1 BCDEFG EBC EDE EFG + ..., ...., A E BC EDE + ......, A 2 6 with total covariant derivative of deformation gradient F. Aa:B = x:aAB = F.Ba: A defined in (2.116) and total covariant derivative of the first PiolaKirchhoff stress Pa. A ( X , t ) given in (4.20). The local material force per unit reference volume in a heterogeneous elastic body is then defined by ∂Ψ 0 = −Π A. B; B , fA = − (6.200) ∂X A exp =
and clearly depends on variations in elastic constants with reference coordinates, as indicated from the last of (6.199). Such variations may arise in crystalline solids, for example, from variations in reference orientation of the crystal lattice (e.g., misoriented grains in a polycrystal or deformation twins), changes in material composition (e.g., inclusions or precipitates with different elastic constants than the surrounding medium), or defects (e.g., a dependence of elastic constants on spatially heterogeneous densities of voids, vacancies, or dislocations). For a homogeneous body, fA = 0 . The sign convention used for the material force is somewhat arbitrary; that of (6.200) parallels the sign convention typically used in particle mechanics (Appendix B), wherein a force is defined as a negative potential energy gradient with respect to position of a particle (see e.g., (B.2)). A total force acting on a volume V enclosed by surface S with unit normal N can be found by integrating (6.200) over the volume and application of the divergence theorem of Section 2.7.1 in reference coordinates: ∂Ψ 0 FA = ∫ fA dV = − ∫ dV = − ∫ Π A.B; B dV = − ∫ Π A. B N B dS , (6.201) A ∂ X exp V V V S where reference basis vectors G A ( X ) are presumed constant over the domain of integration of covector field fA ( X , t ) . When V contains a singular
320
6 Elastoplasticity
ity—for example a discontinuity in elastic constants at the boundary surface between an inclusion or crack and the surrounding medium—energy density Ψ 0 may not be differentiable or even continuous, fA may not be bounded, and the divergence theorem cannot be applied as in (6.201). In that case, a force acting on a singularity can be defined directly as the surface integral FA = − ∫ Π A.B N B dS , (6.202) S
where S may fully or partially enclose the defect or source of singularity. Two different surfaces S enclosing or bordering the same defect or source of heterogeneity will produce the same force FA because fA vanishes in regions of V where elastic constants are uniform and where defects do not exist. In this sense, surface integral (6.202) is said to be path independent. Extensions of the Eshelby stress of nonlinear elastostatics have addressed second grade elasticity (Eshelby 1975; Le and Stumpf 1996b, c), Cosserat media (Epstein and Elzanowski 2007), dynamics and inertia (Eshelby 1951; Maugin 1994; Cermelli and Fried 1997), nonlinear electrostatics of dielectrics (Epstein and Maugin 1990), and ductile fracture (Maugin 1994). In the context of a multiplicative decomposition of the deformation gradient, differentialgeometric identities for the divergence of Π in terms of connection coefficients formed from a latticepreserving deformation map were derived by Epstein and Maugin (1990). Entire texts have been devoted to the subject of material forces or mechanics in material space (Maugin 1993; Kienzler and Herrmann 2000). In such treatments (see also Maugin 1995), governing equations of continuum mechanics are written entirely referred to referential or material coordinates, with such equations often involving Eshelbytype stress measures. A quantity similar, but not identical, to π of (6.192) was introduced by Eshelby (1951) to describe the force per unit volume acting on a singularity in an otherwise linear elastic body. In linear elasticity, (6.194)(6.202) are replaced by their linearized spatial analogs as follows. Quasistatic momentum balances, in the absence of body forces, are σ ;abb = 0 , σ ab = σ ba , (6.203) constitutive equations (5.273) and (5.275) are ∂Ψ ∂Ψ = σ ab = , Ψ =Ψ ( ε, g a ( x), x ) , (6.204) ∂ε ab ∂u( a ;b ) and strain energy density (5.304) in the absence of temperature effects is 1 abcd 1 abcd Ψ = ε abε cd = ua ;b uc ; d , (6.205) 2 2
6.6 The Eshelby Stress
321
where generally anisotropic, secondorder elastic constants satisfy symmetry conditions abcd (g a ( x), x) = ( ab )(cd ) . The spatial gradient of the strain energy density is ∂Ψ ∂Ψ ∂Ψ ∂Ψ g b;a + a Ψ ,a = a = ε bc ;a + ∂x ∂ε bc ∂g b ∂x exp (6.206) ∂Ψ ∂Ψ ∂Ψ ∂Ψ = = (ub;ca − u[b;c ]a ) + a , ub;ca + a ∂ε bc ∂x exp ∂ub;c ∂x exp where the explicit gradient with respect to position of the particle in question is defined by ∂Ψ ∂Ψ ∂Ψ = a =Ψ ,a − (6.207) ub;ca . a ∂x exp ∂x uab;b =const. ∂ub;c x = const. (a ≠ b )
From (6.203)(6.207), and from the compatibility conditions ua;[bc] = 0 ,
π a.b;b =Ψ ,bδ a.b − (σ bc uc ;a );b =Ψ , a − σ ;cbb uc ;a − σ bc uc ;ab =Ψ ,a −
∂Ψ ∂Ψ ∂Ψ uc ;ab =Ψ ,a − uc ;ba =Ψ ,a − ub ;ca ∂ub;c ∂ub;c ∂ub;c
(6.208)
∂Ψ 1 bcde = ...., a ε bc ε de , a ∂x exp 2 where the original Eshelby stress measure in linear elastostatics, π , is defined as (Eshelby 1951) π =Ψ 1 − σ∇u , π a.b =Ψδ a.b − σ bc uc;a . (6.209) Notice that π of (6.192) differs from π of (6.209) by the presence of the displacement gradient in the rightmost term of the latter. The local material force per unit volume in a heterogeneous elastic body is defined as ∂Ψ 1 bcde fa = − a (6.210) = −π a.b;b = − ...., a ub ; c ud ;e , ∂x exp 2 =
and depends on variations in elastic constants with coordinates x a . A total force acting on volume v enclosed by surface s with unit normal n can be found by integrating (6.210) over that volume and application of the divergence theorem of Section 2.7.1 in spatial coordinates: ∂Ψ Fa = ∫ fa dv = − ∫ a dv = − ∫ π a.b;b dv = − ∫ π a.b nb ds , (6.211) x exp v v ∂ v s where basis vectors g a ( x) are required to be constant over the domain of integration. When volume v contains a singularity (e.g., a jump discontinuity in the gradient of strain energy density across an internal boundary
322
6 Elastoplasticity
within v), the divergence theorem cannot be applied as in (6.211). In that case, the material force can be defined as the surface integral Fa = − ∫ π a.b nb ds , (6.212) s
where s may fully or partially enclose the defect, heterogeneity, or source of singularity. Because fa = 0 in parts of volume v where elastic constants are uniform and where defects do not exist, (6.212) is path independent. For situations in which a region of the body contains a singularity, strain energy density may not be differentiable or even continuous within the region. For example, for a stressed region containing a void or crack, a jump in mass density and hence strain energy per unit volume may exist between the elastic medium ( ρ 0 > 0 ) and the empty region inside the void or open crack ( ρ0 = 0 ). In such cases, the gradient of the strain energy density is not bounded, and the divergence theorem cannot be applied as in (6.211). Similarly, (6.207) and (6.211) would not apply for a region containing a dislocation or disclination line or loop in the context of linear elasticity (Sections C.1 and C.2 of Appendix C). For example, from (C.152) the energy gradient per unit length of dislocation line is singular as R→0: 2 ˆ 2 ⎛ R ⎞⎤ ˆ 2 ∂ ⎡ Kb ˆ b ln ⎜⎛ R ⎟⎞ + Kb xa , (6.213) ln = K ⎢ ⎥ ⎜ ⎟ , a ∂x a ⎢⎣ 4π ⎝ RC ⎠ ⎥⎦ 4π ⎝ RC ⎠ 4π R 2 where the first term on the right of (6.213) is nonzero if elastic coefficient Kˆ is permitted to vary with x, though the analytical derivation of (C.152) assumes constant elastic moduli. While the total energy of the dislocation will not depend on its position in an infinite medium, this energy can depend on position in a finite medium (Phillips 2001). For the elastic sphereinhole models of point defects of Section C.3 (Bitter 1931; Eshelby 1954, 1956; Teodosiu 1982), the divergence theorem used in (6.211) would also not apply, since the strain energy density is not necessarily differentiable or even continuous across the interface between the sphere (defect) and the surrounding medium. In all of these situations involving singularities, one can still define a global material force acting on the singularity via a surface integral of the type (6.212), presuming that the integrand π a.b nb is well defined along the surface of integration. Surface s may or may or may not completely enclose the defect, and the surface integral is path independent so long each path considered bounds the same defect(s). For a body containing a notch or crack, the projection in the direction of extension e1 of surface integral π a.b nb along an open contour c (dotted line
6.7 Elastoplasticity of Grade Two
323
in Fig. 6.2) enclosing the notch tip or crack tip can be associated with the Jintegral of fracture mechanics (Rice 1968; Maugin 1993, 1994, 1995): J = e1 i ∫ πndc = ∫ (Ψ n1 − t a ua ,1 )dc . (6.214) c
c
The quantity J exhibits dimensions of energy per unit area and is often called an energy release rate. This quantity can be compared to the energy required to generate free surface area, i.e., to extend a sharp crack, within an elastic solid (Griffith 1921): crack extension is predicted when J attains a threshold value for a particular material. When contour c is collapsed to the free surface of a smooth notch tip c′ , ⎡ ⎤ J = lim ⎢e1 i ∫ πndc ⎥ = ∫Ψ nie1dc′ , (6.215) c →c ′ ⎣ c ⎦ c′ since traction t a = σ ab nb vanishes along free surface c′ . When c is taken as a closed contour about a region containing no defects or heterogeneities, J vanishes identically for that region, implying path independence of the Jintegral of (6.214) (Rice 1968). Extensions of the Jintegral to nonlinear and inelastic behavior are possible (Rice 1968; Maugin 1993, 1994, 1995).
Fig. 6.2 Contour used in evaluation of Jintegral about a notch or crack tip
6.7 Elastoplasticity of Grade Two The present Section generalizes second grade nonlinear elasticity of Section 5.7 to crystals with defects. Specifically, the present kinematic description follows from decomposition (6.1): x.,aA = F. Aa = F L.aα F Pα. A . A version of Hamilton’s principle is employed in which the stressfree intermediate configuration B of Fig. 3.4, and hence components of plastic deformation F Pα. A , remain stationary with respect to variational derivatives. This version of Hamilton’s principle furnishes equilibrium equations and traction boundary conditions for the instantaneous elastic response from the intermediate configuration. Kinetic equations for
324
6 Elastoplasticity
evolution of the plastic deformation and relaxed intermediate configuration are not provided by this approach, which deals only with nondissipative part of the response, in the absence of heat conduction, heat sources, and temperature gradients. Much of what follows in Section 6.7 is based on the theory of Teodosiu (1967a, b, 1968). Similar, but not identical, approaches generalizing Toupin’s second grade elasticity theory (Toupin 1962, 1964; see also Section 5.7) to account for plastic slip and multiplicative kinematics were forwarded by Le and Stumpf (1996b, c) and Garikipati (2003). 6.7.1 Covariant and Variational Derivatives
Recall from (3.70) that the lattice deformation gradient F L ( X , t ) provides a firstorder accurate approximation of the length and direction of a differential line element mapped from the intermediate configuration to the current configuration: dx = F L dx . A secondorder accurate approximation is obtained by writing the inverse of (3.68) and retaining the secondorder term in the Taylor series expansion, leading to 1 dx a ( X ) = F La.α dxα + F Laα :β dxα dx β , (6.216) X X 2 where the base point of the differential line element is assigned to location X of the material particle. The total covariant derivative of the lattice deformation is, from the inverted form of (3.69) and the definition in the last of (3.36) of partial differentiation with respect to anholonomic coordinates xα , F La.α :β = F La.α , β − Γ g
= ( F L.aα ,b + Γ
g
βα
F La. χ + Γ
.. a bc
F Lc.α ) F Lb. β − Γ
.. χ
g
= ( F L.aχ ,b F L −1.χc + Γ g
= (Γ g
= (Γ
.. a bc
..a bc
F Lc.α F Lb.β .. χ
βα
F La. χ
) F Lc.α F Lb.β − Γ
.. a bc
− F La. χ F L −1.χc ,b ) F Lc.α F Lb.β − Γ
.. a bc
− Γ bc..a ) F Lc.α F Lb.β − Γ
.. χ
βα
.. χ
βα
.. χ
βα
F La. χ
(6.217)
F La. χ
F La.χ , g
where Γ bc..a are components of the crystal connection of (3.190) and Γ and Γ
.. χ
βα
..a bc
are coefficients of connection coefficients used for coordinate
systems on B and B , respectively. In general, F La.α :β consists of 27 inde
6.7 Elastoplasticity of Grade Two
325
pendent entries. When the torsion of crystal connection vanishes corresponding to a vanishing of the dislocation density tensor of (3.214), and when a symmetric connection is used for the intermediate configuration, then the following conditions hold: χ La La La La a Γ [..bca ] = 0 , Γ ..[ βα ] = 0 , F .[α :β ] = F .[α ; β ] = F .[α , β ] = 0 , F .α = x.,α , (6.218) in which case F La.α :β = F La.(α :β ) consists only of up to 18 independent entries. From the last of (6.218), when such conditions hold, the lattice deformation is integrable and the elastic response of grade two becomes identical to that addressed in Section 5.7 of Chapter 5, with reference coordinates X A of Section 5.7 replaced with (now holonomic) intermediate coordinates xα . However, for the general situation considered in what follows in Section 6.7, (6.218) does not apply, the crystal may contain defects such as dislocations, and the constitutive response may differ from that predicted in the context of holonomic elasticity of grade two discussed in Section 5.7. Extending (5.413) and results of Eringen (1962), and specifying intermediate external basis vectors with vanishing Christoffel symbols (i.e., Γ ..βαχ = 0 ), the following identity applies: g ⎛ ⎞ (6.219) F La.α :β = ⎜ F La.α ,b + Γ ..bca F Lc.α ⎟ F Lb.β = ( F La.α );b F Lb.β , ⎝ ⎠ from which it follows that for the inverse of the lattice deformation, 0 = ( F La.α F L −1α.c );b ⇒ F L −1α.c ;b = − F L −1α.a F L −1.βb F L −1.χc F L .aχ :β . (6.220)
Recall from Section 5.6.1 the definition of the variational derivative. Let x a = x a ( X A , Λ ) , where Λ is a scalar parameter. In the present setting, the first variation of x is defined as follows, generalizing (5.373): ∂x a δ xa = dΛ , (6.221) ∂Λ X ,F P Λ =0
where by definition, reference coordinates X A of material particle at X and values of plastic deformation gradient F Pα. A ( X ) = F L −1α.a F. Aa are held fixed during the variation (Teodosiu 1967a). For a scalar function f = f ( x a , F La.α , F La.α :β ,...) depending on spatial position, lattice deformation gradient, and total covariant derivatives of lattice deformation, the first variation is ∂f (6.222) δf = dΛ . ∂Λ X ,FP Λ =0
Since reference coordinates are held fixed in the variational derivative,
326
6 Elastoplasticity
δ ( f, A ) = (δ f ), A = δ f, A .
(6.223) The first variation does not commute with partial differentiation in the spatial frame ∂ a = ∂ / ∂x a , as indicated in (5.379) which also applies here. For anholonomic partial derivatives, δ ( f ,α ) = δ ( f, A F P −1.Aα ) = F P −1.Aα δ ( f, A ) = F P −1.Aα δ f, A = (δ f ),α , (6.224) since plastic deformation is stationary during the variation: δ ( F Pα. A ) = 0 , δ ( F P −1.Aα ) = 0 , δ J P = 0 , δ J P −1 = 0 . (6.225) The following formulae for variations of kinematic quantities are useful, following from (5.376)(5.378), (6.1), and (6.225): δ F La.α = δ ( x.,aA F P −1.Aα ) = F P −1.Aα [(δ x a ), A + F. Aa;bδ xb ] (6.226) = F P −1.Aα (δ x a );b F. Ab = (δ x a );b F Lb.α ,
δ F L −1α.a = δ ( F Pα. A X .,Aa ) = F Pα. Aδ ( X .,Aa ) = − F Pα. A F −1.Ab F −1.Ba (δ xb ); B = − F L −1α.b (δ xb );a ,
(6.227)
δ J L = δ ( J P −1 J ) = J P −1δ J = J P −1 J (δ F. Aa ) F −1.Aa = J L (δ x a );a . (6.228) The first variation of total anholonomic covariant derivative of the lattice deformation, F La.α :β , is found using (5.376), (6.219), (6.224), (6.226), and (6.227), as given by Teodosiu (1967a): δ ( F L.aα :β ) = δ ( F La.α ;b F Lb.β ) = F Lb.β δ ( F La.α ;b ) + F La.α ;bδ ( F Lb.β )
= F Lb.β ⎡⎣δ ( F L.aα ;χ F L −1.χb ) ⎤⎦ + F La.α ;b (δ x b );c F Lc.β = F Lb.β ⎡⎣δ ( F L.aα ;χ ) F L −1.χb + F La.α ;χ (δ F L −1.χb ) ⎤⎦ + F La.α ;b (δ x b );β = F Lb.β ⎡⎣δ ( F L.aα ); χ F L −1.χb − F La.α ; χ F L −1.χc (δ x c );b ⎤⎦ + F La.α ;b (δ xb ); β = F Lb. β δ ( F La.α );b − F La.α ;b (δ xb ); β + F La.α ;b (δ xb ); β
(6.229)
= F Lb. β δ ( F La.α );b . 6.7.2 Constitutive Assumptions and Governing Equations
Consider an elasticplastic material featuring an instantaneous response from the intermediate configuration, with this response characterized by hyperelasticity of grade two. The strain energy of the solid depends on the total covariant derivative of the lattice deformation (6.217) in addition to the lattice deformation gradient, reference position of a material particle (in the case of heterogeneity) and intermediate basis vectors (in the case of anisotropy). The strain energy density is written in functional form as
6.7 Elastoplasticity of Grade Two
ρψ =Ψ =Ψ ( F La.α , F La.α :β , X , gα ) .
327
(6.230)
By assertion, the balance of mass in (4.10)(4.12) applies, as do (3.48)(3.50) and (6.2): (6.231) ρ0 = ρ J = ρ g / G det F = ρ J L J P , ρ = ρ J L = ρ 0 J P −1 . Contrarily, stress and traction definitions in Section 4.1.1, linear and angular momentum balances in Section 4.1.3, and the treatment of thermodynamics of crystalline solids in Sections 4.1.4 and 4.2 do not apply for the generalized continuum theory described in what follows in Section 6.7. In the present Section, entropy production and temperature rates are assumed to vanish; hence free energy and internal energy are considered equivalent to strain energy. Heat conduction, heat sources, and temperature gradients are not considered in the present Section. Internal state variables are not considered explicitly, but it will be demonstrated later in Section 6.7.3 that the skew part of the total covariant derivative of the lattice deformation is directly related to the dislocation density tensor for a crystalline solid and hence can be used to represent the strain energy contribution from dislocations. Furthermore, considered for simplicity in what follows is the quasistatic case, in which velocities and accelerations are omitted. Potential energies from conservative body forces are also omitted for simplicity of presentation, but these forces could be incorporated easily by subtracting the appropriate term from the Lagrangian. A Lagrangian density function L per unit intermediate volume V and Lagrangian functional L of (5.394) become simply L = −Ψ , L = ∫ LdV = −E = − ∫Ψ dV = − ∫ ρψ dV = − ∫ ρψ dv , (6.232) V
V
V
v
since kinetic energy K = 0 and global potential energy Φ = 0 by definition in the present simplified case. The appropriate generalization of Hamilton’s principle (5.380) is written as follows in the spatial configuration, in accordance with (5.421): t2 t2 ⎡ ⎤ ⎡ ⎤ δ A + ∫ ⎢ ∫ ( b iδ x ) dv ⎥ dt + ∫ ⎢ ∫ ( t iδ x + hi Dδ x ) ds ⎥ dt = 0 , (6.233) t1 ⎣ v t1 ⎣ s ⎦ ⎦ with h( x, t ) a generalized surface traction (force per unit spatial length) work conjugate to the normal derivative of the variation of spatial motion at the surface, Dδ xa = (δ xa );b nb (Teodosiu 1967a). Recall that the normal derivative D of an arbitrary function is introduced in (5.416), along with tangential derivative Da . The body force vector per unit current volume is b ( x, t ) , and t ( x, t ) is a surface traction (force per unit spatial area). Substituting from (6.232),
328
6 Elastoplasticity t2
t2
⎛
t1
t1
⎝V
⎞
δ A = δ ∫ L dt = δ ∫ ⎜ ∫ LdV ⎟ dt ⎠
⎛ ⎞ ⎛ ⎞ = − ∫ ⎜ ∫ δΨ dV ⎟ dt = − ∫ ⎜ ∫ δΨ ( J L −1dv) ⎟ dt , t1 ⎝ V t1 ⎝ v ⎠ ⎠ P P since δ V = δ ( J V ) = J δ V = 0 . Thus the equality t2
t2
− ∫ J L −1δΨ dv + ∫ baδ x a dv + ∫ ⎡⎣taδ x a + ha D (δ x a ) ⎤⎦ ds = 0 v
v
(6.234)
(6.235)
s
must hold for each time in the (arbitrary) interval t1 ≤ t ≤ t2 . The first integral on the left side of (6.235) can be written using (6.230) as ⎡ ∂Ψ ⎤ ∂Ψ δ ( F La.α :β ) ⎥ dv , (6.236) − ∫ J L −1δΨ dv = − ∫ J L −1 ⎢ La δ F La.α + La ∂F .α :β v v ⎣⎢ ∂F .α ⎦⎥ where the integrand on the right of (6.236) is expressed as follows: ∂Ψ ∂Ψ J L −1 L a δ F La.α + J L −1 La δ ( F La.α :β ) ∂F .α ∂F .α :β ⎡ ⎛ ⎞ ⎤ ∂Ψ ∂Ψ = ⎢ J L −1 La − ⎜ J L −1 La F Lb.β ⎟ ⎥ δ F La.α ⎟ ⎥ ∂F .α ⎜⎝ ∂F .α :β ⎢ ⎠;b ⎦ ⎣ ⎡ ⎤ ∂Ψ + ⎢ J L −1 La F Lb.β δ F La.α ⎥ ∂F .α :β ⎣⎢ ⎦⎥ ;b
(6.237)
⎡ ⎛ ⎞ ⎤ ∂Ψ ∂Ψ = ⎢ J L −1 La − ⎜ J L −1 La F Lb.β ⎟ ⎥ F Lc.α (δ x a );c ⎟ ⎥ ∂F .α :β ∂F .α ⎜⎝ ⎢ ⎠ ;b ⎦ ⎣ ⎡ ⎤ ∂Ψ + ⎢ J L −1 La F Lb.β F Lc.α (δ x a );c ⎥ , ∂F .α :β ⎢⎣ ⎥⎦ ;b which follows from the product rule, (6.219), (6.226), and (6.229), since ⎡ L −1 ∂Ψ ⎤ F Lb.β δ F La.α ⎥ ⎢J La ∂F .α :β ⎣⎢ ⎦⎥ ;b (6.238) ⎡ L −1 ∂Ψ ⎤ ∂Ψ Lb La L −1 La δ ( F .α :β ). = ⎢J F .β ⎥ δ F .α + J ∂F La.α :β ∂F L.aα :β ⎣⎢ ⎦⎥ ;b Secondorder stress tensor σ dc ( x, t ) and thirdorder hyperstress tensor H bdc ( x, t ) are defined, respectively, as follows:
6.7 Elastoplasticity of Grade Two
⎡
σ dc = g daσ a.c = g da ⎢ J L −1 ⎢ ⎣
329
⎛ L −1 ∂Ψ ⎞ ⎤ Lc ∂Ψ Lb ⎥ F .α , − J F ⎜ ⎟ .β ⎟ ∂F L.aα ⎝⎜ ∂F La.α :β ⎠;b ⎥⎦
(6.239)
∂Ψ F Lb.β F Lc.α . ∂F La.α :β
(6.240)
H bdc = g da H ab.c = J L −1 g da
The stress in (6.239) exhibits, in physical components, dimensions of force per unit spatial area or energy per unit spatial volume, while the hyperstress in (6.240) exhibits dimensions of force per unit spatial length or energy per unit spatial area. When (6.218) applies, ( J L −1 F La.α );a = 0 and H bdc = H cdb , but in general the hyperstress (6.240) consists of 27 independent components, in contrast to that of the holonomic theory in (5.428) for which such symmetry conditions hold. The rank two stress of (6.239) consists of up to 9 independent entries. The first and last contravariant indices of the hyperstress in (6.240) are transposed in the definition used by Teodosiu (1967a). Substituting stress definitions (6.239) and (6.240) into (6.236), J L −1δΨ = σ a.c (δ x a );c + ⎡⎣ H ab.c (δ x a );c ⎤⎦ ;b (6.241) .c a .c a = (σ a δ x );c − (σ a );c δ x + ⎡⎣ H ab.c (δ x a );c ⎤⎦ . ;b Applying the divergence theorem (2.193) in spatial coordinates leads to
{
}
− ∫ J L −1δΨ dv = − ∫ (σ a.cδ x a );c − σ a.c;cδ x a + ⎡⎣ H ab.c (δ x a );c ⎤⎦ dv ;b v
v
= ∫ σ a.c;cδ x a dv − ∫ ⎡⎣σ a.cδ x a + H ab.c (δ x a );b ⎤⎦ nc ds. v
(6.242)
s
Using (5.416)(5.418), Stokes’s theorem (2.198), and integration by parts, the rightmost term in the surface integral in (6.242) can be expressed as follows (Teodosiu 1967a), similarly to (5.431): b .c a b .c a a ∫ H a (δ x );b nc ds = ∫ H a [ D(δ x )nb + Db (δ x )]nc ds s
s
= ∫ H n n D (δ x a )ds − ∫ H ab.c (κ .dd nb nc − κ bc )δ x a ds b .c a b c
s
(6.243)
s
− ∫ Db ( H ac .b )ncδ x a ds, s
where Db ( H ) = H ac.;.bb − D( H ac .b ) nb is the surface gradient of the hyperc .b a
stress and κ bc = − Db nc is the symmetric second fundamental form of the oriented surface given in (5.418). Contravariant indices on the hyperstress
330
6 Elastoplasticity
in the final integrand of (6.243) are transposed with those of (5.431). Substituting (6.242) and (6.243) into (6.235), .c a b .c a ∫ (σ a;c + ba )δ x dv = ∫ ⎡⎣ H a nb nc − ha ⎤⎦ D(δ x )ds v
S
+ ∫ ⎡⎣σ n − H ab.c (κ .dd nb nc − κ bc ) − Db ( H ac.b ) nc − ta ⎤⎦ δ xa ds, .c a c
(6.244)
s
similarly to (5.432). Requiring that (6.244) must hold for arbitrary variations δ x a and normal surface variations D(δ x a ) , the following equilibrium equations and boundary conditions emerge: σ a.c;c + ba = 0 , (6.245) ta = σ a.c nc − H ab.c (κ .dd nb nc − κ bc ) − Dc ( H ab.c ) nb ,
(6.246)
(6.247) ha = H n n . Relation (6.245) is the static balance of linear momentum. Relation (6.246) is the boundary condition for the traction. Relation (6.247) is the boundary condition for the hypertraction. When H ab.c = H ac.b , (6.245)(6.247) are identical with (5.433)(5.435) as originally derived by Toupin (1962) in the context of second grade nonlinear elasticity. However, the stress and hyperstress of (6.239) and (6.240) entering these equilibrium equations and boundary conditions differ from those of Toupin (1962, 1964) and Section 5.7 since those used here are defined as derivatives of strain energy with respect to the lattice deformation and its covariant derivative as opposed to the total deformation and its covariant derivative. For the particular case when strain energy density does not depend on the total covariant derivative of the lattice deformation gradient, i.e., when (6.230) reduces to Ψ =Ψ ( F La.α , X , gα ) , the stress σ dc becomes identical to the Cauchy stress of nonlinear elastoplasticity (i.e., (6.27) and (6.239) become equivalent when the strain energy does not depend on internal state variables or F La.α :β ), and the hyperstress H bdc = 0 in (6.240). Thus, b .c a b c
in that particular case, (6.245) reduces to linear momentum balance (4.17) in the absence of spatial acceleration, traction boundary condition (6.246) becomes Cauchy’s relation (4.3), and the right side of (6.247) vanishes identically. A local balance of angular momentum can be obtained by forcing the strain energy density to remain invariant under rigid body rotations of the spatial frame, following procedures outlined in Sections 5.6 and 5.7. Consider a finite rotation F. Aa → Qˆ.ab F. Ab as discussed in Sections 4.2.1 and 5.6.2. From (6.8), the lattice deformation and its total covariant derivative transform in this case as F La.α → Qˆ .ab F Lb.α and F La.α :β → Qˆ .ab F Lb.α :β . An infini
6.7 Elastoplasticity of Grade Two
331
ac tesimal rotation is Qˆ .ab = δ .ba + gbc Ωˆ ac , where skew rotation Ωˆ ac = Ωˆ [ ] . According to Toupin (1964), invariance of the strain energy density under infinitesimal rotations is sufficient to ensure invariance under finite rotations. Extending (5.409), the differential change of strain energy density under small rotations is ⎡ ∂Ψ ⎤ ∂Ψ J L −1dΨ = J L −1 ⎢ F Lb.α + F Lb.α :β ⎥ dQˆ.ab a Le a Le ˆ ˆ ∂ (Q.e F .α :β ) ⎢⎣ ∂ (Q.e F .α ) ⎥⎦
⎡ ∂Ψ ⎤ ∂Ψ = J L −1 ⎢ La F Lb.α + F Lb.α :β ⎥ d Ωˆ .ba La ∂F .α :β ⎣⎢ ∂F .α ⎦⎥
(6.248)
⎡ ∂Ψ ⎤ ∂Ψ F L bα :β ⎥ d Ωˆ ab . = J L −1 ⎢ La F L bα + La ∂F .α :β ⎣⎢ ∂F .α ⎦⎥ Requiring that (6.248) must vanish under small but otherwise arbitrary roab tations d Ωˆ [ ] leads to the local balance of angular momentum for elasticplastic materials of grade two: ⎡ ∂Ψ ⎤ ∂Ψ L J L −1dΨ = 0 ⇒ J L −1 ⎢ L[ a F L b]α + F ⎥ = 0 . (6.249) b : α β ] a [ ∂F L.α :β ⎢⎣ ∂F .α ⎥⎦ From the product rule, the rank two stress in (6.239) can be expressed as ∂Ψ ∂Ψ σ a.b = J L −1 La F Lb.α + J L −1 La F Lc.β F Lb.α ;c ∂F .α ∂F .α :β ⎛ ⎞ ∂Ψ − ⎜ J L −1 L a F Lc.β F Lb.α ⎟ ⎜ ⎟ ∂F .α :β ⎝ ⎠;c
(6.250)
⎡ ∂Ψ ⎤ ∂Ψ F Lb.α :β ⎥ − H .ca.;bc . = J L −1 ⎢ La F Lb.α + La ∂F .α :β ⎣⎢ ∂F .α ⎦⎥ Substituting the antisymmetric part from (6.249) into (6.250) gives ⎡ ∂Ψ ⎤ ∂Ψ b c ab F L.α]:β ⎥ − H ...;[ c ] σ [ab] = J L −1 ⎢ L F L.bα] + L F F ∂ ∂ (6.251) ⎢⎣ ⎥⎦ [a α [ a α :β = H ...;[ c ] = M ...;abcc , c ba
where the rank three couple stress M abc and rank two couple stress md.c are constructed from certain antisymmetric parts of the hyperstress: 1 c ba c ba M abc = ε abd md.c = H [ ] , md.c = ε dab M abc = ε dab H [ ] = −ε dab H cab . (6.252) 2
332
6 Elastoplasticity
Local angular momentum balance (6.251) can thus be written as follows: 1 (6.253) σ [ab] − M ...;abcc = σ [ab] − ε abd md.c;c = 0 ⇔ ε abcσ ab − mc.d;d = 0 . 2 The symmetric part of the hyperstress, H c( ab ) = H cba − M abc , while not affecting the angular momentum balance, does not generally vanish and is considered to result from a distribution of selfequilibrating internal forces. Relations (6.252) and (6.253) differ from (5.440) and (5.441) due to different ordering of indices on the definitions of hyperstress and couple stress. Only when H ab.c = H ac.b , as would result from compatibility conditions (6.218) on the lattice deformation, do the two sets of relations coincide. A frame indifferent version of strain energy function (6.230) is (Teodosiu 1968) L L (6.254) Ψ =Ψ Eαβ , Bαβχ , X , gα ,
(
)
where the symmetric lattice strain 2 Eαβ = Cαβ − gαβ = F La.α g ab F Lb.β − gαβ as L
L
in (6.4), and the covariant second lattice gradient (i.e., a kind of strain and rotation gradient) referred to the intermediate configuration satisfies L (6.255) Bαβχ = F L aα F L.aβ :χ Contravariant hyperstress and stress tensors are then computed, respectively, from the chain rule as L Le ∂Ψ ∂ ( F eχ F .δ :ε ) Lb Lc H bdc = J L −1 g da L F .β F .α ∂F La.α :β ∂Bχδε (6.256) L −1 ∂Ψ Ld Lb Lc F . χ F .β F .α , =J L ∂Bχαβ L L ⎡ ∂Ψ ∂Eχδ ∂Ψ ∂Bχδε ⎤ Lc F .α + La La ⎥ L L ⎣⎢ ∂Eχδ ∂F .α ∂Bχδε ∂F .α ⎦⎥
σ dc = g da J L −1 ⎢
L ⎡⎛ ⎞ ⎤ Lc ∂Ψ ∂Bχδε Lb ⎥F F − g da ⎢⎜ J L −1 L .β ⎟ ⎟ ⎥ .α ∂Bχδε ∂F L.aα :β ⎢⎜⎝ ⎠ ; b ⎣ ⎦
=J
L −1
⎡ ∂Ψ Ld ⎤ Lc ∂Ψ Ld ⎢ L F . χ + L F β :χ ⎥ F .α ∂Bαβχ ⎢⎣ ∂Eαχ ⎥⎦
(6.257)
⎡⎛ ⎞ ⎤ ∂Ψ − ⎢⎜ J L −1 L F Ld. χ F Lb.β ⎟ ⎥ F Lc.α . ⎟ ⎥ ∂Bχαβ ⎢⎜⎝ ⎠ ;b ⎦ ⎣ As an illustrative simple example, strain energy density (6.254) is written as a Taylor series expansion to second order in lattice strains and sec
6.7 Elastoplasticity of Grade Two
333
ondorder lattice deformation gradients about a reference state at which F La.α = g.aα and F La.α :β = 0 :
Ψ =Ψ 0 +
αβ
L L Eαβ + Dαβχ Bαβχ +
1 2
αβχδ
L L Eαβ Eχδ
(6.258) 1 αβχδεφ L L L αβχδε L + D Bαβχ Bδεφ + K Eαβ Bχδε , 2 where Ψ 0 =Ψ (0,0, X , gα ) is the strain energy density per unit volume at the reference state and the constant material coefficients at a material point X are defined as αβ
=
∂Ψ L ∂Eαβ
, Dαβχ = EL = 0 BL = 0
Dαβχδεφ =
∂ 2Ψ L ∂Bαβχ ∂Bδεφ L
∂Ψ L ∂Bαβχ
,
αβχδ
EL = 0 BL =0
, Kαβχδε = EL = 0 BL = 0
=
∂ 2Ψ L L ∂Eαβ ∂Eχδ
∂ 2Ψ L L ∂Eαβ ∂Bχδε
,
(6.259)
EL = 0 BL = 0
.
(6.260)
EL = 0 BL = 0
A natural state in which both the stress and hyperstress vanish everywhere may not exist for a given material, and such a state may be an exceptional case rather than the norm. None of the constants in (6.259) and (6.260) need vanish entirely in general, though certain symmetry properties result L automatically from Eαβ = E(Lαβ ) . Spatial invariance of (6.254) ensures that (6.249) and angular momentum balance (6.253) are satisfied identically. 6.7.3 Relationship to Dislocation Theory
Recall from Section 3.3.2 the definitions of the secondorder geometrically necessary dislocation density tensor referred to B , specifically (3.222) and (3.224) that combine to yield α αβ = J L ε abc F L −1α.b ,c F L −1.βa = J Lε abc F L −1α.d ( F Ld. χ F L −1.χb ,c ) F L −1.βa = J L ε abc F L −1α.d Γ cb..d F L −1.βa
(6.261)
= J L ε abc F L −1α.d Tcb..d F L −1.βa , where the torsion of the crystal connection is, from (3.190) and (3.191), Tbc..a = Γ [..bca ] = F La.α ∂ [b F L −1α.c] (6.262) = F La.α F L −1α.[c ,b] = − F La.α ,[b F L −1α.c] .
334
6 Elastoplasticity
From (6.217), the skew part of the total covariant derivative of the lattice deformation is g
F La.[α :β ] = (Γ
.. a bc
1 g = (Γ 2 1 g = (Γ 2 g
= (Γ
− Γ bc..a ) F Lc.[α F Lb.β ] − Γ
.. χ
[ βα ] F
La .χ
.. a bc
− Γ bc..a )( F Lc.α F Lb.β − F Lc.β F Lb.α )
.. a bc
−Γ
.. a [bc]
g
.. a cb
− Γ bc..a + Γ cb..a )( F Lc.α F Lb. β )
(6.263)
− Γ [..bca ] ) F Lc.α F Lb.β
= Tcb..a F Lc.α F Lb.β , g
since Γ
.. a [bc ]
= 0 by definition (2.58), and where Γ
.. χ
[ βα ] = 0 ,
i.e., an external
intermediate coordinate system with symmetric connection has been assumed. Combining (6.261)(6.263), the dislocation density tensor can be expressed as α αβ = J Lε abc F L −1α.d ( F L −1cχ. F Ld.[ χ :δ ] F L −1δ.b ) F L −1.βa . (6.264) Assume next for illustrative purposes that the strain energy density of (6.230) depends on the covariant derivative of the lattice deformation gradient only through the dislocation density tensor: Ψ =Ψ ( F L.aα ,α αβ ( F La.α , F La.α :β ), X , gα ) . (6.265) Stress (6.239) and hyperstress (6.240) then become, in this particular case, ⎡ ⎛ ⎞ ⎤ ∂Ψ ∂Ψ ∂α χδ σ dc = g da ⎢ J L −1 La − ⎜ J L −1 χδ F Lb.β ⎟ ⎥ F Lc.α La ⎟ ⎥ ∂F .α ⎜⎝ ∂α ∂F .α :β ⎢ ⎠;b ⎦ ⎣ ∂Ψ = J L −1 g da (6.266) F Lc.α La ∂F .α
⎛ ∂Ψ ⎞ α β − g da ⎜ χδ ε fgh F L −1.χa F L −1[.h F L −1.g] F L −1δ. f F Lb.β ⎟ F Lc.α , ⎝ ∂α ⎠;b H bdc = J L −1 g da = J L −1 g da = g da
∂Ψ ∂α χδ F Lb.β F Lc.α ∂α χδ ∂F La.α :β ∂Ψ α β ( J Lε fgh F L −1.χa F L −1[.h F L −1. g] F L −1δ. f ) F Lb.β F Lc.α (6.267) ∂α χδ
∂Ψ bd c (ε fbc F L −1.χa F L −1δ. f ) = H [ ] , ∂α χδ
6.7 Elastoplasticity of Grade Two
335
since from (6.264), ∂α χδ ∂ = [ J Lε abc F L −1.χd ( F L −1.εc F L .d[ε :φ ] F L −1φ.b ) F L −1δ.a ] Le ∂F .α :β ∂F Le.α :β = J Lε abc F L −1.χd F L −1.εcδ .de δ .α[ε δ .φβ] F L −1φ.b F L −1δ.a
(6.268)
= J Lε abc F L −1.χe F L −1.[cα F L −1.βb] F L −1δ.a . From (6.267), the hyperstress consists of only 9 independent components when (6.265) is used in place of (6.230). The hyperstress vanishes when dislocation density (6.261) vanishes, in which case ∂Ψ / ∂α χδ = 0 . Relationships between hyperstress or couple stress and dislocation density were derived by Kroner (1963b). Garikipati (2003) demonstrated relationships among slip gradients, threebody terms in interatomic potentials reflecting bond angle dependence of interatomic forces, and hyperstresses in the context of Toupin’s nonlinear elastic theory of grade two (Toupin 1962). The approach outlined Section 6.7 accounts for the second grade hyperelastic response of the material from intermediate configuration B , but does not account for evolution of this intermediate configuration, since kinetic relations for the time rate of plastic deformation, F P , are not addressed. Postulation of such relations in a thermodynamically admissible manner requires consideration of the dissipation equality and thermal effects, phenomena which are excluded by use of Hamilton’s principle for conservative systems (Eringen 1962). More recent approaches considering dissipative thermodynamics of materials whose free energy may depend on higherorder gradients of lattice deformation include those of Le and Stumpf (1996b, c), Bammann (2001), Regueiro et al. (2002), and Clayton et al. (2004b, 2006). In these approaches, generalized conservation laws for momentum and energy are often postulated directly rather than derived from the first variation of an action integral. Presumably, the kinetic law for the rate of plastic deformation should include a dependence on tensors F La.α :β or α αβ , since geometrically necessary dislocations are thought to affect strain hardening (Ashby 1970; Fleck and Hutchinson 1993; Fleck et al. 1994; Steinmann 1996; Gao et al. 1999; Gurtin 2000, 2002; Acharya 2001; Regueiro et al. 2002; Voyiadjis and Abu AlRub 2005; Abu AlRub and Voyiadjis 2006). Zubelewicz (2008) developed a constitutive model, based on nonequilibrium thermodynamics and a measure of slip incompatibility, for describing heterogeneous dislocation microstructures and strong dynamic strain hardening that emerge in crystalline metals subjected to shock loading. A complete continuum theory incorporating dependence of thermodynamic potentials and kinetic relations on the dislocation density tensor, as well as the disclination density tensor (see Section
336
6 Elastoplasticity
3.3.3), is presented later in Section 9.4 of Chapter 9, a Chapter dealing with inelasticity theories of a more general scope.
7 Residual Deformation from Lattice Defects
An element of crystalline material through which a net flux of dislocations has passed exhibits plastic shape change. Dislocation lines within the element, i.e., displacement discontinuities across the slip plane in the context of Volterra defects may also contribute to this plastic deformation. However, plastic deformation, according to traditional definitions, does not address additional changes in dimensions of the body resulting from residual elastic deformation associated with local stress fields induced by defects. Mura (1982) labels these local, selfequilibrated stresses (i.e., residual stresses) eigenstresses. Dislocation glide preserves the volume of the crystal, and purely tangential displacement discontinuities such as crystallographic slip do not alter the volume occupied by the material. Yet ample evidence suggests that dislocation lines affect the total volume of crystals (Zener 1942; Schmid and Boas 1950; Holder and Granato 1969; Wright 1982). Stored energies associated with elastic fields of defects are important because they affect recrystallization (Schmid and Boas 1950; Taheri et al. 2006) and the fraction of stress power converted to temperature rise at high deformation rates (Rosakis et al. 2000) that can result in shear localization in metals during dynamic failure events. Large numbers of dislocations, twins, and stacking faults can be generated during shock or impact loading (Rohatgi and Vecchio 2002), and presumably the corresponding volume changes, shape changes, and stored energies associated with local stress fields of these defects affect the observed material response under such conditions (Clayton 2009a, c). Defects of interest in Sections 7.17.3 of Chapter 7 are those that can be described by displacement discontinuities tangential to an internal surface (i.e., crystallographic plane) in a volume element of the solid. These include gliding straight or curved dislocations lines, dislocation loops, as well as partial dislocations. Motion of dislocations through a region of the crystal results in plastic shape change as mentioned above, but preserves the lattice spacing (Bilby and Smith 1956; Bilby et al. 1957), as discussed in detail in Section 3.2 of Chapter 3; this requires cooperative motion of leading and trailing partials for the case of partial dislocations. Residual elastic stress fields from disclination lines and loops are also considered in
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_7, © Springer Science+Business Media B.V. 2011
337
338
7 Residual Deformation from Lattice Defects
Chapter 7, though their contribution to the plastic shape change (Li and Gilman 1970) is not addressed explicitly here. Considered in Section 7.4 are point defects (Eshelby 1954, 1956) that may have finite intrinsic volumes (e.g., volume changes per defect on the order of the atomic volume). In Chapter 7, a threeterm decomposition of the deformation gradient, F = F E F I F P , is assigned to describe the kinematics of a volume element of crystalline material containing lattice defects, following (3.137). In order to delineate residual elastic deformation from recoverable elastic deformation and from plastic deformation, terms entering this decomposition are defined in a precise manner in Section 7.2. Some repetition of definitions given in Chapter 3 is unavoidable. For simplicity, isothermal conditions are assumed throughout Chapter 7, meaning thermal expansion is omitted. Elastic tangent map F E accounts for deformation due to applied stresses as well as rigid body rotations of the lattice. Plastic tangent map F P results from the cumulative effects of fluxes of dislocations (Orowan 1940; Mura 1968; Lardner 1969) and from slip discontinuities associated with defects within the element (Teodosiu 1970; Rice 1971). Intermediate term F I (or its stretch or rotational components) has been introduced in a number of works with various definitions (Kratochvil 1972; Bammann 2001; Regueiro et al. 2002; Clayton and McDowell 2003a; Hartley 2003; Clayton et al. 2004b, 2005, 2006; Gerken and Dawson 2008). In Section 3.2.9, a derivation of F I was obtained in (3.148) by volume averaging local continuum fields over an element of a (poly)crystal featuring elasticplastic responses of the form in (3.145) at a lower length scale. In contrast, F I as defined in Chapter 7 represents the average residual elastic deformation of the element of crystal induced by the local stress and strain fields of the defects contained within it. Thus, in Chapter 7, it corresponds exactly to the volume average of the residual elastic deformation in the context of defect field theories (Kroner and Seeger 1959; Willis 1967; Teodosiu 1982). In Section 7.2, the externally unloaded volume element of crystalline material is treated as a hyperelastic body of grade one with homogeneous elastic constants, in static equilibrium, and containing internal displacement discontinuities across which traction is continuous. The element is free of external traction but may support internal (i.e., residual) stresses. Selfequilibrium conditions result in an integral equation for F I . For linear elastic constitutive behavior, F I reduces to the unit tensor in rectangular Cartesian coordinates, but F I does not so reduce for nonlinear constitutive behavior. Analytical elasticity solutions for defect energies (Appendix C) are considered along with experimental data (Clarebrough et al. 1957)
7.1 Multiplicative Kinematics
339
to confirm accuracy of the theory for predicting residual volume changes associated with line defects. In Section 7.3, the externally unloaded volume element is identified as a set of discrete atoms in static equilibrium and free of external forces. The lattice statics description of Section B.2 in Appendix B applies. According to this description, interatomic forces vanish in a perfect crystal free of defects, but nonzero forces may exist among atoms when they are arranged in an imperfect way (i.e., when defects are present). The selfequilibrium conditions are equivalent to vanishing of static components of the average virial stress for the set of atoms (Huang 1950; Zhou 2003). When atomic interactions are harmonic, equilibrium demands that F I as defined in Section 7.3 should reduce to the unit tensor. In the more general case of anharmonic interactions that may be physically significant in the vicinity of defect cores where large atomic displacements arise, the derivations in Section 7.3 suggest that F I could be nonnegligible. In Section 7.4, average deformations of an element of crystal containing a distribution of point defects are addressed. Multiplicative decomposition (3.128) applies, F L = F E F V , with F V accounting for volume changes from point defects and F L the total lattice deformation. The total volume change per point defect is derived by combining the volume change per defect predicted by the linear elastic sphereinhole model of Section C.3 of Appendix C (Bitter 1931; Teodosiu 1982) with a correction for nonlinear elasticity (Eshelby 1954; Holder and Granato 1969). Analytical solutions are considered with experimental data (Nilan and Granato 1965) to confirm accuracy of the theory for predicting residual volume changes associated with vacancies.
7.1 Multiplicative Kinematics Consider a volume element of a crystal containing lattice defects. This element is larger than the average atomic spacing, but may be of smaller dimensions than the entire crystal. Static (i.e., null inertia) and isothermal conditions are assumed. Deformation of the element is described by mappings between tangent spaces of configurations, as shown in Fig. 7.1. Reference configuration B0 is treated as a perfect lattice. The position vector R j of atom j (e.g., the equilibrium position of its nucleus) relative to the origin of a Cartesian coordinate system in an infinite lattice in the reference configuration is given by periodicity relations (3.4) and (B.38):
340
7 Residual Deformation from Lattice Defects
R
3
j
= R ( lk ) = R ( 0k ) + R ( l ) = ∑ (mi + l i ) A i , ( l i ∈ ] , 0 ≤ mi < 1 ).
(7.1)
i =1
In (7.1), R (0k ) is a basis vector for atom k of the basis at each Bravais lattice point, R (l ) is a Bravais lattice vector denoting the position of primitive unit cell l, and Ai is a primitive Bravais lattice vector. Recall that in a monatomic lattice with one atom per unit cell, basis vectors are redundant and R (0k ) = 0 , though the treatment of Chapter 7 is not restricted to monatomic crystal structures.
Fig. 7.1 Configurations, surface coordinates and tractions, and tangent maps
7.1.1 Plastic Deformation Intermediate configuration B in Fig. 7.1 differs from B0 as a result of influences of cumulative motion of lattice defects and perturbations of atomic positions resulting from these defects. Configuration B is by definition free of external traction ( t = 0 ) and free of internal stresses. For a crystal containing a single dislocation, a singular plastic deformation map can be defined as in (3.85): F P = 1 + b ⊗ Mδ X, M χ , (7.2) where 1 is the unit tensor, b is the Burgers vector, M is the normal to the slip surface in the reference configuration, δ (.) is Dirac’s delta function, and χ is the characteristic function that is unity at reference coordinates X on slipped surface Σ and zero elsewhere. The Cartesian coordinate sys
7.1 Multiplicative Kinematics
341
tem for X is chosen with its origin in the slip plane. A singular dislocation density tensor corresponding to (7.2) and first listed in (3.86) is α 0 = b ⊗ ξ 0δ ( L ) , (7.3) where ξ 0 is the unit tangent to dislocation line of length L in the reference configuration. For a collection of j straight stationary dislocation line populations of density (length per unit reference volume) ρ0i , Burgers vector b i , and unit tangent ξ i , dislocation density (7.3) can be extended to 0
j
α 0 = V −1 ∫ b ⊗ ξ 0 dL = ∑ ρ 0i b i ⊗ ξ i0 ,
(7.4)
i =1
L
as indicated in (3.87). The total volume occupied by the crystal element in the reference configuration is denoted by V. The second of (7.4) pertains to a total of j dislocation populations with the same tangent line and local Burgers vector for each value of i. A more general definition, first listed in (3.97), of average plastic deformation accounts for the history of generation and motion of defects within a material element, in which case F P = LP F P , F P = 1. (7.5) t =0
P
The average plastic velocity gradient L is dictated by the flux ς of mobile dislocations as in (3.98)(3.99), written in indicial notation as j
LPα.β = ςαχδ ε χδβ , ςαχδ = V −1 ∫ b iα ξ i χ v iδ dL = ∑ ρ i b iα ξ iχ v iδ ,
(7.6)
i =1
L
where ξ i and v i are respectively the uniform tangent line and velocity of every dislocation in population i. Since dislocation segments have perpendicular velocities and tangent lines, the isochoric plastic deformation conditions J P = J P tr(LP ) = 0 and J P = 1 follow automatically from (7.6). In i , the unit normal to the slip plane and s i , a troducing two quantities— m unit vector in the direction of slip—(7.6) reduces to (3.100), as typically encountered in crystal plasticity theory of Sections 3.2.6 and 6.3: i = ∑ γ i s i ⊗ m i. LP = ∑ ρ i b i v i s i ⊗ m (7.7) i
i
i , again J P = 0 and J P = 1 . In summary, according to deSince s i ⊥ m scriptions in terms of single dislocations (7.2), dislocation flux (7.6), or crystal plasticity (7.7), plastic deformation is always isochoric.
342
7 Residual Deformation from Lattice Defects
7.1.2 Lattice Deformation Let F E denote the tangent map to externally stressed configuration B , as denoted generally by t ≠ 0 in Fig. 7.1, from selfequilibrated configuration B , with t = 0 in Fig. 7.1. Let ai denote a primitive Bravais lattice vector of (7.1) mapped to intermediate tangent bundle TB : ai = F I A i , aiα = F I .αβ g.βA AiA
(7.8)
with g.βA the shifter between coordinate frames in B0 and B , omitted in the direct tensor notation in the first of (7.8). When coincident coordinate systems are used in these two configurations, g.βA = δ .βA . Note that lattice vectors are not affected by F P , in accordance with (3.107). Lattice vectors deform from TB to TB according to (3.109): ai = F E ai = F L A i , aia = F E .aα aiα = F Lα.β g.βA AiA . (7.9) where the total lattice deformation for the volume element is F L = F E F I . Under a homogeneous deformation, basis vectors R (0k ) in (7.1) deform similarly to primitive Bravais lattice vectors Ai in (7.8) and (7.9), and the final position of atom j may also change by a translation that is uniform for each species in the basis but that may differ among species (Born and Huang 1954). This translation may be due, for example, to polarization in an applied electric field or inner displacements among sublattices in a noncentrosymmetric polyatomic crystal (Cousins 1978). Relations (7.8) and (7.9) generalize the CauchyBorn hypothesis (Born and Huang 1954) of Section 3.1.2, distinguishing effects of recoverable ( F E ) and residual ( F I ) deformations. Rigid body rotations of the element are included in the rotational part of the polar decomposition of F L , denoted by R L . Reference Bravais lattice vectors Ai are uniform with respect to position in a sample of a perfect single crystal. However, when defects are contained within the volume, deformed primitive lattice vectors ai and ai represent suitable averages of local lattice vectors a′i and ai′ that may not be spatially constant, just as in (3.111): ai = V −1 ∫ a′i dV , ai = V −1 ∫ ai′dV . (7.10) V
V
By cutting the volume element out of the stressed body thereby relieving the external traction, relaxing any possible internal viscous and inertial forces, and then rotating this element by R E −1 , configuration B can be obtained from spatial configuration B. If experiments could be performed in which the average lattice vectors were measured in each of configurations
7.1 Multiplicative Kinematics
343
B0 , B , and B, then (7.8) and the first of (7.9) would each provide nine equations involving nine unknown components of F I or F E . However, configuration B can only be realized for a solid with a heterogeneous internal stress field by removing all traction from the surface of each microscopic, residually stressed subelement within that solid, physically corresponding to cutting or breaking it into small parts (Eckart 1948), in practice a prohibitively destructive laboratory experiment. In Sections 7.2 and 7.3, theoretical methods are offered for computing F I that, in principle, would alleviate the need for such difficult experiments.
7.1.3 Multiplicative Decomposition of Total Deformation The total deformation F is defined by the surface integral (Hill 1972, 1984; Clayton and McDowell 2004) F = V −1 ∫ x ⊗ NdS , (7.11) S
where x are spatial coordinates of the deformed image of reference surface S enclosing the volume element with unit outward reference normal N, as illustrated in Fig. 7.1. The volume element may contain discontinuities in the internal displacement field and gradients of displacement; when such discontinuities are absent and after Gauss’s theorem (2.194) is applied, (7.11) reduces to F. Aa = V −1 ∫ x.,aA dV , where x a = x a ( X A , t ) are now differentiable functions of reference position X within volume element of reference volume V. In contrast to notation used in Chapter 2, capital symbols are reserved in Chapter 7 for the total (average) deformation gradient F for a volume element and its constituents: F E , F I , F L , and F P . In contrast, the local deformation gradient within the volume element is written in Chapter 7 as x.,aA . Assume that the total deformation gradient F is imposed on a volume element of material via (7.11), and that the decomposition F = FEF I F P = FLF P (7.12) P applies, as implied by Fig. 7.1. Plastic deformation F is known from integration of (7.5) with (7.6) or (7.7), presuming kinetic laws are available for the mobile dislocation velocity, for example those described in Section 6.2, or slip rates on each slip system, for example those described in Section 6.3. Under isothermal conditions, the crystal in a particular orientation responds to applied loading elastically such that Σ = Σ ( UE ) ⇔ UE = UE ( Σ ) , (7.13)
344
7 Residual Deformation from Lattice Defects
where stretch tensor U E = R E −1F E = (F ET F E )1/ 2 is an invertible function of conjugate stress measure Σ that vanishes when the traction t = 0 along deformed surface s of the element in Fig. 7.1. The particular form of (7.13) will depend upon the orientation of the lattice in B (e.g., choice of coordinate system with respect to orientation of the sample) because of anisotropy. For example, for a hyperelasticplastic solid with nonvanishing second and thirdorder elastic constants, (7.13) can be interpreted as a version of (6.56) pushed forward to configuration B , in the absence of temperature changes. Henceforth in Chapter 7 it is assumed that FL = R E U EF I = R L U E U I , FI = UI , (7.14) I meaning that F is a stretch (e.g., a symmetric tensor with six independent entries in covariant Cartesian coordinates) and that all lattice rotation is embedded in R E . The objective of Sections 7.2 and 7.3 is determination of analytical approaches to obtain F I . If F P is also known at a particular instant, F E = FF P −1F I −1 can then be found from (7.12) and the average external stress supported by the element can be updated according to elastic constitutive relation (7.13).
7.2 Nonlinear Elastic Interpretation of Residual Elasticity The dimensional changes of a nonlinear elastic body in a state of selfstress, i.e., a selfequilibrated body with internal residual stresses but no traction applied to its external boundaries, are derived in Sections 7.2.17.2.3. The body may contain one or more internal surfaces across which traction is continuous but tangential displacements are not. The treatment is specialized in Section 7.2.4 to address volume changes in cubic crystals and isotropic materials. Formulae for volume changes attributed to local elastic stress fields of line defects are derived in the isotropic approximation in Section 7.2.5. Derivations and discussion in Sections 7.2.17.2.5 consolidate and extend prior work of a number of authors (Zener 1942; Seeger and Haasen 1958; Toupin and Rivlin 1960; Holder and Granato 1969; Teodosiu 1982; Clayton and Bammann 2009). Additional analysis and examples follow in Sections 7.2.6 and 7.2.7. Since the derivations frequently involve integration of vector and tensor fields over regions of space occupied by the body, coincident Cartesian coordinates are used throughout the remainder of Chapter 7 unless noted otherwise. The procedure of Toupin (1956) outlined in (3.95) and (3.96) could be used instead
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
345
if curvilinear coordinates are desired, but such steps are omitted in order to provide a more concise presentation.
7.2.1 Selfequilibrium Conditions Local balance of linear momentum (4.21) is written in rectangular Cartesian coordinates as P..,aAA + B a = ρ0 Aa , (7.15) with B a the body force per unit reference volume, ρ 0 the reference mass density, and Aa the material acceleration. In reference coordinates X A , application of the product rule then provides the local relation ( X A P aB ) , B = P aA + ( ρ0 Aa − B a ) X A . (7.16) Consider a body of reference volume V with external surface S. The body may contain internal surfaces across which the motion x a ( X , t ) from the reference state (e.g., a perfect lattice), deformation gradient x.,aA ( X , t ) , and stress components are generally discontinuous, but traction per unit reference area t0a of (4.4) across internal surfaces is continuous: ct a f = t + a − t − a = ( P + aA − P − aA ) M = 0 , (on Σ ), (7.17) 0 A ed 0 hg 0 where + and – denote limiting values of a quantity near the surface as it is approached from either side, M A is a unit normal covariant vector to an internal surface, and Σ denotes the union of such internal surfaces. The source of displacement discontinuities across Σ is arbitrary in (7.17); for the particular case of dislocation(s) within V, jump(s) in displacement across slip planes comprising Σ are attributed to Burgers vector(s) introduced in (7.2). Integrating (7.16) over V and applying the divergence theorem, aA A aB A + aB − aB ∫ P dV = ∫ X P N B dS + ∫ X ( P − P ) M B d Σ V
Σ
S
(7.18)
+ ∫ X ( B − ρ 0 Aa ) dV , A
a
V
where N B are components of the external normal to V along S as introduced in (7.11). Applying (4.4) and (7.17) and considering a body in static equilibrium, aA A aB a A (7.19) ∫ P dV = ∫ X P N B dS = ∫ t0 X dS . V
S
S
For a selfequilibrated body, t0a = 0 by definition, and (7.19) reduces to
346
7 Residual Deformation from Lattice Defects
V −1 ∫ P aA dV = 0 ,
(7.20)
V
meaning that the volumeaveraged first PiolaKirchhoff stress vanishes over the reference volume. Now consider the spatial balance of linear momentum σ ..,abb + b a = ρ a a , (7.21) with σ ab = det( X .,Aa ) P aA x.,bA the symmetric local Cauchy stress tensor, b a the body force per current volume, ρ = ρ 0 det( X .,Aa ) the current mass den
sity, and a a the spatial acceleration. Spatial analogs of (7.16)(7.18) are ( x bσ ac ) ,c = σ ab + ( ρ a a − b a ) x b , (7.22) ct a f = t + a − t − a = (σ + ab − σ − ab )m = 0 , (on σ ), (7.23) b ed hg
∫σ v
ab
dv = ∫ xbσ ac nc ds + ∫ xb (σ + ac − σ − ac ) mc dσ + ∫ xb (b a − ρ a a ) dv , (7.24) σ
s
v
with x a = x a ( X , t ) spatial coordinates, t a the traction per unit current area of (4.3), σ the union of internal surfaces across which reference coordinates X A ( x, t ) may be discontinuous functions of spatial position and inverse deformation gradient X .,Aa may be singular, ma the unit normal covector to such surfaces, na the unit normal covector to external surface s (Fig. 7.1), and v the spatial volume of the body enclosed by s. For a body in static equilibrium, (7.24) becomes ab b ac a b (7.25) ∫ σ dv = ∫ x σ nc ds = ∫ t x ds , v
s
s
and for a selfequilibrated body , by definition t a = 0 along s, and hence the average Cauchy stress vanishes by (7.25): v −1 ∫ σ ab dv = 0 . (7.26) v
Relation (7.26) was derived by Toupin and Rivlin (1960) and Hoger (1986) in the context of residually stressed bodies. 7.2.2 Hyperelasticity
In the present treatment, the local, mechanically reversible part of the constitutive response of the material is assumed hyperelastic of grade one, with effects of temperature change neglected. Let Ψ 0 =Ψ 0 ( E AB ) denote the strain energy per unit reference volume of the solid, with the symmetric right CauchyGreen strain of (2.156) in Cartesian coordinates
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
347
1 1 E AB = ( x.,aAδ ab x.,bB − δ AB ) = δ .aAu( a , B ) + uc , Au.,cB , (7.27) 2 2 where u a = x a − δ .aA X A is the local displacement of (2.137) when coincident coordinate systems are used in each configuration. Let 1 1 Ψ 0 = ^ ABCD E AB ECD + ^ ABCDEF E AB ECD EEF + ... , (7.28) 2 6 where second and thirdorder elastic constants are evaluated from a series expansion of the energy density about the unstrained state as in (5.65) and (5.66). The local first PiolaKirchhoff stress, from (5.45) and (7.28), is computed as ∂Ψ 0 ∂Ψ 0 ∂Ψ 0 = x.,aB = x.,aB P aA = ∂xa , A ∂EBA ∂E AB (7.29) 1 ABCDEF ⎞ a ⎛ ABCD = x., B ⎜ ^ ECD + ^ ECD EEF + ... ⎟ . 2 ⎝ ⎠ Using symmetry properties in (5.57) and (5.58) and omitting terms of degree higher than three in referential displacement gradient (i.e., distortion) u A, B = δ .bAub , B , strain energy function (7.29) can be written (Toupin and Rivlin 1960) 1 1 1 Ψ 0 = ^ ABCD u A, B uC , D + ^ ABCD u A, B uE ,C u.,ED + ^ ABCDEF u A, B uC , D uE , F . (7.30) 2 2 6 7.2.3 Average Residual Elastic Strain Consider the externally unloaded configuration of the volume element labeled B in Fig. 7.1. This configuration corresponds to the deformed but selfequilibrated body obeying (7.20) and (7.26). The reference configuration with internal displacement discontinuities described in (7.2)(7.4) now corresponds to stressfree intermediate configuration B of Fig. 7.1. As discussed in detail in Section C.1 of Appendix C and noted by De Wit (1973), displacement discontinuities attributed to Volterra dislocations lead to discontinuities or singularities in local plastic strain and rotation fields across the slip planes or internal surfaces Σ within the volume, which owing to the isochoric nature of slip, is preserved via V = J PV = V . Such effects are quantified according to (3.85)(3.90) and (7.2)(7.4), wherein discontinuities or singularities are introduced by plastic deformation F P between configurations B0 and B . Residual deformations are introduced within the element from the mapping between configurations B
348
7 Residual Deformation from Lattice Defects
and B . Locally1, such deformations are treated as differentiable and elastic between B and B , with corresponding local displacement gradient and Lagrangian strain fields (i.e., eigenstrains) within the element denoted by u A, B and E AB , respectively. The corresponding definition for the average residual elastic deformation gradient entering (7.12) and (7.14) is, in Cartesian coordinates (Clayton and Bammann 2009) F I AB = V −1 ∫ x( A, B ) dV = δ AB + V −1 ∫ u( A, B ) dV . (7.31) V
V
Singular surfaces Σ and singular lines (e.g., defect cores) are excluded from the domain of integration V in (7.31). Contributions to F from singular surfaces (e.g., plastic slip) are incorporated via plastic deformation map F P , not F I . Relation (7.31) is a key definition used often later. In generalized coordinates, F I = F I AB G A ⊗ G B = F I AB ( g Aα g α ⊗ g.Bβ g β ) = F I α.β g α ⊗ g β . (7.32) Mapping selfequilibrium conditions (7.26) to the reference configuration and substituting from (7.29), ∂Ψ 0 δ .aAδ .bB ∫ σ ab dv = δ .aAδ .bB ∫ x.,bC P aC dV = ∫ (δ .CB + u.,BC ) dV = 0 . (7.33) u A,C ∂ v V V The integral on the right side of (7.33) becomes, upon substitution of (7.30) and omission of terms higher than second order in displacement gradients in the expression for the stress, ∂Ψ 0 0 = ∫ (δ .CB + u.,BC ) dV = ∫ ^ ABCD uC , D dV ∂ u A, C V V
+ ∫ (^ AECD u.,BE + ^ BECD u.,AE )uC , D dV
(7.34)
V
1 1 ^ ABCD u E ,C u.,ED dV + ∫ ^ ABCDEF uC , D u E , F dV . ∫ 2V 2V When products of order two in displacement gradients are omitted, as would be the case for a linear elastic body with spatially constant moduli, (7.34) reduces to ^ ABCD ∫ uC , D dV = 0 ⇒ ∫ u(C , D ) dV = 0 ⇒ F I CD = δ CD (7.35) +
V
V
In configuration B , if defects are envisioned within the element, u A ( X , t ) is a discontinuous function of position X across singular surfaces, and hence u A, B is 1
singular along such surfaces (recall Fig. 3.11). Thus u A is globally discontinuous.
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
349
since ^ ABCD is assumed positive definite. The linear elastic approximation (7.35) states that no average elastic shape or volume change occurs in a selfequilibrated body with homogeneous elastic properties. The latter would be true even if the local elastic dilatation from defects does not vanish, as is exhibited in straight line edge dislocation and wedge and twist disclination solutions in (C.35), (C.107), and (C.140) for linear elastic isotropic bodies. On the other hand, for a nonlinear elastic body with spatially constant moduli, components of the integrated symmetric displacement gradient are given by the six independent integral equations ^ ABCD ∫ u( C , D ) dV = −^ AECD ∫ u.,BE uC , D dV − ^ BECD ∫ u.,AE uC , D dV V
V
V
1 1 − ^ ABCD ∫ u E ,C u.,ED dV − ^ ABCDEF ∫ uC , D u E , F dV . 2 2 V V
(7.36)
Hence, from (7.31) and (7.36), components of F I may be nonnegligible: ⎡ F I MN = δ MN − V −1SMNAB ⎢^ AECD ∫ u.,BE uC , D dV + ^ BECD ∫ u.,AE uC , D dV V V ⎣ (7.37) ⎤ 1 ABCD 1 E ABCDEF + ^ ∫V uE ,C u.,D dV + 2 ^ ∫ uC , DuE ,F dV ⎥⎦ . 2 V The rank four compliance constants at the reference state, SMNAB in (7.37), satisfy conditions listed in (5.149): 2^ CDAB SABMN = δ .CM δ .DN + δ .MD δ .CN . (7.38) By introducing the quantity ˆ CDABEF = ^ AFCDδ BE + ^ BFCDδ AE + ^ EFADδ BC ^
+ ^ EFBDδ AC + ^ ABFDδ CE + ^ ABEDδ CF
(7.39)
, δ −^ δ +^ −^ integral equations (7.36) and (7.37) are written more compactly as (Toupin and Rivlin 1960) 1 ^ ABCD ∫ u(C , D ) dV = ^ ABCD ∫ uC , E u.,ED dV − ^ ABCD ∫ u.,EE uC , D dV 2 V V V (7.40) 1 ˆ CDABEF − ^ ∫ uC , D uE , F dV , 2 V ABCD
EF
ABEF
CD
ABCD EF
350
7 Residual Deformation from Lattice Defects
⎡1 F I MN = δ MN + V −1SMNAB ⎢ ^ ABCD ∫ uC , E u.,ED dV V ⎣2 −^
ABCD
∫u
E ., E C , D
V
u
⎤ 1 ˆ CDABEF dV − ^ uC , D u E , F dV ⎥ . ∫ 2 V ⎦
(7.41)
Notice from (7.37) and (7.41) that both geometric nonlinearity (i.e., quadratic terms in displacement gradients) and material nonlinearity (i.e., thirdorder elastic constants) contribute to F I , and that F I does not necessarily reduce to the unit tensor when thirdorder elastic constants vanish. If the strain energy density in (7.30) is extended to incorporate products of displacement gradients of order higher than three, e.g., fourthorder elastic constants such as those in (5.67), then effects of these higherorder terms will likewise enter the right sides of (7.37) and (7.41). When elastic moduli are not spatially constant, for example in a multiphase composite or body with foreign inclusions, (7.37) and (7.41) do not strictly apply since in that case elastic coefficients cannot be brought outside the volume integrals. If V is the initial volume of a polycrystal with randomly oriented grains, then uniform isotropic elastic properties (i.e., effective moduli) can be assigned to the volume element as an approximation. According to (7.27)(7.30), when the (residual) displacement gradient u A, B vanishes at a material point, strain E AB and (residual) stress vanish at that point. In an isotropic homogeneous elastic body that is regular (i.e., no defects or discontinuities in displacements and displacement gradients), local residual stress must vanish everywhere (Hoger 1985), regardless of the particular form of the strain energy function. Because the average residual elastic deformation results from nonlinear elastic effects, i.e., products of displacement gradients of order two in (7.37) and (7.41), the contribution of the average residual elastic deformation F I to the total deformation gradient F of (7.12) will generally be small in conventional engineering applications wherein defect densities are low to moderate. For example, linear elasticity theory is generally deemed valid beyond some cutoff distance on the order of one to ten lattice parameters from the dislocation core (Teodosiu 1982; Hull and Bacon 1984), beyond which magnitudes of elastic displacement gradients are small, say u A, B < 0.1 , so that contributions from such linearelastic regions to terms in braces in (7.41) will be small. Contrarily, for materials with very large dislocation densities in which core regions comprise a substantial fraction of the volume element, nonlinear elastic contributions could be substantial, in which case the difference F I − 1 would be nonnegligible. The contri
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
351
bution of tensile volumetric and deviatoric parts of local elastic displacement gradients to F I would also be limited by the theoretical strength of the crystal, typically on the order of 10% of an elastic shear modulus (see (C.209) of Section C.4.1), since the material would tend to fracture at elastic strains producing tensile or shear stresses in excess of the theoretical strength. On the other hand, large elastic volumetric compressions are usually sustainable in crystals, as noted in Section 5.3. The effect of residual elasticity would be greatest in materials whose thirdorder elastic constants are substantially larger than secondorder constants; in some crystalline solids, representative thirdorder constants can exceed secondorder constants by an order of magnitude or more (Teodosiu 1982). 7.2.4 Residual Elastic Volume Changes Now consider the average volume change of the body resulting from the field of local residual elastic distortion u A, B . The preceding derivations (and those that follow in Section 7.2.4) apply regardless of whether or not the average shape change resulting from u A, B vanishes. However, for a crystal containing a large number of randomly oriented defects (e.g., dislocation and disclination lines and loops), it may be reasonable to assume that the change in dimensions of the crystal imparted by local stress fields of defects exhibits no preferred directions, implying that the crystal undergoes only a volume change and no shape change (Clayton 2009a, c). The average residual elastic volume change is also of perhaps greater interest than the shape change because the former can be easily measured experimentally for plastically deformed crystals, with results then available to validate the theory. The residual elastic deviatoric shape change, on the other hand, cannot be obtained simply from the deformed shape of a sample of material since the residual elastic shape change cannot be easily delineated from the shape change resulting from dislocation glide. The change in a differential volume of a body in coincident spatial and reference coordinate systems is given by (2.147): 1 dv / dV = det(δ . BA + u.,AB ) = ⎡⎣( x.,AA )3 − 3 x.,AA x.,BC x.,CB + 2 x.,BC x.,CA x.,AB ⎤⎦ 6 (7.42) 1 1 A B A A 2 ≈ 1 + u., A + (u., A ) − u., B u., A , 2 2 where products of order three in referential displacement gradients are omitted in the final expression. In the context of Fig. 7.1, dv is the volume of a differential subelement of the body in configuration B , and
352
7 Residual Deformation from Lattice Defects
dV is the volume of that subelement in B . Integrating (7.42), a secondorder accurate measure of the net volume change attributed to residual elastic deformation within the crystal is 1 ∆V = v − V = ∫ u.,AA dV + ∫ ⎡⎣(u.,AA ) 2 − u.,AB u.,BA ⎤⎦ dV . (7.43) 2V V Right sides of (7.37), (7.41), and (7.43) depend on the local residual elastic displacement gradient fields in the body. For crystals of high symmetry, these relations can be further reduced by appealing to particular forms of the elastic coefficients. Specifically, for cubic crystal systems of the highest symmetry (Laue group CI of Table A.1 in Appendix A), the secondorder moduli consist of three independent coefficients and the thirdorder moduli of six independent coefficients, as is clear from Tables A.8 and A.9, respectively. Consider a coordinate system with axes parallel to the cube axes of the crystal. In Voigt’s notation (A.10), pairs of indices 11 → 1 , 22 → 2 , 33 → 3 , 23 → 4 , 13 → 5 , 12 → 6 , 2 E AB → E A (1 + δ AB ) ,
barred indices span A = 1, 2,...,6 , and nonzero secondorder elastic constants of a cubic crystal are ^11 = ^ 22 = ^33 , ^12 = ^13 = ^ 23 ,
(7.44)
^ =^ =^ . Nonzero thirdorder constants of a cubic crystal of Laue group CI are ^111 = ^ 222 = ^333 , ^144 = ^ 255 = ^366 , ^112 = ^113 = ^122 = ^ 223 = ^133 = ^ 233 , ^123 , (7.45) 155 166 244 266 344 355 456 ^ =^ =^ =^ =^ =^ , ^ . The following notation is common, as indicated in (A.17) and (A.19) of Appendix A: 3K = ^11 +2^12 , (7.46) 2 µ = ^11 − ^12 , 2 µ ′ = 2^ 44 − (^11 − ^12 ), where K is the bulk modulus at the reference state and µ and µ ′ are shear moduli at the reference state. In a cubic crystal, the first term on the right side of strain energy function (7.30) can be written by linearizing (A.17), i.e., replacing the right CauchyGreen strain in (A.17) with the symmetric part of the displacement gradient (Toupin and Rivlin 1960): 44
55
66
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
1 W = ^ ABCD u A, B uC , D 2 1 1 ⎡1 ⎤ = K (u.,AA ) 2 + µ ⎢ (u.,AB u.,BA + u.,AB u.,AB ) − (u.,AA ) 2 ⎥ 2 3 ⎣2 ⎦
353
(7.47)
⎡1 1 2 2 2 3 2⎤ + µ ′ ⎢ (u.,AB u.,BA + u.,AB u .,AB ) − (u.,1 ) − (u.,2 ) − (u.,3 ) ⎥ 2 ⎣ ⎦ = WD + WS + WS′ , where WD is the strain energy of dilatation and WS and WS′ result from elastic shape changes. In an isotropic material such as a polycrystal with no preferred orientations, the number of constants in (7.44) is further reduced to two according to Table A.8 as 2^ 44 = ^11 − ^12 , (7.48) and in (7.45) reduced to three according to Table A.9 as 2^144 = ^112 − ^123 , 4^155 = ^111 − ^112 , (7.49) 8^456 = ^111 − 3^112 + 2^123 . Thus for isotropy, coefficients K and µ of (7.46) and energy densities WD and WS of (7.47) are identical, but µ ′ = 0 in (7.46) and WS′ = 0 in (7.47). Summation over the first two indices of (7.36) and using the first of (7.47) results in the integral equation 1 ^ .AA.CD ∫ u(C , D ) dV = −4 ∫ WdV − ^ .AA.CD ∫ uE ,C u.,ED dV 2 V V V (7.50) 1 A.CDEF − ^A ∫ uC ,D uE ,F dV . 2 V Appealing to (7.40), 1 ^ .AA.CD ∫ u(C , D ) dV = −3∫ WdV + ^ .AA.CD ∫ (uC , E u.,ED − uC , D u.,EE )dV 2 V V V (7.51) 1 ˆ A.CDEF − ^A ∫ uC ,D uE ,F dV . 2 V For a cubic crystal satisfying (7.44)(7.46), equality (7.51) reduces to 3 3K ∫ u.,DD dV = −3∫ WdV − K ∫ ⎡⎣ (u.,AA )2 − u.,AB u.,BA ⎤⎦ dV 2 V V V (7.52) 1 ˆ A.CDEF . u u dV − ^ A ∫ C,D E,F 2 V Then from (7.43), the net volume change for the element of reference volume V is
354
7 Residual Deformation from Lattice Defects
∆V = −
1 1 ˆ A.CDEF WdV − ^A ∫ ∫ uC , D uE , F dV . KV 6K V
(7.53)
Letting j = det( x.,aA ) , where j > 0 , the rightmost term of (7.53) can be written for a cubic crystal that remains cubic during deformation as (Toupin and Rivlin 1960) 1 ˆ A.CDEF ^A ∫ uC , D uE , F dV 6 V
=
j ∂K j ∂µ j ∂µ ′ WD dV + WS dV + WS′dV K ∂j V∫ µ ∂j V∫ µ ′ ∂j V∫
=
∂ ln K ∂ ln µ ∂ ln µ ′ WD dV + WS dV + WS′dV , ∫ ∫ ∂ ln j V ∂ ln j V ∂ ln j V∫
(7.54)
where K , µ , and µ ′ are tangent elastic coefficients for a cubic crystal with respective constant values K , µ , and µ ′ in the reference state. Volume derivatives of elastic coefficients are evaluated at the reference state in the last of (7.54). Following (5.188)(5.193) and (5.205), ∂ (.) ∂p ∂ (.) K ∂ (.) = =− , (7.55) ∂j ∂j ∂p j ∂p where p = −σ .aa / 3 is the Cauchy pressure. Substituting (7.47) and (7.54)(7.55) into (7.53), the residual volume change is ⎞ ⎛ K ∂µ ⎞ 1 ⎡⎛ ∂K ∆V = ⎢⎜ − 1⎟ ∫ WD dV + ⎜ − 1⎟ ∫ WS dV K ⎣⎝ ∂p ⎠V ⎝ µ ∂p ⎠ V (7.56) ⎤ ⎛ K ∂µ ′ ⎞ +⎜ − 1⎟ ∫ WS′dV ⎥ , ⎝ µ ′ ∂p ⎠V ⎦ where derivatives with respect to pressure of K , µ , and µ ′ are evaluated at a stressfree reference state. In particular, recall that the pressure derivative of the bulk modulus can be estimated from the Gruneisen parameter using (5.237). After defining average strain energies on a per unit reference volume basis as WD = V −1 ∫ WD dV , WS = V −1 ∫ WS dV , WS′ = V −1 ∫ WS′dV , (7.57) V
V
and the quantity
∆V
V
v = , (7.58) V V the normalized volume change for a selfequilibrated, cubic nonlinear elastic solid of grade one is J =1+
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
J =1+
1 K
355
⎡⎛ ∂K ⎞ ⎛ K ∂µ ⎞ − 1⎟WD + ⎜ − 1⎟WS ⎢⎜ p ∂ ⎠ ⎝ µ ∂p ⎠ ⎣⎝
⎛ K ∂µ ′ ⎞ ⎤ +⎜ − 1⎟WS′ ⎥ ⎝ µ ′ ∂p ⎠ ⎦ ⎡⎛ ∂ ln K 1 ⎞ ⎛ ∂ ln µ 1 ⎞ = 1 + ⎢⎜ − ⎟WD + ⎜ − ⎟WS K⎠ K⎠ ⎝ ∂p ⎣⎝ ∂p
(7.59)
⎛ ∂ ln µ ′ 1 ⎞ ⎤ +⎜ − ⎟W ′⎥ . K⎠ ⎦ ⎝ ∂p In (7.59) and henceforward, overbars on tangent elastic coefficients are dropped, and it is understood that all elastic constants and their pressure derivatives are evaluated at the reference state. If the cubic secondorder elastic coefficients, their pressure derivatives, and each of the average strain energy densities of (7.57) are known, the volumetric deformation can be computed from (7.59). So long as strain energy densities in (7.57) are always positive, if coefficients of the energy densities in (7.59) are all of the same algebraic sign, then the overall volume change will be of that sign. If only the total strain energy density W = WD + WS + WS′ is known, for example from experiments (Clarebrough et al. 1957; Wright 1982), then (7.47) and (7.59) can be combined to establish bounds on the normalized volume change (Toupin and Rivlin 1960). Bounds of this sort have been validated by experimental data for several polycrystalline cubic metals (Wright 1982), wherein the volume changes induced by defects such as dislocations and stacking faults were always found to be positive by theory and experiment. For an isotropic solid, (7.59) reduces to ⎞ 1 ⎛ ∂K 1 ⎛ ∂µ µ ⎞ J =1+ ⎜ − 1⎟WD + ⎜ − ⎟W K ⎝ ∂p µ ⎝ ∂p K ⎠ S ⎠ (7.60) ⎛ ∂ ln K 1 ⎞ ⎛ ∂ ln µ 1 ⎞ =1+ ⎜ − ⎟WD + ⎜ − ⎟WS . K⎠ K⎠ ⎝ ∂p ⎝ ∂p In an isotropic body, pressure derivatives of tangent bulk and shear moduli K and µ are related to thirdorder elastic constants in (A.26). Formula (7.59) for cubic crystals is attributed to Toupin and Rivlin (1960), while (7.60) was developed earlier by Zener (1942) using nonlinear isotropic elasticity and thermodynamic arguments. Isotropic formula (7.60) for the case when the dilatational energy vanishes agrees with that of Holder and Granato (1969) obtained from thermodynamic arguments:
356
7 Residual Deformation from Lattice Defects
∂Ge ( p,θ ) 1 ⎛ ∂µe µe ⎞ 1 ⎛ ∂µ µ ⎞ = ⎜ − ⎟ Ge = ⎜ e − e ⎟ E ρT 0 , (7.61) V ∂p µe ⎝ ∂p K ⎠ µe ⎝ ∂p K ⎠ where Ge is the Gibbs free energy change from defects, per unit reference volume that depends on pressure p and temperature θ , and µe is an effective elastic coefficient that depends upon the mathematical form of the strain energy of the particular defect. In the final term of (7.61), E is the elastic strain energy per unit length of the defect and ρT 0 is the total length per unit reference volume of the defect. For a number of kinds of crystals, Holder and Granato (1969) found that delineation between dilatational and deviatoric energies and incorporation of effects of cubic anisotropy had little influence on volume changes from straight dislocations predicted using (7.61). The source of the local displacement gradient and residual strain energy in the body to this point has been arbitrary, so long as (7.23), (7.26), and (7.30) apply, that is, traction is continuous across internal surfaces, the body is selfequilibrated, and the local constitutive response is described by hyperelasticity with terms of order higher than three in referential displacement gradients omitted in the strain energy. Defects induce such displacement gradients and residual strain energies. These may include, for example, dislocation and disclination lines and loops, stacking faults, grain boundaries, twin boundaries, and slip bands. Volume changes attributed to point defects (e.g., substitutional atoms, interstitials, and vacancies), phase transformations, voids, and open cracks are not considered in the present treatment, since dimensional changes computed according to the present theory account only for volume and shape changes resulting from stress fields of defects and not volume and shape changes associated with defects themselves. However, the additional volume change induced by a point defect—for example the volume change in addition to the misfit dilatation in a sphereinhole model—attributed to elastic nonlinearity can be estimated from (7.61) for an isotropic elastic body (Eshelby 1954; Holder and Granato 1969), as illustrated later in Section 7.4. Anisotropy cannot be directly addressed in (7.59) when tangent elastic moduli may change with position, for example grain boundaries and twin boundaries across which lattice orientations may differ. However, isotropic approximation (7.60) could still be used as an estimate in these cases, as in previous applications towards polycrystals (Seeger and Haasen 1958) and single crystals of lower symmetry (Clayton 2009a). The isotropic approach is further developed for line defects in Sections 7.2.5 and 7.2.7. Also neglected in the foregoing continuum elastic analysis are explicit effects of defect cores on the residual deformation of the body. For exam
∆V
=
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
357
ple, elastic strain, stress, and strain energies imparted by Volterra line defects diverge as the radial distance from the line shrinks to zero, as is clear from linear elastic solutions given in Sections C.1 and C.2, and even nonlinear elasticity is inadequate for describing nonconvex energy distributions imparted by highly distorted crystal structures within defect cores. In the present continuum treatment, one can imagine each defect line to be surrounded by a tractionfree cylindrical boundary delineating the core region from the surrounding elastic continuum of reference volume V. In linear elasticity, stresses and strains resulting from traction acting on the cylindrical boundary of the core decay as R −3 , where R is the distance from the defect line, and hence are usually neglected (Teodosiu 1982). The elastic continuum is thus selfequilibrated in this approximation, and (7.26) applies. 7.2.5 Straight Edge and Screw Dislocations
Consider volume changes imparted by dislocation lines in the isotropic approximation. The energy per unit length (linear elastic energy plus core and interaction energies) of a straight dislocation embedded in an infinite isotropic medium, with elastic energies given in (C.48) and (C.69), is ⎧1 − ν (edge dislocation) µb2 ⎛ R ⎞ ˆ ln ⎜ (7.62) E= ⎟+E , k =⎨ 4π k ⎝ RC ⎠ ⎩1 (screw dislocation) where b is the magnitude of the Burgers vector that is treated as a constant, ν = (3K − 2µ ) /(6 K + 2µ ) is Poisson’s ratio (see Table A.10), R is the radial distance from the dislocation core, RC is the radius of the dislocation core, and Eˆ is a correction to the linear elastic solutions that accounts for core energy, line curvature, interaction energies from other defects and boundaries, and stacking faults associated with partial dislocations. Denoted by E E = E − Eˆ is the elastic strain energy density per unit line length L of straight, noninteracting edge dislocations, separated into dilatational and shear contributions as in (C.49) and (C.50): µ b 2 1 −ν − 2ν 2 ⎛ R ⎞ E µ b 2 2 − 2ν + 2ν 2 ⎛ R ⎞ EDE = ln ⎜ ln ⎜ ⎟ , ES = ⎟ , (7.63) 12π (1 −ν ) 2 12π (1 − ν ) 2 ⎝ RC ⎠ ⎝ RC ⎠ where superscript E refers to an edge dislocation. Relating energies per unit reference volume to energies per unit length using the equalities WDV = EDE L , WSV = ESE L , (7.64) and multiplying (7.60) by V / L , the volume change per unit length of edge dislocation line is (Seeger and Haasen 1958; Teodosiu 1982)
358
7 Residual Deformation from Lattice Defects
∆V L
= Edge
⎞ 1 ⎛ ∂K 1 ⎛ ∂µ µ ⎞ E − 1⎟ EDE + ⎜ − ⎟ ES ⎜ K ⎝ ∂p µ ⎝ ∂p K ⎠ ⎠
(7.65) ⎞ 2 − 2ν + 2ν 2 ⎛ ∂µ µ ⎞ ⎤ E E ⎡1 − ν − 2ν 2 ⎛ ∂K = − 1⎟ + − ⎟⎥ , ⎢ ⎜ ⎜ 3 ⎣ (1 − ν ) K ⎝ ∂p (1 − ν ) µ ⎝ ∂p K ⎠ ⎦ ⎠ where E E = EDE + ESE is the total elastic line energy of an edge dislocation. Analogously, denote by E S = E − Eˆ the strain energy per unit line length L of straight, noninteracting screw dislocations, partitioned as in (C.68) and (C.69): µb2 ⎛ R ⎞ (7.66) EDS = 0 , ESS = ln ⎜ ⎟, 4π ⎝ RC ⎠ Setting the deviatoric energy in the second of (7.57) equal to the product of the line length and energy per unit length (7.66) gives WSV = ESS L = E S L , (7.67) where E S is the total elastic line energy of a screw dislocation. Multiplying (7.60) by V / L , the volume change per unit length of straight screw dislocation lines is (Seeger and Haasen 1958; Teodosiu 1982) ∆V E S ⎛ ∂µ µ ⎞ (7.68) = − ⎟. ⎜ L Screw µ ⎝ ∂p K ⎠ Now let the total dislocation line density per unit reference volume be given by the sum ρT 0 = L / V = ρ E 0 + ρ S 0 , (7.69) where now L is the total length of edge and screw dislocations in volume V, ρ E 0 is the density of edge dislocations, and ρ S 0 is the density of screw dislocations, both measured per unit reference volume. Define from (7.62) an energy per unit length µ b2 ⎛ R ⎞ ET = kE E = E S = (7.70) ln ⎜ ⎟, 4π ⎝ RC ⎠ and let χ = ρ E 0 / ρT 0 be the fraction of pure edge dislocations in the total dislocation density. Superposing volume changes from (7.65) and (7.68) and using (7.58), (7.60) becomes
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
J = 1 + ρE0
∆V L
+ ρS 0 Edge
359
∆V L
Screw
⎧⎪ χ ⎡1 − ν − 2ν 2 ⎛ ∂K ⎞ 2 − 2ν + 2ν 2 ⎛ ∂µ µ ⎞ ⎤ (7.71) = 1+ ⎨ ⎢ − 1⎟ + − ⎟⎥ ⎜ ⎜ (1 − ν ) µ ⎝ ∂p K ⎠ ⎦ ⎠ ⎪⎩ 3k ⎣ (1 − ν ) K ⎝ ∂p 1 − χ ⎛ ∂µ µ ⎞ ⎫⎪ + − ⎟ ⎬ ET ρT 0 . ⎜ µ ⎝ ∂p K ⎠ ⎭⎪ Relation (7.71) yields the volume change associated with straight, noninteracting pure screw and edge dislocation lines in an isotropic body with homogeneous elastic properties. While terms in braces in (7.71) include nonlinear elastic effects (i.e., pressure derivatives of the elastic moduli or thirdorder elastic constants), dislocation line energy ET does not account explicitly for nonlinearity or energy of dislocation cores. Thus, (7.71) represents the product of thirdorder nonlinear elasticity (terms in braces) and linear elasticity (defect energy ET ). Products of purely linear elastic origin would yield null volume change, as implied by (7.35), while higherorder products of nonlinear origin (e.g., products of pressure derivatives of moduli with contributions of nonlinear elasticity to dislocation energies) are neglected. Relation (7.71) can be used directly to estimate the volume change of a (poly)crystal if line densities of edge and screw dislocations, their energies per unit length, and the requisite elastic constants are known. The preceding analysis assumes that defect densities are negligible in the reference configuration. When dislocation densities are substantial in the initial state, the predicted volume change between initial and final configurations corresponds only to the change in defect density that occurs during deformation between initial and final states, rather than that associated with the absolute density of dislocations. Viewed another way, if the absolute defect density is used in the calculation, then the computed volume change will be measured from a stressfree reference configuration B0 in which the dislocation line density and residual elastic energy vanish. Dislocation line densities in the preceding developments are defined per unit reference volume V = V , equivalent in configurations B0 and B of Fig. 7.1 because J P = 1 . When the dislocation line density is measured in the externally unloaded but internally stressed configuration B as ρT , then ρT 0 = J ρT in (7.71) such that
360
7 Residual Deformation from Lattice Defects
⎧⎪ χ ⎡1 − ν − 2ν 2 ⎛ ∂K ⎞ 2 − 2ν + 2ν 2 ⎛ ∂µ µ ⎞ ⎤ J −1 = 1 − ⎨ ⎢ − 1⎟ + − ⎟⎥ ⎜ ⎜ (1 − ν ) µ ⎝ ∂p K ⎠ ⎦ ⎠ ⎪⎩ 3k ⎣ (1 − ν ) K ⎝ ∂p
(7.72) 1 − χ ⎛ ∂µ µ ⎞ ⎫⎪ + − ⎟⎬ E ρ . ⎜ µ ⎝ ∂p K ⎠ ⎭⎪ T T However, the distinction between configurations used to define the dislocation line density will have a trivial effect on computed values of J for small volume changes ( 1 + ∆V / V ≈ 1/(1 − ∆V / V ) ), and in these cases preferential use of (7.72) over (7.71) is probably not justified considering uncertainty in dislocation densities that can be measured experimentally. The elastic dislocation line energy depends on the core radius RC and the cutoff radius R. A standard approximation, also listed in (6.118), is (Kocks et al. 1975; Hull and Bacon 1984) 1 ⎛ R ⎞ ln ⎜ ET = Λµb 2 , 0.5 < Λ = (7.73) ⎟ < 1.0 . 4π ⎝ RC ⎠ Introducing the dimensionless quantities ⎞ 2 − 2ν + 2ν 2 ⎛ ∂µ µ ⎞ ⎤ E ρ ⎡1 − ν − 2ν 2 ⎛ ∂K AE = T T 0 ⎢ − 1⎟ + − ⎟⎥ , ⎜ ⎜ 3k ⎣ (1 −ν ) K ⎝ ∂p (1 − ν ) µ ⎝ ∂p K ⎠ ⎦ ⎠
(7.74)
ET ρT 0 ⎛ ∂µ µ ⎞ − ⎟, (7.75) ⎜ µ ⎝ ∂p K ⎠ the volume change in (7.71) becomes (7.76) ∆V / V = J − 1 = AE χ + AS (1 − χ ) . Thus, ∆V / V for a mixture of straight, noninteracting edge and screw dislocations will fall between volume change AE resulting from the same density of pure edge dislocations and volume change AS resulting from the same density of pure screw dislocations. AS =
7.2.6 Approximate Volume Changes
Returning to the overall dimensional changes of the body induced by averaged local displacement gradients, consider (7.31). Defining the quantities α = V −1 ∫ u.,AA dV , β 2 = V −2 ∫ u.,AB dV ∫ u.,BA dV , (7.77) V
V
V
and, to secondorder accuracy in referential displacement gradients, the analog of (7.42) is
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
361
1 1 (7.78) det(F I ) = 1 + α + α 2 − β 2 . 2 2 Recall from (7.42) and (7.58) that the true volume change satisfies, to second order in the local distortion, 1 J = 1 + α + ∫ ⎡⎣(u.,AA ) 2 − u.,AB u.,BA ⎤⎦ dV . (7.79) 2V Therefore quantities in (7.78) and (7.79) are related as follows: 1 1 J = det(F I ) − (α 2 − β 2 ) + ∫ ⎡⎣(u.,AA ) 2 − u.,AB u.,BA ⎤⎦ dV . (7.80) 2 2V At least to firstorder accuracy in displacement gradients, J = det(F I ) . Possible differences between J and det(F I ) may arise because the determinant operation and volume integration do not commute. When products of distortions and their averages are small, tr(F I ) = α + 3 ≈ det(F I ) + 2 and J ≈ det(F I ) . Recall from (7.14) and (7.31) that F I AB = F I ( AB ) as defined
in Chapter 7 is a stretch with no rotation. Even though in some cases defects impart no local dilatation in the linear elastic approximation (e.g., Volterra screw dislocations in isotropic solids as in (C.59)), a volume change can still result (e.g., (7.79) with J ≠ 1 ) because of nonlinear elastic effects. 7.2.7 Examples: Dislocations and Disclinations in Copper Table 7.1 lists strain energies per unit line length E of a number of defects whose elasticity solutions are described in detail in Appendix C: straight edge and screw dislocations discussed already in Section 7.2.5; circular screw and prismatic dislocation loops; and straight wedge disclinations and circular twist and wedge disclination loops of Frank vector ω . In each case, the core radius, i.e., inner radial coordinate at which the elastic solution is truncated, is labeled RC . For straight line defects, the radial distance from the core is labeled R; for defect loops, the radius of the circular loop is labeled A, as in Fig. C.3. Energies all correspond to defects in infinitely extended, isotropic linear elastic solids. Analytical formulae for defect line energies follow from references quoted in Table 7.1 and corresponding equations of Appendix C, while normalized volume changes ∆V / V ÷ ρT 0 a 2 computed for copper follow from (7.65) for edge dislocations and from (7.61) for the other defects, using properties listed in Tables 7.2 and 7.3.
362
7 Residual Deformation from Lattice Defects
Table 7.1 Line defect energies and residual volume changes in copper Line defect Edge dislocation(1) µb2 R ln E= 4π (1 −ν ) RC Screw dislocation(1) µb2 R ln E= 4π RC Screw dislocation loop(2) µb2 E≈ 12π (1 −ν ) ⎡ ⎤ 8A × ⎢3 (1 −ν ) ln − 9 + 10ν ⎥ R C ⎣ ⎦ Prismatic dislocation loop(2) µb2 ⎡ 8 A ⎤ E≈ − 2⎥ ⎢ln 4π (1 −ν ) ⎣ RC ⎦
Wedge disclination(3) µω 2 R 2 E= 16π (1 −ν )
Equation in Appendix C (C.48)
Energy/length Volume change E [eV/Å] ∆V / V ÷ ρT 0a2 3.30 0.89
(C.67)
2.12
0.51
(C.160)
2.00
0.49
(C.162)
3.32
0.81
(C.149)
2.65
0.64
(C.167)
9.86
2.4
(C.170)
7.74
1.9

0.81.1
2 ⎡ ⎛ R ⎞2 ⎛R ⎞ × ⎢1 − ⎜ C ⎟ − 4 ⎜ C ⎟ ⎝ R ⎠ ⎢⎣ ⎝ R ⎠ −1 ⎤ ⎛ ⎛ RC ⎞ 2 ⎞ 2 ⎛ RC ⎞ ⎥ ln ⎜1 − ⎜ ⎟ ⎜ R ⎟⎥ ⎜ ⎝ R ⎟⎠ ⎟ ⎝ ⎠ ⎝ ⎠ ⎦ (3) Twist disclination loop µω 2 R 2 ⎡ 8 A 8 ⎤ − ⎥ E≈ ⎢ln 4π ⎣ RC 3 ⎦
Wedge disclination loop(4) µω 2 R 2 ⎡ 8 A 8 ⎤ − ⎥ E≈ ⎢ln 8π (1 −ν ) ⎣ RC 3 ⎦
Experiment(5) (1) Hirth and Lothe (1982) (2) Owen and Mura (1967) (3) Huang and Mura (1970) (4) Liu and Li (1971); Kuo and Mura (1972) (5) Clarebrough et al. (1957)
7.2 Nonlinear Elastic Interpretation of Residual Elasticity
363
Table 7.2 Properties for line defects in copper a [Å](1) b [Å] A [Å] RC [Å] R/RC, A/RC** R/RC, A/RC*** ω* 3.62 2.56 10.0 106 10 π /2 10.0 (1) Rounded up from 3.61496 Å at a temperature of 291 K (Wyckoff 1963) * Full disclination in cubic crystal (Li 1972) ** Dislocation lines and loops *** Disclination lines and loops
Table 7.3 Elastic properties for polycrystalline copper (1)
µ [GPa]
K [GPa] ν 47 152 0.36 (1) Seeger and Haasen (1958)
∂µ/∂p 0.8
∂K/∂p 4.4
For defects besides edge dislocations, the strain energy density is treated as deviatoric, leading to the linear relationship between volume change and defect density given in (7.61). This is a rigorous assertion for screw dislocation loops and twist disclination loops but not for prismatic loops or wedge disclinations, though it has been used elsewhere for these defects (Li and Gilman 1970; Liu and Li 1971) and should provide a reasonable approximation to volume change predictions for many metals (Holder and Granato 1969), including Cu. Again, ρT 0 is the line length per unit reference volume of the defect, and a is the lattice parameter of the conventional FCC unit cell in a perfect crystal at room temperature, as defined generically in (3.2). The magnitude of the Burgers vector, treated as a constant, is b = a 2 / 2 from Table 3.4. Experimental results for polycrystalline Cu are provided for comparison (Clarebrough et al. 1957); the range of volume changes reported in Table 7.1 for the experiments corresponds to estimates of dislocation line length from energy measurements after plastic compressive strains ranging from 0.3 to 0.7. The character of the defects (e.g., edge versus screw, straight lines versus loops) was not reported in that experimental investigation. From Table 7.1, normalized volume changes predicted for various kinds of dislocations agree with the experimental findings within a factor of ~2 and are very close for edge dislocations and prismatic loops. Volume changes per unit defect length in Cu are positive (i.e., defects cause expansion) and small. For example, a 1% volume increase would require a very high density of edge dislocations on the order of ρT 0 ≈ 0.01a −2 ≈ 1017 m −2 , corresponding to an average dislocation spacing on the order of 10a. For small volume changes ( ∆V / V < 0.01 ), the value of det(F I ) is expected
364
7 Residual Deformation from Lattice Defects
provide an accurate approximation of J according to (7.80). Disclination energies and volume changes are comparable to those for dislocations for the small cutoff radii or small loops considered here (i.e., R = 10 RC or A = 10 RC in Table 7.2) but would diverge quickly at large distances R from the core of straight disclinations or for larger disclination loops. Elastic anisotropy of grains within the polycrystal, defect core energies, and interaction energies among defects and between defects and the external boundary of the body (e.g., image forces) are omitted in this application of the model; such effects presumably contribute to discrepancies between theory and experiment. Results of Table 7.1, along with experimental data summarized by Wright (1982), suggest that volume changes resulting from residual elasticity associated with dislocations should be relatively small in metallic crystals of cubic symmetry deformed in compression or shear to strains on the order of unity, under quasistatic conditions. Experimental results in the final row of Table 7.1 (Clarebrough et al. 1957) correspond to dislocation densities on the order of ρT 0 ≈ 1015 m −2 , leading to volume changes on the order of ∆V / V ≈ 10−4 . Such small volume changes would seem inconsequential in the context of measured yield properties of materials in unconfined loading, when specimens are free to expand or contract laterally. However, under lateral confinement, for example uniaxial strain conditions occurring in shock loading (Rohatgi and Vecchio 2002; Clayton 2009a), small volume changes can noticeably affect the measured hydrostatic pressure. Volume changes cannot be accommodated by dislocation glide as noted in Section 7.1.1; hence, any residual volume increase from defects must be compensated by an elastic volume decrease and corresponding hydrostatic pressure. Extremely high dislocation densities, ρT 0 ≈ 1016 m −2 , have been observed for metals such as Cu deformed in shock conditions (Rohatgi and Vecchio 2002). A dislocation density of 1016 m −2 would lead to an expansion on the order of 0.1%, which would in turn require an offsetting pressure on the order of 0.1% of the bulk modulus, around 150 MPa in Cu. Such contributions of defects to pressure or volume change would manifest implicitly in the measured equation of state (i.e., pressurevolumetemperature relationship—see Section 5.3), bulk modulus, and pressure derivatives of the bulk modulus obtained from shock physics experiments. Substantial effects of large dislocation densities on tangent elastic moduli of metallic single crystals deformed in uniaxial strain have also been predicted using atomistic methods (Clayton and Chung 2006). Very large dislocation densities comprising dislocation walls in subdivided grains have been observed in metals subject to severe
7.3 Atomistic Interpretation of Residual Elasticity
365
plastic deformation (Hughes et al. 2003); presumably, residual elastic volume changes could be significant in highly defective regions of such materials. While closedform analytical solutions are not available for the deviatoric part of F I in terms of stored energy and elastic constants, magnitudes of its deviatoric components are expected to be of the same order as its volumetric part, i.e., small except in cases where defect densities are extremely large. Meant by small are conditions F I AB − δ AB < 0.001 for de fect densities ρT 0 < 1015 m −2 in cubic metals such as copper, though larger average residual elastic deformations would be conceivable in crystals that feature stronger pressure sensitivity of the elastic coefficients. Because deviatoric deformation can be accommodated by plastic slip, there seems to be no capacity available to delineate contributions from residual elasticity versus dislocation flux to the plastic properties of materials (e.g., yield and flow properties) measured in experiments on single or polycrystals. The effect of F I is implicitly included in such experimental measurements. Notice that F I and its spatial gradient implicitly affect defect density measures defined in Section 3.3 in terms of the lattice deformation F L , e.g., (3.214), since F L = F E F I by (7.14).
7.3 Atomistic Interpretation of Residual Elasticity The volume element of crystalline solid is treated in what follows in Section 7.3 as an ensemble L of discrete atoms rather than a (nonlinear) elastic continuum. Relevant background discussions pertinent to atomicscale stress measures and atomic interactions are provided in Sections 7.3.1 and 7.3.2, respectively, in the context of discrete lattice statics. Additional, more extensive background treatment of lattice statics is contained in Section B.2 of Appendix B. Section 7.3.3 describes the selfequilibrated, relaxed intermediate configuration of an element of a crystal from an atomistic perspective and suggests a means to compute F I entering (7.12) from atomic quantities. The atomicscale derivation of F I that follows in Section 7.3.3 may prove useful in the context of multiscale computations of nonlinear elastic and plastic properties of crystals (Horstemeyer and Baskes 1999; Clayton and Chung 2006) and offers a more accurate treatment of defect cores than classical continuum elasticity used in Section 7.2.
366
7 Residual Deformation from Lattice Defects
7.3.1 Atomic Stress Measures A number definitions of stress based on atomic level quantities have been suggested, as discussed in Section B.2.2. In the context of lattice statics (i.e., null atomic velocities and accelerations), the average virial stress for a group of atoms is often considered equivalent to the average Cauchy stress, the former defined according to (B.35): 1 σ= (7.81) ∑ r ⊗ f ij , 2Ω i ≠ j ij where Ω is the total volume occupied by the group L of atoms, i.e., the sum of all atomic volumes, in spatial configuration B. The summation convention written in (7.81) is a compact notation that replaces the explicit double sum used in (B.35); that used here proceeds over all pairs of distinct (i ≠ j ) atoms. The factor of two arises in (7.81) because summation proceeds over all i ≠ j , and because r ij = −r ji , and f ij = −f ji . Spatial coordinates of atoms in a fixed, rectilinear coordinate frame are written as r i , and interatomic separations in the current configuration are defined as in (B.20):
r ij = r j − r i .
(7.82)
Interatomic forces arise from potential energy Φ as in (B.21) and (B.22): ∂Φ f ij = , Φ = Φ r ij i , j∈L . (7.83) ∂r ij i≠ j
( )
Now consider a homogeneous deformation F as in (B.37) and (B.43), applied to all atoms in L, leading to r ij = FR ij (Huang 1950; Born and Huang 1954), with R ij = R
j
− R i fixed separations between atoms of
the reference lattice as in (B.41). The discrete analog of continuum hyperelastic relation (7.29) is given by (B.54): b 1 1 ∂Φ ∂r ij ∂Φ aA δ ab b R Aij , = P = (7.84) ∑ ∑ b 2Ω0 i ≠ j ∂r ij ∂FaA 2Ω0 i ≠ j ∂r ij with Ω0 (italic font) the total volume of the atomic ensemble in B0 . Atomic volume Ω 0 (nonitalic font) introduced in Section 3.1.1 is equal to Ω0 divided by the number of atoms in L. When L is a primitive cell of a monatomic crystal, Ω0 = Ω0 , but in general Ω0 Ω0 . Relation (7.84) is a consequence of affine deformation of all atoms resulting in
7.3 Atomistic Interpretation of Residual Elasticity
367
∂r bij / ∂FaA = δ ab R Aij . The average atomic Cauchy stress or average static virial stress is
σ ab = det( F −1.Aa ) PbA F. Aa ⎞ a (7.85) ∂Φ 1 ⎟ F. A = r aij δ bc c , ∑ ⎟ 2Ω i ≠ j ∂r ij ⎠ in agreement with (7.81). The present analysis applies only to materials described by atomic force potentials of the general form (7.83) and for which stress definitions (7.81), (7.84), and (7.85) are appropriate. For example, metals that can be modeled by combinations of pair potentials and multibody potentials such as the embedded atom method (Daw and Baskes 1983, 1984) are included. Not admitted are piezoelectric crystals (e.g., noncentrosymmetric ionic solids), some of whose atoms (sublattices) may display a relative shift when polarized, and for which hyperelastic relation (7.84) may not be sufficient. In these cases, lattice vibrations may provide insight into origins of stress and material coefficients (Huang 1950; Born and Huang 1954; Mindlin 1968, 1972). Also excluded from the present treatment are noncentrosymmetric polyatomic lattices such as diamond and silicon that may incur inner displacements (Cousins 1978; Tadmor et al. 1999). =
Ω0 ⎛ 1 ∂Φ ⎜ ∑ δ bc ∂r c R Aij Ω ⎜⎝ 2Ω0 i ≠ j ij
7.3.2 Harmonic and Anharmonic Interactions Expanding the potential energy of (7.83) in a series about the reference state,
Φ = Φ0 + ∑ i≠ j
∂Φ ∂r aij
q aij + r=R
1 ∂ 2Φ ∑ 2 i ≠ j ∂r aij ∂r bkl
1 ∂ 3Φ + ∑ a b c 6 i ≠ j ∂r ij ∂r kl ∂r mn k≠l m≠ n
k≠l
q aij q bkl r=R
(7.86) a ij
b kl
q q q
c mn
+ ...
r=R
where Φ0 is a cohesive or total ground state energy (i.e., zeropoint kinetic and potential energies of electrons and nuclei) of the reference lattice, conventionally negative in sign and q ij = r ij − R ij is the relative displacement for an atomic pair. Henceforward it is assumed that the second term vanishes, meaning that the reference configuration B0 is explicitly chosen (or approximated) as free of external and internal forces:
368
7 Residual Deformation from Lattice Defects
H aij = δ ab
∂Φ ∂r bij
= 0,
(7.87)
r =R
though such a condition need not strictly apply in all cases2. Following the scheme used in (7.81) and Section B.2.5, repeated use of the summation symbol is omitted in (7.86). Hence, the summation in the second term on the right of (7.86) applies over two sets of repeated atomic labels, that in the third term over four sets, and that in the fourth term over six sets. The energy per unit reference volume Φ / Ω0 differs from the strain energy per reference volume Ψ 0 used in Section 7.2 by the additive constant Φ0 / Ω0 , since the continuum strain energy (7.28) vanishes in the undistorted reference state. Introducing the matrix notation for atomic stiffness coefficients H abijkl = δ acδ bd
∂ 2Φ ∂r cij ∂r dkl
= δ ad δ beδ cf , H abc ijklmn r=R
∂ 3Φ f ∂r dij ∂r ekl ∂r mn
, (7.88) r=R
and noting ∂q akl / ∂r bkl = δ .ba , the stress of (7.81) and (7.85) becomes
σ ab =
1 2Ω
∑r i≠ j k ≠l
a ij
H bcijkl δ cd q dkl +
1 4Ω
∑r
i≠ j k ≠l m≠n
a ij
H bce δ q d δ q fmn + .... (7.89) ijklmn cd kl ef
Under a homogeneous deformation q ij = (F − 1) R ij , the twopoint stress tensor of (7.84) is 1 1 P aA = H abijkl δ bc q ckl R Aij + ∑ ∑ H abc δ bd q dkl δ ce q emn R Aij + .... (7.90) 2Ω0 i ≠ j 4Ω0 i ≠ j ijklmn k ≠l
k ≠l m≠ n
In the harmonic approximation (Maradudin et al. 1971), products of order higher than two in atomic displacements are dropped from the crystal’s potential energy, leading to the linear forcedisplacement relationship f ija = ∑ H abijkl δ bc q ckl , (7.91) k ≠l
and to resulting stress measures 1 1 σ ab = ∑ r a H bc δ cd q dkl , P aA = 2Ω 2Ω i ≠ j ij ijkl 0 k ≠l
∑H i≠ j k ≠l
ab ijkl
δ bc q ckl R Aij . (7.92)
Second and thirdorder elastic constants derived from an atomic potential in Appendix B, (B.75) and (B.77), are repeated here as, respectively, 2
When (7.87) does not apply and H aij ≠ 0 , this term’s contribution to forces,
stresses, and energy can be incorporated in a straightforward manner.
7.3 Atomistic Interpretation of Residual Elasticity
^ ABCD = ^ ABCDEF =
1 2Ω0
1
∑H i≠ j k ≠l
∑H
2Ω0 i ≠ j
ab ijkl
abc ijklmn
δ .aA R Bij δ .Cb R Dkl ,
369
(7.93)
R Aij R Ckl R Emn δ .aBδ .bDδ .cF
k ≠l m≠ n
− − −
1 2Ω0 1 2Ω0 1 2Ω0
∑H i≠ j k ≠l
ab ijkl
δ .aA R Cij δ .bE R Fkl δ BD (7.94)
∑H
ab ijkl
δ .aA R Eij δ .Cb R Dkl δ BF
∑H
ab ijkl
δ .aA R Bij δ .Cb R Ekl δ DF .
i≠ j k ≠l
i≠ j k ≠l
Relation (7.94) indicates that third (and higherorder) elastic constants depend in part on anharmonic terms in the potential, as noted by Thurston and Brugger (1964) and Maugin (1999). Derivations (7.89), (7.90), (7.92), (7.93), and (7.94) rely on uniformity of the atomistic deformation (Huang 1950; Born and Huang 1954) such that the relationship between current position vector r and reference position vector R is linear in the mapping F. In this atomistic context, F is regarded as a linear transformation for the primitive Bravais lattice vectors similar to F L in (7.9), and though it acts uniformly over atoms in an individual volume element, neither F nor F L need be the gradient of any macroscopic vector field spanning neighboring volume elements (Clayton and Chung 2006). Expansion (7.86), while generic in the sense that many types of interactions (e.g., pairwise and multibody, central and noncentral force) are admitted, may be cumbersome for computation of elastic constants for specific potentials that are not typically expressed explicitly in terms of interatomic separation vectors. For example, explicit expressions for second and thirdorder elastic constants are given in Section B.2.6 of Appendix B for pair potentials and embedded atom potentials. 7.3.3 Residual Deformation in a Selfequilibrated Lattice
Now consider the selfequilibrated configuration B of Fig. 7.1. Slip may have occurred in achieving this configuration from the reference state, but the atoms occupy perfect lattice sites apart from the effects of any defects
370
7 Residual Deformation from Lattice Defects
remaining within the element that either (i) are also present in reference configuration B0 or (ii) are generated during the course of plastic deformation. Not considered in Section 7.3 is the (former) class of defects present initially in B0 . Although positions of specific atoms may differ in configurations B and B as a result of translations by Burgers vectors of dis0
locations that have passed through the volume element, coordinates R i can still be used to identify positions of atoms occupying perfect lattice sites in B , as discussed in Section 3.2.10. The volume element may either be treated as an isolated ensemble of atoms with free boundaries or as part of an infinite medium with a periodic defect distribution. The former case is more consistent with the fundamental definition of the isolated unloaded configuration given in Section 7.1 (Eckart 1948), although free surfaces can give rise to atomic or ionic displacements (and corresponding surface energy contributions), even for otherwise perfect and undeformed crystal structures. Such free surface effects are usually considered negligible when the crystal volume element contains a sufficiently large number of atoms; correspondingly, such surface effects are not considered in the context of usual continuum nonlinear elasticity of Section 7.2. The latter case—which implicitly includes effects of image forces of defects in neighboring volume elements—may be more practical from the standpoint of lattice statics calculations with periodic boundary conditions (Chung and Clayton 2007). Previous definitions for achieving the slipped configuration B discussed in Section 7.1.2 still apply here, but dislocation fluxes contributing to plastic deformation are interpreted in terms of velocities of atoms comprising each line defect rather than as continuum quantities. External forces vanish by definition in B , as do dynamics (i.e., atomic velocities and accelerations), so lattice statics relations (B.16) and (7.81) apply for a selfequilibrated lattice. However, because of the presence of defects, the total energy of the ensemble L of atoms in B is a local minimum (Gallego and Ortiz 1993; Chung and Clayton 2007) as opposed to the global minimum corresponding to the perfect reference lattice in B0 . This implies that some atoms occupy metastable positions; some interatomic forces do not vanish within the element in B as they do in B0 via (7.87); and the potential energy of the ensemble of atoms in B exceeds Φ0 . The position of atom i in configuration B is denoted by r i . Because B is selfequilibrated, average static atomic stress measures vanish by definition:
7.3 Atomistic Interpretation of Residual Elasticity
σ ab =
1 2Ω
∑r i≠ j
a ij
δ bc
∂Φ 1 = 0 , P aA = c ∂r ij 2Ω0
∑δ i≠ j
ab
∂Φ A R =0. ∂r ijb ij
371
(7.95)
with Ω = J Ω0 the system volume in B , Φ the potential energy of (7.83), and r ij = r j − r i . Because atomic coordinates are not mapped homogeneously from their positions in B0 to their positions in B , the average first PiolaKirchhoff stress measure in the second of (7.95) does not follow from a linear transformation such as used in the chain rule in (7.84); it is instead introduced in (7.95) as a fundamental definition. Equation (7.95) contains discrete analogs of continuum selfequilibrium conditions (7.20) and (7.26). As in (7.86), the potential energy is expanded in a series about a perfect reference configuration: 1 Φ = Φ0 + ∑ H abijkl δ ac q cij δ bd q dkl 2 i≠ j k ≠l
+
1 ∑ H abc δ ad q dij δ be q ekl δ cf q mnf + ..., 6 i ≠ j ijklmn
(7.96)
k ≠l m≠n
with q ij = r ij − R ij the displacement difference between two atoms in the defective selfequilibrated lattice, and where (7.88) has been used to define atomic stiffness coefficients. Substituting (7.96) into the first of (7.95) and multiplying through by J , the null average atomic stress relation becomes 1 0 = J σ fa = ∑ r f H ab δ bc q ckl 2Ω0 i ≠ j ij ijkl k ≠l
+
1
∑ r ijf H abcijklmn δbd q dkl δ ce q emn + ....
(7.97)
4Ω0 i ≠ j
k ≠l m≠n
As in (7.33)(7.37), vanishing of the average symmetric stress measured in the reference configuration leads by definition to six equations for six unknown components of symmetric deformation map F I . Identifying harmonic terms in the atomic definition of the average stress with linear terms in the continuum elastic definition of the average stress: 1 1 A B (7.98) ^ ABCD uC , D dV ⇔ δ . f δ.a ∑ r ijf H abijkl δ bc q ckl , ∫ VV 2Ω0 i≠ j
k ≠l
continuum elasticity discrete lattice statics
the following definition emerges (Clayton and Bammann 2009):
372
7 Residual Deformation from Lattice Defects
^ ABCD ( F I CD − δ CD ) =
1 2Ω0
=−
δ . Af δ .aB ∑ r ijf H abijkl δ bc q ckl i≠ j k ≠l
1 4Ω0
δ . Af δ .aB ∑ r ijf H abc δ q d δ q e − ..., ijklmn bd kl ce mn
(7.99)
i≠ j k ≠l m≠ n
with the second equality in (7.99) following directly from (7.97). Assuming as usual that the reference stiffness of the perfect lattice ^ ABCD is positive definite, 1 1 SCDAB [( δ. Af δ.aB ) ∑ r ijf H abc F I CD = δ CD − δ q d δ q e + ...] , (7.100) ijklmn bd kl ce mn 4 Ω0 i≠ j k ≠l m≠n
where secondorder elastic compliance SCDAB satisfies (7.38) and can be found from inverting the secondorder reference moduli (7.93). The series in brackets on the right of (7.100) accounts for anharmonic interactions, and includes terms of orders two and higher in relative atomic displacements q aij in the locally deformed, yet selfequilibrated, defective lattice.
= 0 and/or quadratic For harmonic lattice statics, in which case H abc ijklmn and higherorder terms in q aij are dropped from (7.100), the bracketed series degenerates to zero and F I CD = δ CD , analogously to linear continuum description (7.35). The definition for F I CD implied by the first of (7.99), while not unique, is motivated by its analogous continuum definition F I CD = V −1 ∫ x( C , D ) dV = V −1SCDAB ^ ABEF ∫ x( E , F ) dV in (7.31). Following Section 7.2.6, the firstorder accurate residual volume change is J = Ω / Ω0 ≈ det(F I ) ≈ tr(F I ) − 2 , where continuum and discrete measures of reference and intermediate volumes are related, respectively, by Ω0 = V and Ω = V + ∆V . Calculation of this volume change does not require identification of a bounding surface delineating the volume occupied by the atoms in configuration B ; i.e., the atoms can occupy an arbitrary shape so long as their interaction forces selfequilibrate. If such a surface can be identified in a lattice statics calculation, for example an ensemble of atoms in a defective state contained within a hexahedral bounding box, it should be possible to compute Ω trivially (i.e., Ω is then the volume of the box) and then compare results with predictions of (7.100), so long as the average static virial stress vanishes over the defective ensemble of atoms. An apparent advantage of the atomistic approach of Section 7.3 over
7.4 Point Defects and Residual Elasticity
373
the continuum approach of Section 7.2 is that effects of defect cores are accurately incorporated in the former, presuming that the atomic potential is sufficiently robust to model defect core structures. An apparent disadvantage is that solutions to (7.100) must be computed numerically, while the continuum approach pioneered by Zener (1942), Seeger and Haasen (1958), Toupin and Rivlin (1960), and Holder and Granato (1969) provides convenient analytical formulae for volume changes such as (7.59)(7.61).
7.4 Point Defects and Residual Elasticity In continuum and solid state physics, point defects are often idealized as spheres embedded in an elastic medium (Bitter 1931; Eshelby 1954, 1956; Holder and Granato 1969). Since spheres have finite volume, formation of such defects necessarily involves a volume change, regardless of the rigidity of the surrounding medium. This situation is in contrast to idealized line defects of the sort addressed in Section 7.2, e.g., dislocation and disclination lines, which have no intrinsic volume, though the surrounding elastic medium can still undergo dilatation as a result of the presence of such line defects. In Section 7.4.1, a model for the deformation gradient contribution resulting from generation of a point defect and its elastic fields is suggested, combining results of Sections 3.2.8, 7.2, and C.4 of Appendix C. In Section 7.4.2, the particular example of a monovacancy in copper is discussed and predictions are compared with experimental observations.
7.4.1 Spherical Deformation from a Point Defect Recall from Section 3.2.8 that the total lattice deformation gradient for an elastic body with an isotropic distribution of spherical point defects can be written as FL = FEFV , (7.101) where the residual volumetric deformation from defects is (7.102) F V α.β = (1 − φ )−1/ 3 δ .αβ = J V 1/ 3δ .αβ , J V = det(F V ) . As shown in Fig. 3.10, F V : TB → TB , where externally unloaded configuration B is analogous to that in Fig. 7.1. From (3.133)(3.135), the volume fraction of point defects per unit volume in B is φ = αξ = [ ±Ω0 + (1 + Γ)∆v ]ξ , (7.103)
374
7 Residual Deformation from Lattice Defects
where ξ is the number of defects per unit volume in B and α is the net volume change per defect. When F = F L , (7.103) can also be written as φ0 = αξ0 = [ ±Ω0 + (1 + Γ)∆v ]ξ0 , (7.104) where φ0 = J V φ and ξ 0 = J V ξ are defined per unit reference volume. Recall from Section 3.2.8 that ±Ω0 → Ω0 in (7.103)(7.104) when a vacancy enters the volume element (e.g., via diffusion at a free surface) and free volume of the crystal increases by atomic volume Ω0 , while ±Ω0 → −Ω0 in (7.103)(7.104) when an atom moves from a lattice site to an interstitial position in the idealized situation when no vacancy is left behind. For a substitutional atom, the ±Ω 0 term is omitted, and α = (1 + Γ)∆v . The algebraic sign of ∆v is positive for an interstitial or a substitutional atom of larger size than the atom it replaces. The algebraic sign of ∆v is negative for a vacancy or a substitutional atom smaller than the atom it replaces. In a polyatomic crystal, the magnitude and sign of ∆v will generally depend on the atomic species of the defect under consideration, as well as any possible electric charge associated with the defect (e.g., in an ionic crystal). The magnitude of relaxation volume ∆v depends on the interaction of the point defect with the surrounding crystalline medium. In the linear elastic approximation, idealizing the surrounding crystalline material as isotropic and the point defect as a rigid sphere, analytical solutions are available, as presented in Sections C.3.1 and C.3.2, respectively, for an infinitely extended elastic medium and an elastic medium of finite dimensions. An analytical solution is also available for a deformable elastic sphere embedded in a finite medium (Section C.3.3 of Appendix C), but such a model is not invoked here in the context of point defects because assignment of continuum elastic constants to a sphere of dimensions of a single atom is deemed too severe an assumption. The simplest model, discussed in Section C.3.1, idealizes the defect as a rigid sphere and the surrounding medium as infinitely extended. The relaxation volume is given by (C.188): ∆v = δ V = 4π A , (7.105) where A is a misfit parameter that must be determined from experiments or atomic scale calculations. The average strain energy density of the elastic medium surrounding a single defect is purely deviatoric, as listed in (C.187):
7.4 Point Defects and Residual Elasticity
375
3 6 µ A2 ⎡ ⎛ r0 ⎞ ⎤ 6 µ A2 WS = 3 3 3 ⎢1 − ⎜ ⎟ ⎥ ≈ 3 3 ( R0 − r0 ) r0 ⎢ ⎝ R0 ⎠ ⎥ ( R0 / r0 − 1) r06 ⎣ ⎦ (7.106) 2 2 6µ A 8πµ A (32 / 3)π 2 µ A2 (2 / 3) µ (δ V ) 2 . ≈ 3 3 = = = R0 r0 [(4π / 3)r03 ]R03 Ω 0 (4π / 3) R03 Ω 0 (4π / 3) R03
The radius of the spherical point defect is r0 , and the radius of a spherical region of the surrounding medium is R0 . Successive approximations in (7.106) correspond to R03 / r03 1 , i.e., a very small defect in a much larger sample of material. For N dilute defects in the case where interactions among defects are reasonably omitted, (7.106) is extended to 2µ N 2µ = (δ V )2 (δ V ) 2 ξ 0 , WS ≈ (7.107) 3 3Ω0 (4π / 3) R0 3Ω0 with ξ0 = N / V the number of defects per unit reference volume as in (7.104). The relaxation volume can then be estimated by equating the product of (7.107) and the reference volume V with formation energy EF of a single ( N = 1 ) point defect: 1/ 2
⎛ 3Ω E ⎞ 4π 3 2µ (δ V ) 2 ⇒ δ V = ± ⎜ 0 F ⎟ = ∆v . (7.108) EF = R0WS = 3 3Ω 0 ⎝ 2µ ⎠ The description of Section C.3.2 treats the defect as a rigid sphere embedded in a finite volume of isotropic elastic material. The volume change, from (C.195), is ⎡ 4µ ⎤ ⎡ 3(1 − ν ) ⎤ (7.109) ∆v = 4π A ⎢1 + = 4π A ⎢ ⎥ ⎥, ⎣ 3K ⎦ ⎣ 1 +ν ⎦ where the misfit parameter −1
3 δ V ⎡ 4µ ⎛ r0 ⎞ ⎤ ⎢1 + A= ⎜ ⎟ ⎥ . 4π ⎢ 3K ⎝ R0 ⎠ ⎥
(7.110) ⎣ ⎦ The radius of the spherical point defect is r0 , and the tractionfree external surface of the surrounding crystal is located at radial coordinate R0 . For R03 / r03 1 , −1
3 ⎡ 3(1 − ν ) ⎤ ⎡ 4µ ⎛ r0 ⎞ ⎤ ⎡ 3(1 − ν ) ⎤ ⎢ ∆v = ⎢ 1+ ⎜ ⎟ ⎥ δV ≈ ⎢ ⎥ ⎥ δ V = cδ V , ⎣ 1 + ν ⎦ ⎢⎣ 3K ⎝ R0 ⎠ ⎥⎦ ⎣ 1 +ν ⎦
(7.111)
where the dimensionless elastic constant c = 3(1 − ν ) /(1 + ν ) . The strain energy density is not purely deviatoric, since local pressure and elastic
376
7 Residual Deformation from Lattice Defects
dilatation are nonzero in (C.194). However, inserting (7.111) into (7.108) as an approximation, the relaxation volume is estimated as 1/ 2
1/ 2
⎛ 3Ω E ⎞ ⎡ 3(1 −ν ) ⎤ ⎛ 3Ω0 EF ⎞ ∆v = cδ V = ± c ⎜ 0 F ⎟ = ± ⎢ ⎟ . (7.112) ⎥⎜ ⎣ 1 + ν ⎦ ⎝ 2µ ⎠ ⎝ 2µ ⎠ The additional volume change resulting from nonlinear elastic effects is estimated using (7.60), assuming the strain energy density is deviatoric, following Eshelby (1954): ⎤ ⎛ ∂µ µ ⎞ ⎡ 2 ∆V 1 ⎛ ∂µ µ ⎞ ≈ ⎜ − ⎟WS ≈ ⎜ − ⎟⎢ (δ V ) 2 ξ 0 ⎥ V µ ⎝ ∂p K ⎠ ⎝ ∂p K ⎠ ⎣ 3Ω0 ⎦ (7.113) 1 ⎛ ∂µ µ ⎞ = ⎜ − ⎟ EF ξ 0 . µ ⎝ ∂p K ⎠ Thus, in (7.103) and (7.104), the additional volume change per defect resulting from nonlinearity is estimated as ∆V / V 1 ⎛ ∂µ µ ⎞ Γ∆v = = ⎜ − ⎟E . (7.114) ξ0 µ ⎝ ∂p K ⎠ F When point defects are embedded in an infinite medium, (7.108) gives 1/ 2
⎛ ∂µ µ ⎞ ⎛ 2 EF ⎞ ∆V / V ⎛ ∂µ µ ⎞ EF (7.115) Γ= =⎜ − ⎟ = ±⎜ − ⎟⎜ ⎟ . ξ0 ∆v ⎝ ∂p K ⎠ µ∆v ⎝ ∂p K ⎠⎝ 3µΩ0 ⎠ When point defects are embedded in a finite medium, (7.112) gives 1/ 2
1/ 2
⎡ 1 + ν ⎤ ⎛ ∂µ µ ⎞ ⎛ 2 EF ⎞ 1 ⎛ ∂µ µ ⎞ ⎛ 2 EF ⎞ Γ=± ⎜ − ⎟⎜ − ⎟⎜ ⎟ = ±⎢ ⎟ . (7.116) ⎥⎜ c ⎝ ∂p K ⎠ ⎝ 3µΩ 0 ⎠ ⎣ 3(1 − ν ) ⎦ ⎝ ∂p K ⎠ ⎝ 3µΩ0 ⎠ Algebraic signs for the ± symbols in (7.115) and (7.116) match those of corresponding relaxation volume ∆v . Correction factor Γ can be positive or negative in sign depending on algebraic signs of ∆v and the term ∂µ / ∂p − µ / K . 7.4.2 Example: Vacancies in Copper
Representative results of the theory outlined in Section 7.4.1 are listed in Table 7.5 for copper, applied to single point vacancies (i.e., monovacancies). Properties used in the calculations correspond to those listed in Tables 7.3 and 7.4. The atomic volume for a monatomic FCC crystal (four atoms per conventional unit cell) is Ω0 = a 3 / 4 = b3 / 2 . Poisson’s ratio ν used to obtain elastic constant c is listed in Table 7.3. The vacancy formation energy EF and defect energy per atomic volume change
7.4 Point Defects and Residual Elasticity
377
EF Ω0 / α were obtained from independent experiments (Simmons and Balluffi 1963; Nilan and Granato 1965). The experimental value of EF listed in Table 7.4 is used, however, in the model predictions of relaxation volume ∆v , nonlinear elastic corrector Γ , and total volume change α listed in columns 24 of Table 7.5. Table 7.4 Properties for copper Vacancy formation energy 3 − 3ν EF (1) [eV/atom] 1 +ν 11.81 1.41 1.17 (1) Simmons and Balluffi (1963) Atomic volume Ω0 [Å3]
c=
Table 7.5 Volume changes from vacancies in copper Model or experiment
Relaxation ∆v / Ω 0 Infinite medium 0.71 Finite medium 1.01 Experiment(1) (1) Nilan and Granato (1965)
Nonlinear correction Γ 0.23 0.16 
Total volume change α / Ω0 0.45 0.16 0.32
EF Ω 0 / α [eV/atom] 2.6 7.3 3.7
Values in the first row of results in Table 7.5 correspond to the model of a point defect in an infinitely extended elastic body of the sort described in Section C.3.1, specifically relations (7.108) and (7.115). Values in the second row of results in Table 7.5 correspond to the model of a point defect in a finite elastic body with traction free outer surface as addressed in Section C.3.2, specifically (7.111) and (7.116). Negative algebraic signs apply for ∆v and hence Γ , since the relaxation volume is negative for a vacancy (i.e., surrounding atoms are pulled towards the vacant lattice site) and since ∂µ / ∂p − µ / K = 0.49 > 0 for copper. The total normalized volume change from (7.103) or (7.104) applied to a vacancy is then computed, per atomic volume, as α ∆v = 1 + (1 + Γ ) . (7.117) Ω0 Ω0 Experimental results listed in Table 7.5 are obtained from measurements of volume changes and energy released during annealing of deuteronirradiated, i.e., radiationdamaged, copper foils (Nilan and Granato 1965). The total volume changes predicted by the two continuum models bound the experimental results from above and below, and all predictions agree with model results within a factor of two. Predicted relaxation volumes
378
7 Residual Deformation from Lattice Defects
are on the order of the atomic volume, and nonlinear elastic effects are nonnegligible since  Γ  is not small compared to unity.
8 Mechanical Twinning in Crystal Plasticity
Twinning in a general sense may encompass a variety of energyinvariant transformations of a crystal structure. A twin in a crystalline solid is usually defined as two regions of a crystal separated by a coherent planar interface called a twin boundary, though interpenetrating twins with irregular interfaces are also possible. Limiting values of deformation gradients in each region, on either side of the interface, differ by a simple shear. Twinning can be induced by a variety of mechanical, thermal, electrical, or chemical stimuli. Annealing twins or growth twins emerge during growth of a crystal. Another notable example is a set of finely twinned layers or lamina associated with kinematically compatible, low energy configurations emerging at or near the transformation temperature in the crystallographic theory of martensite (Ball and James 1987; Bhattacharya 1991), i.e., solidsolid polymorphic phase transformations. The present Chapter does not address such phase transformations, annealing, or crystal growth. Rather, the focus of Chapter 8 is a particular kind of twinning labeled mechanical twinning, which by definition is induced by mechanical stresses (Kosevich and Boiko 1971; James 1981). The part of the mechanical stress tensor responsible for twinning is most typically a resolved shear stress acting on the normal to the plane of the twin, in the direction of twinning shear or twin propagation. The term deformation twinning (Christian and Mahajan 1995) is used interchangeably with mechanical twinning. When subjected to large deformations or large mechanical stresses, crystalline solids may deform via a number of mechanisms. As discussed in Chapter 6, when dislocation mobility is sufficiently high in an adequate number of directions, dislocation glide is the predominant accommodation mode for deviatoric deformations in ductile crystals at stresses above the elastic limit. On the other hand, depending on the particular kind of crystal and the loading conditions, inelastic deformation may be supported by other mechanisms such as deformation twinning. As reviewed by Christian and Mahajan (1995), a number of theories, some complementary and some competing, exist that describe twin nucleation and propagation. Differences in twinning behaviors, or lack thereof, among crystals of various compositions and structures inhibit the formula
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_8, © Springer Science+Business Media B.V. 2011
379
380
8 Mechanical Twinning in Crystal Plasticity
tion of a universal theory for kinetics of deformation twinning in crystals of arbitrary composition and structure. In treatments of thermodynamics and kinetics that follow later in Chapter 8, deformation twinning is associated with thermodynamically irreversible shape deformation in correspondence with collective motion of partial dislocations and formation of stacking faults (Bilby and Crocker 1965; Christian and Mahajan 1995). Deformation twinning is thought to be preferred over slip in cases wherein resistances to dislocation glide are very large in certain directions (Hirth and Lothe 1982), such as often occurs in crystal systems of noncubic symmetry. For example, in hexagonal crystals, twinning is often favored over slip in directions not contained within the basal plane. In certain hexagonal or rhombohedral ceramics such as alumina (i.e., sapphire or corundum), slipmediated shearing on basal and prismatic planes is often the preferred inelastic deformation mechanism, with slip resistances in directions normal to the basal plane extremely high (Veit 1921; Kronberg 1957; Bourne et al. 2007; Clayton 2009a). This phenomena occurs similarly in many hexagonal metals, including certain alloys of zirconium (Tome et al. 1991; Kalidindi 1998), titanium (Schoenfeld and Kad 2002), and magnesium (Staroselsky and Anand 2003), though secondary slip on pyramidal systems is sometimes possible. In many cases, deformation twinning, as opposed to slip, may be the only viable mechanism for accommodating deformation normal to the basal plane, in lieu of fracture. Twinning is often preferable to slip at lower temperatures in crystals with cubic symmetry, especially those with low stacking fault energy (Meyers et al. 2001; Bernstein and Tadmor 2004). For example, it has been observed that aluminum (stacking fault energy 170 mJ/m 2 ) is less likely to twin than copper (stacking fault energy 60 mJ/m 2 ). The description set forth in Chapter 8 accounts for mechanisms of elasticity, plastic slip, and deformation twinning in single crystals. Each mechanism is addressed independently via an individual term within a threeterm multiplicative decomposition of the deformation gradient. According to this representation, plastic deformation is deemed latticepreserving (i.e., dislocation glide does not affect the Bravais lattice vectors or stored elastic energy of the crystal), following treatments of Chapter 3 (Section 3.2) and Chapter 6. In contrast, twinning is modeled here distinctly from dislocation plasticity via the use of an intermediate term in the deformation gradient decomposition. Threeterm decompositions were suggested by Kratochvil (1972) and Clayton et al. (2005), who introduced intermediate terms within threeterm decompositions to account for irreversible deformations distinct from those arising from dislocation glide. Following the scheme of continuum crystal plasticity theory of Sections
8.1 Mechanisms: Elasticity, Slip, and Twinning
381
3.2.6 and 6.3, plastic deformation takes place via slip on one or more discrete systems. Twinning takes place via shears of predefined magnitude, with the rate of shearing determined by the rate of increase in volume fraction of the twin relative to the parent crystal (Chin et al. 1969; Van Houtte 1978; Kalidindi 1998; Staroselsky and Anand 1998, 2003). Microscopic strain fields associated with lattice defects may also contribute to irreversible deformation. In particular, net volume changes associated with residual strain fields of defects, as derived in Section 7.2.4, are directly incorporated into the extended crystal plasticity theory of Chapter 8. Finally, thermomechanically reversible deformation of the lattice is addressed via the elastic term in the decomposition, encompassing both the recoverable deformation associated with mechanical stresses and thermal expansion or contraction associated with temperature changes. A constitutive framework based on internal state variable theory provides thermodynamic relationships among independent and dependent state variables as well as appropriate driving forces for evolution of internal state variables and rates of inelastic deformations. Here, internal state variables consist of dislocation and twin boundary densities, and inelastic deformation rates include rates of slip and of twinned volume fractions. Dislocation densities are partitioned into geometrically necessary dislocations associated with slip gradients and statistically stored dislocations associated with homogeneous plastic flow and dislocation loops. Recall that formal definitions of dislocation densities are given in Section 3.3.2. Interface partial dislocations at propagating twin boundaries (Scott and Orr 1983) are demonstrated to contribute to the geometrically necessary dislocation density tensor. Thermodynamic restrictions on kinetic relations follow naturally from energy conservation requirements and the entropy production inequality. Averaging concepts are invoked to describe effects of twinning on the thermoelastic response of an element of crystal containing one or more twins, leading to effective anisotropic moduli and dissipation rates that depend upon volume fractions of twins in the crystal. In Section 8.1, brief physical descriptions of elasticity, plasticity, and twinning in crystalline solids are provided, with a focus on twinning. These descriptions serve to clarify the distinctions among the three deformation mechanisms and provide sufficient physical basis for the corresponding model framework that follows in Section 8.2. The framework of Section 8.2 may be applied to describe any crystalline solid that undergoes large deformations via elasticity, plasticity, and/or twinning, including many metallic and ceramic crystals and crystalline minerals.
382
8 Mechanical Twinning in Crystal Plasticity
8.1 Mechanisms: Elasticity, Slip, and Twinning Elasticity, slip, and twinning are described in Sections 8.1.1, 8.1.2, and 8.1.3, respectively. Regarding elasticity and slip, some redundancy with previous descriptions given in Sections 3.1 and 3.2 is unavoidable, but necessary, in order to enable a complete description of mechanical twinning. 8.1.1 Elasticity
Elastic deformation is addressed in detail in Chapter 3 (Section 3.1) and Chapter 5. A crystal is said to deform elastically in the absence of generation or motion of defects. At the atomic scale, elastic deformation alters distances and/or orientations between neighboring atoms within each crystallographic unit cell. The resulting changes in interatomic forces produce mechanical stresses when the crystal is viewed as a continuous solid. Removal of mechanical stresses restores the original lattice without any dissipation of energy; hence, according to the usual idealization, such elastic deformation is said to be thermodynamically reversible. Elastic deformation as defined in Chapter 8 also includes changes in interatomic bond vectors induced by changes in temperature. At the atomistic scale of resolution, increases in local thermal vibration of atoms about their reference positions (i.e., phonons), result in expansion of the lattice in the absence of mechanical stresses. Such thermal deformations are also idealized as reversible, since presumably, in the absence of other applied stimuli, atoms of the crystal will return to their reference mean or equilibrium arrangement as the temperature is reduced to its original value. Let F E ( X , t ) denote the twopoint tensor of large (i.e., geometrically nonlinear) thermoelastic deformation, simply referred to as the elastic deformation in Chapter 8. When the crystal contains defects (e.g., dislocations), the elastic deformation will generally not be associated with the true derivative of any displacement field, and correspondingly, the compatibility conditions F E −1α.[a ,b] = 0 are not satisfied in general, in contrast to
(2.203) which apply for the total deformation gradient F ( X , t ) . Let Ai ( i = 1, 2,3 ) denote primitive Bravais lattice vectors of (3.1). Then according to the CauchyBorn hypothesis (Born and Huang 1954; Ericksen 1984) of Section 3.1.2 and (3.17), when the total deformation is elastic, ai = F E A i , ( i = 1, 2,3 ), (8.1)
8.1 Mechanisms: Elasticity, Slip, and Twinning
383
with ai the primitive Bravais lattice vectors in the deformed crystal. Elastic deformation of a primitive noncubic lattice is illustrated in Fig. 8.1(a); note the deformation of a representative primitive Bravais lattice vector a1 = F E A1 .
Fig. 8.1 Deformation mechanisms and lattice vectors: (a) elasticity, (b) plastic slip, (c) twinning
Let ψ denote the Helmholtz free energy per unit mass of the crystal, as first introduced in Table 4.2. This energy is postulated, for illustrative purposes in Section 8.1, to depend only on the elastic deformation at particular material location X and at a given time t. Then the free energy satisfies the usual constraints imposed by invariance and material symmetry: ˆ E H, X ≥ ψ (1, X ) = ψ QH ˆ ,X . ψ ( F E , X ) = ψ QF (8.2)
(
ˆ =Q ˆ In (8.2), 1 is the unit tensor, Q
)
(
)
−T
represents any rigid body rotation of ˆ = +1 , and H ∈ H is any member the spatial coordinate frame with det Q of the group H of affine transformations of the Bravais lattice that does not affect its free energy. The point group of symmetry operations (i.e., rotations, reflections, and inversions) for the crystal class to which the material belongs is a subset of this potentially larger group of energy invariant transformations, i.e., ∈ H . The first of (8.2) corresponds to (A.1) of Appendix A when F E = F and H = Q ∈ , where Q is a member of the point group as introduced in Section 5.1.5 in the context of elastic symmetry. Point groups and crystal classes are discussed in more detail in Section A.1 of Appendix A. Matrix H is not necessarily orthogonal and hence may fall outside the point group, as demonstrated explicitly later in Section 8.1.3 wherein H is associated with twinning shear. Relation (8.2) implies that the state characterized by null elastic deformation, F E = 1 , correlates with a local minimum of the free energy density ψ at point X.
384
8 Mechanical Twinning in Crystal Plasticity
8.1.2 Plastic Slip Plastic deformation is discussed at length in Section 3.2 of Chapter 3 from the perspective of kinematics and in Chapter 6 from the perspective of thermomechanics and kinetics. Plastic deformation as addressed in this context occurs via glide of dislocations of edge, screw, and/or mixed character, including loops, and encompassing crossslip but not dislocation climb. As discussed in Section 3.2.2, as full dislocations travel through a region of the lattice, the shape of the material will change, but the interatomic bond vectors remain the same (upon translation of planes by an integer multiple of the Burgers vector), so long as no defects are left behind within the region. In this sense, the plastic deformation is said to be latticepreserving. Collective motion of leading and trailing partial dislocations is also latticepreserving, since trailing partial(s) erase the stacking faults left in the wake of leading partials and hence restore the lattice periodicity. Mechanical stresses are conventionally required to enact glide of dislocations, apart from random thermal fluctuations such as occurring in kink migration. For example, according to Schmid’s law, resolved shear stresses in (6.70) or (6.86) must exceed a threshold stress consisting of superposition of the Peierls barrier (C.248) and influences from other defects as in (6.99). Plastic deformation is thermomechanically irreversible, since the reference shape of the material is not recovered upon removal of mechanical stresses, and since heat is dissipated by moving dislocations as a result of lattice friction, phonon drag, and other mechanisms (Kocks et al. 1975; Gilman 1979). Plastic dissipation converted to temperature rise is evident from (6.43) and (6.45)(6.47). Because the crystal lattice remains unchanged apart from steps on its surface, plastic deformation itself does not affect the strain energy of the crystal. However, defects generated during the course of plastic deformation that remain within the material lead to energy storage as a result of the local stress fields supported by these defects. Such effects are captured in continuum theories by internal state variables, leading for example to a TaylorQuinney parameter β ′ < 1 in (6.46) during some part of the deformation history. Let F P ( X , t ) denote the twopoint tensor of potentially large plastic deformation. The plastic deformation will generally not be the derivative (i.e., true material gradient) of a displacement function, and correspondingly, compatibility conditions F Pα.[ A, B] = 0 are not always satisfied, imply
ing existence of geometrically necessary dislocations in the crystal, as is evident from kinematic relations (3.217)(3.227) of Section 3.3.2. Plastic deformation is illustrated conceptually for a noncubic lattice in Fig. 8.1(b). On the right side of the figure, the slip plane is denoted by the
8.1 Mechanisms: Elasticity, Slip, and Twinning
385
dashed line. Note that the lattice vector A1 is unchanged by the action of the plastic deformation, in agreement with (3.107). As demonstrated in (3.116) the corresponding implication in crystal plasticity theory is that slip directions and slip plane normal vectors are unaffected by F P . Since plastic deformation is latticepreserving and consists of shearing in one or more directions, the volume of the material remains unaffected, and hence J P = 1 , as emphasized in Section 7.1.1. Furthermore, because the (continuum) plastic deformation by definition consists only of relative shear displacements of crystallographic planes in integer multiples of the Burgers vector, the free energy density of the crystal cannot depend explicitly on FP : ∂ψ = 0, (8.3) ∂F P FE ,θ ,α where elastic deformation, temperature, and internal state variable(s) are held fixed in the partial derivative. At the atomic scale, slip can be further understood by considering the generalized stacking fault energy (Vitek 1966; Zimmerman et al. 2000; Ogata et al. 2005): EGSF (∆x) = EGSF (∆x + li b) , EGSF (0) = EGSF (li b) = 0 , ( li ∈ ). (8.4) The relative shear displacement between two neighboring crystallographic planes is denoted by ∆x , li is any integer, and b is the Burgers vector of a full dislocation. The energy in (8.4) is minimal at null relative displacement, corresponding to a perfect reference lattice, and exhibits periodic total minima for rigid translations of planes by integer multiples of the Burgers vector. Local minima in generalized stacking fault energy surfaces, often called γsurfaces, can be associated with metastable stacking faults, i.e., partial dislocations. The total energy of the atomic ensemble also includes energies of defect cores and residual stress fields of defects; in complementary continuum treatments such energetic contributions are measured by internal state variables, as discussed in Section 4.2.1. 8.1.3 Deformation Twinning
Deformation twinning results in two connected regions in the lattice separated by a twin boundary (i.e., the dotted line on the right side of Fig. 1 (c)) whose shape deformations differ by a simple shear. The original region of the crystal is termed the parent, while the sheared region is termed the twin. According to the classical definition of a deformation twin, atomic positions, and hence primitive Bravais lattice vectors and basis vectors, within each region differ by a proper or improper rotation, typically either
386
8 Mechanical Twinning in Crystal Plasticity
a reflection or 180° rotation (Christian and Mahajan 1995), though more general relationships are possible. The stacking sequence of atomic planes in the twin is altered or reversed with respect to that in the parent, and hence crystals with low stacking fault energies are usually more prone to twin formation than those with high stacking fault energies. Nucleation and propagation of deformation twins are though to take place by one or more mechanisms, often involving the formation and motion of partial dislocations (e.g., dissociation of full dislocations into partials) and possible atomic shuffles needed to maintain the orientation relationships between the twin and parent (Cottrell and Bilby 1951; Bilby and Crocker 1965; Hirth and Lothe 1982; Pirouz 1987; Zanzotto 1996; Lagerlof et al. 2002). Partial dislocations associated with twin growth are often labeled as twinning dislocations, and these twinning dislocations often have Burgers vectors whose magnitudes are very small fractions of full dislocations in the same crystal structure. In some cases, e.g., the standard twinning modes for BCC and FCC crystals listed in Table 8.1, twins can be formed by simple shearing of the Bravais lattice vectors alone. In other cases, atomic shuffles, i.e., additional displacements of only some of the atoms in the twin, are required in order to maintain the orientation relationship among all atoms in twin and parent. Such shuffles or relative displacements are usually mandatory in polyatomic crystals, i.e., those with a basis of more than one atom per primitive unit cell. Twinning is not regarded as latticepreserving in the sense of slip, since twinning involves rotation of the lattice, as evidenced by crystallographic texture measurements (Van Houtte 1978; Tome et al. 1991). The involvement of partial dislocations and atomic shuffles, for example, induces the rotational change of the twinned lattice relative to that of the parent. Such changes in the lattice orientation do not occur under plastic deformation arising from the slip of full dislocations, as shown in Fig. 8.1(b). Deformation twinning is also distinguished from plastic slip in that the former occurs by collective motion of defects, resulting in a quantized amount of shear, denoted by γ j on twin system j, that preserves a particular orientation relationship between the twin and parent. In contrast, plastic deformation may conceivably result in shearing of any maximum magnitude, with the lower limit of relative displacement between two lattice planes limited by the Burgers vector for slip. The shear strain associated with deformation twinning is usually mechanically irreversible, since fully formed twins remain in single crystals after mechanical stresses are removed1. Twins of1 Elastic twinning is physically possible (Cooper 1962; Kosevich and Boiko 1971). Elastic twins partially or fully disappear upon load relaxation, though dissipation associated with hysteresis can still be significant if the loading is cyclical.
8.1 Mechanisms: Elasticity, Slip, and Twinning
387
ten seem to propagate very rapidly relative to slipped regions or slip bands (Christian and Mahajan 1995), even in low strain rate experiments as evidenced by load drops in the stressstrain response (Kronberg 1968; Scott and Orr 1983). When driving stresses are sufficiently large, tapered twin lamellae can extend or grow at velocities exceeding the elastic shear wave speed of the crystal, though the velocity of the twin resolved in the direction normal to its boundary surface must remain subsonic (Rosakis and Tsai 1995). Much slower twin growth kinetics has also been reported. Cooper (1962) measured velocities in transparent calcite that were only a small fraction of the elastic wave speed and were not strongly dependent on the applied shear stress. Another difference between slip and twinning is that twinning is polarized while slip is not. Geometry of the lattice tends to prevent twinning shears of equal magnitude and opposite directions on the same plane, while typically slip may initiate in opposite directions on the same plane. In typical crystal plasticity models, the initial resistance to slip is assumed the same in forward and reverse directions, though this assumption is not always warranted in BCC crystals (Vitek 1976; Lee et al. 1999) or in nonmetals such as lowsymmetry ceramics (Clayton 2009a, 2010c). Dislocation motion resulting in shear deformation in the opposite direction to the twinning direction on the same set of planes is known as antitwinning, and is physically possible. However, the mechanical resistance, in terms of shear stress, to antitwinning, can be several times greater than the resistance to twinning (Paxton et al. 1991).
Fig. 8.2 Twin geometry and notation (Christian and Mahajan 1995) Wedgeshaped elastic twins have been observed experimentally in semiinfinite crystals subjected to concentrated surface forces, for example knifeedge loading. If the region of the parent (matrix) is plastically deformed, then such an induced twin will not be elastic, but will instead remain present in the material upon unloading as a result of the constraint of the surrounding plastically deformed matrix. Thus, elastic twinning appears more common in certain nonmetals such as calcite wherein twinning is much easier than slip, and less common in metals that tend to undergo plastic slip and twinning simultaneously (Cooper 1962).
388
8 Mechanical Twinning in Crystal Plasticity
A geometric depiction of twinning is provided in Fig. 8.2, following the classical notational scheme of Bilby and Crocker (1965) and Christian and Mahajan (1995). The geometry of the twin is characterized by the four twinning elements {K1 , K 2 , η1 , η2 } . The surface of composition separating parent and twinned regions of crystal is often called the habit plane and is labeled K1 . The direction of relative shear is η1 . The plane S, called the plane of shear, contains both η1 and the normal to K1 . Plane K 2 is called the second undistorted plane, and contains those vectors that are only rotated, but not stretched, by the simple shearing operation associated with twinning. Vector η2 , referred to as the conjugate shear direction, is the intersection of planes S and K 2 . A twinning mode can be defined by values of either the pair {K1 , η2 } or the pair {K 2 , η1} , though it is customary to specify all four elements plus the magnitude of shear γ j . When components of {K 1 , η2 } in Miller index notation—see Section 3.1.1—consist of rational numbers, the twin is said to be of type I, while when components {K 2 , η1} are rational in Miller index notation, the twin is said to be of type II. When components of all four elements {K1 , K 2 , η1 , η2 } are rational, the twin is said to be compound. Primitive Bravais lattice vectors in the twin and parent in a type I twin are related by either a reflection in K1 (type Ia) or rotation of 180° about the direction normal to K1 (type Ib). For a type II twin, the lattice vectors are related by either a rotation of 180° about η1 (type IIa) or a reflection in the plane normal to η1 (type IIb). Mathematically, in Cartesian coordinates, the orthogonal transformations ⎧ 1 − 2m 0 ⊗ m 0 , ⎪ 2m ⊗ m − 1, ⎪ 0 0 Q=⎨ s s 1, 2 ⊗ − 0 ⎪ 0 ⎪⎩ 1 − 2s 0 ⊗ s0 ,
(type Ia), (type Ib), (type IIa),
(8.5)
(type IIb)
relate a primitive Bravais lattice vector in the parent, A i , to a vector in the twin ai , via ai = QA i , as shown in Fig. 8.1(c) for i = 1 . A unit vector normal to the habit plane K 1 is denoted by m 0 . A unit vector parallel to the shear direction η1 is denoted by s 0 . Transformations for types Ib and IIa are rotations or proper orthogonal transformations, while transformations for types Ia and IIb are reflections or improper orthogonal transfor
8.1 Mechanisms: Elasticity, Slip, and Twinning
389
mations2. All transformation matrices listed in (8.5) will generally have different numerical components. However, in centrosymmetric crystal structures, types Ia and Ib are crystallographically equivalent, and types IIa and IIb are crystallographically equivalent (Christian and Mahajan 1995), since the point group of a centrosymmetric crystal class includes the inversion (see Table A.1 for specifics). In more complex crystal structures without a center of symmetry, the reflection and rotation operations listed in (8.5) all result in different configurations of the atomic structure, and hence four distinct transformation matrices need be considered (i.e., two for each type of twin). In a compound twin in a centrosymmetric crystal of the type shown in Fig. 8.1(c), all four definitions in (8.5) are crystallographically equivalent. Alternative (i.e., nonclassical) descriptions of twinning kinematics are also possible. For example, Bevis and Crocker (1968) developed a generalized mathematical treatment of twinned lattices that encompasses nonconventional or degenerate twinning modes not addressed by (8.5). Table 8.1 Representative twin systems in crystals (Christian and Mahajan 1995) Crystal BCC FCC HCP
K1
K2
{1 12} {11 1} {10 12} {1012} {112} {111}
η1 1 11
η2 111
112
112
10 1 1
101 1
S
{1 10} {1 10} {1210}
Shear γ j
Partial bP
1/ 2
1/ 6 1 11
1/ 2
1/ 6 112
c /a − 3 3 c/a
A 10 1 1 *
2
2
* A = [3 − (c/a) 2 ]/[3 + (c/a) 2 ]
Table 8.1 lists common twin systems in metallic crystals with cubic and hexagonal structures. The complete twinning elements {K1 , K 2 , η1 , η2 } , the plane of shear S, the magnitude of shear deformation γ j , and the partial Burgers vector b P of dislocations whose collective motion is thought to account for the twinning shear are all listed in Table 8.1. Shear γ j ≥ 0 is always nonnegative by definition. Hence, twinning does not occur on the same plane in opposite directions. Care must be taken to ensure the correct directional sense of twinning is prescribed; Table 8.2 lists individual planes and directions for families of twin systems in Table 8.1. An orthogonal transformation satisfies QT = Q −1 , with det Q = +1 for a proper transformation and det Q = −1 for an improper transformation. Since matrices in (8.5) are symmetric and orthogonal, Q = QT = Q −1 = Q −T . 2
390
8 Mechanical Twinning in Crystal Plasticity
All twinning elements are rational for the twin systems listed in Table 8.1; hence all describe compound twins. No atomic shuffles are required for monatomic BCC and FCC crystals undergoing those particular twinning modes listed in Table 8.1. The list of twin systems in Table 8.1 is far from comprehensive, as numerous other systems have been observed in various alloys, polyatomic lattices, and crystal structures of lower symmetry (Schmid and Boas 1950; Christian and Mahajan 1995). Table 8.1 can be compared with Table 3.4 that lists slip systems and full Burgers vectors for dislocation glide in cubic and hexagonal crystal structures. In hexagonal crystals (labeled HCP in Table 8.1, as in Table 3.4, though the c/a ratio may deviate from the ideal value of 1.633), the direction of shear η1 is reversed for ratios of lattice parameters c2 /a 2 3 , twinning occurs when a single crystal is compressed parallel to the caxis, while for c2 /a 2 0 and det F + > 0 . Let m 0 be a unit normal vector to Σ, pointing from the – side to the + side. The compatibility requirement that the interface be coherent (i.e., continuous coordinates x1 (Σ) = x 2 (Σ) along the surface of composition) necessitates that Hadamard’s jump conditions apply (James 1981; Bhattacharya 1991): F = F + − F − = a ⊗ m0 , F + = F − + γ j s ⊗ m0 , (8.9) where γ
is a scalar magnitude of the twinning deformation, s = a / γ j is ˆ in (8.9) is a proper orthogonal transformation differa unit vector, and Q ˆ ≠ 1 ). Treating F − and F + as elastic deing from the unit tensor3 (i.e., Q j
ˆ = 1 then F + = F − M for some matrix M ∈ H . In that case, the elasWhen Q tic response (e.g., the stress state) of the twin is indistinguishable from that of the parent when each are subjected to the same further deformation, and the twin is said to be a false twin (James 1981). True twins satisfy (8.9) and demonstrate dif3
8.1 Mechanisms: Elasticity, Slip, and Twinning
393
formations in strain energy density function (8.2) for illustrative purposes4, ˆ − H ) = ψ (F − ) , meaning that strain consider the conditions ψ (F + ) = ψ (QF energy densities in the twin and parent regions are presumed identical in this particular case. Hence, in addition to (8.9), it follows that ˆ − H , where H ∈ H is an energy invariant transformation, not necF + = QF essarily an orthogonal tensor (James 1981). Choosing a single global Cartesian coordinate system, and assuming that H does not induce volume changes (i.e., H is unimodular with det H = 1 , since the converse assertion would permit the strain energy of a sample of fixed mass to remain constant as the volume of the sample is increased without bound), the following identities apply5: ˆ − H ) = det F − = det(F − + a ⊗ m ) det F + = det(QF 0 (8.10) − − −1 j = det F det(1 + γ (F ) s ⊗ m 0 ) = det F − [1 + γ j s 0 , m 0 ].
Since det F − > 0 and γ j > 0 , it follows from (8.10) that the pull back of s must be orthogonal to unit normal m 0 in the reference configuration: (F − )−1 s , m 0 = s0 , m 0 = 0 , s0 = (F − ) −1 s .
(8.11)
When region 1 (parent) is taken as a perfect reference lattice with F = 1 , then s0 = s and s , m 0 = 0 . Since s ⊥ m 0 , F + = 1 + γ j s ⊗ m 0 is ˆ a simple shear. In that case, F + = QH is also a simple shear, possibly of −
large magnitude, that shifts the perfect crystal to another minimum energy configuration, with the strain energy density of this configuration equivalent to that of the (original) parent. The associated strain energy density function can be interpreted as a multiwell potential, with global minima ˆ ) = 0 . The preceding treatment corresponding to conditions ψ (1) = ψ (QH ferent responses, for example anisotropic elastic constants defined with respect to a global coordinate system will differ on either side of the twin boundary. 4 A twinned crystal remains elastic only when defect (i.e., dislocation) motion within the twin and surrounding material does not occur (Christian and Mahajan 1995). In many cases, elasticity theory may apply (Parry 1980; James 1981) to describe the reversible response of a crystal that has already twinned. In other cases, dislocation plasticity may render application of elasticity alone inappropriate. In the theory developed in Section 8.2, twin propagation itself is not regarded as an elastic deformation mechanism, but rather a thermodynamically irreversible process dictated by collective motion of partial dislocations and atomic shuffles. 5 Identities det A det B = det( AB ) and det(1 + a ⊗ b ) = 1 + aib for two matrices A and B and two vectors a and b are used. Recall also that matrix A is said to be unimodular when det A = ±1 .
394
8 Mechanical Twinning in Crystal Plasticity
does not account for any (surface) energy associated with defects along the boundary of the twin, which can be reflected in continuum theories via augmentation of the free energy function with internal state variables. Recall also that the preceding analysis restricts the boundary to be coherent, in contrast to more general treatments permitting discontinuous displacements across interfaces that may occur in some kinds of phase transformations or in solids with other kinds of defects (Cermelli and Gurtin 1994).
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes A constitutive framework for crystals undergoing large thermoelastic, plastic, and twinning deformations is developed in what follows. The treatment of Section 8.2 extends those of geometrically nonlinear crystal plasticity of Sections 3.2.6 and 6.3 to incorporate kinematics, mechanics, thermodynamics, and kinetics of twinning. Residual elastic volume changes discussed in Sections 7.2.47.2.7 are also incorporated in the model framework of Section 8.2, as are geometrically necessary dislocations and statistically stored dislocations of Section 3.3.2. Plastic deformation is limited to that resulting from dislocation glide, and twinning deformation is limited to mechanical twinning. 8.2.1 Kinematics
Deformation gradient F ( X , t ) for an element of crystalline material, as defined in (2.112), is decomposed multiplicatively into the following series of terms: (8.12) F = F E F I F W F P = F E F = F L Fˆ = F E F W F P , with the notation F L = F E J 1/ 3 , F = FWFP , Fˆ = F W F P , (8.13) I 1/ 3 W 1/ 3 W F = J 1, F =J F . Elastic deformation F E accounts for recoverable thermoelastic deformation, as discussed in Section 8.1.1, and also includes any rigid body rotation of the element. Spherical tensor F I accounts for residual elastic volume changes associated with defects. Specifically, such volume changes are addressed by the Jacobian determinant J , as discussed in Chapter 7. Plastic deformation F P accounts for latticepreserving slip resulting from dislocation glide, as discussed in Section 8.1.2. Contributions to the de
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
395
formation gradient from twinning shears are addressed by the term F W . (The W superscript is chosen to denote contributions from twinning rather than the T superscript, to avoid confusion with the transpose (2.125)). The total irreversible deformation is F . The total elastic lattice deformation (recoverable and residual) is denoted by F L = F E F I = F E J 1/ 3 , and the total deformation resulting from defect motion (i.e., both dislocation glide and twinning) is denoted by Fˆ = F W F P . Residual elastic deformation F I arising from distributed defects such as dislocation lines follows from the assertion that in continuum nonlinear elasticity, the average strain of a body containing residual stress fields arising from internal displacement discontinuities need not vanish even if traction on its external surfaces vanishes (Toupin and Rivlin 1960). Presently, only volume changes ( J ) are considered, e.g., corresponding to random defect distributions imparting no preferred directions in average residual elastic strains, though shape changes are not precluded in the general treatment of Section 7.2.3, specifically (7.31), (7.37), and (7.41). The relationship between J and defect densities is given later in Section 8.2.4, implementing earlier derivations of Section 7.2.4. In the present context, F P and F W account for isochoric (shape) deformations resulting from respective motions of slip dislocations and twinning partials, while J accounts for volume changes resulting from the residual stress fields of the defects themselves. In the model developed in the present Section, individual twins within the volume element of crystal are not modeled explicitly, nor are shapes and sizes of twinned regions. Rather, F W accounts for the sum of shears resulting from evolving volume fractions of the material occupying each twin system (Chin et al. 1969; Kalidindi 1998). In this sense, F W is a kind of average irreversible shape deformation acting over the volume element of crystal. Geometries of individual twin boundaries are likewise not represented, but the total twin boundary area density per unit volume is represented with an internal state variable. The resolution of twinning in Section 8.2 is thus comparable to that of slip in crystal plasticity of Section 6.3, wherein velocities of individual dislocations are not resolved explicitly, but the cumulative shearing on each slip system results in plastic deformation F P . Line densities of dislocations per unit volume are also represented by internal state variables. Introduced next are sets of contravariant and covariant vectors denoting directions and planes, respectively, for slip and twinning. When referred to the reference lattice prior to any reorientation by twinning, these are de
396
8 Mechanical Twinning in Crystal Plasticity
noted by {si0 , m i0 } for each slip system i, and {s0j , m 0j } for each twin system j. The total number of slip systems is denoted by n, and the total number of twin systems is denoted by w. Recall that for metallic crystals of high symmetry, typical slip systems are listed in Table 3.4, and typical twin systems are listed in Table 8.1, all in Miller index notation. Reference directions and plane normals are all of unit length, and each pair of contravariant shear direction and covariant plane normal is orthogonal: si0 , m 0i = 0, s0i = m 0i =1, (∀i =1,...n); (8.14) s0j , m 0j = 0, s0j = m 0j =1, (∀j = 1,...w).
During the course of twinning deformation, one or more parts (i.e., twins) of the volume element of crystal undergoes a rotation relative to the parent. In a volume fraction of the crystal undergoing twinning via mode j, slip directions and slip plane normals transform in the reference configuration according to the usual rules for contravariant and covariant vectors: (8.15) si0 j = Q j si0 , m i0 j = m i0 Q jT , (∀i =1,...n; ∀j =1,...w), where Q j is the reflection or rotation found from (8.5) corresponding to particular twin system j; e.g., if j is a type Ia twin, Q j = 1 − 2m 0j ⊗ m 0j , or if j is a type IIa twin, Q j = 2s 0j ⊗ s 0j − 1 . Notice from (8.15) that, within each twin volume, updated slip directions si0 j and slip plane normals mi0 j remain orthogonal and of unit length for each i, since from (8.14), si0 j , mi0 j = Q j si0 , mi0 Q jT = Q.jBA s0i B m0i C Q.jA−1C = s0i A m0i A = 0 .
(8.16)
For simplicity, successive twinning (including detwinning as a particular example) is not considered; the present theory can readily be extended to address such phenomena via addition of appropriate kinematics and kinetics. Hence, secondary twins that could form within already twinned regions, leading to reorientation of sets {s0j , m 0j } , are not represented here. Further reorientation of transformed directors in (8.15) is likewise prohibited once a twin is fully formed. Rotations (8.15) do not apply to the volume of crystal comprising the parent. Elastic twinning phenomena are also not addressed in the present theory. Plastic deformation F P and twinning deformation F W do not directly alter directions associated with slip and twinning. The former is latticepreserving, as discussed in Section 8.1.2, while the latter only affects lattice orientation indirectly via (8.15) and evolution of the twin volume frac
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
397
tion for each system j to be discussed later. However, thermoelastic deformation and residual elastic volume change do affect the directors6: si = F L si0 , mi = mi0 F L −1 ⎫⎪ ⎬ (∀i =1,...n ∈ parent); s0i = J 1/ 3si0 , m i0 = mi0 J −1/ 3 ⎪⎭ ⎫⎪ sij = F L si0 j , mij = m i0 j F L −1 (∀i =1,...n ∈ twins j =1,...w); i 1/ 3 i i i −1/ 3 ⎬ s0 j = J s0 j , m 0 j = m 0 j J ⎪⎭
(8.17)
s j = F L s 0j , m j = m 0j F L −1 ⎪⎫ ⎬ (∀j =1,...w ∈ parent). s0j = J 1/ 3s0j , m 0j = m 0j J −1/ 3 ⎪⎭ Figure 8.3 depicts the physics underlying (8.12)(8.17) for an element of crystal with a single slip system and a single twin. Multiplicative decomposition (8.12) implies a series of configurations of the material element. The reference configuration is labeled B0 with corresponding coordinates X, the spatial configuration is labeled B with corresponding coordinates x, and the elastically unloaded intermediate configuration is labeled B , as in Fig. 7.1 of Chapter 7. Since F E −1 and F are in general not integrable, continuous coordinates spanning anholonomic configuration B do not exist, following arguments in Sections 2.8 and 3.2.2. However, elastic and inelastic deformations act as tangent mappings between configurations via F E : TB → TB and F :TB0 → TB . In Fig. 8.3, mappings F W and F P constituting F cannot be separately resolved because of the implicit effect of twinning on the orientation of the reference lattice. Another intermediate configuration, not shown in Fig. 8.3, is labeled B , attained via the tangent mappings F L :TB → TB and Fˆ :TB0 → TB .
6 The effect of J on the slip director vectors and slip plane normal covectors was omitted in earlier work (Clayton 2009a).
398
8 Mechanical Twinning in Crystal Plasticity
Fig. 8.3 Deformations and slip system geometry for crystal element deforming by elasticity, slip, and twinning
The spatial velocity gradient of (2.176) is expanded via application of the product rule, (8.12), and (8.13) as L = FF −1 (8.18) = F E F E −1 + F E F W F W −1F E −1 + F E F W F P F P −1F W −1F E −1 + (1/ 3) JJ −11.
The inelastic velocity gradient referred to configuration B is FF −1 = F W F W −1 + F W F P F P −1F W −1 + (1/ 3) JJ −1 1 = LW + LP + (1/ 3) JJ −11,
(8.19)
where w
LW = F W F W −1 = ∑ f j γ j s0j ⊗ m 0j
(8.20)
j =1
twinning in parent crystal
results from twinning shears, and n w ⎛ LP = F W LP F W −1 = (1 − fT )∑ γ i s0i ⊗ m i0 + ∑ ⎜ f i =1 j =1 ⎝ slip in parent crystal
j
n
∑γ i =1
⎞ s ⊗ mi0 j ⎟ ⎠
i i j 0j
(8.21)
slip in twinned crystal
accounts for slip in the parent and in twinned regions. The usual plastic velocity gradient is written LP = F P F P −1 , as in (3.58). In (8.20), γ j > 0 is the predefined shear deformation associated with twin system j, a positive scalar that is fixed for all twins belonging to a given family of twin systems. Recall that magnitudes of γ j are listed in Table 8.1 for BCC, FCC,
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
399
and hexagonal crystal structures. In (8.21), γ i is the slip rate on system i in the parent, and γ ij is the slip rate on system i within reoriented twin fraction j. The volume fraction of crystal occupied by twin j, e.g., measured per unit volume in configuration B , is labeled by scalar f j ≥ 0 , with time rate f
j
(Chin et al. 1969; Van Houtte 1978). The total volume fracw
tion of twinned crystal is fT = Σ f j , subject to restriction 0 ≤ fT ≤ 1 . j =1
Since detwinning is not considered in the present theory, f j ≥ 0 . In the inner sum within the rightmost term of (8.21), slip directors and plane normals in twinned regions are obtained from (8.15), where the particular form of rotation or reflection Q j corresponds to twin with associated volume fraction f j in the outer sum. Because twinning is isochoric (see (8.22)), f j is also equivalent to the mass fraction of an element of material occupied by twin system j. Since for each slip or twin system, shear directions and plane normals are orthogonal, (8.22) J W = J W tr(LW ) = 0 ⇒ J W = 1 , J P tr(LP ) = 0 ⇒ J P = 1 , upon assuming that at t = 0 , F W = 1 and F P = 1 . Thus, (8.20)(8.22) properly reflect the isochoric nature of slip and twinning, and together with (8.12) and (8.13), require that all volume changes be accommodated thermoelastically via J E and/or by defect generation via J , such that J = g / G det F = g / G det F E det F = J E J = J L . (8.23) When J = 1 and f j = 0 for all j, then F W = 1 , F E = F L , F = F P , and LP = LP in (8.21) reduces to its usual definition from crystal plasticity theory, (3.120). In this situation, all inelastic deformation occurs via slip, F is latticepreserving, and slip directors and slip plane normals remain unchanged between configurations B0 and B . On the other hand, when twinning does takes place, F W does not act as a true elastic lattice deformation in the sense of (3.17), (8.1), and Born and Huang (1954). Rather, only that part of the lattice within the twinned volume undergoes a transformation, and this transformation occurs via improper rotation (8.15) and does not include any stretch of the lattice directors, even though shearing associated with F W involves both stretch and rotation. Extending (3.217)(3.222), defect content in the crystal is measured, in part, by the secondorder, twopoint geometrically necessary dislocation tensor α 0 ( X , t ) satisfying
400
8 Mechanical Twinning in Crystal Plasticity
Bα = − ∫ F L −1α.a dx a = − ∫ Fˆ. αA dX A = ∫ α 0α A N A dA , c
C
(8.24)
A
where Bα are components of a total Burgers vector associated with circuit c in the spatial frame or circuit C in the reference frame, A is the area enclosed by C with unit normal N A , ε ABC are components of permutation tensor (2.64), and (8.25) α 0α A = ε ABC Fˆ. Bα,C = ε ABC Fˆ.[αB ,C ] = ε ABC Fˆ.[αB ;C ] = ε ABC Fˆ.[αB:C ] . Stokes’s theorem of Section 2.7.2 is used to convert from the line integral to the area integral in the third equality of (8.24). Then from (8.12), (8.13), and the product rule, (8.26) α 0α A = ε ABC Fˆ. Bα,C = ε ABC F W α. β F P.βB ,C + ε ABC F W α.β ,C F P.βB . slip gradients
twin gradients
Contributions of plastic slip gradients to the geometrically necessary dislocation density tensor, corresponding to the first term following the second equality in (8.26), are well documented in the continuum theory of dislocations (Ashby 1970; Teodosiu 1970; Fleck et al. 1994; Arsenlis and Parks 1999; Voyiadjis and Abu AlRub 2005, 2007; Rezvanian et al. 2007), as discussed at length in Section 3.3.2. The second term in the sum on the right in (8.26) arises from gradients of twinning deformation, for example gradients of twin volume fractions arising during propagation of tapered twins (Scott and Orr 1983; Christian and Mahajan 1995); the contribution to the dislocation density tensor in this context would be partial dislocations at interfaces between the twin and parent or at interfaces between intersecting twins (Kosevich and Boiko 1971). Applying Nanson’s formula (2.227) to (8.24): Bα = ∫ α 0α A N A dA = ∫ α 0α A ( Jˆ −1 Fˆ. Aβ nβ ) da = ∫ αˆ αβ nβ da , (8.27) A
a
a
a geometrically necessary dislocation tensor referred to intermediate configuration B , labeled αˆ , is found as αˆ αβ = Jˆ −1 Fˆ. Aβ α 0α A = J L F L −1.βaε abc F Lα.[b ,c ] (8.28) = V −1 ∫ b α ξ β dL = ∑ ρ k b kα ξ k β , k
where Jˆ = J W J P = 1 by (8.22), and the second equality in (8.28) follows from (3.225). The integral following the third equality in (8.28) is carried out over all dislocation lines of length L, local Burgers vector b , and orientation ξ in intermediate volume element V . Finally, the final sum on the right of (8.28) is the discrete form of this integral similar to (3.226), where ρ k is the length per unit intermediate volume of dislocation seg
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
401
ments with unit tangent line vector ξ k and Burgers vector b k . In (8.24)(8.28), sufficient smoothness (i.e., differentiability) of F L , F W , and F P has been assumed. Discontinuities in the deformation gradient of the lattice at the microscale, for example singularities across slipped regions as in (3.85) and jumps in microscopic deformation gradient across twin boundaries as discussed in Section 8.1.3 are not resolved explicitly in the present continuum framework that addresses defects via continuous distributions. Two nondimensional internal state variables are introduced to represent energetic changes associated with other kinds of defects in the crystal. The first internal state variable is a measure of the density of statistically stored dislocations (see (3.238)(3.240)) that accumulate with homogeneous slip, α = b ρS , (8.29) where b is a scalar magnitude of the Burgers vector—or a constant on the order of a lattice parameter when the crystal exhibits slip on systems with different Burgers vectors—and ρ S ( X , t ) is the length of such dislocations per unit volume in configuration B . Statistically stored dislocations include closed loops and dipoles that do not contribute to the total Burgers vector Bα in (8.24). The second internal state variable measures the total density of twin boundaries, β = bηW , (8.30) with ηW ( X , t ) the area of twin boundaries measured per unit volume in configuration B . 8.2.2 Constitutive Assumptions
Let ρ ( x, t ) and ρ 0 ( X ) denote the mass density of the solid in current and reference configurations, respectively, related by ρ0 = ρ J as in (4.10), recalling from (8.23) that J = J L in the present context. Let ρ = ρ J E = ρ 0 J −1
(8.31)
denote the mass density in configuration B . The forthcoming thermodynamic analysis is conducted in B , the intermediate configuration that serves as an evolving reference configuration for the instantaneous thermoelastic response of the crystal, analogous to the role of configuration B in the thermodynamic treatment of finite elastoplasticity in Section 6.1. Because F L = J 1/ 3F E , configurations B and B differ by the residual elastic volume change J . When explicit delineation of residual elasticity is
402
8 Mechanical Twinning in Crystal Plasticity
omitted, then F L = F E and configurations B of Chapter 6 and B of Chapter 8 coincide. The Helmholtz free energy per unit volume in configuration B is written as Ψ = ρψ = J −1Ψ 0 = J EΨ , (8.32) where ψ is the free energy per unit mass. The free energy is assumed to exhibit the dependencies Ψ =Ψ ( EE ,θ , αˆ ,α , β ,{ f j }, X , gα ) , (8.33) where θ ( X , t ) is the absolute temperature and gα ( X ) are coordinate basis vectors on configuration B . Variables αˆ , α , and β are respectively related to densities of geometrically necessary dislocations, statistically stored dislocations, and twin boundaries, as discussed in Section 8.2.1. The set { f j } includes each of the twin fractions j = 1, 2,...w , and 1 E 1 E Eαβ = (Cαβ − gαβ ) = ( F E .aα g ab F E .bβ − gαβ ) (8.34) 2 2 is a finite elastic strain tensor associated with the covariant elastic deformation tensor CE . Components of the metric tensor in anholonomic configuration B are denoted by gαβ = gα i g β , and are assumed stationary with respect to time. In agreement with physical arguments of Sections 8.1.2 and 8.1.3, the free energy does not depend explicitly on plastic deformation gradient F P or the contribution from twinning shear F W . Notice that each of the independent state variables entering the function (8.33) is invariant with respect to rigid body motions of the spatial coordinate frame. In particular, the scalars are always invariant and tensors EE and αˆ have all indicial components referred to intermediate configurations B and B , respectively. Dependence of free energy on elastic strain EE accounts for energy storage in stretched or misaligned atomic bonds, in association with mechanical stresses. The free energy depends on temperature for the same reasons discussed in Chapters 5 and 6, e.g., to account for specific heat capacity and thermal expansion, among other phenomena. A dependence on αˆ , α , and β accounts for line, surface, and/or interaction energies of dislocations and twin boundaries. The rationale for inclusion of { f j } in the list of state variables will become clear in Section 8.2.4, wherein effective elastic coefficients of the volume element depend explicitly on volume fractions of twins, with each twin exhibiting its own local anisotropic elastic coefficients. Dependence on X accounts for possibly heterogeneous
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
403
material properties, while gα are included to reflect anisotropy, e.g., elastic constants of the parent dependent upon orientation of the sample of material with respect to a global coordinate system. Analogous functional forms to (8.33) can be written for entropy, stress, and time rates of internal state variables. An expression for the heat flux can also be written, incorporating dependence of temperature gradient. Dependence of the Helmholtz free energy on the temperature gradient has been omitted a priori in (8.33), but such dependence could be included and then eliminated by exercising thermodynamic arguments, as was done in Sections 5.1.2 and 6.1.2. 8.2.3 Thermodynamics
Local forms of the balance of energy and dissipation inequality, each referred to the reference configuration, are given respectively by (4.39) and (4.71), repeated below: G 1 G ρ 0 e = Σ : E − ∇, Q + ρ0 r , Σ : E − ρ0 (ψ + ηθ ) − ∇ θ , Q ≥ 0 . (8.35)
θ
Recall that e = ψ + θη is the internal energy per unit mass, with η the entropy per unit mass. The symmetric second PiolaKirchhoff stress Σ is related to the first PiolaKirchhoff stress P and the symmetric Cauchy stress σ by equalities listed in Table 4.1: (8.36) Σ AB = F −1.Aa P aB = JF −1.Aaσ ab F −1.Bb . The symmetric tensor E = (1/ 2)(FT F − G ) is the right CauchyGreen strain of (2.156), Q is the heat flux vector referred to the reference configuration B0 , and scalar r denotes other heat sources of energy per unit mass. The stress power per unit intermediate volume in configuration B can be written, similarly to (6.15), as J −1Σ AB E AB = J Eσ ab Lab = ( J E F E −1.βbσ a.b F E .aα )( F E −1α.e Le.d F E .dβ ) (8.37) = M α.β L.αβ , where a version of Mandel’s stress (Mandel 1974) and symmetric elastic second PiolaKirchhoff stress are, respectively, M = CE Σ , Σ = J E F E −1σF E −T , (8.38) or in indicial notation, E M α.β = J E F E .aα σ a.b F E −1.βb = Cαδ Σ δβ , Σ αβ = J E F E −1α.aσ ab F E −1.βb . (8.39) The total velocity gradient of (8.18) pulled back to configuration B is
404
8 Mechanical Twinning in Crystal Plasticity
1 (8.40) J1. 3J The time rate of free energy change per unit intermediate configuration volume is, similarly to (6.19), d Ψ = ( ρψ ) = J −1 ρ 0 (ψ − F. αA F .−α1 Aψ ) dt (8.41) L = F E −1LF E = F E −1F E + LW + LP +
= ρψ −Ψ ( JJ −1 + J W J W −1 + LP.αα ) = ρψ −Ψ JJ −1 , where (8.22), (8.31), and (8.32) have been used. Following from (8.37), (8.40), and the symmetry of Σ and EE , 1 (8.42) M α.β L.αβ = Σ βδ EδβE + M α.β LW α.β + M α.β LP.βα + JM α.α . 3J Expanding the rate of free energy Ψ of (8.33) using the chain rule (Coleman and Noll 1963; Coleman and Gurtin 1967), ∂Ψ ∂Ψ ∂Ψ ∂Ψ ∂Ψ ∂Ψ Ψ = E : EE + θ+ : αˆ + α+ β + j f j , (8.43) ∂E ∂θ ∂αˆ ∂α ∂β ∂f with summation implied over w twin fractions j, the entropy inequality in (8.35) can be written ⎛ W ⎛ J ⎞ ∂Ψ ⎞ E ⎛ ∂Ψ ⎞ P 1⎟ ⎜Σ − E ⎟:E −⎜ N + ⎟θ + Π : ⎜⎜ L + L + ∂E ⎠ ∂θ ⎠ 3J ⎟⎠ ⎝ ⎝ ⎝ (8.44) ∂Ψ ∂Ψ ∂Ψ ∂Ψ j 1 α− β − j f − ∇θ , q ≥ 0. − : αˆ − θ ∂αˆ ∂α ∂β ∂f
As introduced in (8.44), N = ρη is the entropy per unit intermediate volume, ∇α θ = θ , A F .−α1 A = θ ,a F E .aα is an anholonomic intermediate temperature gradient similar to (6.6), q = J −1FQ = J E F E −1q is the intermediate heat flux similar to (6.7), and Π = M −Ψ 1 (8.45) is a (negative) version of Eshelby’s elastic energymomentum tensor (see Section 6.6) pushed forward to configuration B , similar to (6.33). Following arguments akin to those used in Sections 5.1.2 and 6.1.2, admissible stresselastic strain and entropytemperature relations are deduced as ∂Ψ ∂Ψ ∂Ψ E b 1 ∂Ψ F .β , η = − . (8.46) Σ αβ = E , N = − , σ ab = J E −1 F E .aα E ∂Eαβ ∂θ ∂Eαβ ρ ∂θ Angular momentum balance (4.26) is satisfied consistently: σ ab = σ ba . The final term on the left of (8.44) always contributes positively to dissipation upon prescription of a conduction law similar to (6.30):
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
q = −K∇θ , − ∇θ , q = ∇θ , K∇θ ≥ 0 ,
405
(8.47)
where K ( X , t ) is a symmetric and positive semidefinite matrix of thermal conductivity. Applying (8.46) and (8.47),
Π : LW + Π : LP + (1/ 3) JJ −1tr(Π) (8.48) ∂Ψ ∂Ψ ∂Ψ ∂Ψ 1 : αˆ + α+ β + j f j − ∇θ , K∇ θ ∂αˆ ∂α ∂β ∂f θ is the reduced dissipation inequality. In the absence of temperature gradients (e.g., an adiabatic process), (8.48) requires that the energy dissipated by twinning, slip, and residual volume changes must exceed the rate of energy storage associated with defects, specifically geometrically necessary and statistically stored dislocations, twin boundaries, and twin fractions. From (8.17)(8.22) and (8.39), dissipated energies from slip and twinning, respectively, can be written n w n w ⎛ ⎞ Π : LP = (1 − fT )∑τ i γ i + ∑ ⎜ f j ∑τ jiγ ij ⎟ , Π : LW = ∑τ j f j γ j , (8.49) j =1 i =1 j =1 ⎝ i =1 ⎠ where the driving forces are resolved stresses on each twin (habit) plane or slip plane, acting in the direction of shear: τ i = s0iα Πα.β m i0 β = J E s i aσ a.b mi b , (slip in parent); ≥
τ ji = s0i jα Πα.β m i0 j β = J E s ij aσ a.b mijb , (slip in twins);
(8.50)
τ j = s0jα Πα.β m 0j β = J E s j aσ a.b m j b , (twinning); since twinning and slip are isochoric. Resolved shear stress τ i is related to τ i of crystal plasticity theory introduced in (6.85)(6.86) by τ i = J τ i . The specific heat capacity at constant elastic strain and internal state variables, measured per unit volume in configuration B , is introduced as ∂E ∂ 2Ψ . (8.51) C( X ,t) = = −θ ∂θ EE ,αˆ ,α , β ,{ f j } ∂θ 2 where (8.46) has been used and E = ρ e is the internal energy per intermediate volume. Multiplying the first of (8.35) by J −1 , and following a procedure analogous to that of (6.36)(6.43), the energy balance can be written in the relaxed intermediate configuration B as7
The factor of 3 preceding the term θ (∂Ψ /∂θ ) = −θ N in (8.52) was incorrectly omitted in (3.29) and (3.43) of a previous article (Clayton 2009a). This misprint is corrected in (8.52) of the present text. 7
406
8 Mechanical Twinning in Crystal Plasticity
Cθ
Π : ( LW + LP )
=
temperature change
dissipation from slip and twinning
⎛ ∂Ψ ⎞ J + ⎜ tr(Π ) + 3θ ⎟ ∂θ ⎠ 3 J ⎝ dissipation from defect generation
⎛ ∂Ψ ∂ 2Ψ ⎞ − θ β : EE − ⎜ −θ ⎟ : αˆ ∂θ αˆ ⎠ ⎝ ∂αˆ thermoelastic coupling
strain energy of geometrically necessary dislocations
⎛ ∂Ψ ⎛ ∂Ψ ∂ 2Ψ ⎞ ∂ 2Ψ ⎞ −⎜ −θ −θ ⎟α − ⎜ ⎟β ∂θ∂α ⎠ ∂θ∂β ⎠ ⎝ ∂α ⎝ ∂β strain energy of statistically stored dislocations
⎛ ∂Ψ ∂ 2Ψ ⎞ −⎜ j −θ ⎟f ∂θ∂f j ⎠ ⎝ ∂f
(8.52)
surface energy of twin boundaries
ˆ , K∇ θ + ρ r . + ∇
j
energy of lattice reorientation from twinning
heat conduction
heat supply
Stresstemperature coefficients in (8.52) are defined according to
β αβ = −
∂ 2Ψ E ∂θ∂Eαβ
(8.53) j
αˆ ,α , β ,{ f }
and the anholonomic covariant derivative in (8.52) is performed similarly to that of (6.38) and (6.39): ˆ (. ) = ∇ (. ) + J −1 (. ) F β ∇ ( JF −1 A ) ∇ .A .α α α β (8.54) −1 A −1 −1 A = (. ): A F .α + J (. )( JF .α ): A . ˆ = ∇ when compatibility conditions F α = 0 apply, in Notice that ∇ α
.[ A:B ]
α
which case Piola’s identity (2.146) gives ( JF
) = (∂J / ∂F. αA ): A = 0 .
−1 A .α :A
8.2.4 Representative Free Energy
A particular form of (8.33) is now introduced for anisotropic single crystals that may undergo large elastic deformations, temperature changes, twinning, and dislocation accumulation. The free energy is decomposed additively as Ψ =Ψ E ( EE ,θ ,{ f j }, X , gα ) +Ψ R ( αˆ , α , β ,θ , X , gα ) , (8.55) where, as in (6.48), Ψ E accounts for the thermoelastic response and Ψ R accounts for residual free energy of lattice defects. As in Section 6.1.3, effects of defect densities besides twin volume fractions on the thermoelastic
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
407
energy are neglected, implying that the thermoelastic coefficients do not depend explicitly on dislocation density or twin boundary area. The thermoelastic energy is expanded in a Taylor series about a referE ence state characterized by Eαβ = 0 and ∆θ = θ − θ 0 , and here consists of four terms, similarly to (6.49): 1 αβχδ E E 1 ΨE= Eαβ Eχδ + 2 6
αβχδεφ
E − β αβ Eαβ ∆θ − Cθ ln
E E Eαβ Eχδ EεφE
(8.56)
θ . θ0
The first term on the right side of (8.56) accounts for materially linear, but geometrically nonlinear, mechanical effects. The second accounts for materially nonlinear elastic effects important at high pressures, and the third accounts for thermoelastic coupling. Constant θ 0 is a positive temperature at which the lattice parameters exhibit their reference values in a defectfree crystal, and the remaining coefficients in (8.56) consist of partial derivatives of the thermoelastic part of the free energy per unit intermediate volume at null elastic strain and at the reference temperature: αβχδ
=
∂ 2Ψ E E E ∂Eαβ ∂Eχδ
β αβ = −
αβχδεφ
,
=
EE = 0 θ =θ0
∂ 2Ψ E E ∂θ∂Eαβ
∂ 3Ψ E E E ∂Eαβ ∂Eχδ ∂EεφE
,
(8.57)
EE = 0 θ =θ0
⎛ ∂ 2Ψ E ⎞ , C = − ⎜θ . 2 ⎟ ⎝ ∂θ ⎠ EE = 0 EE = 0
(8.58)
θ =θ0
θ =θ0
(αβ )( χδ )
The usual symmetry relations = , = ( )( )( ) , and β αβ = β (αβ ) follow automatically from (8.57) and (8.58). Thermoelastic constants and specific heat constant in (8.58) are particular values of coefficients introduced already in (8.53) and (8.51), respectively. Similarly to (6.52)(6.55), coefficients in (8.57) and (8.58) are related to those of nonlinear elasticity theory introduced in (5.66) and (5.85) at the same material point X as αβχδ = J −1 ABCD g.αA g.βB g.χC g.δD , (8.59) αβχδ
αβχδεφ
= J −1
ABCDEF
αβ
=J β
β
−1
g.αA g.βB g.χC g.δD g.εE g.φF , AB
α
β
g. A g. B ,
C = ρ c = J ρ 0 c = J C0 . −1
αβχδεφ
−1
αβ χδ εφ
(8.60) (8.61) (8.62)
Since gα = 0 and G A = 0 (e.g., see discussion in Section 2.5.1), the shifter g.αA = g α , G A at X does not depend on time. When residual elastic vol
408
8 Mechanical Twinning in Crystal Plasticity
ume changes vanish ( J = 1 ) and when coincident coordinate systems are used in reference and intermediate configurations so that g.αA = δ .αA , numerical values of material coefficients on left and right sides of each of (8.59)(8.62) are equal. When J ( X , t ) ≠ 0 , then coefficients on both sides of (8.59)(8.62) cannot all be constant for all t > 0 . If the left sides are taken as constant in time, then the elastic coefficients and specific heat per unit reference volume on the right sides increase with increases in residual volume change. In that case, if the elastic strain is held fixed, an increase in residual elastic volume would have no effect on the measured Cauchy stress σ ( x, t ) or on the intermediate symmetric stress Σ as will be clear in (8.65) and (8.69), but would affect the stresses Σ( X , t ) and P ( X , t ) referred to the reference configuration, the latter evident from (8.70). Since J resulting from dislocations is expected to be very close to unity for most situations, i.e., J − 1 < 10−3 for dislocation densities < 1015 m −2 as explained in Section 7.2.7, differences among definitions of material coefficients listed in (8.59)(8.62) will be trivial in such cases, i.e., less than ~0.1% error, and presumably will be much smaller than uncertainties in experimental measurements of such constants. Possible influences of the dislocation densities (αˆ and α ) and twin boundaries ( β ) on the effective elastic moduli that may emerge in crystals at large defect densities (Smith 1953; Clayton and Chung 2006; Chung and Clayton 2007) are precluded by (8.55) since couplings between elastic strain EE and defects (αˆ ,α , β ) are not included. Such effects could be incorporated by generalization of (8.55) if deemed relevant for applications of interest (Clayton et al. 2004a, b), as demonstrated in Section 9.4.6 of Chapter 9. The present assumption that elastic strain and defect densities are decoupled in the free energy would become suspect at large defect densities wherein the residual volume change J could have a noticeable effect on elastic and thermal coefficients measured per unit reference volume, i.e., the right sides of (8.59)(8.62). In anisotropic solids, tensorvalued coefficients in (8.56) depend upon the orientation of the lattice in configuration B , via dependence of these coefficients on { f j } and gα . When twinning takes place, orientations of the original Bravais lattice (parent) and each twinned region differ. A straightforward averaging method is used to define the effective material coefficients for a volume element consisting of the parent and one or more twins. It is assumed that elastic deformation F E and elastic strain EE act uniformly over the parent and twins comprising this volume element. The
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
409
thermoelastic free energy density of (8.55) is thus partitioned into contributions from the parent and each twin: 1 1 E αβχδ E E αβχδεφ E Ψ E = (1 − fT ) Eαβ Eχδ + (1 − fT ) Eαβ Eχδ EεφE 0 0 2 6 E (8.63) − (1 − fT ) β 0αβ Eαβ ∆θ w ⎛ 1 E αβχδ E 1 E αβχδεφ E E ⎞ E + ∑ f j ⎜ Eαβ ∆θ ⎟ , Eχδ + Eαβ j Eχδ Eεφ − β jαβ Eαβ j 2 6 ⎝ ⎠ j =1 αβχδεφ αβ where αβχδ , , and β refer to material constants corresponding 0 0 0 to the orientation of the parent lattice relative to the external coordinate system, and where for each twin j (Van Houtte 1978; Kalidindi 1998) the elastic coefficients are mapped from original to twinned orientation via αβχδ = Q.εjα Q.φj β Q.ϕj χ Q.γj δ εφϕγ , β αβ = Q.jχα Q.δj β β 0χδ , 0 j j (8.64) αβχδεφ = Q.ϕj α Q.γj β Q.ηj χ Q.ιj δ Q.κj ε Q.jλφ ϕγηικλ . 0 j
Components of Q in (8.64) are related to those used in (8.16) by the shifter: Q.jβα = Q.jBA g.αA g.Bβ . Since transformation matrix Q always occurs in pairs in even rank coefficients of (8.64), the choice of reflection or rotation in (8.5) is irrelevant; i.e., Q and −Q will give the same updated coefficients in (8.64). The coefficients will differ, however, when computed for a type I versus type II twin, unless of course the twin is compound. The same considerations regarding symmetry of reference material coefficients discussed in Section 5.1.5 and Appendix A hold for referential thermoelas, αβχδεφ , and β 0αβ . To convert symmetry relations in tic constants αβχδ 0 0 Section 5.1.5 and Appendix A to the present context, reference indices in capital Roman font are replaced with intermediate indices in Greek font. Stressstraintemperature relations following from (8.46), (8.55), (8.56), and (8.63) are 1 αβχδεφ E E Σ αβ = αβχδ EχδE + Eχδ Eεφ − β αβ ∆θ 2 1 E E = (1 − fT ) αβχδ Eχδ + (1 − fT ) αβχδεφ Eχδ EεφE − (1 − fT ) β 0αβ ∆θ (8.65) 0 0 2 w 1 αβχδεφ E E ⎛ ⎞ E + ∑ f j ⎜ αβχδ Eχδ + Eχδ Eεφ − β αβ j j j ∆θ ⎟, 2 ⎝ ⎠ j =1 implying that the elastic stress Σ for a heterogeneous (twinned) crystal is equivalent to the volume average of the local stresses supported by the parent and each twin. Effective thermoelastic coefficients for the volume element entering (8.56), (8.63), and (8.65) are thus
410
8 Mechanical Twinning in Crystal Plasticity αβχδ
({ f
αβχδεφ
j
({ f
}, X , gα ) = (1 − fT ) j
}, X , gα ) = (1 − fT )
αβχδ 0
w
+∑ f
j
j =1
αβχδεφ 0
w
+∑ f j =1
αβχδ j
j
,
αβχδεφ j
,
(8.66)
w
β αβ ({ f j }, X , gα ) = (1 − fT ) β0αβ + ∑ f j β jαβ . j =1
Coefficients in (8.66) can be interpreted as Voigt averages (see generic definition (A.33) of Appendix A) and hence provide upper bounds on the elastic stiffness (Hill 1952; Mura 1982). From (8.63), the necessity of inclusion of twin fractions { f j } in free energy function (8.33) is evident, since the effective thermoelastic moduli (8.66) depend on evolving twin fractions. In the absence of twinning, (8.66) reduces to the coefficients of the parent crystal. The symmetry exhibited by coefficients on the left of (8.66) is minimally triclinic; the averaging process used to compute effective coefficients generally does not preserve the symmetry properties of the parent and each individual twin. Anisotropic thermal conductivity of (8.47) for a twinned element of material can be defined in the same way as the thermal stress coefficients in the last of (8.66). The associated time rate of thermoelastic free energy change from the rates of twin fractions is ∂Ψ E j f = A j f j , (summed over j = 1, 2,...w) , (8.67) ∂f j where for each twin system, the quantity 1 E αβχδ 1 E αβχδεφ E E ( j − αβχδ ) Eχδ ( j ) Eχδ A j = Eαβ + Eαβ − αβχδεφ EεφE 0 0 2 6 (8.68) E αβ ) . − ( β αβ − E ∆ β θ j 0 αβ From (8.65), the Cauchy stress and first PiolaKirchhoff stress are, respectively, 1 αβχδεφ E E ⎛ ⎞ (8.69) σ ab = J E −1 F E .aα F Eb.β ⎜ αβχδ EχδE + Eχδ Eεφ − β αβ ∆θ ⎟ , 2 ⎝ ⎠ 1 αβχδεφ E E ⎛ ⎞ E P aA = J 2 / 3 F P −1.Aγ F W −1.γβ F E .aα ⎜ αβχδ Eχδ Eχδ Eεφ − β αβ ∆θ ⎟ . (8.70) + 2 ⎝ ⎠ As noted previously, if the residual volume change measured by J is increased (decreased) at fixed elastic strain and temperature, the Cauchy stress of (8.69) remains fixed but the first PiolaKirchhoff stress of (8.70) will increase (decrease).
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
411
E Consider a situation in which strains Eαβ = ααβ ∆θ arise from tempera
ture change. The following relationship emerges between thermal stress, thermal expansion ( ααβ ), and elasticity coefficients:
β αβ = (
αβχδ
α χδ +
αβχδεφ
α χδ α εφ ∆θ / 2 )
θ0
=
αβχδ
α χδ
θ0
.
(8.71)
Relationship (8.71) is analogous to (5.161) of nonlinear thermoelasticity theory and (6.57) in the context of finite plasticity theory. The residual Helmholtz free energy per unit intermediate volume of (8.55) is specified as the following polynomial form: 1 Ψ R = Kˆ ⎡⎣κ1α 2 + κ 2 β 2 + κ 3l 2 N (αˆ : αˆ ) N + κ 4α 2 β 2 2 (8.72) 2N N 2 2N N 2 + κ 5l (αˆ : αˆ ) α + κ 6l (αˆ : αˆ ) β ⎤⎦ .
Energy factor Kˆ (θ , X , gα ) depends on anisotropic elastic constants, temperature, and orientation of the crystal relative to orientations of defects contained within. For straight dislocation lines whose energies are characterized via anisotropic linear elasticity solutions, Kˆ is defined in terms of secondorder elastic constants in Appendix C, Section C.1.6. In an isotropic linear elastic body, Kˆ (θ , X ) = µ (θ , X ) , i.e., the elastic shear modulus that may depend on temperature. Denoted by κ1 , κ 2 , κ 3 , κ 4 , κ 5 , and κ 6 are dimensionless constants that scale energies in each internal variable and their pairwise products. Also, l is a nonnegative scalar with dimensions of length, required from dimensional considerations in gradient theories (Fleck et al. 1994; Regueiro et al. 2002; Clayton et al. 2004a, b; Voyiadjis and Abu AlRub 2005), and N is a constant. From (8.72), Ψ R = 0 when all defect densities vanish; this state of vanishing defects is always of minimum residual free energy when all coefficients κ1 , κ 2 , κ 3 , κ 4 , κ 5 , and κ 6 are nonnegative. Recalling from definition (8.29) that α = b ρ S , the first term on the right of (8.72) provides for a linear dependence of residual energy on the line density of statistically stored dislocations, following Regueiro et al. (2002) and Clayton et al. (2004b, 2006) and references therein. Assuming that energy per unit line length of statistically stored dislocations can be represented by linear elastic solutions (C.152) or (6.117), simple arguments then show that, similarly to (6.118) and (6.119),
κ1 ˆ 2 κ1 ˆ 2 ˆ 2 ρ , 0.5 < Λ < 1.0, 1.0 < κ < 2.0 , Kα = Kb ρ S = Λ Kb 1 S 2
2
(8.73)
412
8 Mechanical Twinning in Crystal Plasticity
where self and interaction energies, core energy, and stacking fault energy if the dislocations are partial are absorbed into the constant κ1 . Recalling from (8.30) that β = bηW , the second term in (8.72) provides for a linear dependence of residual energy on the area per unit volume of twin boundaries ηW . Thus, letting WW represent the twin boundary energy per unit area in configuration B , W W κ2 ˆ 2 κ2 K β = µ bηW = WWηW ≈ SF ηW , κ 2 ≈ SF . µb 2 2 2
(8.74)
where the approximation that holds for many crystals, 2WW ≈ WSF , has been used, with WSF the intrinsic or extrinsic stacking fault energy (Hirth and Lothe 1982; Bernstein and Tadmor 2004). Energy factor Kˆ is set equal to the shear modulus in (8.74). The third term in (8.72) accounts for the energy of geometrically necessary dislocations, for which a number of forms for l, N, and κ 3 have been suggested for different crystal structures and different applications (Fleck et al. 1994; Regueiro et al. 2002; Clayton et al. 2004a, b; Voyiadjis and Abu AlRub 2005; Chung and Clayton 2007). The fifth term in (8.72) reflects possible interactions between statistically stored and geometrically necessary dislocations. The fourth and sixth terms in (8.72) reflect interaction energies between twin boundaries and dislocations, for example stress fields and strain energies of dislocation lines may be amplified at the stress concentration caused by a dislocation pileup at a twin boundary (Christian and Mahajan 1995). Methods for determining the content of geometrically necessary versus statistically stored dislocations have been forwarded in recent years (Arsenlis and Parks 1999; ElDasher et al. 2003; Hughes et al. 2003). Such methods could facilitate unique selection of parameters in (8.72) if defect energies are known, for example, through measurements cold work (Clarebrough et al. 1957; Rosakis et al. 2000; Taheri et al. 2006) or atomic scale computer simulations of defect energy. However, in many cases, only the total scalar line density ρT of all dislocations, both geometrically necessary and statistically stored, may be known from historical data. In such cases, it becomes prudent to employ a simple form of (8.72) in terms of total line density per unit intermediate volume in configuration B , denoted by ρT ( X , t ) : 1 Ψ R = µ ⎡⎣κ1α 2 + κ 2 β 2 + κ 4α 2 β 2 ⎤⎦ , (8.75) 2
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
413
where Kˆ (θ , X ) = µ (θ , X ) has been used as an approximation, and where the dimensionless internal state variable α ( X , t ) measures the total scalar dislocation density: α = b ρT . (8.76) Internal state variable in (8.76) is analogous to that defined in (6.100). Comparison of (8.72) and (8.75) implies the following relationships: κ1α 2 = κ1b 2 ρT = κ1b 2 ρ S + κ 3l 2 N (αˆ : αˆ ) N ; (8.77)
κ 4α 2 β 2 = κ 4b 2 ρT β 2 = ⎡⎣κ 4b 2 ρ S + κ 6 l 2 N (αˆ : αˆ ) N ⎤⎦ β 2 ; ρT = ρ S + ρG , ρG = b −1 (αˆ : αˆ )1/ 2 ; l = b , N = 1/ 2 , κ1 = κ 3 , κ 4 = κ 6 , κ 5 = 0 .
(8.78)
(8.79) (8.80) Relations (8.75)(8.80) provide for an equal contribution, per unit line length, of geometrically necessary and statistically stored dislocations to the residual free energy of the crystal. For uniform straight dislocation lines of density αˆ αβ = ρ b α ξ β in configuration B , (8.28) and the second of (8.79) consistently give (8.81) ρG = b −1 ( ρ k b α ξ β ρ k bα ξ β )1/ 2 = ρ k (b / b) = ρ k J −1/ 3 ≈ ρ k . Values of κ1 and κ 2 in (8.75) can be approximated using (8.73) and (8.74), respectively. Since the total dislocation density depends on geometrically necessary and statistically stored dislocations, i.e., α = α (αˆ ,α ) from (8.76) and (8.79), terms entering (8.52) can be expressed as follows via the chain rule: ⎛ ∂Ψ ⎛ ∂Ψ ∂ 2Ψ ⎞ ∂ 2Ψ ⎞ ⎛ ∂α ∂α ⎞ : αˆ + −θ −θ α⎟ ⎜ ⎟α = ⎜ ⎟⎜ ˆ α ∂ ∂ ∂ ∂ ∂ ∂ ∂ ∂α ⎠ α θ α α θ α ⎝ ⎠ ⎝ ⎠⎝ (8.82) ⎛ ∂Ψ ⎛ ∂Ψ ∂ 2Ψ ⎞ ∂ 2Ψ ⎞ =⎜ −θ −θ ⎟ : αˆ + ⎜ ⎟α . ∂θ∂αˆ ⎠ ∂θ∂α ⎠ ⎝ ∂αˆ ⎝ ∂α Using (8.67), (8.75), and (8.82), the rate of temperature increase in (8.52) can then be written in this case as ⎛ ∂Ψ J ⎞ − β : EE ⎟ + ∇ˆ , K∇θ + ρ r , Cθ = β ′W P + θ ⎜ (8.83) ⎜ ∂θ J ⎟ ⎝ ⎠ where
414
8 Mechanical Twinning in Crystal Plasticity
⎧⎪⎛ ∂Ψ ⎛ ∂Ψ ∂ 2Ψ ⎞ ∂ 2Ψ α θ −θ − − ⎟ ⎜ ∂θ∂α ⎠ ∂θ∂β ⎝ ∂β ⎩⎪⎝ ∂α
β ′ = 1 − ⎨⎜
⎛ ∂Ψ ∂ 2Ψ ⎞ j ⎫⎪ P −1 −⎜ j −θ ⎟ f ⎬W ∂θ∂f j ⎠ ⎪⎭ ⎝ ∂f ⎧⎪⎛ ηW ∂µ ⎞ ⎡ b 2 ⎛ = 1 − ⎨⎜ µ − θ ⎟ ⎢ ⎜⎜ κ1 + κ 4 2 θ ∂ ρT ⎠ ⎢⎣ ⎝ ⎪⎩⎝
⎞ ⎟β ⎠
⎞ ⎟ ρT + ⎟ ⎠
(8.84)
⎞ ⎤ ⎛ ∂Aj ⎞ j ⎫⎪ P −1 ⎟ηW ⎥ + ⎜⎜ Aj − θ ⎟⎟ f ⎬W . ⎟ ⎥ θ ∂ ⎝ ⎠ ⎪⎭ ⎠ ⎦ is the TaylorQuinney parameter similar to that in (6.47) and (6.120), such that 1 − β ′ is the ratio of inelastic stress power W P converted to residual elastic energy. The inelastic stress power, per unit volume in configuration B , is, from (8.49), W P = Π : ⎡ LW + LP + (1/ 3) JJ −1 1⎤ ⎣ ⎦ (8.85) w n w n ⎛ ⎞ J tr(Π ). = ∑τ j f j γ j + (1 − fT )∑τ iγ i + ∑ ⎜ f j ∑τ jiγ ij ⎟ + j =1 i =1 j =1 ⎝ i =1 ⎠ 3J Definition (8.84) is expressed in terms of the total dislocation density. A more specific form of (8.84) accounting for distinct contributions from geometrically necessary and statistically stored dislocations can be determined in a straightforward manner by substituting (8.72) into (8.52). Consider next the energy of twin boundaries. Geometric arguments demonstrate that the area of twin boundaries per unit intermediate volume of lamellar twins can be approximated as
ρ b⎛ ⎜ κ 2 + κ 4b3 / 2 T 2 ⎜⎝ ηW
w
w
j =1
j =1
ηW ≈ 2∑ f j / t j , ηW ≈ 2∑ ⎡⎣ f j / t j − f j t j /(t j ) 2 ⎤⎦ ,
(8.86)
where t j is the average thickness of a twin comprising fraction j with volume fraction f j . From (8.84)(8.86), β ′ depends on both the volume fraction and average thickness of each representative twin system. The residual volume change J was introduced in Section 7.2.4 of Chapter 7, specifically following relations (7.43) and (7.58). An estimation of this quantity from nonlinear elasticity theory is given by (7.60): ⎞ ∆V 1 ⎛ ∂K 1 ⎛ ∂µ µ ⎞ = 1+ ⎜ − 1⎟WD + ⎜ − ⎟ WS , J =1+ (8.87) V K ⎝ ∂p µ ⎠ ⎝ ∂p K ⎠
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
415
where µ and K are isotropic shear and bulk moduli, p = −tr(σ) / 3 is the Cauchy pressure, and WD and WS are the dilatational and deviatoric strain energy densities per unit reference volume, respectively, associated with lattice defects. As an approximation, for anisotropic single crystals the bulk and shear elastic coefficients are defined as Voigt averages (A.36) and (A.38): 1 α .β 1 α .β (8.88) K= (3 αβ .α .β , µ = ..αβ − .α . β ) . 9 30 Shear and bulk moduli in (8.88) do not depend on temperature since the right sides of (8.88) are evaluated at the reference state, according to (8.57). Pressure derivatives of bulk modulus and shear modulus in (8.87) are measured at the reference state and are treated as constants. The volume change in (8.87) is measured between reference and intermediate configurations: ∆V = V − V with V the volume in B . Setting the residual free energy of (8.75), measured per unit volume in the reference configuration, equal to the sum of defect energies (Kocks et al. 1975), 1 JΨ R = WD + WS = J µ ⎡⎣κ1α 2 + κ 2 β 2 + κ 4α 2 β 2 ⎤⎦ 2 (8.89) 1 = J µ ⎡⎣κ1b 2 ρT + κ 2bηW + κ 4b3 ρTηW ⎤⎦ ≈ WS , 2 where in the final equality, the energy is approximated as purely deviatoric. From (8.87), 1 ⎛ ∂µ µ ⎞ J ≈1+ J ⎜ − ⎟ (κ1b 2 ρT + κ 2 bηW + κ 4 b3 ρTηW ) 2 ⎝ ∂p K ⎠
⎡ 1 ⎛ ∂µ µ ⎞ ⎤ = ⎢1 − ⎜ − ⎟ (κ1b 2 ρT + κ 2 bηW + κ 4 b3 ρTηW ) ⎥ ⎣ 2 ⎝ ∂p K ⎠ ⎦
−1
(8.90)
1 ⎛ ∂µ µ ⎞ ≈1+ ⎜ − ⎟ (κ1b 2 ρT + κ 2 bηW + κ 4 b3 ρTηW ) , 2 ⎝ ∂p K ⎠ where small residual volume changes J ≈ (1 − ∆V / V ) −1 are assumed in the last expression, following discussion after (7.72). Dependence of residual volume change on twin boundary energy in (8.90) is similar to dependence of volume on generic grain boundaries derived by Holder and Granato (1969). Dilatancy from stacking faults (Kenway 1993) and twin boundaries (Yoo and Lee 1991) has been predicted by atomic simulations. The material time derivative of (8.90) is
416
8 Mechanical Twinning in Crystal Plasticity
1 ⎛ ∂µ µ ⎞ − ⎟ ⎡(κ1b 2 + κ 4b3ηW ) ρT + (κ 2b + κ 4b3 ρT )ηW ⎤⎦ . (8.91) J ≈ ⎜ 2 ⎝ ∂p K ⎠ ⎣ Expressions (8.86), (8.90) and (8.91) can be substituted into (8.85) and (8.84), which in turn enter the energy balance (8.83) and dissipation inequality (8.48). If the shear modulus used to scale the residual free energy in (8.75) is assumed independent of temperature following Voigt approximation (8.88), then θ∂µ / ∂θ = 0 in (8.84). 8.2.5 Kinetics
Rate dependent, i.e., viscoplastic, kinetic laws are often used to describe shearing associated with slip (Hutchinson 1976; Teodosiu and Sidoroff 1976; Asaro 1983) and twinning (Tome et al. 1991; Kalidindi 1998; Wu et al. 2007). Representative kinetic equations can be written as
τi γ = γ0 i τˆ
m
τi , (∀i =1,...n ∈ parent) ; τ i 
i
τi γ = γ 0 ij τˆ j
m
i j
j γ0 τ f = j γ τˆ j j
τ ji τ ji
(8.92)
, (∀i =1,...n ∈ twins j =1,...w) ;
(8.93)
, (∀j =1,...w ∈ parent; fT < 1) .
(8.94)
p
Kinetic equation (8.92) is similar to flow rule (6.106) of crystal plasticity theory, with the resolved shear stress τ i = J E s i aσ a.b mi b in the first of (8.50) the thermodynamic work conjugate to slip rate γ i in the dissipation inequality (8.49) and in the rate of plastic working (8.85). No backstress is included for slip or twin rate equations in (8.92)(8.94), but a term such as χˆ i of (6.106) and (6.115) could be incorporated as appropriate. Relation (8.93) is a flow rule for n × w slip rates γ ij in reoriented regions of the twinned crystal. Resolved shear stress τ ji = J E s ij aσ a.b mijb in the second of (8.50) is the thermodynamic work conjugate to slip rate γ ij in the dissipation inequality (8.49) and in the plastic dissipation (8.85). Symbol γ 0 ≥ 0 denotes a material parameter with dimensions of inverse time that could depend on temperature (but is often taken as constant), and m is the rate sensitivity given by (6.90) in the context of single slip. Evolving resis
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
417
tances to slip on system i in the parent and on system i in twin fraction j are denoted, respectively, by τˆi ( X , t ) in (8.92) and τˆij ( X , t ) in (8.93). In (8.94), the rate of twinning shear f j γ shear stress component τ = J s σ m j
E
ja
.b a
j b
j
is dictated by the resolved
defined in the last of (8.50).
This shear stress is a thermodynamic work conjugate to shearing rate f j γ j in the dissipation inequality (8.49) and in the inelastic power (8.85). The stress in Macaulay brackets satisfies 2 τ j = τ j + τ j ≥ 0 . Because f j = 0 for τ j ≤ 0 , the unidirectional, i.e., polar, nature of twinning discussed in Section 8.1.3 is respected. The rate sensitivity parameter for twinning is written as p, and the resisting stress to twinning is τˆ j ( X , t ) . Conceivably, a different value of γ 0 could be used in each of (8.92)(8.94); in the simple treatment suggested here, differences among kinetic behaviors are assumed to be addressed by different initial values of and evolution equations for the slip resistances. In the limit m → ∞ or p → ∞ , rate independent behavior is attained for slip or twinning, respectively. Since detwinning and successive twinning are not considered here, the constraint f j = 0 applies when the crystal is fully twinned and fT = 1 . Special or alternative forms of (8.94) may be required to address load drops and serrated stressstrain responses observed for some twinned single crystals. From (8.92)(8.94), any nonzero contribution of slip and twinning to the rate of inelastic working (8.85) is always positive, since J tr(Π ) 3J p (8.95) m ⎡w i m n w ⎛ n τj τ ji ⎞ ⎤⎥ j i τ j i ⎢ ⎜ ⎟ = γ 0 ∑τ + (1 − fT )∑ τ +∑ f ∑τj i ≥ 0. ⎢ j =1 τˆ j τˆi τˆ j ⎟ ⎥ i =1 j =1 ⎜ i =1 ⎝ ⎠ ⎦⎥ ⎣⎢ Written generically, evolution equations for slip and twin resistances are expressed as τˆi = τˆi ( EE ,θ , αˆ ,α , β ,{ f j },{τˆ} , X , gα ) , (8.96) WP −
τˆij = τˆij ( EE ,θ , αˆ ,α , β ,{ f j },{τˆ} , X , gα ) ,
τˆ j = τˆ j ( EE ,θ , αˆ ,α , β ,{ f j },{τˆ} , X , gα ) .
(8.97) (8.98)
Hardening rates depend not only on the set of state variables that explicitly enter the free energy function (8.33), but also the set of hidden variables {τˆ} = {τˆi ,τˆij ,τˆ j } with i = 1,...n and j = 1,...w , consisting of all possible
418
8 Mechanical Twinning in Crystal Plasticity
slip and twinning resistances. If the residual free energy depends only the total scalar dislocation density ρT = α 2 / b 2 as in (8.75), it may be possible to replace (8.96)(8.98) with τˆi = τˆi ( EE ,θ ,α , β ,{ f j },{τˆ} , X , gα ) , (8.99)
τˆij = τˆij ( EE ,θ ,α , β ,{ f j },{τˆ} , X , gα ) ,
τˆ j = τˆ j ( EE ,θ ,α , β ,{ f j },{τˆ} , X , gα ) .
(8.100) (8.101)
Resistances to inelastic shearing modes can be described in terms of physical mechanisms by extending the treatments of dislocation kinetics in Sections 6.2 and 6.3 to include effects of twins. Following (6.99), resistance stresses {τˆ} entering (8.96)(8.101) are decomposed into sums of contributions of various mechanisms (Kocks et al. 1975; Clayton 2005a, b, 2009a): τˆi = τˆPi + τˆDi , τˆij = (τˆP )ij + (τˆD )ij , τˆ j = τˆWj + τˆDj . (8.102) In the first of (8.102), τˆPi reflects the initial yield stress in a defectfree crystal for slip on system i in the parent, and τˆDi reflects long range barriers associated with defects that accumulate during the deformation history. Analogous definitions apply for resistance to slip within the twins in the second of (8.102). Resistance to twin propagation in the third of (8.102) is likewise decomposed into a term τˆWj accounting for the initial resistance to twin nucleation and stress τˆDj due to interactions of twins with other twins and dislocations. Both terms in each sum in (8.102) depend on temperature. The initial yield stress (e.g., τˆPi ) depends on short range barriers such as Peierls barriers (see Section C.4.3) that may be significant at low temperatures or in crystals with low initial defect densities and nonmetallic bonds (Friedel 1964; Farber et al. 1993), and at high dislocation velocities also accounts for viscous, phonon, and electron drag (Kocks et al. 1975; Gilman 1979). An approximation often used for the twin nucleation stress follows from the energy required to translate a partial Burgers vector associated with a given twin system (Hirth and Lothe 1982): τˆWj ≈ WSFj / bPj , (8.103) where WSFj is the stacking fault energy associated with the movement of a twinning partial of Burgers magnitude bPj . The twin nucleation stress, like the slip resistance, can also depend on hydrostatic pressure, as indicated in atomic simulations (Xu et al. 2004). As noted in Section C.4.1, the theoretical strength (i.e., Frenkel’s model) has been suggested as a stress crite
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
419
rion for twin nucleation in metallic crystals (Bell and Cahn 1957; Paxton et al. 1991): τˆWj ≈ µγ j /(2π ) . A number of analytical treatments of thermodynamics of twin nucleation have been forwarded (Price 1961; Lee and Yoo 1990; Yoo and Lee 1991; Lebensohn and Tome 1993; Meyers et al. 2001). Such theories often seek the minimum stable size and shape of a twin nucleus via consideration of stationary points in the total Gibbs free energy (including external work, elastic strain energy, and surface energy of the twin boundary), and many of these theories incorporate aspects of Eshelby’s treatment of elastic inclusions and inhomogeneities (Eshelby 1961). In particular, Price (1961) and Lebensohn and Tome (1993) suggested formulae in which the twin nucleation stress is directly proportional to the twin boundary energy. Conceivably, long range barriers in each of (8.102) could depend in a complex manner upon activity of the slip or twin system under consideration (i.e., selfhardening) as well as the activity of all other slip systems (i.e., latent hardening) and twinning systems (Christian and Mahajan 1995; Wu et al. 2007). Possible impedance or facilitation of slip or twinning via slipslip interactions, sliptwin interactions, and twintwin interactions depends in a complex manner on a number of factors, including geometrical relationships among interacting systems, temperature, crystal structure, and defect content (Christian and Mahajan 1995; Kalidindi 1998; Castaing et al. 2002; Wu et al. 2007). Experimental data enabling unique quantification of these effects is often scarce, and mechanisms responsible for hardening are not fully understood in many materials (Lagerlof et al. 1994; Kalidindi 1998). Because of the large number of parameters required for a complete description of the interactions among individual deformation mechanisms, many experiments may be required, with delineation of effects of a particular mechanism difficult. Initial values of hardness in (8.102) may differ among different slip and twin families in a crystal, and account for periodic lattice resistance in an initially perfect lattice (Peierls 1940; Nabarro 1947), friction stress (Beltz et al. 1996), and other initial barriers, for example those resulting from interstitials in crystals with impurities (Kocks et al. 1975). Short range barriers to dislocation motion are often strongly temperature dependent (KuhlmannWilsdorf 1960; Kocks et al. 1975), since increases in temperature correlate with increased probability of dislocations overcoming such barriers via thermal activation, as discussed in Section 6.2. Long range barriers typically arise from interactions of local stress fields among defects, and generally increase with defect densities that accumulate with strain until saturation. Twinning resistance is often affected by temperature, but at low temperatures may increase less steeply than slip resistance as the temperature is decreased (Christian and
420
8 Mechanical Twinning in Crystal Plasticity
Mahajan 1995). This phenomenon explains the tendency for many solids to favor twinning over slip at low temperatures. The resistance to twinning may even decrease with decreasing temperature (Christian and Mahajan 1995). Twinning is observed frequently in shockloaded metallic and ceramic crystals (Rohatgi and Vecchio 2002; Bourne et al. 2007). Evolution equations for variables α and β , respectively reflecting densities of statistically stored dislocations and twin boundaries as indicated in (8.29) and (8.30), complete the model. A separate evolution equation for the geometrically necessary dislocation density tensor is not needed since αˆ is obtained directly from kinematic relations (8.24)(8.28), leading to the rate equation d αˆ αβ = ⎡⎣ F W .βχ F P.χAε ABC ( F W α.β F P.βB ,C + F W α.β ,C F P.βB )⎤⎦ dt = ( F W. χ β F P.χA + F W .βχ F .PAχ )ε ABC ( F W α.β F P.βB ,C + F W α.β ,C F P.βB ) (8.104) + F W .βχ F P.χAε ABC × ( F W.β α F P.βB ,C + F W.β α,C F P.βB + F W α.β F .PBβ,C + F W α.β ,C F .PBβ ).
Terms entering (8.104) are obtained from updated plastic and twinning deformations, their rates in (8.20) and (8.21), and their partial derivatives taken with respect to material coordinates X A . Analogously to hardening evolution laws listed in (8.96)(8.101), defect densities may depend upon the history of slip and twin activity, as well as crystal structure and material composition. Generic evolution equations are written for statistically stored dislocations and the twin boundary area density, respectively as ρ S = ρ S ( EE ,θ , αˆ ,α , β ,{ f j }, {τˆ} , X , gα ) , (8.105)
ηW = ηW ( EE ,θ , αˆ ,α , β ,{ f j },{τˆ} , X , gα ) .
(8.106)
From (8.105) and (8.106), Helmholtz free energy (8.33) depends on the shear resistances (i.e., hidden variables) {τˆ} implicitly, via their influence on the evolution of the internal state variables. Kinetic equation (8.106) becomes redundant if, instead, an equation for thickness of each twin t j in (8.86) is prescribed. If the residual free energy depends only the total scalar dislocation density as in (8.75), (8.104) need not be exercised, and (8.105) and (8.106) can be replaced with (8.107) ρT = ρT ( EE ,θ , α , β ,{ f j }, {τˆ} , X , gα ) ,
ηW = ηW ( EE ,θ ,α , β ,{ f j },{τˆ} , X , gα ) .
(8.108)
Since a consensus on appropriate functional forms of evolution laws for hardening, (8.96)(8.101), and defect densities, (8.105)(8.108), for generic
8.2 Crystal Plasticity with Twins and Inelastic Volume Changes
421
crystalline solids undergoing simultaneous slip and twinning does not seem to exist, more specific forms of these equations are not included in this text. Examples of kinetic relations are available in the literature for certain metals (Van Houtte 1978; Tome et al. 1991; Kalidindi 1998; Staroselsky and Anand 2003; Wu et al. 2007; Proust et al. 2009) and ceramics (Scott and Orr 1983; Lagerlof et al. 1994; Castaing et al. 2002; Clayton 2009a, 2010c, d). The kinetic relations offered in Section 8.2.5 make no attempt to model geometry of twins (apart from simple relation (8.86)), nor do they capture interface morphology. A more refined treatment of thermodynamics and interface kinetics is required to address such aspects of microstructure evolution (Rosakis and Tsai 1995; Hou et al. 1999).
9 Generalized Inelasticity
The twoterm multiplicative decomposition of the deformation gradient used in Chapter 6 does not explicitly account for residual deformation of the lattice, or in other words, does not account for irreversible deformations that are not latticepreserving. Recall from Section 3.2 that the latticepreserving part of the deformation gradient is attributed to plasticity from crystal dislocations, specifically dislocation glide and relative shearing of crystallographic planes in increments of the Burgers vector for slip. Residual deformations that are not explicitly addressed in the definition of plastic deformation used in this text may emerge from the following physical mechanisms: residual elastic deformation and residual volume changes associated with selfequilibrated stress fields of defects (Section 3.2.9 and Chapter 7), lattice rotations and reflections associated with twinning (Chapter 8), volumetric deformation associated with voids and point defects (Sections 3.2.8 and 7.4), and anisotropic damage mechanisms such as ductile or brittle fracture and material rupture. When treated distinctly from mechanically reversible elastic deformation as in the nonstandard model of thermoelasticity of Section 5.5, deformation associated with thermal strains can also be categorized as a residual deformation mode distinct from plastic deformation. Inelastic deformations accommodated by damage mechanisms are commonplace in brittle crystals, in which dislocations may be scarce, or in which barriers to dislocation motion and twinning may be very large. Large deformations of an element of a brittle solid may be sustained by generation of surfaces within the element and subsequent local motions of these surfaces. The term damage is used in this text to denote generic mechanisms of generation, growth, and motion of such internal surfaces whose creation requires breaking of atomic bonds. Often these surfaces support no mechanical forces, i.e., they are free of mechanical traction, and hence labeled free surfaces. However, damage surfaces are not always required to be traction free; for example, frictional forces may be supported at crack faces in sliding contact. Regardless of the ductility of the crystal, volumetric strains cannot be sustained by dislocation glide since such dislocation motion is conservative, as discussed in Sections 3.2.2, 3.2.5, and 7.1.1. Nor can volumetric strains be accommodated by deformation twin
J.D. Clayton, Nonlinear Mechanics of Crystals, Solid Mechanics and Its Applications 177, DOI 10.1007/9789400703506_9, © Springer Science+Business Media B.V. 2011
423
424
9 Generalized Inelasticity
ning, which is also isochoric, as discussed in Sections 8.1.3 and 8.2.1. Hence, inelastic tensile volumetric deformations are accommodated, out of geometric necessity, through damage mechanisms or increases in free volume, even in ductile crystals1. On the other hand, as discussed in Section 5.3, large compressive volume changes are often accommodated elastically, commensurate with large compressive pressures that suppress damage modes such as void growth or crack opening. Constitutive formulations described in Chapter 9 account explicitly for residual lattice deformations. A generic threeterm decomposition for the deformation gradient, written as F = F E F R F P , is used, as proposed by Kratochvil (1972) in a generalized, geometrically nonlinear kinematic and thermodynamic treatment of elasticplastic crystalline solids. The intermediate or generic residual deformation (tangent map), denoted in Chapter 9 as F R ( X , t ) , accounts for all mechanically irreversible deformations that are not latticepreserving, and may encompass thermal deformations as a particular case. Accordingly, such thermal deformations are not deemed mechanically reversible, but may be reversed by restoration of a crystal to its reference temperature. Intermediate term F R is able to account for porosity increase or reduction, deformation resulting from isotropic or anisotropic damage mechanisms, and residual elastic lattice deformation associated with microscopic stress fields of individual lattice defects or their heterogeneous distributions within a volume element of material whose centroid is located at X. Furthermore, F R encompasses deformations associated with vacancies and twins, as addressed already in Chapters 7 and 8, respectively. In what follows first in Chapter 9, a general thermodynamic analysis is conducted wherein F R is defined in a generic, fully anisotropic sense. The Helmholtz free energy of a volume element of fixed mass of the solid is assumed to depend minimally upon strain associated with the recoverable elastic deformation F E , temperature, position and orientation of the element (i.e., heterogeneity and anisotropy), and a generic internal state variable. This internal state variable could reflect residual stress fields associated with defects or tangent elastic stiffness reduction associated with damage. An explicit dependence of free energy density on F R can be used (Clayton and McDowell 2003a; Clayton et al. 2004b), or temperature and internal state variables can be assumed to encompass free energy variations and constitutive dependencies implicitly associated with variations of F R . 1 Volume changes in crystals can also occur during phase transformations, but the topic of phase transitions falls outside the scope of this text.
9.1 Threeterm Elastoplasticity: General Principles
425
Particular forms of F R corresponding, respectively, to isotropic porosity in the context of the kinematic description of Section 3.2.8 and residual elastic lattice deformation in the context of the kinematic description of Section 3.2.9, are considered in turn in Sections 9.2 and 9.3. Finally, a constitutive framework for thermomechanical behavior of elastoplastic crystals, explicitly incorporating residual elasticity and internal variables of the higher gradient type (Clayton et al. 2004b, 2006), is presented in Section 9.4. Specifically, this framework accounts for continuous distributions of geometrically necessary and statistically stored dislocation and disclination lines, complementing the differentialgeometric description of micropolar kinematics of defective crystals of Section 3.3.3.
9.1 Threeterm Elastoplasticity: General Principles The following topics are addressed in Section 9.1. A kinematic description of solids involving a threeterm multiplicative decomposition of the total deformation gradient for a v